advertisement

www.EasyEngineering.net ww w.E a syE ngi nee rin g.n et **Note : Other Websites/Blogs Owners we requested you, Please do not Copy (or) Republish this Material. This copy is NOT FOR SALE. **Disclimers : EasyEngineering does not own this book/materials, neither created nor scanned. we provide the links which is already available on the internet. For any quarries, Disclaimer are requested to kindly contact us. We assured you we will do our best. We DO NOT SUPPORT PIRACY, this copy was provided for students who are financially troubled but deserving to learn. www.EasyEngineering.net Thank You and God Bless! www.EasyEngineering.net ww w.E asy En gin ee rin g.n et www.EasyEngineering.net www.EasyEngineering.net ww SEMICONDUCTOR DEViCE FUNDAMENTALS w.E as y En gin e Robert F. Pierret eri ng. ne School of Electrical and Computer Eitginecrjttg Pstrduc University t A “V ADDISONWESLEY PUBLTSmNG COMPANY Reading, Massachusetts Mettle Park, Colifornia New York Don Mills. Ontario Wokin,,ham Eisgloed Amstcnijarn Bonn Sydney Singapore Tokyo Madrid Son Joan Milan Paris - - - . - - ‘ ‘ ‘ - - www.EasyEngineering.net —Katherine Harutunian Associate Editor Helen Wythe Se,oor Prodactio,t Sopen’isor Hugh Crawford Manaafactarisag Supervisor Barbara Atkinson Associate Cover Design Supervisor PeterBtaiwas Csverdesign Kenneth J. Wilson Text design Joyce Grandy Copyeditor Sandra Rigney Productis,t Packaging Services 0 & S Typesetters, Inc. Composition Publishers’ Design and Production Services, Inc. Illustrations Library of Congress Cataloging-in-Publication Data Pierret, Robert 1°. Snmicnnductor dnvine fundamentals / Robert F. Pierrei. tentades usdos. ISBN 0-20t-54393-l I, Semiconductors I. Title. TK787l.85.P484 t996 62l.38152—dc2O 95-17387 CIP are claimed Many of the designations used by manufacturers and sellers tn distinguish their products sley was owara of a at trademarks. Where these designations appear in this honk, arid Addison-We caps. cops neat! initial trademark claim, the dnsignanons hate been printed is Morton isa registered trademsrk of Tire MathWnrks, tee., 24 Prima Park Way. Namick. MA 01760-1500. Phone: (5081 653-1415 Fax: (508) 653-2997 E-mail: infu@mathworks.coni WWW hctp / / wwca rsatlicsocko .com . site or nur hh’ortd Access the latest inrfornsation about Addisun-Wesley books from nut Internet gopher Wide Web page: gopher uw.com http://sswv.ocr.com /cseeig / Copyright: © 1996 by Addison-Wesley Publishing Cempany, Inc. Reprintod with corrections March, 1996 system, or Alt rights reserved. No part of this publication may bn reprnducnd. stured in a retrieval er other transmitted in any form or by any ereans, electronic, mechanical, photocopying, encerding. publisher. ef the wise, without thr written permission Prided io ihn United States of America ‘TIte itale voice inside ,tever groiv.s arty older-.” Frank Pierret (1906—1994) www.EasyEngineering.net SEMICONDUCTOR DEViCE ww w. DAMENTALS FUN Ea sy En gin Robert F. Pierret eer School of Electrical and Computer Eitginecrjttg Pstrduc University ing . net A “V ADDISONWESLEY PUBLTSmNG COMPANY Reading, Massachusetts Mettle Park, Colifornia New York Don Mills. Ontario Wokin,,ham Eisgloed Amstcnijarn Bonn Sydney Singapore Tokyo Madrid Son Joan Milan Paris - - - . - - ‘ ‘ ‘ - - www.EasyEngineering.net —Katherine Harutunian Associate Editor Helen Wythe Se,oor Prodactio,t Sopen’isor Hugh Crawford Manaafactarisag Supervisor Barbara Atkinson Associate Cover Design Supervisor PeterBtaiwas Csverdesign Kenneth J. Wilson Text design Joyce Grandy Copyeditor Sandra Rigney Productis,t Packaging Services 0 & S Typesetters, Inc. Composition Publishers’ Design and Production Services, Inc. Illustrations Library of Congress Cataloging-in-Publication Data Pierret, Robert 1°. Snmicnnductor dnvine fundamentals / Robert F. Pierrei. tentades usdos. ISBN 0-20t-54393-l I, Semiconductors I. Title. TK787l.85.P484 t996 62l.38152—dc2O 95-17387 CIP are claimed Many of the designations used by manufacturers and sellers tn distinguish their products sley was owara of a at trademarks. Where these designations appear in this honk, arid Addison-We caps. cops neat! initial trademark claim, the dnsignanons hate been printed is Morton isa registered trademsrk of Tire MathWnrks, tee., 24 Prima Park Way. Namick. MA 01760-1500. Phone: (5081 653-1415 Fax: (508) 653-2997 E-mail: infu@mathworks.coni WWW hctp / / wwca rsatlicsocko .com . site or nur hh’ortd Access the latest inrfornsation about Addisun-Wesley books from nut Internet gopher Wide Web page: gopher uw.com http://sswv.ocr.com /cseeig / Copyright: © 1996 by Addison-Wesley Publishing Cempany, Inc. Reprintod with corrections March, 1996 system, or Alt rights reserved. No part of this publication may bn reprnducnd. stured in a retrieval er other transmitted in any form or by any ereans, electronic, mechanical, photocopying, encerding. publisher. ef the wise, without thr written permission Prided io ihn United States of America ‘TIte itale voice inside ,tever groiv.s arty older-.” Frank Pierret (1906—1994) SEMICONDUCTOR DEViCE FUNDAMENTALS Robert F. Pierret School of Electrical and Computer Eitginecrjttg Pstrduc University A “V ADDISONWESLEY PUBLTSmNG COMPANY Reading, Massachusetts Mettle Park, Colifornia New York Don Mills. Ontario Wokin,,ham Eisgloed Amstcnijarn Bonn Sydney Singapore Tokyo Madrid Son Joan Milan Paris - - - . - - ‘ ‘ ‘ - - www.EasyEngineering.net —Katherine Harutunian Associate Editor Helen Wythe Se,oor Prodactio,t Sopen’isor Hugh Crawford Manaafactarisag Supervisor Barbara Atkinson Associate Cover Design Supervisor PeterBtaiwas Csverdesign Kenneth J. Wilson Text design Joyce Grandy Copyeditor Sandra Rigney Productis,t Packaging Services 0 & S Typesetters, Inc. Composition Publishers’ Design and Production Services, Inc. Illustrations ww w ‘TIte itale voice inside ,tever groiv.s arty older-.” Frank Pierret (1906—1994) Library of Congress Cataloging-in-Publication Data Pierret, Robert 1°. Snmicnnductor dnvine fundamentals / Robert F. Pierrei. .Ea tentades usdos. ISBN 0-20t-54393-l I, Semiconductors I. Title. TK787l.85.P484 t996 62l.38152—dc2O syE ngi 95-17387 CIP nee rin g are claimed Many of the designations used by manufacturers and sellers tn distinguish their products sley was owara of a at trademarks. Where these designations appear in this honk, arid Addison-We caps. cops neat! initial trademark claim, the dnsignanons hate been printed is Morton isa registered trademsrk of Tire MathWnrks, tee., 24 Prima Park Way. Namick. MA 01760-1500. Phone: (5081 653-1415 Fax: (508) 653-2997 E-mail: infu@mathworks.coni WWW hctp / / wwca rsatlicsocko .com .ne t . site or nur hh’ortd Access the latest inrfornsation about Addisun-Wesley books from nut Internet gopher Wide Web page: gopher uw.com http://sswv.ocr.com /cseeig / Copyright: © 1996 by Addison-Wesley Publishing Cempany, Inc. Reprintod with corrections March, 1996 system, or Alt rights reserved. No part of this publication may bn reprnducnd. stured in a retrieval er other transmitted in any form or by any ereans, electronic, mechanical, photocopying, encerding. publisher. ef the wise, without thr written permission Prided io ihn United States of America www.EasyEngineering.net SEMICONDUCTOR DEViCE FUNDAMENTALS Robert F. Pierret School of Electrical and Computer Eitginecrjttg Pstrduc University A “V ADDISONWESLEY PUBLTSmNG COMPANY Reading, Massachusetts Mettle Park, Colifornia New York Don Mills. Ontario Wokin,,ham Eisgloed Amstcnijarn Bonn Sydney Singapore Tokyo Madrid Son Joan Milan Paris - - - . - - ‘ ‘ ‘ - - www.EasyEngineering.net —Katherine Harutunian Associate Editor Helen Wythe Se,oor Prodactio,t Sopen’isor Hugh Crawford Manaafactarisag Supervisor Barbara Atkinson Associate Cover Design Supervisor PeterBtaiwas Csverdesign Kenneth J. Wilson Text design Joyce Grandy Copyeditor Sandra Rigney Productis,t Packaging Services 0 & S Typesetters, Inc. Composition Publishers’ Design and Production Services, Inc. Illustrations Library of Congress Cataloging-in-Publication Data Pierret, Robert 1°. Snmicnnductor dnvine fundamentals / Robert F. Pierrei. tentades usdos. ISBN 0-20t-54393-l I, Semiconductors I. Title. TK787l.85.P484 t996 62l.38152—dc2O 95-17387 CIP are claimed Many of the designations used by manufacturers and sellers tn distinguish their products sley was owara of a at trademarks. Where these designations appear in this honk, arid Addison-We caps. cops neat! initial trademark claim, the dnsignanons hate been printed is Morton isa registered trademsrk of Tire MathWnrks, tee., 24 Prima Park Way. Namick. MA 01760-1500. Phone: (5081 653-1415 Fax: (508) 653-2997 E-mail: infu@mathworks.coni WWW hctp / / wwca rsatlicsocko .com . ‘TIte itale voice inside ,tever groiv.s arty older-.” ww w.E Frank Pierret (1906—1994) asy En gin eer ing .ne site or nur hh’ortd Access the latest inrfornsation about Addisun-Wesley books from nut Internet gopher Wide Web page: gopher uw.com http://sswv.ocr.com /cseeig / Copyright: © 1996 by Addison-Wesley Publishing Cempany, Inc. Reprintod with corrections March, 1996 system, or Alt rights reserved. No part of this publication may bn reprnducnd. stured in a retrieval er other transmitted in any form or by any ereans, electronic, mechanical, photocopying, encerding. publisher. ef the wise, without thr written permission Prided io ihn United States of America www.EasyEngineering.net t www.EasyEngineering.net PREFACE ww Why another text on solid slate devices? The author is aware of at leust 14 undergraduate texts published on the subject during the past decade. Although several motivating factors could be cited, a veiy siguificant factor svas the desire to write a hook for the next milieu niom (a Book 2000 so to speak) that successfully incorporates computer-assisted leurnieg. In a recent survey, members of the Undcrgradttate Corricutem Committee in the Scheet of Electrical and Computer Engineerieg at Puedse University listed integration of the com paler into the learning process m the number eec priority. Nationally, enisersily censor tiums have hccu forissed wlsich emphasize computer-assisted learning. In Janamy 1992. distribution begais of the Student Edition of M.-titoe, essentially a copy of the original MATI.Au manual bundled wish u loss-cost version of she math-loots softsrare. Over 37.000 copies of the bootcJsoftsvarc were sold in the first ycart Tents and books on a variety of topics frose several publishers axe now available that nseke specific ase of the MATLAB software. The direction is clear as soc proceed into the second millennium: Cumpesvr assisted learnusg svill bzcvnie esore and more prevalent. In dealing svith solid state deviccs, lie cmsspsstcr alloses ott to address more realistic prohlems, to more readily experiment mitts “wtsal-if’ scenarios, and to conveniretly ahtain a graphical output. An entire device characteristic can often he cosepuler gesserated with less time and effort than a small set of manually calculated single-point values. It should be clarified Ilsat the present tent is not a totally new entry in the field, but is derived in part from Volumes 1—tv of the Addison-Wesley Modular Series en Solid State Devices. Lest there be a misunderstanding, the latest versions of the volumes in the Modu lar Series were net siesply glued together. To the conlrary, more than half of lhc material coverage in the feor vatanmes was completely rewritten. Moreover, seseral sappleasental sections and two additional chapters snere added to tIre Velnnses I—IV entline. The new lent also contains computer-based tent exercises and end-of-chapter problems, plus a number of other special features that are folly described in the General Introduction. In jest abssut any engineering endeavor there are tradeoffs. Device design is replete with tradeoffs. Tradeofts also enter into the design of a book. For example, a few topics can be covered in detail (depth) or lesser coverage can be given to several topics lbreadsh). Sunilarly one can emphasize she understanding of cosscepss or optissaze the transmission of facteal iaforniatien. Votames I—tv in the Modular Series ore known for streir pedantic depth of coverage emphusiniisg concepts. While retaining she same basic depth of coverage. four “read-only” chapters have been specifically udded herein to broaden she coverage and enhance the transesissien of factoal information. In the read-only chapters the emplsesis is more on describing the enciriug world of modern-day devices. Compound semicondocror devices likesvise receive increased coverage throughout the tent. There in also a natural w.E as y En gin e eri ng. ne t www.EasyEngineering.net Vi nEMle0NDttT0R nuetee raNeeMeNTALn tradeoff betsneen the effort devoted to developing qaulitative insight and she implementa tion of a quantitative aealysis. Careful aoentian has been given to avoid slighting the de velopment of “insuition” in light of the greatly esshaoced qaautitative capabilities arising from she integrated use of the computer. Lastly, sve have not attempted so be all-inclusive in the depth and breadth of coverage—many things we left for later (another coarse, other books). Hopefully, she proper tradeoffs have been echieved whemby sIte reader is reosen ably knowledgeable about the subject matter and acceptably equipped so perform device analyses ufser completing the tent. The present test is intended for andcrgraduatejaniOrs or seniors who have had at leant an introductory enposure to electric field theory. Chapters are gronped into three major divisions or “parts,” snith Port II being further subdivided into IIA and lIE. With some deletions, the materiel in each of the three parts is covered durissg a five-week segment of a ane-sementer, three-credit-bane, junior-senior course in Electrical and Cempuler Engi neering at Purdne University. A day-by-day ratmete outline is supplied an Ihe Instsncter’s Disk arconspanying the Selations Manual. If necessary to meet time cnrstramets, read-only Chapters 4, 9. 13, and 19 could be deleted from the lecture schedule. )An instmetor might preferably assign the chapters us independemst readings and reward compliant students by including entra-credit examination questiests covering the material.) Standard Chapters 12, 14, and 15, encepr fee tlte gesseral field-effect introduction in Sectien l5.t, may otto be omitted ssith little or so less in continuity. Although a complete listing of special featares is given in rhe General Introduction, instructors should take special stole of the Problem Information Tables inserted prior In the end-of-chapter problems. These tables should prove useful in assigning problems and in dealing with hemee’ork graders. When faced with constructing a test, instructors may also he interested in esuminitsg the Review Problem Sets found in lbs teini-chapters (identified by a darkened thnnsb tab) at the esmd of the three honk parts. The Review Problem Sets are derived from old “open-book” and “closed-book” tests. Concerning the cemgoter-based enercises and problems, she use of rilber the student or professional version of MATLAn it recismmended but not reqaired. The its-tent eneecise solutions and the problem answers supplied 10 the iessrucsar, however, do make ase of MATLAn. Although it would be helpful, the asee need not be familiar with the MATLAR progeans at the beginning of the book. The MATLAe problems in successive chapters make increasiagly sophisticated use of the pro gram. In otluer words, the early exercises and hosoesverk problems provide a learning Mus’t.An by rising hulATLAs eapnrietsze. isis critical, however, that the asee complete a large percentage of the computer-based exercises and problems in the first three chapters. The exercises and peablenas found in later chapters sot only assume a reasonably competent use of MATLAB. but also baild span the programs developed in Ihe earlier chapters. The author eratefally acknowledges lIme assistavee of associates, EE3OS students. the cespandeists to an curly marketing survey, the manusrript revtesvers, and Addison-Wesley personnel ie nraking Book 2000 a reality. Desvrvrsg of special lhartks is Alt Keshavarzi for arruagieg the ummthoe’v sabbatical at latel Corporation and for providing photographs of equipment inside the Albnqtmerqsme fobricatrort facility. Prof. Mark Lundstram al Pnrdae Uoiversity seas also most helpfal in supplying key ieformatien aad figares for several book sections. Of the undergraduate students asked to enamine the manascript for readability ‘I raeeeee - and errors, Eric Bragg stands out as especially perceptive and helpful. The very eonsciea tious snanuscripl reviesvers svem Prof. Kenneth A. James, California State Unisersity, Long Beach: Prof. Peter Lanyen, Worcester Polytechnic Institute: Prof. Gary’ S. May, Georgia tnstmtsse of Teelruology: Prof Dieter K. Srhrader, Arizona State University: and Prof. G. Vs. Strllman, Universrmy of Illinois as Urbana-Champaign. In recegvition of u femmimfat associa tion, a speciol thamsks to Don Pawley, the former editor at Addison-Wesley who enlieed the aothae into wriling the book. Last bet trot least, editor Katherine Hamtnnian is Ia be ered iled seith smoothly implesnenliag the project, and enecolive ossistant Anita Devine with chreerfelly handling mmsany of the early details. Prof Roberm F Fiercer School of Electrical and Computer Engineering Purdue University eli www.EasyEngineering.net PREFACE Why another text on solid slate devices? The author is aware of at leust 14 undergraduate texts published on the subject during the past decade. Although several motivating factors could be cited, a veiy siguificant factor svas the desire to write a hook for the next milieu niom (a Book 2000 so to speak) that successfully incorporates computer-assisted leurnieg. In a recent survey, members of the Undcrgradttate Corricutem Committee in the Scheet of Electrical and Computer Engineerieg at Puedse University listed integration of the com paler into the learning process m the number eec priority. Nationally, enisersily censor tiums have hccu forissed wlsich emphasize computer-assisted learning. In Janamy 1992. distribution begais of the Student Edition of M.-titoe, essentially a copy of the original MATI.Au manual bundled wish u loss-cost version of she math-loots softsrare. Over 37.000 copies of the bootcJsoftsvarc were sold in the first ycart Tents and books on a variety of topics frose several publishers axe now available that nseke specific ase of the MATLAB software. The direction is clear as soc proceed into the second millennium: Cumpesvr assisted learnusg svill bzcvnie esore and more prevalent. In dealing svith solid state deviccs, lie cmsspsstcr alloses ott to address more realistic prohlems, to more readily experiment mitts “wtsal-if’ scenarios, and to conveniretly ahtain a graphical output. An entire device characteristic can often he cosepuler gesserated with less time and effort than a small set of manually calculated single-point values. It should be clarified Ilsat the present tent is not a totally new entry in the field, but is derived in part from Volumes 1—tv of the Addison-Wesley Modular Series en Solid State Devices. Lest there be a misunderstanding, the latest versions of the volumes in the Modu lar Series were net siesply glued together. To the conlrary, more than half of lhc material coverage in the feor vatanmes was completely rewritten. Moreover, seseral sappleasental sections and two additional chapters snere added to tIre Velnnses I—IV entline. The new lent also contains computer-based tent exercises and end-of-chapter problems, plus a number of other special features that are folly described in the General Introduction. In jest abssut any engineering endeavor there are tradeoffs. Device design is replete with tradeoffs. Tradeofts also enter into the design of a book. For example, a few topics can be covered in detail (depth) or lesser coverage can be given to several topics lbreadsh). Sunilarly one can emphasize she understanding of cosscepss or optissaze the transmission of facteal iaforniatien. Votames I—tv in the Modular Series ore known for streir pedantic depth of coverage emphusiniisg concepts. While retaining she same basic depth of coverage. four “read-only” chapters have been specifically udded herein to broaden she coverage and enhance the transesissien of factoal information. In the read-only chapters the emplsesis is more on describing the enciriug world of modern-day devices. Compound semicondocror devices likesvise receive increased coverage throughout the tent. There in also a natural ww w.E a syE ngi nee r ing . net www.EasyEngineering.net Vi nEMle0NDttT0R nuetee raNeeMeNTALn tradeoff betsneen the effort devoted to developing qaulitative insight and she implementa tion of a quantitative aealysis. Careful aoentian has been given to avoid slighting the de velopment of “insuition” in light of the greatly esshaoced qaautitative capabilities arising from she integrated use of the computer. Lastly, sve have not attempted so be all-inclusive in the depth and breadth of coverage—many things we left for later (another coarse, other books). Hopefully, she proper tradeoffs have been echieved whemby sIte reader is reosen ably knowledgeable about the subject matter and acceptably equipped so perform device analyses ufser completing the tent. The present test is intended for andcrgraduatejaniOrs or seniors who have had at leant an introductory enposure to electric field theory. Chapters are gronped into three major divisions or “parts,” snith Port II being further subdivided into IIA and lIE. With some deletions, the materiel in each of the three parts is covered durissg a five-week segment of a ane-sementer, three-credit-bane, junior-senior course in Electrical and Cempuler Engi neering at Purdne University. A day-by-day ratmete outline is supplied an Ihe Instsncter’s Disk arconspanying the Selations Manual. If necessary to meet time cnrstramets, read-only Chapters 4, 9. 13, and 19 could be deleted from the lecture schedule. )An instmetor might preferably assign the chapters us independemst readings and reward compliant students by including entra-credit examination questiests covering the material.) Standard Chapters 12, 14, and 15, encepr fee tlte gesseral field-effect introduction in Sectien l5.t, may otto be omitted ssith little or so less in continuity. Although a complete listing of special featares is given in rhe General Introduction, instructors should take special stole of the Problem Information Tables inserted prior In the end-of-chapter problems. These tables should prove useful in assigning problems and in dealing with hemee’ork graders. When faced with constructing a test, instructors may also he interested in esuminitsg the Review Problem Sets found in lbs teini-chapters (identified by a darkened thnnsb tab) at the esmd of the three honk parts. The Review Problem Sets are derived from old “open-book” and “closed-book” tests. Concerning the cemgoter-based enercises and problems, she use of rilber the student or professional version of MATLAn it recismmended but not reqaired. The its-tent eneecise solutions and the problem answers supplied 10 the iessrucsar, however, do make ase of MATLAn. Although it would be helpful, the asee need not be familiar with the MATLAR progeans at the beginning of the book. The MATLAe problems in successive chapters make increasiagly sophisticated use of the pro gram. In otluer words, the early exercises and hosoesverk problems provide a learning Mus’t.An by rising hulATLAs eapnrietsze. isis critical, however, that the asee complete a large percentage of the computer-based exercises and problems in the first three chapters. The exercises and peablenas found in later chapters sot only assume a reasonably competent use of MATLAB. but also baild span the programs developed in Ihe earlier chapters. The author eratefally acknowledges lIme assistavee of associates, EE3OS students. the cespandeists to an curly marketing survey, the manusrript revtesvers, and Addison-Wesley personnel ie nraking Book 2000 a reality. Desvrvrsg of special lhartks is Alt Keshavarzi for arruagieg the ummthoe’v sabbatical at latel Corporation and for providing photographs of equipment inside the Albnqtmerqsme fobricatrort facility. Prof. Mark Lundstram al Pnrdae Uoiversity seas also most helpfal in supplying key ieformatien aad figares for several book sections. Of the undergraduate students asked to enamine the manascript for readability ‘I raeeeee - and errors, Eric Bragg stands out as especially perceptive and helpful. The very eonsciea tious snanuscripl reviesvers svem Prof. Kenneth A. James, California State Unisersity, Long Beach: Prof. Peter Lanyen, Worcester Polytechnic Institute: Prof. Gary’ S. May, Georgia tnstmtsse of Teelruology: Prof Dieter K. Srhrader, Arizona State University: and Prof. G. Vs. Strllman, Universrmy of Illinois as Urbana-Champaign. In recegvition of u femmimfat associa tion, a speciol thamsks to Don Pawley, the former editor at Addison-Wesley who enlieed the aothae into wriling the book. Last bet trot least, editor Katherine Hamtnnian is Ia be ered iled seith smoothly implesnenliag the project, and enecolive ossistant Anita Devine with chreerfelly handling mmsany of the early details. Prof Roberm F Fiercer School of Electrical and Computer Engineering Purdue University eli PREFACE Why another text on solid slate devices? The author is aware of at leust 14 undergraduate texts published on the subject during the past decade. Although several motivating factors could be cited, a veiy siguificant factor svas the desire to write a hook for the next milieu niom (a Book 2000 so to speak) that successfully incorporates computer-assisted leurnieg. In a recent survey, members of the Undcrgradttate Corricutem Committee in the Scheet of Electrical and Computer Engineerieg at Puedse University listed integration of the com paler into the learning process m the number eec priority. Nationally, enisersily censor tiums have hccu forissed wlsich emphasize computer-assisted learning. In Janamy 1992. distribution begais of the Student Edition of M.-titoe, essentially a copy of the original MATI.Au manual bundled wish u loss-cost version of she math-loots softsrare. Over 37.000 copies of the bootcJsoftsvarc were sold in the first ycart Tents and books on a variety of topics frose several publishers axe now available that nseke specific ase of the MATLAB software. The direction is clear as soc proceed into the second millennium: Cumpesvr assisted learnusg svill bzcvnie esore and more prevalent. In dealing svith solid state deviccs, lie cmsspsstcr alloses ott to address more realistic prohlems, to more readily experiment mitts “wtsal-if’ scenarios, and to conveniretly ahtain a graphical output. An entire device characteristic can often he cosepuler gesserated with less time and effort than a small set of manually calculated single-point values. It should be clarified Ilsat the present tent is not a totally new entry in the field, but is derived in part from Volumes 1—tv of the Addison-Wesley Modular Series en Solid State Devices. Lest there be a misunderstanding, the latest versions of the volumes in the Modu lar Series were net siesply glued together. To the conlrary, more than half of lhc material coverage in the feor vatanmes was completely rewritten. Moreover, seseral sappleasental sections and two additional chapters snere added to tIre Velnnses I—IV entline. The new lent also contains computer-based tent exercises and end-of-chapter problems, plus a number of other special features that are folly described in the General Introduction. In jest abssut any engineering endeavor there are tradeoffs. Device design is replete with tradeoffs. Tradeofts also enter into the design of a book. For example, a few topics can be covered in detail (depth) or lesser coverage can be given to several topics lbreadsh). Sunilarly one can emphasize she understanding of cosscepss or optissaze the transmission of facteal iaforniatien. Votames I—tv in the Modular Series ore known for streir pedantic depth of coverage emphusiniisg concepts. While retaining she same basic depth of coverage. four “read-only” chapters have been specifically udded herein to broaden she coverage and enhance the transesissien of factoal information. In the read-only chapters the emplsesis is more on describing the enciriug world of modern-day devices. Compound semicondocror devices likesvise receive increased coverage throughout the tent. There in also a natural www.EasyEngineering.net Vi ‘I nEMle0NDttT0R nuetee raNeeMeNTALn tradeoff betsneen the effort devoted to developing qaulitative insight and she implementa tion of a quantitative aealysis. Careful aoentian has been given to avoid slighting the de velopment of “insuition” in light of the greatly esshaoced qaautitative capabilities arising from she integrated use of the computer. Lastly, sve have not attempted so be all-inclusive in the depth and breadth of coverage—many things we left for later (another coarse, other books). Hopefully, she proper tradeoffs have been echieved whemby sIte reader is reosen ably knowledgeable about the subject matter and acceptably equipped so perform device analyses ufser completing the tent. The present test is intended for andcrgraduatejaniOrs or seniors who have had at leant an introductory enposure to electric field theory. Chapters are gronped into three major divisions or “parts,” snith Port II being further subdivided into IIA and lIE. With some deletions, the materiel in each of the three parts is covered durissg a five-week segment of a ane-sementer, three-credit-bane, junior-senior course in Electrical and Cempuler Engi neering at Purdne University. A day-by-day ratmete outline is supplied an Ihe Instsncter’s Disk arconspanying the Selations Manual. If necessary to meet time cnrstramets, read-only Chapters 4, 9. 13, and 19 could be deleted from the lecture schedule. )An instmetor might preferably assign the chapters us independemst readings and reward compliant students by including entra-credit examination questiests covering the material.) Standard Chapters 12, 14, and 15, encepr fee tlte gesseral field-effect introduction in Sectien l5.t, may otto be omitted ssith little or so less in continuity. Although a complete listing of special featares is given in rhe General Introduction, instructors should take special stole of the Problem Information Tables inserted prior In the end-of-chapter problems. These tables should prove useful in assigning problems and in dealing with hemee’ork graders. When faced with constructing a test, instructors may also he interested in esuminitsg the Review Problem Sets found in lbs teini-chapters (identified by a darkened thnnsb tab) at the esmd of the three honk parts. The Review Problem Sets are derived from old “open-book” and “closed-book” tests. Concerning the cemgoter-based enercises and problems, she use of rilber the student or professional version of MATLAn it recismmended but not reqaired. The its-tent eneecise solutions and the problem answers supplied 10 the iessrucsar, however, do make ase of MATLAn. Although it would be helpful, the asee need not be familiar with the MATLAR progeans at the beginning of the book. The MATLAe problems in successive chapters make increasiagly sophisticated use of the pro gram. In otluer words, the early exercises and hosoesverk problems provide a learning Mus’t.An by rising hulATLAs eapnrietsze. isis critical, however, that the asee complete a large percentage of the computer-based exercises and problems in the first three chapters. The exercises and peablenas found in later chapters sot only assume a reasonably competent use of MATLAB. but also baild span the programs developed in Ihe earlier chapters. The author eratefally acknowledges lIme assistavee of associates, EE3OS students. the cespandeists to an curly marketing survey, the manusrript revtesvers, and Addison-Wesley personnel ie nraking Book 2000 a reality. Desvrvrsg of special lhartks is Alt Keshavarzi for arruagieg the ummthoe’v sabbatical at latel Corporation and for providing photographs of equipment inside the Albnqtmerqsme fobricatrort facility. Prof. Mark Lundstram al Pnrdae Uoiversity seas also most helpfal in supplying key ieformatien aad figares for several book sections. Of the undergraduate students asked to enamine the manascript for readability ww w .Ea syE ngi nee rin g .ne t www.EasyEngineering.net raeeeee - and errors, Eric Bragg stands out as especially perceptive and helpful. The very eonsciea tious snanuscripl reviesvers svem Prof. Kenneth A. James, California State Unisersity, Long Beach: Prof. Peter Lanyen, Worcester Polytechnic Institute: Prof. Gary’ S. May, Georgia tnstmtsse of Teelruology: Prof Dieter K. Srhrader, Arizona State University: and Prof. G. Vs. Strllman, Universrmy of Illinois as Urbana-Champaign. In recegvition of u femmimfat associa tion, a speciol thamsks to Don Pawley, the former editor at Addison-Wesley who enlieed the aothae into wriling the book. Last bet trot least, editor Katherine Hamtnnian is Ia be ered iled seith smoothly implesnenliag the project, and enecolive ossistant Anita Devine with chreerfelly handling mmsany of the early details. Prof Roberm F Fiercer School of Electrical and Computer Engineering Purdue University eli PREFACE Why another text on solid slate devices? The author is aware of at leust 14 undergraduate texts published on the subject during the past decade. Although several motivating factors could be cited, a veiy siguificant factor svas the desire to write a hook for the next milieu niom (a Book 2000 so to speak) that successfully incorporates computer-assisted leurnieg. In a recent survey, members of the Undcrgradttate Corricutem Committee in the Scheet of Electrical and Computer Engineerieg at Puedse University listed integration of the com paler into the learning process m the number eec priority. Nationally, enisersily censor tiums have hccu forissed wlsich emphasize computer-assisted learning. In Janamy 1992. distribution begais of the Student Edition of M.-titoe, essentially a copy of the original MATI.Au manual bundled wish u loss-cost version of she math-loots softsrare. Over 37.000 copies of the bootcJsoftsvarc were sold in the first ycart Tents and books on a variety of topics frose several publishers axe now available that nseke specific ase of the MATLAB software. The direction is clear as soc proceed into the second millennium: Cumpesvr assisted learnusg svill bzcvnie esore and more prevalent. In dealing svith solid state deviccs, lie cmsspsstcr alloses ott to address more realistic prohlems, to more readily experiment mitts “wtsal-if’ scenarios, and to conveniretly ahtain a graphical output. An entire device characteristic can often he cosepuler gesserated with less time and effort than a small set of manually calculated single-point values. It should be clarified Ilsat the present tent is not a totally new entry in the field, but is derived in part from Volumes 1—tv of the Addison-Wesley Modular Series en Solid State Devices. Lest there be a misunderstanding, the latest versions of the volumes in the Modu lar Series were net siesply glued together. To the conlrary, more than half of lhc material coverage in the feor vatanmes was completely rewritten. Moreover, seseral sappleasental sections and two additional chapters snere added to tIre Velnnses I—IV entline. The new lent also contains computer-based tent exercises and end-of-chapter problems, plus a number of other special features that are folly described in the General Introduction. In jest abssut any engineering endeavor there are tradeoffs. Device design is replete with tradeoffs. Tradeofts also enter into the design of a book. For example, a few topics can be covered in detail (depth) or lesser coverage can be given to several topics lbreadsh). Sunilarly one can emphasize she understanding of cosscepss or optissaze the transmission of facteal iaforniatien. Votames I—tv in the Modular Series ore known for streir pedantic depth of coverage emphusiniisg concepts. While retaining she same basic depth of coverage. four “read-only” chapters have been specifically udded herein to broaden she coverage and enhance the transesissien of factoal information. In the read-only chapters the emplsesis is more on describing the enciriug world of modern-day devices. Compound semicondocror devices likesvise receive increased coverage throughout the tent. There in also a natural Vi nEMle0NDttT0R nuetee raNeeMeNTALn tradeoff betsneen the effort devoted to developing qaulitative insight and she implementa tion of a quantitative aealysis. Careful aoentian has been given to avoid slighting the de velopment of “insuition” in light of the greatly esshaoced qaautitative capabilities arising from she integrated use of the computer. Lastly, sve have not attempted so be all-inclusive in the depth and breadth of coverage—many things we left for later (another coarse, other books). Hopefully, she proper tradeoffs have been echieved whemby sIte reader is reosen ably knowledgeable about the subject matter and acceptably equipped so perform device analyses ufser completing the tent. The present test is intended for andcrgraduatejaniOrs or seniors who have had at leant an introductory enposure to electric field theory. Chapters are gronped into three major divisions or “parts,” snith Port II being further subdivided into IIA and lIE. With some deletions, the materiel in each of the three parts is covered durissg a five-week segment of a ane-sementer, three-credit-bane, junior-senior course in Electrical and Cempuler Engi neering at Purdne University. A day-by-day ratmete outline is supplied an Ihe Instsncter’s Disk arconspanying the Selations Manual. If necessary to meet time cnrstramets, read-only Chapters 4, 9. 13, and 19 could be deleted from the lecture schedule. )An instmetor might preferably assign the chapters us independemst readings and reward compliant students by including entra-credit examination questiests covering the material.) Standard Chapters 12, 14, and 15, encepr fee tlte gesseral field-effect introduction in Sectien l5.t, may otto be omitted ssith little or so less in continuity. Although a complete listing of special featares is given in rhe General Introduction, instructors should take special stole of the Problem Information Tables inserted prior In the end-of-chapter problems. These tables should prove useful in assigning problems and in dealing with hemee’ork graders. When faced with constructing a test, instructors may also he interested in esuminitsg the Review Problem Sets found in lbs teini-chapters (identified by a darkened thnnsb tab) at the esmd of the three honk parts. The Review Problem Sets are derived from old “open-book” and “closed-book” tests. Concerning the cemgoter-based enercises and problems, she use of rilber the student or professional version of MATLAn it recismmended but not reqaired. The its-tent eneecise solutions and the problem answers supplied 10 the iessrucsar, however, do make ase of MATLAn. Although it would be helpful, the asee need not be familiar with the MATLAR progeans at the beginning of the book. The MATLAe problems in successive chapters make increasiagly sophisticated use of the pro gram. In otluer words, the early exercises and hosoesverk problems provide a learning Mus’t.An by rising hulATLAs eapnrietsze. isis critical, however, that the asee complete a large percentage of the computer-based exercises and problems in the first three chapters. The exercises and peablenas found in later chapters sot only assume a reasonably competent use of MATLAB. but also baild span the programs developed in Ihe earlier chapters. The author eratefally acknowledges lIme assistavee of associates, EE3OS students. the cespandeists to an curly marketing survey, the manusrript revtesvers, and Addison-Wesley personnel ie nraking Book 2000 a reality. Desvrvrsg of special lhartks is Alt Keshavarzi for arruagieg the ummthoe’v sabbatical at latel Corporation and for providing photographs of equipment inside the Albnqtmerqsme fobricatrort facility. Prof. Mark Lundstram al Pnrdae Uoiversity seas also most helpfal in supplying key ieformatien aad figares for several book sections. Of the undergraduate students asked to enamine the manascript for readability ‘I www.EasyEngineering.net raeeeee - eli and errors, Eric Bragg stands out as especially perceptive and helpful. The very eonsciea tious snanuscripl reviesvers svem Prof. Kenneth A. James, California State Unisersity, Long Beach: Prof. Peter Lanyen, Worcester Polytechnic Institute: Prof. Gary’ S. May, Georgia tnstmtsse of Teelruology: Prof Dieter K. Srhrader, Arizona State University: and Prof. G. Vs. Strllman, Universrmy of Illinois as Urbana-Champaign. In recegvition of u femmimfat associa tion, a speciol thamsks to Don Pawley, the former editor at Addison-Wesley who enlieed the aothae into wriling the book. Last bet trot least, editor Katherine Hamtnnian is Ia be ered iled seith smoothly implesnenliag the project, and enecolive ossistant Anita Devine with chreerfelly handling mmsany of the early details. ww w.E Prof Roberm F Fiercer School of Electrical and Computer Engineering Purdue University asy En gin eer ing .ne www.EasyEngineering.net t www.EasyEngineering.net CONTENTS General Introduction ww xxi Part I Semiconductor Fundamentals Chapter 1 Sensicundssrtors: A General introduction w.E 1.1 General Material l’roperties 1.1.1 Composition 1.1.2 Parity 1.1.3 Strttcture as y En gin e eri ng. ne t 3 3 5 6 1.2 Crystal Structure 1.2.1 TIte Uttit Cell Cotteept 1.2.2 Sinspte 3-D Unit Cells 1.2.3 Semicandt,ctor Lattices 1.2.4 Miller Indices 7 8 9 12 1.3 Crystal Growth 1.3.1 Gbtaiaiug Ultrapare Si 1.3.2 Siagle-Crystal Parmation 16 17 6 16 .4 Santmary 19 Problems 19 Chapter 2 Carrier Modeling 23 2.1 The Qnautizasion Concept 23 2.2 Semiconductor Models 2.2.1 Eooding Model 2.2.2 Energy Eansi Model 2.2.3 Carriers 2.2.4 Band Gap atsd Material Ctassifiratioa 2.3 Carrier Properties 26 26 29 31 25 32 32 32 34 2.3.1 Charge 2.3.2 Effective Mass 2.3.3 Carrier Nambers in Intrinsic Material www.EasyEngineering.net a neutcoNunceon DEVtCE ruouuMuNTALn 2.3.4 Mattipalatiats af Carrier Nambers—Daping 2.3.5 Carrier-Related Termiavlagy CONTENTS 35 40 2.4 State and Carrier Distributiass 2.4.1 Detttity af States 2.4.2 The Perttti Psmctioa 2.4.3 Equilibriuits Distribution of Carriers 40 41 42 46 2.5 Eqailibriate Carrier Concentrations 2.5.1 Pormelas for a aed ta 2.5.2 Altureative Eepressiees fare and p 2.5.3 a aed the tsp Pradact 2.5.4 Charge Neutrality Relationship 2.5.5 Cttrrier Concentration Calcalatians 2.5.6 Determitsation of Er 2.5.7 Carrier Concentration Temperature Dependence 49 49 52 53 57 59 61 65 2.6 Summary end Concluding Comments 67 Problems 69 Chapter 3 Carrier Action 3.1 Drift 3.1.1 3.1.2 3.1.3 3.1.4 3.1.5 75 75 Deheition—Visnaliaation DriE Carrent Mobility Resistivity Band Bendiag 3.2 Diffusion 3.2.! Dehnitioa —Visoalization 3.2.2 Hot-Poitst Probe Measurement 3.2.3 Diffasion and Total CnrrcoLs Diffasion Carrent.s Total Cnrrettts 3.2.4 Relatitsg Diffasion Coeffirients/Mobilisies Cottstancy of the Fermi Level Ctsrreut Plow Under Eqailibriam Conditions Einstein Relationship 3.3 Recombinatims—Generation 3.3.1 Debnitiost—Visnatieation Band-to-Baad Recombinatiaa 75 76 79 85 89 94 94 97 98 98 99 99 99 tot lot 105 105 105 R—f5 Center Recombitaation Aager Recombination Generation Processes 3.3.2 Mamensam Considerations 3.3.3 R—G Statistics Photogeneration Indirect Thermal Recombination—Generation 3.3.4 Minority Carrier Lifetimes General Information A Lifetime Measurement 3.4 Equations of Slate 3.4.1 Conlinuity Equations 3.4.2 Minority Carrier Diffusion Equations 3.4.3 Simptifications and Solations 3.4.4 Problem Solving Sample Problem No. I Sample Problem Na. 2 3.5 Supplemental Concepts 3.5.1 Diffusion Lengths 3.5.2 Quasi-Permi Levels 105 107 107 107 Ito to 112 116 116 116 t20 121 122 124 124 124 128 131 13 t 132 3.6 Summary and Concluding Comtoents 136 Problems 138 Chapter 4 Rasicn of Device Fabrication 4.1 Pabrication Processea 4.1.1 4.1.2 4.1.3 4.1.4 4.1.5 Gsidatian Diffusion lao Inaplantalian Lithography Thin-Filrtr Deposition Evstporation Spattering Chemical Vapor Deposition (CVD) 4.1.6 Epitasy 4.2 Device Fabrication Examples 4.2.1 pa Junction Diode Fabrication 4.2.2 Computer CPU Process Plow 4.3 Sammary 149 149 149 152 155 159 162 162 162 164 164 165 166 166 174 ul www.EasyEngineering.net CONTENTS General Introduction xxi Part I Semiconductor Fundamentals ww Chapter 1 Sensicundssrtors: A General introduction w.E a 1.1 General Material l’roperties 1.1.1 Composition 1.1.2 Parity 1.1.3 Strttcture 3 3 5 6 syE ngi 1.2 Crystal Structure 1.2.1 TIte Uttit Cell Cotteept 1.2.2 Sinspte 3-D Unit Cells 1.2.3 Semicandt,ctor Lattices 1.2.4 Miller Indices 1.3 Crystal Growth 1.3.1 Gbtaiaiug Ultrapare Si 1.3.2 Siagle-Crystal Parmation 6 7 8 9 12 nee r .4 Santmary Problems Chapter 2 Carrier Modeling ing . 16 16 17 net 19 19 23 2.1 The Qnautizasion Concept 23 2.2 Semiconductor Models 2.2.1 Eooding Model 2.2.2 Energy Eansi Model 2.2.3 Carriers 2.2.4 Band Gap atsd Material Ctassifiratioa 2.3 Carrier Properties 26 26 29 31 25 32 32 32 34 2.3.1 Charge 2.3.2 Effective Mass 2.3.3 Carrier Nambers in Intrinsic Material www.EasyEngineering.net a neutcoNunceon DEVtCE ruouuMuNTALn 2.3.4 Mattipalatiats af Carrier Nambers—Daping 2.3.5 Carrier-Related Termiavlagy CONTENTS 35 40 2.4 State and Carrier Distributiass 2.4.1 Detttity af States 2.4.2 The Perttti Psmctioa 2.4.3 Equilibriuits Distribution of Carriers 40 41 42 46 2.5 Eqailibriate Carrier Concentrations 2.5.1 Pormelas for a aed ta 2.5.2 Altureative Eepressiees fare and p 2.5.3 a aed the tsp Pradact 2.5.4 Charge Neutrality Relationship 2.5.5 Cttrrier Concentration Calcalatians 2.5.6 Determitsation of Er 2.5.7 Carrier Concentration Temperature Dependence 49 49 52 53 57 59 61 65 2.6 Summary end Concluding Comments 67 Problems 69 Chapter 3 Carrier Action 3.1 Drift 3.1.1 3.1.2 3.1.3 3.1.4 3.1.5 75 75 Deheition—Visnaliaation DriE Carrent Mobility Resistivity Band Bendiag 3.2 Diffusion 3.2.! Dehnitioa —Visoalization 3.2.2 Hot-Poitst Probe Measurement 3.2.3 Diffasion and Total CnrrcoLs Diffasion Carrent.s Total Cnrrettts 3.2.4 Relatitsg Diffasion Coeffirients/Mobilisies Cottstancy of the Fermi Level Ctsrreut Plow Under Eqailibriam Conditions Einstein Relationship 3.3 Recombinatims—Generation 3.3.1 Debnitiost—Visnatieation Band-to-Baad Recombinatiaa 75 76 79 85 89 94 94 97 98 98 99 99 99 tot lot 105 105 105 R—f5 Center Recombitaation Aager Recombination Generation Processes 3.3.2 Mamensam Considerations 3.3.3 R—G Statistics Photogeneration Indirect Thermal Recombination—Generation 3.3.4 Minority Carrier Lifetimes General Information A Lifetime Measurement 3.4 Equations of Slate 3.4.1 Conlinuity Equations 3.4.2 Minority Carrier Diffusion Equations 3.4.3 Simptifications and Solations 3.4.4 Problem Solving Sample Problem No. I Sample Problem Na. 2 3.5 Supplemental Concepts 3.5.1 Diffusion Lengths 3.5.2 Quasi-Permi Levels 105 107 107 107 Ito to 112 116 116 116 t20 121 122 124 124 124 128 131 13 t 132 3.6 Summary and Concluding Comtoents 136 Problems 138 Chapter 4 Rasicn of Device Fabrication 4.1 Pabrication Processea 4.1.1 4.1.2 4.1.3 4.1.4 4.1.5 Gsidatian Diffusion lao Inaplantalian Lithography Thin-Filrtr Deposition Evstporation Spattering Chemical Vapor Deposition (CVD) 4.1.6 Epitasy 4.2 Device Fabrication Examples 4.2.1 pa Junction Diode Fabrication 4.2.2 Computer CPU Process Plow 4.3 Sammary 149 149 149 152 155 159 162 162 162 164 164 165 166 166 174 ul CONTENTS General Introduction xxi Part I Semiconductor Fundamentals Chapter 1 Sensicundssrtors: A General introduction 1.1 General Material l’roperties 1.1.1 Composition 1.1.2 Parity 1.1.3 Strttcture 3 3 5 6 1.2 Crystal Structure 1.2.1 TIte Uttit Cell Cotteept 1.2.2 Sinspte 3-D Unit Cells 1.2.3 Semicandt,ctor Lattices 1.2.4 Miller Indices 7 8 9 12 1.3 Crystal Growth 1.3.1 Gbtaiaiug Ultrapare Si 1.3.2 Siagle-Crystal Parmation 16 17 6 16 .4 Santmary 19 Problems 19 Chapter 2 Carrier Modeling 23 2.1 The Qnautizasion Concept 23 2.2 Semiconductor Models 2.2.1 Eooding Model 2.2.2 Energy Eansi Model 2.2.3 Carriers 2.2.4 Band Gap atsd Material Ctassifiratioa 2.3 Carrier Properties 26 26 29 31 25 32 32 32 34 2.3.1 Charge 2.3.2 Effective Mass 2.3.3 Carrier Nambers in Intrinsic Material www.EasyEngineering.net a neutcoNunceon DEVtCE ruouuMuNTALn CONTENTS 2.3.4 Mattipalatiats af Carrier Nambers—Daping 2.3.5 Carrier-Related Termiavlagy 35 40 2.4 State and Carrier Distributiass 2.4.1 Detttity af States 2.4.2 The Perttti Psmctioa 2.4.3 Equilibriuits Distribution of Carriers 40 41 42 46 2.5 Eqailibriate Carrier Concentrations 2.5.1 Pormelas for a aed ta 2.5.2 Altureative Eepressiees fare and p 2.5.3 a aed the tsp Pradact 2.5.4 Charge Neutrality Relationship 2.5.5 Cttrrier Concentration Calcalatians 2.5.6 Determitsation of Er 2.5.7 Carrier Concentration Temperature Dependence 49 49 52 53 57 59 61 65 ww w .Ea syE 2.6 Summary end Concluding Comments Problems Chapter 3 Carrier Action ngi 3.1 Drift 3.1.1 3.1.2 3.1.3 3.1.4 3.1.5 Deheition—Visnaliaation DriE Carrent Mobility Resistivity Band Bendiag 67 69 75 nee rin g 3.2 Diffusion 3.2.! Dehnitioa —Visoalization 3.2.2 Hot-Poitst Probe Measurement 3.2.3 Diffasion and Total CnrrcoLs Diffasion Carrent.s Total Cnrrettts 3.2.4 Relatitsg Diffasion Coeffirients/Mobilisies Cottstancy of the Fermi Level Ctsrreut Plow Under Eqailibriam Conditions Einstein Relationship 3.3 Recombinatims—Generation 3.3.1 Debnitiost—Visnatieation Band-to-Baad Recombinatiaa 75 75 76 79 85 89 .ne t 94 94 97 98 98 99 99 99 tot lot 105 105 105 www.EasyEngineering.net R—f5 Center Recombitaation Aager Recombination Generation Processes 3.3.2 Mamensam Considerations 3.3.3 R—G Statistics Photogeneration Indirect Thermal Recombination—Generation 3.3.4 Minority Carrier Lifetimes General Information A Lifetime Measurement 3.4 Equations of Slate 3.4.1 Conlinuity Equations 3.4.2 Minority Carrier Diffusion Equations 3.4.3 Simptifications and Solations 3.4.4 Problem Solving Sample Problem No. I Sample Problem Na. 2 3.5 Supplemental Concepts 3.5.1 Diffusion Lengths 3.5.2 Quasi-Permi Levels 105 107 107 107 Ito to 112 116 116 116 t20 121 122 124 124 124 128 131 13 t 132 3.6 Summary and Concluding Comtoents 136 Problems 138 Chapter 4 Rasicn of Device Fabrication 4.1 Pabrication Processea 4.1.1 4.1.2 4.1.3 4.1.4 4.1.5 Gsidatian Diffusion lao Inaplantalian Lithography Thin-Filrtr Deposition Evstporation Spattering Chemical Vapor Deposition (CVD) 4.1.6 Epitasy 4.2 Device Fabrication Examples 4.2.1 pa Junction Diode Fabrication 4.2.2 Computer CPU Process Plow 4.3 Sammary 149 149 149 152 155 159 162 162 162 164 164 165 166 166 174 ul CONTENTS General Introduction xxi Part I Semiconductor Fundamentals Chapter 1 Sensicundssrtors: A General introduction 1.1 General Material l’roperties 1.1.1 Composition 1.1.2 Parity 1.1.3 Strttcture 3 3 5 6 1.2 Crystal Structure 1.2.1 TIte Uttit Cell Cotteept 1.2.2 Sinspte 3-D Unit Cells 1.2.3 Semicandt,ctor Lattices 1.2.4 Miller Indices 7 8 9 12 1.3 Crystal Growth 1.3.1 Gbtaiaiug Ultrapare Si 1.3.2 Siagle-Crystal Parmation 16 17 6 16 .4 Santmary 19 Problems 19 Chapter 2 Carrier Modeling 23 2.1 The Qnautizasion Concept 23 2.2 Semiconductor Models 2.2.1 Eooding Model 2.2.2 Energy Eansi Model 2.2.3 Carriers 2.2.4 Band Gap atsd Material Ctassifiratioa 2.3 Carrier Properties 26 26 29 31 25 32 32 32 34 2.3.1 Charge 2.3.2 Effective Mass 2.3.3 Carrier Nambers in Intrinsic Material www.EasyEngineering.net a neutcoNunceon DEVtCE ruouuMuNTALn 2.3.4 Mattipalatiats af Carrier Nambers—Daping 2.3.5 Carrier-Related Termiavlagy CONTENTS 35 40 2.4 State and Carrier Distributiass 2.4.1 Detttity af States 2.4.2 The Perttti Psmctioa 2.4.3 Equilibriuits Distribution of Carriers 40 41 42 46 2.5 Eqailibriate Carrier Concentrations 2.5.1 Pormelas for a aed ta 2.5.2 Altureative Eepressiees fare and p 2.5.3 a aed the tsp Pradact 2.5.4 Charge Neutrality Relationship 2.5.5 Cttrrier Concentration Calcalatians 2.5.6 Determitsation of Er 2.5.7 Carrier Concentration Temperature Dependence 49 49 52 53 57 59 61 65 2.6 Summary end Concluding Comments 67 Problems 69 Chapter 3 Carrier Action 3.1 Drift 3.1.1 3.1.2 3.1.3 3.1.4 3.1.5 75 75 Deheition—Visnaliaation DriE Carrent Mobility Resistivity Band Bendiag 3.2 Diffusion 3.2.! Dehnitioa —Visoalization 3.2.2 Hot-Poitst Probe Measurement 3.2.3 Diffasion and Total CnrrcoLs Diffasion Carrent.s Total Cnrrettts 3.2.4 Relatitsg Diffasion Coeffirients/Mobilisies Cottstancy of the Fermi Level Ctsrreut Plow Under Eqailibriam Conditions Einstein Relationship 3.3 Recombinatims—Generation 3.3.1 Debnitiost—Visnatieation Band-to-Baad Recombinatiaa 75 76 79 85 89 94 94 97 98 98 99 99 99 tot lot 105 105 105 R—f5 Center Recombitaation Aager Recombination 105 107 107 107 Ito Generation Processes 3.3.2 Mamensam Considerations 3.3.3 R—G Statistics to Photogeneration Indirect Thermal Recombination—Generation 3.3.4 Minority Carrier Lifetimes General Information A Lifetime Measurement ww w.E 112 116 116 116 3.4 Equations of Slate 3.4.1 Conlinuity Equations 3.4.2 Minority Carrier Diffusion Equations 3.4.3 Simptifications and Solations 3.4.4 Problem Solving Sample Problem No. I Sample Problem Na. 2 3.5 Supplemental Concepts asy En 3.5.1 Diffusion Lengths 3.5.2 Quasi-Permi Levels gin 3.6 Summary and Concluding Comtoents Problems Chapter 4 Rasicn of Device Fabrication Gsidatian Diffusion lao Inaplantalian Lithography Thin-Filrtr Deposition Evstporation Spattering Chemical Vapor Deposition (CVD) 4.1.6 Epitasy 4.2 Device Fabrication Examples 4.2.1 pa Junction Diode Fabrication 4.2.2 Computer CPU Process Plow 4.3 Sammary t20 121 122 124 124 124 128 131 13 t 132 eer 4.1 Pabrication Processea 4.1.1 4.1.2 4.1.3 4.1.4 4.1.5 ul ing 136 138 .ne 149 149 149 152 155 159 162 162 162 164 164 165 166 166 174 www.EasyEngineering.net t www.EasyEngineering.net aeMicoNuncron DEOICE FusuaMENruLu nit 75 AlteruativelSnplttementol Reading List 175 Figure SoarcesiCited References 177 Review List of Tenets 170 Part I—Review Probleitt Sets uitd Answers 195 5.1 Prelimieuries t9S 5.1.1 Jeoction Tertninology/ltlealized Profiles 5.1.2 Peissmt’s Equation 5.1.3 Qualitative Soletion 5.1.4 The Built-ic Potential (V j) 5 5.1.5 The Depletion Approximation w.E 6.1 4 Evaivinution of Results Ideal I—V 249 240 249 Tite Sattiratinit Current 250 Carrier Currents 254 as y En gin e 5.2.2 Step Junction with V Soludou forp Solutioe forT = Sotetioo for V Sulutiou for .e tied 5.2.3 Step Jnurtioe with V sO 5.2.4 Evaiuiuatioe/Evtropolatiun of Results 5.2.5 Linearly Graded Juucitoux 5.3 Sunsorary 195 Avuluoching 264 Zener Process 260 6.2.3 The R—G Current 6.2.4 V V High-Current Pltottomeua Series Resistance ng. ne 284 286 213 6.4 Suusutary and Concluding Cousuteats 288 2t5 Probtemv 289 2t9 223 226 227 t -‘ ,., Chapter 7 pet junction Diode: Small-Signal Admittance 301 7.1 Iutrodoetiou 301 7.2 Reverse-Bias Junetiou Capaci:aece 301 7.2.1 General Informutious 7.2.2 C—V Relationships 7.2.3 Parameter Extraction/Profiling 7.2.4 Reverse-Bias Couduetoorn 235 235 6.t.t Qualitative Derivation 0.1.2 Quantitative Solution Strategy 282 294 Current Derivatioe t.imitieg Cuses/Pueeh-Throtugh 210 212 0.1 Ttte Ideal Diode Equation 279 281 6.3.1 Charge Coatrol Approach 0.3.2 Narrow-Base Diode 210 I—V Characteristics 277 278 6.3 Specittl Cottsiderations 210 Ptoblenrs 270 High- Level Injection 209 209 eri 260 263 197 200 0 260 6.2.1 Ideal Theory Versus Esperiuueitt 6.2.2 Reverse-Him Bteakdowu 198 5.2.1 Assuutplious/Defiuitious 255 62 Drsiarious front the Ideal 203 5.2 Quantitative Electrostatic Relatioeslupv Chapter 6 po Junction Diode: 247 Carrier Coitreetrutious 193 ChapterS po Jonetion Electrostatics ww ‘‘Gaitte Plan’’ Suetitiary 0.1.3 Derivation Proper 179 Part hA pnJunction Diodes .1 aiti CONTENTS itt l’ttrl I Supplement antI Review 235 301 305 309 3t3 241 7.3 Forsvard-Bius Diffusion Admittanre 315 241 1 Geeeral Information 7.3 7.3.2 Admittance Relationships 316 Geeetul Cousiderutious Quasiueulral Region Coouiderutiouu 242 Depletion Regiun Cottsiderutious Boundary Conditions 244 243 315 7.4 Suatmuu’y 323 Ptoblems 324 www.EasyEngineering.net unnncOsnuctOs uuvtcn roauuaeNrutn is dunTeNru Chapter 8 pet Junction Diode: Transient Response 8.1 Turn-GE Transient 8.1. t Introduction 8.1.2 Qualitative Aoalysis 8.1.3 The Storage Deloy Tune Quantitative Analysts Measurement 8.1.4 General Information 327 329 333 333 334 338 8.2 Turn-Ga Transient 338 343 Problems 344 9.1 Introduction Baue Transport Furtor Coutmnu Ease d.c. Cuetent Guiu Common Emitter d.c. Current Gain 327 8.3 Summary Chapter 9 Optoelectronic Diodes .—‘ 327 10.6 Summary Problems Chapter 11 BJT Static Characteristics 11.1 Ideal Transistor Analysis lI.t.t Solution Strategy Basic Assumptions t 347 9.2.1 pu Junction Photodioden 9.2.2 p-i-n and Avalanche Photodiodes p-u-ri Photodrodes 9.3 Solar Cells ‘ 0 P n() in the Ease 356 . . 9.3.1 Solar Cell Bastes 556 9.3.2 Efficiency Consideratiotrs 9.3.3 Solar Cell Technology 300 9.4 LEDv 9.4.1 General Gvers’iew 9.4.2 Commercial LEGs 9.4.3 LED Packaging and Fhotou Enrraelioo Pail IIB BJTs and Other Junction Devices Chapter 10 EJT Eundnmentals 390 Performance Parameters/Terminoj Currents I 1.1.3 Simplified Reloliooships ( W 4 L ) 5 352 391 361 362 360 369 371 10.1 Tertoieology 371 10.2 Fabricatiour 374 10.3 Electrostatics 378 10.4 Introductory Gperalionul Consideralions 10.5 Ferformarree Parameters Emitter Effirinurey 380 382 382 389 389 390 392 383 393 Emitter/Colleetor Region Solutions Avalanche Phorodiodes 389 389 Notation Ease Region Solution 349 352 395 385 Diffusion Equations/Boundary Conditions Campatatioual Relationships 11.1.2 General Solution (W Arbitrary) 347 9.2 Photodindes 383 393 384 Performance Parameters 11.1.4 fihers—Moll Equations and Model 11.2 Deviations from the Ideal 11.2.1 Ideal Thrary/Esperimoul Comparison 11.2 2 Base Width Modulation 394 395 397 390 399 403 407 407 410 11.2.3 Ponob-Thrungb 412 1 1.2.4 Avalanche Multiplication and Breakdown Common Base Common Emitter 11.2.5 Geometrical Effects 414 414 414 420 Emirlrr Area S Colleetnr Area Senes Resistances 420 421 Current Ciowdiug — 11.2.6 Rerombirratiou—Genemoou Cnrreoi 11.2.7 Graded Ease 11.2.8 Figures of Merit 421 422 423 424 I 1.3 Modern BJT Stmerures 11.3.1 Folysiliron Enrittnr EJT 1 1.3.2 Hererojuncrian Bipolar Transistor IHBT) 426 429 420 an www.EasyEngineering.net aeMicoNuncron DEOICE FusuaMENruLu nit 75 AlteruativelSnplttementol Reading List 175 Figure SoarcesiCited References 177 Review List of Tenets 170 Part I—Review Probleitt Sets uitd Answers 195 5.1 Prelimieuries t9S 5.1.1 Jeoction Tertninology/ltlealized Profiles 5.1.2 Peissmt’s Equation 5.1.3 Qualitative Soletion 5.1.4 The Built-ic Potential (V j) 5 5.1.5 The Depletion Approximation 6.1 4 Evaivinution of Results Ideal I—V 249 240 249 Tite Sattiratinit Current 250 Carrier Currents 254 = ww 195 198 203 200 6.2.1 Ideal Theory Versus Esperiuueitt 6.2.2 Reverse-Him Bteakdowu 6.2.3 The R—G Current 6.2.4 V V High-Current Pltottomeua Series Resistance Ptoblenrs 227 294 nee r 6.4 Suusutary and Concluding Cousuteats -‘ 223 ,., Chapter 7 pet junction Diode: Small-Signal Admittance 7.1 Iutrodoetiou 7.2 Reverse-Bias Junetiou Capaci:aece 7.2.1 General Informutious 7.2.2 C—V Relationships 7.2.3 Parameter Extraction/Profiling 7.2.4 Reverse-Bias Couduetoorn 235 235 6.t.t Qualitative Derivation 0.1.2 Quantitative Solution Strategy 282 Probtemv 2t9 0.1 Ttte Ideal Diode Equation 279 281 213 226 277 278 syE ngi 2t5 5.3 Sunsorary 270 Current Derivatioe t.imitieg Cuses/Pueeh-Throtugh 210 I—V Characteristics 264 260 w.E a 212 Sulutiou for .e tied 5.2.3 Step Jnurtioe with V sO 5.2.4 Evaiuiuatioe/Evtropolatiun of Results 5.2.5 Linearly Graded Juucitoux Avuluoching Zener Process 6.3.1 Charge Coatrol Approach 0.3.2 Narrow-Base Diode 210 210 Sotetioo for V 260 263 6.3 Specittl Cottsiderations 209 0 260 High- Level Injection 209 5.2.1 Assuutplious/Defiuitious 255 62 Drsiarious front the Ideal 197 5.2 Quantitative Electrostatic Relatioeslupv Chapter 6 po Junction Diode: 247 Carrier Coitreetrutious 193 ChapterS po Jonetion Electrostatics 5.2.2 Step Junction with V Soludou forp Solutioe forT ‘‘Gaitte Plan’’ Suetitiary 0.1.3 Derivation Proper 179 Part hA pnJunction Diodes .1 aiti CONTENTS itt l’ttrl I Supplement antI Review 235 284 286 ing . 288 289 net 301 301 301 301 305 309 3t3 241 7.3 Forsvard-Bius Diffusion Admittanre 315 241 1 Geeeral Information 7.3 7.3.2 Admittance Relationships 316 Geeetul Cousiderutious Quasiueulral Region Coouiderutiouu 242 Depletion Regiun Cottsiderutious Boundary Conditions 244 243 315 7.4 Suatmuu’y 323 Ptoblems 324 www.EasyEngineering.net unnncOsnuctOs uuvtcn roauuaeNrutn is dunTeNru Chapter 8 pet Junction Diode: Transient Response 8.1 Turn-GE Transient 8.1. t Introduction 8.1.2 Qualitative Aoalysis 8.1.3 The Storage Deloy Tune Quantitative Analysts Measurement 8.1.4 General Information 327 329 333 333 334 338 8.2 Turn-Ga Transient 338 343 Problems 344 9.1 Introduction Baue Transport Furtor Coutmnu Ease d.c. Cuetent Guiu Common Emitter d.c. Current Gain 327 8.3 Summary Chapter 9 Optoelectronic Diodes .—‘ 327 10.6 Summary Problems Chapter 11 BJT Static Characteristics 11.1 Ideal Transistor Analysis lI.t.t Solution Strategy Basic Assumptions t 347 9.2.1 pu Junction Photodioden 9.2.2 p-i-n and Avalanche Photodiodes p-u-ri Photodrodes 9.3 Solar Cells ‘ 0 P n() in the Ease 356 . . 9.3.1 Solar Cell Bastes 556 9.3.2 Efficiency Consideratiotrs 9.3.3 Solar Cell Technology 300 9.4 LEDv 9.4.1 General Gvers’iew 9.4.2 Commercial LEGs 9.4.3 LED Packaging and Fhotou Enrraelioo Pail IIB BJTs and Other Junction Devices Chapter 10 EJT Eundnmentals 390 Performance Parameters/Terminoj Currents I 1.1.3 Simplified Reloliooships ( W 4 L ) 5 352 391 361 362 360 369 371 10.1 Tertoieology 371 10.2 Fabricatiour 374 10.3 Electrostatics 378 10.4 Introductory Gperalionul Consideralions 10.5 Ferformarree Parameters Emitter Effirinurey 380 382 382 389 389 390 392 383 393 Emitter/Colleetor Region Solutions Avalanche Phorodiodes 389 389 Notation Ease Region Solution 349 352 395 385 Diffusion Equations/Boundary Conditions Campatatioual Relationships 11.1.2 General Solution (W Arbitrary) 347 9.2 Photodindes 383 393 384 Performance Parameters 11.1.4 fihers—Moll Equations and Model 11.2 Deviations from the Ideal 11.2.1 Ideal Thrary/Esperimoul Comparison 11.2 2 Base Width Modulation 394 395 397 390 399 403 407 407 410 11.2.3 Ponob-Thrungb 412 1 1.2.4 Avalanche Multiplication and Breakdown Common Base Common Emitter 11.2.5 Geometrical Effects 414 414 414 420 Emirlrr Area S Colleetnr Area Senes Resistances 420 421 Current Ciowdiug — 11.2.6 Rerombirratiou—Genemoou Cnrreoi 11.2.7 Graded Ease 11.2.8 Figures of Merit 421 422 423 424 I 1.3 Modern BJT Stmerures 11.3.1 Folysiliron Enrittnr EJT 1 1.3.2 Hererojuncrian Bipolar Transistor IHBT) 426 429 420 an aeMicoNuncron DEOICE FusuaMENruLu nit 75 AlteruativelSnplttementol Reading List 175 Figure SoarcesiCited References 177 Review List of Tenets 170 Part I—Review Probleitt Sets uitd Answers 247 6.1 4 Evaivinution of Results Ideal I—V 249 240 249 Tite Sattiratinit Current 250 Carrier Currents 254 Carrier Coitreetrutious 193 ChapterS po Jonetion Electrostatics 195 5.1 Prelimieuries t9S 5.1.1 Jeoction Tertninology/ltlealized Profiles 5.1.2 Peissmt’s Equation 5.1.3 Qualitative Soletion 5.1.4 The Built-ic Potential (V j) 5 5.1.5 The Depletion Approximation 5.2.2 Step Junction with V Soludou forp Solutioe forT = 195 Avuluoching 264 Zener Process 260 6.2.3 The R—G Current 6.2.4 V V High-Current Pltottomeua Series Resistance 284 286 213 6.4 Suusutary and Concluding Cousuteats 288 2t5 Probtemv 289 2t9 -‘ 223 5.3 Sunsorary 226 Ptoblenrs 227 ,., Chapter 7 pet junction Diode: Small-Signal Admittance 301 7.1 Iutrodoetiou 301 7.2 Reverse-Bias Junetiou Capaci:aece 301 7.2.1 General Informutious 7.2.2 C—V Relationships 7.2.3 Parameter Extraction/Profiling 7.2.4 Reverse-Bias Couduetoorn 235 235 6.t.t Qualitative Derivation 0.1.2 Quantitative Solution Strategy 282 294 Current Derivatioe t.imitieg Cuses/Pueeh-Throtugh 210 212 0.1 Ttte Ideal Diode Equation 279 281 6.3.1 Charge Coatrol Approach 0.3.2 Narrow-Base Diode 210 I—V Characteristics 277 278 6.3 Specittl Cottsiderations 210 Sulutiou for .e tied 5.2.3 Step Jnurtioe with V sO 5.2.4 Evaiuiuatioe/Evtropolatiun of Results 5.2.5 Linearly Graded Juucitoux 270 High- Level Injection 209 209 Sotetioo for V 260 263 197 200 0 260 6.2.1 Ideal Theory Versus Esperiuueitt 6.2.2 Reverse-Him Bteakdowu 198 5.2.1 Assuutplious/Defiuitious 255 62 Drsiarious front the Ideal 203 5.2 Quantitative Electrostatic Relatioeslupv Chapter 6 po Junction Diode: ‘‘Gaitte Plan’’ Suetitiary 0.1.3 Derivation Proper 179 Part hA pnJunction Diodes .1 aiti CONTENTS itt l’ttrl I Supplement antI Review 235 301 305 309 3t3 241 7.3 Forsvard-Bius Diffusion Admittanre 315 241 1 Geeeral Information 7.3 7.3.2 Admittance Relationships 316 Geeetul Cousiderutious Quasiueulral Region Coouiderutiouu 242 Depletion Regiun Cottsiderutious Boundary Conditions 244 243 315 7.4 Suatmuu’y 323 Ptoblems 324 www.EasyEngineering.net unnncOsnuctOs uuvtcn roauuaeNrutn is dunTeNru Chapter 8 pet Junction Diode: Transient Response 8.1 Turn-GE Transient 8.1. t Introduction 8.1.2 Qualitative Aoalysis 8.1.3 The Storage Deloy Tune Quantitative Analysts Measurement 8.1.4 General Information 327 327 329 333 333 334 338 8.2 Turn-Ga Transient ww w 343 Problems 344 .Ea Chapter 11 BJT Static Characteristics 11.1 Ideal Transistor Analysis lI.t.t Solution Strategy Basic Assumptions t 347 9.1 Introduction 9.2 Photodindes 10.6 Summary Problems 338 8.3 Summary Chapter 9 Optoelectronic Diodes .—‘ Baue Transport Furtor Coutmnu Ease d.c. Cuetent Guiu Common Emitter d.c. Current Gain 327 syE p-u-ri Photodrodes ngi Avalanche Phorodiodes 9.3 Solar Cells 9.3.1 Solar Cell Bastes 9.3.2 Efficiency Consideratiotrs 9.3.3 Solar Cell Technology 9.4 LEDv 390 Performance Parameters/Terminoj Currents I 1.1.3 Simplified Reloliooships ( W 4 L ) 5 ‘ nee rin g 352 9.4.1 General Gvers’iew 9.4.2 Commercial LEGs 9.4.3 LED Packaging and Fhotou Enrraelioo Pail IIB BJTs and Other Junction Devices Chapter 10 EJT Eundnmentals 0 P n() in the Ease 356 . . 556 .ne t 300 391 361 362 360 369 371 10.1 Tertoieology 371 10.2 Fabricatiour 374 10.3 Electrostatics 378 10.4 Introductory Gperalionul Consideralions 10.5 Ferformarree Parameters Emitter Effirinurey 380 382 382 www.EasyEngineering.net 389 389 390 392 383 393 Ease Region Solution 349 352 389 389 Notation Emitter/Colleetor Region Solutions 9.2.1 pu Junction Photodioden 9.2.2 p-i-n and Avalanche Photodiodes 395 385 Diffusion Equations/Boundary Conditions Campatatioual Relationships 11.1.2 General Solution (W Arbitrary) 347 383 393 384 Performance Parameters 11.1.4 fihers—Moll Equations and Model 11.2 Deviations from the Ideal 11.2.1 Ideal Thrary/Esperimoul Comparison 11.2 2 Base Width Modulation 394 395 397 390 399 403 407 407 410 11.2.3 Ponob-Thrungb 412 1 1.2.4 Avalanche Multiplication and Breakdown Common Base Common Emitter 11.2.5 Geometrical Effects 414 414 414 420 Emirlrr Area S Colleetnr Area Senes Resistances 420 421 Current Ciowdiug — 11.2.6 Rerombirratiou—Genemoou Cnrreoi 11.2.7 Graded Ease 11.2.8 Figures of Merit 421 422 423 424 I 1.3 Modern BJT Stmerures 11.3.1 Folysiliron Enrittnr EJT 1 1.3.2 Hererojuncrian Bipolar Transistor IHBT) 426 429 420 an aeMicoNuncron DEOICE FusuaMENruLu nit 75 AlteruativelSnplttementol Reading List 175 Figure SoarcesiCited References 177 Review List of Tenets 170 Part I—Review Probleitt Sets uitd Answers 195 5.1 Prelimieuries t9S 5.1.1 Jeoction Tertninology/ltlealized Profiles 5.1.2 Peissmt’s Equation 5.1.3 Qualitative Soletion 5.1.4 The Built-ic Potential (V j) 5 5.1.5 The Depletion Approximation 6.1 4 Evaivinution of Results Ideal I—V 249 240 249 Tite Sattiratinit Current 250 Carrier Currents 254 = 195 Avuluoching 264 Zener Process 260 6.2.3 The R—G Current 6.2.4 V V High-Current Pltottomeua Series Resistance 284 286 213 6.4 Suusutary and Concluding Cousuteats 288 2t5 Probtemv 289 2t9 -‘ 223 5.3 Sunsorary 226 Ptoblenrs 227 ,., Chapter 7 pet junction Diode: Small-Signal Admittance 301 7.1 Iutrodoetiou 301 7.2 Reverse-Bias Junetiou Capaci:aece 301 7.2.1 General Informutious 7.2.2 C—V Relationships 7.2.3 Parameter Extraction/Profiling 7.2.4 Reverse-Bias Couduetoorn 235 235 6.t.t Qualitative Derivation 0.1.2 Quantitative Solution Strategy 282 294 Current Derivatioe t.imitieg Cuses/Pueeh-Throtugh 210 212 0.1 Ttte Ideal Diode Equation 279 281 6.3.1 Charge Coatrol Approach 0.3.2 Narrow-Base Diode 210 I—V Characteristics 277 278 6.3 Specittl Cottsiderations 210 Sulutiou for .e tied 5.2.3 Step Jnurtioe with V sO 5.2.4 Evaiuiuatioe/Evtropolatiun of Results 5.2.5 Linearly Graded Juucitoux 270 High- Level Injection 209 209 Sotetioo for V 260 263 197 200 0 260 6.2.1 Ideal Theory Versus Esperiuueitt 6.2.2 Reverse-Him Bteakdowu 198 5.2.1 Assuutplious/Defiuitious 255 62 Drsiarious front the Ideal 203 5.2 Quantitative Electrostatic Relatioeslupv Chapter 6 po Junction Diode: 247 Carrier Coitreetrutious 193 ChapterS po Jonetion Electrostatics 5.2.2 Step Junction with V Soludou forp Solutioe forT ‘‘Gaitte Plan’’ Suetitiary 0.1.3 Derivation Proper 179 Part hA pnJunction Diodes .1 aiti CONTENTS itt l’ttrl I Supplement antI Review 235 301 305 309 3t3 241 7.3 Forsvard-Bius Diffusion Admittanre 315 241 1 Geeeral Information 7.3 7.3.2 Admittance Relationships 316 Geeetul Cousiderutious Quasiueulral Region Coouiderutiouu 242 Depletion Regiun Cottsiderutious Boundary Conditions 244 243 315 7.4 Suatmuu’y 323 Ptoblems 324 www.EasyEngineering.net unnncOsnuctOs uuvtcn roauuaeNrutn is dunTeNru Chapter 8 pet Junction Diode: Transient Response 8.1 Turn-GE Transient 8.1. t Introduction 8.1.2 Qualitative Aoalysis 8.1.3 The Storage Deloy Tune Quantitative Analysts Measurement 8.1.4 General Information 327 329 333 333 334 338 8.2 Turn-Ga Transient 338 343 Problems 344 9.1 Introduction Baue Transport Furtor Coutmnu Ease d.c. Cuetent Guiu Common Emitter d.c. Current Gain 327 8.3 Summary Chapter 9 Optoelectronic Diodes .—‘ 327 p-u-ri Photodrodes ww w.E 347 349 352 390 390 392 383 393 asy Emitter/Colleetor Region Solutions Ease Region Solution 394 gin 395 397 0 P n() in the Ease 356 9.3.2 Efficiency Consideratiotrs 9.3.3 Solar Cell Technology 300 Pail IIB BJTs and Other Junction Devices Notation Diffusion Equations/Boundary Conditions Campatatioual Relationships En ‘ . . Chapter 10 EJT Eundnmentals 389 389 Performance Parameters/Terminoj Currents I 1.1.3 Simplified Reloliooships ( W 4 L ) 5 352 556 9.4.1 General Gvers’iew 9.4.2 Commercial LEGs 9.4.3 LED Packaging and Fhotou Enrraelioo 389 11.1.2 General Solution (W Arbitrary) 347 9.3.1 Solar Cell Bastes 9.4 LEDv 389 11.1 Ideal Transistor Analysis lI.t.t Solution Strategy Basic Assumptions Avalanche Phorodiodes 9.3 Solar Cells 395 385 Chapter 11 BJT Static Characteristics 9.2 Photodindes 9.2.1 pu Junction Photodioden 9.2.2 p-i-n and Avalanche Photodiodes 383 393 384 10.6 Summary Problems t 391 361 362 360 369 371 10.1 Tertoieology 371 10.2 Fabricatiour 374 10.3 Electrostatics 378 10.4 Introductory Gperalionul Consideralions 10.5 Ferformarree Parameters Emitter Effirinurey 380 382 382 an 390 Performance Parameters 11.1.4 fihers—Moll Equations and Model 11.2 Deviations from the Ideal eer 11.2.1 Ideal Thrary/Esperimoul Comparison 11.2 2 Base Width Modulation 11.2.3 Ponob-Thrungb 1 1.2.4 Avalanche Multiplication and Breakdown Common Base Common Emitter 11.2.5 Geometrical Effects Emirlrr Area S Colleetnr Area Senes Resistances 399 403 ing 407 407 410 .ne 412 414 414 414 420 420 421 Current Ciowdiug — 11.2.6 Rerombirratiou—Genemoou Cnrreoi 11.2.7 Graded Ease 11.2.8 Figures of Merit 421 422 423 424 I 1.3 Modern BJT Stmerures 11.3.1 Folysiliron Enrittnr EJT 1 1.3.2 Hererojuncrian Bipolar Transistor IHBT) 426 429 420 www.EasyEngineering.net t www.EasyEngineering.net ntwcoNnacenrt anmen FaN050nreraLs ii eoNvcNTn 11.4 Summary 432 14.2.4 Teaevieot Reapoitse 496 Problems 433 14.3 Practical Contact Convideeatinav 497 497 498 Chapter 12 BJT Dynamic Response Modeling 12.1 SmalI-Siguat Equivalent Circuits 452 Figure Sources/Cited References 454 454 Reciem List of Terms 507 Part It—Review Problem Sets and Answers 508 456 as y En gin e 463 13.2 SCR Opeeatiottal Theory 465 13.3.2 Additional Triggering Meeltanisios 13.3.3 Shorted-Cathode Configuration eri 13.3.4 di/dt and dn/dt Effects 13.3.5 TeiggeriitgTiine 13.3.6 Switchieg Adsantages/Disadvantages 15.1 Oenenil Introduction 525 530 152.1 Inteodoctian 530 531 536 547 15,2.2 Qualitative Theory of Opeeatinn 15.2.3 Qnaotoative ‘nt’o Relationships ng. ne -470 15.2.4 ac. Response 471 15.3 MESPET 471 473 473 523 525 t5.2 2-PET 470 472 505 506 Chapter IS Field Effect Introdnetion—TIie J-FET and MESFET 459 463 505 List Part Ill Field Effect Devices 458 13.1 Silicoo Controlled Rectifier ISCRI 13.3.1 Circuit Opetation / Altceuative/Sapplemental Reading 457 Chapter 13 PNPN Devices Chapter 14 R2 Part II Sopptement and Review 449 Tore—off Tratisietti 12.2.4 Practical Considerations 12.3 Seminary 501 449 12.2.3 Quantitative Analysis Tore-os Transient w.E 500 Peobleitts 446 12.2.1 Qualitative Ohsersatious 12.2.2 Charge Coutrol Relatiouships 13.3 Practical Tsen-onlTurn-off Considerations 4.4 Ssntmary 443 12.2 Transient ISmitchingi Rcspoase Peob Ic mu Rectifyittg Conlacts 4.3.2 Ohittic Contacts 443 12.1.1 Geocotl iced Two-Port Model 12.1.2 Hybuid-Pi Models ww 14.3.1 443 153.1 Oeneral Information 15.3.2 Sheet-Channel Consiàerations t Variahle Mobility Model Saturated Velocity Model 550 550 552 553 554 355 13.4 Other PNPN Devices 474 MS 477 15.4 Snesmary 14.1 Ideal MS Contacts 477 Problems 557 14.2 Scltotthy Diode 463 Chapter t6 MOS Pondamentals 563 Contacts and Sehottky Diodes 14.2.1 Electrostatics Two-Region Model 483 Bnilt-in Voltage 483 p. ‘3, V 485 Depletion Width 14.2.2 I—V Characteristics 14.2.3 ac. Response 16.1 Ideal Strnctare Definition 16.2 Rteetrostatics—Mostly Qualitative 16.2.1 Vivualteation Aids 486 Energy Band Diagram 487 Bloch Charge Diagrams 493 ash 557 563 565 565 565 566 www.EasyEngineering.net ‘iii neoteoNnueTnn nestcn rucsnAomceus 6.2.2 Effect of an Applied Bias General Obseevatious Specihc Diosing Regions 16.3 Electrnstaticn—Quantitative Pnrmalotion 16.3.1 Semiconductor Eleetroslatics Peeparatnry Considerations Delta-Depletion Selatins 16.3.2 Gate Voltage Relationship 1 b.4 Capacitance—Voltage Characteristics 16.4.1 Theory aod Analysis Qualitative Theory Delta-Depletion Atialysis 16.4.2 Computations and Dbueevatiuus Exact Cnmputotions Practical Observations eoreenecen 567 Sb? 568 18.2.1 General Information 18.2.2 Mobile tans 571 571 571 578 580 18.2.3 The Pined Charge 18.2.4 lsleefaeial Traps 18.2.5 Induced Charges Radietioe Effects Negative-Bias Instability 18.2.6 At-’ 0 Sommaey 584 584 584 590 591 591 595 16.5 Summary and Concluding Comments 599 Problems dOO Chapter 17 MOSFETs—TIte Easeoldols 182 Daide Charges flIt 18.3 MOSFET Tlmeeshold Considerations 183.1 Vv Relationships 18.3.2 Theeshold, Ternsisnlagy. and Technology 18.3.3 Thresltold Adjustment I 8.3.4 Back Biasing 8.3.5 Threshold Sammary Problems 691 691 694 694 897 898 700 700 700 fill 19.1.1 Introduction 617 19.1.2 Threshold Voltage Modification Effective Mobility 17.2.2 Square-Law Theory 17.2.3 Bulk-Charge Thevry 17.2.4 Charge-Sheet and ffveet-Chaeee Theories 17.3 ac. Response 17.3.1 Snialt-Sigeal EqnivaleutCircnitv 17.3.2 Cutoff Frequency 17.3.3 Small-Signet Characteristics 17.4 Summary 637 Problems 638 Chapter 88 Nonideal MOS 18.1 Metal—Semieondtietoe Woekl’enetiun Difference Short Clmannel Narrow Width — 19.1.3 Parasitic BJT Actinim I9.l.4 Hot-Caeeierffffeetv Oxide Churging Velocity Satneatien Velocity OvershootiBattistie Tcanspoct 830 630 633 834 645 645 89 I 19.1 Small Dimension Effects 17.1 Qualitative Theory of Opeeatiun 617 617 6t8 620 625 628 874 675 678 678 880 881 884 Chapter 19 Modern FET Stroctures 17.2 Qnautilative a ’a Relationships 1 17.2. t Prelitsinaey Considerations Threshold Voltage 850 850 853 658 882 668 668 689 870 19.2 Select Slrtictoec Survey 19.2.1 MOSFET Structures LDD Transistors DMOS Buried-Chauttel MOSPET SiGe Devices SOl Strnetums 19.2.2 MOOPET (HEMT) Peabteten 7111 702 702 702 703 704 704 705 707 710 am www.EasyEngineering.net ntwcoNnacenrt anmen FaN050nreraLs ii 11.4 Summary 432 14.2.4 Teaevieot Reapoitse 496 Problems 433 14.3 Practical Contact Convideeatinav 497 497 498 Chapter 12 BJT Dynamic Response Modeling 12.1 SmalI-Siguat Equivalent Circuits 12.1.1 Geocotl iced Two-Port Model 12.1.2 Hybuid-Pi Models 12.2 Transient ISmitchingi Rcspoase 4.4 Ssntmary 501 449 R2 Part II Sopptement and Review 449 Altceuative/Sapplemental Reading Tore—off Tratisietti 12.2.4 Practical Considerations 457 456 458 459 ww 13.1 Silicoo Controlled Rectifier ISCRI 463 13.2 SCR Opeeatiottal Theory 465 13.3 Practical Tsen-onlTurn-off Considerations 470 13.3.1 Circuit Opetation -470 13.3.2 Additional Triggering Meeltanisios 13.3.3 Shorted-Cathode Configuration 471 13.3.4 di/dt and dn/dt Effects 13.3.5 TeiggeriitgTiine 472 505 List 505 Figure Sources/Cited References 506 Reciem List of Terms w.E a 507 508 Part It—Review Problem Sets and Answers Part Ill Field Effect Devices 523 syE ngi Chapter IS Field Effect Introdnetion—TIie J-FET and MESFET 463 525 15.1 Oenenil Introduction 525 t5.2 2-PET 530 nee r 152.1 Inteodoctian 15,2.2 Qualitative Theory of Opeeatinn 15.2.3 Qnaotoative ‘nt’o Relationships 15.2.4 ac. Response 15.3 MESPET 471 153.1 Oeneral Information 15.3.2 Sheet-Channel Consiàerations 473 473 Variahle Mobility Model Saturated Velocity Model ing . 530 531 536 547 550 net 550 552 553 554 355 13.4 Other PNPN Devices 474 MS 477 15.4 Snesmary 14.1 Ideal MS Contacts 477 Problems 557 14.2 Scltotthy Diode 463 Chapter t6 MOS Pondamentals 563 Contacts and Sehottky Diodes 14.2.1 Electrostatics 483 p. ‘3, V 485 Depletion Width 14.2.2 I—V Characteristics 14.2.3 ac. Response Two-Region Model 483 Bnilt-in Voltage 16.1 557 Ideal Strnctare Definition 16.2 Rteetrostatics—Mostly Qualitative 16.2.1 Vivualteation Aids 486 Energy Band Diagram 487 Bloch Charge Diagrams 493 ash 500 Peobleitts 446 454 454 13.3.6 Switchieg Adsantages/Disadvantages / 443 452 Chapter 13 PNPN Devices Rectifyittg Conlacts 4.3.2 Ohittic Contacts 443 12.2.3 Quantitative Analysis Tore-os Transient Peob Ic mu 14.3.1 443 12.2.1 Qualitative Ohsersatious 12.2.2 Charge Coutrol Relatiouships 12.3 Seminary Chapter 14 eoNvcNTn 563 565 565 565 566 www.EasyEngineering.net ‘iii neoteoNnueTnn nestcn rucsnAomceus 6.2.2 Effect of an Applied Bias General Obseevatious Specihc Diosing Regions 16.3 Electrnstaticn—Quantitative Pnrmalotion 16.3.1 Semiconductor Eleetroslatics Peeparatnry Considerations Delta-Depletion Selatins 16.3.2 Gate Voltage Relationship 1 b.4 Capacitance—Voltage Characteristics 16.4.1 Theory aod Analysis Qualitative Theory Delta-Depletion Atialysis 16.4.2 Computations and Dbueevatiuus Exact Cnmputotions Practical Observations eoreenecen 567 Sb? 568 18.2.1 General Information 18.2.2 Mobile tans 571 571 571 578 580 18.2.3 The Pined Charge 18.2.4 lsleefaeial Traps 18.2.5 Induced Charges Radietioe Effects Negative-Bias Instability 18.2.6 At-’ 0 Sommaey 584 584 584 590 591 591 595 16.5 Summary and Concluding Comments 599 Problems dOO Chapter 17 MOSFETs—TIte Easeoldols 182 Daide Charges flIt 18.3 MOSFET Tlmeeshold Considerations 183.1 Vv Relationships 18.3.2 Theeshold, Ternsisnlagy. and Technology 18.3.3 Thresltold Adjustment I 8.3.4 Back Biasing 8.3.5 Threshold Sammary Problems 691 691 694 694 897 898 700 700 700 fill 19.1.1 Introduction 617 19.1.2 Threshold Voltage Modification Effective Mobility 17.2.2 Square-Law Theory 17.2.3 Bulk-Charge Thevry 17.2.4 Charge-Sheet and ffveet-Chaeee Theories 17.3 ac. Response 17.3.1 Snialt-Sigeal EqnivaleutCircnitv 17.3.2 Cutoff Frequency 17.3.3 Small-Signet Characteristics 17.4 Summary 637 Problems 638 Chapter 88 Nonideal MOS 18.1 Metal—Semieondtietoe Woekl’enetiun Difference Short Clmannel Narrow Width — 19.1.3 Parasitic BJT Actinim I9.l.4 Hot-Caeeierffffeetv Oxide Churging Velocity Satneatien Velocity OvershootiBattistie Tcanspoct 830 630 633 834 645 645 89 I 19.1 Small Dimension Effects 17.1 Qualitative Theory of Opeeatiun 617 617 6t8 620 625 628 874 675 678 678 880 881 884 Chapter 19 Modern FET Stroctures 17.2 Qnautilative a ’a Relationships 1 17.2. t Prelitsinaey Considerations Threshold Voltage 850 850 853 658 882 668 668 689 870 19.2 Select Slrtictoec Survey 19.2.1 MOSFET Structures LDD Transistors DMOS Buried-Chauttel MOSPET SiGe Devices SOl Strnetums 19.2.2 MOOPET (HEMT) Peabteten 7111 702 702 702 703 704 704 705 707 710 am ntwcoNnacenrt anmen FaN050nreraLs ii eoNvcNTn 11.4 Summary 432 14.2.4 Teaevieot Reapoitse 496 Problems 433 14.3 Practical Contact Convideeatinav 497 497 498 Chapter 12 BJT Dynamic Response Modeling 12.1 SmalI-Siguat Equivalent Circuits 4.4 Ssntmary 443 R2 Part II Sopptement and Review 449 Altceuative/Sapplemental Reading 452 Figure Sources/Cited References 454 454 Reciem List of Terms 507 Part It—Review Problem Sets and Answers 508 12.2.3 Quantitative Analysis Tore-os Transient Tore—off Tratisietti 12.2.4 Practical Considerations 457 456 12.3 Seminary 458 459 Chapter 13 PNPN Devices 463 13.2 SCR Opeeatiottal Theory 465 13.3 Practical Tsen-onlTurn-off Considerations 470 13.3.1 Circuit Opetation -470 13.3.2 Additional Triggering Meeltanisios 13.3.3 Shorted-Cathode Configuration 471 13.3.4 di/dt and dn/dt Effects 13.3.5 TeiggeriitgTiine 472 505 List 505 506 Part Ill Field Effect Devices 523 Chapter IS Field Effect Introdnetion—TIie J-FET and MESFET 463 13.1 Silicoo Controlled Rectifier ISCRI 525 15.1 Oenenil Introduction 525 t5.2 2-PET 530 152.1 Inteodoctian 530 531 536 547 15,2.2 Qualitative Theory of Opeeatinn 15.2.3 Qnaotoative ‘nt’o Relationships 15.2.4 ac. Response 15.3 MESPET 471 153.1 Oeneral Information 15.3.2 Sheet-Channel Consiàerations 473 473 13.3.6 Switchieg Adsantages/Disadvantages 501 449 12.2.1 Qualitative Ohsersatious 12.2.2 Charge Coutrol Relatiouships Peob Ic mu 500 Peobleitts 446 12.2 Transient ISmitchingi Rcspoase / Rectifyittg Conlacts 4.3.2 Ohittic Contacts 443 12.1.1 Geocotl iced Two-Port Model 12.1.2 Hybuid-Pi Models Chapter 14 14.3.1 443 Variahle Mobility Model Saturated Velocity Model 550 550 552 553 554 355 13.4 Other PNPN Devices 474 MS 477 15.4 Snesmary 14.1 Ideal MS Contacts 477 Problems 557 14.2 Scltotthy Diode 463 Chapter t6 MOS Pondamentals 563 Contacts and Sehottky Diodes 14.2.1 Electrostatics Two-Region Model 483 Bnilt-in Voltage 483 p. ‘3, V 485 Depletion Width 16.1 Ideal Strnctare Definition 16.2 Rteetrostatics—Mostly Qualitative 16.2.1 Vivualteation Aids 486 14.2.2 I—V Characteristics 14.2.3 ac. Response Energy Band Diagram 487 Bloch Charge Diagrams 493 ash 557 563 565 565 565 566 www.EasyEngineering.net ‘iii neoteoNnueTnn nestcn rucsnAomceus eoreenecen 6.2.2 Effect of an Applied Bias General Obseevatious 567 Sb? 568 Specihc Diosing Regions 16.3 Electrnstaticn—Quantitative Pnrmalotion Peeparatnry Considerations Delta-Depletion Selatins 16.3.2 Gate Voltage Relationship 1 b.4 Capacitance—Voltage Characteristics 16.4.1 Theory aod Analysis 16.4.2 Computations and Dbueevatiuus Exact Cnmputotions syE Practical Observations 16.5 Summary and Concluding Comments ngi Problems Chapter 17 MOSFETs—TIte Easeoldols 17.1 Qualitative Theory of Opeeatiun 17.2 Qnautilative a ’a Relationships 1 17.2. t Prelitsinaey Considerations Threshold Voltage Effective Mobility 17.2.2 Square-Law Theory 17.2.3 Bulk-Charge Thevry 18.2.3 The Pined Charge 18.2.4 lsleefaeial Traps 18.2.5 Induced Charges Radietioe Effects Negative-Bias Instability 18.2.6 At-’ 0 Sommaey 584 584 584 590 591 591 595 Qualitative Theory Delta-Depletion Atialysis .Ea 18.2.1 General Information 18.2.2 Mobile tans 571 571 571 578 580 16.3.1 Semiconductor Eleetroslatics ww w 182 Daide Charges 599 dOO nee rin g 17.2.4 Charge-Sheet and ffveet-Chaeee Theories 17.3 ac. Response flIt 18.3 MOSFET Tlmeeshold Considerations 183.1 Vv Relationships 18.3.2 Theeshold, Ternsisnlagy. and Technology 18.3.3 Thresltold Adjustment I 8.3.4 Back Biasing 8.3.5 Threshold Sammary Problems 17.3.3 Small-Signet Characteristics 691 fill 19.1.1 Introduction 617 19.1.2 Threshold Voltage Modification 691 694 694 897 898 700 700 700 617 617 6t8 620 625 628 .ne t 630 633 834 637 Problems 638 645 18.1 Metal—Semieondtietoe Woekl’enetiun Difference 89 I 19.1 Small Dimension Effects 17.4 Summary Chapter 88 Nonideal MOS 874 675 678 678 880 881 884 Chapter 19 Modern FET Stroctures Short Clmannel Narrow Width — 19.1.3 Parasitic BJT Actinim I9.l.4 Hot-Caeeierffffeetv Oxide Churging Velocity Satneatien Velocity OvershootiBattistie Tcanspoct 830 17.3.1 Snialt-Sigeal EqnivaleutCircnitv 17.3.2 Cutoff Frequency 850 850 853 658 882 668 668 689 870 645 19.2 Select Slrtictoec Survey 19.2.1 MOSFET Structures LDD Transistors DMOS Buried-Chauttel MOSPET SiGe Devices SOl Strnetums 19.2.2 MOOPET (HEMT) Peabteten www.EasyEngineering.net 7111 702 702 702 703 704 704 705 707 710 am ntwcoNnacenrt anmen FaN050nreraLs ii 11.4 Summary 432 14.2.4 Teaevieot Reapoitse 496 Problems 433 14.3 Practical Contact Convideeatinav 497 497 498 Chapter 12 BJT Dynamic Response Modeling 12.1 SmalI-Siguat Equivalent Circuits 12.1.1 Geocotl iced Two-Port Model 12.1.2 Hybuid-Pi Models 12.2 Transient ISmitchingi Rcspoase 4.4 Ssntmary 501 449 R2 Part II Sopptement and Review 449 Altceuative/Sapplemental Reading 452 Figure Sources/Cited References 454 454 Reciem List of Terms 507 Part It—Review Problem Sets and Answers 508 456 458 459 463 13.2 SCR Opeeatiottal Theory 465 13.3 Practical Tsen-onlTurn-off Considerations 470 13.3.1 Circuit Opetation -470 13.3.2 Additional Triggering Meeltanisios 13.3.3 Shorted-Cathode Configuration 471 13.3.4 di/dt and dn/dt Effects 13.3.5 TeiggeriitgTiine 472 505 List 505 506 Part Ill Field Effect Devices 523 Chapter IS Field Effect Introdnetion—TIie J-FET and MESFET 463 13.1 Silicoo Controlled Rectifier ISCRI 525 15.1 Oenenil Introduction 525 t5.2 2-PET 530 152.1 Inteodoctian 530 531 536 547 15,2.2 Qualitative Theory of Opeeatinn 15.2.3 Qnaotoative ‘nt’o Relationships 15.2.4 ac. Response 15.3 MESPET 471 550 153.1 Oeneral Information 15.3.2 Sheet-Channel Consiàerations 473 473 550 552 553 554 355 Variahle Mobility Model Saturated Velocity Model 13.4 Other PNPN Devices 474 MS 477 15.4 Snesmary 14.1 Ideal MS Contacts 477 Problems 557 14.2 Scltotthy Diode 463 Chapter t6 MOS Pondamentals 563 Contacts and Sehottky Diodes 14.2.1 Electrostatics 483 p. ‘3, V 485 Depletion Width 14.2.2 I—V Characteristics 14.2.3 ac. Response Two-Region Model 483 Bnilt-in Voltage 16.1 557 Ideal Strnctare Definition 563 16.2 Rteetrostatics—Mostly Qualitative 565 565 565 566 16.2.1 Vivualteation Aids 486 Energy Band Diagram 487 Bloch Charge Diagrams 493 ash 500 Peobleitts 446 457 13.3.6 Switchieg Adsantages/Disadvantages / 443 Tore—off Tratisietti 12.2.4 Practical Considerations Chapter 13 PNPN Devices Rectifyittg Conlacts 4.3.2 Ohittic Contacts 443 12.2.3 Quantitative Analysis Tore-os Transient 12.3 Seminary 14.3.1 443 12.2.1 Qualitative Ohsersatious 12.2.2 Charge Coutrol Relatiouships Peob Ic mu Chapter 14 eoNvcNTn www.EasyEngineering.net ‘iii neoteoNnueTnn nestcn rucsnAomceus 6.2.2 Effect of an Applied Bias General Obseevatious Specihc Diosing Regions 16.3 Electrnstaticn—Quantitative Pnrmalotion 16.3.1 Semiconductor Eleetroslatics Peeparatnry Considerations Delta-Depletion Selatins 16.3.2 Gate Voltage Relationship 1 b.4 Capacitance—Voltage Characteristics 16.4.1 Theory aod Analysis eoreenecen 567 Sb? 568 182 Daide Charges 584 18.2.5 Induced Charges Radietioe Effects Negative-Bias Instability 18.2.6 At-’ 0 Sommaey 16.5 Summary and Concluding Comments ww w.E 599 Problems Problems dOO 16.4.2 Computations and Dbueevatiuus Exact Cnmputotions Practical Observations Chapter 17 MOSFETs—TIte Easeoldols flIt 850 853 658 882 668 668 689 870 18.2.3 The Pined Charge 18.2.4 lsleefaeial Traps 584 584 590 591 591 595 Qualitative Theory Delta-Depletion Atialysis 850 18.2.1 General Information 18.2.2 Mobile tans 571 571 571 578 580 18.3 MOSFET Tlmeeshold Considerations Vv Relationships 18.3.2 Theeshold, Ternsisnlagy. and Technology 18.3.3 Thresltold Adjustment I 8.3.4 Back Biasing 8.3.5 Threshold Sammary asy En Chapter 19 Modern FET Stroctures 19.1 Small Dimension Effects 884 89 I gin 691 17.1 Qualitative Theory of Opeeatiun fill 19.1.1 Introduction 617 19.1.2 Threshold Voltage Modification Effective Mobility 17.2.2 Square-Law Theory 17.2.3 Bulk-Charge Thevry 17.2.4 Charge-Sheet and ffveet-Chaeee Theories 17.3 ac. Response 17.3.1 Snialt-Sigeal EqnivaleutCircnitv 17.3.2 Cutoff Frequency 17.3.3 Small-Signet Characteristics 617 617 6t8 620 625 628 17.4 Summary 637 Problems 638 Chapter 88 Nonideal MOS 18.1 Metal—Semieondtietoe Woekl’enetiun Difference Short Clmannel Narrow Width — 19.1.3 Parasitic BJT Actinim I9.l.4 Hot-Caeeierffffeetv Oxide Churging Velocity Satneatien 645 645 eer Velocity OvershootiBattistie Tcanspoct 830 630 633 834 874 675 678 678 880 881 183.1 17.2 Qnautilative a ’a Relationships 1 17.2. t Prelitsinaey Considerations Threshold Voltage 19.2 Select Slrtictoec Survey ing 691 694 694 897 898 700 700 700 .ne 7111 702 19.2.1 MOSFET Structures LDD Transistors DMOS Buried-Chauttel MOSPET SiGe Devices SOl Strnetums 19.2.2 MOOPET (HEMT) Peabteten am 702 702 703 704 704 705 707 710 www.EasyEngineering.net t www.EasyEngineering.net us srMicONDncTeR nuotcu FuNuaMuNTacs R3 Purl Ill 1 Snp d cunenh antI Review 713 Alicrtmafxe/Supltlettreitiul Reading List 713 Figute Sotirces/Ciled References Rcxiew List of ‘l’eetus 714 717 Ptnn Ibl—Reumrw Problem Sets and Answers 7lfl Appendices 733 Appenulix A Elements ww of Qnuntum Mechanics 733 A.t The Qtiattticatietn Coucepi A.l.t Blackbedy Radiation 733 733 w.E A.t.2 The BuhrAiein A. 1.3 Wave-Particle Duality 733 737 as y En gin e A 2 Basic Pettitalistis 739 A.3 Electronic States in Abuts A.3.l The Hydrogen Atom 741 741 A.3.2 Muhti-Ehectroit Abuts Appendix B 744 MOS Semicnnductor Electroutatieu—Exuct Solution eri Defittitien of Panaivesers Exact Solution Appendix C GENERAL INTRODUCTION MOS C—v Supplement Appendix D MOS 1—V Supplement 749 750 ng. ne 753 755 Appendix E List oh’ Symbols Appendix M MATLAB 749 757 Program Script 771 19.2 (BJT_Eband) Exescisc 11.7 (BITI and Exercise 11.10 lBlTplus) Exercise ib.5 (MDS_.CV( 77fl Index 791 Esessise 771 774 t Cotticident with the wtitittp of this book, there lint been considerable teedia disrnssion abate the “Information Superhighway.” The envisioned highway itself, the physical link beimeee points sultporting the infortvation traffic, is fiber optic cable. Relative to tlte topic of this book, the oit and elf camps, whielt insert aitd extract the information from the higlt way, are scoticooductor (solid state) devices. Traffic control, the information procesning and the cetixemion to and from the haitian interface, is performed by computers. The ccxteal priicessinp unit (CPU). meotory, and oilier major coeipoueets inside the computer are again seivicendoeierdexiees lv the moderit machI, semiconductor devices are incorporated iv just about every muior system from automobiles to washing machines. Alihonglt toughly a half-ceitiury old, the field of stndy associated with semicendactor devices eontinnes to be dyunnnc and exeitieg. New end improved devices are beiitg slevel 1 aped st an almost maddexiog pace. While die device count in complex iotegrated circuits increases through the millions and the side-length of chips is itseasured in centimeters, the individuel devices are literally beiog shrank to atonue dimensions. Moreover, semiconduc tar propertieu desired for a given device nirecmnre but net usuiluble in tulane me being pnednced urtilicially; in essence, the semiconductor properties themselves tire now being engivecred to fit device specifications. This bock should ne viewed as u gateway in what the reader svill hnpefully agree is the faseinatnig realm of semiconductor devices. Ii was suriutex for junioror senior-level sin deitis olin hxxe at least an inlredacuary eupesnne ia electric field theory. The coverage esclades a representative sampling of infornietion about a wide variety of devices. Priivery einphosis, however, is placed en developing a fundamental nitderstanding of the internal workings of the tenre basic device structures. Au detailed below, thin book contains a num ber of unique features to assist the render in learning the material. Alerted at an curly stage to their existence, the render can plan to take full advantage of the cited features. • Conipuier-Bexed Ererciaes and End-nf Clusprer (Henss’trei-k) Problems. The majarily of chapters contain one er core Mw’rrxn-bunrd exercises requiring the use of a com puter MATLAB in a ninth-tools software program that has hees adapted to mu on most computer platfurms. A low-cast student edition of Mwrt.xu, which can be used to run all at the files associated with this beak, is available in bath IBM-compatible and Mue iniosh versions. The MATLAB program scripts yielding exercise answers are listed in the text and are uvailuble in elecx’ouic form an detailed below. Computer-based problems, identified by a bullet (•) before the problem number, make up approximately 25% of the www.EasyEngineering.net ueoiceuuuCTen Device FONnAMENTAL5 problem total. Although oilier math-tools programs could he employed, the use of MA1’LAn is recommended in answering computer-based prublems. Because computerbased evenuisex xxd pmblnmx in the early chapters are spccitieally designed to progres sively enhunce MATLAO-use proficiexcy, the suer need net be familiar with the MATLAn program at the beginning of the beak, It is very important, however, to eoixplete a large percentage of the cattuputer-bused exercises and problems in the first three chapters. The exercises end probleies found ie later chapters vol anly assume a reasonably competent use of MAcLAB. hut also build upon the programs developed in the earlier chapters. • Ceitipuier Pregresni Fiiex. Program files of the MATLAB scripts ussactated with cam puier-baned exercises err available via the loterurt (ftp.nothworkn.com in the di rectory pub/beekn/piurret) ur on u floppy disk disiribuwd free of charge by Math Works, Inc. A pull-out card ix provided herein fat obtaining the free program disk ns’hieh is formatted for use with either an IBM-uemupsixble or Macintosh cemputem’. Each floppy disk enotains two sets al “m-files” to be used respectively ssith the pre-d.fl (stu dent 1st edition) or posm-d.fl (student 2nd edition) versions of MATLAB. The listings in the text are specifically derived from the Macintosh pest-dO version, bet they me iden tical to the corresponding IBM-uompsilibte version except far the occasional appearance of a Greek letier. • Snpdaleineul and Res’iuu’ Mini-Chepmrrs. The beak is divided eta three parts.. At the end of each part is a Supplement and Review’ mini-chapter. The mini-chapters, identified by darkened thunifi mab. contain as alicreatiee/supplemental reading list end infonmclteo table, reference citations for the preceding chxpicrs, an extrusive review-list of terms, and rcviem problem sets with answers. The revicss problem sets are derived from “closed-book” and “open-book” examinatinns. • t I, esiilQmily Chopteta. Chapteis 4, 9, 13, ned 19 have bern classified as “read-only.” Chapters with the read-nuly designation contain usostly qualitative inforniatten of a sup plemental nature. Tsse of the chapiers snrsey some of the latest device structures. In truded to be fax-reading, the read-only chapters are strategically placed to provide a change of pace. The chapters cantain oaly a small number of equations, no exercises, and few, if any. end-uf-cheptcr pcabletxs. In a course format, the chapters cnutd be skipped suith little lixss in continuity or preferably assigned as indnpendeut ncadtngs. • Preblem Pitferinutios Tablea. A compact table containing information abate the cad-of chapierprebleixs in a given chapter is leserted just before the problems. The information provided is (i) the text section or sabseclien after svhich the problem can be completed, (ii) the estiixated problem difficulty en a scale of 1 (emy or straightforward) to 5 (very difficult er exlrcesely time consuming). (di) suggested enedit tic peiut weigluing. and (iv) a short problem description. A bullet before the problem nnmber iduetifles a com puter-based problem. Au asturisk indicates campoter usage for pact of the problem. • Equiuxntt Stitneisiriex. The xery basic carrier niedeliug equations in Chapter 2 and the carrier action equations iv Chapter 3, equaf ens referenced thrnnghoet the text, ate as ganiaed and repeated itt Tables 2.4 end 3.3, respectively. These tables would be ideal us “crib sheets’ for closed-book exumiuamieus covering the material ix Part I of the text. auNeoum. iNneonuxcioN • Munxurumeittx cod Date. Contrary to the impression sometimes left by the sketches aud idealiced plots often feuud in iotroductery texrs. device characteristics are neat, seldem perfect, and are ceutioely recorded in measurement laberaturies. Herein a sampling of measurement deluils and results, derived from an undergraduate EE laboratory adminis tered by the author, is included in an attempt to convey the proper sense of reality. Par added details ou the described measurements, end fee a description af additional mea surements, the reader is refermd mx R. P. Pierret, Semiconductor Meumsruuieotx Lehure inuy Djaeratiuua Manual, Supplement A in the Modular Sectes en Solid State Devices, Addison-Wesley Publishing Caotpavy, Readiug MA. © t991. • Alternative Trnnunetit. Section 2.1 provides the mieimum required tneutturn; on the topic nf energy quautiaatiox is atateic systems. Appendix A. e’hich contains a mere indepth introduction to the queutieatieu concept and related topics. hm been iacladrd for those desiring snpphemeittal information. Section 2.1 may be tetally replaced by Appen din A wilh no loss in continuity. nufli www.EasyEngineering.net us srMicONDncTeR nuotcu FuNuaMuNTacs R3 Purl Ill 1 Snp d cunenh antI Review 713 Alicrtmafxe/Supltlettreitiul Reading List 713 Figute Sotirces/Ciled References Rcxiew List of ‘l’eetus 714 717 Ptnn Ibl—Reumrw Problem Sets and Answers 7lfl Appendices 733 Appenulix A Elements of Qnuntum Mechanics 733 A.t The Qtiattticatietn Coucepi A.l.t Blackbedy Radiation 733 733 A.t.2 The BuhrAiein A. 1.3 Wave-Particle Duality 733 737 A 2 Basic Pettitalistis 739 A.3 Electronic States in Abuts A.3.l The Hydrogen Atom 741 741 A.3.2 Muhti-Ehectroit Abuts Appendix B Appendix C 744 MOS Semicnnductor Electroutatieu—Exuct Solution 749 Defittitien of Panaivesers Exact Solution 750 MOS C—v Supplement 749 753 Appendix D MOS 1—V Supplement 755 Appendix E List oh’ Symbols 757 Appendix M MATLAB Program Script 771 19.2 (BJT_Eband) Exescisc 11.7 (BITI and Exercise 11.10 lBlTplus) Exercise ib.5 (MDS_.CV( 77fl Index 791 Esessise 771 774 GENERAL INTRODUCTION Cotticident with the wtitittp of this book, there lint been considerable teedia disrnssion abate the “Information Superhighway.” The envisioned highway itself, the physical link beimeee points sultporting the infortvation traffic, is fiber optic cable. Relative to tlte topic of this book, the oit and elf camps, whielt insert aitd extract the information from the higlt way, are scoticooductor (solid state) devices. Traffic control, the information procesning and the cetixemion to and from the haitian interface, is performed by computers. The ccxteal priicessinp unit (CPU). meotory, and oilier major coeipoueets inside the computer are again seivicendoeierdexiees lv the moderit machI, semiconductor devices are incorporated iv just about every muior system from automobiles to washing machines. Alihonglt toughly a half-ceitiury old, the field of stndy associated with semicendactor devices eontinnes to be dyunnnc and exeitieg. New end improved devices are beiitg slevel 1 aped st an almost maddexiog pace. While die device count in complex iotegrated circuits increases through the millions and the side-length of chips is itseasured in centimeters, the individuel devices are literally beiog shrank to atonue dimensions. Moreover, semiconduc tar propertieu desired for a given device nirecmnre but net usuiluble in tulane me being pnednced urtilicially; in essence, the semiconductor properties themselves tire now being engivecred to fit device specifications. This bock should ne viewed as u gateway in what the reader svill hnpefully agree is the faseinatnig realm of semiconductor devices. Ii was suriutex for junioror senior-level sin deitis olin hxxe at least an inlredacuary eupesnne ia electric field theory. The coverage esclades a representative sampling of infornietion about a wide variety of devices. Priivery einphosis, however, is placed en developing a fundamental nitderstanding of the internal workings of the tenre basic device structures. Au detailed below, thin book contains a num ber of unique features to assist the render in learning the material. Alerted at an curly stage to their existence, the render can plan to take full advantage of the cited features. ww w.E a syE ngi nee r ing . net • Conipuier-Bexed Ererciaes and End-nf Clusprer (Henss’trei-k) Problems. The majarily of chapters contain one er core Mw’rrxn-bunrd exercises requiring the use of a com puter MATLAB in a ninth-tools software program that has hees adapted to mu on most computer platfurms. A low-cast student edition of Mwrt.xu, which can be used to run all at the files associated with this beak, is available in bath IBM-compatible and Mue iniosh versions. The MATLAB program scripts yielding exercise answers are listed in the text and are uvailuble in elecx’ouic form an detailed below. Computer-based problems, identified by a bullet (•) before the problem number, make up approximately 25% of the www.EasyEngineering.net ueoiceuuuCTen Device FONnAMENTAL5 problem total. Although oilier math-tools programs could he employed, the use of MA1’LAn is recommended in answering computer-based prublems. Because computerbased evenuisex xxd pmblnmx in the early chapters are spccitieally designed to progres sively enhunce MATLAO-use proficiexcy, the suer need net be familiar with the MATLAn program at the beginning of the beak, It is very important, however, to eoixplete a large percentage of the cattuputer-bused exercises and problems in the first three chapters. The exercises end probleies found ie later chapters vol anly assume a reasonably competent use of MAcLAB. hut also build upon the programs developed in the earlier chapters. • Ceitipuier Pregresni Fiiex. Program files of the MATLAB scripts ussactated with cam puier-baned exercises err available via the loterurt (ftp.nothworkn.com in the di rectory pub/beekn/piurret) ur on u floppy disk disiribuwd free of charge by Math Works, Inc. A pull-out card ix provided herein fat obtaining the free program disk ns’hieh is formatted for use with either an IBM-uemupsixble or Macintosh cemputem’. Each floppy disk enotains two sets al “m-files” to be used respectively ssith the pre-d.fl (stu dent 1st edition) or posm-d.fl (student 2nd edition) versions of MATLAB. The listings in the text are specifically derived from the Macintosh pest-dO version, bet they me iden tical to the corresponding IBM-uompsilibte version except far the occasional appearance of a Greek letier. • Snpdaleineul and Res’iuu’ Mini-Chepmrrs. The beak is divided eta three parts.. At the end of each part is a Supplement and Review’ mini-chapter. The mini-chapters, identified by darkened thunifi mab. contain as alicreatiee/supplemental reading list end infonmclteo table, reference citations for the preceding chxpicrs, an extrusive review-list of terms, and rcviem problem sets with answers. The revicss problem sets are derived from “closed-book” and “open-book” examinatinns. • t I, esiilQmily Chopteta. Chapteis 4, 9, 13, ned 19 have bern classified as “read-only.” Chapters with the read-nuly designation contain usostly qualitative inforniatten of a sup plemental nature. Tsse of the chapiers snrsey some of the latest device structures. In truded to be fax-reading, the read-only chapters are strategically placed to provide a change of pace. The chapters cantain oaly a small number of equations, no exercises, and few, if any. end-uf-cheptcr pcabletxs. In a course format, the chapters cnutd be skipped suith little lixss in continuity or preferably assigned as indnpendeut ncadtngs. • Preblem Pitferinutios Tablea. A compact table containing information abate the cad-of chapierprebleixs in a given chapter is leserted just before the problems. The information provided is (i) the text section or sabseclien after svhich the problem can be completed, (ii) the estiixated problem difficulty en a scale of 1 (emy or straightforward) to 5 (very difficult er exlrcesely time consuming). (di) suggested enedit tic peiut weigluing. and (iv) a short problem description. A bullet before the problem nnmber iduetifles a com puter-based problem. Au asturisk indicates campoter usage for pact of the problem. • Equiuxntt Stitneisiriex. The xery basic carrier niedeliug equations in Chapter 2 and the carrier action equations iv Chapter 3, equaf ens referenced thrnnghoet the text, ate as ganiaed and repeated itt Tables 2.4 end 3.3, respectively. These tables would be ideal us “crib sheets’ for closed-book exumiuamieus covering the material ix Part I of the text. auNeoum. iNneonuxcioN • Munxurumeittx cod Date. Contrary to the impression sometimes left by the sketches aud idealiced plots often feuud in iotroductery texrs. device characteristics are neat, seldem perfect, and are ceutioely recorded in measurement laberaturies. Herein a sampling of measurement deluils and results, derived from an undergraduate EE laboratory adminis tered by the author, is included in an attempt to convey the proper sense of reality. Par added details ou the described measurements, end fee a description af additional mea surements, the reader is refermd mx R. P. Pierret, Semiconductor Meumsruuieotx Lehure inuy Djaeratiuua Manual, Supplement A in the Modular Sectes en Solid State Devices, Addison-Wesley Publishing Caotpavy, Readiug MA. © t991. • Alternative Trnnunetit. Section 2.1 provides the mieimum required tneutturn; on the topic nf energy quautiaatiox is atateic systems. Appendix A. e’hich contains a mere indepth introduction to the queutieatieu concept and related topics. hm been iacladrd for those desiring snpphemeittal information. Section 2.1 may be tetally replaced by Appen din A wilh no loss in continuity. nufli us srMicONDncTeR nuotcu FuNuaMuNTacs R3 Purl Ill 1 Snp d cunenh antI Review 713 Alicrtmafxe/Supltlettreitiul Reading List 713 Figute Sotirces/Ciled References Rcxiew List of ‘l’eetus 714 717 Ptnn Ibl—Reumrw Problem Sets and Answers 7lfl Appendices 733 Appenulix A Elements of Qnuntum Mechanics 733 A.t The Qtiattticatietn Coucepi A.l.t Blackbedy Radiation 733 733 A.t.2 The BuhrAiein A. 1.3 Wave-Particle Duality 733 737 A 2 Basic Pettitalistis 739 A.3 Electronic States in Abuts A.3.l The Hydrogen Atom 741 741 A.3.2 Muhti-Ehectroit Abuts Appendix B Appendix C 744 MOS Semicnnductor Electroutatieu—Exuct Solution 749 Defittitien of Panaivesers Exact Solution 750 749 MOS C—v Supplement 753 Appendix D MOS 1—V Supplement 755 Appendix E List oh’ Symbols Appendix M MATLAB 757 Program Script 771 19.2 (BJT_Eband) Exescisc 11.7 (BITI and Exercise 11.10 lBlTplus) Exercise ib.5 (MDS_.CV( 77fl Index 791 Esessise 771 774 GENERAL INTRODUCTION Cotticident with the wtitittp of this book, there lint been considerable teedia disrnssion abate the “Information Superhighway.” The envisioned highway itself, the physical link beimeee points sultporting the infortvation traffic, is fiber optic cable. Relative to tlte topic of this book, the oit and elf camps, whielt insert aitd extract the information from the higlt way, are scoticooductor (solid state) devices. Traffic control, the information procesning and the cetixemion to and from the haitian interface, is performed by computers. The ccxteal priicessinp unit (CPU). meotory, and oilier major coeipoueets inside the computer are again seivicendoeierdexiees lv the moderit machI, semiconductor devices are incorporated iv just about every muior system from automobiles to washing machines. Alihonglt toughly a half-ceitiury old, the field of stndy associated with semicendactor devices eontinnes to be dyunnnc and exeitieg. New end improved devices are beiitg slevel 1 aped st an almost maddexiog pace. While die device count in complex iotegrated circuits increases through the millions and the side-length of chips is itseasured in centimeters, the individuel devices are literally beiog shrank to atonue dimensions. Moreover, semiconduc tar propertieu desired for a given device nirecmnre but net usuiluble in tulane me being pnednced urtilicially; in essence, the semiconductor properties themselves tire now being engivecred to fit device specifications. This bock should ne viewed as u gateway in what the reader svill hnpefully agree is the faseinatnig realm of semiconductor devices. Ii was suriutex for junioror senior-level sin deitis olin hxxe at least an inlredacuary eupesnne ia electric field theory. The coverage esclades a representative sampling of infornietion about a wide variety of devices. Priivery einphosis, however, is placed en developing a fundamental nitderstanding of the internal workings of the tenre basic device structures. Au detailed below, thin book contains a num ber of unique features to assist the render in learning the material. Alerted at an curly stage to their existence, the render can plan to take full advantage of the cited features. • Conipuier-Bexed Ererciaes and End-nf Clusprer (Henss’trei-k) Problems. The majarily of chapters contain one er core Mw’rrxn-bunrd exercises requiring the use of a com puter MATLAB in a ninth-tools software program that has hees adapted to mu on most computer platfurms. A low-cast student edition of Mwrt.xu, which can be used to run all at the files associated with this beak, is available in bath IBM-compatible and Mue iniosh versions. The MATLAB program scripts yielding exercise answers are listed in the text and are uvailuble in elecx’ouic form an detailed below. Computer-based problems, identified by a bullet (•) before the problem number, make up approximately 25% of the www.EasyEngineering.net auNeoum. iNneonuxcioN ueoiceuuuCTen Device FONnAMENTAL5 problem total. Although oilier math-tools programs could he employed, the use of MA1’LAn is recommended in answering computer-based prublems. Because computerbased evenuisex xxd pmblnmx in the early chapters are spccitieally designed to progres sively enhunce MATLAO-use proficiexcy, the suer need net be familiar with the MATLAn program at the beginning of the beak, It is very important, however, to eoixplete a large percentage of the cattuputer-bused exercises and problems in the first three chapters. The exercises end probleies found ie later chapters vol anly assume a reasonably competent use of MAcLAB. hut also build upon the programs developed in the earlier chapters. • Ceitipuier Pregresni Fiiex. Program files of the MATLAB scripts ussactated with cam puier-baned exercises err available via the loterurt (ftp.nothworkn.com in the di rectory pub/beekn/piurret) ur on u floppy disk disiribuwd free of charge by Math Works, Inc. A pull-out card ix provided herein fat obtaining the free program disk ns’hieh is formatted for use with either an IBM-uemupsixble or Macintosh cemputem’. Each floppy disk enotains two sets al “m-files” to be used respectively ssith the pre-d.fl (stu dent 1st edition) or posm-d.fl (student 2nd edition) versions of MATLAB. The listings in the text are specifically derived from the Macintosh pest-dO version, bet they me iden tical to the corresponding IBM-uompsilibte version except far the occasional appearance of a Greek letier. ww w .Ea syE ngi • Snpdaleineul and Res’iuu’ Mini-Chepmrrs. The beak is divided eta three parts.. At the end of each part is a Supplement and Review’ mini-chapter. The mini-chapters, identified by darkened thunifi mab. contain as alicreatiee/supplemental reading list end infonmclteo table, reference citations for the preceding chxpicrs, an extrusive review-list of terms, and rcviem problem sets with answers. The revicss problem sets are derived from “closed-book” and “open-book” examinatinns. nee rin g • t I, esiilQmily Chopteta. Chapteis 4, 9, 13, ned 19 have bern classified as “read-only.” Chapters with the read-nuly designation contain usostly qualitative inforniatten of a sup plemental nature. Tsse of the chapiers snrsey some of the latest device structures. In truded to be fax-reading, the read-only chapters are strategically placed to provide a change of pace. The chapters cantain oaly a small number of equations, no exercises, and few, if any. end-uf-cheptcr pcabletxs. In a course format, the chapters cnutd be skipped suith little lixss in continuity or preferably assigned as indnpendeut ncadtngs. .ne t • Preblem Pitferinutios Tablea. A compact table containing information abate the cad-of chapierprebleixs in a given chapter is leserted just before the problems. The information provided is (i) the text section or sabseclien after svhich the problem can be completed, (ii) the estiixated problem difficulty en a scale of 1 (emy or straightforward) to 5 (very difficult er exlrcesely time consuming). (di) suggested enedit tic peiut weigluing. and (iv) a short problem description. A bullet before the problem nnmber iduetifles a com puter-based problem. Au asturisk indicates campoter usage for pact of the problem. • Equiuxntt Stitneisiriex. The xery basic carrier niedeliug equations in Chapter 2 and the carrier action equations iv Chapter 3, equaf ens referenced thrnnghoet the text, ate as ganiaed and repeated itt Tables 2.4 end 3.3, respectively. These tables would be ideal us “crib sheets’ for closed-book exumiuamieus covering the material ix Part I of the text. www.EasyEngineering.net • Munxurumeittx cod Date. Contrary to the impression sometimes left by the sketches aud idealiced plots often feuud in iotroductery texrs. device characteristics are neat, seldem perfect, and are ceutioely recorded in measurement laberaturies. Herein a sampling of measurement deluils and results, derived from an undergraduate EE laboratory adminis tered by the author, is included in an attempt to convey the proper sense of reality. Par added details ou the described measurements, end fee a description af additional mea surements, the reader is refermd mx R. P. Pierret, Semiconductor Meumsruuieotx Lehure inuy Djaeratiuua Manual, Supplement A in the Modular Sectes en Solid State Devices, Addison-Wesley Publishing Caotpavy, Readiug MA. © t991. • Alternative Trnnunetit. Section 2.1 provides the mieimum required tneutturn; on the topic nf energy quautiaatiox is atateic systems. Appendix A. e’hich contains a mere indepth introduction to the queutieatieu concept and related topics. hm been iacladrd for those desiring snpphemeittal information. Section 2.1 may be tetally replaced by Appen din A wilh no loss in continuity. nufli us srMicONDncTeR nuotcu FuNuaMuNTacs R3 Purl Ill 1 Snp d cunenh antI Review 713 Alicrtmafxe/Supltlettreitiul Reading List 713 Figute Sotirces/Ciled References Rcxiew List of ‘l’eetus 714 717 Ptnn Ibl—Reumrw Problem Sets and Answers 7lfl Appendices 733 Appenulix A Elements of Qnuntum Mechanics 733 A.t The Qtiattticatietn Coucepi A.l.t Blackbedy Radiation 733 733 A.t.2 The BuhrAiein A. 1.3 Wave-Particle Duality 733 737 A 2 Basic Pettitalistis 739 A.3 Electronic States in Abuts A.3.l The Hydrogen Atom 741 741 A.3.2 Muhti-Ehectroit Abuts Appendix B Appendix C 744 MOS Semicnnductor Electroutatieu—Exuct Solution 749 Defittitien of Panaivesers Exact Solution 750 MOS C—v Supplement Appendix D MOS 1—V Supplement Appendix E List oh’ Symbols Appendix M MATLAB Program Script 749 753 755 757 771 19.2 (BJT_Eband) Exescisc 11.7 (BITI and Exercise 11.10 lBlTplus) Exercise ib.5 (MDS_.CV( 77fl Index 791 Esessise 771 774 GENERAL INTRODUCTION Cotticident with the wtitittp of this book, there lint been considerable teedia disrnssion abate the “Information Superhighway.” The envisioned highway itself, the physical link beimeee points sultporting the infortvation traffic, is fiber optic cable. Relative to tlte topic of this book, the oit and elf camps, whielt insert aitd extract the information from the higlt way, are scoticooductor (solid state) devices. Traffic control, the information procesning and the cetixemion to and from the haitian interface, is performed by computers. The ccxteal priicessinp unit (CPU). meotory, and oilier major coeipoueets inside the computer are again seivicendoeierdexiees lv the moderit machI, semiconductor devices are incorporated iv just about every muior system from automobiles to washing machines. Alihonglt toughly a half-ceitiury old, the field of stndy associated with semicendactor devices eontinnes to be dyunnnc and exeitieg. New end improved devices are beiitg slevel 1 aped st an almost maddexiog pace. While die device count in complex iotegrated circuits increases through the millions and the side-length of chips is itseasured in centimeters, the individuel devices are literally beiog shrank to atonue dimensions. Moreover, semiconduc tar propertieu desired for a given device nirecmnre but net usuiluble in tulane me being pnednced urtilicially; in essence, the semiconductor properties themselves tire now being engivecred to fit device specifications. This bock should ne viewed as u gateway in what the reader svill hnpefully agree is the faseinatnig realm of semiconductor devices. Ii was suriutex for junioror senior-level sin deitis olin hxxe at least an inlredacuary eupesnne ia electric field theory. The coverage esclades a representative sampling of infornietion about a wide variety of devices. Priivery einphosis, however, is placed en developing a fundamental nitderstanding of the internal workings of the tenre basic device structures. Au detailed below, thin book contains a num ber of unique features to assist the render in learning the material. Alerted at an curly stage to their existence, the render can plan to take full advantage of the cited features. • Conipuier-Bexed Ererciaes and End-nf Clusprer (Henss’trei-k) Problems. The majarily of chapters contain one er core Mw’rrxn-bunrd exercises requiring the use of a com puter MATLAB in a ninth-tools software program that has hees adapted to mu on most computer platfurms. A low-cast student edition of Mwrt.xu, which can be used to run all at the files associated with this beak, is available in bath IBM-compatible and Mue iniosh versions. The MATLAB program scripts yielding exercise answers are listed in the text and are uvailuble in elecx’ouic form an detailed below. Computer-based problems, identified by a bullet (•) before the problem number, make up approximately 25% of the www.EasyEngineering.net auNeoum. iNneonuxcioN ueoiceuuuCTen Device FONnAMENTAL5 problem total. Although oilier math-tools programs could he employed, the use of MA1’LAn is recommended in answering computer-based prublems. Because computerbased evenuisex xxd pmblnmx in the early chapters are spccitieally designed to progres sively enhunce MATLAO-use proficiexcy, the suer need net be familiar with the MATLAn program at the beginning of the beak, It is very important, however, to eoixplete a large percentage of the cattuputer-bused exercises and problems in the first three chapters. The exercises end probleies found ie later chapters vol anly assume a reasonably competent use of MAcLAB. hut also build upon the programs developed in the earlier chapters. • Ceitipuier Pregresni Fiiex. Program files of the MATLAB scripts ussactated with cam puier-baned exercises err available via the loterurt (ftp.nothworkn.com in the di rectory pub/beekn/piurret) ur on u floppy disk disiribuwd free of charge by Math Works, Inc. A pull-out card ix provided herein fat obtaining the free program disk ns’hieh is formatted for use with either an IBM-uemupsixble or Macintosh cemputem’. Each floppy disk enotains two sets al “m-files” to be used respectively ssith the pre-d.fl (stu dent 1st edition) or posm-d.fl (student 2nd edition) versions of MATLAB. The listings in the text are specifically derived from the Macintosh pest-dO version, bet they me iden tical to the corresponding IBM-uompsilibte version except far the occasional appearance of a Greek letier. • Snpdaleineul and Res’iuu’ Mini-Chepmrrs. The beak is divided eta three parts.. At the end of each part is a Supplement and Review’ mini-chapter. The mini-chapters, identified by darkened thunifi mab. contain as alicreatiee/supplemental reading list end infonmclteo table, reference citations for the preceding chxpicrs, an extrusive review-list of terms, and rcviem problem sets with answers. The revicss problem sets are derived from “closed-book” and “open-book” examinatinns. • t I, esiilQmily Chopteta. Chapteis 4, 9, 13, ned 19 have bern classified as “read-only.” Chapters with the read-nuly designation contain usostly qualitative inforniatten of a sup plemental nature. Tsse of the chapiers snrsey some of the latest device structures. In truded to be fax-reading, the read-only chapters are strategically placed to provide a change of pace. The chapters cantain oaly a small number of equations, no exercises, and few, if any. end-uf-cheptcr pcabletxs. In a course format, the chapters cnutd be skipped suith little lixss in continuity or preferably assigned as indnpendeut ncadtngs. nufli • Munxurumeittx cod Date. Contrary to the impression sometimes left by the sketches aud idealiced plots often feuud in iotroductery texrs. device characteristics are neat, seldem perfect, and are ceutioely recorded in measurement laberaturies. Herein a sampling of measurement deluils and results, derived from an undergraduate EE laboratory adminis tered by the author, is included in an attempt to convey the proper sense of reality. Par added details ou the described measurements, end fee a description af additional mea surements, the reader is refermd mx R. P. Pierret, Semiconductor Meumsruuieotx Lehure inuy Djaeratiuua Manual, Supplement A in the Modular Sectes en Solid State Devices, Addison-Wesley Publishing Caotpavy, Readiug MA. © t991. • Alternative Trnnunetit. Section 2.1 provides the mieimum required tneutturn; on the topic nf energy quautiaatiox is atateic systems. Appendix A. e’hich contains a mere indepth introduction to the queutieatieu concept and related topics. hm been iacladrd for those desiring snpphemeittal information. Section 2.1 may be tetally replaced by Appen din A wilh no loss in continuity. ww w.E asy En gin eer ing .ne • Preblem Pitferinutios Tablea. A compact table containing information abate the cad-of chapierprebleixs in a given chapter is leserted just before the problems. The information provided is (i) the text section or sabseclien after svhich the problem can be completed, (ii) the estiixated problem difficulty en a scale of 1 (emy or straightforward) to 5 (very difficult er exlrcesely time consuming). (di) suggested enedit tic peiut weigluing. and (iv) a short problem description. A bullet before the problem nnmber iduetifles a com puter-based problem. Au asturisk indicates campoter usage for pact of the problem. • Equiuxntt Stitneisiriex. The xery basic carrier niedeliug equations in Chapter 2 and the carrier action equations iv Chapter 3, equaf ens referenced thrnnghoet the text, ate as ganiaed and repeated itt Tables 2.4 end 3.3, respectively. These tables would be ideal us “crib sheets’ for closed-book exumiuamieus covering the material ix Part I of the text. www.EasyEngineering.net t www.EasyEngineering.net PART ww w.E I as y En gin e SEMICONDUCTOR FUNDAM ENTALS eri ng. ne t www.EasyEngineering.net 1 Semiconductors: A General Introduction 1.1 GENERAL MATERIAL PROPERTIES The vast majority of all solid state devices on the market today are fobricated from a class of materials known as semiconductors. It is therefore appropriate that we begin the discusSian by examining the general nature of semicondacting materials. 1.1.1 Composition Table I I lists the atomic compositions of semiconductor-u that are likely to be encountered in the device literature. As noted, tlsc semtcoaductar family of matenals includes the ele mental semiconductors Si and Ge, compound semiconductors such as GaAs and ZnSe, and As.t Due in large part to the advanced state of its fabrication tech 0 _ 1 alloys like Al,Ga nology, Si is far and away the must mportant of the semicundactors, totally dominatrng die prevent cumuserciai market. The s’ast majority of discrete devices and integrated circuits (ICs). iucludirtg the central processing unit (CPU) in microcomputers and the ignition mod ule in itrodern automobiles, are made from this material. GaAs. exhibiting snperiorelectrott transport properties and special optical properties, is employed in a srguificttul number of applications ranging from laser diodes to high-speed tCs. The remaining semicotrdnctors are utilized in “niche” applications that are invariably of a high-speed, high-temperature, or optoelectronic nature. Given its present position of dominance, we will tend to focus our attention on Si in the text development. Where feasible, boss ever, GaAs will be gtven com parable consideratisru and otlter semiconductors will be featured irs the discussion warraats. Although the number of xemiconducttug materials is rmsunubly large, the list is actu ally quite limited considering the total number nf elements and possible combinations of elementv. Note that, referring to the abbreviated periodic chart of’ the eleurents in Table 1.2, only a certaitt group of elements and elemental combinations typically gtvc rtse to semiconducting motterials. Except for the lV-Vl compounds, all of the setniconductors listed itt Table 1.1 are composed at elements appearing in Coloton IV of the Periodic Table or are a combination of clements in Periodic Table columns an eqaal dismancr to either stde of The v (Or 7.1 iv attoy rormuirr ira traction tying brivonru 0 rvd t AtcrGrr,,/io would isOieorsaeareria( with 3 At and 7 Cr cr0105 wrovnry tu As amums. www.EasyEngineering.net ww PART I SEMIC w.E ONDUCTOR as AM ENTALS FUND yE ngi nee r ing . net www.EasyEngineering.net 1 Semiconductors: A General Introduction 1.1 GENERAL MATERIAL PROPERTIES The vast majority of all solid state devices on the market today are fobricated from a class of materials known as semiconductors. It is therefore appropriate that we begin the discusSian by examining the general nature of semicondacting materials. 1.1.1 Composition Table I I lists the atomic compositions of semiconductor-u that are likely to be encountered in the device literature. As noted, tlsc semtcoaductar family of matenals includes the ele mental semiconductors Si and Ge, compound semiconductors such as GaAs and ZnSe, and As.t Due in large part to the advanced state of its fabrication tech 0 _ 1 alloys like Al,Ga nology, Si is far and away the must mportant of the semicundactors, totally dominatrng die prevent cumuserciai market. The s’ast majority of discrete devices and integrated circuits (ICs). iucludirtg the central processing unit (CPU) in microcomputers and the ignition mod ule in itrodern automobiles, are made from this material. GaAs. exhibiting snperiorelectrott transport properties and special optical properties, is employed in a srguificttul number of applications ranging from laser diodes to high-speed tCs. The remaining semicotrdnctors are utilized in “niche” applications that are invariably of a high-speed, high-temperature, or optoelectronic nature. Given its present position of dominance, we will tend to focus our attention on Si in the text development. Where feasible, boss ever, GaAs will be gtven com parable consideratisru and otlter semiconductors will be featured irs the discussion warraats. Although the number of xemiconducttug materials is rmsunubly large, the list is actu ally quite limited considering the total number nf elements and possible combinations of elementv. Note that, referring to the abbreviated periodic chart of’ the eleurents in Table 1.2, only a certaitt group of elements and elemental combinations typically gtvc rtse to semiconducting motterials. Except for the lV-Vl compounds, all of the setniconductors listed itt Table 1.1 are composed at elements appearing in Coloton IV of the Periodic Table or are a combination of clements in Periodic Table columns an eqaal dismancr to either stde of The v (Or 7.1 iv attoy rormuirr ira traction tying brivonru 0 rvd t AtcrGrr,,/io would isOieorsaeareria( with 3 At and 7 Cr cr0105 wrovnry tu As amums. PART I SEMICONDUCTOR FUNDAM ENTALS www.EasyEngineering.net 1 Semiconductors: A General Introduction ww w 1.1 GENERAL MATERIAL PROPERTIES .Ea The vast majority of all solid state devices on the market today are fobricated from a class of materials known as semiconductors. It is therefore appropriate that we begin the discusSian by examining the general nature of semicondacting materials. syE 1.1.1 Composition ngi nee rin g .ne t Table I I lists the atomic compositions of semiconductor-u that are likely to be encountered in the device literature. As noted, tlsc semtcoaductar family of matenals includes the ele mental semiconductors Si and Ge, compound semiconductors such as GaAs and ZnSe, and As.t Due in large part to the advanced state of its fabrication tech 0 _ 1 alloys like Al,Ga nology, Si is far and away the must mportant of the semicundactors, totally dominatrng die prevent cumuserciai market. The s’ast majority of discrete devices and integrated circuits (ICs). iucludirtg the central processing unit (CPU) in microcomputers and the ignition mod ule in itrodern automobiles, are made from this material. GaAs. exhibiting snperiorelectrott transport properties and special optical properties, is employed in a srguificttul number of applications ranging from laser diodes to high-speed tCs. The remaining semicotrdnctors are utilized in “niche” applications that are invariably of a high-speed, high-temperature, or optoelectronic nature. Given its present position of dominance, we will tend to focus our attention on Si in the text development. Where feasible, boss ever, GaAs will be gtven com parable consideratisru and otlter semiconductors will be featured irs the discussion warraats. Although the number of xemiconducttug materials is rmsunubly large, the list is actu ally quite limited considering the total number nf elements and possible combinations of elementv. Note that, referring to the abbreviated periodic chart of’ the eleurents in Table 1.2, only a certaitt group of elements and elemental combinations typically gtvc rtse to semiconducting motterials. Except for the lV-Vl compounds, all of the setniconductors listed itt Table 1.1 are composed at elements appearing in Coloton IV of the Periodic Table or are a combination of clements in Periodic Table columns an eqaal dismancr to either stde of The v (Or 7.1 iv attoy rormuirr ira traction tying brivonru 0 rvd t AtcrGrr,,/io would isOieorsaeareria( with 3 At and 7 Cr cr0105 wrovnry tu As amums. www.EasyEngineering.net PART I SEMICONDUCTOR FUNDAM ENTALS www.EasyEngineering.net 1 Semiconductors: A General Introduction ww w.E 1.1 GENERAL MATERIAL PROPERTIES The vast majority of all solid state devices on the market today are fobricated from a class of materials known as semiconductors. It is therefore appropriate that we begin the discusSian by examining the general nature of semicondacting materials. 1.1.1 Composition asy En Table I I lists the atomic compositions of semiconductor-u that are likely to be encountered in the device literature. As noted, tlsc semtcoaductar family of matenals includes the ele mental semiconductors Si and Ge, compound semiconductors such as GaAs and ZnSe, and As.t Due in large part to the advanced state of its fabrication tech 0 _ 1 alloys like Al,Ga nology, Si is far and away the must mportant of the semicundactors, totally dominatrng die prevent cumuserciai market. The s’ast majority of discrete devices and integrated circuits (ICs). iucludirtg the central processing unit (CPU) in microcomputers and the ignition mod ule in itrodern automobiles, are made from this material. GaAs. exhibiting snperiorelectrott transport properties and special optical properties, is employed in a srguificttul number of applications ranging from laser diodes to high-speed tCs. The remaining semicotrdnctors are utilized in “niche” applications that are invariably of a high-speed, high-temperature, or optoelectronic nature. Given its present position of dominance, we will tend to focus our attention on Si in the text development. Where feasible, boss ever, GaAs will be gtven com parable consideratisru and otlter semiconductors will be featured irs the discussion warraats. Although the number of xemiconducttug materials is rmsunubly large, the list is actu ally quite limited considering the total number nf elements and possible combinations of elementv. Note that, referring to the abbreviated periodic chart of’ the eleurents in Table 1.2, only a certaitt group of elements and elemental combinations typically gtvc rtse to semiconducting motterials. Except for the lV-Vl compounds, all of the setniconductors listed itt Table 1.1 are composed at elements appearing in Coloton IV of the Periodic Table or are a combination of clements in Periodic Table columns an eqaal dismancr to either stde of gin eer ing .ne The v (Or 7.1 iv attoy rormuirr ira traction tying brivonru 0 rvd t AtcrGrr,,/io would isOieorsaeareria( with 3 At and 7 Cr cr0105 wrovnry tu As amums. www.EasyEngineering.net t www.EasyEngineering.net Table 1.1 SEMICONDUCTORS: A GENERAL INTRODUCTION Scirricoirductor Materials. SriiiirO5ieta’t0r l’iciieral Synthol Nsssne Si GC Silicon Germaniani (a) IV-1V SiC Silicon caibide )b) Ill—V AlP AlAs AlSb GaN GaP GaAs GaSh loP InAs InSli Aleiiiinnns phosphide Alaniiitam arsenidC Atanriourn aotinsonidr Gallinos mir.de Gallium phosphide Gallinur arsenide Gallisno aotimonide ludisnr shospliide Indium arsenide Indian: aetesronide ZsG ZeS ZnSe ZnTe CdS CdSe CdTe 1-IgS Zinc oxide PbS PbSe PbTe Lead sulfide Lead seleoide Load ielleride Classification I I I Eleroental Table 1.2 II 5 Abhrevialed Periodic Chart of the Elemenrs. II Ill IV VI V (2) Compounds ww )c) w.E Il-VI as y En gin e Id) IV-VI Zinc sulfide Zinc selenide Zioc nellaride Cadoiinos salfide Cadmiurss seleiside Cadmium telloride Mercory sulfide eri (3) Alloys (a) Binary Si ,,Ge, (b) Ternary Al,Ga _,As. 1 ,As Al,1o — Cd..,Mn,Te GaAs_,P, Ga, ln ,As Ga,le_,P ,Cd,Te 1 Hg — )e) Qaalernary Colamn IV. The Column Ill clesneur Ga plus the Cotame V elemeet As yields the Ill-V compouod semicoudactor GaAs; the Column II element Zn pIes ihe Cotamn VI elnisrcol Se yields the Il-Vt compoand sennscooductorZnSe; the fractional combination of the Cot ansu Ill elneneots Al arid Go plsis time Colusoo V element As yields the alloy semivondnrror Al, Ga ,As. This very general property is related to the chemical bouding in semicoedne tors, mherc, on tIre average. Ilseve ore four valence electroos per atom. ng. ne (or Ga_, Al, As) (at Ini Al,As) - (or In ,Ga, As) .,Ga,P) 1 )arIn . 1 —n 1 _As Sb kl,Ga 1 I As Ga In — t 1.1.2 Purity As mill be euplained in Chapter 2. extremely minate traces of imporily atoms catted “dopanrs” can have a drastic effect on the electrical properties of semiconductors. For this reason, the compositional parity of semiconductors nsust he very carefully controlled and, in fact, modere seroicondociors are some of the pnrest solid materials in existence In Sr. for esampte, the nuinrenisonal content of depart atoms is rondnely less than one atom per try Si atoms. To assist the reader in attempting to eusoprehend this incredible level of parity, let us suppose a forest of niaple trees mas planted frons coast to coast, border to border, at 50-fr centers across the United States (including Alaska). Ao imparity level of one pm’r pnr I0 mould vocresporsd to hnding ahoat 25 crabapple trees iu the maple tree formt covering the United Sroresl Jr shonld he emphasieed that the cited material parity refers to nesinrenriorrat undesired impurities. Typically, dopavi atomos at levels ranging from musely added 5 one part per I0 to one impnrily alerts per try semiconductor atoms svill be pmnr so the semiconductor to control Is electrical properties. www.EasyEngineering.net 6 neeieoNnsc’rOR FaNoaMreeAt.u — , nEMIC0NDnCTGRS A GENERAL nsnRonucnsoN achieve thin goal, sec first examine how one goes about describing the spatial position ing of atoms within crystals. Nest, a bit of “visualiearion” practice wills simple three dimensional lattices (atomic arrangements) is presented prior to examining semieoodoetor lattices themselves. The section coucledes with an introduction to the related topic of Mil ler indices. Miller indices are a convenient shorthand notosion widely employed for iden tifying specific planes and diteclious within crystals. lot Aemosrusoas 0 recounisahie v iunu’sanee osaer 151 tnt vssnsssOmor Comnpiemeiy esdsmsd mr seemenis IsI CsysmeOuee Eemmme mesa is mode aver slums is en erdemir smmsv Figare 1.1 General elassihcauao of solids based an rho darrea af atomic ordev (a) amorphaas, (hI polycrysratlise, and (el cryssallinc. 1.1.3 Structure The spatial arrangement of atoms mithso a snuteriol plays an important role in determining the precise properties nf the material. As shomn schemsiatically in Pig. 1.1. the atomic ar rangement withnn a solid cannes is to he placed into one of three broad elmsiflcatinns; naosely. omoephons, polycrvstalline. nr erystullose. Aa amorphous solid is a material in which there is no recagnieahle long-range order in the positioning of atoms within the material. The atomic arrangemeot in any given section of an amoenhoas material mill look differeot from the atomic arrangemees in any oilier section of the material. Crystatlioe solids lie at the opposite cud of the order’ spectrum: in a crystalline material the atoms are arravged in an orderly three-dimensional array. Given any section of a eeystallioe na tertal. one can readily reprodoee the atomic arrangement in awe other section of Ihe mote rial. Poterystalline solids comprise ae intermediate ease io svhich the solid is coviposed of crystallisse sebsections that me disjointed or misorieoled relative to one another. Upon esaniiiiing the mossy solid store devices io existence, one readily finds euamvtes of of three structural foress. An antorphoos-Si thin-flint seaesissor is ased as the ssvirehing element in liquid crystal disgtcys )LCDs): polycrystattiae Si gates are employed in Metal Gside-Sessucondsrcsor Field-Effect Traosistors tlstGSFETsi. In rhe vast ntajorits of de vices, hosvever, the active region of he device is siteared svithin a crystalline semi condarsoc The ovemarhelmiog netober of devices fabricated soitay employ riyatu)Iisrc semicondactors. 1.2.1 The Unit Cell Concept Simply stated, a unit cell is a small portion of any givers crystal that could be used to reprodoce the crystal. To help establish the null cell (or building-block) concept, let an consider ihe two-disoerssional lattice shosvn is Fig. l.2(a). To describe this lattice or to totally specify the physical ehuracteristies of the lattice, oue need ooly provide the unit cell shown in Pig. 1.2(b), As indicated in Pig. l.2(r), she original lattice can be readily repro duced by merely dophieatmcg the unit cell and siuckiog the doptieares next io each other in uo orderly fashion. In dealing wish unit cells there often arises a misunderstundieg, and hence confesion, relative to two points. Psrsr, evil cells are uos necessarily anique. The unit cell shown in Pig. 1.2(d) ss as aceeplable as the Pig. 1.2(b) unil cell for specifying the original lattice of 00000 00000 00000 ‘0 0 0 Q aIco 0 0 0 lot d/5mes 000 1.2 CRYSTAL STRUCTURE Tire disessssion at the end of she preceding seetiou leads nicely iuro the topic of this section. Strive sri-use semiconductors are typically erystalliue in form, it seems reasonable to seek oar additional inforthotion absmot the crystalline state. Gor nsojor gout here is to present more detailed picture of the atomic arrangement within the principal semiconsteetors. To ibl Id lal 1.2 Introdsermon me he unit cell meshed uf describing umomic arrungemeems within crystals (a) Sampto iwo-dmmssensmunul lattice. (b) Gob cell corrospnnmding In she gwt (a) laltice. (ci Reprndac nor: of mIre origioot bruce. (d) As alseruasiso unit cell. Figure 7 www.EasyEngineering.net Table 1.1 SEMICONDUCTORS: A GENERAL INTRODUCTION Scirricoirductor Materials. SriiiirO5ieta’t0r l’iciieral Synthol Nsssne Si GC Silicon Germaniani (a) IV-1V SiC Silicon caibide )b) Ill—V AlP AlAs AlSb GaN GaP GaAs GaSh loP InAs InSli Aleiiiinnns phosphide Alaniiitam arsenidC Atanriourn aotinsonidr Gallinos mir.de Gallium phosphide Gallinur arsenide Gallisno aotimonide ludisnr shospliide Indium arsenide Indian: aetesronide ZsG ZeS ZnSe ZnTe CdS CdSe CdTe 1-IgS Zinc oxide PbS PbSe PbTe Lead sulfide Lead seleoide Load ielleride Classification I I I Eleroental Table 1.2 II 5 Abhrevialed Periodic Chart of the Elemenrs. II Ill IV VI V (2) Compounds )c) Il-VI Id) IV-VI Zinc sulfide Zinc selenide Zioc nellaride Cadoiinos salfide Cadmiurss seleiside Cadmium telloride Mercory sulfide (3) Alloys (a) Binary Si ,,Ge, (b) Ternary Al,Ga _,As. 1 ,As Al,1o — Cd..,Mn,Te GaAs_,P, Ga, ln ,As Ga,le_,P ,Cd,Te 1 Hg — )e) Qaalernary (or Ga_, Al, As) (at Ini Al,As) - (or In ,Ga, As) .,Ga,P) 1 )arIn . 1 —n 1 _As Sb kl,Ga 1 I As Ga In ww w.E a syE ngi Colamn IV. The Column Ill clesneur Ga plus the Cotame V elemeet As yields the Ill-V compouod semicoudactor GaAs; the Column II element Zn pIes ihe Cotamn VI elnisrcol Se yields the Il-Vt compoand sennscooductorZnSe; the fractional combination of the Cot ansu Ill elneneots Al arid Go plsis time Colusoo V element As yields the alloy semivondnrror Al, Ga ,As. This very general property is related to the chemical bouding in semicoedne tors, mherc, on tIre average. Ilseve ore four valence electroos per atom. nee r ing . — 1.1.2 Purity net As mill be euplained in Chapter 2. extremely minate traces of imporily atoms catted “dopanrs” can have a drastic effect on the electrical properties of semiconductors. For this reason, the compositional parity of semiconductors nsust he very carefully controlled and, in fact, modere seroicondociors are some of the pnrest solid materials in existence In Sr. for esampte, the nuinrenisonal content of depart atoms is rondnely less than one atom per try Si atoms. To assist the reader in attempting to eusoprehend this incredible level of parity, let us suppose a forest of niaple trees mas planted frons coast to coast, border to border, at 50-fr centers across the United States (including Alaska). Ao imparity level of one pm’r pnr I0 mould vocresporsd to hnding ahoat 25 crabapple trees iu the maple tree formt covering the United Sroresl Jr shonld he emphasieed that the cited material parity refers to nesinrenriorrat undesired impurities. Typically, dopavi atomos at levels ranging from musely added 5 one part per I0 to one impnrily alerts per try semiconductor atoms svill be pmnr so the semiconductor to control Is electrical properties. www.EasyEngineering.net 6 neeieoNnsc’rOR FaNoaMreeAt.u — , nEMIC0NDnCTGRS A GENERAL nsnRonucnsoN achieve thin goal, sec first examine how one goes about describing the spatial position ing of atoms within crystals. Nest, a bit of “visualiearion” practice wills simple three dimensional lattices (atomic arrangements) is presented prior to examining semieoodoetor lattices themselves. The section coucledes with an introduction to the related topic of Mil ler indices. Miller indices are a convenient shorthand notosion widely employed for iden tifying specific planes and diteclious within crystals. lot Aemosrusoas 0 recounisahie v iunu’sanee osaer 151 tnt vssnsssOmor Comnpiemeiy esdsmsd mr seemenis IsI CsysmeOuee Eemmme mesa is mode aver slums is en erdemir smmsv Figare 1.1 General elassihcauao of solids based an rho darrea af atomic ordev (a) amorphaas, (hI polycrysratlise, and (el cryssallinc. 1.1.3 Structure The spatial arrangement of atoms mithso a snuteriol plays an important role in determining the precise properties nf the material. As shomn schemsiatically in Pig. 1.1. the atomic ar rangement withnn a solid cannes is to he placed into one of three broad elmsiflcatinns; naosely. omoephons, polycrvstalline. nr erystullose. Aa amorphous solid is a material in which there is no recagnieahle long-range order in the positioning of atoms within the material. The atomic arrangemeot in any given section of an amoenhoas material mill look differeot from the atomic arrangemees in any oilier section of the material. Crystatlioe solids lie at the opposite cud of the order’ spectrum: in a crystalline material the atoms are arravged in an orderly three-dimensional array. Given any section of a eeystallioe na tertal. one can readily reprodoee the atomic arrangement in awe other section of Ihe mote rial. Poterystalline solids comprise ae intermediate ease io svhich the solid is coviposed of crystallisse sebsections that me disjointed or misorieoled relative to one another. Upon esaniiiiing the mossy solid store devices io existence, one readily finds euamvtes of of three structural foress. An antorphoos-Si thin-flint seaesissor is ased as the ssvirehing element in liquid crystal disgtcys )LCDs): polycrystattiae Si gates are employed in Metal Gside-Sessucondsrcsor Field-Effect Traosistors tlstGSFETsi. In rhe vast ntajorits of de vices, hosvever, the active region of he device is siteared svithin a crystalline semi condarsoc The ovemarhelmiog netober of devices fabricated soitay employ riyatu)Iisrc semicondactors. 1.2.1 The Unit Cell Concept Simply stated, a unit cell is a small portion of any givers crystal that could be used to reprodoce the crystal. To help establish the null cell (or building-block) concept, let an consider ihe two-disoerssional lattice shosvn is Fig. l.2(a). To describe this lattice or to totally specify the physical ehuracteristies of the lattice, oue need ooly provide the unit cell shown in Pig. 1.2(b), As indicated in Pig. l.2(r), she original lattice can be readily repro duced by merely dophieatmcg the unit cell and siuckiog the doptieares next io each other in uo orderly fashion. In dealing wish unit cells there often arises a misunderstundieg, and hence confesion, relative to two points. Psrsr, evil cells are uos necessarily anique. The unit cell shown in Pig. 1.2(d) ss as aceeplable as the Pig. 1.2(b) unil cell for specifying the original lattice of 00000 00000 00000 ‘0 0 0 Q aIco 0 0 0 lot d/5mes 000 1.2 CRYSTAL STRUCTURE Tire disessssion at the end of she preceding seetiou leads nicely iuro the topic of this section. Strive sri-use semiconductors are typically erystalliue in form, it seems reasonable to seek oar additional inforthotion absmot the crystalline state. Gor nsojor gout here is to present more detailed picture of the atomic arrangement within the principal semiconsteetors. To ibl Id lal 1.2 Introdsermon me he unit cell meshed uf describing umomic arrungemeems within crystals (a) Sampto iwo-dmmssensmunul lattice. (b) Gob cell corrospnnmding In she gwt (a) laltice. (ci Reprndac nor: of mIre origioot bruce. (d) As alseruasiso unit cell. Figure 7 Table 1.1 SEMICONDUCTORS: A GENERAL INTRODUCTION Scirricoirductor Materials. SriiiirO5ieta’t0r l’iciieral Classification I I I Eleroental Synthol Nsssne Si GC Silicon Germaniani Table 1.2 II 5 Abhrevialed Periodic Chart of the Elemenrs. II Ill IV VI V (2) Compounds (a) IV-1V SiC Silicon caibide )b) Ill—V AlP AlAs AlSb GaN GaP GaAs GaSh loP InAs InSli Aleiiiinnns phosphide Alaniiitam arsenidC Atanriourn aotinsonidr Gallinos mir.de Gallium phosphide Gallinur arsenide Gallisno aotimonide ludisnr shospliide Indium arsenide Indian: aetesronide Il-VI ZsG ZeS ZnSe ZnTe CdS CdSe CdTe 1-IgS Zinc oxide PbS PbSe PbTe Lead sulfide Lead seleoide Load ielleride )c) Id) IV-VI Zinc sulfide Zinc selenide Zioc nellaride Cadoiinos salfide Cadmiurss seleiside Cadmium telloride Mercory sulfide Colamn IV. The Column Ill clesneur Ga plus the Cotame V elemeet As yields the Ill-V compouod semicoudactor GaAs; the Column II element Zn pIes ihe Cotamn VI elnisrcol Se yields the Il-Vt compoand sennscooductorZnSe; the fractional combination of the Cot ansu Ill elneneots Al arid Go plsis time Colusoo V element As yields the alloy semivondnrror Al, Ga ,As. This very general property is related to the chemical bouding in semicoedne tors, mherc, on tIre average. Ilseve ore four valence electroos per atom. — 1.1.2 Purity As mill be euplained in Chapter 2. extremely minate traces of imporily atoms catted “dopanrs” can have a drastic effect on the electrical properties of semiconductors. For this reason, the compositional parity of semiconductors nsust he very carefully controlled and, in fact, modere seroicondociors are some of the pnrest solid materials in existence In Sr. for esampte, the nuinrenisonal content of depart atoms is rondnely less than one atom per try Si atoms. To assist the reader in attempting to eusoprehend this incredible level of parity, let us suppose a forest of niaple trees mas planted frons coast to coast, border to border, at 50-fr centers across the United States (including Alaska). Ao imparity level of one pm’r pnr I0 mould vocresporsd to hnding ahoat 25 crabapple trees iu the maple tree formt covering the United Sroresl Jr shonld he emphasieed that the cited material parity refers to nesinrenriorrat undesired impurities. Typically, dopavi atomos at levels ranging from musely added 5 one part per I0 to one impnrily alerts per try semiconductor atoms svill be pmnr so the semiconductor to control Is electrical properties. (3) Alloys (a) Binary Si ,,Ge, (b) Ternary Al,Ga _,As. 1 ,As Al,1o — Cd..,Mn,Te GaAs_,P, Ga, ln ,As Ga,le_,P ,Cd,Te 1 Hg — )e) Qaalernary (or Ga_, Al, As) (at Ini Al,As) - (or In ,Ga, As) .,Ga,P) 1 )arIn . 1 —n 1 _As Sb kl,Ga 1 I As Ga In www.EasyEngineering.net 6 neeieoNnsc’rOR FaNoaMreeAt.u — , nEMIC0NDnCTGRS A GENERAL nsnRonucnsoN achieve thin goal, sec first examine how one goes about describing the spatial position ing of atoms within crystals. Nest, a bit of “visualiearion” practice wills simple three dimensional lattices (atomic arrangements) is presented prior to examining semieoodoetor lattices themselves. The section coucledes with an introduction to the related topic of Mil ler indices. Miller indices are a convenient shorthand notosion widely employed for iden tifying specific planes and diteclious within crystals. lot Aemosrusoas 151 tnt vssnsssOmor Comnpiemeiy esdsmsd mr seemenis 0 recounisahie v iunu’sanee osaer ww w IsI CsysmeOuee Eemmme mesa is mode aver slums is en erdemir smmsv Figare 1.1 General elassihcauao of solids based an rho darrea af atomic ordev (a) amorphaas, (hI polycrysratlise, and (el cryssallinc. 1.1.3 Structure .Ea syE The spatial arrangement of atoms mithso a snuteriol plays an important role in determining the precise properties nf the material. As shomn schemsiatically in Pig. 1.1. the atomic ar rangement withnn a solid cannes is to he placed into one of three broad elmsiflcatinns; naosely. omoephons, polycrvstalline. nr erystullose. Aa amorphous solid is a material in which there is no recagnieahle long-range order in the positioning of atoms within the material. The atomic arrangemeot in any given section of an amoenhoas material mill look differeot from the atomic arrangemees in any oilier section of the material. Crystatlioe solids lie at the opposite cud of the order’ spectrum: in a crystalline material the atoms are arravged in an orderly three-dimensional array. Given any section of a eeystallioe na tertal. one can readily reprodoee the atomic arrangement in awe other section of Ihe mote rial. Poterystalline solids comprise ae intermediate ease io svhich the solid is coviposed of crystallisse sebsections that me disjointed or misorieoled relative to one another. Upon esaniiiiing the mossy solid store devices io existence, one readily finds euamvtes of of three structural foress. An antorphoos-Si thin-flint seaesissor is ased as the ssvirehing element in liquid crystal disgtcys )LCDs): polycrystattiae Si gates are employed in Metal Gside-Sessucondsrcsor Field-Effect Traosistors tlstGSFETsi. In rhe vast ntajorits of de vices, hosvever, the active region of he device is siteared svithin a crystalline semi condarsoc The ovemarhelmiog netober of devices fabricated soitay employ riyatu)Iisrc semicondactors. ngi 1.2.1 The Unit Cell Concept Simply stated, a unit cell is a small portion of any givers crystal that could be used to reprodoce the crystal. To help establish the null cell (or building-block) concept, let an consider ihe two-disoerssional lattice shosvn is Fig. l.2(a). To describe this lattice or to totally specify the physical ehuracteristies of the lattice, oue need ooly provide the unit cell shown in Pig. 1.2(b), As indicated in Pig. l.2(r), she original lattice can be readily repro duced by merely dophieatmcg the unit cell and siuckiog the doptieares next io each other in uo orderly fashion. In dealing wish unit cells there often arises a misunderstundieg, and hence confesion, relative to two points. Psrsr, evil cells are uos necessarily anique. The unit cell shown in Pig. 1.2(d) ss as aceeplable as the Pig. 1.2(b) unil cell for specifying the original lattice of nee rin g 00000 00000 00000 ‘0 0 0 Q aIco 0 0 0 .ne t lot ibl d/5mes 000 1.2 CRYSTAL STRUCTURE Tire disessssion at the end of she preceding seetiou leads nicely iuro the topic of this section. Strive sri-use semiconductors are typically erystalliue in form, it seems reasonable to seek oar additional inforthotion absmot the crystalline state. Gor nsojor gout here is to present more detailed picture of the atomic arrangement within the principal semiconsteetors. To www.EasyEngineering.net Id lal 1.2 Introdsermon me he unit cell meshed uf describing umomic arrungemeems within crystals (a) Sampto iwo-dmmssensmunul lattice. (b) Gob cell corrospnnmding In she gwt (a) laltice. (ci Reprndac nor: of mIre origioot bruce. (d) As alseruasiso unit cell. Figure 7 Table 1.1 SriiiirO5ieta’t0r l’iciieral Classification I I I Eleroental 5 SEMICONDUCTORS: A GENERAL INTRODUCTION Scirricoirductor Materials. Synthol Nsssne Si GC Silicon Germaniani Table 1.2 II Abhrevialed Periodic Chart of the Elemenrs. II IV Ill VI V (2) Compounds (a) IV-1V SiC Silicon caibide )b) Ill—V AlP AlAs AlSb GaN GaP GaAs GaSh loP InAs InSli Aleiiiinnns phosphide Alaniiitam arsenidC Atanriourn aotinsonidr Gallinos mir.de Gallium phosphide Gallinur arsenide Gallisno aotimonide ludisnr shospliide Indium arsenide Indian: aetesronide Il-VI ZsG ZeS ZnSe ZnTe CdS CdSe CdTe 1-IgS Zinc oxide PbS PbSe PbTe Lead sulfide Lead seleoide Load ielleride )c) Id) IV-VI Zinc sulfide Zinc selenide Zioc nellaride Cadoiinos salfide Cadmiurss seleiside Cadmium telloride Mercory sulfide (3) Alloys (a) Binary Si ,,Ge, (b) Ternary Al,Ga _,As. 1 ,As Al,1o — Cd..,Mn,Te GaAs_,P, Ga, ln ,As Ga,le_,P ,Cd,Te 1 Hg — )e) Qaalernary (or Ga_, Al, As) (at Ini Al,As) - (or In ,Ga, As) .,Ga,P) 1 )arIn . 1 —n 1 _As Sb kl,Ga 1 I As Ga In Colamn IV. The Column Ill clesneur Ga plus the Cotame V elemeet As yields the Ill-V compouod semicoudactor GaAs; the Column II element Zn pIes ihe Cotamn VI elnisrcol Se yields the Il-Vt compoand sennscooductorZnSe; the fractional combination of the Cot ansu Ill elneneots Al arid Go plsis time Colusoo V element As yields the alloy semivondnrror Al, Ga ,As. This very general property is related to the chemical bouding in semicoedne tors, mherc, on tIre average. Ilseve ore four valence electroos per atom. — 1.1.2 Purity As mill be euplained in Chapter 2. extremely minate traces of imporily atoms catted “dopanrs” can have a drastic effect on the electrical properties of semiconductors. For this reason, the compositional parity of semiconductors nsust he very carefully controlled and, in fact, modere seroicondociors are some of the pnrest solid materials in existence In Sr. for esampte, the nuinrenisonal content of depart atoms is rondnely less than one atom per try Si atoms. To assist the reader in attempting to eusoprehend this incredible level of parity, let us suppose a forest of niaple trees mas planted frons coast to coast, border to border, at 50-fr centers across the United States (including Alaska). Ao imparity level of one pm’r pnr I0 mould vocresporsd to hnding ahoat 25 crabapple trees iu the maple tree formt covering the United Sroresl Jr shonld he emphasieed that the cited material parity refers to nesinrenriorrat undesired impurities. Typically, dopavi atomos at levels ranging from musely added 5 one part per I0 to one impnrily alerts per try semiconductor atoms svill be pmnr so the semiconductor to control Is electrical properties. www.EasyEngineering.net 6 neeieoNnsc’rOR FaNoaMreeAt.u — nEMIC0NDnCTGRS A GENERAL nsnRonucnsoN , 7 achieve thin goal, sec first examine how one goes about describing the spatial position ing of atoms within crystals. Nest, a bit of “visualiearion” practice wills simple three dimensional lattices (atomic arrangements) is presented prior to examining semieoodoetor lattices themselves. The section coucledes with an introduction to the related topic of Mil ler indices. Miller indices are a convenient shorthand notosion widely employed for iden tifying specific planes and diteclious within crystals. lot Aemosrusoas 0 recounisahie v iunu’sanee osaer 151 tnt vssnsssOmor Comnpiemeiy esdsmsd mr seemenis IsI CsysmeOuee Eemmme mesa is mode aver slums is en erdemir smmsv Figare 1.1 General elassihcauao of solids based an rho darrea af atomic ordev (a) amorphaas, (hI polycrysratlise, and (el cryssallinc. 1.1.3 Structure The spatial arrangement of atoms mithso a snuteriol plays an important role in determining the precise properties nf the material. As shomn schemsiatically in Pig. 1.1. the atomic ar rangement withnn a solid cannes is to he placed into one of three broad elmsiflcatinns; naosely. omoephons, polycrvstalline. nr erystullose. Aa amorphous solid is a material in which there is no recagnieahle long-range order in the positioning of atoms within the material. The atomic arrangemeot in any given section of an amoenhoas material mill look differeot from the atomic arrangemees in any oilier section of the material. Crystatlioe solids lie at the opposite cud of the order’ spectrum: in a crystalline material the atoms are arravged in an orderly three-dimensional array. Given any section of a eeystallioe na tertal. one can readily reprodoee the atomic arrangement in awe other section of Ihe mote rial. Poterystalline solids comprise ae intermediate ease io svhich the solid is coviposed of crystallisse sebsections that me disjointed or misorieoled relative to one another. Upon esaniiiiing the mossy solid store devices io existence, one readily finds euamvtes of of three structural foress. An antorphoos-Si thin-flint seaesissor is ased as the ssvirehing element in liquid crystal disgtcys )LCDs): polycrystattiae Si gates are employed in Metal Gside-Sessucondsrcsor Field-Effect Traosistors tlstGSFETsi. In rhe vast ntajorits of de vices, hosvever, the active region of he device is siteared svithin a crystalline semi condarsoc The ovemarhelmiog netober of devices fabricated soitay employ riyatu)Iisrc semicondactors. 1.2.1 The Unit Cell Concept Simply stated, a unit cell is a small portion of any givers crystal that could be used to reprodoce the crystal. To help establish the null cell (or building-block) concept, let an consider ihe two-disoerssional lattice shosvn is Fig. l.2(a). To describe this lattice or to totally specify the physical ehuracteristies of the lattice, oue need ooly provide the unit cell shown in Pig. 1.2(b), As indicated in Pig. l.2(r), she original lattice can be readily repro duced by merely dophieatmcg the unit cell and siuckiog the doptieares next io each other in uo orderly fashion. In dealing wish unit cells there often arises a misunderstundieg, and hence confesion, relative to two points. Psrsr, evil cells are uos necessarily anique. The unit cell shown in Pig. 1.2(d) ss as aceeplable as the Pig. 1.2(b) unil cell for specifying the original lattice of ww w.E En 00000 00000 00000 ‘0 0 0 Q aIco 0 0 0 lot gin eer ing ibl .ne d/5mes 000 1.2 CRYSTAL STRUCTURE Tire disessssion at the end of she preceding seetiou leads nicely iuro the topic of this section. Strive sri-use semiconductors are typically erystalliue in form, it seems reasonable to seek oar additional inforthotion absmot the crystalline state. Gor nsojor gout here is to present more detailed picture of the atomic arrangement within the principal semiconsteetors. To asy Id lal 1.2 Introdsermon me he unit cell meshed uf describing umomic arrungemeems within crystals (a) Sampto iwo-dmmssensmunul lattice. (b) Gob cell corrospnnmding In she gwt (a) laltice. (ci Reprndac nor: of mIre origioot bruce. (d) As alseruasiso unit cell. Figure www.EasyEngineering.net t www.EasyEngineering.net 8 SEMICONDUCTOR FUNDAMENTALS SEMICONDUCTORS: A GENERAL INTRODUCTION Pig. .2(n). Second. a unit ccli need not be prinsitise (the smallest unit cell possible). In fact, II is usually odnautageons to employ n slightly larger Unit cell with arthngnual sides instead of Opt iitiitive ccli with nonerrhosmial sides. This is especially rcoe in three dinien— siotis where nencobic Unit cells are quite difhcult In describe and nisnalice. ‘siion, u. Wheo siemed ounniul In the base plane. atoms in u given piano ure pnsitioued directly acer atoms in a tcwer-lyiug platte. Pigutus t.3(c( arid I 3(4) display lice cononon 3-0 celts that nrc suniewhut inure coinpies bol still closely related to the sitnple cube cell i’be onir cell of Pig. 1.3(c) bus an atom added at the centeu of the cube; this cunfigonutinu ii upprupriutely cuflrd the body centered cubic (bee) unit cell. The face centered cubic (fcc) unit cell of Pig. 1.3(d) contuios on ulnm at each face of tire cube in udditiou to the atoms ai cacti cornec. (Note. linwecer. ihut wily one-half uf each focn abut aetnatty lies inside the fcc unit ccli.) Whereas the simnple cubic cotl coutuitis cite .itnus (1/8 nf an ulnm at cuch of tire eight cube cornrrsl, tire suiocmltat cure cumplec bce and (cc cello enoruin Iwo and four atoms, respecticely. ike reader should cerify these facts and cisootice the luttices associated ssirhi the bce and fcc cells. 1.2.2 Simple 3-C Unit Cells Setincnoduclnrcey)tals Are ihree-diineesinnnl and are tlieeefnre cthscribed in ternis of thcee diosensinnul (3D) unit cells. In Pig. 1.3(a) we linne pictured die simplest af all three dinietisinnal nttit cells, the sitnpte enbic nnit cell. The simple cubic cell is an equal-sided hon or cnbc mitts ott stein pnsitinned at cacti cncner of ibe cube. The simple cubic lattice asseciated with thin cell is constrncted it u maCncr paralleling rIte two-diniensiunal case. In dning so. Irumeser, it should be noted thai nitty 118 of cccli canter alum 5 acaialty inside the cetl, us pictured io Fig. l.3(hl. Dupliculing the Pig. l.3(bl cell oud stacking the dopli eaten like blocks in n nncsery yields t se simple cubic luaice. Specifically, the prnccdnte generates planes nf atoms like that preciously sliowu itt Pig. 1.2(a). Planes ef atoms parultel In rite base plane are separated from one anuilter by U unit cell side leitgtlr or lattice curt ww (C) Exercine 1.1 w.E as y En gin e The test-associated softscare distribslesh cur tire lrtteeuet or on floppy disk u contains o directory Ar folder named MacMolecule. Files stored inside this directory or folder are ASCII inpul files generated by tire audmer (hr use with a computer pregront by the Sante name. Time MacMolecsmte progrcm. copyriglrled by the Unisemily of Aricona, is dmstnihnred free of charge to ocodenric users and in ovoiloble at many academic sites. As tIm ueme implies, the program runs etmly on Macintosh personal conipoters. Thu input files supplied to IRM-compotiblu users, however, cumt be readily concerted for use ant a public-access Macirmtcmshm. MacMolecule geocralos and dmspluys u “boti-arrd-stick” 3-0 color rendering of molecules. unit cells, and tatrices. The immpnt files supplied by the uuthuu can be used to help cisrialice tIre simple enbie, bee, and (cc uttit cells, plus the diamond ond aloe blende unit cells described in rite nest subsection. The About-MacMolecule file thot is distributed wilh the MacMolecule program prosides detnihed iuformation about Ihe use of the program and the gencrariomm)roodifieatioms of input files. The rnadcr is urged to iorestigote and play suith the MucMolecule saftwure, The initiul display is olssays a c-directior viem and in typically pneodo-two-dimensional eri (a) Simmmplu cobic 9 ng. ne (b) Podauticully cowed simple cubic t in nature. A moore informative ciem is obtained by rotntirlg the model. Rutctioo is best ucconmptithed by “grahbiog and dragging” the edges of the model. The morn adxen turesonme may wish In Icy their humid ut modiiog Ihe esistiog input files or generat ing ness input ftles. 1.2.3 Semiconductor Lattices (ci buc (dl fcc Figuru 1.3 Simple ihruc.dioiensionul urn cells. lal Siinplu cAine uuh colt. Ib) Pudunticulty correct simple cubic anh ccli iuctoding only the fraetiunul pustiun 11181 of ouch ecrune Atom actually mitten the cull cube. (ci Budy ceusused cubic unit cetl. (dl Puce centered cubic unit cult. We are finally in u position to supply deroils relulise to the positioning of utoms scithin the priociput semiconductors. In Si (and Ge) the lotlice structure is described by the omit cell pictured iu Pig. 1.4(u). The Pig. 1.4(u) arrangement is kucwn as the dininaird loltice onit cell because it also chorucrerlees diamond, o form of the Column IV element corbon. Ru umining the diumoud lattice unit cell. we ode thur the cell is cubic, with atoms ut each www.EasyEngineering.net Ill SEMICONDUCTOR PUNnAMEIeraLU SEMICONDUCTORS: A GENERAL INTRuOuCTION — lob 11 holly identicnd to the diumond lattice. eneept thur lorries sites ore apportioned eqoolly be tween two diffemnt uhoms. Go uccopius sites on one of the two intecpenetrut ing fcc sublurtices; arsenic (As) populates Ihe other fcc subluttice. Now thut the poniliuning of atoms snithin the principal semicondoclom has been esrnh lished, the question moy arise us to the pructicul nlilicotion of such teformutron. Allhnugh seserol upplicotions could he cited, geometticul-lype coicolutiuns constitute a very cam moo oud readily esplained one of the unit cell !ormalism. Par esomple, in Si 01 cnom rem perutnre the unit cell side length (a) is 5.43 A (where I A = 10 -n cm). Since thore ore eight Si ntoms per unit cell und the solume of the unit cell is o. it follosss that there urn 5 at ulmost ecuclly 5 on l0°° utums/em 8/a t in the Si lattice. Similnr coiculutions could be performed to determine olomic radii, the dislunce between uromic plnnen, nnd so forth. Por the purposeo of the development herein, howeser, a mojur reason for the discassiou of semiconductor luttices wus to esroblish thor, as emphosieed In Fig. 1.4(c), atoms in the diamond and cinchiende lonicec hare four nearest neighburo. The chemicnl bonding (or cryntolline glue) within Ike major semiconductors is therefore dnminolcd by the ottroction kctweeo any gioen alum and its four closest neighbors. This is on itnpoetout fuel thot should be filed owoy foe futore reference. tbl Exercise 1.2 id Figure 1.4 (u) Diamond lattice unit coil. thi Ziucbtnudc loif en unit cell (GuAs used fur illustie oo:il. id P.ulsigcd top cornc 01 ihe putt la) diamond luttice etnphuoiciug thu funn.nrmmr-nuighbus bonding icithin ihu stroennue. Thu cube side length. u, is 5.43 A and 5.b5 A At T = 308 K hr Si und , Gififit by John Wiley & Sans, 1 GaAs. respeetisety Ilu) .hdopted from Shockleyci. (hi From gent Inc. Reprinted wiilli pesmissior.( — F: If thu lattice coosnuc or unit cell side-lrngflt in Si is a = 5.43 on I0 cm, whal in the dislunce (d) from the center of one Si olom to thn center of lhs nearest ueighboc7 St As noted ic thn Pig. 1.4 caption, the atom in the upper front cornier of the Si 001; cell and the otom olong the enbe diogonal one-(ouehh of the moy down the diogonol ore nearest neighbors. Since hhn diugonol of u cube /. corner and oh mmli face of the cube sitnilac to Ike fcc cell. The interior of tkc Pig. 1.4(u) cell. howeser. contains four additional atotos. One of [he interior crams is Iccared along a coke body diagonal exactly one-quarter of the wAy dawn the diogocal (cots the top (coot lefI-hund corner of the cnbe. The other three inlcrior atoms ace displaced ene-qnortcr of [lie body diagoool length along the previously noted body diagonal direction from the (runt, rap, and left-side face atoms, respectively. Altltoogli iI may be difficolt In visoaliee frnnt Pig. 1.4(o), the diamond lattice can also be described us corking osore thun 1550 interpene tailing fcc lattices. The corner and face otoirss of the auit cell con be viesced us belonging to one fcc lattice, while the arotes ioiully contained wtthin the cell belong to the second (cc lattice. The second lottice is disaloced one-quarter of a body diogonol along a bridy diogo nal direction relative to the first fcc lattice. Most of the UI-V semicoudoclais, imrcluding GaAs, ceyslallice in the chicblende struc ture. The cinchlende lattice, typified by the GoAs oisit cell shown in Pig. 1.4(b), is essec (C) Exeroine 1.3 Pt Construct o MATLAO program Ihul computes the oombnc of 5 atoms/cm in cubic crystals. Use the MATLAn lapse fnnctian to cuter the number of atoms/unit-cell and the unit cell side length (n) (era specific crystal. Moke a listing of your program ond record the progrcm ressll schen applied to silicott. 5: MATLAn prngcam script... %Rcercise 1.3 FeComputotian of the number of utoms/cm3 in o cubic lattice N =input(’inpol nnmber of uicms/nml cell, N = u=inpot(’Iutticnconclamtt in oogsteont, 0 = ( 1.0e24)/(o”3) Feanmber of atoms/emS 5 otmdcnN www.EasyEngineering.net 8 SEMICONDUCTOR FUNDAMENTALS SEMICONDUCTORS: A GENERAL INTRODUCTION Pig. .2(n). Second. a unit ccli need not be prinsitise (the smallest unit cell possible). In fact, II is usually odnautageons to employ n slightly larger Unit cell with arthngnual sides instead of Opt iitiitive ccli with nonerrhosmial sides. This is especially rcoe in three dinien— siotis where nencobic Unit cells are quite difhcult In describe and nisnalice. ‘siion, u. Wheo siemed ounniul In the base plane. atoms in u given piano ure pnsitioued directly acer atoms in a tcwer-lyiug platte. Pigutus t.3(c( arid I 3(4) display lice cononon 3-0 celts that nrc suniewhut inure coinpies bol still closely related to the sitnple cube cell i’be onir cell of Pig. 1.3(c) bus an atom added at the centeu of the cube; this cunfigonutinu ii upprupriutely cuflrd the body centered cubic (bee) unit cell. The face centered cubic (fcc) unit cell of Pig. 1.3(d) contuios on ulnm at each face of tire cube in udditiou to the atoms ai cacti cornec. (Note. linwecer. ihut wily one-half uf each focn abut aetnatty lies inside the fcc unit ccli.) Whereas the simnple cubic cotl coutuitis cite .itnus (1/8 nf an ulnm at cuch of tire eight cube cornrrsl, tire suiocmltat cure cumplec bce and (cc cello enoruin Iwo and four atoms, respecticely. ike reader should cerify these facts and cisootice the luttices associated ssirhi the bce and fcc cells. 1.2.2 Simple 3-C Unit Cells Setincnoduclnrcey)tals Are ihree-diineesinnnl and are tlieeefnre cthscribed in ternis of thcee diosensinnul (3D) unit cells. In Pig. 1.3(a) we linne pictured die simplest af all three dinietisinnal nttit cells, the sitnpte enbic nnit cell. The simple cubic cell is an equal-sided hon or cnbc mitts ott stein pnsitinned at cacti cncner of ibe cube. The simple cubic lattice asseciated with thin cell is constrncted it u maCncr paralleling rIte two-diniensiunal case. In dning so. Irumeser, it should be noted thai nitty 118 of cccli canter alum 5 acaialty inside the cetl, us pictured io Fig. l.3(hl. Dupliculing the Pig. l.3(bl cell oud stacking the dopli eaten like blocks in n nncsery yields t se simple cubic luaice. Specifically, the prnccdnte generates planes nf atoms like that preciously sliowu itt Pig. 1.2(a). Planes ef atoms parultel In rite base plane are separated from one anuilter by U unit cell side leitgtlr or lattice curt 9 ww (C) Exercine 1.1 w.E a The test-associated softscare distribslesh cur tire lrtteeuet or on floppy disk u contains o directory Ar folder named MacMolecule. Files stored inside this directory or folder are ASCII inpul files generated by tire audmer (hr use with a computer pregront by the Sante name. Time MacMolecsmte progrcm. copyriglrled by the Unisemily of Aricona, syE ngi is dmstnihnred free of charge to ocodenric users and in ovoiloble at many academic sites. As tIm ueme implies, the program runs etmly on Macintosh personal conipoters. Thu input files supplied to IRM-compotiblu users, however, cumt be readily concerted (a) Simmmplu cobic for use ant a public-access Macirmtcmshm. MacMolecule geocralos and dmspluys u “boti-arrd-stick” 3-0 color rendering of molecules. unit cells, and tatrices. The immpnt files supplied by the uuthuu can be used to help cisrialice tIre simple enbie, bee, and (cc uttit cells, plus the diamond ond aloe blende unit cells described in rite nest subsection. The About-MacMolecule file thot is distributed wilh the MacMolecule program prosides detnihed iuformation about Ihe use of the program and the gencrariomm)roodifieatioms of input files. The rnadcr is urged to iorestigote and play suith the MucMolecule saftwure, The initiul display is olssays a c-directior viem and in typically pneodo-two-dimensional nee r ing . (b) Podauticully cowed simple cubic net in nature. A moore informative ciem is obtained by rotntirlg the model. Rutctioo is best ucconmptithed by “grahbiog and dragging” the edges of the model. The morn adxen turesonme may wish In Icy their humid ut modiiog Ihe esistiog input files or generat ing ness input ftles. 1.2.3 Semiconductor Lattices (ci buc (dl fcc Figuru 1.3 Simple ihruc.dioiensionul urn cells. lal Siinplu cAine uuh colt. Ib) Pudunticulty correct simple cubic anh ccli iuctoding only the fraetiunul pustiun 11181 of ouch ecrune Atom actually mitten the cull cube. (ci Budy ceusused cubic unit cetl. (dl Puce centered cubic unit cult. We are finally in u position to supply deroils relulise to the positioning of utoms scithin the priociput semiconductors. In Si (and Ge) the lotlice structure is described by the omit cell pictured iu Pig. 1.4(u). The Pig. 1.4(u) arrangement is kucwn as the dininaird loltice onit cell because it also chorucrerlees diamond, o form of the Column IV element corbon. Ru umining the diumoud lattice unit cell. we ode thur the cell is cubic, with atoms ut each www.EasyEngineering.net Ill SEMICONDUCTOR PUNnAMEIeraLU SEMICONDUCTORS: A GENERAL INTRuOuCTION — lob 11 holly identicnd to the diumond lattice. eneept thur lorries sites ore apportioned eqoolly be tween two diffemnt uhoms. Go uccopius sites on one of the two intecpenetrut ing fcc sublurtices; arsenic (As) populates Ihe other fcc subluttice. Now thut the poniliuning of atoms snithin the principal semicondoclom has been esrnh lished, the question moy arise us to the pructicul nlilicotion of such teformutron. Allhnugh seserol upplicotions could he cited, geometticul-lype coicolutiuns constitute a very cam moo oud readily esplained one of the unit cell !ormalism. Par esomple, in Si 01 cnom rem perutnre the unit cell side length (a) is 5.43 A (where I A = 10 -n cm). Since thore ore eight Si ntoms per unit cell und the solume of the unit cell is o. it follosss that there urn 5 at ulmost ecuclly 5 on l0°° utums/em 8/a t in the Si lattice. Similnr coiculutions could be performed to determine olomic radii, the dislunce between uromic plnnen, nnd so forth. Por the purposeo of the development herein, howeser, a mojur reason for the discassiou of semiconductor luttices wus to esroblish thor, as emphosieed In Fig. 1.4(c), atoms in the diamond and cinchiende lonicec hare four nearest neighburo. The chemicnl bonding (or cryntolline glue) within Ike major semiconductors is therefore dnminolcd by the ottroction kctweeo any gioen alum and its four closest neighbors. This is on itnpoetout fuel thot should be filed owoy foe futore reference. tbl Exercise 1.2 id Figure 1.4 (u) Diamond lattice unit coil. thi Ziucbtnudc loif en unit cell (GuAs used fur illustie oo:il. id P.ulsigcd top cornc 01 ihe putt la) diamond luttice etnphuoiciug thu funn.nrmmr-nuighbus bonding icithin ihu stroennue. Thu cube side length. u, is 5.43 A and 5.b5 A At T = 308 K hr Si und , Gififit by John Wiley & Sans, 1 GaAs. respeetisety Ilu) .hdopted from Shockleyci. (hi From gent Inc. Reprinted wiilli pesmissior.( — F: If thu lattice coosnuc or unit cell side-lrngflt in Si is a = 5.43 on I0 cm, whal in the dislunce (d) from the center of one Si olom to thn center of lhs nearest ueighboc7 St As noted ic thn Pig. 1.4 caption, the atom in the upper front cornier of the Si 001; cell and the otom olong the enbe diogonal one-(ouehh of the moy down the diogonol ore nearest neighbors. Since hhn diugonol of u cube /. corner and oh mmli face of the cube sitnilac to Ike fcc cell. The interior of tkc Pig. 1.4(u) cell. howeser. contains four additional atotos. One of [he interior crams is Iccared along a coke body diagonal exactly one-quarter of the wAy dawn the diogocal (cots the top (coot lefI-hund corner of the cnbe. The other three inlcrior atoms ace displaced ene-qnortcr of [lie body diagoool length along the previously noted body diagonal direction from the (runt, rap, and left-side face atoms, respectively. Altltoogli iI may be difficolt In visoaliee frnnt Pig. 1.4(o), the diamond lattice can also be described us corking osore thun 1550 interpene tailing fcc lattices. The corner and face otoirss of the auit cell con be viesced us belonging to one fcc lattice, while the arotes ioiully contained wtthin the cell belong to the second (cc lattice. The second lottice is disaloced one-quarter of a body diogonol along a bridy diogo nal direction relative to the first fcc lattice. Most of the UI-V semicoudoclais, imrcluding GaAs, ceyslallice in the chicblende struc ture. The cinchlende lattice, typified by the GoAs oisit cell shown in Pig. 1.4(b), is essec (C) Exeroine 1.3 Pt Construct o MATLAO program Ihul computes the oombnc of 5 atoms/cm in cubic crystals. Use the MATLAn lapse fnnctian to cuter the number of atoms/unit-cell and the unit cell side length (n) (era specific crystal. Moke a listing of your program ond record the progrcm ressll schen applied to silicott. 5: MATLAn prngcam script... %Rcercise 1.3 FeComputotian of the number of utoms/cm3 in o cubic lattice N =input(’inpol nnmber of uicms/nml cell, N = u=inpot(’Iutticnconclamtt in oogsteont, 0 = ( 1.0e24)/(o”3) Feanmber of atoms/emS 5 otmdcnN 8 SEMICONDUCTOR FUNDAMENTALS SEMICONDUCTORS: A GENERAL INTRODUCTION Pig. .2(n). Second. a unit ccli need not be prinsitise (the smallest unit cell possible). In fact, II is usually odnautageons to employ n slightly larger Unit cell with arthngnual sides instead of Opt iitiitive ccli with nonerrhosmial sides. This is especially rcoe in three dinien— siotis where nencobic Unit cells are quite difhcult In describe and nisnalice. ‘siion, u. Wheo siemed ounniul In the base plane. atoms in u given piano ure pnsitioued directly acer atoms in a tcwer-lyiug platte. Pigutus t.3(c( arid I 3(4) display lice cononon 3-0 celts that nrc suniewhut inure coinpies bol still closely related to the sitnple cube cell i’be onir cell of Pig. 1.3(c) bus an atom added at the centeu of the cube; this cunfigonutinu ii upprupriutely cuflrd the body centered cubic (bee) unit cell. The face centered cubic (fcc) unit cell of Pig. 1.3(d) contuios on ulnm at each face of tire cube in udditiou to the atoms ai cacti cornec. (Note. linwecer. ihut wily one-half uf each focn abut aetnatty lies inside the fcc unit ccli.) Whereas the simnple cubic cotl coutuitis cite .itnus (1/8 nf an ulnm at cuch of tire eight cube cornrrsl, tire suiocmltat cure cumplec bce and (cc cello enoruin Iwo and four atoms, respecticely. ike reader should cerify these facts and cisootice the luttices associated ssirhi the bce and fcc cells. 1.2.2 Simple 3-C Unit Cells Setincnoduclnrcey)tals Are 9 ihree-diineesinnnl and are tlieeefnre cthscribed in ternis of thcee diosensinnul (3D) unit cells. In Pig. 1.3(a) we linne pictured die simplest af all three dinietisinnal nttit cells, the sitnpte enbic nnit cell. The simple cubic cell is an equal-sided hon or cnbc mitts ott stein pnsitinned at cacti cncner of ibe cube. The simple cubic lattice asseciated with thin cell is constrncted it u maCncr paralleling rIte two-diniensiunal case. In dning so. Irumeser, it should be noted thai nitty 118 of cccli canter alum 5 acaialty inside the cetl, us pictured io Fig. l.3(hl. Dupliculing the Pig. l.3(bl cell oud stacking the dopli eaten like blocks in n nncsery yields t se simple cubic luaice. Specifically, the prnccdnte generates planes nf atoms like that preciously sliowu itt Pig. 1.2(a). Planes ef atoms parultel In rite base plane are separated from one anuilter by U unit cell side leitgtlr or lattice curt (C) Exercine 1.1 The test-associated softscare distribslesh cur tire lrtteeuet or on floppy disk u contains o directory Ar folder named MacMolecule. Files stored inside this directory or folder are ASCII inpul files generated by tire audmer (hr use with a computer pregront by the Sante name. Time MacMolecsmte progrcm. copyriglrled by the Unisemily of Aricona, is dmstnihnred free of charge to ocodenric users and in ovoiloble at many academic sites. As tIm ueme implies, the program runs etmly on Macintosh personal conipoters. Thu input files supplied to IRM-compotiblu users, however, cumt be readily concerted (a) Simmmplu cobic for use ant a public-access Macirmtcmshm. MacMolecule geocralos and dmspluys u “boti-arrd-stick” 3-0 color rendering of molecules. unit cells, and tatrices. The immpnt files supplied by the uuthuu can be used to help cisrialice tIre simple enbie, bee, and (cc uttit cells, plus the diamond ond aloe blende unit cells described in rite nest subsection. The About-MacMolecule file thot is distributed wilh the MacMolecule program prosides detnihed iuformation about Ihe use of the program and the gencrariomm)roodifieatioms of input files. The rnadcr is urged to iorestigote and play suith the MucMolecule saftwure, The initiul display is olssays a c-directior viem and in typically pneodo-two-dimensional (b) Podauticully cowed simple cubic in nature. A moore informative ciem is obtained by rotntirlg the model. Rutctioo is best ucconmptithed by “grahbiog and dragging” the edges of the model. The morn adxen turesonme may wish In Icy their humid ut modiiog Ihe esistiog input files or generat ing ness input ftles. 1.2.3 Semiconductor Lattices (ci buc (dl fcc Figuru 1.3 Simple ihruc.dioiensionul urn cells. lal Siinplu cAine uuh colt. Ib) Pudunticulty correct simple cubic anh ccli iuctoding only the fraetiunul pustiun 11181 of ouch ecrune Atom actually mitten the cull cube. (ci Budy ceusused cubic unit cetl. (dl Puce centered cubic unit cult. We are finally in u position to supply deroils relulise to the positioning of utoms scithin the priociput semiconductors. In Si (and Ge) the lotlice structure is described by the omit cell pictured iu Pig. 1.4(u). The Pig. 1.4(u) arrangement is kucwn as the dininaird loltice onit cell because it also chorucrerlees diamond, o form of the Column IV element corbon. Ru umining the diumoud lattice unit cell. we ode thur the cell is cubic, with atoms ut each www.EasyEngineering.net Ill SEMICONDUCTOR PUNnAMEIeraLU SEMICONDUCTORS: A GENERAL INTRuOuCTION — lob ww w .Ea syE ngi holly identicnd to the diumond lattice. eneept thur lorries sites ore apportioned eqoolly be tween two diffemnt uhoms. Go uccopius sites on one of the two intecpenetrut ing fcc sublurtices; arsenic (As) populates Ihe other fcc subluttice. Now thut the poniliuning of atoms snithin the principal semicondoclom has been esrnh lished, the question moy arise us to the pructicul nlilicotion of such teformutron. Allhnugh seserol upplicotions could he cited, geometticul-lype coicolutiuns constitute a very cam moo oud readily esplained one of the unit cell !ormalism. Par esomple, in Si 01 cnom rem perutnre the unit cell side length (a) is 5.43 A (where I A = 10 -n cm). Since thore ore eight Si ntoms per unit cell und the solume of the unit cell is o. it follosss that there urn 5 at ulmost ecuclly 5 on l0°° utums/em 8/a t in the Si lattice. Similnr coiculutions could be performed to determine olomic radii, the dislunce between uromic plnnen, nnd so forth. Por the purposeo of the development herein, howeser, a mojur reason for the discassiou of semiconductor luttices wus to esroblish thor, as emphosieed In Fig. 1.4(c), atoms in the diamond and cinchiende lonicec hare four nearest neighburo. The chemicnl bonding (or cryntolline glue) within Ike major semiconductors is therefore dnminolcd by the ottroction kctweeo any gioen alum and its four closest neighbors. This is on itnpoetout fuel thot should be filed owoy foe futore reference. tbl id 11 Exercise 1.2 nee rin g Figure 1.4 (u) Diamond lattice unit coil. thi Ziucbtnudc loif en unit cell (GuAs used fur illustie oo:il. id P.ulsigcd top cornc 01 ihe putt la) diamond luttice etnphuoiciug thu funn.nrmmr-nuighbus bonding icithin ihu stroennue. Thu cube side length. u, is 5.43 A and 5.b5 A At T = 308 K hr Si und , Gififit by John Wiley & Sans, 1 GaAs. respeetisety Ilu) .hdopted from Shockleyci. (hi From gent Inc. Reprinted wiilli pesmissior.( — .ne t corner and oh mmli face of the cube sitnilac to Ike fcc cell. The interior of tkc Pig. 1.4(u) cell. howeser. contains four additional atotos. One of [he interior crams is Iccared along a coke body diagonal exactly one-quarter of the wAy dawn the diogocal (cots the top (coot lefI-hund corner of the cnbe. The other three inlcrior atoms ace displaced ene-qnortcr of [lie body diagoool length along the previously noted body diagonal direction from the (runt, rap, and left-side face atoms, respectively. Altltoogli iI may be difficolt In visoaliee frnnt Pig. 1.4(o), the diamond lattice can also be described us corking osore thun 1550 interpene tailing fcc lattices. The corner and face otoirss of the auit cell con be viesced us belonging to one fcc lattice, while the arotes ioiully contained wtthin the cell belong to the second (cc lattice. The second lottice is disaloced one-quarter of a body diogonol along a bridy diogo nal direction relative to the first fcc lattice. Most of the UI-V semicoudoclais, imrcluding GaAs, ceyslallice in the chicblende struc ture. The cinchlende lattice, typified by the GoAs oisit cell shown in Pig. 1.4(b), is essec www.EasyEngineering.net F: If thu lattice coosnuc or unit cell side-lrngflt in Si is a = 5.43 on I0 cm, whal in the dislunce (d) from the center of one Si olom to thn center of lhs nearest ueighboc7 St As noted ic thn Pig. 1.4 caption, the atom in the upper front cornier of the Si 001; cell and the otom olong the enbe diogonal one-(ouehh of the moy down the diogonol ore nearest neighbors. Since hhn diugonol of u cube /. (C) Exeroine 1.3 Pt Construct o MATLAO program Ihul computes the oombnc of 5 atoms/cm in cubic crystals. Use the MATLAn lapse fnnctian to cuter the number of atoms/unit-cell and the unit cell side length (n) (era specific crystal. Moke a listing of your program ond record the progrcm ressll schen applied to silicott. 5: MATLAn prngcam script... %Rcercise 1.3 FeComputotian of the number of utoms/cm3 in o cubic lattice N =input(’inpol nnmber of uicms/nml cell, N = u=inpot(’Iutticnconclamtt in oogsteont, 0 = ( 1.0e24)/(o”3) Feanmber of atoms/emS 5 otmdcnN 8 SEMICONDUCTOR FUNDAMENTALS SEMICONDUCTORS: A GENERAL INTRODUCTION Pig. .2(n). Second. a unit ccli need not be prinsitise (the smallest unit cell possible). In fact, II is usually odnautageons to employ n slightly larger Unit cell with arthngnual sides instead of Opt iitiitive ccli with nonerrhosmial sides. This is especially rcoe in three dinien— siotis where nencobic Unit cells are quite difhcult In describe and nisnalice. ‘siion, u. Wheo siemed ounniul In the base plane. atoms in u given piano ure pnsitioued directly acer atoms in a tcwer-lyiug platte. Pigutus t.3(c( arid I 3(4) display lice cononon 3-0 celts that nrc suniewhut inure coinpies bol still closely related to the sitnple cube cell i’be onir cell of Pig. 1.3(c) bus an atom added at the centeu of the cube; this cunfigonutinu ii upprupriutely cuflrd the body centered cubic (bee) unit cell. The face centered cubic (fcc) unit cell of Pig. 1.3(d) contuios on ulnm at each face of tire cube in udditiou to the atoms ai cacti cornec. (Note. linwecer. ihut wily one-half uf each focn abut aetnatty lies inside the fcc unit ccli.) Whereas the simnple cubic cotl coutuitis cite .itnus (1/8 nf an ulnm at cuch of tire eight cube cornrrsl, tire suiocmltat cure cumplec bce and (cc cello enoruin Iwo and four atoms, respecticely. ike reader should cerify these facts and cisootice the luttices associated ssirhi the bce and fcc cells. 1.2.2 Simple 3-C Unit Cells Setincnoduclnrcey)tals Are 9 ihree-diineesinnnl and are tlieeefnre cthscribed in ternis of thcee diosensinnul (3D) unit cells. In Pig. 1.3(a) we linne pictured die simplest af all three dinietisinnal nttit cells, the sitnpte enbic nnit cell. The simple cubic cell is an equal-sided hon or cnbc mitts ott stein pnsitinned at cacti cncner of ibe cube. The simple cubic lattice asseciated with thin cell is constrncted it u maCncr paralleling rIte two-diniensiunal case. In dning so. Irumeser, it should be noted thai nitty 118 of cccli canter alum 5 acaialty inside the cetl, us pictured io Fig. l.3(hl. Dupliculing the Pig. l.3(bl cell oud stacking the dopli eaten like blocks in n nncsery yields t se simple cubic luaice. Specifically, the prnccdnte generates planes nf atoms like that preciously sliowu itt Pig. 1.2(a). Planes ef atoms parultel In rite base plane are separated from one anuilter by U unit cell side leitgtlr or lattice curt (C) Exercine 1.1 The test-associated softscare distribslesh cur tire lrtteeuet or on floppy disk u contains o directory Ar folder named MacMolecule. Files stored inside this directory or folder are ASCII inpul files generated by tire audmer (hr use with a computer pregront by the Sante name. Time MacMolecsmte progrcm. copyriglrled by the Unisemily of Aricona, is dmstnihnred free of charge to ocodenric users and in ovoiloble at many academic sites. As tIm ueme implies, the program runs etmly on Macintosh personal conipoters. Thu input files supplied to IRM-compotiblu users, however, cumt be readily concerted (a) Simmmplu cobic for use ant a public-access Macirmtcmshm. MacMolecule geocralos and dmspluys u “boti-arrd-stick” 3-0 color rendering of molecules. unit cells, and tatrices. The immpnt files supplied by the uuthuu can be used to help cisrialice tIre simple enbie, bee, and (cc uttit cells, plus the diamond ond aloe blende unit cells described in rite nest subsection. The About-MacMolecule file thot is distributed wilh the MacMolecule program prosides detnihed iuformation about Ihe use of the program and the gencrariomm)roodifieatioms of input files. The rnadcr is urged to iorestigote and play suith the MucMolecule saftwure, The initiul display is olssays a c-directior viem and in typically pneodo-two-dimensional (b) Podauticully cowed simple cubic in nature. A moore informative ciem is obtained by rotntirlg the model. Rutctioo is best ucconmptithed by “grahbiog and dragging” the edges of the model. The morn adxen turesonme may wish In Icy their humid ut modiiog Ihe esistiog input files or generat ing ness input ftles. 1.2.3 Semiconductor Lattices (ci buc (dl fcc Figuru 1.3 Simple ihruc.dioiensionul urn cells. lal Siinplu cAine uuh colt. Ib) Pudunticulty correct simple cubic anh ccli iuctoding only the fraetiunul pustiun 11181 of ouch ecrune Atom actually mitten the cull cube. (ci Budy ceusused cubic unit cetl. (dl Puce centered cubic unit cult. We are finally in u position to supply deroils relulise to the positioning of utoms scithin the priociput semiconductors. In Si (and Ge) the lotlice structure is described by the omit cell pictured iu Pig. 1.4(u). The Pig. 1.4(u) arrangement is kucwn as the dininaird loltice onit cell because it also chorucrerlees diamond, o form of the Column IV element corbon. Ru umining the diumoud lattice unit cell. we ode thur the cell is cubic, with atoms ut each www.EasyEngineering.net Ill SEMICONDUCTOR PUNnAMEIeraLU SEMICONDUCTORS: A GENERAL INTRuOuCTION — lob 11 holly identicnd to the diumond lattice. eneept thur lorries sites ore apportioned eqoolly be tween two diffemnt uhoms. Go uccopius sites on one of the two intecpenetrut ing fcc sublurtices; arsenic (As) populates Ihe other fcc subluttice. Now thut the poniliuning of atoms snithin the principal semicondoclom has been esrnh lished, the question moy arise us to the pructicul nlilicotion of such teformutron. Allhnugh seserol upplicotions could he cited, geometticul-lype coicolutiuns constitute a very cam moo oud readily esplained one of the unit cell !ormalism. Par esomple, in Si 01 cnom rem perutnre the unit cell side length (a) is 5.43 A (where I A = 10 -n cm). Since thore ore eight Si ntoms per unit cell und the solume of the unit cell is o. it follosss that there urn 5 at ulmost ecuclly 5 on l0°° utums/em 8/a t in the Si lattice. Similnr coiculutions could be performed to determine olomic radii, the dislunce between uromic plnnen, nnd so forth. Por the purposeo of the development herein, howeser, a mojur reason for the discassiou of semiconductor luttices wus to esroblish thor, as emphosieed In Fig. 1.4(c), atoms in the diamond and cinchiende lonicec hare four nearest neighburo. The chemicnl bonding (or cryntolline glue) within Ike major semiconductors is therefore dnminolcd by the ottroction kctweeo any gioen alum and its four closest neighbors. This is on itnpoetout fuel thot should be filed owoy foe futore reference. tbl ww w.E Exercise 1.2 id Figure 1.4 (u) Diamond lattice unit coil. thi Ziucbtnudc loif en unit cell (GuAs used fur illustie oo:il. id P.ulsigcd top cornc 01 ihe putt la) diamond luttice etnphuoiciug thu funn.nrmmr-nuighbus bonding icithin ihu stroennue. Thu cube side length. u, is 5.43 A and 5.b5 A At T = 308 K hr Si und , Gififit by John Wiley & Sans, 1 GaAs. respeetisety Ilu) .hdopted from Shockleyci. (hi From gent Inc. Reprinted wiilli pesmissior.( — corner and oh mmli face of the cube sitnilac to Ike fcc cell. The interior of tkc Pig. 1.4(u) cell. howeser. contains four additional atotos. One of [he interior crams is Iccared along a coke body diagonal exactly one-quarter of the wAy dawn the diogocal (cots the top (coot lefI-hund corner of the cnbe. The other three inlcrior atoms ace displaced ene-qnortcr of [lie body diagoool length along the previously noted body diagonal direction from the (runt, rap, and left-side face atoms, respectively. Altltoogli iI may be difficolt In visoaliee frnnt Pig. 1.4(o), the diamond lattice can also be described us corking osore thun 1550 interpene tailing fcc lattices. The corner and face otoirss of the auit cell con be viesced us belonging to one fcc lattice, while the arotes ioiully contained wtthin the cell belong to the second (cc lattice. The second lottice is disaloced one-quarter of a body diogonol along a bridy diogo nal direction relative to the first fcc lattice. Most of the UI-V semicoudoclais, imrcluding GaAs, ceyslallice in the chicblende struc ture. The cinchlende lattice, typified by the GoAs oisit cell shown in Pig. 1.4(b), is essec asy En gin F: If thu lattice coosnuc or unit cell side-lrngflt in Si is a = 5.43 on I0 cm, whal in the dislunce (d) from the center of one Si olom to thn center of lhs nearest ueighboc7 eer St As noted ic thn Pig. 1.4 caption, the atom in the upper front cornier of the Si 001; cell and the otom olong the enbe diogonal one-(ouehh of the moy down the diogonol ore nearest neighbors. Since hhn diugonol of u cube (C) Exeroine 1.3 ing .ne Pt Construct o MATLAO program Ihul computes the oombnc of 5 atoms/cm in cubic crystals. Use the MATLAn lapse fnnctian to cuter the number of atoms/unit-cell and the unit cell side length (n) (era specific crystal. Moke a listing of your program ond record the progrcm ressll schen applied to silicott. 5: MATLAn prngcam script... %Rcercise 1.3 FeComputotian of the number of utoms/cm3 in o cubic lattice N =input(’inpol nnmber of uicms/nml cell, N = u=inpot(’Iutticnconclamtt in oogsteont, 0 = ( 1.0e24)/(o”3) Feanmber of atoms/emS 5 otmdcnN www.EasyEngineering.net t /. www.EasyEngineering.net 12 nmMtcaNnacsoR FaNllAunN’raLs nrMtcouoac’ronn; AaENRnnt.tevnat’aacl’tON 13 Program otttpal for Si inpat nasrber of alosavianit cell, N = lattice convlsist in axgsltota, a 5.43 atmdess = .4 OOfifiei’22 1,2.4 Miller Indices Single crystaln of silicon axed in device pracessing narmalty assnme the thin, eased form exhibited in Fig. 1.5. The pictored plate-like nixgte crystals, helter know nan Si wafern, are typical of the starticy nabstrates prencntly employed by erajor tnanafactnrers. Of parttcelar interest here in the fact that the snrface of a wafer is cacefnlly preerleeled to lie along a specific crynlotlographic plane. Moreover, n “fiat” oe “notch” In graced along the periph ery af the wafer to identify a reference direction within the narface plane. Precise narfaca oricntattaa ix critical in certaia device pracesning stcps and directly affects the character inticn exhibited by a aambcr of devices. The fiat or notch in raatiarly employed, far ex ample, to orient device arrays aa the wafer no an to achieve high yields daring device ww w.E as y En gin e (c) separatiaa. The point ‘so wish to make is that the sprcificatioo of crystallagrapbic plastes and directives is of practical importance. Miller indices, cnemplihed by the (100) place sad (011] dicrctiaa designaliatts axed ia Fig. 1.5, caaslilale the canveatioasl means af ideatifyiag plaaex and dicectiaas withia a crystal. The Miller indices far any givea plaae of slams within a crystal are obtained by fatlaw ing a ssraigitslarward faxr-step procedare. The pracedaro is drtailed hetow, alang soith the sietaltaaeoas sample ittdcning of the place shown in Fig. l.6)a). eri lttdesiog Procedaro ng. ne t Figure 1,5 Single-crystal silicon wafarn typical af the starting sabstrases presently nmplnyad by mnjar dnvice manafarsarars. The tIlt asia 16 irab) and 200 mm (6 inch) wafers are seminally g.625 mm sad 0.725 salts thick, raspactivaly. The facing sarfacc is polished and etched yielding a daasaga-free, mirror-tiRe hnish. Thy hgore dramatizes rho atitity of Mittrr indices enamplihad by the (tOO) plann and [01) diractiaa dosigaatians. (Phatagraph caartrvy af Intel Carparatiaa.l (hI (a) Figure 1,6 Saosple cabic crystal planes. (a) The (632) plane asad is asplaiaisg the Miller indrniag pracedsra. (b) The (001) plara. Ic) The 1221) plane. Sample Imylameatasian After setting ap caardinara scat along the edgas of the oait call, note wltrre the plaaa to ha tedanad iatercopts the axes. Divide each intarrrpt valae by the unit call length along the raxpwtioa coordinate avis. Record the resalting rarmalizod (paw-nrmhcr) intercept srtin tlte ordne x, y, c Invert the intercept xalom; that is, form Illintarooptls. 1, ½, ½ Using an appropnate waltrpliar, eonvea the I/intercept set to the smallest pnvsibln set af whola nnmbers. 6, 3, 2 Lactose the wholo-aumbar satin oarviltnaar brackats. 1632) 1,2,3 Ta complete the description of the plane-indexing pracedare, the 05cr shoold alsa be aware of the fallasoing special facts: (i) If the plane to be indexed is parallel to a coordinate axis, the “intercept” alang the axis is taken lobe at infinity. Than, far example, the place shown in Fig. 1.0(b) inter cepts the coordinate aries alas, m, I, and ix therefore a (001) plane. www.EasyEngineering.net 14 nEatCONDUcTaR FaNDAMENTaLn sn?utcoNanc’eaen: A nORmAL tN’eRoDacxtaN (ii) If the plane to be indened han an intercept along the negattve portion of a coardtaate axis, a nsinas sign is placed 00cr the corresponding index nambec Than the Fig. 1.6(c) plane is designated a (221) plane. Tuble 1,3 (iii) Referring lathe diamond lattice of Fig. 1.4(a), nate that the sin planes passing throagh the cabr faces cantain identical atom arrangements; that is, becoase of crystal sym metry, isis impassible to dislingaish between the “eqatoalens” (100), (010), (001), (100). (010), and (001) planes; or, it is impossible to distiagninh between (l00} places. A gronp of eqaivalent planes is concisely referenced tn the Mtller notation throagh the use ef I ) braces. (hk() fOol ( (iv) Miller iadices cannot he established far a plane passing throagh the origin of caordi colon. The origin of coordinates muss ho mooed to a lattice point not an the plare to be indexed. This pracodxre is acceptable bncaase of the rqrttvolenl cobra of parnllnl m. planes. *-::;*L S½ ii Miller Convention Santtoary. lrtret’pretoriatr Coarettriort I)thl] (hk() Crystal plane Eqoivatcnt planes Crystal direction Eqaivalent direclians Using the simple enbic colt as n reference, the three wasl commottly rnraantnrrd crystal line planes are vixaaliord in Fig. 1.7(o). TIne Miller indices for diversions are established in a manner analagaas to the wallknown pracedara for finding the components of a vectoc First, set np a vector of arbilrary length in the direction of inlnrevl. Next, drcontpasc tIre vector into its components by noting the projncsianv of the vector along the coordinate axes. Using an appropriate mallt plier. coavert the companottt ralacs into the smallest possible whole-number srI. This of caxrsc changes che length of the original vector ha; not its direction. Finally, etrclooo the whole-namber sot in brackets. Sqnarc brackets, [I, are nsnd to designate specific directions within a crystal; triangalor brttckels, 0 designate an eqaivalcol set of directions. Cammolt direction vectors and Ihoir corresponding Miller indices are displnyed in Fig. 1.7(b). A vammary of the Miller bracketing canvexrian far planes and directions in given in Table 1.3. In she foregoing discansion we presented the prorndnrc for progressing from a given plane or direction in a crystal to the corresponding Miller indices, Marc oflca than nor, axe is fared with she inverse pracexs—visaalieissg the crystalline plane or direclina correspond ing to a given set of indices. Portnaalrly, ace seldom eneaanlers other than low-index planes and directions sach as (111), (110), (00)]. Than it is possible to become fairly adept at the inverse process by simply mcmariring she artcntations for plonr.s sad directions associated soith satall-eawbor indices. Is in also helpfai so note that, for esrbir cryorals, a p/atte ann rho dirersiws norroat ro the aiorte hare precisely rOe sante indices—e.g.. the 1110) direction is tormol to the (110) plonr. Of coarse. any ptaae yr direction can alsooys be deduced by reversing the indexing pracedare. Enercinel,4 /)‘‘ PI For a cable crystal lattice: )b) (a) Determine the Miller indices for she plane and direction vector shown ia Pig. LId(s). Pigare 1.7 Visoahenhan ted Mdlrr irdicer at cawwonly encaoosowd (a) crysrollser glares and Ib) direction ractacs. (b) Sketch she place and direction vector eltaracterized by (UI I) assd ill], cc npcctis’ety’. 15 www.EasyEngineering.net 12 nmMtcaNnacsoR FaNllAunN’raLs nrMtcouoac’ronn; AaENRnnt.tevnat’aacl’tON 13 Program otttpal for Si inpat nasrber of alosavianit cell, N = lattice convlsist in axgsltota, a 5.43 atmdess = .4 OOfifiei’22 1,2.4 Miller Indices Single crystaln of silicon axed in device pracessing narmalty assnme the thin, eased form exhibited in Fig. 1.5. The pictored plate-like nixgte crystals, helter know nan Si wafern, are typical of the starticy nabstrates prencntly employed by erajor tnanafactnrers. Of parttcelar interest here in the fact that the snrface of a wafer is cacefnlly preerleeled to lie along a specific crynlotlographic plane. Moreover, n “fiat” oe “notch” In graced along the periph ery af the wafer to identify a reference direction within the narface plane. Precise narfaca oricntattaa ix critical in certaia device pracesning stcps and directly affects the character inticn exhibited by a aambcr of devices. The fiat or notch in raatiarly employed, far ex ample, to orient device arrays aa the wafer no an to achieve high yields daring device ww (hI (a) (c) Figure 1,6 Saosple cabic crystal planes. (a) The (632) plane asad is asplaiaisg the Miller indrniag pracedsra. (b) The (001) plara. Ic) The 1221) plane. w.E a separatiaa. The point ‘so wish to make is that the sprcificatioo of crystallagrapbic plastes and directives is of practical importance. Miller indices, cnemplihed by the (100) place sad (011] dicrctiaa designaliatts axed ia Fig. 1.5, caaslilale the canveatioasl means af ideatifyiag plaaex and dicectiaas withia a crystal. The Miller indices far any givea plaae of slams within a crystal are obtained by fatlaw ing a ssraigitslarward faxr-step procedare. The pracedaro is drtailed hetow, alang soith the sietaltaaeoas sample ittdcning of the place shown in Fig. l.6)a). syE ngi nee r lttdesiog Procedaro Figure 1,5 Single-crystal silicon wafarn typical af the starting sabstrases presently nmplnyad by mnjar dnvice manafarsarars. The tIlt asia 16 irab) and 200 mm (6 inch) wafers are seminally g.625 mm sad 0.725 salts thick, raspactivaly. The facing sarfacc is polished and etched yielding a daasaga-free, mirror-tiRe hnish. Thy hgore dramatizes rho atitity of Mittrr indices enamplihad by the (tOO) plann and [01) diractiaa dosigaatians. (Phatagraph caartrvy af Intel Carparatiaa.l ing . Sample Imylameatasian After setting ap caardinara scat along the edgas of the oait call, note wltrre the plaaa to ha tedanad iatercopts the axes. Divide each intarrrpt valae by the unit call length along the raxpwtioa coordinate avis. Record the resalting rarmalizod (paw-nrmhcr) intercept srtin tlte ordne x, y, c Invert the intercept xalom; that is, form Illintarooptls. 1,2,3 1, ½, ½ Using an appropnate waltrpliar, eonvea the I/intercept set to the smallest pnvsibln set af whola nnmbers. 6, 3, 2 Lactose the wholo-aumbar satin oarviltnaar brackats. 1632) net Ta complete the description of the plane-indexing pracedare, the 05cr shoold alsa be aware of the fallasoing special facts: (i) If the plane to be indexed is parallel to a coordinate axis, the “intercept” alang the axis is taken lobe at infinity. Than, far example, the place shown in Fig. 1.0(b) inter cepts the coordinate aries alas, m, I, and ix therefore a (001) plane. www.EasyEngineering.net 14 nEatCONDUcTaR FaNDAMENTaLn sn?utcoNanc’eaen: A nORmAL tN’eRoDacxtaN (ii) If the plane to be indened han an intercept along the negattve portion of a coardtaate axis, a nsinas sign is placed 00cr the corresponding index nambec Than the Fig. 1.6(c) plane is designated a (221) plane. Tuble 1,3 (iii) Referring lathe diamond lattice of Fig. 1.4(a), nate that the sin planes passing throagh the cabr faces cantain identical atom arrangements; that is, becoase of crystal sym metry, isis impassible to dislingaish between the “eqatoalens” (100), (010), (001), (100). (010), and (001) planes; or, it is impossible to distiagninh between (l00} places. A gronp of eqaivalent planes is concisely referenced tn the Mtller notation throagh the use ef I ) braces. (hk() fOol ( (iv) Miller iadices cannot he established far a plane passing throagh the origin of caordi colon. The origin of coordinates muss ho mooed to a lattice point not an the plare to be indexed. This pracodxre is acceptable bncaase of the rqrttvolenl cobra of parnllnl m. planes. *-::;*L S½ ii Miller Convention Santtoary. lrtret’pretoriatr Coarettriort I)thl] (hk() Crystal plane Eqoivatcnt planes Crystal direction Eqaivalent direclians Using the simple enbic colt as n reference, the three wasl commottly rnraantnrrd crystal line planes are vixaaliord in Fig. 1.7(o). TIne Miller indices for diversions are established in a manner analagaas to the wallknown pracedara for finding the components of a vectoc First, set np a vector of arbilrary length in the direction of inlnrevl. Next, drcontpasc tIre vector into its components by noting the projncsianv of the vector along the coordinate axes. Using an appropriate mallt plier. coavert the companottt ralacs into the smallest possible whole-number srI. This of caxrsc changes che length of the original vector ha; not its direction. Finally, etrclooo the whole-namber sot in brackets. Sqnarc brackets, [I, are nsnd to designate specific directions within a crystal; triangalor brttckels, 0 designate an eqaivalcol set of directions. Cammolt direction vectors and Ihoir corresponding Miller indices are displnyed in Fig. 1.7(b). A vammary of the Miller bracketing canvexrian far planes and directions in given in Table 1.3. In she foregoing discansion we presented the prorndnrc for progressing from a given plane or direction in a crystal to the corresponding Miller indices, Marc oflca than nor, axe is fared with she inverse pracexs—visaalieissg the crystalline plane or direclina correspond ing to a given set of indices. Portnaalrly, ace seldom eneaanlers other than low-index planes and directions sach as (111), (110), (00)]. Than it is possible to become fairly adept at the inverse process by simply mcmariring she artcntations for plonr.s sad directions associated soith satall-eawbor indices. Is in also helpfai so note that, for esrbir cryorals, a p/atte ann rho dirersiws norroat ro the aiorte hare precisely rOe sante indices—e.g.. the 1110) direction is tormol to the (110) plonr. Of coarse. any ptaae yr direction can alsooys be deduced by reversing the indexing pracedare. Enercinel,4 /)‘‘ PI For a cable crystal lattice: )b) (a) Determine the Miller indices for she plane and direction vector shown ia Pig. LId(s). Pigare 1.7 Visoahenhan ted Mdlrr irdicer at cawwonly encaoosowd (a) crysrollser glares and Ib) direction ractacs. (b) Sketch she place and direction vector eltaracterized by (UI I) assd ill], cc npcctis’ety’. 15 12 nmMtcaNnacsoR FaNllAunN’raLs nrMtcouoac’ronn; AaENRnnt.tevnat’aacl’tON 13 Program otttpal for Si inpat nasrber of alosavianit cell, N = lattice convlsist in axgsltota, a 5.43 atmdess = .4 OOfifiei’22 1,2.4 Miller Indices Single crystaln of silicon axed in device pracessing narmalty assnme the thin, eased form exhibited in Fig. 1.5. The pictored plate-like nixgte crystals, helter know nan Si wafern, are typical of the starticy nabstrates prencntly employed by erajor tnanafactnrers. Of parttcelar interest here in the fact that the snrface of a wafer is cacefnlly preerleeled to lie along a specific crynlotlographic plane. Moreover, n “fiat” oe “notch” In graced along the periph ery af the wafer to identify a reference direction within the narface plane. Precise narfaca oricntattaa ix critical in certaia device pracesning stcps and directly affects the character inticn exhibited by a aambcr of devices. The fiat or notch in raatiarly employed, far ex ample, to orient device arrays aa the wafer no an to achieve high yields daring device (hI (a) (c) Figure 1,6 Saosple cabic crystal planes. (a) The (632) plane asad is asplaiaisg the Miller indrniag pracedsra. (b) The (001) plara. Ic) The 1221) plane. separatiaa. The point ‘so wish to make is that the sprcificatioo of crystallagrapbic plastes and directives is of practical importance. Miller indices, cnemplihed by the (100) place sad (011] dicrctiaa designaliatts axed ia Fig. 1.5, caaslilale the canveatioasl means af ideatifyiag plaaex and dicectiaas withia a crystal. The Miller indices far any givea plaae of slams within a crystal are obtained by fatlaw ing a ssraigitslarward faxr-step procedare. The pracedaro is drtailed hetow, alang soith the sietaltaaeoas sample ittdcning of the place shown in Fig. l.6)a). lttdesiog Procedaro Figure 1,5 Single-crystal silicon wafarn typical af the starting sabstrases presently nmplnyad by mnjar dnvice manafarsarars. The tIlt asia 16 irab) and 200 mm (6 inch) wafers are seminally g.625 mm sad 0.725 salts thick, raspactivaly. The facing sarfacc is polished and etched yielding a daasaga-free, mirror-tiRe hnish. Thy hgore dramatizes rho atitity of Mittrr indices enamplihad by the (tOO) plann and [01) diractiaa dosigaatians. (Phatagraph caartrvy af Intel Carparatiaa.l Sample Imylameatasian After setting ap caardinara scat along the edgas of the oait call, note wltrre the plaaa to ha tedanad iatercopts the axes. Divide each intarrrpt valae by the unit call length along the raxpwtioa coordinate avis. Record the resalting rarmalizod (paw-nrmhcr) intercept srtin tlte ordne x, y, c Invert the intercept xalom; that is, form Illintarooptls. 1, ½, ½ Using an appropnate waltrpliar, eonvea the I/intercept set to the smallest pnvsibln set af whola nnmbers. 6, 3, 2 Lactose the wholo-aumbar satin oarviltnaar brackats. 1632) 1,2,3 Ta complete the description of the plane-indexing pracedare, the 05cr shoold alsa be aware of the fallasoing special facts: (i) If the plane to be indexed is parallel to a coordinate axis, the “intercept” alang the axis is taken lobe at infinity. Than, far example, the place shown in Fig. 1.0(b) inter cepts the coordinate aries alas, m, I, and ix therefore a (001) plane. www.EasyEngineering.net 14 nEatCONDUcTaR FaNDAMENTaLn sn?utcoNanc’eaen: A nORmAL tN’eRoDacxtaN (ii) If the plane to be indened han an intercept along the negattve portion of a coardtaate axis, a nsinas sign is placed 00cr the corresponding index nambec Than the Fig. 1.6(c) plane is designated a (221) plane. Tuble 1,3 (iii) Referring lathe diamond lattice of Fig. 1.4(a), nate that the sin planes passing throagh the cabr faces cantain identical atom arrangements; that is, becoase of crystal sym metry, isis impassible to dislingaish between the “eqatoalens” (100), (010), (001), (100). (010), and (001) planes; or, it is impossible to distiagninh between (l00} places. A gronp of eqaivalent planes is concisely referenced tn the Mtller notation throagh the use ef I ) braces. (hk() fOol ( (iv) Miller iadices cannot he established far a plane passing throagh the origin of caordi colon. The origin of coordinates muss ho mooed to a lattice point not an the plare to be indexed. This pracodxre is acceptable bncaase of the rqrttvolenl cobra of parnllnl m. planes. ww w S½ .Ea syE ngi *-::;*L nee rin g ii .ne t Miller Convention Santtoary. lrtret’pretoriatr Coarettriort I)thl] (hk() Crystal plane Eqoivatcnt planes Crystal direction Eqaivalent direclians Using the simple enbic colt as n reference, the three wasl commottly rnraantnrrd crystal line planes are vixaaliord in Fig. 1.7(o). TIne Miller indices for diversions are established in a manner analagaas to the wallknown pracedara for finding the components of a vectoc First, set np a vector of arbilrary length in the direction of inlnrevl. Next, drcontpasc tIre vector into its components by noting the projncsianv of the vector along the coordinate axes. Using an appropriate mallt plier. coavert the companottt ralacs into the smallest possible whole-number srI. This of caxrsc changes che length of the original vector ha; not its direction. Finally, etrclooo the whole-namber sot in brackets. Sqnarc brackets, [I, are nsnd to designate specific directions within a crystal; triangalor brttckels, 0 designate an eqaivalcol set of directions. Cammolt direction vectors and Ihoir corresponding Miller indices are displnyed in Fig. 1.7(b). A vammary of the Miller bracketing canvexrian far planes and directions in given in Table 1.3. In she foregoing discansion we presented the prorndnrc for progressing from a given plane or direction in a crystal to the corresponding Miller indices, Marc oflca than nor, axe is fared with she inverse pracexs—visaalieissg the crystalline plane or direclina correspond ing to a given set of indices. Portnaalrly, ace seldom eneaanlers other than low-index planes and directions sach as (111), (110), (00)]. Than it is possible to become fairly adept at the inverse process by simply mcmariring she artcntations for plonr.s sad directions associated soith satall-eawbor indices. Is in also helpfai so note that, for esrbir cryorals, a p/atte ann rho dirersiws norroat ro the aiorte hare precisely rOe sante indices—e.g.. the 1110) direction is tormol to the (110) plonr. Of coarse. any ptaae yr direction can alsooys be deduced by reversing the indexing pracedare. Enercinel,4 /)‘‘ PI For a cable crystal lattice: )b) (a) Determine the Miller indices for she plane and direction vector shown ia Pig. LId(s). Pigare 1.7 Visoahenhan ted Mdlrr irdicer at cawwonly encaoosowd (a) crysrollser glares and Ib) direction ractacs. (b) Sketch she place and direction vector eltaracterized by (UI I) assd ill], cc npcctis’ety’. www.EasyEngineering.net 15 12 nmMtcaNnacsoR FaNllAunN’raLs nrMtcouoac’ronn; AaENRnnt.tevnat’aacl’tON 13 Program otttpal for Si inpat nasrber of alosavianit cell, N = lattice convlsist in axgsltota, a 5.43 atmdess = .4 OOfifiei’22 1,2.4 Miller Indices Single crystaln of silicon axed in device pracessing narmalty assnme the thin, eased form exhibited in Fig. 1.5. The pictored plate-like nixgte crystals, helter know nan Si wafern, are typical of the starticy nabstrates prencntly employed by erajor tnanafactnrers. Of parttcelar interest here in the fact that the snrface of a wafer is cacefnlly preerleeled to lie along a specific crynlotlographic plane. Moreover, n “fiat” oe “notch” In graced along the periph ery af the wafer to identify a reference direction within the narface plane. Precise narfaca oricntattaa ix critical in certaia device pracesning stcps and directly affects the character inticn exhibited by a aambcr of devices. The fiat or notch in raatiarly employed, far ex ample, to orient device arrays aa the wafer no an to achieve high yields daring device (hI (a) (c) Figure 1,6 Saosple cabic crystal planes. (a) The (632) plane asad is asplaiaisg the Miller indrniag pracedsra. (b) The (001) plara. Ic) The 1221) plane. separatiaa. The point ‘so wish to make is that the sprcificatioo of crystallagrapbic plastes and directives is of practical importance. Miller indices, cnemplihed by the (100) place sad (011] dicrctiaa designaliatts axed ia Fig. 1.5, caaslilale the canveatioasl means af ideatifyiag plaaex and dicectiaas withia a crystal. The Miller indices far any givea plaae of slams within a crystal are obtained by fatlaw ing a ssraigitslarward faxr-step procedare. The pracedaro is drtailed hetow, alang soith the sietaltaaeoas sample ittdcning of the place shown in Fig. l.6)a). lttdesiog Procedaro Figure 1,5 Single-crystal silicon wafarn typical af the starting sabstrases presently nmplnyad by mnjar dnvice manafarsarars. The tIlt asia 16 irab) and 200 mm (6 inch) wafers are seminally g.625 mm sad 0.725 salts thick, raspactivaly. The facing sarfacc is polished and etched yielding a daasaga-free, mirror-tiRe hnish. Thy hgore dramatizes rho atitity of Mittrr indices enamplihad by the (tOO) plann and [01) diractiaa dosigaatians. (Phatagraph caartrvy af Intel Carparatiaa.l Sample Imylameatasian After setting ap caardinara scat along the edgas of the oait call, note wltrre the plaaa to ha tedanad iatercopts the axes. Divide each intarrrpt valae by the unit call length along the raxpwtioa coordinate avis. Record the resalting rarmalizod (paw-nrmhcr) intercept srtin tlte ordne x, y, c Invert the intercept xalom; that is, form Illintarooptls. 1, ½, ½ Using an appropnate waltrpliar, eonvea the I/intercept set to the smallest pnvsibln set af whola nnmbers. 6, 3, 2 Lactose the wholo-aumbar satin oarviltnaar brackats. 1632) 1,2,3 Ta complete the description of the plane-indexing pracedare, the 05cr shoold alsa be aware of the fallasoing special facts: (i) If the plane to be indexed is parallel to a coordinate axis, the “intercept” alang the axis is taken lobe at infinity. Than, far example, the place shown in Fig. 1.0(b) inter cepts the coordinate aries alas, m, I, and ix therefore a (001) plane. www.EasyEngineering.net 14 nEatCONDUcTaR FaNDAMENTaLn sn?utcoNanc’eaen: A nORmAL tN’eRoDacxtaN (ii) If the plane to be indened han an intercept along the negattve portion of a coardtaate axis, a nsinas sign is placed 00cr the corresponding index nambec Than the Fig. 1.6(c) plane is designated a (221) plane. Tuble 1,3 (iii) Referring lathe diamond lattice of Fig. 1.4(a), nate that the sin planes passing throagh the cabr faces cantain identical atom arrangements; that is, becoase of crystal sym metry, isis impassible to dislingaish between the “eqatoalens” (100), (010), (001), (100). (010), and (001) planes; or, it is impossible to distiagninh between (l00} places. A gronp of eqaivalent planes is concisely referenced tn the Mtller notation throagh the use ef I ) braces. (hk() fOol ( (iv) Miller iadices cannot he established far a plane passing throagh the origin of caordi colon. The origin of coordinates muss ho mooed to a lattice point not an the plare to be indexed. This pracodxre is acceptable bncaase of the rqrttvolenl cobra of parnllnl m. planes. Miller Convention Santtoary. lrtret’pretoriatr Coarettriort I)thl] Crystal plane Eqoivatcnt planes Crystal direction Eqaivalent direclians (hk() ww w.E Using the simple enbic colt as n reference, the three wasl commottly rnraantnrrd crystal line planes are vixaaliord in Fig. 1.7(o). TIne Miller indices for diversions are established in a manner analagaas to the wallknown pracedara for finding the components of a vectoc First, set np a vector of arbilrary length in the direction of inlnrevl. Next, drcontpasc tIre vector into its components by noting the projncsianv of the vector along the coordinate axes. Using an appropriate mallt plier. coavert the companottt ralacs into the smallest possible whole-number srI. This of caxrsc changes che length of the original vector ha; not its direction. Finally, etrclooo the whole-namber sot in brackets. Sqnarc brackets, [I, are nsnd to designate specific directions within a crystal; triangalor brttckels, 0 designate an eqaivalcol set of directions. Cammolt direction vectors and Ihoir corresponding Miller indices are displnyed in Fig. 1.7(b). A vammary of the Miller bracketing canvexrian far planes and directions in given in Table 1.3. In she foregoing discansion we presented the prorndnrc for progressing from a given plane or direction in a crystal to the corresponding Miller indices, Marc oflca than nor, axe is fared with she inverse pracexs—visaalieissg the crystalline plane or direclina correspond ing to a given set of indices. Portnaalrly, ace seldom eneaanlers other than low-index planes and directions sach as (111), (110), (00)]. Than it is possible to become fairly adept at the inverse process by simply mcmariring she artcntations for plonr.s sad directions associated soith satall-eawbor indices. Is in also helpfai so note that, for esrbir cryorals, a p/atte ann rho dirersiws norroat ro the aiorte hare precisely rOe sante indices—e.g.. the 1110) direction is tormol to the (110) plonr. Of coarse. any ptaae yr direction can alsooys be deduced by reversing the indexing pracedare. asy En *-::;*L S½ ii gin eer ing .ne Enercinel,4 /)‘‘ 15 PI For a cable crystal lattice: )b) (a) Determine the Miller indices for she plane and direction vector shown ia Pig. LId(s). Pigare 1.7 Visoahenhan ted Mdlrr irdicer at cawwonly encaoosowd (a) crysrollser glares and Ib) direction ractacs. (b) Sketch she place and direction vector eltaracterized by (UI I) assd ill], cc npcctis’ety’. www.EasyEngineering.net t www.EasyEngineering.net 16 SEMICONDUCTOR FUNDAMENTALS SEMICONDUCTORS: A GENERAL INTRODUCTION S: (a) The Intercepts of the platte are I. I, antI 2 along the x. y, and e eaorthOatc axes, respectively. Taking [l/intcrceptls yields I, I, 1/2. Multiplying by 2 to obtatit the lossest whole-number set, aitd enelostng itt parentheses, gives for Site Miller indices of the plane. TIte direction vector has projections of 2 u, a. attd 0 along the a, y, aitd coordiitatc axes, respectively. Tite Miller indices for the direction are then J. 17 — sari, — S:Iiva — Rntucvd is pmrsrrvs nrC (b) For the (Oil) plane, [1/interceptls 0, 1, 1. The normalized a, y, intercepts of the plane are Ilterefore m, I, I; the plane intersects the y-axis at a, intersects the c-axis air,, and is parallel to Site a-axis. In acubic crystal the [Oil) direction is normal to tile (fill) plane. The dedneed plane and directiots arc as sketched in Fig. El.4(b). ww Chior,nurnd ..._.[Zi a 0 aru Disi,iied, eta. øj pornn fieduard iv imydrognr atmosphere Figure 1,8 Summary of lie process osnployed to produce ultrapure silicon. z w.E (a) as y En gin e Figure E1.4 1.3 CRYSTAL GROWTH 1.3.1 Obtaining Ultrapure Si separated material. The ingcnioas separation and purification process that has evolved is saimrritarizcd is Fig. 1.8. Low-grade silicon or ferrosilticun is first produced by heating silica ss’ith carbon in an electric furnace. The carbon essentially pails tlte oxygen away from Ilte impure SiC, (i.e., redace.s the SiO,), leaving behind impure Si. Nest, the ferrosilicon is cltlorinated to yield SiCI 4 or SiRCI,, both of wltich are liquids at room temperature Al lhonglt appeariug odd al first glance, the liqtiefactiou process is actually a clever maneuver. Whereas solids are very difiicalt to purify. a number of slandard procedures are available for purifying liquids. Au ultrapure SiCla (or SiHCI,) is the sosult after multiple distillation aud other liquid purification procedures. Lastly, the higit-parity halide is chentically re duced, yielding the desired ultrapure elemental silicou. TIus is accomplished, for example, by heating SiCI 5 in a hydrogen atmosphere [SiCI 5 + 2Ha 4 HCI + Si). 5 (b) eri 1.3.2 Single-Crystal Formation ng. ne Given tlte obviotts general availability and widespread use of semiconductor materials, par ticularly Si. it is seasonable to wonder about the origin of the single-crystal St used in modern-day device production. Could it be that Si is readily available in sandstone de posits?—No. Perhaps, as a sort of by-product, Si single crystals come from South African dinittond mines?—Wrong again. As suggested recently in a low.budgcl science l’tction toovie, maybe Si is scooped front the ocean bottom by special submarines?—Sorry, no. Althongit Si is the second most abundant element in the earth’s crust and a component in nomeeous compounds, chief of svhich are silica (impure SiO,) and the silicates (St ± 0 + another element), silicon never occurs alone in natore us an eletnent. Single-crystal Si used in device production, it turns out, is a man-made material. Given the preceding introduction, it should be clear that Ihe initial step in producing desicc-qnality silicon must involve separating Si from its comnoonds and purifying the Although ultrapure, the silicon derived from the separation and purification process as just described is not a single crystal, but is iastead polycrystalline. Additional processing is ilserefore required to form the large single crystals used in device fabrication. The most coiunsanly employed method yielding large sittgle crystals of Si is known as the Czochral. ski method. In this uiel)mod the altraparu polycrystalliue silicott is placed in a quartz cru cible and heated juan ittert atmosphere to form a melt, as shown in Fig. 1.9. A small single crystal, or Si “seed” crystal, with the normal to its bottom face carefully aligned along a predetermined dinectiox (typically a Ut I) or (lOG) ditection). is then clamped lou metal rod and dipped into the melt. Once thermal equilibrium is established, the temperature of the nelt in the vicinity of the seed crystal is reduced, and silieou from thu melt begins to freeze 0111 onto tite seed crystal, the added material being a structurally perfect extension of the seed crystal. Subsequeittly. the seed crystal is slowly rotated and withdrawn from the melt; this permits store and inure silicou to freeze ovit on the boltom of rIte growing crystal. A pitotograph shosvjng a crystal after being pulled from the melt is displayed in Fig. 1.9(c). Toe large, cylindrically shaped single crystal of silicon, also kitowo as an ingot, is routinely up to 200 mm (8 inches) in diameter and 1 to 2 meters in lengtis. The Si svafers used ix device processieg, such as those previously pictured in Fig. 1.5, are ultimately produced by cutting the ingot ioto thin sections using a diamond-edged saw. t www.EasyEngineering.net 18 SEMICONDUCTOR FUNDAMENTALS unMicoNoucroRn: A GENERAL INTRODUC110N - 1.4 SUMMARY This chapter provides basic information about semicondnctors in general aitd silicon in particular. Esansluing the elemental cotnpouitionn of semiconductors. one finds that Iltere are. on average, four valence electrons per atom. Moreover, device-quality semiconductors are typically single crystals of high compositional parity. Si crystalltzes in the diamond lattice. GaAs crystallizes in the ainchlende lattice, and Ike lattice atoms in both cases have four nearest neighbors. Miller indices, introduced herein us an adjunct to the crystal struc ture discnssion. ate the accepted means for identifying planes and directious within a crystal. Finally. large single crystals of device-grade Si are commonly produced by the Czochralski method. PROBLEMS CHAPTER I P hI PROBLEM INFORMATION TABLE Complete Dtfficulty After Level 1.1 1.4 1 • 1.5 1.2.4 2—3 •H’ 1.6 Figure 1.9 Sitienir crystal-palling oppara toe and resulting singie crystal. (a) Photo grip> sfa compntemr-cisuirollcd Ccochratski ci’ysrat pallor. )h) Sinipli)ind scbamuiic dma’ingot the paller. Ic) Sitiauo ingot. ha) and Ic) courtesy of Wacker Silrmsroiu. )b) From Zahlehncr and Habar ; reprinted mm oirlr permission.) Photographs Suggested Point Weighuing tO (a:h-l. i-2) S/lore Description Short answer res’iew Nearn;borl 15 (a-2, b-2, c-3, d-3, e-y) A,utos/cm on planes 1 t (2 each subpart) 1.7 “ I 16 (2 each purl) Given (hkl), sketch plane 1.8 “ 1 16 (2 each purl) Given I hkl], sketch direction 1 8 (4 each pan) Perpendicular directions 1.10 “ 2 10 Direction on wafer surface Consbination question 1.9 Determine Miller indices III “ 2 10 (a-S. b-2, e-3. d-2) 1,12 “ 2 12(2 each part) Eqaivulent planes/directions 1.13 1.2.3 3 20 (5 each part) % of volume occupied 1.1 Quick Quiz. Answer the follosving questions as concisely as possible. (a) Name (i) oue elemental semiconductor and (ii) one Ill-V catnpuultd semicunductor. (b) What is the difference between a crystalline and a polycrystalline material? (c) Give a word definition of unit cell. )d) How many atomns are there io a simple cubic unit cell? in u her unit cell? unit cell? in the unit cell ritaracterizing the diamottd lattice? in a fcc 19 www.EasyEngineering.net 16 SEMICONDUCTOR FUNDAMENTALS SEMICONDUCTORS: A GENERAL INTRODUCTION S: (a) The Intercepts of the platte are I. I, antI 2 along the x. y, and e eaorthOatc axes, respectively. Taking [l/intcrceptls yields I, I, 1/2. Multiplying by 2 to obtatit the lossest whole-number set, aitd enelostng itt parentheses, gives for Site Miller indices of the plane. TIte direction vector has projections of 2 u, a. attd 0 along the a, y, aitd coordiitatc axes, respectively. Tite Miller indices for the direction are then J. 17 — sari, — S:Iiva — Rntucvd is pmrsrrvs nrC (b) For the (Oil) plane, [1/interceptls 0, 1, 1. The normalized a, y, intercepts of the plane are Ilterefore m, I, I; the plane intersects the y-axis at a, intersects the c-axis air,, and is parallel to Site a-axis. In acubic crystal the [Oil) direction is normal to tile (fill) plane. The dedneed plane and directiots arc as sketched in Fig. El.4(b). Disi,iied, eta. øj pornn fieduard iv imydrognr atmosphere Figure 1,8 Summary of lie process osnployed to produce ultrapure silicon. ww z separated material. The ingcnioas separation and purification process that has evolved is saimrritarizcd is Fig. 1.8. Low-grade silicon or ferrosilticun is first produced by heating silica ss’ith carbon in an electric furnace. The carbon essentially pails tlte oxygen away from Ilte impure SiC, (i.e., redace.s the SiO,), leaving behind impure Si. Nest, the ferrosilicon is cltlorinated to yield SiCI 4 or SiRCI,, both of wltich are liquids at room temperature Al lhonglt appeariug odd al first glance, the liqtiefactiou process is actually a clever maneuver. Whereas solids are very difiicalt to purify. a number of slandard procedures are available for purifying liquids. Au ultrapure SiCla (or SiHCI,) is the sosult after multiple distillation aud other liquid purification procedures. Lastly, the higit-parity halide is chentically re duced, yielding the desired ultrapure elemental silicou. TIus is accomplished, for example, by heating SiCI 5 in a hydrogen atmosphere [SiCI 5 + 2Ha 4 HCI + Si). 5 (a) Chior,nurnd ..._.[Zi a 0 aru (b) Figure E1.4 w.E a syE ngi nee r 1.3.2 Single-Crystal Formation ing . Although ultrapure, the silicon derived from the separation and purification process as just described is not a single crystal, but is iastead polycrystalline. Additional processing is ilserefore required to form the large single crystals used in device fabrication. The most coiunsanly employed method yielding large sittgle crystals of Si is known as the Czochral. ski method. In this uiel)mod the altraparu polycrystalliue silicott is placed in a quartz cru cible and heated juan ittert atmosphere to form a melt, as shown in Fig. 1.9. A small single crystal, or Si “seed” crystal, with the normal to its bottom face carefully aligned along a predetermined dinectiox (typically a Ut I) or (lOG) ditection). is then clamped lou metal rod and dipped into the melt. Once thermal equilibrium is established, the temperature of the nelt in the vicinity of the seed crystal is reduced, and silieou from thu melt begins to freeze 0111 onto tite seed crystal, the added material being a structurally perfect extension of the seed crystal. Subsequeittly. the seed crystal is slowly rotated and withdrawn from the melt; this permits store and inure silicou to freeze ovit on the boltom of rIte growing crystal. A pitotograph shosvjng a crystal after being pulled from the melt is displayed in Fig. 1.9(c). Toe large, cylindrically shaped single crystal of silicon, also kitowo as an ingot, is routinely up to 200 mm (8 inches) in diameter and 1 to 2 meters in lengtis. The Si svafers used ix device processieg, such as those previously pictured in Fig. 1.5, are ultimately produced by cutting the ingot ioto thin sections using a diamond-edged saw. 1.3 CRYSTAL GROWTH 1.3.1 Obtaining Ultrapure Si Given tlte obviotts general availability and widespread use of semiconductor materials, par ticularly Si. it is seasonable to wonder about the origin of the single-crystal St used in modern-day device production. Could it be that Si is readily available in sandstone de posits?—No. Perhaps, as a sort of by-product, Si single crystals come from South African dinittond mines?—Wrong again. As suggested recently in a low.budgcl science l’tction toovie, maybe Si is scooped front the ocean bottom by special submarines?—Sorry, no. Althongit Si is the second most abundant element in the earth’s crust and a component in nomeeous compounds, chief of svhich are silica (impure SiO,) and the silicates (St ± 0 + another element), silicon never occurs alone in natore us an eletnent. Single-crystal Si used in device production, it turns out, is a man-made material. Given the preceding introduction, it should be clear that Ihe initial step in producing desicc-qnality silicon must involve separating Si from its comnoonds and purifying the net www.EasyEngineering.net 18 SEMICONDUCTOR FUNDAMENTALS unMicoNoucroRn: A GENERAL INTRODUC110N - 1.4 SUMMARY This chapter provides basic information about semicondnctors in general aitd silicon in particular. Esansluing the elemental cotnpouitionn of semiconductors. one finds that Iltere are. on average, four valence electrons per atom. Moreover, device-quality semiconductors are typically single crystals of high compositional parity. Si crystalltzes in the diamond lattice. GaAs crystallizes in the ainchlende lattice, and Ike lattice atoms in both cases have four nearest neighbors. Miller indices, introduced herein us an adjunct to the crystal struc ture discnssion. ate the accepted means for identifying planes and directious within a crystal. Finally. large single crystals of device-grade Si are commonly produced by the Czochralski method. PROBLEMS CHAPTER I P hI PROBLEM INFORMATION TABLE Complete Dtfficulty After Level 1.1 1.4 1 • 1.5 1.2.4 2—3 •H’ 1.6 Figure 1.9 Sitienir crystal-palling oppara toe and resulting singie crystal. (a) Photo grip> sfa compntemr-cisuirollcd Ccochratski ci’ysrat pallor. )h) Sinipli)ind scbamuiic dma’ingot the paller. Ic) Sitiauo ingot. ha) and Ic) courtesy of Wacker Silrmsroiu. )b) From Zahlehncr and Habar ; reprinted mm oirlr permission.) Photographs Suggested Point Weighuing tO (a:h-l. i-2) S/lore Description Short answer res’iew Nearn;borl 15 (a-2, b-2, c-3, d-3, e-y) A,utos/cm on planes 1 t (2 each subpart) 1.7 “ I 16 (2 each purl) Given (hkl), sketch plane 1.8 “ 1 16 (2 each purl) Given I hkl], sketch direction 1 8 (4 each pan) Perpendicular directions 1.10 “ 2 10 Direction on wafer surface Consbination question 1.9 Determine Miller indices III “ 2 10 (a-S. b-2, e-3. d-2) 1,12 “ 2 12(2 each part) Eqaivulent planes/directions 1.13 1.2.3 3 20 (5 each part) % of volume occupied 1.1 Quick Quiz. Answer the follosving questions as concisely as possible. (a) Name (i) oue elemental semiconductor and (ii) one Ill-V catnpuultd semicunductor. (b) What is the difference between a crystalline and a polycrystalline material? (c) Give a word definition of unit cell. )d) How many atomns are there io a simple cubic unit cell? in u her unit cell? unit cell? in the unit cell ritaracterizing the diamottd lattice? in a fcc 19 16 SEMICONDUCTOR FUNDAMENTALS SEMICONDUCTORS: A GENERAL INTRODUCTION S: (a) The Intercepts of the platte are I. I, antI 2 along the x. y, and e eaorthOatc axes, respectively. Taking [l/intcrceptls yields I, I, 1/2. Multiplying by 2 to obtatit the lossest whole-number set, aitd enelostng itt parentheses, gives for Site Miller indices of the plane. TIte direction vector has projections of 2 u, a. attd 0 along the a, y, aitd coordiitatc axes, respectively. Tite Miller indices for the direction are then J. 17 — sari, — S:Iiva — Rntucvd is pmrsrrvs nrC (b) For the (Oil) plane, [1/interceptls 0, 1, 1. The normalized a, y, intercepts of the plane are Ilterefore m, I, I; the plane intersects the y-axis at a, intersects the c-axis air,, and is parallel to Site a-axis. In acubic crystal the [Oil) direction is normal to tile (fill) plane. The dedneed plane and directiots arc as sketched in Fig. El.4(b). Chior,nurnd ..._.[Zi a 0 aru Disi,iied, eta. øj pornn fieduard iv imydrognr atmosphere Figure 1,8 Summary of lie process osnployed to produce ultrapure silicon. z separated material. The ingcnioas separation and purification process that has evolved is saimrritarizcd is Fig. 1.8. Low-grade silicon or ferrosilticun is first produced by heating silica ss’ith carbon in an electric furnace. The carbon essentially pails tlte oxygen away from Ilte impure SiC, (i.e., redace.s the SiO,), leaving behind impure Si. Nest, the ferrosilicon is cltlorinated to yield SiCI 4 or SiRCI,, both of wltich are liquids at room temperature Al lhonglt appeariug odd al first glance, the liqtiefactiou process is actually a clever maneuver. Whereas solids are very difiicalt to purify. a number of slandard procedures are available for purifying liquids. Au ultrapure SiCla (or SiHCI,) is the sosult after multiple distillation aud other liquid purification procedures. Lastly, the higit-parity halide is chentically re duced, yielding the desired ultrapure elemental silicou. TIus is accomplished, for example, by heating SiCI 5 in a hydrogen atmosphere [SiCI 5 + 2Ha 4 HCI + Si). 5 (a) (b) Figure E1.4 1.3.2 Single-Crystal Formation Although ultrapure, the silicon derived from the separation and purification process as just described is not a single crystal, but is iastead polycrystalline. Additional processing is ilserefore required to form the large single crystals used in device fabrication. The most coiunsanly employed method yielding large sittgle crystals of Si is known as the Czochral. ski method. In this uiel)mod the altraparu polycrystalliue silicott is placed in a quartz cru cible and heated juan ittert atmosphere to form a melt, as shown in Fig. 1.9. A small single crystal, or Si “seed” crystal, with the normal to its bottom face carefully aligned along a predetermined dinectiox (typically a Ut I) or (lOG) ditection). is then clamped lou metal rod and dipped into the melt. Once thermal equilibrium is established, the temperature of the nelt in the vicinity of the seed crystal is reduced, and silieou from thu melt begins to freeze 0111 onto tite seed crystal, the added material being a structurally perfect extension of the seed crystal. Subsequeittly. the seed crystal is slowly rotated and withdrawn from the melt; this permits store and inure silicou to freeze ovit on the boltom of rIte growing crystal. A pitotograph shosvjng a crystal after being pulled from the melt is displayed in Fig. 1.9(c). Toe large, cylindrically shaped single crystal of silicon, also kitowo as an ingot, is routinely up to 200 mm (8 inches) in diameter and 1 to 2 meters in lengtis. The Si svafers used ix device processieg, such as those previously pictured in Fig. 1.5, are ultimately produced by cutting the ingot ioto thin sections using a diamond-edged saw. 1.3 CRYSTAL GROWTH 1.3.1 Obtaining Ultrapure Si Given tlte obviotts general availability and widespread use of semiconductor materials, par ticularly Si. it is seasonable to wonder about the origin of the single-crystal St used in modern-day device production. Could it be that Si is readily available in sandstone de posits?—No. Perhaps, as a sort of by-product, Si single crystals come from South African dinittond mines?—Wrong again. As suggested recently in a low.budgcl science l’tction toovie, maybe Si is scooped front the ocean bottom by special submarines?—Sorry, no. Althongit Si is the second most abundant element in the earth’s crust and a component in nomeeous compounds, chief of svhich are silica (impure SiO,) and the silicates (St ± 0 + another element), silicon never occurs alone in natore us an eletnent. Single-crystal Si used in device production, it turns out, is a man-made material. Given the preceding introduction, it should be clear that Ihe initial step in producing desicc-qnality silicon must involve separating Si from its comnoonds and purifying the www.EasyEngineering.net 18 SEMICONDUCTOR FUNDAMENTALS unMicoNoucroRn: A GENERAL INTRODUC110N - 1.4 SUMMARY This chapter provides basic information about semicondnctors in general aitd silicon in particular. Esansluing the elemental cotnpouitionn of semiconductors. one finds that Iltere are. on average, four valence electrons per atom. Moreover, device-quality semiconductors are typically single crystals of high compositional parity. Si crystalltzes in the diamond lattice. GaAs crystallizes in the ainchlende lattice, and Ike lattice atoms in both cases have four nearest neighbors. Miller indices, introduced herein us an adjunct to the crystal struc ture discnssion. ate the accepted means for identifying planes and directious within a crystal. Finally. large single crystals of device-grade Si are commonly produced by the Czochralski method. ww w PROBLEMS .Ea CHAPTER I P syE ngi hI PROBLEM INFORMATION TABLE Complete Dtfficulty After Level 1.1 1.4 1 • 1.5 1.2.4 2—3 •H’ nee rin g 1.6 Figure 1.9 Sitienir crystal-palling oppara toe and resulting singie crystal. (a) Photo grip> sfa compntemr-cisuirollcd Ccochratski ci’ysrat pallor. )h) Sinipli)ind scbamuiic dma’ingot the paller. Ic) Sitiauo ingot. ha) and Ic) courtesy of Wacker Silrmsroiu. )b) From Zahlehncr and Habar ; reprinted mm oirlr permission.) .ne t Photographs Suggested Point Weighuing tO (a:h-l. i-2) S/lore Description Short answer res’iew Nearn;borl 15 (a-2, b-2, c-3, d-3, e-y) A,utos/cm on planes 1 t (2 each subpart) 1.7 “ I 16 (2 each purl) Given (hkl), sketch plane 1.8 “ 1 16 (2 each purl) Given I hkl], sketch direction 1 8 (4 each pan) Perpendicular directions 1.10 “ 2 10 Direction on wafer surface Consbination question 1.9 Determine Miller indices III “ 2 10 (a-S. b-2, e-3. d-2) 1,12 “ 2 12(2 each part) Eqaivulent planes/directions 1.13 1.2.3 3 20 (5 each part) % of volume occupied 1.1 Quick Quiz. Answer the follosving questions as concisely as possible. (a) Name (i) oue elemental semiconductor and (ii) one Ill-V catnpuultd semicunductor. (b) What is the difference between a crystalline and a polycrystalline material? (c) Give a word definition of unit cell. )d) How many atomns are there io a simple cubic unit cell? in u her unit cell? unit cell? in the unit cell ritaracterizing the diamottd lattice? www.EasyEngineering.net in a fcc 19 16 SEMICONDUCTOR FUNDAMENTALS SEMICONDUCTORS: A GENERAL INTRODUCTION S: (a) The Intercepts of the platte are I. I, antI 2 along the x. y, and e eaorthOatc axes, respectively. Taking [l/intcrceptls yields I, I, 1/2. Multiplying by 2 to obtatit the lossest whole-number set, aitd enelostng itt parentheses, gives for Site Miller indices of the plane. TIte direction vector has projections of 2 u, a. attd 0 along the a, y, aitd coordiitatc axes, respectively. Tite Miller indices for the direction are then J. 17 — sari, — S:Iiva — Rntucvd is pmrsrrvs nrC (b) For the (Oil) plane, [1/interceptls 0, 1, 1. The normalized a, y, intercepts of the plane are Ilterefore m, I, I; the plane intersects the y-axis at a, intersects the c-axis air,, and is parallel to Site a-axis. In acubic crystal the [Oil) direction is normal to tile (fill) plane. The dedneed plane and directiots arc as sketched in Fig. El.4(b). Chior,nurnd ..._.[Zi a 0 aru Disi,iied, eta. øj pornn fieduard iv imydrognr atmosphere Figure 1,8 Summary of lie process osnployed to produce ultrapure silicon. z separated material. The ingcnioas separation and purification process that has evolved is saimrritarizcd is Fig. 1.8. Low-grade silicon or ferrosilticun is first produced by heating silica ss’ith carbon in an electric furnace. The carbon essentially pails tlte oxygen away from Ilte impure SiC, (i.e., redace.s the SiO,), leaving behind impure Si. Nest, the ferrosilicon is cltlorinated to yield SiCI 4 or SiRCI,, both of wltich are liquids at room temperature Al lhonglt appeariug odd al first glance, the liqtiefactiou process is actually a clever maneuver. Whereas solids are very difiicalt to purify. a number of slandard procedures are available for purifying liquids. Au ultrapure SiCla (or SiHCI,) is the sosult after multiple distillation aud other liquid purification procedures. Lastly, the higit-parity halide is chentically re duced, yielding the desired ultrapure elemental silicou. TIus is accomplished, for example, by heating SiCI 5 in a hydrogen atmosphere [SiCI 5 + 2Ha 4 HCI + Si). 5 (a) (b) Figure E1.4 1.3.2 Single-Crystal Formation Although ultrapure, the silicon derived from the separation and purification process as just described is not a single crystal, but is iastead polycrystalline. Additional processing is ilserefore required to form the large single crystals used in device fabrication. The most coiunsanly employed method yielding large sittgle crystals of Si is known as the Czochral. ski method. In this uiel)mod the altraparu polycrystalliue silicott is placed in a quartz cru cible and heated juan ittert atmosphere to form a melt, as shown in Fig. 1.9. A small single crystal, or Si “seed” crystal, with the normal to its bottom face carefully aligned along a predetermined dinectiox (typically a Ut I) or (lOG) ditection). is then clamped lou metal rod and dipped into the melt. Once thermal equilibrium is established, the temperature of the nelt in the vicinity of the seed crystal is reduced, and silieou from thu melt begins to freeze 0111 onto tite seed crystal, the added material being a structurally perfect extension of the seed crystal. Subsequeittly. the seed crystal is slowly rotated and withdrawn from the melt; this permits store and inure silicou to freeze ovit on the boltom of rIte growing crystal. A pitotograph shosvjng a crystal after being pulled from the melt is displayed in Fig. 1.9(c). Toe large, cylindrically shaped single crystal of silicon, also kitowo as an ingot, is routinely up to 200 mm (8 inches) in diameter and 1 to 2 meters in lengtis. The Si svafers used ix device processieg, such as those previously pictured in Fig. 1.5, are ultimately produced by cutting the ingot ioto thin sections using a diamond-edged saw. 1.3 CRYSTAL GROWTH 1.3.1 Obtaining Ultrapure Si Given tlte obviotts general availability and widespread use of semiconductor materials, par ticularly Si. it is seasonable to wonder about the origin of the single-crystal St used in modern-day device production. Could it be that Si is readily available in sandstone de posits?—No. Perhaps, as a sort of by-product, Si single crystals come from South African dinittond mines?—Wrong again. As suggested recently in a low.budgcl science l’tction toovie, maybe Si is scooped front the ocean bottom by special submarines?—Sorry, no. Althongit Si is the second most abundant element in the earth’s crust and a component in nomeeous compounds, chief of svhich are silica (impure SiO,) and the silicates (St ± 0 + another element), silicon never occurs alone in natore us an eletnent. Single-crystal Si used in device production, it turns out, is a man-made material. Given the preceding introduction, it should be clear that Ihe initial step in producing desicc-qnality silicon must involve separating Si from its comnoonds and purifying the www.EasyEngineering.net 18 SEMICONDUCTOR FUNDAMENTALS 19 unMicoNoucroRn: A GENERAL INTRODUC110N - 1.4 SUMMARY This chapter provides basic information about semicondnctors in general aitd silicon in particular. Esansluing the elemental cotnpouitionn of semiconductors. one finds that Iltere are. on average, four valence electrons per atom. Moreover, device-quality semiconductors are typically single crystals of high compositional parity. Si crystalltzes in the diamond lattice. GaAs crystallizes in the ainchlende lattice, and Ike lattice atoms in both cases have four nearest neighbors. Miller indices, introduced herein us an adjunct to the crystal struc ture discnssion. ate the accepted means for identifying planes and directious within a crystal. Finally. large single crystals of device-grade Si are commonly produced by the Czochralski method. ww w.E PROBLEMS CHAPTER I P hI PROBLEM INFORMATION TABLE 1.1 1.4 • 1.5 1.2.4 •H’ 1.6 Figure 1.9 Sitienir crystal-palling oppara toe and resulting singie crystal. (a) Photo grip> sfa compntemr-cisuirollcd Ccochratski ci’ysrat pallor. )h) Sinipli)ind scbamuiic dma’ingot the paller. Ic) Sitiauo ingot. ha) and Ic) courtesy of Wacker Silrmsroiu. )b) From Zahlehncr and Habar ; reprinted mm oirlr permission.) Photographs asy Complete Dtfficulty After Level 1 2—3 Suggested Point Weighuing En tO (a:h-l. i-2) S/lore Description gin Short answer res’iew Nearn;borl eer 15 (a-2, b-2, c-3, d-3, e-y) A,utos/cm on planes 1 t (2 each subpart) 1.7 “ I 16 (2 each purl) 1.8 “ 1 16 (2 each purl) 1 8 (4 each pan) Perpendicular directions 1.10 “ 2 10 Direction on wafer surface 1.9 Determine Miller indices ing Given (hkl), sketch plane .ne Given I hkl], sketch direction III “ 2 10 (a-S. b-2, e-3. d-2) Consbination question 1,12 “ 2 12(2 each part) Eqaivulent planes/directions 1.13 1.2.3 3 20 (5 each part) % of volume occupied 1.1 Quick Quiz. Answer the follosving questions as concisely as possible. (a) Name (i) oue elemental semiconductor and (ii) one Ill-V catnpuultd semicunductor. (b) What is the difference between a crystalline and a polycrystalline material? (c) Give a word definition of unit cell. )d) How many atomns are there io a simple cubic unit cell? in u her unit cell? unit cell? in the unit cell ritaracterizing the diamottd lattice? in a fcc www.EasyEngineering.net t www.EasyEngineering.net 20 SEMICONDUCTOR FUNDAMENTALS SEMICONDUCTORS. A DENERAt, INTRODUCTION (e) iAw?cm. (b) Assuming tite crystal structure to he cubic, deterunne tIre Miller indices for (i) the plane and (ii) the vector pictured iu Fig. P1 fm)b). )f) In terms of the lattice coostaot a, what is the dtstaoce betweeo ocarest.Seighbor stows ia a sittiplc cobic lattice? (g) Floss stony ttearest-ueiglthor atoms are tltete itt the diamond and the eiochlende lattices? (h) What is being indicated by the bracket sets indesing scheme? (). [(, ( vuciut and)) as employed in the Millar (i) Desctibe the Ceochualuki method far obtaining large siSgle crystals of silicoo. 1.2 The GaAs Unit cell is pictured in P. l.4(bl. Describe (or sketch) the unit cell for ww Al G 5 a Au. lul 1.3 (a) The lattice constant ofGe at room tewperatnw is a w.E 1110 ttntttber of Ge atntits/cin . t 1.7 Assuming a cubic crystal system. make a sketch of time following planes. (o) (001), (b) (11 I), (ci (123), (d) (ItO), • (b) Copies of computer-required exercises etoployitmg MArt.Ao are included on disk. Run the Eoercise .3 program to verify your resolt frota part (a). as y En gin e (e) (010), 1.4 In teruts of the lattire cottstant a, what is the distance between oearcst’netghbor atoms in (a) a hcc lattice? (b) an fcc lattice? ng. ne (a) Sketch the placement of Si atoms on the surface of the suafee. (b) Detenittine the number of atattis per cwt at tlte surface of the wafer. (c) 1(d) Repeat parts (a) and (b), this time taking the surface of the Si wafer to be a (110) plane. • )e) Primarily for practice in utilieing MATLAR, construct a MAmAS program that corn pntes the narface deusity of atoms on (100) planet of cubic crystals. The number of utotna with centers on the (100) face of the unit cell, and the lattice constant tn A, are to be lie input oariablex. Confirm the result obtained manually in part (b). (f( (iii), (g) (221), (h) lOb). 0.8 Assurnttig a cubic crystal system, use an appropriately directed arrow so ideusify each of the following directions: eri 1.5 The surface of a Si wafer is a (100) plane. hbl Figure P1.6 5.63 X lO cm. Dntcrmtoe (a) [010). (b) (101), (c) 00), (dl (I II), (e) [001), (0 (g) (OtO), (h) (123). (110), 1.9 Identify two crystalline directions in a cubic crystal which are perpendicular tu (a) the (100) direcrion, t (h) the jlll[directioe. NOTE: The cosine of the angle 6 between two arbitrary directions, (h. O in a cubic crystal is cos(6) — — 0], 0 1) and [%k + /5ika + t a 1 i ((h’g+k) ± i))(ht) + 62 +h9) Conseqaenrly, foe two directions to be perpendicular, coa(O) 0 und one must have 1.6 Record all intermediate steps in anuseeriug the following questions. hIi, + ‘i a + t 6 a 1 i (a) As ultuwu in Fig. P1.6(a), u crystalline plane has intercepts of In. 3a, uod In on the x, y, ued cases, respectively, a is the cubic cell tide length. 1.10 As pictured in Pig. 1.5, (01 I (is the direction in the surface plane nurmal to the major fiat wheit the surface of the Si wafer in a (100) plane. To construct a particular deuicu structure, a parallel set of grooves must be etched in the (100) surface plane along ihe (010) direction. Make a sketch indicating how the grooves are to be oriented on the wafer’s 5crfoce. Enplaia how you arrived at your sketch. (i) What is the Miller indes notation for the pluue? (6) What is the Miller mdcc notation for the direction normal to the plane? 0. www.EasyEngineering.net 2 SEMiCONDUCTOR FaRnAMEIrrALS v 1.11 A crystalline lattice is churacterieed by the cubic unit cell pictured itt Pig. P1.11. The cell has a single atom positioned at the center of the cobe. 2 Carrier Modeling Carriers are the estmtirs that transport charge from place to place inside a material and bruce give rise In electrical currents. to everyday life the most commonly encountered type of carrier is the electron, the sobotomic particle responsible for charge trausport in metallic wires Withiu semiconductors one again encounters the familiar electron, but there is also a second equally important type of carrier—the hole. Electrons and holes we the focal Figure P1.11 (a) What is the uause of the lattice generated by the given unit cell? (b) Deterntiiir the uuniber of atoms per urit volume in the crystal. (Your answer should be in terms of the lattice constant. u.) (c) Suppose the crystol hot a (110) sorface plane. Determine thu number of atoms per nuit area whose centers lie on the (110) plane. (d) A direction vector is drason through the center of the atom io the unit cell. Specify the Miller indices of the direction vector. 41.12 Given a cobic lattice. itidicatu how many equivaleot planes (parts (a) tO (c)( uruqaiva lent directions (parts (d) to (f)) are associated with each of the fottowing desigeationu: (a) (100), (b) (110), (c) (Ill), (d) (100), (e) (110), (f) (Ill). 1.13 Treaaitg atoms as rigid spheres with radii equal to one-half the distance bcoveen nearest neighbors, show that the ratio of the volume occupied by the atoms to the coral available volame in the various crystal stracturut is (a) n/fl or 52% for the sinsple cubic lattice. (b) ‘s/In/fl or 6fl% for the body centered cubic lattice. (c) /Ia’/fl or 74% for the face cestered cabic lattice. point of this chapter, wherein we examine carrier related concepts, models. properlics, and terminology. Although reminders will be periodically intetjected. it should be emphasieed from the very start that the development throughout this chapter assumes eqaiIibriam couditious esint withia the semiconductor. “Equihibriam” is the term used to describe the unperturbed state of a system. Under eqoitibriam conditines there are no external voltages, maguetic fields, tlresses, or other perturbing forces acting on the semiconductor. All ubservables are ievariaat with time. This ‘rest” condition, as me will see, provides an encellcutfrumc of reference. lieing able to eharactenice thu semiconductor nuder equihibriam conditions perwits one to extrapolate and ascertain the semicnuductor’s condition when a perturbation has been applied. The reader should be foressarncd that a number of formulun and facts will be presented mithootjustificntiou in this chapter. We would like to provide a complele discussion, prop erly developing every concept and deriving every formula. Uafortasatcly, this is sot pos sible. It in our ummderlying phrilosophy, moreover, Ihot being able to derive a result is second ary to katowing how to immmcmprem and San a result One can, of rosrse, fill ie any information gap tlrroogh snpptrmeemal readmugs Por suggested references see the napplementoh reading list am the end of Part I Lantly pleauc Role that Appc’adot A irn’rideu a jjloreiolaAepfili uflfio*tCdibn. le the qjnantiiatnun concept ppd related tu,pie.4 h s4IJlc4el jgasAetJblPL ar ‘ecttun 2J maylae replaced by Appindirç A wIIinuiom )n.gntinukfy. 1’ — (d) ‘s/In! 16 or 34% for the diamond lattice. 2.1 THE QUANTIZATION CONCEPT luttead of attempting to deal immediately with electrons in crystalline Si, where there are Id electrons per atom and 5 X tO atoms/cm , sve will taken more realistic approach and t first establish certain ground rules by esamining much simpler otowic systems. We begin 21 www.EasyEngineering.net 20 SEMICONDUCTOR FUNDAMENTALS SEMICONDUCTORS. A DENERAt, INTRODUCTION (e) iAw?cm. )f) In terms of the lattice coostaot a, what is the dtstaoce betweeo ocarest.Seighbor stows ia a sittiplc cobic lattice? (b) Assuming tite crystal structure to he cubic, deterunne tIre Miller indices for (i) the plane and (ii) the vector pictured iu Fig. P1 fm)b). (g) Floss stony ttearest-ueiglthor atoms are tltete itt the diamond and the eiochlende lattices? (h) What is being indicated by the bracket sets indesing scheme? (). [(, ( vuciut and)) as employed in the Millar (i) Desctibe the Ceochualuki method far obtaining large siSgle crystals of silicoo. 1.2 The GaAs Unit cell is pictured in P. l.4(bl. Describe (or sketch) the unit cell for Al G 5 a Au. 1.3 (a) The lattice constant ofGe at room tewperatnw is a 5.63 X lO cm. Dntcrmtoe 1110 ttntttber of Ge atntits/cin . t • (b) Copies of computer-required exercises etoployitmg MArt.Ao are included on disk. Run the Eoercise .3 program to verify your resolt frota part (a). ww lul w.E a 1.7 Assuming a cubic crystal system. make a sketch of time following planes. (o) (001), (b) (11 I), (ci (123), (d) (ItO), syE ngi (e) (010), 1.4 In teruts of the lattire cottstant a, what is the distance between oearcst’netghbor atoms in (a) a hcc lattice? (f( (iii), (g) (221), (h) lOb). 0.8 Assurnttig a cubic crystal system, use an appropriately directed arrow so ideusify each of the following directions: (b) an fcc lattice? 1.5 The surface of a Si wafer is a (100) plane. hbl Figure P1.6 nee r (a) [010). (b) (101), (c) 00), (dl (I II), (e) [001), (0 (g) (OtO), (h) (123). (110), ing . 1.9 Identify two crystalline directions in a cubic crystal which are perpendicular tu (a) Sketch the placement of Si atoms on the surface of the suafee. (b) Detenittine the number of atattis per cwt at tlte surface of the wafer. (h) the jlll[directioe. (c) 1(d) Repeat parts (a) and (b), this time taking the surface of the Si wafer to be a (110) plane. NOTE: The cosine of the angle 6 between two arbitrary directions, (h. O in a cubic crystal is (a) the (100) direcrion, • )e) Primarily for practice in utilieing MATLAR, construct a MAmAS program that corn pntes the narface deusity of atoms on (100) planet of cubic crystals. The number of utotna with centers on the (100) face of the unit cell, and the lattice constant tn A, are to be lie input oariablex. Confirm the result obtained manually in part (b). cos(6) — — + /5ika + t a 1 i ((h’g+k) ± i))(ht) + 62 net 0], 0 1) and [%k +h9) Conseqaenrly, foe two directions to be perpendicular, coa(O) 0 und one must have 1.6 Record all intermediate steps in anuseeriug the following questions. hIi, + ‘i a + t 6 a 1 i (a) As ultuwu in Fig. P1.6(a), u crystalline plane has intercepts of In. 3a, uod In on the x, y, ued cases, respectively, a is the cubic cell tide length. 1.10 As pictured in Pig. 1.5, (01 I (is the direction in the surface plane nurmal to the major fiat wheit the surface of the Si wafer in a (100) plane. To construct a particular deuicu structure, a parallel set of grooves must be etched in the (100) surface plane along ihe (010) direction. Make a sketch indicating how the grooves are to be oriented on the wafer’s 5crfoce. Enplaia how you arrived at your sketch. (i) What is the Miller indes notation for the pluue? (6) What is the Miller mdcc notation for the direction normal to the plane? 0. www.EasyEngineering.net 2 SEMiCONDUCTOR FaRnAMEIrrALS v 1.11 A crystalline lattice is churacterieed by the cubic unit cell pictured itt Pig. P1.11. The cell has a single atom positioned at the center of the cobe. 2 Carrier Modeling Carriers are the estmtirs that transport charge from place to place inside a material and bruce give rise In electrical currents. to everyday life the most commonly encountered type of carrier is the electron, the sobotomic particle responsible for charge trausport in metallic wires Withiu semiconductors one again encounters the familiar electron, but there is also a second equally important type of carrier—the hole. Electrons and holes we the focal Figure P1.11 (a) What is the uause of the lattice generated by the given unit cell? (b) Deterntiiir the uuniber of atoms per urit volume in the crystal. (Your answer should be in terms of the lattice constant. u.) (c) Suppose the crystol hot a (110) sorface plane. Determine thu number of atoms per nuit area whose centers lie on the (110) plane. (d) A direction vector is drason through the center of the atom io the unit cell. Specify the Miller indices of the direction vector. 41.12 Given a cobic lattice. itidicatu how many equivaleot planes (parts (a) tO (c)( uruqaiva lent directions (parts (d) to (f)) are associated with each of the fottowing desigeationu: (a) (100), (b) (110), (c) (Ill), (d) (100), (e) (110), (f) (Ill). 1.13 Treaaitg atoms as rigid spheres with radii equal to one-half the distance bcoveen nearest neighbors, show that the ratio of the volume occupied by the atoms to the coral available volame in the various crystal stracturut is (a) n/fl or 52% for the sinsple cubic lattice. (b) ‘s/In/fl or 6fl% for the body centered cubic lattice. (c) /Ia’/fl or 74% for the face cestered cabic lattice. point of this chapter, wherein we examine carrier related concepts, models. properlics, and terminology. Although reminders will be periodically intetjected. it should be emphasieed from the very start that the development throughout this chapter assumes eqaiIibriam couditious esint withia the semiconductor. “Equihibriam” is the term used to describe the unperturbed state of a system. Under eqoitibriam conditines there are no external voltages, maguetic fields, tlresses, or other perturbing forces acting on the semiconductor. All ubservables are ievariaat with time. This ‘rest” condition, as me will see, provides an encellcutfrumc of reference. lieing able to eharactenice thu semiconductor nuder equihibriam conditions perwits one to extrapolate and ascertain the semicnuductor’s condition when a perturbation has been applied. The reader should be foressarncd that a number of formulun and facts will be presented mithootjustificntiou in this chapter. We would like to provide a complele discussion, prop erly developing every concept and deriving every formula. Uafortasatcly, this is sot pos sible. It in our ummderlying phrilosophy, moreover, Ihot being able to derive a result is second ary to katowing how to immmcmprem and San a result One can, of rosrse, fill ie any information gap tlrroogh snpptrmeemal readmugs Por suggested references see the napplementoh reading list am the end of Part I Lantly pleauc Role that Appc’adot A irn’rideu a jjloreiolaAepfili uflfio*tCdibn. le the qjnantiiatnun concept ppd related tu,pie.4 h s4IJlc4el jgasAetJblPL ar ‘ecttun 2J maylae replaced by Appindirç A wIIinuiom )n.gntinukfy. 1’ — (d) ‘s/In! 16 or 34% for the diamond lattice. 2.1 THE QUANTIZATION CONCEPT luttead of attempting to deal immediately with electrons in crystalline Si, where there are Id electrons per atom and 5 X tO atoms/cm , sve will taken more realistic approach and t first establish certain ground rules by esamining much simpler otowic systems. We begin 21 20 SEMICONDUCTOR FUNDAMENTALS SEMICONDUCTORS. A DENERAt, INTRODUCTION (e) iAw?cm. )f) In terms of the lattice coostaot a, what is the dtstaoce betweeo ocarest.Seighbor stows ia a sittiplc cobic lattice? (b) Assuming tite crystal structure to he cubic, deterunne tIre Miller indices for (i) the plane and (ii) the vector pictured iu Fig. P1 fm)b). (g) Floss stony ttearest-ueiglthor atoms are tltete itt the diamond and the eiochlende lattices? (h) What is being indicated by the bracket sets indesing scheme? (). [(, ( vuciut and)) as employed in the Millar (i) Desctibe the Ceochualuki method far obtaining large siSgle crystals of silicoo. 1.2 The GaAs Unit cell is pictured in P. l.4(bl. Describe (or sketch) the unit cell for Al G 5 a Au. lul 1.3 (a) The lattice constant ofGe at room tewperatnw is a hbl Figure P1.6 5.63 X lO cm. Dntcrmtoe 1110 ttntttber of Ge atntits/cin . t • (b) Copies of computer-required exercises etoployitmg MArt.Ao are included on disk. Run the Eoercise .3 program to verify your resolt frota part (a). 1.7 Assuming a cubic crystal system. make a sketch of time following planes. (o) (001), (b) (11 I), (ci (123), (d) (ItO), (e) (010), 1.4 In teruts of the lattire cottstant a, what is the distance between oearcst’netghbor atoms in (a) a hcc lattice? (b) an fcc lattice? 1.5 The surface of a Si wafer is a (100) plane. (f( (iii), (g) (221), (h) lOb). 0.8 Assurnttig a cubic crystal system, use an appropriately directed arrow so ideusify each of the following directions: (a) [010). (b) (101), (c) 00), (dl (I II), (e) [001), (0 (g) (OtO), (h) (123). (110), 1.9 Identify two crystalline directions in a cubic crystal which are perpendicular tu (a) Sketch the placement of Si atoms on the surface of the suafee. (b) Detenittine the number of atattis per cwt at tlte surface of the wafer. (a) the (100) direcrion, (c) 1(d) Repeat parts (a) and (b), this time taking the surface of the Si wafer to be a (110) plane. • )e) Primarily for practice in utilieing MATLAR, construct a MAmAS program that corn pntes the narface deusity of atoms on (100) planet of cubic crystals. The number of utotna with centers on the (100) face of the unit cell, and the lattice constant tn A, are to be lie input oariablex. Confirm the result obtained manually in part (b). (h) the jlll[directioe. NOTE: The cosine of the angle 6 between two arbitrary directions, (h. O in a cubic crystal is cos(6) — — 0], 0 1) and [%k + /5ika + t a 1 i ((h’g+k) ± i))(ht) + 62 +h9) Conseqaenrly, foe two directions to be perpendicular, coa(O) 0 und one must have 1.6 Record all intermediate steps in anuseeriug the following questions. hIi, + ‘i a + t 6 a 1 i (a) As ultuwu in Fig. P1.6(a), u crystalline plane has intercepts of In. 3a, uod In on the x, y, ued cases, respectively, a is the cubic cell tide length. 1.10 As pictured in Pig. 1.5, (01 I (is the direction in the surface plane nurmal to the major fiat wheit the surface of the Si wafer in a (100) plane. To construct a particular deuicu structure, a parallel set of grooves must be etched in the (100) surface plane along ihe (010) direction. Make a sketch indicating how the grooves are to be oriented on the wafer’s 5crfoce. Enplaia how you arrived at your sketch. (i) What is the Miller indes notation for the pluue? (6) What is the Miller mdcc notation for the direction normal to the plane? 0. www.EasyEngineering.net 2 SEMiCONDUCTOR FaRnAMEIrrALS v 1.11 A crystalline lattice is churacterieed by the cubic unit cell pictured itt Pig. P1.11. The cell has a single atom positioned at the center of the cobe. ww w 2 Carrier Modeling Carriers are the estmtirs that transport charge from place to place inside a material and bruce give rise In electrical currents. to everyday life the most commonly encountered type of carrier is the electron, the sobotomic particle responsible for charge trausport in metallic wires Withiu semiconductors one again encounters the familiar electron, but there is also a second equally important type of carrier—the hole. Electrons and holes we the focal point of this chapter, wherein we examine carrier related concepts, models. properlics, and terminology. Figure P1.11 .Ea (a) What is the uause of the lattice generated by the given unit cell? (b) Deterntiiir the uuniber of atoms per urit volume in the crystal. (Your answer should be syE in terms of the lattice constant. u.) (c) Suppose the crystol hot a (110) sorface plane. Determine thu number of atoms per nuit area whose centers lie on the (110) plane. ngi (d) A direction vector is drason through the center of the atom io the unit cell. Specify the Miller indices of the direction vector. nee rin g 41.12 Given a cobic lattice. itidicatu how many equivaleot planes (parts (a) tO (c)( uruqaiva lent directions (parts (d) to (f)) are associated with each of the fottowing desigeationu: (a) (100), (b) (110), (c) (Ill), (d) (100), (e) (110), (f) (Ill). .ne t 1.13 Treaaitg atoms as rigid spheres with radii equal to one-half the distance bcoveen nearest neighbors, show that the ratio of the volume occupied by the atoms to the coral available volame in the various crystal stracturut is (a) n/fl or 52% for the sinsple cubic lattice. (b) ‘s/In/fl or 6fl% for the body centered cubic lattice. (c) /Ia’/fl or 74% for the face cestered cabic lattice. Although reminders will be periodically intetjected. it should be emphasieed from the very start that the development throughout this chapter assumes eqaiIibriam couditious esint withia the semiconductor. “Equihibriam” is the term used to describe the unperturbed state of a system. Under eqoitibriam conditines there are no external voltages, maguetic fields, tlresses, or other perturbing forces acting on the semiconductor. All ubservables are ievariaat with time. This ‘rest” condition, as me will see, provides an encellcutfrumc of reference. lieing able to eharactenice thu semiconductor nuder equihibriam conditions perwits one to extrapolate and ascertain the semicnuductor’s condition when a perturbation has been applied. The reader should be foressarncd that a number of formulun and facts will be presented mithootjustificntiou in this chapter. We would like to provide a complele discussion, prop erly developing every concept and deriving every formula. Uafortasatcly, this is sot pos sible. It in our ummderlying phrilosophy, moreover, Ihot being able to derive a result is second ary to katowing how to immmcmprem and San a result One can, of rosrse, fill ie any information gap tlrroogh snpptrmeemal readmugs Por suggested references see the napplementoh reading list am the end of Part I Lantly pleauc Role that Appc’adot A irn’rideu a jjloreiolaAepfili uflfio*tCdibn. le the qjnantiiatnun concept ppd related tu,pie.4 h s4IJlc4el jgasAetJblPL ar ‘ecttun 2J maylae replaced by Appindirç A wIIinuiom )n.gntinukfy. 1’ — (d) ‘s/In! 16 or 34% for the diamond lattice. 2.1 THE QUANTIZATION CONCEPT luttead of attempting to deal immediately with electrons in crystalline Si, where there are Id electrons per atom and 5 X tO atoms/cm , sve will taken more realistic approach and t first establish certain ground rules by esamining much simpler otowic systems. We begin www.EasyEngineering.net 21 20 SEMICONDUCTOR FUNDAMENTALS SEMICONDUCTORS. A DENERAt, INTRODUCTION (e) iAw?cm. )f) In terms of the lattice coostaot a, what is the dtstaoce betweeo ocarest.Seighbor stows ia a sittiplc cobic lattice? (b) Assuming tite crystal structure to he cubic, deterunne tIre Miller indices for (i) the plane and (ii) the vector pictured iu Fig. P1 fm)b). (g) Floss stony ttearest-ueiglthor atoms are tltete itt the diamond and the eiochlende lattices? (h) What is being indicated by the bracket sets indesing scheme? (). [(, ( vuciut and)) as employed in the Millar (i) Desctibe the Ceochualuki method far obtaining large siSgle crystals of silicoo. 1.2 The GaAs Unit cell is pictured in P. l.4(bl. Describe (or sketch) the unit cell for Al G 5 a Au. lul 1.3 (a) The lattice constant ofGe at room tewperatnw is a hbl Figure P1.6 5.63 X lO cm. Dntcrmtoe 1110 ttntttber of Ge atntits/cin . t • (b) Copies of computer-required exercises etoployitmg MArt.Ao are included on disk. Run the Eoercise .3 program to verify your resolt frota part (a). 1.7 Assuming a cubic crystal system. make a sketch of time following planes. (o) (001), (b) (11 I), (ci (123), (d) (ItO), (e) (010), 1.4 In teruts of the lattire cottstant a, what is the distance between oearcst’netghbor atoms in (a) a hcc lattice? (b) an fcc lattice? 1.5 The surface of a Si wafer is a (100) plane. (f( (iii), (g) (221), (h) lOb). 0.8 Assurnttig a cubic crystal system, use an appropriately directed arrow so ideusify each of the following directions: (a) [010). (b) (101), (c) 00), (dl (I II), (e) [001), (0 (g) (OtO), (h) (123). (110), 1.9 Identify two crystalline directions in a cubic crystal which are perpendicular tu (a) Sketch the placement of Si atoms on the surface of the suafee. (b) Detenittine the number of atattis per cwt at tlte surface of the wafer. (a) the (100) direcrion, (c) 1(d) Repeat parts (a) and (b), this time taking the surface of the Si wafer to be a (110) plane. • )e) Primarily for practice in utilieing MATLAR, construct a MAmAS program that corn pntes the narface deusity of atoms on (100) planet of cubic crystals. The number of utotna with centers on the (100) face of the unit cell, and the lattice constant tn A, are to be lie input oariablex. Confirm the result obtained manually in part (b). (h) the jlll[directioe. NOTE: The cosine of the angle 6 between two arbitrary directions, (h. O in a cubic crystal is cos(6) + /5ika + t a 1 i — — 0], 0 1) and [%k ((h’g+k) ± i))(ht) + 62 +h9) Conseqaenrly, foe two directions to be perpendicular, coa(O) 0 und one must have 1.6 Record all intermediate steps in anuseeriug the following questions. hIi, + ‘i a + t 6 a 1 i (a) As ultuwu in Fig. P1.6(a), u crystalline plane has intercepts of In. 3a, uod In on the x, y, ued cases, respectively, a is the cubic cell tide length. 1.10 As pictured in Pig. 1.5, (01 I (is the direction in the surface plane nurmal to the major fiat wheit the surface of the Si wafer in a (100) plane. To construct a particular deuicu structure, a parallel set of grooves must be etched in the (100) surface plane along ihe (010) direction. Make a sketch indicating how the grooves are to be oriented on the wafer’s 5crfoce. Enplaia how you arrived at your sketch. (i) What is the Miller indes notation for the pluue? (6) What is the Miller mdcc notation for the direction normal to the plane? 0. www.EasyEngineering.net 2 SEMiCONDUCTOR FaRnAMEIrrALS v 1.11 A crystalline lattice is churacterieed by the cubic unit cell pictured itt Pig. P1.11. The cell has a single atom positioned at the center of the cobe. 2 Carrier Modeling Carriers are the estmtirs that transport charge from place to place inside a material and bruce give rise In electrical currents. to everyday life the most commonly encountered type of carrier is the electron, the sobotomic particle responsible for charge trausport in metallic wires Withiu semiconductors one again encounters the familiar electron, but there is also ww w.E a second equally important type of carrier—the hole. Electrons and holes we the focal Figure P1.11 (a) What is the uause of the lattice generated by the given unit cell? (b) Deterntiiir the uuniber of atoms per urit volume in the crystal. (Your answer should be in terms of the lattice constant. u.) (c) Suppose the crystol hot a (110) sorface plane. Determine thu number of atoms per nuit area whose centers lie on the (110) plane. (d) A direction vector is drason through the center of the atom io the unit cell. Specify the Miller indices of the direction vector. 41.12 Given a cobic lattice. itidicatu how many equivaleot planes (parts (a) tO (c)( uruqaiva lent directions (parts (d) to (f)) are associated with each of the fottowing desigeationu: (a) (100), (b) (110), (c) (Ill), (d) (100), (e) (110), (f) (Ill). 1.13 Treaaitg atoms as rigid spheres with radii equal to one-half the distance bcoveen nearest neighbors, show that the ratio of the volume occupied by the atoms to the coral available volame in the various crystal stracturut is (a) n/fl or 52% for the sinsple cubic lattice. (b) ‘s/In/fl or 6fl% for the body centered cubic lattice. (c) /Ia’/fl or 74% for the face cestered cabic lattice. point of this chapter, wherein we examine carrier related concepts, models. properlics, and terminology. Although reminders will be periodically intetjected. it should be emphasieed from the very start that the development throughout this chapter assumes eqaiIibriam couditious esint withia the semiconductor. “Equihibriam” is the term used to describe the unperturbed state of a system. Under eqoitibriam conditines there are no external voltages, maguetic fields, tlresses, or other perturbing forces acting on the semiconductor. All ubservables are ievariaat with time. This ‘rest” condition, as me will see, provides an encellcutfrumc of reference. lieing able to eharactenice thu semiconductor nuder equihibriam conditions perwits one to extrapolate and ascertain the semicnuductor’s condition when a perturbation has been applied. The reader should be foressarncd that a number of formulun and facts will be presented mithootjustificntiou in this chapter. We would like to provide a complele discussion, prop erly developing every concept and deriving every formula. Uafortasatcly, this is sot pos sible. It in our ummderlying phrilosophy, moreover, Ihot being able to derive a result is second ary to katowing how to immmcmprem and San a result One can, of rosrse, fill ie any information gap tlrroogh snpptrmeemal readmugs Por suggested references see the napplementoh reading list am the end of Part I asy En gin eer ing .ne Lantly pleauc Role that Appc’adot A irn’rideu a jjloreiolaAepfili uflfio*tCdibn. le the qjnantiiatnun concept ppd related tu,pie.4 h s4IJlc4el jgasAetJblPL ar ‘ecttun 2J maylae replaced by Appindirç A wIIinuiom )n.gntinukfy. 1’ — (d) ‘s/In! 16 or 34% for the diamond lattice. 2.1 THE QUANTIZATION CONCEPT luttead of attempting to deal immediately with electrons in crystalline Si, where there are Id electrons per atom and 5 X tO atoms/cm , sve will taken more realistic approach and t first establish certain ground rules by esamining much simpler otowic systems. We begin www.EasyEngineering.net t 21 www.EasyEngineering.net 24 SEMICONDUCTOR FUNDAMENTALS CARRIER MODELING wills the nitsrplens of oIl asattsse sysssmsss, the isolated Isydrogen sstatsn. Tltsr atolls, sIn tise reader may recall frosst a eanene in moderss physics, avon andes intense nernoiny at the ssssrt of she twentieslt seotory. Scientists of that sittne knew the Ityslsagems atovt contained a osg;t lively oltargest particle in orbit oboist a tttare snanrive positively ehstrgesl ttttslestr. Wirsts tlsey sonld 101 eslrlaso was the nolore of the ligltt ettnittsd from sIte rynsettt mites she isydrogett 01001 wan lteated loan elevated testtpevslssre. Specifically, lbs ststissed light was observed at ooly certain discrete wavelossgths; aocordistg to she prevailing iitsory of tlte tints, roiesstistn expected a sotssinoom of wavelengths. 1913 Nssls Salty proposed a salstliott to lbs dilemosa. Bolts hypashenioed thsst tire H- 25 H tilcat sort it odi atolls electron was restricted to rertusiss woll-dehoed orbits; or eqaiv;sletttly, Bolts assomed tlsat she orbiting electron coold take as srnly ssstoiss saisses of ongstlar mnottteotatn. Thin “qsmsmstioasion” ol lbs electron’s ongotlar stsamentnm was, its tore, conpied directly Ia estergy qstststtisatsms As can be readily estoblislted, if she elestromt’r angitlas stsostsentttm in asrastsed ww lobe nls, sisess w.E F19UeR 2.2 For oar pnrposes, Its tttost important idea to he obtaioed frottt the Bohr model is that the energy of electrons in atomic systems is restricted too Ittotted set of valoss.t Relative to the hydrogen atoot. tIne energy level scheme io a toolti-oteetroo otom like stltsoo ts, as one might iotoitivoly espeet. dosidodly more somplos. It is still a relatively easy task, how mq° — = 5 _ n1,2,3,... as y En gin e fin) 0 2(n’s 5 5 mm Setisototic rol:’Osootatior OF as isolated SI atom. i2.l) svhere (also see Fig. 2.1) F 5 is she eleesvoo biadiog energy svillsin she hydrogen atom, ns° in tlse toots of a free electron, q in the mogsitstde ssf Its electronic charge. e iv Ise peresit tsvstv of free space, h ss Planek’s constant, h = h/2or, ostd n is tlts energy qaasmtatn namber or orbit tdsntmflsr. 1eetronoofseV1itannisofenergysstoaltj.bxIll—ssjoalsv. Now, wsth tlss sleetramt limited to sertaiss ettergien inside the Isydrogest stoso. st follows frotts the Bans nsodel thsst the transition from a higlser n to a lower n osbit will relears qmsamsticed energies of light; this explains the obsosvosion of ensitted light at only oersoin discrete wavelsngtlss. eri ng. ne t ever, to dssorihs the saliottt energy-related foatoses of ao isolated siliean atom. As pietored in Fig. 2.2. ten of the 14 Si-atottt electrons oceapy very deep-lying energy levels otsd are ttghtly hoond to the oneleos of the atoto. The binding is so stroneio focI that these ten electrons rottj_ssetttioIIs on gawrbed daring shettrical reactions or normal atom—atom intoeostionn, ssith tlso ten-electron-plns-noclens sombin,ation often being referred In as the otoot. The eetttatntisg fottr Si-otoos electrons, on the other hood, are rothov weakly bostod attd ore colleotively called the volcnsyslsrezrurtykocagao_gLtheie sOsong p.&trtieigotiott jg ehenaioal wastiotto. An stopItosized in Fig 2.2, tlso foss valence eleetroos. if nttpertnsbed. osonpy foor of the eight allowed slots (or states) hosing the nest highest ,enssgy above the deep-lyittg rose levels. Ftnally, we shoald note. for sotopletenoss, tlsat the electronic vonligaratiott in tlss 32-electron Ge-atom (gormaitiam being the ttthor elemental nenticandststar( iv essentially identical to lbs Si-atom sanfigaration except that lbs Go-core ssstttainv 28 eleetsatts. 2.2 SEMICONDUCTOR MODELS Boilditig on the information prevented in psestonv sections. sos tnnxasloee and describe in this nestion tsvo very impartattt tnodsls or vivnalisation aids tttat are stsed extensively in the 10 s —t.atov analysis of vowicondnstor devtsev. The toslnnina of vemicondostoe tttodels in a chapter devoted to carrier nsodelino way appear odd at first glance bat iv actoally qoits appropriate. We are, in effect, modeling the carries “container;’ the sewieondnstor crystal. —s.aav Fieare 2.1 otters TIre hydmurgon atom—idoaltesd sepsosetttasioo nhosvirg she tiwl Ibsen attowod oteoseoe and Iso asonsiatsd energy qoarsiooriotr. rvrtnattv. sot anty ornrtry bus rmrurv rttsnrrhsrp r,shtos sIstine In itnmss.uioed possistns nec qsartssed. An snIde Qoantuce Utectssnims. trio bees durstrpnd so drrsdbe Ar propoesicri and assess of sssioro-airod hstd as study. potholes ova rystsmt www.EasyEngineering.net 26 UEMICGN5OCTOR raNnanEa’rnLn CARRIER MODELING C’ irs to sop so son In of a rarsisordassar fog.. Oil Fiemarn 2.3 Tho bonding model. tot 2,2.1 Bonding Model The isolated St atom, Ge 0 Si atom not interacting with otlser atatos, mat foond to contain foor valence electrons. Si atoms incorporated in the diamond lattice, on the other hand, evltibit a bonding that involvon an attraction betwseo gash atom and its font nearest ttotglt hors (refer to Fig. l.4s). The implication here is that, in going from isolated GIants to the collective esyntollino state, Si atttms same to abase one of their saletsee electrons seitlt each of the font nearest osighbovv. This sovalent bottdittg, as sqoal vhasiog of valence electrons with nearest neighbors, and lbs moss fast that atoson in the diamond lattice Itave foar nearest oeighboss. give rite to the idealised vemisoodnetas representation, the bonding model, shanvo in Fig. 2.3. Bash circle in the Fig. 2.3 bandittg tnstdel represents the sore of a nomi sovdtmetav atotn, while sash line sepsevonts a rhatod valence eleotson. (These are eight lines soovestod to each atom besaare any gives atom oat only sansribnsea fonr shared electrons bat most also aeeeat fonr shared electrons ham adjacent atoms.) The two-dimensiottal satavs of the ntodel in, of soovss, an idealisatian that facilitates mental visnalisatiasv. Alslsongh sooniderable ass will be mode of the bottdittg tnodsl in snbvsqttettt discos siGns, it is ssvertltelern worthwhile at this point to evatnine ratnple appiisatiotts of sha model so provide toots indisotios of the model’s ntility. Two sample applisattona ace prosorted in Fig. 2.4. Iv Fig. 2.dta( we nse the bonding yodel to pistose n paint dsfest, a missing atom, in the louise stmssnrs. In Fig. 2.41b( sen visaaliss ths beeaktng of an atom to-atans hood attd the associated release as freeing of on sleotson. [Bomtd breaking (at T> o K( and defesta asons natnmlly in all semisondnstasa. and hoses (if sve maybe natttewhat avstoritisal( ttte basis model of Ftg. 2.3 is strictly valid for an snttre settntsondastor only at T 0 K svhno the semisandostor iv ssneatiott sontaitta no defects and tto itnptmrity atotns.( 2.2.2 Energy Band Model If any interests mess restricted to describing the spatial aspects of events taking place mithia nemisandostor, the bonding model olono svoold probably be adsqnatn. QUito often. howeves, one is more intoreated in the nmsesgy-selated aspects of an nosat. In vosh instances the botsdiny model, which nays nothing abant electron energies. iv of httle valne and tito ettesgy batsd model besotsass the pritnary vivoalisation aid. O Figure 2.4 Sample atilisation of the bonding model. (01 Visoalieation of n misting atom or poist dofost. (b) Smoking of an atom.to-atom bond and fmeiog of an eteoteos. Let ns bngin the sonseptoal path leading to the energy band asosdel by recalling the sitaation inside an isolated Si atom. Reviewing the Section 2.1 dissnssion, ten nf the 14 electrons maids on isolated Si atam are tightly boond to the nosleas and are anlikely to be significantly pertorbed by normal atom—atom snteroetions. The rematetng foas obeIsant are mthos weakly boond and, if noportarbed, osonpy font of the eight ollawed energy stales immediately above the last ease level. Moreover, it in implicitly nnderstood that the elec tronic energy states within a groap of Si atoms, nay N Si atoms, are all idevtteal—as lang as thn atoms are isolated, that in, foe enoagh apart so that they are 000intnsasting. Given the foregoing knowjsdge of the isolated atotn sitaatian, the qtaevtion neal arises an to whether we coo are the Itnawledge to dedose information ahoot the crystalline slate. Assaredly we cnn omit any farther tnentson of the sore electrons besanse these electrons are not vigniSsantly pestasbed by normal interatomic forces. The opposite, however, is trae of the valence eleetsotnn. If N atoms are brooght into close prasimity (the ease in crystalline Si), is is qoite reasonable to sagest a modification in the energy states of the valence electrons. The modification ih the valense-eleslmn energy slates aetoally known to take place is snnamaeised in Fig. 2.5. Stastiog ssith V-isolated Si atoms, and sonsoplnally bringing the atoons closer and closer together. one hsads -thniastrmlomie forces lead IT a progressive spread in the allowed energies.. The spread in energies giver rise to slosoly spaced sets of allofrgdstatesknawn as eoevgv baodn. At the interatomic distance eossospoodirg to the Si lattice spacing, the distrihotian of allowed slales consists of two bands seposaled by an interseaing energy gap. The apper band nf allowed states is called the soodttstmost band; the lower band of allowed states, the valence bond; and the intervening energy gap, the forbidden gap or band gop. In filling the allowed energy band states, electrons tend to gravitate In the lawmt possible energies. Notingthat electrons are eesrrieted to single os enpansy in allowed states (the Pooh ovolnsion principle) and rsmaemhesiog that the 4ff valence band states san joso accommodate what were formerly 4ff valence electrons, we typically find that the valence band is almost completely filled with electrons and the 27 www.EasyEngineering.net 24 SEMICONDUCTOR FUNDAMENTALS CARRIER MODELING wills the nitsrplens of oIl asattsse sysssmsss, the isolated Isydrogen sstatsn. Tltsr atolls, sIn tise reader may recall frosst a eanene in moderss physics, avon andes intense nernoiny at the ssssrt of she twentieslt seotory. Scientists of that sittne knew the Ityslsagems atovt contained a osg;t lively oltargest particle in orbit oboist a tttare snanrive positively ehstrgesl ttttslestr. Wirsts tlsey sonld 101 eslrlaso was the nolore of the ligltt ettnittsd from sIte rynsettt mites she isydrogett 01001 wan lteated loan elevated testtpevslssre. Specifically, lbs ststissed light was observed at ooly certain discrete wavelossgths; aocordistg to she prevailing iitsory of tlte tints, roiesstistn expected a sotssinoom of wavelengths. 1913 Nssls Salty proposed a salstliott to lbs dilemosa. Bolts hypashenioed thsst tire H- 25 H tilcat sort it odi atolls electron was restricted to rertusiss woll-dehoed orbits; or eqaiv;sletttly, Bolts assomed tlsat she orbiting electron coold take as srnly ssstoiss saisses of ongstlar mnottteotatn. Thin “qsmsmstioasion” ol lbs electron’s ongotlar stsamentnm was, its tore, conpied directly Ia estergy qstststtisatsms As can be readily estoblislted, if she elestromt’r angitlas stsostsentttm in asrastsed lobe nls, sisess mq° — fin) 0 2(n’s 5 = 5 _ 5 mm n1,2,3,... i2.l) svhere (also see Fig. 2.1) F 5 is she eleesvoo biadiog energy svillsin she hydrogen atom, ns° in tlse toots of a free electron, q in the mogsitstde ssf Its electronic charge. e iv Ise peresit tsvstv of free space, h ss Planek’s constant, h = h/2or, ostd n is tlts energy qaasmtatn namber or orbit tdsntmflsr. 1eetronoofseV1itannisofenergysstoaltj.bxIll—ssjoalsv. Now, wsth tlss sleetramt limited to sertaiss ettergien inside the Isydrogest stoso. st follows frotts the Bans nsodel thsst the transition from a higlser n to a lower n osbit will relears qmsamsticed energies of light; this explains the obsosvosion of ensitted light at only oersoin discrete wavelsngtlss. ww F19UeR 2.2 w.E a Setisototic rol:’Osootatior OF as isolated SI atom. For oar pnrposes, Its tttost important idea to he obtaioed frottt the Bohr model is that the energy of electrons in atomic systems is restricted too Ittotted set of valoss.t Relative to the hydrogen atoot. tIne energy level scheme io a toolti-oteetroo otom like stltsoo ts, as one might iotoitivoly espeet. dosidodly more somplos. It is still a relatively easy task, how syE ngi ever, to dssorihs the saliottt energy-related foatoses of ao isolated siliean atom. As pietored in Fig. 2.2. ten of the 14 Si-atottt electrons oceapy very deep-lying energy levels otsd are ttghtly hoond to the oneleos of the atoto. The binding is so stroneio focI that these ten electrons rottj_ssetttioIIs on gawrbed daring shettrical reactions or normal atom—atom intoeostionn, ssith tlso ten-electron-plns-noclens sombin,ation often being referred In as the otoot. The eetttatntisg fottr Si-otoos electrons, on the other hood, are rothov weakly bostod attd ore colleotively called the volcnsyslsrezrurtykocagao_gLtheie sOsong p.&trtieigotiott jg ehenaioal wastiotto. An stopItosized in Fig 2.2, tlso foss valence eleetroos. if nttpertnsbed. osonpy foor of the eight allowed slots (or states) hosing the nest highest ,enssgy above the deep-lyittg rose levels. Ftnally, we shoald note. for sotopletenoss, tlsat the electronic vonligaratiott in tlss 32-electron Ge-atom (gormaitiam being the ttthor elemental nenticandststar( iv essentially identical to lbs Si-atom sanfigaration except that lbs Go-core ssstttainv 28 eleetsatts. nee r ing . net 2.2 SEMICONDUCTOR MODELS Boilditig on the information prevented in psestonv sections. sos tnnxasloee and describe in this nestion tsvo very impartattt tnodsls or vivnalisation aids tttat are stsed extensively in the 10 s —t.atov analysis of vowicondnstor devtsev. The toslnnina of vemicondostoe tttodels in a chapter devoted to carrier nsodelino way appear odd at first glance bat iv actoally qoits appropriate. We are, in effect, modeling the carries “container;’ the sewieondnstor crystal. —s.aav Fieare 2.1 otters TIre hydmurgon atom—idoaltesd sepsosetttasioo nhosvirg she tiwl Ibsen attowod oteoseoe and Iso asonsiatsd energy qoarsiooriotr. rvrtnattv. sot anty ornrtry bus rmrurv rttsnrrhsrp r,shtos sIstine In itnmss.uioed possistns nec qsartssed. An snIde Qoantuce Utectssnims. trio bees durstrpnd so drrsdbe Ar propoesicri and assess of sssioro-airod hstd as study. potholes ova rystsmt www.EasyEngineering.net 26 UEMICGN5OCTOR raNnanEa’rnLn CARRIER MODELING C’ irs to sop so son In of a rarsisordassar fog.. Oil Fiemarn 2.3 Tho bonding model. tot 2,2.1 Bonding Model The isolated St atom, Ge 0 Si atom not interacting with otlser atatos, mat foond to contain foor valence electrons. Si atoms incorporated in the diamond lattice, on the other hand, evltibit a bonding that involvon an attraction betwseo gash atom and its font nearest ttotglt hors (refer to Fig. l.4s). The implication here is that, in going from isolated GIants to the collective esyntollino state, Si atttms same to abase one of their saletsee electrons seitlt each of the font nearest osighbovv. This sovalent bottdittg, as sqoal vhasiog of valence electrons with nearest neighbors, and lbs moss fast that atoson in the diamond lattice Itave foar nearest oeighboss. give rite to the idealised vemisoodnetas representation, the bonding model, shanvo in Fig. 2.3. Bash circle in the Fig. 2.3 bandittg tnstdel represents the sore of a nomi sovdtmetav atotn, while sash line sepsevonts a rhatod valence eleotson. (These are eight lines soovestod to each atom besaare any gives atom oat only sansribnsea fonr shared electrons bat most also aeeeat fonr shared electrons ham adjacent atoms.) The two-dimensiottal satavs of the ntodel in, of soovss, an idealisatian that facilitates mental visnalisatiasv. Alslsongh sooniderable ass will be mode of the bottdittg tnodsl in snbvsqttettt discos siGns, it is ssvertltelern worthwhile at this point to evatnine ratnple appiisatiotts of sha model so provide toots indisotios of the model’s ntility. Two sample applisattona ace prosorted in Fig. 2.4. Iv Fig. 2.dta( we nse the bonding yodel to pistose n paint dsfest, a missing atom, in the louise stmssnrs. In Fig. 2.41b( sen visaaliss ths beeaktng of an atom to-atans hood attd the associated release as freeing of on sleotson. [Bomtd breaking (at T> o K( and defesta asons natnmlly in all semisondnstasa. and hoses (if sve maybe natttewhat avstoritisal( ttte basis model of Ftg. 2.3 is strictly valid for an snttre settntsondastor only at T 0 K svhno the semisandostor iv ssneatiott sontaitta no defects and tto itnptmrity atotns.( 2.2.2 Energy Band Model If any interests mess restricted to describing the spatial aspects of events taking place mithia nemisandostor, the bonding model olono svoold probably be adsqnatn. QUito often. howeves, one is more intoreated in the nmsesgy-selated aspects of an nosat. In vosh instances the botsdiny model, which nays nothing abant electron energies. iv of httle valne and tito ettesgy batsd model besotsass the pritnary vivoalisation aid. O Figure 2.4 Sample atilisation of the bonding model. (01 Visoalieation of n misting atom or poist dofost. (b) Smoking of an atom.to-atom bond and fmeiog of an eteoteos. Let ns bngin the sonseptoal path leading to the energy band asosdel by recalling the sitaation inside an isolated Si atom. Reviewing the Section 2.1 dissnssion, ten nf the 14 electrons maids on isolated Si atam are tightly boond to the nosleas and are anlikely to be significantly pertorbed by normal atom—atom snteroetions. The rematetng foas obeIsant are mthos weakly boond and, if noportarbed, osonpy font of the eight ollawed energy stales immediately above the last ease level. Moreover, it in implicitly nnderstood that the elec tronic energy states within a groap of Si atoms, nay N Si atoms, are all idevtteal—as lang as thn atoms are isolated, that in, foe enoagh apart so that they are 000intnsasting. Given the foregoing knowjsdge of the isolated atotn sitaatian, the qtaevtion neal arises an to whether we coo are the Itnawledge to dedose information ahoot the crystalline slate. Assaredly we cnn omit any farther tnentson of the sore electrons besanse these electrons are not vigniSsantly pestasbed by normal interatomic forces. The opposite, however, is trae of the valence eleetsotnn. If N atoms are brooght into close prasimity (the ease in crystalline Si), is is qoite reasonable to sagest a modification in the energy states of the valence electrons. The modification ih the valense-eleslmn energy slates aetoally known to take place is snnamaeised in Fig. 2.5. Stastiog ssith V-isolated Si atoms, and sonsoplnally bringing the atoons closer and closer together. one hsads -thniastrmlomie forces lead IT a progressive spread in the allowed energies.. The spread in energies giver rise to slosoly spaced sets of allofrgdstatesknawn as eoevgv baodn. At the interatomic distance eossospoodirg to the Si lattice spacing, the distrihotian of allowed slales consists of two bands seposaled by an interseaing energy gap. The apper band nf allowed states is called the soodttstmost band; the lower band of allowed states, the valence bond; and the intervening energy gap, the forbidden gap or band gop. In filling the allowed energy band states, electrons tend to gravitate In the lawmt possible energies. Notingthat electrons are eesrrieted to single os enpansy in allowed states (the Pooh ovolnsion principle) and rsmaemhesiog that the 4ff valence band states san joso accommodate what were formerly 4ff valence electrons, we typically find that the valence band is almost completely filled with electrons and the 27 24 SEMICONDUCTOR FUNDAMENTALS CARRIER MODELING wills the nitsrplens of oIl asattsse sysssmsss, the isolated Isydrogen sstatsn. Tltsr atolls, sIn tise reader may recall frosst a eanene in moderss physics, avon andes intense nernoiny at the ssssrt of she twentieslt seotory. Scientists of that sittne knew the Ityslsagems atovt contained a osg;t lively oltargest particle in orbit oboist a tttare snanrive positively ehstrgesl ttttslestr. Wirsts tlsey sonld 101 eslrlaso was the nolore of the ligltt ettnittsd from sIte rynsettt mites she isydrogett 01001 wan lteated loan elevated testtpevslssre. Specifically, lbs ststissed light was observed at ooly certain discrete wavelossgths; aocordistg to she prevailing iitsory of tlte tints, roiesstistn expected a sotssinoom of wavelengths. 1913 Nssls Salty proposed a salstliott to lbs dilemosa. Bolts hypashenioed thsst tire H- 25 H tilcat sort it odi atolls electron was restricted to rertusiss woll-dehoed orbits; or eqaiv;sletttly, Bolts assomed tlsat she orbiting electron coold take as srnly ssstoiss saisses of ongstlar mnottteotatn. Thin “qsmsmstioasion” ol lbs electron’s ongotlar stsamentnm was, its tore, conpied directly Ia estergy qstststtisatsms As can be readily estoblislted, if she elestromt’r angitlas stsostsentttm in asrastsed F19UeR 2.2 Setisototic rol:’Osootatior OF as isolated SI atom. lobe nls, sisess mq° — fin) 0 2(n’s 5 = n1,2,3,... 5 _ 5 mm i2.l) svhere (also see Fig. 2.1) F 5 is she eleesvoo biadiog energy svillsin she hydrogen atom, ns° in tlse toots of a free electron, q in the mogsitstde ssf Its electronic charge. e iv Ise peresit tsvstv of free space, h ss Planek’s constant, h = h/2or, ostd n is tlts energy qaasmtatn namber or orbit tdsntmflsr. 1eetronoofseV1itannisofenergysstoaltj.bxIll—ssjoalsv. Now, wsth tlss sleetramt limited to sertaiss ettergien inside the Isydrogest stoso. st follows frotts the Bans nsodel thsst the transition from a higlser n to a lower n osbit will relears qmsamsticed energies of light; this explains the obsosvosion of ensitted light at only oersoin discrete wavelsngtlss. For oar pnrposes, Its tttost important idea to he obtaioed frottt the Bohr model is that the energy of electrons in atomic systems is restricted too Ittotted set of valoss.t Relative to the hydrogen atoot. tIne energy level scheme io a toolti-oteetroo otom like stltsoo ts, as one might iotoitivoly espeet. dosidodly more somplos. It is still a relatively easy task, how ever, to dssorihs the saliottt energy-related foatoses of ao isolated siliean atom. As pietored in Fig. 2.2. ten of the 14 Si-atottt electrons oceapy very deep-lying energy levels otsd are ttghtly hoond to the oneleos of the atoto. The binding is so stroneio focI that these ten electrons rottj_ssetttioIIs on gawrbed daring shettrical reactions or normal atom—atom intoeostionn, ssith tlso ten-electron-plns-noclens sombin,ation often being referred In as the otoot. The eetttatntisg fottr Si-otoos electrons, on the other hood, are rothov weakly bostod attd ore colleotively called the volcnsyslsrezrurtykocagao_gLtheie sOsong p.&trtieigotiott jg ehenaioal wastiotto. An stopItosized in Fig 2.2, tlso foss valence eleetroos. if nttpertnsbed. osonpy foor of the eight allowed slots (or states) hosing the nest highest ,enssgy above the deep-lyittg rose levels. Ftnally, we shoald note. for sotopletenoss, tlsat the electronic vonligaratiott in tlss 32-electron Ge-atom (gormaitiam being the ttthor elemental nenticandststar( iv essentially identical to lbs Si-atom sanfigaration except that lbs Go-core ssstttainv 28 eleetsatts. 2.2 SEMICONDUCTOR MODELS Boilditig on the information prevented in psestonv sections. sos tnnxasloee and describe in this nestion tsvo very impartattt tnodsls or vivnalisation aids tttat are stsed extensively in the analysis of vowicondnstor devtsev. The toslnnina of vemicondostoe tttodels in a chapter devoted to carrier nsodelino way appear odd at first glance bat iv actoally qoits appropriate. We are, in effect, modeling the carries “container;’ the sewieondnstor crystal. 10 s —t.atov —s.aav Fieare 2.1 otters TIre hydmurgon atom—idoaltesd sepsosetttasioo nhosvirg she tiwl Ibsen attowod oteoseoe and Iso asonsiatsd energy qoarsiooriotr. rvrtnattv. sot anty ornrtry bus rmrurv rttsnrrhsrp r,shtos sIstine In itnmss.uioed possistns nec qsartssed. An snIde Qoantuce Utectssnims. trio bees durstrpnd so drrsdbe Ar propoesicri and assess of sssioro-airod hstd as study. potholes ova rystsmt www.EasyEngineering.net 26 UEMICGN5OCTOR raNnanEa’rnLn CARRIER MODELING C’ irs to sop so son In of a rarsisordassar fog.. Oil Fiemarn 2.3 Tho bonding model. ww w tot Figure 2.4 2,2.1 Bonding Model dofost. (b) Smoking of an atom.to-atom bond and fmeiog of an eteoteos. The isolated St atom, Ge 0 Si atom not interacting with otlser atatos, mat foond to contain foor valence electrons. Si atoms incorporated in the diamond lattice, on the other hand, evltibit a bonding that involvon an attraction betwseo gash atom and its font nearest ttotglt hors (refer to Fig. l.4s). The implication here is that, in going from isolated GIants to the collective esyntollino state, Si atttms same to abase one of their saletsee electrons seitlt each of the font nearest osighbovv. This sovalent bottdittg, as sqoal vhasiog of valence electrons with nearest neighbors, and lbs moss fast that atoson in the diamond lattice Itave foar nearest oeighboss. give rite to the idealised vemisoodnetas representation, the bonding model, shanvo in Fig. 2.3. Bash circle in the Fig. 2.3 bandittg tnstdel represents the sore of a nomi sovdtmetav atotn, while sash line sepsevonts a rhatod valence eleotson. (These are eight lines soovestod to each atom besaare any gives atom oat only sansribnsea fonr shared electrons bat most also aeeeat fonr shared electrons ham adjacent atoms.) The two-dimensiottal satavs of the ntodel in, of soovss, an idealisatian that facilitates mental visnalisatiasv. Alslsongh sooniderable ass will be mode of the bottdittg tnodsl in snbvsqttettt discos siGns, it is ssvertltelern worthwhile at this point to evatnine ratnple appiisatiotts of sha model so provide toots indisotios of the model’s ntility. Two sample applisattona ace prosorted in Fig. 2.4. Iv Fig. 2.dta( we nse the bonding yodel to pistose n paint dsfest, a missing atom, in the louise stmssnrs. In Fig. 2.41b( sen visaaliss ths beeaktng of an atom to-atans hood attd the associated release as freeing of on sleotson. [Bomtd breaking (at T> o K( and defesta asons natnmlly in all semisondnstasa. and hoses (if sve maybe natttewhat avstoritisal( ttte basis model of Ftg. 2.3 is strictly valid for an snttre settntsondastor only at T 0 K svhno the semisandostor iv ssneatiott sontaitta no defects and tto itnptmrity atotns.( .Ea Sample atilisation of the bonding model. (01 Visoalieation of n misting atom or poist syE ngi nee rin g .ne t 2.2.2 Energy Band Model If any interests mess restricted to describing the spatial aspects of events taking place mithia nemisandostor, the bonding model olono svoold probably be adsqnatn. QUito often. howeves, one is more intoreated in the nmsesgy-selated aspects of an nosat. In vosh instances the botsdiny model, which nays nothing abant electron energies. iv of httle valne and tito ettesgy batsd model besotsass the pritnary vivoalisation aid. O www.EasyEngineering.net Let ns bngin the sonseptoal path leading to the energy band asosdel by recalling the sitaation inside an isolated Si atom. Reviewing the Section 2.1 dissnssion, ten nf the 14 electrons maids on isolated Si atam are tightly boond to the nosleas and are anlikely to be significantly pertorbed by normal atom—atom snteroetions. The rematetng foas obeIsant are mthos weakly boond and, if noportarbed, osonpy font of the eight ollawed energy stales immediately above the last ease level. Moreover, it in implicitly nnderstood that the elec tronic energy states within a groap of Si atoms, nay N Si atoms, are all idevtteal—as lang as thn atoms are isolated, that in, foe enoagh apart so that they are 000intnsasting. Given the foregoing knowjsdge of the isolated atotn sitaatian, the qtaevtion neal arises an to whether we coo are the Itnawledge to dedose information ahoot the crystalline slate. Assaredly we cnn omit any farther tnentson of the sore electrons besanse these electrons are not vigniSsantly pestasbed by normal interatomic forces. The opposite, however, is trae of the valence eleetsotnn. If N atoms are brooght into close prasimity (the ease in crystalline Si), is is qoite reasonable to sagest a modification in the energy states of the valence electrons. The modification ih the valense-eleslmn energy slates aetoally known to take place is snnamaeised in Fig. 2.5. Stastiog ssith V-isolated Si atoms, and sonsoplnally bringing the atoons closer and closer together. one hsads -thniastrmlomie forces lead IT a progressive spread in the allowed energies.. The spread in energies giver rise to slosoly spaced sets of allofrgdstatesknawn as eoevgv baodn. At the interatomic distance eossospoodirg to the Si lattice spacing, the distrihotian of allowed slales consists of two bands seposaled by an interseaing energy gap. The apper band nf allowed states is called the soodttstmost band; the lower band of allowed states, the valence bond; and the intervening energy gap, the forbidden gap or band gop. In filling the allowed energy band states, electrons tend to gravitate In the lawmt possible energies. Notingthat electrons are eesrrieted to single os enpansy in allowed states (the Pooh ovolnsion principle) and rsmaemhesiog that the 4ff valence band states san joso accommodate what were formerly 4ff valence electrons, we typically find that the valence band is almost completely filled with electrons and the 27 24 SEMICONDUCTOR FUNDAMENTALS CARRIER MODELING wills the nitsrplens of oIl asattsse sysssmsss, the isolated Isydrogen sstatsn. Tltsr atolls, sIn tise reader may recall frosst a eanene in moderss physics, avon andes intense nernoiny at the ssssrt of she twentieslt seotory. Scientists of that sittne knew the Ityslsagems atovt contained a osg;t lively oltargest particle in orbit oboist a tttare snanrive positively ehstrgesl ttttslestr. Wirsts tlsey sonld 101 eslrlaso was the nolore of the ligltt ettnittsd from sIte rynsettt mites she isydrogett 01001 wan lteated loan elevated testtpevslssre. Specifically, lbs ststissed light was observed at ooly certain discrete wavelossgths; aocordistg to she prevailing iitsory of tlte tints, roiesstistn expected a sotssinoom of wavelengths. 1913 Nssls Salty proposed a salstliott to lbs dilemosa. Bolts hypashenioed thsst tire H- 25 H tilcat sort it odi atolls electron was restricted to rertusiss woll-dehoed orbits; or eqaiv;sletttly, Bolts assomed tlsat she orbiting electron coold take as srnly ssstoiss saisses of ongstlar mnottteotatn. Thin “qsmsmstioasion” ol lbs electron’s ongotlar stsamentnm was, its tore, conpied directly Ia estergy qstststtisatsms As can be readily estoblislted, if she elestromt’r angitlas stsostsentttm in asrastsed F19UeR 2.2 Setisototic rol:’Osootatior OF as isolated SI atom. lobe nls, sisess mq° — fin) 0 2(n’s 5 = 5 _ 5 mm n1,2,3,... i2.l) svhere (also see Fig. 2.1) F 5 is she eleesvoo biadiog energy svillsin she hydrogen atom, ns° in tlse toots of a free electron, q in the mogsitstde ssf Its electronic charge. e iv Ise peresit tsvstv of free space, h ss Planek’s constant, h = h/2or, ostd n is tlts energy qaasmtatn namber or orbit tdsntmflsr. 1eetronoofseV1itannisofenergysstoaltj.bxIll—ssjoalsv. Now, wsth tlss sleetramt limited to sertaiss ettergien inside the Isydrogest stoso. st follows frotts the Bans nsodel thsst the transition from a higlser n to a lower n osbit will relears qmsamsticed energies of light; this explains the obsosvosion of ensitted light at only oersoin discrete wavelsngtlss. For oar pnrposes, Its tttost important idea to he obtaioed frottt the Bohr model is that the energy of electrons in atomic systems is restricted too Ittotted set of valoss.t Relative to the hydrogen atoot. tIne energy level scheme io a toolti-oteetroo otom like stltsoo ts, as one might iotoitivoly espeet. dosidodly more somplos. It is still a relatively easy task, how ever, to dssorihs the saliottt energy-related foatoses of ao isolated siliean atom. As pietored in Fig. 2.2. ten of the 14 Si-atottt electrons oceapy very deep-lying energy levels otsd are ttghtly hoond to the oneleos of the atoto. The binding is so stroneio focI that these ten electrons rottj_ssetttioIIs on gawrbed daring shettrical reactions or normal atom—atom intoeostionn, ssith tlso ten-electron-plns-noclens sombin,ation often being referred In as the otoot. The eetttatntisg fottr Si-otoos electrons, on the other hood, are rothov weakly bostod attd ore colleotively called the volcnsyslsrezrurtykocagao_gLtheie sOsong p.&trtieigotiott jg ehenaioal wastiotto. An stopItosized in Fig 2.2, tlso foss valence eleetroos. if nttpertnsbed. osonpy foor of the eight allowed slots (or states) hosing the nest highest ,enssgy above the deep-lyittg rose levels. Ftnally, we shoald note. for sotopletenoss, tlsat the electronic vonligaratiott in tlss 32-electron Ge-atom (gormaitiam being the ttthor elemental nenticandststar( iv essentially identical to lbs Si-atom sanfigaration except that lbs Go-core ssstttainv 28 eleetsatts. 2.2 SEMICONDUCTOR MODELS Boilditig on the information prevented in psestonv sections. sos tnnxasloee and describe in this nestion tsvo very impartattt tnodsls or vivnalisation aids tttat are stsed extensively in the 10 s —t.atov analysis of vowicondnstor devtsev. The toslnnina of vemicondostoe tttodels in a chapter devoted to carrier nsodelino way appear odd at first glance bat iv actoally qoits appropriate. We are, in effect, modeling the carries “container;’ the sewieondnstor crystal. —s.aav Fieare 2.1 otters TIre hydmurgon atom—idoaltesd sepsosetttasioo nhosvirg she tiwl Ibsen attowod oteoseoe and Iso asonsiatsd energy qoarsiooriotr. rvrtnattv. sot anty ornrtry bus rmrurv rttsnrrhsrp r,shtos sIstine In itnmss.uioed possistns nec qsartssed. An snIde Qoantuce Utectssnims. trio bees durstrpnd so drrsdbe Ar propoesicri and assess of sssioro-airod hstd as study. potholes ova rystsmt www.EasyEngineering.net 26 UEMICGN5OCTOR raNnanEa’rnLn 27 CARRIER MODELING C’ irs to sop so son In of a rarsisordassar fog.. Oil Fiemarn 2.3 Tho bonding model. 2,2.1 Bonding Model The isolated St atom, Ge 0 Si atom not interacting with otlser atatos, mat foond to contain foor valence electrons. Si atoms incorporated in the diamond lattice, on the other hand, evltibit a bonding that involvon an attraction betwseo gash atom and its font nearest ttotglt hors (refer to Fig. l.4s). The implication here is that, in going from isolated GIants to the collective esyntollino state, Si atttms same to abase one of their saletsee electrons seitlt each of the font nearest osighbovv. This sovalent bottdittg, as sqoal vhasiog of valence electrons with nearest neighbors, and lbs moss fast that atoson in the diamond lattice Itave foar nearest oeighboss. give rite to the idealised vemisoodnetas representation, the bonding model, shanvo in Fig. 2.3. Bash circle in the Fig. 2.3 bandittg tnstdel represents the sore of a nomi sovdtmetav atotn, while sash line sepsevonts a rhatod valence eleotson. (These are eight lines soovestod to each atom besaare any gives atom oat only sansribnsea fonr shared electrons bat most also aeeeat fonr shared electrons ham adjacent atoms.) The two-dimensiottal satavs of the ntodel in, of soovss, an idealisatian that facilitates mental visnalisatiasv. Alslsongh sooniderable ass will be mode of the bottdittg tnodsl in snbvsqttettt discos siGns, it is ssvertltelern worthwhile at this point to evatnine ratnple appiisatiotts of sha model so provide toots indisotios of the model’s ntility. Two sample applisattona ace prosorted in Fig. 2.4. Iv Fig. 2.dta( we nse the bonding yodel to pistose n paint dsfest, a missing atom, in the louise stmssnrs. In Fig. 2.41b( sen visaaliss ths beeaktng of an atom to-atans hood attd the associated release as freeing of on sleotson. [Bomtd breaking (at T> o K( and defesta asons natnmlly in all semisondnstasa. and hoses (if sve maybe natttewhat avstoritisal( ttte basis model of Ftg. 2.3 is strictly valid for an snttre settntsondastor only at T 0 K svhno the semisandostor iv ssneatiott sontaitta no defects and tto itnptmrity atotns.( 2.2.2 Energy Band Model If any interests mess restricted to describing the spatial aspects of events taking place mithia nemisandostor, the bonding model olono svoold probably be adsqnatn. QUito often. howeves, one is more intoreated in the nmsesgy-selated aspects of an nosat. In vosh instances the botsdiny model, which nays nothing abant electron energies. iv of httle valne and tito ettesgy batsd model besotsass the pritnary vivoalisation aid. O ww w.E Figure 2.4 tot Sample atilisation of the bonding model. (01 Visoalieation of n misting atom or poist dofost. (b) Smoking of an atom.to-atom bond and fmeiog of an eteoteos. asy Let ns bngin the sonseptoal path leading to the energy band asosdel by recalling the sitaation inside an isolated Si atom. Reviewing the Section 2.1 dissnssion, ten nf the 14 electrons maids on isolated Si atam are tightly boond to the nosleas and are anlikely to be significantly pertorbed by normal atom—atom snteroetions. The rematetng foas obeIsant are mthos weakly boond and, if noportarbed, osonpy font of the eight ollawed energy stales immediately above the last ease level. Moreover, it in implicitly nnderstood that the elec tronic energy states within a groap of Si atoms, nay N Si atoms, are all idevtteal—as lang as thn atoms are isolated, that in, foe enoagh apart so that they are 000intnsasting. Given the foregoing knowjsdge of the isolated atotn sitaatian, the qtaevtion neal arises an to whether we coo are the Itnawledge to dedose information ahoot the crystalline slate. Assaredly we cnn omit any farther tnentson of the sore electrons besanse these electrons are not vigniSsantly pestasbed by normal interatomic forces. The opposite, however, is trae of the valence eleetsotnn. If N atoms are brooght into close prasimity (the ease in crystalline Si), is is qoite reasonable to sagest a modification in the energy states of the valence electrons. The modification ih the valense-eleslmn energy slates aetoally known to take place is snnamaeised in Fig. 2.5. Stastiog ssith V-isolated Si atoms, and sonsoplnally bringing the atoons closer and closer together. one hsads -thniastrmlomie forces lead IT a progressive spread in the allowed energies.. The spread in energies giver rise to slosoly spaced sets of allofrgdstatesknawn as eoevgv baodn. At the interatomic distance eossospoodirg to the Si lattice spacing, the distrihotian of allowed slales consists of two bands seposaled by an interseaing energy gap. The apper band nf allowed states is called the soodttstmost band; the lower band of allowed states, the valence bond; and the intervening energy gap, the forbidden gap or band gop. In filling the allowed energy band states, electrons tend to gravitate In the lawmt possible energies. Notingthat electrons are eesrrieted to single os enpansy in allowed states (the Pooh ovolnsion principle) and rsmaemhesiog that the 4ff valence band states san joso accommodate what were formerly 4ff valence electrons, we typically find that the valence band is almost completely filled with electrons and the En gin eer ing .ne www.EasyEngineering.net t www.EasyEngineering.net 26 nnnneorinooyon r000granoToLs , 000niEn u000Lirao 29 , .. a cttcrvt)________ I ::::---ñ F tO T _ tcrondy v/pip IL-settitttIatIhdl Frvs ON p-stairs tot:tt SN n-nmatei mid (4N eteetniss total) ww 4N tttcwnd stain Figure 2.6 The energy havd dittgram—widety etnployed sirnplifted versioit of the energy band states a, cv tttodsl. attawot stains (va/nice hilled Oaottl Crvstzdlets at N-Ateni w.E atotned in a perfect crystal, one sees the same allowed-stale confignration. Wn therefore conctode that fore perfect crystal onder cqnilihriam condirrons a plot of the allowed dcc Iron energres verv,rs drslance along any preselected crystalline direction (always called the x-dtrection) io as shown on the right-hand side of Ftg. 2.5. The cited plot, a plot of allowed electron energy slatesas a fnnclion of position, is thn bosie energy band model. E 5 intro dirced tn the Fig. 2.5 plot is the lossesr possible condoction hand energy, is the highest possibte valence hand energy, and ff 5 iv the band gap energy. F 0 = N. Finally, Fig. 2.6 displays thn form of the basic energy band modet nnconntered in practrce. In this widely eotploynd “shorthand” version. the lise to rndicale the rep energy tn the condoetion bend, the line to indtratn the bottom energy in thn valence band, the fill pattern drawtng attention to mostly fitted states in the valence band, the labeling of the y or electron-energy aais, and the labeling of the x- or posrtion antt ann all onderoood to mist tmplirirl. bat are not shown evptiritly. t — as y En gin e issittad Si aternn am worn spacing eri Si lattice sparing 2.2.3 Carriers ng. ne - Figure 2.5 Cenreptaai develepmeet ef the eeengy heed model starting with N melded Si atems en the tep left and ceeeleding with e “dmtsed-ep” vereiee ef the energy heed teedel ett the tep right. With the semicondortor models having been firmly established, we am now in o position to introdoce and to visnaliee the correot-earrying entities wtthin semieoodaetors. Referring to Ftg. 2.7. we note first from part (a) that there are no carriers or possible correct flow if tire bnndrng modet has no broken bonds. Eqoisalently, in the energy band model, if the valence band as completely fitted with electrons and the eondortion band as dnvoid of elec trons. there ate no carriers or possible corrent flow. This lack of carriers and associated rarrenl flow as easy to nodersrand in lertos of the bondang model svhnrn the shared electrons are viesved as being tied to the atomic corey. As arcnratety portrayed in the energy bond model, however, the valenen band elnetroas actoatly move aboot in the crystal. Hem is it then that no rnrrent can arise from this groap of electrons? As it bras oat, the momentom of the electrons is qnontieod in addition to their energy. Moreover, for each and every possible oromenram state in a band, there is another state svith an oppositely directed me meotam of eqoal magnitode. Thos, tf a band is completely filled with electrons, the net momentnm of the electrons in the band is almoys identically zero. tt follows that no corrent can arise from the electrons in a completely filled energy hand. The electrons that do give rise to charge trarsport are visnalized in Fig. 2.7(b). When a Si—St band is broken and the associated electroti is free to wander ahont the lattice, the released eleetros it a carrier. Eqoivalently. in terms of the energy band model, oneilation of vulenre band electrons into the condoetioin band creates carriers; that iv, eleetvoits in the t cendectioa hand is all bat deveid of electrees. tedeed, the valence band is eemplntely filled ned the coedectioe heed completely empty at temperatares appreaehieg T = 0 K. To complete onr pleesibilieatioe of the eneegy bend mede!, we need to ietrodace and ntiliee nan addilioeat fact: Celike the veleace eloctroes in the isolated-clew case, the hand electrons in crystalline silicon are net lied to er avsociated snub any one pecticolar atoet. Troe, on the averogn, one will typically find fear etecteonv hemp shared betwentt any given Si atom and its fonr nearest neighbors (es in the bonding model). However, the identity of dtc shared electrons changm as a fonction of lime, with the eloctrons moving amend from point to point in the crystal. In othnc wordy, the allowed electronic states are no longer atomic states hot em ovvnciated with the crystol as a whole; indepnndnnt of thn potat en- www.EasyEngineering.net r ‘ - 39 nnre008noeTon raNnouorer’alo cannion M000LtNa scheme, the empty slate in the valence band, is the second type of carrier foand in semi roodorrors_tho hole. Althoagh perhaps not ohvioos from the preceding introdoctory description, the va lence bond hole is an enltty on an eqnal footing with the condacrion bond eleerroat. Both electrons and holes parttripoge in the oporation of most semirandortor devices Hales are even the primary carrier in some devices. As one’s fantiliarity with carrier madding grows, the comparable staloo of electrons and holes beeotaes more and morn apparent. Ultimately, it iv commonplace to conceive of the hole as o lype of sobasonsie particle. ernyty en Csmptonly OIled (a) No saednri 2.2.4 Band Gap and Material Classiflicaflion C- We coarlade this section by cIting a very important lie between the band gop of a material, rho nomber of carriers ovatlablo for transport in a material, and the overall nalare of a material. As it tarns oat, allhoagh specifically established for semicoedartors, the energy band toodel of Ftg. 2.6 can ho applied with only slight modification to all matoriols. The major difference between malerials lies nor in the natare of the energy bands, bat rather in the irsagnirode of the energy gap between the bands. Insolarors, as illostrared in Fig. 2.fl(a), are characterized by very vvide band gaps, with E far the insalating materials diamond aed ShOe being =5 eV and wfl cv, respectively. In these wtde band gap malertals the thermal energy available at room temperarare oneiles very fesv eleetrans from the valence band into the roodnerian band; thas very few carriers moist instde the material and the material is therefore a poor condacror of earront. The band (0) Ttrooteeitor ‘—0 C, Is) tao anti Figure 2.7 Visrialieariott of carriers osirg ttto bonding modnl (left) and tho energy hand model (right), (a) No’earriorsits:artoe; (hi vivaalieacioo of att eleetrtro: (ci visoetioatioo o(a lasle. ae reitdortiott bairn are rovvirvs. Note that Ste eovrgy reqaired to break a bead in the bondivg model ttvd the band gap energy. En. are one and tire sottsv thing. Likrwive, bred bandingmodel electrons and romtdaetion band electrons amy jost different tames for the sante elec trons; in sshveqoent divcassinav the word ‘electrons.’ svhen ased svithoat a modifier, ssill be nndervtnod to refer in these roedortion band electrons. tn addition to releasing an electron, the breaking of a Si—Si bottd also creates a otissisg boisd or void in the bonding stracanre. Thiolsing in terms of the bonding model, one can vtsoaliee the toonetoeni of rhiv missing bond from place to place in the lattice as a revolt of nearby boond eieerrtrov jamping into the void (see Fig. 2.?r). Altornativrly. otte can think in tertvs nf the energy band model where the removal of an eleetror from the valence band creates an eorpry state in an nthero’ise vast sea of filled states. The empty vtatr, like a bobble in a liqaid. roovov aboor rather freely in the lattice becanse of the cooperative roorintt of the valence band electrons. What we have been deseribiag, the missing bond in the bonding I [‘es e—uv)go S evlaoneod) en !a) tswetor 0 C = I 5 e = 1.12 2 iv (Gaas) iv (Oil cv = 0.00 rV (Gel (Onorn ternriturn’, (hi Seoieoeacstor or Is) idrtal Figaro 2,8 (e) Enpasattov of the distinction borreoen Ic) insalators, (b) somivesdaoiors and aerials ovine the energy band model. 31 www.EasyEngineering.net 26 nnnneorinooyon r000granoToLs , 000niEn u000Lirao 29 , .. a cttcrvt)________ I ::::---ñ F 4N tttcwnd stain Frvs ON p-stairs tot:tt SN n-nmatei mid (4N eteetniss total) tO T _ tcrondy v/pip IL-settitttIatIhdl am Figure 2.6 The energy havd dittgram—widety etnployed sirnplifted versioit of the energy band states a, cv tttodsl. attawot stains (va/nice hilled Oaottl Crvstzdlets at N-Ateni atotned in a perfect crystal, one sees the same allowed-stale confignration. Wn therefore conctode that fore perfect crystal onder cqnilihriam condirrons a plot of the allowed dcc Iron energres verv,rs drslance along any preselected crystalline direction (always called the x-dtrection) io as shown on the right-hand side of Ftg. 2.5. The cited plot, a plot of allowed electron energy slatesas a fnnclion of position, is thn bosie energy band model. E 5 intro dirced tn the Fig. 2.5 plot is the lossesr possible condoction hand energy, is the highest possibte valence hand energy, and ff 5 iv the band gap energy. F 0 = N. Finally, Fig. 2.6 displays thn form of the basic energy band modet nnconntered in practrce. In this widely eotploynd “shorthand” version. the lise to rndicale the rep energy tn the condoetion bend, the line to indtratn the bottom energy in thn valence band, the fill pattern drawtng attention to mostly fitted states in the valence band, the labeling of the y or electron-energy aais, and the labeling of the x- or posrtion antt ann all onderoood to mist tmplirirl. bat are not shown evptiritly. ww t w.E a 2.2.3 Carriers — syE ngi nee r ing . With the semicondortor models having been firmly established, we am now in o position issittad Si aternn worn spacing Si lattice sparing to introdoce and to visnaliee the correot-earrying entities wtthin semieoodaetors. Referring to Ftg. 2.7. we note first from part (a) that there are no carriers or possible correct flow if tire bnndrng modet has no broken bonds. Eqoisalently, in the energy band model, if the valence band as completely fitted with electrons and the eondortion band as dnvoid of elec trons. there ate no carriers or possible corrent flow. This lack of carriers and associated rarrenl flow as easy to nodersrand in lertos of the bondang model svhnrn the shared electrons are viesved as being tied to the atomic corey. As arcnratety portrayed in the energy bond model, however, the valenen band elnetroas actoatly move aboot in the crystal. Hem is it then that no rnrrent can arise from this groap of electrons? As it bras oat, the momentom of the electrons is qnontieod in addition to their energy. Moreover, for each and every possible oromenram state in a band, there is another state svith an oppositely directed me meotam of eqoal magnitode. Thos, tf a band is completely filled with electrons, the net momentnm of the electrons in the band is almoys identically zero. tt follows that no corrent can arise from the electrons in a completely filled energy hand. The electrons that do give rise to charge trarsport are visnalized in Fig. 2.7(b). When a Si—St band is broken and the associated electroti is free to wander ahont the lattice, the released eleetros it a carrier. Eqoivalently. in terms of the energy band model, oneilation of vulenre band electrons into the condoetioin band creates carriers; that iv, eleetvoits in the - Figure 2.5 Cenreptaai develepmeet ef the eeengy heed model starting with N melded Si atems en the tep left and ceeeleding with e “dmtsed-ep” vereiee ef the energy heed teedel ett the tep right. cendectioa hand is all bat deveid of electrees. tedeed, the valence band is eemplntely filled ned the coedectioe heed completely empty at temperatares appreaehieg T = 0 K. To complete onr pleesibilieatioe of the eneegy bend mede!, we need to ietrodace and ntiliee nan addilioeat fact: Celike the veleace eloctroes in the isolated-clew case, the hand electrons in crystalline silicon are net lied to er avsociated snub any one pecticolar atoet. Troe, on the averogn, one will typically find fear etecteonv hemp shared betwentt any given Si atom and its fonr nearest neighbors (es in the bonding model). However, the identity of dtc shared electrons changm as a fonction of lime, with the eloctrons moving amend from point to point in the crystal. In othnc wordy, the allowed electronic states are no longer atomic states hot em ovvnciated with the crystol as a whole; indepnndnnt of thn potat en- net www.EasyEngineering.net r ‘ - 39 nnre008noeTon raNnouorer’alo cannion M000LtNa scheme, the empty slate in the valence band, is the second type of carrier foand in semi roodorrors_tho hole. Althoagh perhaps not ohvioos from the preceding introdoctory description, the va lence bond hole is an enltty on an eqnal footing with the condacrion bond eleerroat. Both electrons and holes parttripoge in the oporation of most semirandortor devices Hales are even the primary carrier in some devices. As one’s fantiliarity with carrier madding grows, the comparable staloo of electrons and holes beeotaes more and morn apparent. Ultimately, it iv commonplace to conceive of the hole as o lype of sobasonsie particle. ernyty en Csmptonly OIled (a) No saednri 2.2.4 Band Gap and Material Classiflicaflion C- We coarlade this section by cIting a very important lie between the band gop of a material, rho nomber of carriers ovatlablo for transport in a material, and the overall nalare of a material. As it tarns oat, allhoagh specifically established for semicoedartors, the energy band toodel of Ftg. 2.6 can ho applied with only slight modification to all matoriols. The major difference between malerials lies nor in the natare of the energy bands, bat rather in the irsagnirode of the energy gap between the bands. Insolarors, as illostrared in Fig. 2.fl(a), are characterized by very vvide band gaps, with E far the insalating materials diamond aed ShOe being =5 eV and wfl cv, respectively. In these wtde band gap malertals the thermal energy available at room temperarare oneiles very fesv eleetrans from the valence band into the roodnerian band; thas very few carriers moist instde the material and the material is therefore a poor condacror of earront. The band (0) Ttrooteeitor ‘—0 C, Is) tao anti Figure 2.7 Visrialieariott of carriers osirg ttto bonding modnl (left) and tho energy hand model (right), (a) No’earriorsits:artoe; (hi vivaalieacioo of att eleetrtro: (ci visoetioatioo o(a lasle. ae reitdortiott bairn are rovvirvs. Note that Ste eovrgy reqaired to break a bead in the bondivg model ttvd the band gap energy. En. are one and tire sottsv thing. Likrwive, bred bandingmodel electrons and romtdaetion band electrons amy jost different tames for the sante elec trons; in sshveqoent divcassinav the word ‘electrons.’ svhen ased svithoat a modifier, ssill be nndervtnod to refer in these roedortion band electrons. tn addition to releasing an electron, the breaking of a Si—Si bottd also creates a otissisg boisd or void in the bonding stracanre. Thiolsing in terms of the bonding model, one can vtsoaliee the toonetoeni of rhiv missing bond from place to place in the lattice as a revolt of nearby boond eieerrtrov jamping into the void (see Fig. 2.?r). Altornativrly. otte can think in tertvs nf the energy band model where the removal of an eleetror from the valence band creates an eorpry state in an nthero’ise vast sea of filled states. The empty vtatr, like a bobble in a liqaid. roovov aboor rather freely in the lattice becanse of the cooperative roorintt of the valence band electrons. What we have been deseribiag, the missing bond in the bonding I [‘es e—uv)go S evlaoneod) en !a) tswetor 0 C = I 5 e = 1.12 2 iv (Gaas) iv (Oil cv = 0.00 rV (Gel (Onorn ternriturn’, (hi Seoieoeacstor or Is) idrtal Figaro 2,8 (e) Enpasattov of the distinction borreoen Ic) insalators, (b) somivesdaoiors and aerials ovine the energy band model. 31 26 nnnneorinooyon r000granoToLs , 000niEn u000Lirao 29 , .. a cttcrvt)________ I ::::---ñ F 4N tttcwnd stain Frvs ON p-stairs tot:tt SN n-nmatei mid (4N eteetniss total) tO T _ am tcrondy v/pip IL-settitttIatIhdl Figure 2.6 The energy havd dittgram—widety etnployed sirnplifted versioit of the energy band states a, cv tttodsl. attawot stains (va/nice hilled Oaottl Crvstzdlets at N-Ateni atotned in a perfect crystal, one sees the same allowed-stale confignration. Wn therefore conctode that fore perfect crystal onder cqnilihriam condirrons a plot of the allowed dcc Iron energres verv,rs drslance along any preselected crystalline direction (always called the x-dtrection) io as shown on the right-hand side of Ftg. 2.5. The cited plot, a plot of allowed electron energy slatesas a fnnclion of position, is thn bosie energy band model. E 5 intro dirced tn the Fig. 2.5 plot is the lossesr possible condoction hand energy, is the highest possibte valence hand energy, and ff 5 iv the band gap energy. F 0 = N. Finally, Fig. 2.6 displays thn form of the basic energy band modet nnconntered in practrce. In this widely eotploynd “shorthand” version. the lise to rndicale the rep energy tn the condoetion bend, the line to indtratn the bottom energy in thn valence band, the fill pattern drawtng attention to mostly fitted states in the valence band, the labeling of the y or electron-energy aais, and the labeling of the x- or posrtion antt ann all onderoood to mist tmplirirl. bat are not shown evptiritly. t — 2.2.3 Carriers issittad Si aternn worn spacing Si lattice sparing With the semicondortor models having been firmly established, we am now in o position to introdoce and to visnaliee the correot-earrying entities wtthin semieoodaetors. Referring to Ftg. 2.7. we note first from part (a) that there are no carriers or possible correct flow if tire bnndrng modet has no broken bonds. Eqoisalently, in the energy band model, if the valence band as completely fitted with electrons and the eondortion band as dnvoid of elec trons. there ate no carriers or possible corrent flow. This lack of carriers and associated rarrenl flow as easy to nodersrand in lertos of the bondang model svhnrn the shared electrons are viesved as being tied to the atomic corey. As arcnratety portrayed in the energy bond model, however, the valenen band elnetroas actoatly move aboot in the crystal. Hem is it then that no rnrrent can arise from this groap of electrons? As it bras oat, the momentom of the electrons is qnontieod in addition to their energy. Moreover, for each and every possible oromenram state in a band, there is another state svith an oppositely directed me meotam of eqoal magnitode. Thos, tf a band is completely filled with electrons, the net momentnm of the electrons in the band is almoys identically zero. tt follows that no corrent can arise from the electrons in a completely filled energy hand. The electrons that do give rise to charge trarsport are visnalized in Fig. 2.7(b). When a Si—St band is broken and the associated electroti is free to wander ahont the lattice, the released eleetros it a carrier. Eqoivalently. in terms of the energy band model, oneilation of vulenre band electrons into the condoetioin band creates carriers; that iv, eleetvoits in the - Figure 2.5 Cenreptaai develepmeet ef the eeengy heed model starting with N melded Si atems en the tep left and ceeeleding with e “dmtsed-ep” vereiee ef the energy heed teedel ett the tep right. cendectioa hand is all bat deveid of electrees. tedeed, the valence band is eemplntely filled ned the coedectioe heed completely empty at temperatares appreaehieg T = 0 K. To complete onr pleesibilieatioe of the eneegy bend mede!, we need to ietrodace and ntiliee nan addilioeat fact: Celike the veleace eloctroes in the isolated-clew case, the hand electrons in crystalline silicon are net lied to er avsociated snub any one pecticolar atoet. Troe, on the averogn, one will typically find fear etecteonv hemp shared betwentt any given Si atom and its fonr nearest neighbors (es in the bonding model). However, the identity of dtc shared electrons changm as a fonction of lime, with the eloctrons moving amend from point to point in the crystal. In othnc wordy, the allowed electronic states are no longer atomic states hot em ovvnciated with the crystol as a whole; indepnndnnt of thn potat en- www.EasyEngineering.net r ‘ - 39 nnre008noeTon raNnouorer’alo cannion M000LtNa scheme, the empty slate in the valence band, is the second type of carrier foand in semi roodorrors_tho hole. Althoagh perhaps not ohvioos from the preceding introdoctory description, the va lence bond hole is an enltty on an eqnal footing with the condacrion bond eleerroat. Both electrons and holes parttripoge in the oporation of most semirandortor devices Hales are even the primary carrier in some devices. As one’s fantiliarity with carrier madding grows, the comparable staloo of electrons and holes beeotaes more and morn apparent. Ultimately, it iv commonplace to conceive of the hole as o lype of sobasonsie particle. ernyty en Csmptonly OIled (a) No saednri ww w 2.2.4 Band Gap and Material Classiflicaflion .Ea C- We coarlade this section by cIting a very important lie between the band gop of a material, rho nomber of carriers ovatlablo for transport in a material, and the overall nalare of a material. As it tarns oat, allhoagh specifically established for semicoedartors, the energy band toodel of Ftg. 2.6 can ho applied with only slight modification to all matoriols. The major difference between malerials lies nor in the natare of the energy bands, bat rather in the irsagnirode of the energy gap between the bands. Insolarors, as illostrared in Fig. 2.fl(a), are characterized by very vvide band gaps, with E far the insalating materials diamond aed ShOe being =5 eV and wfl cv, respectively. In these wtde band gap malertals the thermal energy available at room temperarare oneiles very fesv eleetrans from the valence band into the roodnerian band; thas very few carriers moist instde the material and the material is therefore a poor condacror of earront. The band syE (0) Ttrooteeitor ngi nee rin g ‘—0 Is) tao anti C, .ne t Figure 2.7 Visrialieariott of carriers osirg ttto bonding modnl (left) and tho energy hand model (right), (a) No’earriorsits:artoe; (hi vivaalieacioo of att eleetrtro: (ci visoetioatioo o(a lasle. reitdortiott bairn are rovvirvs. Note that Ste eovrgy reqaired to break a bead in the bondivg model ttvd the band gap energy. En. are one and tire sottsv thing. Likrwive, bred bandingmodel electrons and romtdaetion band electrons amy jost different tames for the sante elec trons; in sshveqoent divcassinav the word ‘electrons.’ svhen ased svithoat a modifier, ssill be nndervtnod to refer in these roedortion band electrons. tn addition to releasing an electron, the breaking of a Si—Si bottd also creates a otissisg boisd or void in the bonding stracanre. Thiolsing in terms of the bonding model, one can vtsoaliee the toonetoeni of rhiv missing bond from place to place in the lattice as a revolt of nearby boond eieerrtrov jamping into the void (see Fig. 2.?r). Altornativrly. otte can think in tertvs nf the energy band model where the removal of an eleetror from the valence band creates an eorpry state in an nthero’ise vast sea of filled states. The empty vtatr, like a bobble in a liqaid. roovov aboor rather freely in the lattice becanse of the cooperative roorintt of the valence band electrons. What we have been deseribiag, the missing bond in the bonding www.EasyEngineering.net ae I [‘es e—uv)go S evlaoneod) en !a) tswetor 0 C = I 5 e = 1.12 2 iv (Gaas) iv (Oil cv = 0.00 rV (Gel (Onorn ternriturn’, (hi Seoieoeacstor or Is) idrtal Figaro 2,8 (e) Enpasattov of the distinction borreoen Ic) insalators, (b) somivesdaoiors and aerials ovine the energy band model. 31 26 nnnneorinooyon r000granoToLs , 000niEn u000Lirao 29 , .. a cttcrvt)________ I ::::---ñ F 4N tttcwnd stain Frvs ON p-stairs tot:tt SN n-nmatei mid (4N eteetniss total) tO T _ tcrondy v/pip IL-settitttIatIhdl am Figure 2.6 The energy havd dittgram—widety etnployed sirnplifted versioit of the energy band states a, cv tttodsl. attawot stains (va/nice hilled Oaottl Crvstzdlets at N-Ateni atotned in a perfect crystal, one sees the same allowed-stale confignration. Wn therefore conctode that fore perfect crystal onder cqnilihriam condirrons a plot of the allowed dcc Iron energres verv,rs drslance along any preselected crystalline direction (always called the x-dtrection) io as shown on the right-hand side of Ftg. 2.5. The cited plot, a plot of allowed electron energy slatesas a fnnclion of position, is thn bosie energy band model. E 5 intro dirced tn the Fig. 2.5 plot is the lossesr possible condoction hand energy, is the highest possibte valence hand energy, and ff 5 iv the band gap energy. F 0 = N. Finally, Fig. 2.6 displays thn form of the basic energy band modet nnconntered in practrce. In this widely eotploynd “shorthand” version. the lise to rndicale the rep energy tn the condoetion bend, the line to indtratn the bottom energy in thn valence band, the fill pattern drawtng attention to mostly fitted states in the valence band, the labeling of the y or electron-energy aais, and the labeling of the x- or posrtion antt ann all onderoood to mist tmplirirl. bat are not shown evptiritly. t — 2.2.3 Carriers issittad Si aternn worn spacing Si lattice sparing With the semicondortor models having been firmly established, we am now in o position to introdoce and to visnaliee the correot-earrying entities wtthin semieoodaetors. Referring to Ftg. 2.7. we note first from part (a) that there are no carriers or possible correct flow if tire bnndrng modet has no broken bonds. Eqoisalently, in the energy band model, if the valence band as completely fitted with electrons and the eondortion band as dnvoid of elec trons. there ate no carriers or possible corrent flow. This lack of carriers and associated rarrenl flow as easy to nodersrand in lertos of the bondang model svhnrn the shared electrons are viesved as being tied to the atomic corey. As arcnratety portrayed in the energy bond model, however, the valenen band elnetroas actoatly move aboot in the crystal. Hem is it then that no rnrrent can arise from this groap of electrons? As it bras oat, the momentom of the electrons is qnontieod in addition to their energy. Moreover, for each and every possible oromenram state in a band, there is another state svith an oppositely directed me meotam of eqoal magnitode. Thos, tf a band is completely filled with electrons, the net momentnm of the electrons in the band is almoys identically zero. tt follows that no corrent can arise from the electrons in a completely filled energy hand. The electrons that do give rise to charge trarsport are visnalized in Fig. 2.7(b). When a Si—St band is broken and the associated electroti is free to wander ahont the lattice, the released eleetros it a carrier. Eqoivalently. in terms of the energy band model, oneilation of vulenre band electrons into the condoetioin band creates carriers; that iv, eleetvoits in the - Figure 2.5 Cenreptaai develepmeet ef the eeengy heed model starting with N melded Si atems en the tep left and ceeeleding with e “dmtsed-ep” vereiee ef the energy heed teedel ett the tep right. cendectioa hand is all bat deveid of electrees. tedeed, the valence band is eemplntely filled ned the coedectioe heed completely empty at temperatares appreaehieg T = 0 K. To complete onr pleesibilieatioe of the eneegy bend mede!, we need to ietrodace and ntiliee nan addilioeat fact: Celike the veleace eloctroes in the isolated-clew case, the hand electrons in crystalline silicon are net lied to er avsociated snub any one pecticolar atoet. Troe, on the averogn, one will typically find fear etecteonv hemp shared betwentt any given Si atom and its fonr nearest neighbors (es in the bonding model). However, the identity of dtc shared electrons changm as a fonction of lime, with the eloctrons moving amend from point to point in the crystal. In othnc wordy, the allowed electronic states are no longer atomic states hot em ovvnciated with the crystol as a whole; indepnndnnt of thn potat en- r ‘ www.EasyEngineering.net - 39 nnre008noeTon raNnouorer’alo cannion M000LtNa scheme, the empty slate in the valence band, is the second type of carrier foand in semi roodorrors_tho hole. Althoagh perhaps not ohvioos from the preceding introdoctory description, the va lence bond hole is an enltty on an eqnal footing with the condacrion bond eleerroat. Both electrons and holes parttripoge in the oporation of most semirandortor devices Hales are even the primary carrier in some devices. As one’s fantiliarity with carrier madding grows, the comparable staloo of electrons and holes beeotaes more and morn apparent. Ultimately, it iv commonplace to conceive of the hole as o lype of sobasonsie particle. ernyty en Csmptonly OIled (a) No saednri 2.2.4 Band Gap and Material Classiflicaflion ww w.E C- We coarlade this section by cIting a very important lie between the band gop of a material, rho nomber of carriers ovatlablo for transport in a material, and the overall nalare of a material. As it tarns oat, allhoagh specifically established for semicoedartors, the energy band toodel of Ftg. 2.6 can ho applied with only slight modification to all matoriols. The major difference between malerials lies nor in the natare of the energy bands, bat rather in the irsagnirode of the energy gap between the bands. Insolarors, as illostrared in Fig. 2.fl(a), are characterized by very vvide band gaps, with E far the insalating materials diamond aed ShOe being =5 eV and wfl cv, respectively. In these wtde band gap malertals the thermal energy available at room temperarare oneiles very fesv eleetrans from the valence band into the roodnerian band; thas very few carriers moist instde the material and the material is therefore a poor condacror of earront. The band (0) Ttrooteeitor asy En ‘—0 C, Is) tao anti Figure 2.7 Visrialieariott of carriers osirg ttto bonding modnl (left) and tho energy hand model (right), (a) No’earriorsits:artoe; (hi vivaalieacioo of att eleetrtro: (ci visoetioatioo o(a lasle. ae reitdortiott bairn are rovvirvs. Note that Ste eovrgy reqaired to break a bead in the bondivg model ttvd the band gap energy. En. are one and tire sottsv thing. Likrwive, bred bandingmodel electrons and romtdaetion band electrons amy jost different tames for the sante elec trons; in sshveqoent divcassinav the word ‘electrons.’ svhen ased svithoat a modifier, ssill be nndervtnod to refer in these roedortion band electrons. tn addition to releasing an electron, the breaking of a Si—Si bottd also creates a otissisg boisd or void in the bonding stracanre. Thiolsing in terms of the bonding model, one can vtsoaliee the toonetoeni of rhiv missing bond from place to place in the lattice as a revolt of nearby boond eieerrtrov jamping into the void (see Fig. 2.?r). Altornativrly. otte can think in tertvs nf the energy band model where the removal of an eleetror from the valence band creates an eorpry state in an nthero’ise vast sea of filled states. The empty vtatr, like a bobble in a liqaid. roovov aboor rather freely in the lattice becanse of the cooperative roorintt of the valence band electrons. What we have been deseribiag, the missing bond in the bonding I gin eer [‘es e—uv)go S evlaoneod) en !a) tswetor ing 0 C = I 5 e = 1.12 .ne 2 iv (Gaas) iv (Oil cv = 0.00 rV (Gel (Onorn ternriturn’, (hi Seoieoeacstor or Is) idrtal Figaro 2,8 (e) Enpasattov of the distinction borreoen Ic) insalators, (b) somivesdaoiors and aerials ovine the energy band model. www.EasyEngineering.net t 31 www.EasyEngineering.net 32 SEMICONDUCTOR FUNDAMENTALS CASRIUR MODELING gap in metals, by way of contportson, is either very small, or no band gap exists at all dan to att overlap of the valence and eandaetion bands (see Fig. 2 .8c). Tirere is always an abnndattee of carriers in metals, and hence atetals are excellent cxndttrtxrs. Sentiran dactors present alt interosediate case betsseess insalators and otetais. wrature 1 (3notn text 00K), E t L42 eV in GaAs. ff 0 .=1J2 eV in Sf and E 5 . = 0.66 5 in Ge.I Tlterttsal ettergy, by exciting electrons frotn the valence bond ittto the eontlstction hand, creates a tooderette nntnbcr of carriers itt thcsc tnaterials, giving rise ix turn to a cuerettt carrying capability intermediate bctwern poor attd excellent. cv (a) 2.3 CARRIER PROPERTIES ww Figure 2.9 Httvtttg formally itttrodnend the electron attd the hole, sxn next seek to tram as ntaclt as possible abont tlte nalstre of these carriers. In tltisparticolar section we examine a collage of carcier-related inforsoation, ittformntion of a gencral nature incloding general facts, properties, and terminology. thi wittnin a samnicondaatsnr orystaL w.E as y En gin e Electrons nruovisrg inside a semicondootor crystal will collide voith sensicandttoror atauctv, thereby eassiog a periodic deceleration of the carriers. However, shoold not Eq. (2.2) apply to the portion of tlta electronic snotion occurring beturaats collisiorta? l’hc anssver is again sna. Its addition to fire aplulied electric held, etacsrosts iso crystal are also sabjacttsr csssnptes crystalline fields not specifically incloded in Eq. (2.2). ‘l’he foregoing discossioss delineated certain issspoetant differettees betsueess electrons in c crystal and electrons in a voettam, hot it left onresolved the equally important qoestios as to how smne properly describes rIse mosion of carriers in a crystal. Strictly speaking, Olue notion of carriers in a crystal can be described only by oaieg Qstantans Mechanics, tIre formaiism appropriate for atomic-sieed systems. Fortonotely, if the dimensions of the crys tal are large compared to atostssc ditneovions, the complex qnanssnsn meehasticat farunulation for tire carrier notion hetweest collisions simplifies to yield on equation of motion identical to Eq. (2.21, except that mum 0 is replaced by an effective carrier tnass. In other words, for the Fig. 2.9(b) aleetrotsy sIne ruin write 2.3.1 Charge Both electrons and holes are charged entities. Electrons are tegatively eltoeged, holes are posttively eltttrged, and the mngssiraela of tlte carrier charge, q, is the souse for the two types of carriecs. To tltree-plaee aecamey in MKS units, t5 coal. Please note 0 1.60 X l p that, ttnder the eanvrntton adopted herein, the electron aod hole charges are —q and +q, respnetivnly, i.e.. the sign of the charge is displayed eapltettly. eri 2.3.2 Effective Mass (hi hit electron nuving rn mepoosa to an applied alectrtc hotd (at within a sacasusts, aod ng. ne Mass, like charge, is another very basic property of electrons ard Itoles. Unlike charge, hownoer, the carrier mass is not a sitopln property and cannot be disposed of simply by qsoting a nntnber. Indeed, the apparent or “effective” osass of rlreoons within a crystal is a fnstesiott of the seminondactor material (St. Gn, etc.) and is different from the mass of electrons within a vacnart. Seeking to obtain titsight into the effnctivn mass concept, tnt as first coesider the mo tion of nlecteons in a oaeaom. If, as itlostrated in Fig. 2.9)a), an electron of rest osass a is 0t ttsoving in a voennm between two parallel plotes under the influence of an electric fieldS, tltea. according to Newton’s second law, the force F on tire electron will be t F —qRm (2.3) where tn is Ihe electron effective moss. A similar equation can be wrilten for holes with m. In each ease the internal crystalline fields assd qoatstato —q —a q and ns osechanicat effects arc all snitably lumped into the effective mass factor multiplying em/eu. This is a very significant reantt. ds allan’s usa to cossraire of t’imctrons and holes as qsast c/ssssirsslFamsirtas and so employ rtossirotporricla t’e/ariona/ssps itt moat darien ussatyvaa. Although the effective mass formulation is a significant simplification, it should be roentioned tttat the carrier acceleration cats vary with the direerson of travel iou emystat: i.e., the eft’eetivc masses eon have multiple compottenta. MoreoeeL depending on how a mac roscopic observable is related to the carrier motion, a different groupisrg of usass cossrpo neota can land to a different m 5 hemp oritieed in a particslar relationship. Tlsner are, for example, cyclotron ecsottauee effective masses, conductivity effective masses, density of — where n is the electron velocity and t is time. Nest consider electrons (coodaction band electrons) moving between the two parallnl nod faces of a snmicoodnetor crystal under the influence of an applied electric field, as envisioned in Pig. 2.9(b). Dons Eq. (2.2) also de scribe the overall motiosr of electrons within the semieondaetar crystal? Thn answer is so. www.EasyEngineering.net CARRIUR M000L5NG Table 2.1 Density of States Effective Masses at 300 K. ddateriot 5 as/m m/ssa Si Gn GaAs docrion bond atrtomatieatty creates a valence bond hole along svith the coodnetian band ‘electron. Also note that the intrinsic carrier concentration , allhoogh large is an absolute sense, ts relatseely small compared with the number of bonds that could be broken. For example, In Sm them are 5 at 1002 atoms/cm 3 and foor bonds pee atom, making a grand total of 2 at l0’ hoods or talcum band electrons per . Since n, 3 em 10 itlem one finds less than one bond in lO broken in Si at rootn temperatom. To aceoratety represent the situotson inside iotrinaic Si at room temperature, we could cover all the oniversiry chalkboards ix the world with the bonding model and possibly show only ooe broken bond. 0.61 0.36 0.52 1.16 0.55 0.066 , stares effective masses, among others. It is also probably not too sorprising rhtt the effeetron masses vary oosonsvhat with tempnratare. l’lereie we make drreet use of only the density of states effective messes (see Sabseerion 2.4.1). The density of stales effective mosses for electrons and holes in Si, Go, and GaAs at 300 K are listed in Table 2.1. 2.3.3 Carrier Numbers in Intrinsic Material The :erm isariesir semiconductor in common asagn refers to an aetremely pare semleon dactor sanspln containing an insignificant omonnl of itoparity atoms. More precisely, an intrinsic semiconductor is a semicondartor whose properties are native to the mornriol (that is, not caused by external additives). The namber of carriers in an intrinsic semiconductor fits into the scheme of things in that it is an identifiahle intrinsic properly of the marerral. Defining, quite generally, n = somber of electrons/cm 3 p = nombar of holes/ama existing inside a setnrcouduator, Ihen, given on intrinsic seminondoetor under eqotlabrmnt cooditions, one hrrds npn a, 2 x 5 10°/cm 5 I at be/cm 2 x lO’ / 5 em’ (2.4) in GaAs in Si at roots temperatare in Ge The electron and hole concentrations in an intrinsic semicondoetor are equal because carriers within a very pare material eon be created only in pairs. Eeferring to Fig. 2.?, tf semicondoator bond iv broken, a free electron and a missing bond or hale are created si tnslrooeoosly. Likewise, the excitation of on electron from the valence band into the con- 2.3.4 Manipulation of Carrier Numbers—Doping Doping, in semicourdavtor terminology, is the addition of controlled astsnnots of specific imparity atoms with the express parposc of increasing either the electron or the hole eon ceolcation. The addition of dopants in controlled amoants to snmieondnctor materials oc curs rootinety in the fabrication of almost all semicondont or devices. Common Si dopoora me tustad in Table 2.2. To increase the electron concentration , one can add either phospho ens. arsente, or aotsmooy aroma to the Si crystal, with pho.sphoros followed closely by arsenic brtng the most eom,uoonly employed donor (rlrctroo-iucreas)ne) dopanus. To in emenor the hole concentration, one adds either boron, gallinos, indiom, or nlnmioom atoms to the Si crystal, with boron briog thr most commonly employed acceptor (kote-iocreosiog) dopont. To understood how the addition of impurity atoms non lead lou manipolntinu of carrier numbers, It t5 umportant to note that the Table 2.2 donors are alt from Column V in the Purnodic Table of Elements, while all of the cited acceptors mu from Column Ill in the Periodic Table of Elements. As visoalieed in Pig. 2 .lO(a) using the bonding model, when a Column V ulrmrot mats five valence electrons is sobasitnted for a Si atoor in the semiaoo doctor lattice, four of the flee valence electrons fit snugly into the bonding strnctnre. The fifth donor electron, hosvever, does not fit into the bonding stractoeg and is weakly bostod to rIte donor site. Ar room temperature this electron is readily freed to mara’buf’ifie botttee and hence becomes a carrier. Please note that this donotnon (hence the name “do nor”) of carrier electrons does nut iocrense the hole 35 www.EasyEngineering.net 32 SEMICONDUCTOR FUNDAMENTALS CASRIUR MODELING gap in metals, by way of contportson, is either very small, or no band gap exists at all dan to att overlap of the valence and eandaetion bands (see Fig. 2 .8c). Tirere is always an abnndattee of carriers in metals, and hence atetals are excellent cxndttrtxrs. Sentiran dactors present alt interosediate case betsseess insalators and otetais. wrature 1 (3notn text 00K), E t L42 eV in GaAs. ff 0 .=1J2 eV in Sf and E 5 . = 0.66 5 in Ge.I Tlterttsal ettergy, by exciting electrons frotn the valence bond ittto the eontlstction hand, creates a tooderette nntnbcr of carriers itt thcsc tnaterials, giving rise ix turn to a cuerettt carrying capability intermediate bctwern poor attd excellent. cv (a) 2.3 CARRIER PROPERTIES Httvtttg formally itttrodnend the electron attd the hole, sxn next seek to tram as ntaclt as possible abont tlte nalstre of these carriers. In tltisparticolar section we examine a collage of carcier-related inforsoation, ittformntion of a gencral nature incloding general facts, properties, and terminology. ww 2.3.1 Charge Both electrons and holes are charged entities. Electrons are tegatively eltoeged, holes are posttively eltttrged, and the mngssiraela of tlte carrier charge, q, is the souse for the two types of carriecs. To tltree-plaee aecamey in MKS units, t5 coal. Please note 0 1.60 X l p that, ttnder the eanvrntton adopted herein, the electron aod hole charges are —q and +q, respnetivnly, i.e.. the sign of the charge is displayed eapltettly. Figure 2.9 (hi hit electron nuving rn mepoosa to an applied alectrtc hotd (at within a sacasusts, aod thi wittnin a samnicondaatsnr orystaL w.E a Electrons nruovisrg inside a semicondootor crystal will collide voith sensicandttoror atauctv, thereby eassiog a periodic deceleration of the carriers. However, shoold not Eq. (2.2) apply to the portion of tlta electronic snotion occurring beturaats collisiorta? l’hc anssver is again sna. Its addition to fire aplulied electric held, etacsrosts iso crystal are also sabjacttsr csssnptes crystalline fields not specifically incloded in Eq. (2.2). ‘l’he foregoing discossioss delineated certain issspoetant differettees betsueess electrons in c crystal and electrons in a voettam, hot it left onresolved the equally important qoestios as to how smne properly describes rIse mosion of carriers in a crystal. Strictly speaking, Olue notion of carriers in a crystal can be described only by oaieg Qstantans Mechanics, tIre formaiism appropriate for atomic-sieed systems. Fortonotely, if the dimensions of the crys tal are large compared to atostssc ditneovions, the complex qnanssnsn meehasticat farunulation for tire carrier notion hetweest collisions simplifies to yield on equation of motion identical to Eq. (2.21, except that mum 0 is replaced by an effective carrier tnass. In other words, for the Fig. 2.9(b) aleetrotsy sIne ruin write syE ngi nee r 2.3.2 Effective Mass ing . Mass, like charge, is another very basic property of electrons ard Itoles. Unlike charge, hownoer, the carrier mass is not a sitopln property and cannot be disposed of simply by qsoting a nntnber. Indeed, the apparent or “effective” osass of rlreoons within a crystal is a fnstesiott of the seminondactor material (St. Gn, etc.) and is different from the mass of electrons within a vacnart. Seeking to obtain titsight into the effnctivn mass concept, tnt as first coesider the mo tion of nlecteons in a oaeaom. If, as itlostrated in Fig. 2.9)a), an electron of rest osass a is 0t ttsoving in a voennm between two parallel plotes under the influence of an electric fieldS, tltea. according to Newton’s second law, the force F on tire electron will be F —qRm net where tn is Ihe electron effective moss. A similar equation can be wrilten for holes with m. In each ease the internal crystalline fields assd qoatstato —q —a q and ns osechanicat effects arc all snitably lumped into the effective mass factor multiplying em/eu. This is a very significant reantt. ds allan’s usa to cossraire of t’imctrons and holes as qsast c/ssssirsslFamsirtas and so employ rtossirotporricla t’e/ariona/ssps itt moat darien ussatyvaa. Although the effective mass formulation is a significant simplification, it should be roentioned tttat the carrier acceleration cats vary with the direerson of travel iou emystat: i.e., the eft’eetivc masses eon have multiple compottenta. MoreoeeL depending on how a mac roscopic observable is related to the carrier motion, a different groupisrg of usass cossrpo neota can land to a different m 5 hemp oritieed in a particslar relationship. Tlsner are, for example, cyclotron ecsottauee effective masses, conductivity effective masses, density of — where n is the electron velocity and t is time. Nest consider electrons (coodaction band electrons) moving between the two parallnl nod faces of a snmicoodnetor crystal under the influence of an applied electric field, as envisioned in Pig. 2.9(b). Dons Eq. (2.2) also de scribe the overall motiosr of electrons within the semieondaetar crystal? Thn answer is so. www.EasyEngineering.net CARRIUR M000L5NG Table 2.1 Density of States Effective Masses at 300 K. ddateriot 5 as/m m/ssa Si Gn GaAs docrion bond atrtomatieatty creates a valence bond hole along svith the coodnetian band ‘electron. Also note that the intrinsic carrier concentration , allhoogh large is an absolute sense, ts relatseely small compared with the number of bonds that could be broken. For example, In Sm them are 5 at 1002 atoms/cm 3 and foor bonds pee atom, making a grand total of 2 at l0’ hoods or talcum band electrons per . Since n, 3 em 10 itlem one finds less than one bond in lO broken in Si at rootn temperatom. To aceoratety represent the situotson inside iotrinaic Si at room temperature, we could cover all the oniversiry chalkboards ix the world with the bonding model and possibly show only ooe broken bond. 0.61 0.36 0.52 1.16 0.55 0.066 , stares effective masses, among others. It is also probably not too sorprising rhtt the effeetron masses vary oosonsvhat with tempnratare. l’lereie we make drreet use of only the density of states effective messes (see Sabseerion 2.4.1). The density of stales effective mosses for electrons and holes in Si, Go, and GaAs at 300 K are listed in Table 2.1. 2.3.3 Carrier Numbers in Intrinsic Material The :erm isariesir semiconductor in common asagn refers to an aetremely pare semleon dactor sanspln containing an insignificant omonnl of itoparity atoms. More precisely, an intrinsic semiconductor is a semicondartor whose properties are native to the mornriol (that is, not caused by external additives). The namber of carriers in an intrinsic semiconductor fits into the scheme of things in that it is an identifiahle intrinsic properly of the marerral. Defining, quite generally, n = somber of electrons/cm 3 p = nombar of holes/ama existing inside a setnrcouduator, Ihen, given on intrinsic seminondoetor under eqotlabrmnt cooditions, one hrrds npn a, 2 x 5 10°/cm 5 I at be/cm 2 x lO’ / 5 em’ (2.4) in GaAs in Si at roots temperatare in Ge The electron and hole concentrations in an intrinsic semicondoetor are equal because carriers within a very pare material eon be created only in pairs. Eeferring to Fig. 2.?, tf semicondoator bond iv broken, a free electron and a missing bond or hale are created si tnslrooeoosly. Likewise, the excitation of on electron from the valence band into the con- (2.3) 2.3.4 Manipulation of Carrier Numbers—Doping Doping, in semicourdavtor terminology, is the addition of controlled astsnnots of specific imparity atoms with the express parposc of increasing either the electron or the hole eon ceolcation. The addition of dopants in controlled amoants to snmieondnctor materials oc curs rootinety in the fabrication of almost all semicondont or devices. Common Si dopoora me tustad in Table 2.2. To increase the electron concentration , one can add either phospho ens. arsente, or aotsmooy aroma to the Si crystal, with pho.sphoros followed closely by arsenic brtng the most eom,uoonly employed donor (rlrctroo-iucreas)ne) dopanus. To in emenor the hole concentration, one adds either boron, gallinos, indiom, or nlnmioom atoms to the Si crystal, with boron briog thr most commonly employed acceptor (kote-iocreosiog) dopont. To understood how the addition of impurity atoms non lead lou manipolntinu of carrier numbers, It t5 umportant to note that the Table 2.2 donors are alt from Column V in the Purnodic Table of Elements, while all of the cited acceptors mu from Column Ill in the Periodic Table of Elements. As visoalieed in Pig. 2 .lO(a) using the bonding model, when a Column V ulrmrot mats five valence electrons is sobasitnted for a Si atoor in the semiaoo doctor lattice, four of the flee valence electrons fit snugly into the bonding strnctnre. The fifth donor electron, hosvever, does not fit into the bonding stractoeg and is weakly bostod to rIte donor site. Ar room temperature this electron is readily freed to mara’buf’ifie botttee and hence becomes a carrier. Please note that this donotnon (hence the name “do nor”) of carrier electrons does nut iocrense the hole 35 32 SEMICONDUCTOR FUNDAMENTALS CASRIUR MODELING gap in metals, by way of contportson, is either very small, or no band gap exists at all dan to att overlap of the valence and eandaetion bands (see Fig. 2 .8c). Tirere is always an abnndattee of carriers in metals, and hence atetals are excellent cxndttrtxrs. Sentiran dactors present alt interosediate case betsseess insalators and otetais. wrature 1 (3notn text 00K), E t L42 eV in GaAs. ff 0 .=1J2 eV in Sf and E 5 . = 0.66 5 in Ge.I Tlterttsal ettergy, by exciting electrons frotn the valence bond ittto the eontlstction hand, creates a tooderette nntnbcr of carriers itt thcsc tnaterials, giving rise ix turn to a cuerettt carrying capability intermediate bctwern poor attd excellent. cv (a) 2.3 CARRIER PROPERTIES Figure 2.9 Httvtttg formally itttrodnend the electron attd the hole, sxn next seek to tram as ntaclt as possible abont tlte nalstre of these carriers. In tltisparticolar section we examine a collage of carcier-related inforsoation, ittformntion of a gencral nature incloding general facts, properties, and terminology. (hi hit electron nuving rn mepoosa to an applied alectrtc hotd (at within a sacasusts, aod thi wittnin a samnicondaatsnr orystaL Electrons nruovisrg inside a semicondootor crystal will collide voith sensicandttoror atauctv, thereby eassiog a periodic deceleration of the carriers. However, shoold not Eq. (2.2) apply to the portion of tlta electronic snotion occurring beturaats collisiorta? l’hc anssver is again sna. Its addition to fire aplulied electric held, etacsrosts iso crystal are also sabjacttsr csssnptes crystalline fields not specifically incloded in Eq. (2.2). ‘l’he foregoing discossioss delineated certain issspoetant differettees betsueess electrons in c crystal and electrons in a voettam, hot it left onresolved the equally important qoestios as to how smne properly describes rIse mosion of carriers in a crystal. Strictly speaking, Olue notion of carriers in a crystal can be described only by oaieg Qstantans Mechanics, tIre formaiism appropriate for atomic-sieed systems. Fortonotely, if the dimensions of the crys tal are large compared to atostssc ditneovions, the complex qnanssnsn meehasticat farunulation for tire carrier notion hetweest collisions simplifies to yield on equation of motion identical to Eq. (2.21, except that mum 0 is replaced by an effective carrier tnass. In other words, for the Fig. 2.9(b) aleetrotsy sIne ruin write 2.3.1 Charge Both electrons and holes are charged entities. Electrons are tegatively eltoeged, holes are posttively eltttrged, and the mngssiraela of tlte carrier charge, q, is the souse for the two types of carriecs. To tltree-plaee aecamey in MKS units, t5 coal. Please note 0 1.60 X l p that, ttnder the eanvrntton adopted herein, the electron aod hole charges are —q and +q, respnetivnly, i.e.. the sign of the charge is displayed eapltettly. 2.3.2 Effective Mass Mass, like charge, is another very basic property of electrons ard Itoles. Unlike charge, hownoer, the carrier mass is not a sitopln property and cannot be disposed of simply by qsoting a nntnber. Indeed, the apparent or “effective” osass of rlreoons within a crystal is a fnstesiott of the seminondactor material (St. Gn, etc.) and is different from the mass of electrons within a vacnart. Seeking to obtain titsight into the effnctivn mass concept, tnt as first coesider the mo tion of nlecteons in a oaeaom. If, as itlostrated in Fig. 2.9)a), an electron of rest osass a is 0t ttsoving in a voennm between two parallel plotes under the influence of an electric fieldS, tltea. according to Newton’s second law, the force F on tire electron will be F —qRm (2.3) where tn is Ihe electron effective moss. A similar equation can be wrilten for holes with m. In each ease the internal crystalline fields assd qoatstato —q —a q and ns osechanicat effects arc all snitably lumped into the effective mass factor multiplying em/eu. This is a very significant reantt. ds allan’s usa to cossraire of t’imctrons and holes as qsast c/ssssirsslFamsirtas and so employ rtossirotporricla t’e/ariona/ssps itt moat darien ussatyvaa. Although the effective mass formulation is a significant simplification, it should be roentioned tttat the carrier acceleration cats vary with the direerson of travel iou emystat: i.e., the eft’eetivc masses eon have multiple compottenta. MoreoeeL depending on how a mac roscopic observable is related to the carrier motion, a different groupisrg of usass cossrpo neota can land to a different m 5 hemp oritieed in a particslar relationship. Tlsner are, for example, cyclotron ecsottauee effective masses, conductivity effective masses, density of — where n is the electron velocity and t is time. Nest consider electrons (coodaction band electrons) moving between the two parallnl nod faces of a snmicoodnetor crystal under the influence of an applied electric field, as envisioned in Pig. 2.9(b). Dons Eq. (2.2) also de scribe the overall motiosr of electrons within the semieondaetar crystal? Thn answer is so. www.EasyEngineering.net CARRIUR M000L5NG Table 2.1 Density of States Effective Masses at 300 K. ddateriot 5 as/m m/ssa Si Gn GaAs docrion bond atrtomatieatty creates a valence bond hole along svith the coodnetian band ‘electron. Also note that the intrinsic carrier concentration , allhoogh large is an absolute sense, ts relatseely small compared with the number of bonds that could be broken. For example, In Sm them are 5 at 1002 atoms/cm 3 and foor bonds pee atom, making a grand total of 2 at l0’ hoods or talcum band electrons per . Since n, 3 em 10 itlem one finds less than one bond in lO broken in Si at rootn temperatom. To aceoratety represent the situotson inside iotrinaic Si at room temperature, we could cover all the oniversiry chalkboards ix the world with the bonding model and possibly show only ooe broken bond. 0.61 0.36 0.52 1.16 0.55 0.066 , stares effective masses, among others. It is also probably not too sorprising rhtt the effeetron masses vary oosonsvhat with tempnratare. l’lereie we make drreet use of only the density of states effective messes (see Sabseerion 2.4.1). The density of stales effective mosses for electrons and holes in Si, Go, and GaAs at 300 K are listed in Table 2.1. ww w .Ea 2.3.3 Carrier Numbers in Intrinsic Material syE The :erm isariesir semiconductor in common asagn refers to an aetremely pare semleon dactor sanspln containing an insignificant omonnl of itoparity atoms. More precisely, an intrinsic semiconductor is a semicondartor whose properties are native to the mornriol (that is, not caused by external additives). The namber of carriers in an intrinsic semiconductor fits into the scheme of things in that it is an identifiahle intrinsic properly of the marerral. Defining, quite generally, ngi nee rin g n = somber of electrons/cm 3 p = nombar of holes/ama .ne t existing inside a setnrcouduator, Ihen, given on intrinsic seminondoetor under eqotlabrmnt cooditions, one hrrds npn a, 2 x 5 10°/cm 5 I at be/cm 2 x lO’ / 5 em’ (2.4) in GaAs in Si at roots temperatare in Ge The electron and hole concentrations in an intrinsic semicondoetor are equal because carriers within a very pare material eon be created only in pairs. Eeferring to Fig. 2.?, tf semicondoator bond iv broken, a free electron and a missing bond or hale are created si tnslrooeoosly. Likewise, the excitation of on electron from the valence band into the con- www.EasyEngineering.net 2.3.4 Manipulation of Carrier Numbers—Doping Doping, in semicourdavtor terminology, is the addition of controlled astsnnots of specific imparity atoms with the express parposc of increasing either the electron or the hole eon ceolcation. The addition of dopants in controlled amoants to snmieondnctor materials oc curs rootinety in the fabrication of almost all semicondont or devices. Common Si dopoora me tustad in Table 2.2. To increase the electron concentration , one can add either phospho ens. arsente, or aotsmooy aroma to the Si crystal, with pho.sphoros followed closely by arsenic brtng the most eom,uoonly employed donor (rlrctroo-iucreas)ne) dopanus. To in emenor the hole concentration, one adds either boron, gallinos, indiom, or nlnmioom atoms to the Si crystal, with boron briog thr most commonly employed acceptor (kote-iocreosiog) dopont. To understood how the addition of impurity atoms non lead lou manipolntinu of carrier numbers, It t5 umportant to note that the Table 2.2 donors are alt from Column V in the Purnodic Table of Elements, while all of the cited acceptors mu from Column Ill in the Periodic Table of Elements. As visoalieed in Pig. 2 .lO(a) using the bonding model, when a Column V ulrmrot mats five valence electrons is sobasitnted for a Si atoor in the semiaoo doctor lattice, four of the flee valence electrons fit snugly into the bonding strnctnre. The fifth donor electron, hosvever, does not fit into the bonding stractoeg and is weakly bostod to rIte donor site. Ar room temperature this electron is readily freed to mara’buf’ifie botttee and hence becomes a carrier. Please note that this donotnon (hence the name “do nor”) of carrier electrons does nut iocrense the hole 35 32 SEMICONDUCTOR FUNDAMENTALS CASRIUR MODELING gap in metals, by way of contportson, is either very small, or no band gap exists at all dan to att overlap of the valence and eandaetion bands (see Fig. 2 .8c). Tirere is always an abnndattee of carriers in metals, and hence atetals are excellent cxndttrtxrs. Sentiran dactors present alt interosediate case betsseess insalators and otetais. wrature 1 (3notn text 00K), E t L42 eV in GaAs. ff 0 .=1J2 eV in Sf and E 5 . = 0.66 5 in Ge.I Tlterttsal ettergy, by exciting electrons frotn the valence bond ittto the eontlstction hand, creates a tooderette nntnbcr of carriers itt thcsc tnaterials, giving rise ix turn to a cuerettt carrying capability intermediate bctwern poor attd excellent. cv (a) 2.3 CARRIER PROPERTIES Figure 2.9 Httvtttg formally itttrodnend the electron attd the hole, sxn next seek to tram as ntaclt as possible abont tlte nalstre of these carriers. In tltisparticolar section we examine a collage of carcier-related inforsoation, ittformntion of a gencral nature incloding general facts, properties, and terminology. (hi hit electron nuving rn mepoosa to an applied alectrtc hotd (at within a sacasusts, aod thi wittnin a samnicondaatsnr orystaL Electrons nruovisrg inside a semicondootor crystal will collide voith sensicandttoror atauctv, thereby eassiog a periodic deceleration of the carriers. However, shoold not Eq. (2.2) apply to the portion of tlta electronic snotion occurring beturaats collisiorta? l’hc anssver is again sna. Its addition to fire aplulied electric held, etacsrosts iso crystal are also sabjacttsr csssnptes crystalline fields not specifically incloded in Eq. (2.2). ‘l’he foregoing discossioss delineated certain issspoetant differettees betsueess electrons in c crystal and electrons in a voettam, hot it left onresolved the equally important qoestios as to how smne properly describes rIse mosion of carriers in a crystal. Strictly speaking, Olue notion of carriers in a crystal can be described only by oaieg Qstantans Mechanics, tIre formaiism appropriate for atomic-sieed systems. Fortonotely, if the dimensions of the crys tal are large compared to atostssc ditneovions, the complex qnanssnsn meehasticat farunulation for tire carrier notion hetweest collisions simplifies to yield on equation of motion identical to Eq. (2.21, except that mum 0 is replaced by an effective carrier tnass. In other words, for the Fig. 2.9(b) aleetrotsy sIne ruin write 2.3.1 Charge Both electrons and holes are charged entities. Electrons are tegatively eltoeged, holes are posttively eltttrged, and the mngssiraela of tlte carrier charge, q, is the souse for the two types of carriecs. To tltree-plaee aecamey in MKS units, t5 coal. Please note 0 1.60 X l p that, ttnder the eanvrntton adopted herein, the electron aod hole charges are —q and +q, respnetivnly, i.e.. the sign of the charge is displayed eapltettly. 2.3.2 Effective Mass Mass, like charge, is another very basic property of electrons ard Itoles. Unlike charge, hownoer, the carrier mass is not a sitopln property and cannot be disposed of simply by qsoting a nntnber. Indeed, the apparent or “effective” osass of rlreoons within a crystal is a fnstesiott of the seminondactor material (St. Gn, etc.) and is different from the mass of electrons within a vacnart. Seeking to obtain titsight into the effnctivn mass concept, tnt as first coesider the mo tion of nlecteons in a oaeaom. If, as itlostrated in Fig. 2.9)a), an electron of rest osass a is 0t ttsoving in a voennm between two parallel plotes under the influence of an electric fieldS, tltea. according to Newton’s second law, the force F on tire electron will be F —qRm (2.3) where tn is Ihe electron effective moss. A similar equation can be wrilten for holes with m. In each ease the internal crystalline fields assd qoatstato —q —a q and ns osechanicat effects arc all snitably lumped into the effective mass factor multiplying em/eu. This is a very significant reantt. ds allan’s usa to cossraire of t’imctrons and holes as qsast c/ssssirsslFamsirtas and so employ rtossirotporricla t’e/ariona/ssps itt moat darien ussatyvaa. Although the effective mass formulation is a significant simplification, it should be roentioned tttat the carrier acceleration cats vary with the direerson of travel iou emystat: i.e., the eft’eetivc masses eon have multiple compottenta. MoreoeeL depending on how a mac roscopic observable is related to the carrier motion, a different groupisrg of usass cossrpo neota can land to a different m 5 hemp oritieed in a particslar relationship. Tlsner are, for example, cyclotron ecsottauee effective masses, conductivity effective masses, density of — where n is the electron velocity and t is time. Nest consider electrons (coodaction band electrons) moving between the two parallnl nod faces of a snmicoodnetor crystal under the influence of an applied electric field, as envisioned in Pig. 2.9(b). Dons Eq. (2.2) also de scribe the overall motiosr of electrons within the semieondaetar crystal? Thn answer is so. www.EasyEngineering.net CARRIUR M000L5NG Table 2.1 Density of States Effective Masses at 300 K. ddateriot 5 as/m m/ssa Si Gn GaAs 0.61 0.36 0.52 1.16 0.55 0.066 , stares effective masses, among others. It is also probably not too sorprising rhtt the effeetron masses vary oosonsvhat with tempnratare. l’lereie we make drreet use of only the density of states effective messes (see Sabseerion 2.4.1). The density of stales effective mosses for electrons and holes in Si, Go, and GaAs at 300 K are listed in Table 2.1. 2.3.3 Carrier Numbers in Intrinsic Material The :erm isariesir semiconductor in common asagn refers to an aetremely pare semleon dactor sanspln containing an insignificant omonnl of itoparity atoms. More precisely, an intrinsic semiconductor is a semicondartor whose properties are native to the mornriol (that is, not caused by external additives). The namber of carriers in an intrinsic semiconductor fits into the scheme of things in that it is an identifiahle intrinsic properly of the marerral. Defining, quite generally, n = somber of electrons/cm 3 p = nombar of holes/ama existing inside a setnrcouduator, Ihen, given on intrinsic seminondoetor under eqotlabrmnt cooditions, one hrrds npn a, 2 x 5 10°/cm 5 I at be/cm 2 x lO’ / 5 em’ (2.4) 2.3.4 Manipulation of Carrier Numbers—Doping ww w.E Doping, in semicourdavtor terminology, is the addition of controlled astsnnots of specific imparity atoms with the express parposc of increasing either the electron or the hole eon ceolcation. The addition of dopants in controlled amoants to snmieondnctor materials oc curs rootinety in the fabrication of almost all semicondont or devices. Common Si dopoora me tustad in Table 2.2. To increase the electron concentration , one can add either phospho ens. arsente, or aotsmooy aroma to the Si crystal, with pho.sphoros followed closely by arsenic brtng the most eom,uoonly employed donor (rlrctroo-iucreas)ne) dopanus. To in emenor the hole concentration, one adds either boron, gallinos, indiom, or nlnmioom atoms to asy En the Si crystal, with boron briog thr most commonly employed acceptor (kote-iocreosiog) dopont. gin To understood how the addition of impurity atoms non lead lou manipolntinu of carrier numbers, It t5 umportant to note that the Table 2.2 donors are alt from Column V in the Purnodic Table of Elements, while all of the cited acceptors mu from Column Ill in the Periodic Table of Elements. As visoalieed in Pig. 2 .lO(a) using the bonding model, when a Column V ulrmrot mats five valence electrons is sobasitnted for a Si atoor in the semiaoo doctor lattice, four of the flee valence electrons fit snugly into the bonding strnctnre. The fifth donor electron, hosvever, does not fit into the bonding stractoeg and is weakly bostod to rIte donor site. Ar room temperature this electron is readily freed to mara’buf’ifie botttee and hence becomes a carrier. Please note that this donotnon (hence the name “do nor”) of carrier electrons does nut iocrense the hole eer ing .ne in GaAs in Si 35 docrion bond atrtomatieatty creates a valence bond hole along svith the coodnetian band ‘electron. Also note that the intrinsic carrier concentration , allhoogh large is an absolute sense, ts relatseely small compared with the number of bonds that could be broken. For example, In Sm them are 5 at 1002 atoms/cm 3 and foor bonds pee atom, making a grand total of 2 at l0’ hoods or talcum band electrons per . Since n, 3 em 10 itlem one finds less than one bond in lO broken in Si at rootn temperatom. To aceoratety represent the situotson inside iotrinaic Si at room temperature, we could cover all the oniversiry chalkboards ix the world with the bonding model and possibly show only ooe broken bond. at roots temperatare in Ge The electron and hole concentrations in an intrinsic semicondoetor are equal because carriers within a very pare material eon be created only in pairs. Eeferring to Fig. 2.?, tf semicondoator bond iv broken, a free electron and a missing bond or hale are created si tnslrooeoosly. Likewise, the excitation of on electron from the valence band into the con- www.EasyEngineering.net t www.EasyEngineering.net 36 n SEMICONDUCTOR FUNDAMENTALS Figure 2.11 Ib) a) ww CARRIER MODELING Pseadwhydnugeu atom mudel far the d000e-site band. Figure 2.10 Visaotieatioe of(a) donor and (hi acceptor action lIning tho banding model. In (a) the Colamn V element P is aabstitsted far a Si atom; in (hi the Colamo III element B is sabsiitsted far a Si atom. w.E as y En gin e 2(4wKejs) = ns —0.1 eV 1 K uh where K 5 is the St dtelectrtc constant (K 5 — (2.5) = 11.0). Actaal donor-site binding energies in Si are ltstcd in Table 2.3. The observed bittding energies are seen In be in good agreement The esplanatias of acceptor action follows a similar line of reasotning. The Colititte lii acceptors Itave three valence electrons tmd cannot complete one of the semicondnctor hands mhen subatitated for Si atoms in the nemicondoctoc lattice (sea Fig. 2. lOb). The Colansa III ototo, however, readily accepts (hence the name “acceptor”) an electron from a nearby Si—Si bond, themby completing its own handing scheme and in the pracms cre ating a hale that can wander ahoat the lattice. Here agota there is on incmaae in only ooe type of carrier. The negativety chaeged acceptor ion (acceptor atom pins accepted electron) cannot move, and no electrons are released in the hole-creation process. The foregoing bonding-model-based esplanation of dopant action is reasonably on derstandable. There are, nevertheless, a few loose ends. For one, me noted that the fifth donor electron was rather weakly bound and readily freed at room temperature. How does see interpret the relative term “weakly boand”? It takes 1 eV to break Si—Si bonds and very few of the Si—Si bonds are broken at room lemperatare. Perhaps “weakly bonnd” means a binding energy =0.1 eV or less? The question also agises as to how one visnaliacs dnpaat action in terms of the energy band model. Both of the cited qnestioas, as it lnrns nat, involve energy considerations and are actually interrelated. Let as concentrate first sn the binding energy of the fifth donor electron. Cmdely speaking, the positively charged donor-core-plan-fifth-electron may be likened to a hydro 37 with the Eq. (2.5) estimate and, confirns.iag the earlier speeslation, are ronghly Si band gap energy. = 1/20 the Havtng established the strength of dspant-site bands, we are now in a position to tackle eri ng. ne t the probleiti of how one vtsaaliees dopant Action asing the energy band model. Working on the problem, we note first that when an electron is released from a donor it becomes a cotidnetton band electron. If the energy absorbed at the donor is precisely eqaal to the electron btndmg energy, the released electron will moreover have the lowest possible en ergy it tise condticttng band—namety, Ec. Adding an energy IE Ito the bound electron, in other words, raises the electron’s energy to Ec. Hence, we are led to conclade Ihal the boned electron occaples an allowed electronic level an energy 9 I below the enudnetion 1K band edge, or, as visnaliced tn Fig. 2.12, donor sites can be incorporated ida the energy band scltemn by adding allowed electronic levels at an energy E = E En. Note that the donor energy level is represenled by a set of dashes, inslead of a csnlinaoas linn, he canse an electron bound to a donor site is tocalieed in space; i.e., a bonnd electron does not leave the general So vicinity of Ihe donor. The relative closeness of En to E of conrse refiect.s the fact that (Si). 0 — En = I%l = (l/20)E gen atom (see Pig. 2.11). Conceptually, the donor core replaces the hydrogen-atom nacteas nod the fifth donor electron replaces the hydrogen-atom elnclron. Is the real hydrogen atom the electron moves of conese in a vacuum, can be characterieed by the muss of a free Table 2.3 electron, and, referring to Eq. (2.1), has a groand-slate binding energy of 13.fi eV. lathe pseado-hydrogen atom, on the other hand, the orbiting electron moves throogh a sea of Si atoms and is characserieed hy us effective mast. Hence, in the donor oe psenda-atom case, 0 mnst be the permiltivity of free space mnst be replaced by the permittivily of Si and m replaced by m. We therefore conclude Ilsat the binding energy (En) of the fiftln donor electron is apprssimutely Dopant-Site Binding Energies. Dnssnrs 1 5 E Acceptors Sb F As 0.039eV B Al Ga In j 0 JE — 0.045 eV 0.054eV 0.045 0.0fi7 0.022 0.lfi eV nV eV eV www.EasyEngineering.net 39 5IMtCONDnCtnn FUNDAMENTALS CARRIER MODELING cient energy at temperatures T —s 0 K for a valence band electron to make the transilioe to as acceptnr site. Increasing temperatnre, implying an increased store of thermal energy, (01 facilitates electrons jstopisg from the valence bond onlo the acceptor levels. The remnvol a, s.ta5ev ‘F of etectrons from the valence band of ccavse cmatns holes. At mom tnmperatsre, essentially all of the acceptor sites are filled with an escesnelectran and an increased hole cancentra ttnn is effected in the osaterial. ‘fo complete this sitbsection, a fese w’ords are in order concemittg the doping of nonelemental semiconductorn sach an DeAn. Gopant action in GaAs follow’s the name geoeral Oenor site isJ_t.t2 cv Figure 2.12 Additioti of the £ £ denot tenets in the enengy band diagram. Dashes of width As emphmiee the tmalieed sabre of the hoand donor-situ states. The actanl visaalieatian of dopast action asing thn energy band model is pictared in Pig. 2.13. Enamining the left-hand side of Fig. 2.13(a), one fieds ott the donor sites filled with bonnd electrons at temperatures T —s 0 K. This is trne becanse .eery little thermal energy is available to encite electrons from the donor sites iota Ihe eondnclion band at these very low femserataren. The sitsation changes, of coarse, as the temperatsre is incremed, with more and more of the weakly booed electrons being donated to the condactios band. At eonm temperature the ionication of the donors is all bal total, giving rise to the simatinn pictsred at the estreme right of Fig. 2 .l3(a(. Althoagh we have concenlraled ne donors, the sitnation for acceptors is cottspletnly anatogoss. As vissaliced in Fig. 2.13(b), acceptors introduce allowed electronic levels into the fothiddeo gap at an energy slightly above the valence band edge. Allow’ temperatures, all of these sites will be empty—there is insaffi . a, an e.n.e. principles bat in slightly more tnvolved becanse of the enistence of two differettt latlice-nite atossis. Completely analogous to the doping of a Si crystal, the Column VI elements 5, Se, and Te act as donors when replacing the Catomo V element As in the GaAs lattice. Similarly, the Colame It elements Be, Mg. and Zn act as acceptors when replacing the Column III element Ga. A stew sitsaliou arises when Colume IV elements snch as Si and Ge are incorporated Into GaAs, Si typically mplacen Gag the GaAs lattice,aod is a pnpnlar si-type dopant. Howevev under certain conditions Si can be made to replace An in the GaAs ltittiiC, tisereby functioning anon acceptor. In fact GaAs pit junctions have born fabricated mltere Si ssa.v both the p-side and nt-side dopant. An imparity that can act as either a donor or an acceptor is referred to as an amphnseric dopant. ExerCine 2.1 Eitergy Qoic Pt(a) I eV ms eqaal to ham macy jontes nf energy? )b) gus equal to hosv many eV at 300 K? (ci The toniaatton energy of acceptors and donors in Si in rosghly equal Its ...........? (d) E (Si) 0 0 - OFt unons temperstum tnsseasisn c = (e) E (SiG,) 5 = if) The energy reqaired to iontee a hydrogen atom initially in then St (oil eV (b) fiT 0 r 5 c o tncinasing 0 c ••...... 5 c 00000000 wnum tnmpeiatate 151 Figure 2.13 Vissatieotion of (a) danat and (hi aceepton action Asing the energy baud msdel. = = I state is _? 1.00 x lO jooles. 15 (0.fi17 5 10 li3OOi = 0.0259eV at 300 K. (ci The ionization energy of doponts is eqaal to 1K 5 al the dopant sites. As discussed in Subsection 2.3.4, E m 0.1 eV for dopunts in Si. (di K 5 (Si) = 1.12 eV at 300 K (see Sabsection 2.2.4). (u) E (SiG,) asS eV (see Sabsectiqu 2.2.4). 5 (f) Makitig ate of Eq. (2.1) in Section 2.1, the Isydrogen atom ionioalion energy iv = 13.fieV. I 39 www.EasyEngineering.net 36 n SEMICONDUCTOR FUNDAMENTALS CARRIER MODELING Figure 2.11 Ib) a) Figure 2.10 Visaotieatioe of(a) donor and (hi acceptor action lIning tho banding model. In (a) the Colamn V element P is aabstitsted far a Si atom; in (hi the Colamo III element B is sabsiitsted far a Si atom. The esplanatias of acceptor action follows a similar line of reasotning. The Colititte lii acceptors Itave three valence electrons tmd cannot complete one of the semicondnctor hands mhen subatitated for Si atoms in the nemicondoctoc lattice (sea Fig. 2. lOb). The Colansa III ototo, however, readily accepts (hence the name “acceptor”) an electron from a nearby Si—Si bond, themby completing its own handing scheme and in the pracms cre ating a hale that can wander ahoat the lattice. Here agota there is on incmaae in only ooe type of carrier. The negativety chaeged acceptor ion (acceptor atom pins accepted electron) cannot move, and no electrons are released in the hole-creation process. The foregoing bonding-model-based esplanation of dopant action is reasonably on derstandable. There are, nevertheless, a few loose ends. For one, me noted that the fifth donor electron was rather weakly bound and readily freed at room temperature. How does see interpret the relative term “weakly boand”? It takes 1 eV to break Si—Si bonds and very few of the Si—Si bonds are broken at room lemperatare. Perhaps “weakly bonnd” means a binding energy =0.1 eV or less? The question also agises as to how one visnaliacs dnpaat action in terms of the energy band model. Both of the cited qnestioas, as it lnrns nat, involve energy considerations and are actually interrelated. Let as concentrate first sn the binding energy of the fifth donor electron. Cmdely speaking, the positively charged donor-core-plan-fifth-electron may be likened to a hydro ww 37 Pseadwhydnugeu atom mudel far the d000e-site band. w.E a 2(4wKejs) = ns —0.1 eV 1 K uh where K 5 is the St dtelectrtc constant (K 5 — (2.5) = 11.0). Actaal donor-site binding energies in Si are ltstcd in Table 2.3. The observed bittding energies are seen In be in good agreement syE ngi with the Eq. (2.5) estimate and, confirns.iag the earlier speeslation, are ronghly Si band gap energy. = 1/20 the Havtng established the strength of dspant-site bands, we are now in a position to tackle the probleiti of how one vtsaaliees dopant Action asing the energy band model. Working on the problem, we note first that when an electron is released from a donor it becomes a cotidnetton band electron. If the energy absorbed at the donor is precisely eqaal to the electron btndmg energy, the released electron will moreover have the lowest possible en ergy it tise condticttng band—namety, Ec. Adding an energy IE Ito the bound electron, in other words, raises the electron’s energy to Ec. Hence, we are led to conclade Ihal the boned electron occaples an allowed electronic level an energy 9 I below the enudnetion 1K band edge, or, as visnaliced tn Fig. 2.12, donor sites can be incorporated ida the energy band scltemn by adding allowed electronic levels at an energy E = E En. Note that the donor energy level is represenled by a set of dashes, inslead of a csnlinaoas linn, he canse an electron bound to a donor site is tocalieed in space; i.e., a bonnd electron does not leave the general So vicinity of Ihe donor. The relative closeness of En to E of conrse refiect.s the fact that (Si). 0 — En = I%l = (l/20)E nee r ing . gen atom (see Pig. 2.11). Conceptually, the donor core replaces the hydrogen-atom nacteas nod the fifth donor electron replaces the hydrogen-atom elnclron. Is the real hydrogen atom the electron moves of conese in a vacuum, can be characterieed by the muss of a free Table 2.3 electron, and, referring to Eq. (2.1), has a groand-slate binding energy of 13.fi eV. lathe pseado-hydrogen atom, on the other hand, the orbiting electron moves throogh a sea of Si atoms and is characserieed hy us effective mast. Hence, in the donor oe psenda-atom case, 0 mnst be the permiltivity of free space mnst be replaced by the permittivily of Si and m replaced by m. We therefore conclude Ilsat the binding energy (En) of the fiftln donor electron is apprssimutely net Dopant-Site Binding Energies. Dnssnrs 1 5 E Acceptors Sb F As 0.039eV B Al Ga In j 0 JE — 0.045 eV 0.054eV 0.045 0.0fi7 0.022 0.lfi eV nV eV eV www.EasyEngineering.net 39 5IMtCONDnCtnn FUNDAMENTALS CARRIER MODELING cient energy at temperatures T —s 0 K for a valence band electron to make the transilioe to as acceptnr site. Increasing temperatnre, implying an increased store of thermal energy, (01 facilitates electrons jstopisg from the valence bond onlo the acceptor levels. The remnvol a, s.ta5ev ‘F of etectrons from the valence band of ccavse cmatns holes. At mom tnmperatsre, essentially all of the acceptor sites are filled with an escesnelectran and an increased hole cancentra ttnn is effected in the osaterial. ‘fo complete this sitbsection, a fese w’ords are in order concemittg the doping of nonelemental semiconductorn sach an DeAn. Gopant action in GaAs follow’s the name geoeral Oenor site isJ_t.t2 cv Figure 2.12 Additioti of the £ £ denot tenets in the enengy band diagram. Dashes of width As emphmiee the tmalieed sabre of the hoand donor-situ states. The actanl visaalieatian of dopast action asing thn energy band model is pictared in Pig. 2.13. Enamining the left-hand side of Fig. 2.13(a), one fieds ott the donor sites filled with bonnd electrons at temperatures T —s 0 K. This is trne becanse .eery little thermal energy is available to encite electrons from the donor sites iota Ihe eondnclion band at these very low femserataren. The sitsation changes, of coarse, as the temperatsre is incremed, with more and more of the weakly booed electrons being donated to the condactios band. At eonm temperature the ionication of the donors is all bal total, giving rise to the simatinn pictsred at the estreme right of Fig. 2 .l3(a(. Althoagh we have concenlraled ne donors, the sitnation for acceptors is cottspletnly anatogoss. As vissaliced in Fig. 2.13(b), acceptors introduce allowed electronic levels into the fothiddeo gap at an energy slightly above the valence band edge. Allow’ temperatures, all of these sites will be empty—there is insaffi . a, an e.n.e. principles bat in slightly more tnvolved becanse of the enistence of two differettt latlice-nite atossis. Completely analogous to the doping of a Si crystal, the Column VI elements 5, Se, and Te act as donors when replacing the Catomo V element As in the GaAs lattice. Similarly, the Colame It elements Be, Mg. and Zn act as acceptors when replacing the Column III element Ga. A stew sitsaliou arises when Colume IV elements snch as Si and Ge are incorporated Into GaAs, Si typically mplacen Gag the GaAs lattice,aod is a pnpnlar si-type dopant. Howevev under certain conditions Si can be made to replace An in the GaAs ltittiiC, tisereby functioning anon acceptor. In fact GaAs pit junctions have born fabricated mltere Si ssa.v both the p-side and nt-side dopant. An imparity that can act as either a donor or an acceptor is referred to as an amphnseric dopant. ExerCine 2.1 Eitergy Qoic Pt(a) I eV ms eqaal to ham macy jontes nf energy? )b) gus equal to hosv many eV at 300 K? (ci The toniaatton energy of acceptors and donors in Si in rosghly equal Its ...........? (d) E (Si) 0 0 - OFt unons temperstum tnsseasisn c = (e) E (SiG,) 5 = if) The energy reqaired to iontee a hydrogen atom initially in then St (oil eV (b) fiT 0 r 5 c o tncinasing 0 c ••...... 5 c 00000000 wnum tnmpeiatate 151 Figure 2.13 Vissatieotion of (a) danat and (hi aceepton action Asing the energy baud msdel. = = I state is _? 1.00 x lO jooles. 15 (0.fi17 5 10 li3OOi = 0.0259eV at 300 K. (ci The ionization energy of doponts is eqaal to 1K 5 al the dopant sites. As discussed in Subsection 2.3.4, E m 0.1 eV for dopunts in Si. (di K 5 (Si) = 1.12 eV at 300 K (see Sabsection 2.2.4). (u) E (SiG,) asS eV (see Sabsectiqu 2.2.4). 5 (f) Makitig ate of Eq. (2.1) in Section 2.1, the Isydrogen atom ionioalion energy iv = 13.fieV. I 39 36 n SEMICONDUCTOR FUNDAMENTALS CARRIER MODELING Figure 2.11 Ib) a) Pseadwhydnugeu atom mudel far the d000e-site band. Figure 2.10 Visaotieatioe of(a) donor and (hi acceptor action lIning tho banding model. In (a) the Colamn V element P is aabstitsted far a Si atom; in (hi the Colamo III element B is sabsiitsted far a Si atom. 2(4wKejs) The esplanatias of acceptor action follows a similar line of reasotning. The Colititte lii acceptors Itave three valence electrons tmd cannot complete one of the semicondnctor hands mhen subatitated for Si atoms in the nemicondoctoc lattice (sea Fig. 2. lOb). The Colansa III ototo, however, readily accepts (hence the name “acceptor”) an electron from a nearby Si—Si bond, themby completing its own handing scheme and in the pracms cre ating a hale that can wander ahoat the lattice. Here agota there is on incmaae in only ooe type of carrier. The negativety chaeged acceptor ion (acceptor atom pins accepted electron) cannot move, and no electrons are released in the hole-creation process. The foregoing bonding-model-based esplanation of dopant action is reasonably on derstandable. There are, nevertheless, a few loose ends. For one, me noted that the fifth donor electron was rather weakly bound and readily freed at room temperature. How does see interpret the relative term “weakly boand”? It takes 1 eV to break Si—Si bonds and very few of the Si—Si bonds are broken at room lemperatare. Perhaps “weakly bonnd” means a binding energy =0.1 eV or less? The question also agises as to how one visnaliacs dnpaat action in terms of the energy band model. Both of the cited qnestioas, as it lnrns nat, involve energy considerations and are actually interrelated. Let as concentrate first sn the binding energy of the fifth donor electron. Cmdely speaking, the positively charged donor-core-plan-fifth-electron may be likened to a hydro 37 = ns —0.1 eV 1 K uh where K 5 is the St dtelectrtc constant (K 5 — (2.5) = 11.0). Actaal donor-site binding energies in Si are ltstcd in Table 2.3. The observed bittding energies are seen In be in good agreement with the Eq. (2.5) estimate and, confirns.iag the earlier speeslation, are ronghly Si band gap energy. = 1/20 the Havtng established the strength of dspant-site bands, we are now in a position to tackle the probleiti of how one vtsaaliees dopant Action asing the energy band model. Working on the problem, we note first that when an electron is released from a donor it becomes a cotidnetton band electron. If the energy absorbed at the donor is precisely eqaal to the electron btndmg energy, the released electron will moreover have the lowest possible en ergy it tise condticttng band—namety, Ec. Adding an energy IE Ito the bound electron, in other words, raises the electron’s energy to Ec. Hence, we are led to conclade Ihal the boned electron occaples an allowed electronic level an energy 9 I below the enudnetion 1K band edge, or, as visnaliced tn Fig. 2.12, donor sites can be incorporated ida the energy band scltemn by adding allowed electronic levels at an energy E = E En. Note that the donor energy level is represenled by a set of dashes, inslead of a csnlinaoas linn, he canse an electron bound to a donor site is tocalieed in space; i.e., a bonnd electron does not leave the general So vicinity of Ihe donor. The relative closeness of En to E of conrse refiect.s the fact that (Si). 0 — En = I%l = (l/20)E gen atom (see Pig. 2.11). Conceptually, the donor core replaces the hydrogen-atom nacteas nod the fifth donor electron replaces the hydrogen-atom elnclron. Is the real hydrogen atom the electron moves of conese in a vacuum, can be characterieed by the muss of a free Table 2.3 electron, and, referring to Eq. (2.1), has a groand-slate binding energy of 13.fi eV. lathe pseado-hydrogen atom, on the other hand, the orbiting electron moves throogh a sea of Si atoms and is characserieed hy us effective mast. Hence, in the donor oe psenda-atom case, 0 mnst be the permiltivity of free space mnst be replaced by the permittivily of Si and m replaced by m. We therefore conclude Ilsat the binding energy (En) of the fiftln donor electron is apprssimutely Dopant-Site Binding Energies. Dnssnrs 1 5 E Acceptors Sb F As 0.039eV B Al Ga In j 0 JE — 0.045 eV 0.054eV 0.045 0.0fi7 0.022 0.lfi eV nV eV eV www.EasyEngineering.net 39 5IMtCONDnCtnn FUNDAMENTALS CARRIER MODELING cient energy at temperatures T —s 0 K for a valence band electron to make the transilioe to as acceptnr site. Increasing temperatnre, implying an increased store of thermal energy, (01 facilitates electrons jstopisg from the valence bond onlo the acceptor levels. The remnvol a, s.ta5ev ‘F of etectrons from the valence band of ccavse cmatns holes. At mom tnmperatsre, essentially all of the acceptor sites are filled with an escesnelectran and an increased hole cancentra ttnn is effected in the osaterial. ‘fo complete this sitbsection, a fese w’ords are in order concemittg the doping of nonelemental semiconductorn sach an DeAn. Gopant action in GaAs follow’s the name geoeral Oenor site isJ_t.t2 cv Figure 2.12 Additioti of the £ £ denot tenets in the enengy band diagram. Dashes of width As emphmiee the tmalieed sabre of the hoand donor-situ states. ww w The actanl visaalieatian of dopast action asing thn energy band model is pictared in Pig. 2.13. Enamining the left-hand side of Fig. 2.13(a), one fieds ott the donor sites filled with bonnd electrons at temperatures T —s 0 K. This is trne becanse .eery little thermal .Ea energy is available to encite electrons from the donor sites iota Ihe eondnclion band at these very low femserataren. The sitsation changes, of coarse, as the temperatsre is incremed, with more and more of the weakly booed electrons being donated to the condactios band. At eonm temperature the ionication of the donors is all bal total, giving rise to the simatinn pictsred at the estreme right of Fig. 2 .l3(a(. Althoagh we have concenlraled ne donors, the sitnation for acceptors is cottspletnly anatogoss. As vissaliced in Fig. 2.13(b), acceptors introduce allowed electronic levels into the fothiddeo gap at an energy slightly above the valence band edge. Allow’ temperatures, all of these sites will be empty—there is insaffi syE ngi . e.n.e. 0 - OFt nee rin g unons temperstum tnsseasisn c a, an .ne t principles bat in slightly more tnvolved becanse of the enistence of two differettt latlice-nite atossis. Completely analogous to the doping of a Si crystal, the Column VI elements 5, Se, and Te act as donors when replacing the Catomo V element As in the GaAs lattice. Similarly, the Colame It elements Be, Mg. and Zn act as acceptors when replacing the Column III element Ga. A stew sitsaliou arises when Colume IV elements snch as Si and Ge are incorporated Into GaAs, Si typically mplacen Gag the GaAs lattice,aod is a pnpnlar si-type dopant. Howevev under certain conditions Si can be made to replace An in the GaAs ltittiiC, tisereby functioning anon acceptor. In fact GaAs pit junctions have born fabricated mltere Si ssa.v both the p-side and nt-side dopant. An imparity that can act as either a donor or an acceptor is referred to as an amphnseric dopant. ExerCine 2.1 Eitergy Qoic Pt(a) I eV ms eqaal to ham macy jontes nf energy? )b) gus equal to hosv many eV at 300 K? (ci The toniaatton energy of acceptors and donors in Si in rosghly equal Its ...........? (d) E (Si) 0 (b) fiT r 5 c o tncinasing 0 c ••...... 5 c 00000000 wnum tnmpeiatate 151 Figure 2.13 Vissatieotion of (a) danat and (hi aceepton action Asing the energy baud msdel. www.EasyEngineering.net = if) The energy reqaired to iontee a hydrogen atom initially in then St (oil eV 0 = (e) E (SiG,) 5 = = I state is _? 1.00 x lO jooles. 15 (0.fi17 5 10 li3OOi = 0.0259eV at 300 K. (ci The ionization energy of doponts is eqaal to 1K 5 al the dopant sites. As discussed in Subsection 2.3.4, E m 0.1 eV for dopunts in Si. (di K 5 (Si) = 1.12 eV at 300 K (see Sabsection 2.2.4). (u) E (SiG,) asS eV (see Sabsectiqu 2.2.4). 5 (f) Makitig ate of Eq. (2.1) in Section 2.1, the Isydrogen atom ionioalion energy iv = 13.fieV. I 39 36 n SEMICONDUCTOR FUNDAMENTALS CARRIER MODELING Figure 2.11 Ib) a) Pseadwhydnugeu atom mudel far the d000e-site band. Figure 2.10 Visaotieatioe of(a) donor and (hi acceptor action lIning tho banding model. In (a) the Colamn V element P is aabstitsted far a Si atom; in (hi the Colamo III element B is sabsiitsted far a Si atom. 2(4wKejs) The esplanatias of acceptor action follows a similar line of reasotning. The Colititte lii acceptors Itave three valence electrons tmd cannot complete one of the semicondnctor hands mhen subatitated for Si atoms in the nemicondoctoc lattice (sea Fig. 2. lOb). The Colansa III ototo, however, readily accepts (hence the name “acceptor”) an electron from a nearby Si—Si bond, themby completing its own handing scheme and in the pracms cre ating a hale that can wander ahoat the lattice. Here agota there is on incmaae in only ooe type of carrier. The negativety chaeged acceptor ion (acceptor atom pins accepted electron) cannot move, and no electrons are released in the hole-creation process. The foregoing bonding-model-based esplanation of dopant action is reasonably on derstandable. There are, nevertheless, a few loose ends. For one, me noted that the fifth donor electron was rather weakly bound and readily freed at room temperature. How does see interpret the relative term “weakly boand”? It takes 1 eV to break Si—Si bonds and very few of the Si—Si bonds are broken at room lemperatare. Perhaps “weakly bonnd” means a binding energy =0.1 eV or less? The question also agises as to how one visnaliacs dnpaat action in terms of the energy band model. Both of the cited qnestioas, as it lnrns nat, involve energy considerations and are actually interrelated. Let as concentrate first sn the binding energy of the fifth donor electron. Cmdely speaking, the positively charged donor-core-plan-fifth-electron may be likened to a hydro 37 = ns —0.1 eV 1 K uh where K 5 is the St dtelectrtc constant (K 5 — (2.5) = 11.0). Actaal donor-site binding energies in Si are ltstcd in Table 2.3. The observed bittding energies are seen In be in good agreement with the Eq. (2.5) estimate and, confirns.iag the earlier speeslation, are ronghly Si band gap energy. 1/20 the = Havtng established the strength of dspant-site bands, we are now in a position to tackle the probleiti of how one vtsaaliees dopant Action asing the energy band model. Working on the problem, we note first that when an electron is released from a donor it becomes a cotidnetton band electron. If the energy absorbed at the donor is precisely eqaal to the electron btndmg energy, the released electron will moreover have the lowest possible en ergy it tise condticttng band—namety, Ec. Adding an energy IE Ito the bound electron, in other words, raises the electron’s energy to Ec. Hence, we are led to conclade Ihal the boned electron occaples an allowed electronic level an energy 9 I below the enudnetion 1K band edge, or, as visnaliced tn Fig. 2.12, donor sites can be incorporated ida the energy band scltemn by adding allowed electronic levels at an energy E = E En. Note that the donor energy level is represenled by a set of dashes, inslead of a csnlinaoas linn, he canse an electron bound to a donor site is tocalieed in space; i.e., a bonnd electron does not leave the general So vicinity of Ihe donor. The relative closeness of En to E of conrse refiect.s the fact that (Si). 0 — En = I%l = (l/20)E gen atom (see Pig. 2.11). Conceptually, the donor core replaces the hydrogen-atom nacteas nod the fifth donor electron replaces the hydrogen-atom elnclron. Is the real hydrogen atom the electron moves of conese in a vacuum, can be characterieed by the muss of a free Table 2.3 electron, and, referring to Eq. (2.1), has a groand-slate binding energy of 13.fi eV. lathe pseado-hydrogen atom, on the other hand, the orbiting electron moves throogh a sea of Si atoms and is characserieed hy us effective mast. Hence, in the donor oe psenda-atom case, 0 mnst be the permiltivity of free space mnst be replaced by the permittivily of Si and m replaced by m. We therefore conclude Ilsat the binding energy (En) of the fiftln donor electron is apprssimutely Dopant-Site Binding Energies. Dnssnrs 1 5 E Acceptors Sb F As 0.039eV B Al Ga In j 0 JE — 0.045 eV 0.054eV 0.045 0.0fi7 0.022 0.lfi eV nV eV eV www.EasyEngineering.net 39 5IMtCONDnCtnn FUNDAMENTALS CARRIER MODELING 39 cient energy at temperatures T —s 0 K for a valence band electron to make the transilioe to as acceptnr site. Increasing temperatnre, implying an increased store of thermal energy, (01 facilitates electrons jstopisg from the valence bond onlo the acceptor levels. The remnvol a, s.ta5ev ‘F of etectrons from the valence band of ccavse cmatns holes. At mom tnmperatsre, essentially all of the acceptor sites are filled with an escesnelectran and an increased hole cancentra ttnn is effected in the osaterial. ‘fo complete this sitbsection, a fese w’ords are in order concemittg the doping of nonelemental semiconductorn sach an DeAn. Gopant action in GaAs follow’s the name geoeral Oenor site isJ_t.t2 cv Figure 2.12 Additioti of the £ £ denot tenets in the enengy band diagram. Dashes of width As emphmiee the tmalieed sabre of the hoand donor-situ states. The actanl visaalieatian of dopast action asing thn energy band model is pictared in Pig. 2.13. Enamining the left-hand side of Fig. 2.13(a), one fieds ott the donor sites filled with bonnd electrons at temperatures T —s 0 K. This is trne becanse .eery little thermal energy is available to encite electrons from the donor sites iota Ihe eondnclion band at these very low femserataren. The sitsation changes, of coarse, as the temperatsre is incremed, with more and more of the weakly booed electrons being donated to the condactios band. At eonm temperature the ionication of the donors is all bal total, giving rise to the simatinn pictsred at the estreme right of Fig. 2 .l3(a(. Althoagh we have concenlraled ne donors, the sitnation for acceptors is cottspletnly anatogoss. As vissaliced in Fig. 2.13(b), acceptors introduce allowed electronic levels into the fothiddeo gap at an energy slightly above the valence band edge. Allow’ temperatures, all of these sites will be empty—there is insaffi . a, an e.n.e. 0 - OFt unons temperstum tnsseasisn c principles bat in slightly more tnvolved becanse of the enistence of two differettt latlice-nite atossis. Completely analogous to the doping of a Si crystal, the Column VI elements 5, Se, and Te act as donors when replacing the Catomo V element As in the GaAs lattice. ww w.E Similarly, the Colame It elements Be, Mg. and Zn act as acceptors when replacing the Column III element Ga. A stew sitsaliou arises when Colume IV elements snch as Si and Ge are incorporated Into GaAs, Si typically mplacen Gag the GaAs lattice,aod is a pnpnlar si-type dopant. Howevev under certain conditions Si can be made to replace An in the GaAs ltittiiC, tisereby functioning anon acceptor. In fact GaAs pit junctions have born fabricated mltere Si ssa.v both the p-side and nt-side dopant. An imparity that can act as either a donor or an acceptor is referred to as an amphnseric dopant. asy En ExerCine 2.1 Eitergy Qoic gin Pt(a) I eV ms eqaal to ham macy jontes nf energy? )b) gus equal to hosv many eV at 300 K? eer (e) E (SiG,) 5 = if) The energy reqaired to iontee a hydrogen atom initially in then St (oil eV (b) fiT 0 r 5 c o tncinasing 0 c ••...... 5 c 00000000 wnum tnmpeiatate 151 Figure 2.13 ing (ci The toniaatton energy of acceptors and donors in Si in rosghly equal Its ...........? (d) E (Si) = 0 = = I state is .ne _? 1.00 x lO jooles. 15 (0.fi17 5 10 li3OOi = 0.0259eV at 300 K. (ci The ionization energy of doponts is eqaal to 1K 5 al the dopant sites. As discussed in Subsection 2.3.4, E m 0.1 eV for dopunts in Si. (di K 5 (Si) = 1.12 eV at 300 K (see Sabsection 2.2.4). (u) E (SiG,) asS eV (see Sabsectiqu 2.2.4). 5 (f) Makitig ate of Eq. (2.1) in Section 2.1, the Isydrogen atom ionioalion energy iv = 13.fieV. I Vissatieotion of (a) danat and (hi aceepton action Asing the energy baud msdel. www.EasyEngineering.net t www.EasyEngineering.net 40 CARRIER MODELING SEMICONDUCTOR FUNDAMENTALS 2.4.1 Density of States 2.3.5 Carrier-Related Terminology g nilrce this particotar Since terminology is often a nrnorbling block to noderstandin and the section with section is replete with specialized tennis, it scents appropriate to conclade carnier-rClated alt overniew of carrier-related terrnirrnlogy. Appronirrtately one half of the of rite rcmainder thin tire in nection; ter)ns that follow were intrndnced and defined carlicr and their terms are heinrg tinted here for tIre litsl torte. All of the terms are widely errrplnyed delininions siroald be eorntoinled to rrremnory. amonnts Dnpariia—specifle impurity arents firer are added to senricorrdactors in eorrtrolted n. for the express pat-pose of increasing eitlrer the electron or tire hub eotncentratio saanple nr pore semicortdncr extremely Intrinsic scnnrcnndnctnr—sndoped semicnodnctnr; whose prop cotrtainmnrg an insignificant arnoarrr of iroprttity atoms; a seroienordoclor erties are native to tIre nratenial. properties are Lerrirraic arrrrironrdnr-ror-——dnped senriconrdnclor; a ncntticerrdnctor whose comrnroiled by added iorpority atoras. ww 41 Wherm the energy band nrodel soas first introdacod in Section 2.2 we indicated that the total number of allowed states in each band was fortr tintres the namber of atoms in the crystal. Not mentioned nI the inme was lmnw tire allowed states were distributed inn energy; I e how nnany states were no be foontd at any given enrergy in tire cnndscnian and valence bands We are now nrrteeenred in thmn enrergy dinrrrbatinn of slates, or detraity of staten. as it in more cunnrnnanhy krmown, becaasc tine state distribution in an essential component in detererixing carrier distrrbrnsions and concentortions Ta determnrre the desnrrd density of states, it is necessary rn pcrfnrtmr an analysis based on qaantnm.nnechanical considerations. Herein we will roerely stnmmariee the results of - the analysis, namely, foe energres tot too far remuved from the barnd edges, one finds w.E as y En gin e I EwE. I dopamrt. Donnr—irrrparity arortr rlmat increases the elertron eomreentrarirrnr; n-type dopartc Ar-cepnnr——inapnrity atnnm that increases the hole correentrariont; p-type moore electronn than ri-type nncrnerial—a dannr-doped material; a senrieondeetnr enntaining holes. more holes than p-type nrareriol—an acceptor-doped rrraterial; a nemicondocror containing electrons. sample, elCetrons itt Mn/tinny cot-i-icr—tire rrnmmst abundant Carrier in a given nemicnndaernr ant ri-type material, holes in a p-type material. eri ng. ne snmple; holes in an ildinnnr’iry carrier—the leant rrbnrndanr Carrier in a ginen nnmicondnrror ri-type nraternal. electrons in a p-type material. t N 2.4 STATE AND CARRIER DISTRIBUTIONS properties and lip to thin point in the modeling pmcesa we have concentrated on carrier natnre. Practically information of a rnnceptnral, qrralitatisn, t; at most, semiqnantitativC roost semicon speaking, there in often a treed far none detailed itrfornmatinn. For example, Concentrations rnside doctors are doped, arid the precise notnerical value of the carrier ititerent is tIre distribution doped semnncnndtnctorx is of ranrine ietewst. Another property of this section ff0 bflflin of carriers as a function of energy in the respective energy hands. In pnpnlatinns. The de the procenn of deceloping a nrom derailerl description of the carrier arid concentra velopment will encntrnatly lend to relationships for the carrier disrnibatioas (2.flo) rtru\/tEr (2.flb) wirere g)E) aind g, (E)axe the dentairy of states at an energy H in the conduction and valence bands, respectivel’ What exactly uhoold be krrosrn and remembered ahoat the cited density of stales 5 For one, ntts nmpornaur to grasp the genreral density of states concept. The density of states can be likened to the descrrptrun of the sealing in a football stadium, with the nnmber of seals in tIre sladnnm a gwen distance from the playing field corresponding to the number of states a specified energy interval froth E, or E,.. Second, the general farno of the relationships should be acted. As nllastratefi no Fig. 2.14, g,(E) is zero at A) and increases as flue sqaace root of energy when one proceeds opward into tine conduction bond. Similarly, gjE) is precisely zero at E,, and rncceases with the square rout of energy as one proceeds dowaward from E, into the s’alence band. Also Tome that differences between g,(E and g, (H) stem from differences iii the carrier effective masses. If m were equal nn m, the seating (stares) en both sides of the football field (the baud gap) wonld be mirror imngen of each other Frrrally, considering rbnsely spuced energies H and E + dE in the respective hands, one can stale . fi,(E) eepresenzs the number of condscrinu band states/em t tying in the energy range beisveeo H and H + dE (if Em H,), g,. (H)dE represents the number of valence band states/cm 5 lying in the energy mnge bemween Hand E + dE(ifEm Ej. tions nvimhin snmicoodactors ander eqnilibriam cottduriuns. www.EasyEngineering.net 42 nEMICONDnaCTGR FUNDAMENTALS 43 CARRrER MODELING Ia e,hKl I — 0 eI a n m 1 -0 / cc 1 liar /C-E —a— 0 mar n,lEl—’ c— a K Ibm c a 0K FigurE 2,15 Energy degeedenree of the Pormi fnnnrine. (a) T —nO K; (b) onnernlieed Tm OK plot with the energy coordinate expressed in kyaoirn. El aod g,(EI g l Figurs 2.14 ftoooml energy dependence of g,lEl ond g,(E) new the band edges. 5 ann rite density of statni in rho cnnduerinn and nalonce bondn, respectinely. where Er It therefore follows that g (A) and gJE) themselves are nnmnbgrs/anit volnme-anit energy, or typically, nnmbees/rmr.eV. 2.4.2 The Fermi Function Wheeens the density of staten tells one how many states exist ala given energy H, the Fermi fnnctinnflE) specifies how many of the eninting niates or the energy E will be filled with an electron. oreqoinalearl); 1(E) specrfles, nuder eqnrlibrram conditions, the probability that an available state or an ennrgy H will be occupied by an electron. Mathematically speaking, the Fermi fnnctinn is simply a probability dinrrrbnrinn fnnctioo. In mathematical symbols, - T = Fermi energy or Fermi level = Boltemaon constant (it = temperatcre in Kelvin (K) = fi.fl17 x l0 eV1K) Seekrng tnsrght rntn the nalnre of the nerely inlrndnced fnnction. let us begin by inves tigating the Fermi fnncrton’n energy dependence. Consider first temperatures where T —n OK. As T—n OK, (E Er)IkT.m —m for all energies E <Er and (E Er)/kT_4 mm fm all energies Em Er. Hencef(E < Eg) —a I/[l + exp(—w)} I andf(E> Er) —t 1/ ft + esp(+wJ 0. Thin result ts plotted in Pig. 2 .tS(a) and in simply interpreted as — — —n meaning that all states as- energies below Er wilt be filled and all states at energies above E wrIt be empty for teniperarares T 0 K. In other words, there is a sharp catoff in the fllitng of allowed energy staten at the Fermi energy E when the sysleno temperature ap proaches absobarr cern. Let ns next consider remperatceen Tm 0 K. Examining the Fermi function, we make the following pertinent obseroarions. If E = Er.f)Er) = 1/2. (H) If Em Er 4’ 3k?’, esp[)E )/kT] m I andf(E) 0 E evp(—(E Er)/kTJ. Conse quently, above Er + 3kT the Fermi fanctian or filled-state probability decays expo nentially to zero with increasing energy. Moreover, most states at energies 3kTor mare above Er will be empty. — — El+emnZrmmar (2.7) - www.EasyEngineering.net 40 CARRIER MODELING SEMICONDUCTOR FUNDAMENTALS 41 2.4.1 Density of States 2.3.5 Carrier-Related Terminology g nilrce this particotar Since terminology is often a nrnorbling block to noderstandin and the section with section is replete with specialized tennis, it scents appropriate to conclade carnier-rClated alt overniew of carrier-related terrnirrnlogy. Appronirrtately one half of the of rite rcmainder thin tire in nection; ter)ns that follow were intrndnced and defined carlicr and their terms are heinrg tinted here for tIre litsl torte. All of the terms are widely errrplnyed delininions siroald be eorntoinled to rrremnory. amonnts Dnpariia—specifle impurity arents firer are added to senricorrdactors in eorrtrolted n. for the express pat-pose of increasing eitlrer the electron or tire hub eotncentratio saanple nr pore semicortdncr extremely Intrinsic scnnrcnndnctnr—sndoped semicnodnctnr; whose prop cotrtainmnrg an insignificant arnoarrr of iroprttity atoms; a seroienordoclor erties are native to tIre nratenial. properties are Lerrirraic arrrrironrdnr-ror-——dnped senriconrdnclor; a ncntticerrdnctor whose comrnroiled by added iorpority atoras. Wherm the energy band nrodel soas first introdacod in Section 2.2 we indicated that the total number of allowed states in each band was fortr tintres the namber of atoms in the crystal. Not mentioned nI the inme was lmnw tire allowed states were distributed inn energy; I e how nnany states were no be foontd at any given enrergy in tire cnndscnian and valence bands We are now nrrteeenred in thmn enrergy dinrrrbatinn of slates, or detraity of staten. as it in more cunnrnnanhy krmown, becaasc tine state distribution in an essential component in detererixing carrier distrrbrnsions and concentortions Ta determnrre the desnrrd density of states, it is necessary rn pcrfnrtmr an analysis based on qaantnm.nnechanical considerations. Herein we will roerely stnmmariee the results of - the analysis, namely, foe energres tot too far remuved from the barnd edges, one finds ww dopamrt. Donnr—irrrparity arortr rlmat increases the elertron eomreentrarirrnr; n-type dopartc Ar-cepnnr——inapnrity atnnm that increases the hole correentrariont; p-type moore electronn than ri-type nncrnerial—a dannr-doped material; a senrieondeetnr enntaining holes. more holes than p-type nrareriol—an acceptor-doped rrraterial; a nemicondocror containing electrons. sample, elCetrons itt Mn/tinny cot-i-icr—tire rrnmmst abundant Carrier in a given nemicnndaernr ant ri-type material, holes in a p-type material. snmple; holes in an ildinnnr’iry carrier—the leant rrbnrndanr Carrier in a ginen nnmicondnrror ri-type nraternal. electrons in a p-type material. N 2.4 STATE AND CARRIER DISTRIBUTIONS properties and lip to thin point in the modeling pmcesa we have concentrated on carrier natnre. Practically information of a rnnceptnral, qrralitatisn, t; at most, semiqnantitativC roost semicon speaking, there in often a treed far none detailed itrfornmatinn. For example, Concentrations rnside doctors are doped, arid the precise notnerical value of the carrier ititerent is tIre distribution doped semnncnndtnctorx is of ranrine ietewst. Another property of this section ff0 bflflin of carriers as a function of energy in the respective energy hands. In pnpnlatinns. The de the procenn of deceloping a nrom derailerl description of the carrier arid concentra velopment will encntrnatly lend to relationships for the carrier disrnibatioas w.IE a I EwE. (2.flo) rtru\/tEr syE ngi (2.flb) wirere g)E) aind g, (E)axe the dentairy of states at an energy H in the conduction and valence bands, respectivel’ What exactly uhoold be krrosrn and remembered ahoat the cited density of stales 5 For one, ntts nmpornaur to grasp the genreral density of states concept. The density of states can be likened to the descrrptrun of the sealing in a football stadium, with the nnmber of seals in tIre sladnnm a gwen distance from the playing field corresponding to the number of states a specified energy interval froth E, or E,.. Second, the general farno of the relationships should be acted. As nllastratefi no Fig. 2.14, g,(E) is zero at A) and increases as flue sqaace root of energy when one proceeds opward into tine conduction bond. Similarly, gjE) is precisely zero at E,, and rncceases with the square rout of energy as one proceeds dowaward from E, into the s’alence band. Also Tome that differences between g,(E and g, (H) stem from differences iii the carrier effective masses. If m were equal nn m, the seating (stares) en both sides of the football field (the baud gap) wonld be mirror imngen of each other Frrrally, considering rbnsely spuced energies H and E + dE in the respective hands, one can stale nee r . ing . net fi,(E) eepresenzs the number of condscrinu band states/em t tying in the energy range beisveeo H and H + dE (if Em H,), g,. (H)dE represents the number of valence band states/cm 5 lying in the energy mnge bemween Hand E + dE(ifEm Ej. tions nvimhin snmicoodactors ander eqnilibriam cottduriuns. www.EasyEngineering.net 42 nEMICONDnaCTGR FUNDAMENTALS 43 CARRrER MODELING Ia e,hKl I — 0 eI a n m 1 -0 / cc 1 liar /C-E —a— 0 mar n,lEl—’ c— a K Ibm c a 0K FigurE 2,15 Energy degeedenree of the Pormi fnnnrine. (a) T —nO K; (b) onnernlieed Tm OK plot with the energy coordinate expressed in kyaoirn. El aod g,(EI g l Figurs 2.14 ftoooml energy dependence of g,lEl ond g,(E) new the band edges. 5 ann rite density of statni in rho cnnduerinn and nalonce bondn, respectinely. where Er It therefore follows that g (A) and gJE) themselves are nnmnbgrs/anit volnme-anit energy, or typically, nnmbees/rmr.eV. 2.4.2 The Fermi Function Wheeens the density of staten tells one how many states exist ala given energy H, the Fermi fnnctinnflE) specifies how many of the eninting niates or the energy E will be filled with an electron. oreqoinalearl); 1(E) specrfles, nuder eqnrlibrram conditions, the probability that an available state or an ennrgy H will be occupied by an electron. Mathematically speaking, the Fermi fnnctinn is simply a probability dinrrrbnrinn fnnctioo. In mathematical symbols, - T = Fermi energy or Fermi level = Boltemaon constant (it = temperatcre in Kelvin (K) = fi.fl17 x l0 eV1K) Seekrng tnsrght rntn the nalnre of the nerely inlrndnced fnnction. let us begin by inves tigating the Fermi fnncrton’n energy dependence. Consider first temperatures where T —n OK. As T—n OK, (E Er)IkT.m —m for all energies E <Er and (E Er)/kT_4 mm fm all energies Em Er. Hencef(E < Eg) —a I/[l + exp(—w)} I andf(E> Er) —t 1/ ft + esp(+wJ 0. Thin result ts plotted in Pig. 2 .tS(a) and in simply interpreted as — — —n meaning that all states as- energies below Er wilt be filled and all states at energies above E wrIt be empty for teniperarares T 0 K. In other words, there is a sharp catoff in the fllitng of allowed energy staten at the Fermi energy E when the sysleno temperature ap proaches absobarr cern. Let ns next consider remperatceen Tm 0 K. Examining the Fermi function, we make the following pertinent obseroarions. If E = Er.f)Er) = 1/2. (H) If Em Er 4’ 3k?’, esp[)E )/kT] m I andf(E) 0 E evp(—(E Er)/kTJ. Conse quently, above Er + 3kT the Fermi fanctian or filled-state probability decays expo nentially to zero with increasing energy. Moreover, most states at energies 3kTor mare above Er will be empty. — — El+emnZrmmar (2.7) - 40 CARRIER MODELING SEMICONDUCTOR FUNDAMENTALS 41 2.4.1 Density of States 2.3.5 Carrier-Related Terminology g nilrce this particotar Since terminology is often a nrnorbling block to noderstandin and the section with section is replete with specialized tennis, it scents appropriate to conclade carnier-rClated alt overniew of carrier-related terrnirrnlogy. Appronirrtately one half of the of rite rcmainder thin tire in nection; ter)ns that follow were intrndnced and defined carlicr and their terms are heinrg tinted here for tIre litsl torte. All of the terms are widely errrplnyed delininions siroald be eorntoinled to rrremnory. amonnts Dnpariia—specifle impurity arents firer are added to senricorrdactors in eorrtrolted n. for the express pat-pose of increasing eitlrer the electron or tire hub eotncentratio saanple nr pore semicortdncr extremely Intrinsic scnnrcnndnctnr—sndoped semicnodnctnr; whose prop cotrtainmnrg an insignificant arnoarrr of iroprttity atoms; a seroienordoclor erties are native to tIre nratenial. properties are Lerrirraic arrrrironrdnr-ror-——dnped senriconrdnclor; a ncntticerrdnctor whose comrnroiled by added iorpority atoras. Wherm the energy band nrodel soas first introdacod in Section 2.2 we indicated that the total number of allowed states in each band was fortr tintres the namber of atoms in the crystal. Not mentioned nI the inme was lmnw tire allowed states were distributed inn energy; I e how nnany states were no be foontd at any given enrergy in tire cnndscnian and valence bands We are now nrrteeenred in thmn enrergy dinrrrbatinn of slates, or detraity of staten. as it in more cunnrnnanhy krmown, becaasc tine state distribution in an essential component in detererixing carrier distrrbrnsions and concentortions Ta determnrre the desnrrd density of states, it is necessary rn pcrfnrtmr an analysis based on qaantnm.nnechanical considerations. Herein we will roerely stnmmariee the results of - the analysis, namely, foe energres tot too far remuved from the barnd edges, one finds I EwE. I dopamrt. Donnr—irrrparity arortr rlmat increases the elertron eomreentrarirrnr; n-type dopartc Ar-cepnnr——inapnrity atnnm that increases the hole correentrariont; p-type moore electronn than ri-type nncrnerial—a dannr-doped material; a senrieondeetnr enntaining holes. more holes than p-type nrareriol—an acceptor-doped rrraterial; a nemicondocror containing electrons. sample, elCetrons itt Mn/tinny cot-i-icr—tire rrnmmst abundant Carrier in a given nemicnndaernr ant ri-type material, holes in a p-type material. snmple; holes in an ildinnnr’iry carrier—the leant rrbnrndanr Carrier in a ginen nnmicondnrror ri-type nraternal. electrons in a p-type material. N 2.4 STATE AND CARRIER DISTRIBUTIONS properties and lip to thin point in the modeling pmcesa we have concentrated on carrier natnre. Practically information of a rnnceptnral, qrralitatisn, t; at most, semiqnantitativC roost semicon speaking, there in often a treed far none detailed itrfornmatinn. For example, Concentrations rnside doctors are doped, arid the precise notnerical value of the carrier ititerent is tIre distribution doped semnncnndtnctorx is of ranrine ietewst. Another property of this section ff0 bflflin of carriers as a function of energy in the respective energy hands. In pnpnlatinns. The de the procenn of deceloping a nrom derailerl description of the carrier arid concentra velopment will encntrnatly lend to relationships for the carrier disrnibatioas (2.flo) rtru\/tEr (2.flb) wirere g)E) aind g, (E)axe the dentairy of states at an energy H in the conduction and valence bands, respectivel’ What exactly uhoold be krrosrn and remembered ahoat the cited density of stales 5 For one, ntts nmpornaur to grasp the genreral density of states concept. The density of states can be likened to the descrrptrun of the sealing in a football stadium, with the nnmber of seals in tIre sladnnm a gwen distance from the playing field corresponding to the number of states a specified energy interval froth E, or E,.. Second, the general farno of the relationships should be acted. As nllastratefi no Fig. 2.14, g,(E) is zero at A) and increases as flue sqaace root of energy when one proceeds opward into tine conduction bond. Similarly, gjE) is precisely zero at E,, and rncceases with the square rout of energy as one proceeds dowaward from E, into the s’alence band. Also Tome that differences between g,(E and g, (H) stem from differences iii the carrier effective masses. If m were equal nn m, the seating (stares) en both sides of the football field (the baud gap) wonld be mirror imngen of each other Frrrally, considering rbnsely spuced energies H and E + dE in the respective hands, one can stale . fi,(E) eepresenzs the number of condscrinu band states/em t tying in the energy range beisveeo H and H + dE (if Em H,), g,. (H)dE represents the number of valence band states/cm 5 lying in the energy mnge bemween Hand E + dE(ifEm Ej. tions nvimhin snmicoodactors ander eqnilibriam cottduriuns. www.EasyEngineering.net 42 nEMICONDnaCTGR FUNDAMENTALS 43 CARRrER MODELING Ia e,hKl I — 0 eI a n m 1 -0 / cc 1 liar /C-E —a— 0 mar n,lEl—’ ww w .Ea El aod g,(EI g l Figurs 2.14 ftoooml energy dependence of g,lEl ond g,(E) new the band edges. 5 ann rite density of statni in rho cnnduerinn and nalonce bondn, respectinely. syE ngi K Ibm c a 0K where Er nee rin g It therefore follows that g (A) and gJE) themselves are nnmnbgrs/anit volnme-anit energy, or typically, nnmbees/rmr.eV. 2.4.2 The Fermi Function .ne t Wheeens the density of staten tells one how many states exist ala given energy H, the Fermi fnnctinnflE) specifies how many of the eninting niates or the energy E will be filled with an electron. oreqoinalearl); 1(E) c— a FigurE 2,15 Energy degeedenree of the Pormi fnnnrine. (a) T —nO K; (b) onnernlieed Tm OK plot with the energy coordinate expressed in kyaoirn. specrfles, nuder eqnrlibrram conditions, the probability that an available state or an ennrgy H will be occupied by an electron. Mathematically speaking, the Fermi fnnctinn is simply a probability dinrrrbnrinn fnnctioo. In mathematical symbols, - T = Fermi energy or Fermi level = Boltemaon constant (it = temperatcre in Kelvin (K) = fi.fl17 x l0 eV1K) Seekrng tnsrght rntn the nalnre of the nerely inlrndnced fnnction. let us begin by inves tigating the Fermi fnncrton’n energy dependence. Consider first temperatures where T —n OK. As T—n OK, (E Er)IkT.m —m for all energies E <Er and (E Er)/kT_4 mm fm all energies Em Er. Hencef(E < Eg) —a I/[l + exp(—w)} I andf(E> Er) —t 1/ ft + esp(+wJ 0. Thin result ts plotted in Pig. 2 .tS(a) and in simply interpreted as — — —n meaning that all states as- energies below Er wilt be filled and all states at energies above E wrIt be empty for teniperarares T 0 K. In other words, there is a sharp catoff in the fllitng of allowed energy staten at the Fermi energy E when the sysleno temperature ap proaches absobarr cern. Let ns next consider remperatceen Tm 0 K. Examining the Fermi function, we make the following pertinent obseroarions. If E = Er.f)Er) = 1/2. (H) If Em Er 4’ 3k?’, esp[)E )/kT] m I andf(E) 0 E evp(—(E Er)/kTJ. Conse quently, above Er + 3kT the Fermi fanctian or filled-state probability decays expo nentially to zero with increasing energy. Moreover, most states at energies 3kTor mare above Er will be empty. — — El+emnZrmmar www.EasyEngineering.net (2.7) - 40 CARRIER MODELING SEMICONDUCTOR FUNDAMENTALS 41 2.4.1 Density of States 2.3.5 Carrier-Related Terminology g nilrce this particotar Since terminology is often a nrnorbling block to noderstandin and the section with section is replete with specialized tennis, it scents appropriate to conclade carnier-rClated alt overniew of carrier-related terrnirrnlogy. Appronirrtately one half of the of rite rcmainder thin tire in nection; ter)ns that follow were intrndnced and defined carlicr and their terms are heinrg tinted here for tIre litsl torte. All of the terms are widely errrplnyed delininions siroald be eorntoinled to rrremnory. amonnts Dnpariia—specifle impurity arents firer are added to senricorrdactors in eorrtrolted n. for the express pat-pose of increasing eitlrer the electron or tire hub eotncentratio saanple nr pore semicortdncr extremely Intrinsic scnnrcnndnctnr—sndoped semicnodnctnr; whose prop cotrtainmnrg an insignificant arnoarrr of iroprttity atoms; a seroienordoclor erties are native to tIre nratenial. properties are Lerrirraic arrrrironrdnr-ror-——dnped senriconrdnclor; a ncntticerrdnctor whose comrnroiled by added iorpority atoras. Wherm the energy band nrodel soas first introdacod in Section 2.2 we indicated that the total number of allowed states in each band was fortr tintres the namber of atoms in the crystal. Not mentioned nI the inme was lmnw tire allowed states were distributed inn energy; I e how nnany states were no be foontd at any given enrergy in tire cnndscnian and valence bands We are now nrrteeenred in thmn enrergy dinrrrbatinn of slates, or detraity of staten. as it in more cunnrnnanhy krmown, becaasc tine state distribution in an essential component in detererixing carrier distrrbrnsions and concentortions Ta determnrre the desnrrd density of states, it is necessary rn pcrfnrtmr an analysis based on qaantnm.nnechanical considerations. Herein we will roerely stnmmariee the results of - the analysis, namely, foe energres tot too far remuved from the barnd edges, one finds I EwE. I dopamrt. Donnr—irrrparity arortr rlmat increases the elertron eomreentrarirrnr; n-type dopartc Ar-cepnnr——inapnrity atnnm that increases the hole correentrariont; p-type moore electronn than ri-type nncrnerial—a dannr-doped material; a senrieondeetnr enntaining holes. more holes than p-type nrareriol—an acceptor-doped rrraterial; a nemicondocror containing electrons. sample, elCetrons itt Mn/tinny cot-i-icr—tire rrnmmst abundant Carrier in a given nemicnndaernr ant ri-type material, holes in a p-type material. snmple; holes in an ildinnnr’iry carrier—the leant rrbnrndanr Carrier in a ginen nnmicondnrror ri-type nraternal. electrons in a p-type material. N 2.4 STATE AND CARRIER DISTRIBUTIONS properties and lip to thin point in the modeling pmcesa we have concentrated on carrier natnre. Practically information of a rnnceptnral, qrralitatisn, t; at most, semiqnantitativC roost semicon speaking, there in often a treed far none detailed itrfornmatinn. For example, Concentrations rnside doctors are doped, arid the precise notnerical value of the carrier ititerent is tIre distribution doped semnncnndtnctorx is of ranrine ietewst. Another property of this section ff0 bflflin of carriers as a function of energy in the respective energy hands. In pnpnlatinns. The de the procenn of deceloping a nrom derailerl description of the carrier arid concentra velopment will encntrnatly lend to relationships for the carrier disrnibatioas (2.flo) rtru\/tEr (2.flb) wirere g)E) aind g, (E)axe the dentairy of states at an energy H in the conduction and valence bands, respectivel’ What exactly uhoold be krrosrn and remembered ahoat the cited density of stales 5 For one, ntts nmpornaur to grasp the genreral density of states concept. The density of states can be likened to the descrrptrun of the sealing in a football stadium, with the nnmber of seals in tIre sladnnm a gwen distance from the playing field corresponding to the number of states a specified energy interval froth E, or E,.. Second, the general farno of the relationships should be acted. As nllastratefi no Fig. 2.14, g,(E) is zero at A) and increases as flue sqaace root of energy when one proceeds opward into tine conduction bond. Similarly, gjE) is precisely zero at E,, and rncceases with the square rout of energy as one proceeds dowaward from E, into the s’alence band. Also Tome that differences between g,(E and g, (H) stem from differences iii the carrier effective masses. If m were equal nn m, the seating (stares) en both sides of the football field (the baud gap) wonld be mirror imngen of each other Frrrally, considering rbnsely spuced energies H and E + dE in the respective hands, one can stale . fi,(E) eepresenzs the number of condscrinu band states/em t tying in the energy range beisveeo H and H + dE (if Em H,), g,. (H)dE represents the number of valence band states/cm 5 lying in the energy mnge bemween Hand E + dE(ifEm Ej. tions nvimhin snmicoodactors ander eqnilibriam cottduriuns. www.EasyEngineering.net 42 nEMICONDnaCTGR FUNDAMENTALS 43 CARRrER MODELING Ia e,hKl I — 0 eI a n m 1 -0 / cc 1 liar /C-E —a— 0 mar n,lEl—’ c— a K ww w.E Ibm c a 0K FigurE 2,15 Energy degeedenree of the Pormi fnnnrine. (a) T —nO K; (b) onnernlieed Tm OK plot with the energy coordinate expressed in kyaoirn. El aod g,(EI g l Figurs 2.14 ftoooml energy dependence of g,lEl ond g,(E) new the band edges. 5 ann rite density of statni in rho cnnduerinn and nalonce bondn, respectinely. where Er It therefore follows that g (A) and gJE) themselves are nnmnbgrs/anit volnme-anit energy, or typically, nnmbees/rmr.eV. 2.4.2 The Fermi Function Wheeens the density of staten tells one how many states exist ala given energy H, the Fermi fnnctinnflE) specifies how many of the eninting niates or the energy E will be filled with an electron. oreqoinalearl); 1(E) specrfles, nuder eqnrlibrram conditions, the probability that an available state or an ennrgy H will be occupied by an electron. Mathematically speaking, the Fermi fnnctinn is simply a probability dinrrrbnrinn fnnctioo. In mathematical symbols, - T asy En = Fermi energy or Fermi level = Boltemaon constant (it = temperatcre in Kelvin (K) gin = fi.fl17 x l0 eV1K) eer ing Seekrng tnsrght rntn the nalnre of the nerely inlrndnced fnnction. let us begin by inves tigating the Fermi fnncrton’n energy dependence. Consider first temperatures where T —n OK. As T—n OK, (E Er)IkT.m —m for all energies E <Er and (E Er)/kT_4 mm fm all energies Em Er. Hencef(E < Eg) —a I/[l + exp(—w)} I andf(E> Er) —t 1/ ft + esp(+wJ 0. Thin result ts plotted in Pig. 2 .tS(a) and in simply interpreted as — — —n .ne meaning that all states as- energies below Er wilt be filled and all states at energies above E wrIt be empty for teniperarares T 0 K. In other words, there is a sharp catoff in the fllitng of allowed energy staten at the Fermi energy E when the sysleno temperature ap proaches absobarr cern. Let ns next consider remperatceen Tm 0 K. Examining the Fermi function, we make the following pertinent obseroarions. If E = Er.f)Er) = 1/2. (H) If Em Er 4’ 3k?’, esp[)E )/kT] m I andf(E) 0 E evp(—(E Er)/kTJ. Conse quently, above Er + 3kT the Fermi fanctian or filled-state probability decays expo nentially to zero with increasing energy. Moreover, most states at energies 3kTor mare above Er will be empty. — — El+emnZrmmar (2.7) www.EasyEngineering.net t - _ ____ _______ www.EasyEngineering.net 44 SEMICONDUCTOR FUNDAMENTALS CARRIER MODELINU 1 — cxp)(E — Ev)IST). Below )/6T] 4 1 aitdf(E) 0 (iii) If ES E — 3kT, esp[(E — E — 36T, tltetefore, [1 — f(E)), the probability that a gisen state ssill be eutpe decays eaponeetially to reen with decreasing energy. Mast stales at energies 3kT or tnoee below A 0 will he filled we conclude LvE,. EEr kT — kT (Si). 5 (iv) At eooist temperature (T 300 K), kT 0.0259 eV and 3kT = 0.0777 eV 4 E Compared to the Si bond gap, the 3kT energy interval that appears prominently in the T>OK foretalism is typically quite sotall. ‘.‘ Tlte peopeeties just cited oee eefleeted and somtaocieed in the T>OK Feetni function plot displayed in Fig. 2.15(b). Before concluding the discussion here, it is perhaps worthwhile to reemphasize thus the Fermi function applies only under eqnilibrioto rooditiour. The Fermi fnnctioe, however, is universal in the sense titus it applies with equal validity so all materialo—insalatoin, sctnicottdttctors, ottd metols. Although ieteodoecd in reluliouship to semiconductors, ttse Fermi fusetion is not dependent in any svoy on the special nature of semiconductors bnt is sitttply a statistical function associated with electrons in general Finally, the relative posi ), an item of obvious concern, ts 0 0 (or E tioning of the Fermi energy A 0 compared to A treated in subsequent subsections. ww E. + A Ar The Fermi level is positioned at midgap. w.E as y En gin e ExerCise 2.2 (C) Exeroise 2.3 In this cscretse soc wish to euomine in more detail how the Fermi function varies ssith tentperature, P: The probobility that o slate is filled at the coodoetion band edge (E) is precisely ). Where Is 0 eqoal to the probability that a state is empty at the valence band edge (A the Fermi level located) Pt Successively setting T = 100, 200, 300, and then 400 K, compute and plotf(A) versus iSA = A — Lv for —0.2eV S iSA 40,2 cV. Atlf(E vnrsns AL curves should be superimposed on a single set of coordinates. eri ng. ne St The Fermi fonction, f(A), specifies the probability of electrons occupying states ala given energy A. The probability thot a state is empty (not filled) at a given energy A is equal to I — f(A). Here we are told ) 0 f(A = 1 — S t program script... % Constant kfl.6t7e-5; ToComputation proper for 6=1:4; Tl00°ii; kT=krT; dB(ii,l)no55kT; forjj=t :101 + ewr_ervtc = MATLAB %Fernit Fnsction Calcniation, f(AE,T) Since ) 0 1(A 45 and f(iijj)= 1/) 1 +rup(dB(ii,jj)/kT)); dE(djj+ lfrdB(ii,jj)+0.l°lrT; 1 — f(A ) 0 = — I + ewErv& = 1 ‘+ end ned dB=dBQ,l :jj); etcr_c,1oT %This step strips the mba dO value www.EasyEngineering.net r 45 SEMICONDUCTOR FUNDAMEttL CARRIER MODEiJNU °YoPlottieg result close nr haS aiaerani Dmssa of nuns Occupancy Suitors Comes disu’ibiOma plcs(dE’,f’(; grid; %Note the transpose (‘) to form data columns slahel(’B-BF(rV)’); ylobel(’f(B)’); tcstcos,.2,’T400K’); N tnut(-.03,.l,T=lO0K’); ‘— e,lc] — Program ootput... f arita ‘ c v,iElflc) ,“j flE) crium -fIclI g Ia1 Er abuor midnap iwirors 5 C. u ,ic) — .—-e,1a3 C, H Ej_ 1 1 ‘N lbs tSr near snidgap C, E.Et’leV) o,lu3 -,lff 2.4.3 Equilibrium Distribuflion of Carriers Having cstublished she distribution of ovoilabie band slates and thn probability of filling those states under equilibrium conditions, we can now easily deduce the distribution of carriers iu the respective eeergy bonds. To be specific, the desired distribution is obtained by simply multiplying the oppropriatr density of states by the appropriate occupancy factor—gjA)f(E) yields the distribution of electrons in the conduction bond and “[ j E, fl Id Er below midnap Figure 2.16 Carrierdistribatious )nos drawn to scale) in the respective bands svlier the Permi level is posisiunrd (a) abase midgap, (hI near mideap, and (c) below midgap. Alma sheuu in each emr are coordinated sketchet of the energy band diagram, density of states, and the wespancy faetots (the Fermi Sureties and nne miras the Fermi function). (E) (I 0 g f(A)) yields the distribution of hales (unfilled states) in the vuleoce bond. Sample carrier distribnsions fur three different assomed positions of the Fermi energy — (along with associated eucrgy band diagram, Fermi function, and density of states plots) are pictured in Fig. 2.16. Bnumining Pig. 2.16, wn note in general that all curriec distributions are zero at lhn I; 47 _ ____ _______ www.EasyEngineering.net 44 SEMICONDUCTOR FUNDAMENTALS CARRIER MODELINU 1 — cxp)(E — Ev)IST). Below )/6T] 4 1 aitdf(E) 0 (iii) If ES E — 3kT, esp[(E — E — 36T, tltetefore, [1 — f(E)), the probability that a gisen state ssill be eutpe decays eaponeetially to reen with decreasing energy. Mast stales at energies 3kT or tnoee below A 0 will he filled we conclude LvE,. EEr kT — kT (Si). 5 (iv) At eooist temperature (T 300 K), kT 0.0259 eV and 3kT = 0.0777 eV 4 E Compared to the Si bond gap, the 3kT energy interval that appears prominently in the T>OK foretalism is typically quite sotall. ‘.‘ Tlte peopeeties just cited oee eefleeted and somtaocieed in the T>OK Feetni function plot displayed in Fig. 2.15(b). Before concluding the discussion here, it is perhaps worthwhile to reemphasize thus the Fermi function applies only under eqnilibrioto rooditiour. The Fermi fnnctioe, however, is universal in the sense titus it applies with equal validity so all materialo—insalatoin, sctnicottdttctors, ottd metols. Although ieteodoecd in reluliouship to semiconductors, ttse Fermi fusetion is not dependent in any svoy on the special nature of semiconductors bnt is sitttply a statistical function associated with electrons in general Finally, the relative posi ), an item of obvious concern, ts 0 0 (or E tioning of the Fermi energy A 0 compared to A treated in subsequent subsections. E. + A Ar ww The Fermi level is positioned at midgap. w.E a (C) Exeroise 2.3 syE ngi ExerCise 2.2 In this cscretse soc wish to euomine in more detail how the Fermi function varies ssith tentperature, P: The probobility that o slate is filled at the coodoetion band edge (E) is precisely ). Where Is 0 eqoal to the probability that a state is empty at the valence band edge (A the Fermi level located) Pt Successively setting T = 100, 200, 300, and then 400 K, compute and plotf(A) versus iSA = A — Lv for —0.2eV S iSA 40,2 cV. Atlf(E vnrsns AL curves should be superimposed on a single set of coordinates. St The Fermi fonction, f(A), specifies the probability of electrons occupying states ala given energy A. The probability thot a state is empty (not filled) at a given energy A is equal to I — f(A). Here we are told S ) 0 f(A = 1 = MATLAB nee r ing . program script... %Fernit Fnsction Calcniation, f(AE,T) % Constant kfl.6t7e-5; — ToComputation proper for 6=1:4; Tl00°ii; kT=krT; dB(ii,l)no55kT; forjj=t :101 Since ) 0 1(A 45 + ewr_ervtc and f(iijj)= net 1/) 1 +rup(dB(ii,jj)/kT)); dE(djj+ lfrdB(ii,jj)+0.l°lrT; 1 — f(A ) 0 = — I + ewErv& = 1 ‘+ end ned dB=dBQ,l :jj); etcr_c,1oT %This step strips the mba dO value www.EasyEngineering.net r 45 SEMICONDUCTOR FUNDAMEttL CARRIER MODEiJNU °YoPlottieg result close nr haS aiaerani Dmssa of nuns Occupancy Suitors Comes disu’ibiOma plcs(dE’,f’(; grid; %Note the transpose (‘) to form data columns slahel(’B-BF(rV)’); ylobel(’f(B)’); tcstcos,.2,’T400K’); N tnut(-.03,.l,T=lO0K’); ‘— e,lc] — Program ootput... f arita ‘ c v,iElflc) ,“j flE) crium -fIclI g Ia1 Er abuor midnap iwirors 5 C. u ,ic) — .—-e,1a3 C, H Ej_ 1 1 ‘N lbs tSr near snidgap C, E.Et’leV) o,lu3 -,lff 2.4.3 Equilibrium Distribuflion of Carriers Having cstublished she distribution of ovoilabie band slates and thn probability of filling those states under equilibrium conditions, we can now easily deduce the distribution of carriers iu the respective eeergy bonds. To be specific, the desired distribution is obtained by simply multiplying the oppropriatr density of states by the appropriate occupancy factor—gjA)f(E) yields the distribution of electrons in the conduction bond and “[ j E, fl Id Er below midnap Figure 2.16 Carrierdistribatious )nos drawn to scale) in the respective bands svlier the Permi level is posisiunrd (a) abase midgap, (hI near mideap, and (c) below midgap. Alma sheuu in each emr are coordinated sketchet of the energy band diagram, density of states, and the wespancy faetots (the Fermi Sureties and nne miras the Fermi function). (E) (I 0 g f(A)) yields the distribution of hales (unfilled states) in the vuleoce bond. Sample carrier distribnsions fur three different assomed positions of the Fermi energy — (along with associated eucrgy band diagram, Fermi function, and density of states plots) are pictured in Fig. 2.16. Bnumining Pig. 2.16, wn note in general that all curriec distributions are zero at lhn I; 47 _ ____ _______ 44 SEMICONDUCTOR FUNDAMENTALS CARRIER MODELINU 1 — cxp)(E — Ev)IST). Below )/6T] 4 1 aitdf(E) 0 (iii) If ES E — 3kT, esp[(E — E — 36T, tltetefore, [1 — f(E)), the probability that a gisen state ssill be eutpe decays eaponeetially to reen with decreasing energy. Mast stales at energies 3kT or tnoee below A 0 will he filled we conclude LvE,. EEr kT — kT (Si). 5 (iv) At eooist temperature (T 300 K), kT 0.0259 eV and 3kT = 0.0777 eV 4 E Compared to the Si bond gap, the 3kT energy interval that appears prominently in the T>OK foretalism is typically quite sotall. ‘.‘ 45 Tlte peopeeties just cited oee eefleeted and somtaocieed in the T>OK Feetni function plot displayed in Fig. 2.15(b). Before concluding the discussion here, it is perhaps worthwhile to reemphasize thus the Fermi function applies only under eqnilibrioto rooditiour. The Fermi fnnctioe, however, is universal in the sense titus it applies with equal validity so all materialo—insalatoin, sctnicottdttctors, ottd metols. Although ieteodoecd in reluliouship to semiconductors, ttse Fermi fusetion is not dependent in any svoy on the special nature of semiconductors bnt is sitttply a statistical function associated with electrons in general Finally, the relative posi ), an item of obvious concern, ts 0 0 (or E tioning of the Fermi energy A 0 compared to A treated in subsequent subsections. E. + A Ar The Fermi level is positioned at midgap. (C) Exeroise 2.3 ExerCise 2.2 In this cscretse soc wish to euomine in more detail how the Fermi function varies ssith tentperature, P: The probobility that o slate is filled at the coodoetion band edge (E) is precisely ). Where Is 0 eqoal to the probability that a state is empty at the valence band edge (A the Fermi level located) Pt Successively setting T = 100, 200, 300, and then 400 K, compute and plotf(A) versus iSA = A — Lv for —0.2eV S iSA 40,2 cV. Atlf(E vnrsns AL curves should be superimposed on a single set of coordinates. St The Fermi fonction, f(A), specifies the probability of electrons occupying states ala given energy A. The probability thot a state is empty (not filled) at a given energy A is equal to I — f(A). Here we are told S ) 0 f(A = 1 ToComputation proper for 6=1:4; Tl00°ii; kT=krT; dB(ii,l)no55kT; forjj=t :101 + ewr_ervtc = program script... % Constant kfl.6t7e-5; — Since ) 0 1(A MATLAB %Fernit Fnsction Calcniation, f(AE,T) and f(iijj)= 1/) 1 +rup(dB(ii,jj)/kT)); dE(djj+ lfrdB(ii,jj)+0.l°lrT; 1 — f(A ) 0 = — I + ewErv& = 1 ‘+ end ned dB=dBQ,l :jj); etcr_c,1oT www.EasyEngineering.net 45 %This step strips the mba dO value r SEMICONDUCTOR FUNDAMEttL CARRIER MODEiJNU °YoPlottieg result close nr haS aiaerani Dmssa of nuns Occupancy Suitors Comes disu’ibiOma plcs(dE’,f’(; grid; %Note the transpose (‘) to form data columns slahel(’B-BF(rV)’); ylobel(’f(B)’); tcstcos,.2,’T400K’); N tnut(-.03,.l,T=lO0K’); ‘— e,lc] — Program ootput... f arita ‘ c v,iElflc) ,“j flE) crium -fIclI g ww w Ia1 Er abuor midnap iwirors 5 .Ea C. u ,ic) syE — .—-e,1a3 ngi E.Et’leV) C, nee rin g H Ej_ 1 1 ‘N lbs tSr near snidgap .ne t C, o,lu3 -,lff 2.4.3 Equilibrium Distribuflion of Carriers Having cstublished she distribution of ovoilabie band slates and thn probability of filling those states under equilibrium conditions, we can now easily deduce the distribution of carriers iu the respective eeergy bonds. To be specific, the desired distribution is obtained by simply multiplying the oppropriatr density of states by the appropriate occupancy factor—gjA)f(E) yields the distribution of electrons in the conduction bond and j E, fl Id Er below midnap Figure 2.16 Carrierdistribatious )nos drawn to scale) in the respective bands svlier the Permi level is posisiunrd (a) abase midgap, (hI near mideap, and (c) below midgap. Alma sheuu in each emr are coordinated sketchet of the energy band diagram, density of states, and the wespancy faetots (the Fermi Sureties and nne miras the Fermi function). (E) (I 0 g f(A)) yields the distribution of hales (unfilled states) in the vuleoce bond. Sample carrier distribnsions fur three different assomed positions of the Fermi energy — (along with associated eucrgy band diagram, Fermi function, and density of states plots) are pictured in Fig. 2.16. Bnumining Pig. 2.16, wn note in general that all curriec distributions are zero at lhn www.EasyEngineering.net “[ I; 47 _ ____ _______ 44 SEMICONDUCTOR FUNDAMENTALS CARRIER MODELINU 1 — cxp)(E — Ev)IST). Below )/6T] 4 1 aitdf(E) 0 (iii) If ES E — 3kT, esp[(E — E — 36T, tltetefore, [1 — f(E)), the probability that a gisen state ssill be eutpe decays eaponeetially to reen with decreasing energy. Mast stales at energies 3kT or tnoee below A 0 will he filled we conclude LvE,. EEr kT — kT (Si). 5 (iv) At eooist temperature (T 300 K), kT 0.0259 eV and 3kT = 0.0777 eV 4 E Compared to the Si bond gap, the 3kT energy interval that appears prominently in the T>OK foretalism is typically quite sotall. ‘.‘ 45 Tlte peopeeties just cited oee eefleeted and somtaocieed in the T>OK Feetni function plot displayed in Fig. 2.15(b). Before concluding the discussion here, it is perhaps worthwhile to reemphasize thus the Fermi function applies only under eqnilibrioto rooditiour. The Fermi fnnctioe, however, is universal in the sense titus it applies with equal validity so all materialo—insalatoin, sctnicottdttctors, ottd metols. Although ieteodoecd in reluliouship to semiconductors, ttse Fermi fusetion is not dependent in any svoy on the special nature of semiconductors bnt is sitttply a statistical function associated with electrons in general Finally, the relative posi ), an item of obvious concern, ts 0 0 (or E tioning of the Fermi energy A 0 compared to A treated in subsequent subsections. E. + A Ar The Fermi level is positioned at midgap. (C) Exeroise 2.3 ExerCise 2.2 In this cscretse soc wish to euomine in more detail how the Fermi function varies ssith tentperature, P: The probobility that o slate is filled at the coodoetion band edge (E) is precisely ). Where Is 0 eqoal to the probability that a state is empty at the valence band edge (A the Fermi level located) Pt Successively setting T = 100, 200, 300, and then 400 K, compute and plotf(A) versus iSA = A — Lv for —0.2eV S iSA 40,2 cV. Atlf(E vnrsns AL curves should be superimposed on a single set of coordinates. St The Fermi fonction, f(A), specifies the probability of electrons occupying states ala given energy A. The probability thot a state is empty (not filled) at a given energy A is equal to I — f(A). Here we are told S ) 0 f(A = 1 = program script... % Constant kfl.6t7e-5; — ToComputation proper for 6=1:4; Tl00°ii; kT=krT; dB(ii,l)no55kT; forjj=t :101 Since ) 0 1(A MATLAB %Fernit Fnsction Calcniation, f(AE,T) + ewr_ervtc and f(iijj)= 1/) 1 +rup(dB(ii,jj)/kT)); dE(djj+ lfrdB(ii,jj)+0.l°lrT; 1 — f(A ) 0 = — I + ewErv& = 1 ‘+ end ned dB=dBQ,l :jj); etcr_c,1oT r 45 %This step strips the mba dO value www.EasyEngineering.net SEMICONDUCTOR FUNDAMEttL CARRIER MODEiJNU °YoPlottieg result close nr haS aiaerani Dmssa of nuns Occupancy Suitors Comes disu’ibiOma plcs(dE’,f’(; grid; %Note the transpose (‘) to form data columns slahel(’B-BF(rV)’); ylobel(’f(B)’); tcstcos,.2,’T400K’); N tnut(-.03,.l,T=lO0K’); ‘— e,lc] — Program ootput... arita ‘ ww w.E f c v,iElflc) ,“j flE) crium -fIclI g Ia1 Er abuor midnap iwirors 5 C. — C, asy u ,ic) .—-e,1a3 Ej_ H Eng1 lbs tSr near snidgap C, E.Et’leV) o,lu3 -,lff 2.4.3 Equilibrium Distribuflion of Carriers Having cstublished she distribution of ovoilabie band slates and thn probability of filling those states under equilibrium conditions, we can now easily deduce the distribution of carriers iu the respective eeergy bonds. To be specific, the desired distribution is obtained by simply multiplying the oppropriatr density of states by the appropriate occupancy factor—gjA)f(E) yields the distribution of electrons in the conduction bond and “[ 1 ‘N ine j fl eri E, ng. net Id Er below midnap Figure 2.16 Carrierdistribatious )nos drawn to scale) in the respective bands svlier the Permi level is posisiunrd (a) abase midgap, (hI near mideap, and (c) below midgap. Alma sheuu in each emr are coordinated sketchet of the energy band diagram, density of states, and the wespancy faetots (the Fermi Sureties and nne miras the Fermi function). (E) (I 0 g f(A)) yields the distribution of hales (unfilled states) in the vuleoce bond. Sample carrier distribnsions fur three different assomed positions of the Fermi energy — (along with associated eucrgy band diagram, Fermi function, and density of states plots) are pictured in Fig. 2.16. Bnumining Pig. 2.16, wn note in general that all curriec distributions are zero at lhn I; www.EasyEngineering.net 47 ________ ____________ _ www.EasyEngineering.net 48 SEMICONDUCTOR FUNDAMENTALS CANNIER MODELiNG band edges, ranch a peak volae very rinse so E or E,, and then decay oery rapidly toworsl nero as one moses spword into the conduction band or downward into the onlence hoed. In otiter words, most of the carriers ore grouped estergelienHy in Use near vicinity of the baud edges. Aitother general poistt to tote in site effect of tlte Feritti level pOsiliOtiiog oe the relative nagoitode of the carrier distrihatious. Whest E 0 is positioned in the upper half of the lannd gap (or higher), the electron distribotion greatly oolweighs Ilte hole distrihstiott. Althoogh botit the ftlled-stoteoecopaeey fitctor (f(E)) oitd Ilte esopty-statenecupancy factor [1 f)E7) foil off exponentially as one proceeds froto the bond edges deeper into the condoetion and valence bontls, respectively, (1 iCE)) is clearly ttttteh smaller tltattf(E) at corresponding energies if Er lies in the npper half of the bnttsl gop. Lowering Er effec tively slides the neenpancy pldts downward, givittg rise to a nearly equal ouseber of carriers wltest 5 is at tite middle of sIte gap. Likewise, a predontittoitce of holes results when E lies below the middle of the gap. The orgomeot here ossnmes, of coarse, tltot g,(E( and g(E) ore of the some order of mognitode at eorrespottding energies (as is tlte ease for Si and Ge). Also, referring badk so the previons snbseetion, the statements concerning the occupancy factors fnllistg ttff enpottetttiolly in tlte respective hoods ore valid prooided — 48 E, C, Ci —s---—— Er fl-Y,;—-—— Fignre 2.18 seinicousdossor “At a glance” representation of iisisinsis )lefi), n-type (middle), nod p-type (rightl materials osing the energy hand diagram. — ww w.E Ifr 3kTErtsEr+3kT as y En gin e The information just presented conceroissg the carrier distribsstioos and the relative moguitades of the carrier natnbers finds widespread osage. The information, however, is often conveyed inns abbreviated or shorthand foshioo. Figore 2.17. for example, shows eoms000 may of represesssing the carrier essergy dislribnsiosss. Ttte greatest nusober of circles or dots are drown close to r and E,, reflecting she peak in the carrier roneentrolions oem tlse bond odges. TIse smaller number of doss as one progresses opward into the con dnesiou bassd erodely toodels she rapid falloff in the eleesross density wish increasing eoergy. An extensively sstilieed mratss of eonveyiog the relation mogssisnde of the carrier numbers is displayed in Fig. 2.18. To represent an islrisssie sssaseriol, a dashed line is drown in ap proximately she soiddle of she bond gap nest labeled E . TIse orar-soidgop positissniog of E,, 5 the intrinsic Fermi level, is of coarse consistent svisls she previoasly cited foes that the nec lrois assd hole xnmbers are about eqoal when Er is near she eesster of the bond gap. Sitnilarly, o solid line labeled Er appearing above nsidgap sells one at a glance that the sesoieondsctor in qonstion is n-type; a solid line labeled Er appearing below midgop signifies that the seosieondnesor is p-type. Note fistolly shot she dashed E 5 line also typically appears on the eri ng. ne t energy bassst diagrams ehaeoeterietug exsrisssie semicondeesers. The E 5 tine io sneh eases represents use espersed positioning of she Fermi level (1 the toaserial were iosrinsie, and is serves nsa reference energy level dividing the upper and lower halves of she hood gap 2.5 EQUILIBRIuM CARRIER CONCENTRATIgJIi We have arrived as as important poses in she carrier modeling process For the moss port, this section simply embodies she cetsoinosion of sser modeling efforts, wish working rein tsonshsps for the eqaslibriam carrier cosseentrasiens 8 essablished so complement she heist qoalssassve carrier information presensed is previous soctiors.j(eforsnnetety the emphasis on the developsoens of mathematical relationships makes the float assoall on the eon-icr nodding ssmsois a utile more ardnons (nod perhapsjnss ii his boring). Hopefelly, she reader can slay foensedjA eommesss ts also in order concerning the presenlasien herein of alternasser fornss for use carrier relationships. The alternative fesms eon be likened so she differ ent kinds of wreeches esed, for exsmple, in hotne and ontosnobite repairs. The open-end wrenels, she boo wrench, and she rasehes wrench all serve she some general psrpeso. In souse apphieassosss one can nsn any of the wrenches. in other applications, however, a spe cial sssnasson rostrsess the type of wrench employed or favors the nse of one wrench over 000shec The same is lmc of she olsernalive carrier relationships. Finally, boxes are drawn arenud expresstoes that find widespread usage. A sissgtr-wallrd hon signifies a modomsely important resell; a doable-walled box, a nery imporsans result. 2.5.1 Formulas for .. ... ,A C, qA 0 o p n and p Ssnerg, (E) nE represents she enmbor of conduction band stoles/em 3 tying in the E so E ÷ dE energy range, and f(E) specifies the probability that on available state at en energy E will be oceepsed by on eleclron, it then follows thas g,(E)f(E)dE gives she camber of eondeesiois band eleelrens/em lying is the E so E + dE energy range, and HJE)f(pdff integrated overall conduesson band energies mess yield the total camber of eleesross in the senduesion band. In other words, integration over the equilibriom distribution of electrons in slse soedeetion bond yields the eqettibriom electron enneentrasios. A similar slotemenl ran hr nsode relative so she hole concentration. We therefore senetede e, Figure 2,17 Oehrsnasie reproseisiotiee ef sorrier energy disiribasiens. www.EasyEngineering.net All UEMICONDnCTON FUNDAMENTALS CANNtEN MonnLsrao and also defining = = J’g(fijf() c::, , I gj)l — f(]dE Nv m’s/Th — rem \/E-rE dE I + e5eer10T Jo, 3 nrh New letting q — f’ Jo the “effective” density ef valence bend siales (2.t3b) .23 one obtains ‘IcC 0 = 10 F (q,) N (2.l4o) and, by analogy, C •Ot ‘4-, = 5 N 50 F (q,) (2.14b) (2.lob) yields ° 31 (kY) (2.i3o) “Np” (2. bc) 3 sr°5 [a], 2 p E,) 1sT = mV’ 5 = (2.ioa) 1sT (Er the “effective” density of conduction band stases (2.9) /_ (E—E,) m(kTl 30 (2.flb) Seeking explicit expressioos for the carrier roocentrasions, let as focus our efforts on she st-integral. (The osologons p-integral manipnlosions are lefs so the reader as no exer cise.) Snbssitasing shn Eq. (2.6a) expression for gJE) and the Eq. (2.7) nxprnssios ferf(E) into Eq. (2.8a), one obtains — \,, flQ, (2.8o) ‘q’°dq I + c’s—” (2.11) where q, m (E, )/kT 0 E The Eq. (2.14) relationships are avery general resets, valid for any cusnerixable posi tioning of the Fermi level. The constants N end N me readily ealcnleted; ml 300 K, /cm 3 5 = (2.510 x 10 i )(m / sn (379. The seine of the Fermi integral roche obtained S from available sables, from plots, or by direct cosnpntotion. The general-form relationships, nonetheless, are admittedly combersome and inconvenient to nm in realise analyses. For Innately, simplified closed-form expressions do exist that eon be employed in the vast ma jority of practical problems. To be specific, if Er is restricted to voices Er E, 3kT ibm l/)l ÷ exp(q ropl —(‘si 1 0), and ‘1,)] q,)] for all Em E,(n — — The (2.lOe) simplifleasion on the upper integration limit makes use of she foes that the integrand in qoession falls off rapidly with increasing energy and is essentially euro for energies anly a few kT obeve E,. Hence, extending she upper limit so m has 0 sosaily neg ligible effees on she value of the integral. Even wish the eised simplification, she Eq. (2.11) integral cannot be expressed in a closed form containing simple functions. The integral itself is in foes a sabaloted fnnetion shot can be fnond in a variety of mathematical references. Ideosifying 50 F (q,) JO I + e”” the Fermi-Dirac integral of order 1/2 (2.12) — — 50 F (q,) Likewise, if Er = __ 10r,Oir 0 (2. ISa) E, + 31sT then 50 F (q,) = (2.lSb) 51 ________ ____________ _ www.EasyEngineering.net 48 SEMICONDUCTOR FUNDAMENTALS CANNIER MODELiNG band edges, ranch a peak volae very rinse so E or E,, and then decay oery rapidly toworsl nero as one moses spword into the conduction band or downward into the onlence hoed. In otiter words, most of the carriers ore grouped estergelienHy in Use near vicinity of the baud edges. Aitother general poistt to tote in site effect of tlte Feritti level pOsiliOtiiog oe the relative nagoitode of the carrier distrihatious. Whest E 0 is positioned in the upper half of the lannd gap (or higher), the electron distribotion greatly oolweighs Ilte hole distrihstiott. Althoogh botit the ftlled-stoteoecopaeey fitctor (f(E)) oitd Ilte esopty-statenecupancy factor [1 f)E7) foil off exponentially as one proceeds froto the bond edges deeper into the condoetion and valence bontls, respectively, (1 iCE)) is clearly ttttteh smaller tltattf(E) at corresponding energies if Er lies in the npper half of the bnttsl gop. Lowering Er effec tively slides the neenpancy pldts downward, givittg rise to a nearly equal ouseber of carriers wltest 5 is at tite middle of sIte gap. Likewise, a predontittoitce of holes results when E lies below the middle of the gap. The orgomeot here ossnmes, of coarse, tltot g,(E( and g(E) ore of the some order of mognitode at eorrespottding energies (as is tlte ease for Si and Ge). Also, referring badk so the previons snbseetion, the statements concerning the occupancy factors fnllistg ttff enpottetttiolly in tlte respective hoods ore valid prooided — 48 E, C, Ci —s---—— Er fl-Y,;—-—— Fignre 2.18 seinicousdossor “At a glance” representation of iisisinsis )lefi), n-type (middle), nod p-type (rightl materials osing the energy hand diagram. — Ifr 3kTErtsEr+3kT The information just presented conceroissg the carrier distribsstioos and the relative moguitades of the carrier natnbers finds widespread osage. The information, however, is often conveyed inns abbreviated or shorthand foshioo. Figore 2.17. for example, shows eoms000 may of represesssing the carrier essergy dislribnsiosss. Ttte greatest nusober of circles or dots are drown close to r and E,, reflecting she peak in the carrier roneentrolions oem tlse bond odges. TIse smaller number of doss as one progresses opward into the con dnesiou bassd erodely toodels she rapid falloff in the eleesross density wish increasing eoergy. An extensively sstilieed mratss of eonveyiog the relation mogssisnde of the carrier numbers is displayed in Fig. 2.18. To represent an islrisssie sssaseriol, a dashed line is drown in ap proximately she soiddle of she bond gap nest labeled E . TIse orar-soidgop positissniog of E,, 5 the intrinsic Fermi level, is of coarse consistent svisls she previoasly cited foes that the nec lrois assd hole xnmbers are about eqoal when Er is near she eesster of the bond gap. Sitnilarly, o solid line labeled Er appearing above nsidgap sells one at a glance that the sesoieondsctor in qonstion is n-type; a solid line labeled Er appearing below midgop signifies that the seosieondnesor is p-type. Note fistolly shot she dashed E 5 line also typically appears on the energy bassst diagrams ehaeoeterietug exsrisssie semicondeesers. The E 5 tine io sneh eases represents use espersed positioning of she Fermi level (1 the toaserial were iosrinsie, and is serves nsa reference energy level dividing the upper and lower halves of she hood gap ww w.E a 2.5 EQUILIBRIuM CARRIER CONCENTRATIgJIi nee r ing . 2.5.1 Formulas for .. ... ,A p net n and p Ssnerg, (E) nE represents she enmbor of conduction band stoles/em 3 tying in the E so E ÷ dE energy range, and f(E) specifies the probability that on available state at en energy E will be oceepsed by on eleclron, it then follows thas g,(E)f(E)dE gives she camber of eondeesiois band eleelrens/em lying is the E so E + dE energy range, and HJE)f(pdff integrated overall conduesson band energies mess yield the total camber of eleesross in the senduesion band. In other words, integration over the equilibriom distribution of electrons in slse soedeetion bond yields the eqettibriom electron enneentrasios. A similar slotemenl ran hr nsode relative so she hole concentration. We therefore senetede C, qA 0 o syE ngi We have arrived as as important poses in she carrier modeling process For the moss port, this section simply embodies she cetsoinosion of sser modeling efforts, wish working rein tsonshsps for the eqaslibriam carrier cosseentrasiens 8 essablished so complement she heist qoalssassve carrier information presensed is previous soctiors.j(eforsnnetety the emphasis on the developsoens of mathematical relationships makes the float assoall on the eon-icr nodding ssmsois a utile more ardnons (nod perhapsjnss ii his boring). Hopefelly, she reader can slay foensedjA eommesss ts also in order concerning the presenlasien herein of alternasser fornss for use carrier relationships. The alternative fesms eon be likened so she differ ent kinds of wreeches esed, for exsmple, in hotne and ontosnobite repairs. The open-end wrenels, she boo wrench, and she rasehes wrench all serve she some general psrpeso. In souse apphieassosss one can nsn any of the wrenches. in other applications, however, a spe cial sssnasson rostrsess the type of wrench employed or favors the nse of one wrench over 000shec The same is lmc of she olsernalive carrier relationships. Finally, boxes are drawn arenud expresstoes that find widespread usage. A sissgtr-wallrd hon signifies a modomsely important resell; a doable-walled box, a nery imporsans result. e, Figure 2,17 Oehrsnasie reproseisiotiee ef sorrier energy disiribasiens. www.EasyEngineering.net All UEMICONDnCTON FUNDAMENTALS CANNtEN MonnLsrao and also defining = = J’g(fijf() c::, , I gj)l — f(]dE Nv m’s/Th — rem \/E-rE dE I + e5eer10T Jo, 3 nrh New letting q — f’ Jo the “effective” density ef valence bend siales (2.t3b) .23 one obtains ‘IcC 0 = 10 F (q,) N (2.l4o) and, by analogy, C •Ot ‘4-, = 5 N 50 F (q,) (2.14b) (2.lob) yields ° 31 (kY) (2.i3o) “Np” (2. bc) 3 sr°5 [a], 2 p E,) 1sT = mV’ 5 = (2.ioa) 1sT (Er the “effective” density of conduction band stases (2.9) /_ (E—E,) m(kTl 30 (2.flb) Seeking explicit expressioos for the carrier roocentrasions, let as focus our efforts on she st-integral. (The osologons p-integral manipnlosions are lefs so the reader as no exer cise.) Snbssitasing shn Eq. (2.6a) expression for gJE) and the Eq. (2.7) nxprnssios ferf(E) into Eq. (2.8a), one obtains — \,, flQ, (2.8o) ‘q’°dq I + c’s—” (2.11) where q, m (E, )/kT 0 E The Eq. (2.14) relationships are avery general resets, valid for any cusnerixable posi tioning of the Fermi level. The constants N end N me readily ealcnleted; ml 300 K, /cm 3 5 = (2.510 x 10 i )(m / sn (379. The seine of the Fermi integral roche obtained S from available sables, from plots, or by direct cosnpntotion. The general-form relationships, nonetheless, are admittedly combersome and inconvenient to nm in realise analyses. For Innately, simplified closed-form expressions do exist that eon be employed in the vast ma jority of practical problems. To be specific, if Er is restricted to voices Er E, 3kT ibm l/)l ÷ exp(q ropl —(‘si 1 0), and ‘1,)] q,)] for all Em E,(n — — The (2.lOe) simplifleasion on the upper integration limit makes use of she foes that the integrand in qoession falls off rapidly with increasing energy and is essentially euro for energies anly a few kT obeve E,. Hence, extending she upper limit so m has 0 sosaily neg ligible effees on she value of the integral. Even wish the eised simplification, she Eq. (2.11) integral cannot be expressed in a closed form containing simple functions. The integral itself is in foes a sabaloted fnnetion shot can be fnond in a variety of mathematical references. Ideosifying 50 F (q,) JO I + e”” the Fermi-Dirac integral of order 1/2 (2.12) — — 50 F (q,) Likewise, if Er = __ 10r,Oir 0 (2. ISa) E, + 31sT then 50 F (q,) = (2.lSb) 51 ________ ____________ _ 48 SEMICONDUCTOR FUNDAMENTALS CANNIER MODELiNG band edges, ranch a peak volae very rinse so E or E,, and then decay oery rapidly toworsl nero as one moses spword into the conduction band or downward into the onlence hoed. In otiter words, most of the carriers ore grouped estergelienHy in Use near vicinity of the baud edges. Aitother general poistt to tote in site effect of tlte Feritti level pOsiliOtiiog oe the relative nagoitode of the carrier distrihatious. Whest E 0 is positioned in the upper half of the lannd gap (or higher), the electron distribotion greatly oolweighs Ilte hole distrihstiott. Althoogh botit the ftlled-stoteoecopaeey fitctor (f(E)) oitd Ilte esopty-statenecupancy factor [1 f)E7) foil off exponentially as one proceeds froto the bond edges deeper into the condoetion and valence bontls, respectively, (1 iCE)) is clearly ttttteh smaller tltattf(E) at corresponding energies if Er lies in the npper half of the bnttsl gop. Lowering Er effec tively slides the neenpancy pldts downward, givittg rise to a nearly equal ouseber of carriers wltest 5 is at tite middle of sIte gap. Likewise, a predontittoitce of holes results when E lies below the middle of the gap. The orgomeot here ossnmes, of coarse, tltot g,(E( and g(E) ore of the some order of mognitode at eorrespottding energies (as is tlte ease for Si and Ge). Also, referring badk so the previons snbseetion, the statements concerning the occupancy factors fnllistg ttff enpottetttiolly in tlte respective hoods ore valid prooided — 48 E, C, Ci —s---—— Er fl-Y,;—-—— Fignre 2.18 seinicousdossor “At a glance” representation of iisisinsis )lefi), n-type (middle), nod p-type (rightl materials osing the energy hand diagram. — Ifr 3kTErtsEr+3kT The information just presented conceroissg the carrier distribsstioos and the relative moguitades of the carrier natnbers finds widespread osage. The information, however, is often conveyed inns abbreviated or shorthand foshioo. Figore 2.17. for example, shows eoms000 may of represesssing the carrier essergy dislribnsiosss. Ttte greatest nusober of circles or dots are drown close to r and E,, reflecting she peak in the carrier roneentrolions oem tlse bond odges. TIse smaller number of doss as one progresses opward into the con dnesiou bassd erodely toodels she rapid falloff in the eleesross density wish increasing eoergy. An extensively sstilieed mratss of eonveyiog the relation mogssisnde of the carrier numbers is displayed in Fig. 2.18. To represent an islrisssie sssaseriol, a dashed line is drown in ap proximately she soiddle of she bond gap nest labeled E . TIse orar-soidgop positissniog of E,, 5 the intrinsic Fermi level, is of coarse consistent svisls she previoasly cited foes that the nec lrois assd hole xnmbers are about eqoal when Er is near she eesster of the bond gap. Sitnilarly, o solid line labeled Er appearing above nsidgap sells one at a glance that the sesoieondsctor in qonstion is n-type; a solid line labeled Er appearing below midgop signifies that the seosieondnesor is p-type. Note fistolly shot she dashed E 5 line also typically appears on the energy bassst diagrams ehaeoeterietug exsrisssie semicondeesers. The E 5 tine io sneh eases represents use espersed positioning of she Fermi level (1 the toaserial were iosrinsie, and is serves nsa reference energy level dividing the upper and lower halves of she hood gap 2.5 EQUILIBRIuM CARRIER CONCENTRATIgJIi We have arrived as as important poses in she carrier modeling process For the moss port, this section simply embodies she cetsoinosion of sser modeling efforts, wish working rein tsonshsps for the eqaslibriam carrier cosseentrasiens 8 essablished so complement she heist qoalssassve carrier information presensed is previous soctiors.j(eforsnnetety the emphasis on the developsoens of mathematical relationships makes the float assoall on the eon-icr nodding ssmsois a utile more ardnons (nod perhapsjnss ii his boring). Hopefelly, she reader can slay foensedjA eommesss ts also in order concerning the presenlasien herein of alternasser fornss for use carrier relationships. The alternative fesms eon be likened so she differ ent kinds of wreeches esed, for exsmple, in hotne and ontosnobite repairs. The open-end wrenels, she boo wrench, and she rasehes wrench all serve she some general psrpeso. In souse apphieassosss one can nsn any of the wrenches. in other applications, however, a spe cial sssnasson rostrsess the type of wrench employed or favors the nse of one wrench over 000shec The same is lmc of she olsernalive carrier relationships. Finally, boxes are drawn arenud expresstoes that find widespread usage. A sissgtr-wallrd hon signifies a modomsely important resell; a doable-walled box, a nery imporsans result. 2.5.1 Formulas for .. ... ,A C, qA 0 o e, p n and p Ssnerg, (E) nE represents she enmbor of conduction band stoles/em 3 tying in the E so E ÷ dE energy range, and f(E) specifies the probability that on available state at en energy E will be oceepsed by on eleclron, it then follows thas g,(E)f(E)dE gives she camber of eondeesiois band eleelrens/em lying is the E so E + dE energy range, and HJE)f(pdff integrated overall conduesson band energies mess yield the total camber of eleesross in the senduesion band. In other words, integration over the equilibriom distribution of electrons in slse soedeetion bond yields the eqettibriom electron enneentrasios. A similar slotemenl ran hr nsode relative so she hole concentration. We therefore senetede Figure 2,17 Oehrsnasie reproseisiotiee ef sorrier energy disiribasiens. www.EasyEngineering.net All UEMICONDnCTON FUNDAMENTALS CANNtEN MonnLsrao and also defining = = J’g(fijf() c::, , I gj)l — f(]dE Nv New letting — .Ea m’s/Th — ngi — ° 31 (kY) 3 sr°5 [a], 2 the “effective” density ef valence bend siales ‘q’°dq I + c’s—” (2.t3b) .23 one obtains ‘IcC 0 = 10 F (q,) N (2.l4o) C •Ot ‘4-, (2.ioa) p nee rin g f’ Jo = and, by analogy, E,) yields (2.i3o) “Np” 1sT 1sT the “effective” density of conduction band stases (2.9) (E—E,) (Er = mV’ 5 dE I + e5eer10T /_ syE q rem \/E-rE Jo, 3 nrh m(kTl 30 (2.flb) Seeking explicit expressioos for the carrier roocentrasions, let as focus our efforts on she st-integral. (The osologons p-integral manipnlosions are lefs so the reader as no exer cise.) Snbssitasing shn Eq. (2.6a) expression for gJE) and the Eq. (2.7) nxprnssios ferf(E) into Eq. (2.8a), one obtains ww w \,, flQ, (2.8o) = 5 N 50 F (q,) (2.14b) (2.lob) (2. bc) .ne t (2.11) where q, m (E, )/kT 0 E The Eq. (2.14) relationships are avery general resets, valid for any cusnerixable posi tioning of the Fermi level. The constants N end N me readily ealcnleted; ml 300 K, /cm 3 5 = (2.510 x 10 i )(m / sn (379. The seine of the Fermi integral roche obtained S from available sables, from plots, or by direct cosnpntotion. The general-form relationships, nonetheless, are admittedly combersome and inconvenient to nm in realise analyses. For Innately, simplified closed-form expressions do exist that eon be employed in the vast ma jority of practical problems. To be specific, if Er is restricted to voices Er E, 3kT ibm l/)l ÷ exp(q ropl —(‘si 1 0), and ‘1,)] q,)] for all Em E,(n — — The (2.lOe) simplifleasion on the upper integration limit makes use of she foes that the integrand in qoession falls off rapidly with increasing energy and is essentially euro for energies anly a few kT obeve E,. Hence, extending she upper limit so m has 0 sosaily neg ligible effees on she value of the integral. Even wish the eised simplification, she Eq. (2.11) integral cannot be expressed in a closed form containing simple functions. The integral itself is in foes a sabaloted fnnetion shot can be fnond in a variety of mathematical references. Ideosifying 50 F (q,) JO I + e”” the Fermi-Dirac integral of order 1/2 www.EasyEngineering.net (2.12) — — 50 F (q,) Likewise, if Er = __ 10r,Oir 0 (2. ISa) E, + 31sT then 50 F (q,) = (2.lSb) 51 ________ ____________ _ 48 SEMICONDUCTOR FUNDAMENTALS CANNIER MODELiNG band edges, ranch a peak volae very rinse so E or E,, and then decay oery rapidly toworsl nero as one moses spword into the conduction band or downward into the onlence hoed. In otiter words, most of the carriers ore grouped estergelienHy in Use near vicinity of the baud edges. Aitother general poistt to tote in site effect of tlte Feritti level pOsiliOtiiog oe the relative nagoitode of the carrier distrihatious. Whest E 0 is positioned in the upper half of the lannd gap (or higher), the electron distribotion greatly oolweighs Ilte hole distrihstiott. Althoogh botit the ftlled-stoteoecopaeey fitctor (f(E)) oitd Ilte esopty-statenecupancy factor [1 f)E7) foil off exponentially as one proceeds froto the bond edges deeper into the condoetion and valence bontls, respectively, (1 iCE)) is clearly ttttteh smaller tltattf(E) at corresponding energies if Er lies in the npper half of the bnttsl gop. Lowering Er effec tively slides the neenpancy pldts downward, givittg rise to a nearly equal ouseber of carriers wltest 5 is at tite middle of sIte gap. Likewise, a predontittoitce of holes results when E lies below the middle of the gap. The orgomeot here ossnmes, of coarse, tltot g,(E( and g(E) ore of the some order of mognitode at eorrespottding energies (as is tlte ease for Si and Ge). Also, referring badk so the previons snbseetion, the statements concerning the occupancy factors fnllistg ttff enpottetttiolly in tlte respective hoods ore valid prooided — 48 E, C, Ci —s---—— Er fl-Y,;—-—— Fignre 2.18 seinicousdossor “At a glance” representation of iisisinsis )lefi), n-type (middle), nod p-type (rightl materials osing the energy hand diagram. — Ifr 3kTErtsEr+3kT The information just presented conceroissg the carrier distribsstioos and the relative moguitades of the carrier natnbers finds widespread osage. The information, however, is often conveyed inns abbreviated or shorthand foshioo. Figore 2.17. for example, shows eoms000 may of represesssing the carrier essergy dislribnsiosss. Ttte greatest nusober of circles or dots are drown close to r and E,, reflecting she peak in the carrier roneentrolions oem tlse bond odges. TIse smaller number of doss as one progresses opward into the con dnesiou bassd erodely toodels she rapid falloff in the eleesross density wish increasing eoergy. An extensively sstilieed mratss of eonveyiog the relation mogssisnde of the carrier numbers is displayed in Fig. 2.18. To represent an islrisssie sssaseriol, a dashed line is drown in ap proximately she soiddle of she bond gap nest labeled E . TIse orar-soidgop positissniog of E,, 5 the intrinsic Fermi level, is of coarse consistent svisls she previoasly cited foes that the nec lrois assd hole xnmbers are about eqoal when Er is near she eesster of the bond gap. Sitnilarly, o solid line labeled Er appearing above nsidgap sells one at a glance that the sesoieondsctor in qonstion is n-type; a solid line labeled Er appearing below midgop signifies that the seosieondnesor is p-type. Note fistolly shot she dashed E 5 line also typically appears on the energy bassst diagrams ehaeoeterietug exsrisssie semicondeesers. The E 5 tine io sneh eases represents use espersed positioning of she Fermi level (1 the toaserial were iosrinsie, and is serves nsa reference energy level dividing the upper and lower halves of she hood gap 2.5 EQUILIBRIuM CARRIER CONCENTRATIgJIi We have arrived as as important poses in she carrier modeling process For the moss port, this section simply embodies she cetsoinosion of sser modeling efforts, wish working rein tsonshsps for the eqaslibriam carrier cosseentrasiens 8 essablished so complement she heist qoalssassve carrier information presensed is previous soctiors.j(eforsnnetety the emphasis on the developsoens of mathematical relationships makes the float assoall on the eon-icr nodding ssmsois a utile more ardnons (nod perhapsjnss ii his boring). Hopefelly, she reader can slay foensedjA eommesss ts also in order concerning the presenlasien herein of alternasser fornss for use carrier relationships. The alternative fesms eon be likened so she differ ent kinds of wreeches esed, for exsmple, in hotne and ontosnobite repairs. The open-end wrenels, she boo wrench, and she rasehes wrench all serve she some general psrpeso. In souse apphieassosss one can nsn any of the wrenches. in other applications, however, a spe cial sssnasson rostrsess the type of wrench employed or favors the nse of one wrench over 000shec The same is lmc of she olsernalive carrier relationships. Finally, boxes are drawn arenud expresstoes that find widespread usage. A sissgtr-wallrd hon signifies a modomsely important resell; a doable-walled box, a nery imporsans result. 2.5.1 Formulas for .. ... ,A C, qA 0 o p n and p Ssnerg, (E) nE represents she enmbor of conduction band stoles/em 3 tying in the E so E ÷ dE energy range, and f(E) specifies the probability that on available state at en energy E will be oceepsed by on eleclron, it then follows thas g,(E)f(E)dE gives she camber of eondeesiois band eleelrens/em lying is the E so E + dE energy range, and HJE)f(pdff integrated overall conduesson band energies mess yield the total camber of eleesross in the senduesion band. In other words, integration over the equilibriom distribution of electrons in slse soedeetion bond yields the eqettibriom electron enneentrasios. A similar slotemenl ran hr nsode relative so she hole concentration. We therefore senetede e, Figure 2,17 Oehrsnasie reproseisiotiee ef sorrier energy disiribasiens. www.EasyEngineering.net All UEMICONDnCTON FUNDAMENTALS and also defining = = J’g(fijf() c::, , I gj)l — f(]dE m’s/Th rem \/E-rE dE I + e5eer10T Jo, 3 nrh New letting (2.9) /_ (E—E,) q — f’ Jo ‘q’°dq I + c’s—” (2.i3o) the “effective” density ef valence bend siales (2.11) (2.t3b) .23 one obtains ww w.E ‘IcC 0 = 10 F (q,) N (2.l4o) “Np” asy (2.lob) yields ° 31 (kY) [a], 2 and, by analogy, (2. bc) 3 sr°5 the “effective” density of conduction band stases p E,) 1sT = mV’ 5 = (2.ioa) 1sT (Er m(kTl 30 (2.flb) Nv — \,, flQ, (2.8o) Seeking explicit expressioos for the carrier roocentrasions, let as focus our efforts on she st-integral. (The osologons p-integral manipnlosions are lefs so the reader as no exer cise.) Snbssitasing shn Eq. (2.6a) expression for gJE) and the Eq. (2.7) nxprnssios ferf(E) into Eq. (2.8a), one obtains — C En = 5 N •Ot ‘4-, gin 50 F (q,) (2.14b) eer where q, m (E, )/kT 0 E The Eq. (2.14) relationships are avery general resets, valid for any cusnerixable posi tioning of the Fermi level. The constants N end N me readily ealcnleted; ml 300 K, /cm 3 5 = (2.510 x 10 i )(m / sn (379. The seine of the Fermi integral roche obtained S from available sables, from plots, or by direct cosnpntotion. The general-form relationships, nonetheless, are admittedly combersome and inconvenient to nm in realise analyses. For Innately, simplified closed-form expressions do exist that eon be employed in the vast ma jority of practical problems. To be specific, if Er is restricted to voices Er E, 3kT ibm l/)l ÷ exp(q ropl —(‘si 1 0), and ‘1,)] q,)] for all Em E,(n — ing .ne — The (2.lOe) simplifleasion on the upper integration limit makes use of she foes that the integrand in qoession falls off rapidly with increasing energy and is essentially euro for energies anly a few kT obeve E,. Hence, extending she upper limit so m has 0 sosaily neg ligible effees on she value of the integral. Even wish the eised simplification, she Eq. (2.11) integral cannot be expressed in a closed form containing simple functions. The integral itself is in foes a sabaloted fnnetion shot can be fnond in a variety of mathematical references. Ideosifying 50 F (q,) JO 51 CANNtEN MonnLsrao I + e”” the Fermi-Dirac integral of order 1/2 (2.12) — — 50 F (q,) Likewise, if Er = __ 10r,Oir 0 (2. ISa) E, + 31sT then 50 F (q,) = (2.lSb) www.EasyEngineering.net t www.EasyEngineering.net 52 ‘..e3 s-fl;EwEi.’ r-=; r/75 su)aicossnncvoe s’uuaaeuicsats vere J — —— ... 4, v, aanrrrrie irw,s=,aacrnr vnia. ,no,ron,tatiar — C I Cr aria ... —i )/ILT LOp— y’i is) I(’jt ,i(cy ‘,lLT eAeeceManELtrin (v-ri 1 v:-.tr 2= ‘N’t i Eqaatian (2.21) caps-essex a, ax a fnectian of hnasva qaastisias and can ha axed to campnta ri at a specified tempeeataee or as a fanetiaa of tempeeatara. Namerical vatnes foe she intrinsic carrier caneeaseatiao in Si and Ge at eaam temparatnee svere cited praviaoaly; the best aaaitstbla plots of a, as fanctiaax of temperatara in Si, Ga, and GaAs are displayed in Fig. 2.20 A secand very important a-based relationship faltawa directly frets Eqv. (2.19). trIal siptying the earrexpasdiag sides af Eqs. )2. I 9a) and (2.1 9b) tagether yields sea c, 5 e rrreec,,iia 5L-i,ia,oxaacvir (2.22) Definitina of degaueratoloosdelennrate naintrandartaw. Figure 2.15 ww w.E Er ± It therefore followv that, if E + 3kT Attltangh appaariag trivial, the op peadset relationship (Eq. 2.22) often proves to be extremely nsefal in practical campalatians. If aae of the carrier casceatratians ix lasawa, the rasssaiaing carrier coacentratioa ix readily determined axing Eq. (2.22)—pravided of conrse that the semicotsdactaria in eqailibrians astd nasdeaenerate. E,, — 3k)’ as y En gin e (2.lfla) (C) Exercise 2.4 (2.1 fib) Sabslisassng the Eq. (2.13) definitions af Er and i’/ inta Eq. (2.21), inteadaciag narasatiaatian factaes, and replacing keawn caastaam by their nnmerscal valnrs. one abtaiax = p ,(r,—irr)iar 5 = The atathematical simplification Leading to Eqs. (2.16) a eqatvalcnt to approximating f(E), by simple exponential faocttons—an approsi tite oecapaeey factors,f(E) and 1 motion earlier shown to be valid provided Er wat somewhere tn the band gap no closer is confined, ax noted, to E, + 3kT ar E. than 3kT to either band edge. whenever simply 3hZ instead of cantinoalty repeating the Er restriction, the semteaadartar is band aaid Ia be nandegenerate. Wltenevee r lien in the band gap closer than 3hT to esther edge or actaally penetrates one of the bands, the seaaieoadactor is said to ha degeaerata. These very intpartant teems are also defined psetartatly ta Fig. 2. t9. eri — — ng. ne n and p = Althaagh in closed farm, the Eq. (2.16) reationships are nat in the simplest farm passthle. ma ear and, mace aften than oat. it is the vintptes alternative farm of these retatsonships that eacoasters ia device analyses. The alteroative-farns ratationshtps can be obtained by re and widgap, elate to calling that E,, she Fermi level far an intrinsic semiaaadnctar, lies hence Eqs. (2.16) mast aasaradly apply ta as intrinsic semicaadactar. If this be the ease, = thea speeialiaisg Eqs. (2.16) Ia aa intrinsic sasnieaadactar. ta., settingn = p = a, and Er. one abtains = Ncetfuar . . = 1.028 - (6.11 x to_a)T 0.610 + (7.83 x to -a))’ — — (3.09 5< I0-)I’ (4.46 X 10 -‘)T F: (a) Confirns that the a verses T carve for Si graphed in Fig. 2.20 ix generated employing the mlationshipa nat riled, praeidesd Er in the a, expression in replaced by E EU,, where E, = 0,0074 eV. (In she peevinasly riled article, Barber sug gested axing an canton roeeectian factor of E,, = 0.007 eV. The slightly larger valee employed in the Fig. 2.20 campalatian was specifically chosen to give 01 = 1015, 5 at 300 K.) cm — )2.t7a) ‘.5_i; eCoit’ Er and the effective masses exhibit a weak bat nan-negligible temperatare depan dance. The Er mesas T variation can he modeled to fear-place arcneacy by the fit relationship noted in Frablem 2.1(a). As dedaced from she analysis by Barber [SolidState Electronics, ie, 1039 (1967)). the temperataee dependence of the effective massea aver the range 200 K as Tm 700 K can be approximated by t 2.5.2 Alternative Expressions for () (2.510 X l0in)(v e) it fI’ I’,i,I c www.EasyEngineering.net 56 sesitcoNaucras FUNDAMENTaLs raueice snauLiNa (b) The accepted valae of v, in Si at 300 K has been revised recently to be in agree ment with time experimental a vernal Tdata arqaired by Sproat and Green Jaaenal of Applied Physics. 78, 846 Only 1990). The anthem concluded a, = 1.00 ± 0.03 X l0vaia in Si at 300K. Over the probed Iemprratare range of 275 K ± T 375 K, their esperimensal data raald be fitted by the relationship a = (9.15 x loa)() 9: (a) MATLAn program script. - program script.. %Espenmealal fit of Sproal-Grern ai data (275E 375K) - %ni calcnlatiaa T= 275 :25 : 375 k8.fll7e-5; ci =(9. lSel 9).elTj300).02 aevp(0 5928 /)k°T)) shtaT 5 e Compare the a, cawpated feam this experimental-fit relationship to the part (a) aatpat aver the temperature range of mataal validity. %ssi vs. T ratcalatian far Si (200K (b) MAmAs 700K) axed in Pig. 2.20 %lnitialiratian format short %Castatassts and T-range k8.Gt7e-S; A2.510et9; Erx=0.0074; %Valae wax adjusted to match S&G ni(300K) valne T200:25:700; %Baad Gap vs. T EGO= 1.17; a4.730c-4; b’036; EGEGO-a. °(T. 2)./(T+b); 5 %Dinplay resalt on screen j=tengtb(T); ni\n’); %There are ten spaces between T and ci. fprintf(’\a\n T for 0=’ l:j, fprintf(’ %- I 0.f%-10.3e\n’,T(ii),ai(ii)); end Gatpus from the lava programs in reprodared below. Nate the excellent agreement of the rempasatienal resalts (to svitbia 2%) aver the temperatam mnge of mabel validity. T(K) t ( 5 (a)n ) cw’ 200 275 300 325 350 375 5.246 5< 10 1.059 5< 10 1.000 5< 10:0 6.798 x l0° 3.565 x l0 1.518 x lO 5.449 x lO 400 500 600 700 (cm’ 5 (b)a ) 1.051 x 10 1.006 X IO’ 6.887 5< loin 3.623 5< i5 1.542 5< 10 2.716 X lO 3.908 5< lois 2.865 5< 10 %Effective mass ratio (mar=nan/as0, nsprmp°/nt0) wnr 1.028 ÷ (6.1 ie4).nT )3.09a7).cT. 2; 5 sepr0.fllO ± (7.83e-4).°T (4°6e7)T 2 3 - - %Compatation of ci ni=A.r(IT./300).0(t.5)).c)marowpr).s(0.75)(.aexp(_(EG_Ees)./(2 °k”T)); ¶bl3inplay ontpat as screen jieapsh(T); fprintf(’\n \n T ni\a’); %Tlsrse are tea spares between T and ni. far ii= I:). fpriesf(’%-l 0.f%- 10.3e\n’,T(ii),ai(ii)); end 2.5.4 Charge Neutrality Relationship The relationships established to this point are devoid of an explicit dependence an the dapaat concentrations introdnred into a nemirondarsor. It is the charge neatralsty relation ship that provides she general tie between the earlier and dapaet canrenstasians. To establish the charge centrality relationship, lot av consider a nxmfrrssly doped semi condactar, a semireisdartor wheer the namber af dapant atoms/cm 3 ix the vame every where. Systematically examining little sectians of sIte semicondactor far from any surfaces, and assaming eqnilibriam renditions prevail, one watt inrariably find that each and every section is aharge-nentral, ia., contains canal charge. If this were not the cane, electric fields 57’ 55 ‘..e3 52 s-fl;EwEi.’ r-=; r/75 su)aicossnncvoe s’uuaaeuicsats vere J — —— ... 4, v, aanrrrrie irw,s=,aacrnr vnia. ,no,ron,tatiar — C I Cr aria ... —i ,i(cy I(’jt LOp— y’i ‘,lLT eAeeceManELtrin (v-ri 1 v:-.tr 2= ‘N’t i Eqaatian (2.21) caps-essex a, ax a fnectian of hnasva qaastisias and can ha axed to campnta ri at a specified tempeeataee or as a fanetiaa of tempeeatara. Namerical vatnes foe she intrinsic carrier caneeaseatiao in Si and Ge at eaam temparatnee svere cited praviaoaly; the best aaaitstbla plots of a, as fanctiaax of temperatara in Si, Ga, and GaAs are displayed in Fig. 2.20 A secand very important a-based relationship faltawa directly frets Eqv. (2.19). trIal siptying the earrexpasdiag sides af Eqs. )2. I 9a) and (2.1 9b) tagether yields sea c, www.EasyEngineering.net is) )/ILT 5 e rrreec,,iia 5L-i,ia,oxaacvir (2.22) Definitina of degaueratoloosdelennrate naintrandartaw. Figure 2.15 Er ± It therefore followv that, if E + 3kT ww Attltangh appaariag trivial, the op peadset relationship (Eq. 2.22) often proves to be extremely nsefal in practical campalatians. If aae of the carrier casceatratians ix lasawa, the rasssaiaing carrier coacentratioa ix readily determined axing Eq. (2.22)—pravided of conrse that the semicotsdactaria in eqailibrians astd nasdeaenerate. E,, — 3k)’ ,(r,—irr)iar 5 = (C) Exercise 2.4 (2.1 fib) Sabslisassng the Eq. (2.13) definitions af Er and i’/ inta Eq. (2.21), inteadaciag narasatiaatian factaes, and replacing keawn caastaam by their nnmerscal valnrs. one abtaiax The atathematical simplification Leading to Eqs. (2.16) a eqatvalcnt to approximating f(E), by simple exponential faocttons—an approsi tite oecapaeey factors,f(E) and 1 motion earlier shown to be valid provided Er wat somewhere tn the band gap no closer is confined, ax noted, to E, + 3kT ar E. than 3kT to either band edge. whenever simply 3hZ instead of cantinoalty repeating the Er restriction, the semteaadartar is band aaid Ia be nandegenerate. Wltenevee r lien in the band gap closer than 3hT to esther edge or actaally penetrates one of the bands, the seaaieoadactor is said to ha degeaerata. These very intpartant teems are also defined psetartatly ta Fig. 2. t9. (2.510 X l0in)(v e) — it n and p = ma ear and, mace aften than oat. it is the vintptes alternative farm of these retatsonships that eacoasters ia device analyses. The alteroative-farns ratationshtps can be obtained by re and widgap, elate to calling that E,, she Fermi level far an intrinsic semiaaadnctar, lies hence Eqs. (2.16) mast aasaradly apply ta as intrinsic semicaadactar. If this be the ease, = thea speeialiaisg Eqs. (2.16) Ia aa intrinsic sasnieaadactar. ta., settingn = p = a, and Er. one abtains Ncetfuar . . = 1.028 - (6.11 x to_a)T 0.610 + (7.83 x to -a))’ — — net (3.09 5< I0-)I’ (4.46 X 10 -‘)T F: (a) Confirns that the a verses T carve for Si graphed in Fig. 2.20 ix generated employing the mlationshipa nat riled, praeidesd Er in the a, expression in replaced by E EU,, where E, = 0,0074 eV. (In she peevinasly riled article, Barber sug gested axing an canton roeeectian factor of E,, = 0.007 eV. The slightly larger valee employed in the Fig. 2.20 campalatian was specifically chosen to give 01 = 1015, 5 at 300 K.) cm — )2.t7a) ‘.5_i; eCoit’ ing . Althaagh in closed farm, the Eq. (2.16) reationships are nat in the simplest farm passthle. = n()ee r Er and the effective masses exhibit a weak bat nan-negligible temperatare depan dance. The Er mesas T variation can he modeled to fear-place arcneacy by the fit relationship noted in Frablem 2.1(a). As dedaced from she analysis by Barber [SolidState Electronics, ie, 1039 (1967)). the temperataee dependence of the effective massea aver the range 200 K as Tm 700 K can be approximated by — 2.5.2 Alternative Expressions for syE ngi (2.lfla) = p w.E a fI’ I’,i,I c www.EasyEngineering.net 56 sesitcoNaucras FUNDAMENTaLs raueice snauLiNa (b) The accepted valae of v, in Si at 300 K has been revised recently to be in agree ment with time experimental a vernal Tdata arqaired by Sproat and Green Jaaenal of Applied Physics. 78, 846 Only 1990). The anthem concluded a, = 1.00 ± 0.03 X l0vaia in Si at 300K. Over the probed Iemprratare range of 275 K ± T 375 K, their esperimensal data raald be fitted by the relationship a = (9.15 x loa)() 9: (a) MATLAn program script. - program script.. %Espenmealal fit of Sproal-Grern ai data (275E 375K) - %ni calcnlatiaa T= 275 :25 : 375 k8.fll7e-5; ci =(9. lSel 9).elTj300).02 aevp(0 5928 /)k°T)) shtaT 5 e Compare the a, cawpated feam this experimental-fit relationship to the part (a) aatpat aver the temperature range of mataal validity. %ssi vs. T ratcalatian far Si (200K (b) MAmAs 700K) axed in Pig. 2.20 %lnitialiratian format short %Castatassts and T-range k8.Gt7e-S; A2.510et9; Erx=0.0074; %Valae wax adjusted to match S&G ni(300K) valne T200:25:700; %Baad Gap vs. T EGO= 1.17; a4.730c-4; b’036; EGEGO-a. °(T. 2)./(T+b); 5 %Dinplay resalt on screen j=tengtb(T); ni\n’); %There are ten spaces between T and ci. fprintf(’\a\n T for 0=’ l:j, fprintf(’ %- I 0.f%-10.3e\n’,T(ii),ai(ii)); end Gatpus from the lava programs in reprodared below. Nate the excellent agreement of the rempasatienal resalts (to svitbia 2%) aver the temperatam mnge of mabel validity. T(K) t ( 5 (a)n ) cw’ 200 275 300 325 350 375 5.246 5< 10 1.059 5< 10 1.000 5< 10:0 6.798 x l0° 3.565 x l0 1.518 x lO 5.449 x lO 400 500 600 700 (cm’ 5 (b)a ) 1.051 x 10 1.006 X IO’ 6.887 5< loin 3.623 5< i5 1.542 5< 10 2.716 X lO 3.908 5< lois 2.865 5< 10 %Effective mass ratio (mar=nan/as0, nsprmp°/nt0) wnr 1.028 ÷ (6.1 ie4).nT )3.09a7).cT. 2; 5 sepr0.fllO ± (7.83e-4).°T (4°6e7)T 2 3 - - %Compatation of ci ni=A.r(IT./300).0(t.5)).c)marowpr).s(0.75)(.aexp(_(EG_Ees)./(2 °k”T)); ¶bl3inplay ontpat as screen jieapsh(T); fprintf(’\n \n T ni\a’); %Tlsrse are tea spares between T and ni. far ii= I:). fpriesf(’%-l 0.f%- 10.3e\n’,T(ii),ai(ii)); end 2.5.4 Charge Neutrality Relationship The relationships established to this point are devoid of an explicit dependence an the dapaat concentrations introdnred into a nemirondarsor. It is the charge neatralsty relation ship that provides she general tie between the earlier and dapaet canrenstasians. To establish the charge centrality relationship, lot av consider a nxmfrrssly doped semi condactar, a semireisdartor wheer the namber af dapant atoms/cm 3 ix the vame every where. Systematically examining little sectians of sIte semicondactor far from any surfaces, and assaming eqnilibriam renditions prevail, one watt inrariably find that each and every section is aharge-nentral, ia., contains canal charge. If this were not the cane, electric fields 57’ 55 ‘..e3 52 s-fl;EwEi.’ r-=; r/75 su)aicossnncvoe s’uuaaeuicsats vere J — —— ... 4, aanrrrrie irw,s=,aacrnr vnia. v, ,no,ron,tatiar — C I Cr aria ... —i )/ILT LOp— y’i is) I(’jt ,i(cy ‘,lLT eAeeceManELtrin (v-ri 1 v:-.tr 2= ‘N’t i Eqaatian (2.21) caps-essex a, ax a fnectian of hnasva qaastisias and can ha axed to campnta ri at a specified tempeeataee or as a fanetiaa of tempeeatara. Namerical vatnes foe she intrinsic carrier caneeaseatiao in Si and Ge at eaam temparatnee svere cited praviaoaly; the best aaaitstbla plots of a, as fanctiaax of temperatara in Si, Ga, and GaAs are displayed in Fig. 2.20 A secand very important a-based relationship faltawa directly frets Eqv. (2.19). trIal siptying the earrexpasdiag sides af Eqs. )2. I 9a) and (2.1 9b) tagether yields sea c, 5 e rrreec,,iia 5L-i,ia,oxaacvir (2.22) Definitina of degaueratoloosdelennrate naintrandartaw. Figure 2.15 Er ± It therefore followv that, if E + 3kT Attltangh appaariag trivial, the op peadset relationship (Eq. 2.22) often proves to be extremely nsefal in practical campalatians. If aae of the carrier casceatratians ix lasawa, the rasssaiaing carrier coacentratioa ix readily determined axing Eq. (2.22)—pravided of conrse that the semicotsdactaria in eqailibrians astd nasdeaenerate. E,, — 3k)’ (2.lfla) (C) Exercise 2.4 (2.1 fib) Sabslisassng the Eq. (2.13) definitions af Er and i’/ inta Eq. (2.21), inteadaciag narasatiaatian factaes, and replacing keawn caastaam by their nnmerscal valnrs. one abtaiax = ,(r,—irr)iar 5 = p The atathematical simplification Leading to Eqs. (2.16) a eqatvalcnt to approximating f(E), by simple exponential faocttons—an approsi tite oecapaeey factors,f(E) and 1 motion earlier shown to be valid provided Er wat somewhere tn the band gap no closer is confined, ax noted, to E, + 3kT ar E. than 3kT to either band edge. whenever simply 3hZ instead of cantinoalty repeating the Er restriction, the semteaadartar is band aaid Ia be nandegenerate. Wltenevee r lien in the band gap closer than 3hT to esther edge or actaally penetrates one of the bands, the seaaieoadactor is said to ha degeaerata. These very intpartant teems are also defined psetartatly ta Fig. 2. t9. it n and p = Althaagh in closed farm, the Eq. (2.16) reationships are nat in the simplest farm passthle. ma ear and, mace aften than oat. it is the vintptes alternative farm of these retatsonships that eacoasters ia device analyses. The alteroative-farns ratationshtps can be obtained by re and widgap, elate to calling that E,, she Fermi level far an intrinsic semiaaadnctar, lies hence Eqs. (2.16) mast aasaradly apply ta as intrinsic semicaadactar. If this be the ease, = thea speeialiaisg Eqs. (2.16) Ia aa intrinsic sasnieaadactar. ta., settingn = p = a, and Er. one abtains = Ncetfuar . . = 1.028 - (6.11 x to_a)T 0.610 + (7.83 x to -a))’ — — (3.09 5< I0-)I’ (4.46 X 10 -‘)T F: (a) Confirns that the a verses T carve for Si graphed in Fig. 2.20 ix generated employing the mlationshipa nat riled, praeidesd Er in the a, expression in replaced by E EU,, where E, = 0,0074 eV. (In she peevinasly riled article, Barber sug gested axing an canton roeeectian factor of E,, = 0.007 eV. The slightly larger valee employed in the Fig. 2.20 campalatian was specifically chosen to give 01 = 1015, 5 at 300 K.) cm — )2.t7a) ‘.5_i; eCoit’ Er and the effective masses exhibit a weak bat nan-negligible temperatare depan dance. The Er mesas T variation can he modeled to fear-place arcneacy by the fit relationship noted in Frablem 2.1(a). As dedaced from she analysis by Barber [SolidState Electronics, ie, 1039 (1967)). the temperataee dependence of the effective massea aver the range 200 K as Tm 700 K can be approximated by — 2.5.2 Alternative Expressions for () (2.510 X l0in)(v e) — fI’ I’,i,I c www.EasyEngineering.net 56 sesitcoNaucras FUNDAMENTaLs raueice snauLiNa (b) The accepted valae of v, in Si at 300 K has been revised recently to be in agree ment with time experimental a vernal Tdata arqaired by Sproat and Green Jaaenal of Applied Physics. 78, 846 Only 1990). The anthem concluded a, = 1.00 ± 0.03 X l0vaia in Si at 300K. Over the probed Iemprratare range of 275 K ± T 375 K, their esperimensal data raald be fitted by the relationship a = (9.15 x loa)() 9: (a) MATLAn program script. .Ea %ssi vs. T ratcalatian far Si (200K %lnitialiratian format short syE ngi %Castatassts and T-range k8.Gt7e-S; A2.510et9; Erx=0.0074; %Valae wax adjusted to match S&G ni(300K) valne T200:25:700; %Baad Gap vs. T EGO= 1.17; a4.730c-4; b’036; EGEGO-a. °(T. 2)./(T+b); 5 - %ni calcnlatiaa T= 275 :25 : 375 k8.fll7e-5; ci =(9. lSel 9).elTj300).02 aevp(0 5928 /)k°T)) nee rin g %Effective mass ratio (mar=nan/as0, nsprmp°/nt0) wnr 1.028 ÷ (6.1 ie4).nT )3.09a7).cT. 2; 5 sepr0.fllO ± (7.83e-4).°T (4°6e7)T 2 3 %Dinplay resalt on screen j=tengtb(T); ni\n’); %There are ten spaces between T and ci. fprintf(’\a\n T for 0=’ l:j, fprintf(’ %- I 0.f%-10.3e\n’,T(ii),ai(ii)); end Gatpus from the lava programs in reprodared below. Nate the excellent agreement of the rempasatienal resalts (to svitbia 2%) aver the temperatam mnge of mabel validity. 700K) axed in Pig. 2.20 - program script.. %Espenmealal fit of Sproal-Grern ai data (275E 375K) shtaT 5 e Compare the a, cawpated feam this experimental-fit relationship to the part (a) aatpat aver the temperature range of mataal validity. ww w (b) MAmAs .ne t T(K) t ( 5 (a)n ) cw’ 200 275 300 325 350 375 5.246 5< 10 1.059 5< 10 1.000 5< 10:0 6.798 x l0° 3.565 x l0 1.518 x lO 5.449 x lO 400 500 600 700 (cm’ 5 (b)a ) 1.051 x 10 1.006 X IO’ 6.887 5< loin 3.623 5< i5 1.542 5< 10 2.716 X lO 3.908 5< lois 2.865 5< 10 - - %Compatation of ci ni=A.r(IT./300).0(t.5)).c)marowpr).s(0.75)(.aexp(_(EG_Ees)./(2 °k”T)); ¶bl3inplay ontpat as screen jieapsh(T); fprintf(’\n \n T ni\a’); %Tlsrse are tea spares between T and ni. far ii= I:). fpriesf(’%-l 0.f%- 10.3e\n’,T(ii),ai(ii)); end www.EasyEngineering.net 2.5.4 Charge Neutrality Relationship The relationships established to this point are devoid of an explicit dependence an the dapaat concentrations introdnred into a nemirondarsor. It is the charge neatralsty relation ship that provides she general tie between the earlier and dapaet canrenstasians. To establish the charge centrality relationship, lot av consider a nxmfrrssly doped semi condactar, a semireisdartor wheer the namber af dapant atoms/cm 3 ix the vame every where. Systematically examining little sectians of sIte semicondactor far from any surfaces, and assaming eqnilibriam renditions prevail, one watt inrariably find that each and every section is aharge-nentral, ia., contains canal charge. If this were not the cane, electric fields 57’ 55 ‘..e3 52 s-fl;EwEi.’ r-=; r/75 su)aicossnncvoe s’uuaaeuicsats vere J — —— ... 4, v, aanrrrrie irw,s=,aacrnr vnia. ,no,ron,tatiar — C I Cr aria ... )/ILT —i LOp— y’i is) I(’jt ,i(cy ‘,lLT eAeeceManELtrin (v-ri 1 v:-.tr 2= ‘N’t i Eqaatian (2.21) caps-essex a, ax a fnectian of hnasva qaastisias and can ha axed to campnta ri at a specified tempeeataee or as a fanetiaa of tempeeatara. Namerical vatnes foe she intrinsic carrier caneeaseatiao in Si and Ge at eaam temparatnee svere cited praviaoaly; the best aaaitstbla plots of a, as fanctiaax of temperatara in Si, Ga, and GaAs are displayed in Fig. 2.20 A secand very important a-based relationship faltawa directly frets Eqv. (2.19). trIal siptying the earrexpasdiag sides af Eqs. )2. I 9a) and (2.1 9b) tagether yields sea c, 5 e rrreec,,iia 5L-i,ia,oxaacvir (2.22) Definitina of degaueratoloosdelennrate naintrandartaw. Figure 2.15 Er ± It therefore followv that, if E + 3kT Attltangh appaariag trivial, the op peadset relationship (Eq. 2.22) often proves to be extremely nsefal in practical campalatians. If aae of the carrier casceatratians ix lasawa, the rasssaiaing carrier coacentratioa ix readily determined axing Eq. (2.22)—pravided of conrse that the semicotsdactaria in eqailibrians astd nasdeaenerate. E,, — 3k)’ (2.lfla) (C) Exercise 2.4 (2.1 fib) Sabslisassng the Eq. (2.13) definitions af Er and i’/ inta Eq. (2.21), inteadaciag narasatiaatian factaes, and replacing keawn caastaam by their nnmerscal valnrs. one abtaiax = p ,(r,—irr)iar 5 = The atathematical simplification Leading to Eqs. (2.16) a eqatvalcnt to approximating f(E), by simple exponential faocttons—an approsi tite oecapaeey factors,f(E) and 1 motion earlier shown to be valid provided Er wat somewhere tn the band gap no closer is confined, ax noted, to E, + 3kT ar E. than 3kT to either band edge. whenever simply 3hZ instead of cantinoalty repeating the Er restriction, the semteaadartar is band aaid Ia be nandegenerate. Wltenevee r lien in the band gap closer than 3hT to esther edge or actaally penetrates one of the bands, the seaaieoadactor is said to ha degeaerata. These very intpartant teems are also defined psetartatly ta Fig. 2. t9. it n and p = Althaagh in closed farm, the Eq. (2.16) reationships are nat in the simplest farm passthle. ma ear and, mace aften than oat. it is the vintptes alternative farm of these retatsonships that eacoasters ia device analyses. The alteroative-farns ratationshtps can be obtained by re and widgap, elate to calling that E,, she Fermi level far an intrinsic semiaaadnctar, lies hence Eqs. (2.16) mast aasaradly apply ta as intrinsic semicaadactar. If this be the ease, = thea speeialiaisg Eqs. (2.16) Ia aa intrinsic sasnieaadactar. ta., settingn = p = a, and Er. one abtains = Ncetfuar . . = 1.028 - (6.11 x to_a)T 0.610 + (7.83 x to -a))’ — — (3.09 5< I0-)I’ (4.46 X 10 -‘)T F: (a) Confirns that the a verses T carve for Si graphed in Fig. 2.20 ix generated employing the mlationshipa nat riled, praeidesd Er in the a, expression in replaced by E EU,, where E, = 0,0074 eV. (In she peevinasly riled article, Barber sug gested axing an canton roeeectian factor of E,, = 0.007 eV. The slightly larger valee employed in the Fig. 2.20 campalatian was specifically chosen to give 01 = 1015, 5 at 300 K.) cm — )2.t7a) ‘.5_i; eCoit’ Er and the effective masses exhibit a weak bat nan-negligible temperatare depan dance. The Er mesas T variation can he modeled to fear-place arcneacy by the fit relationship noted in Frablem 2.1(a). As dedaced from she analysis by Barber [SolidState Electronics, ie, 1039 (1967)). the temperataee dependence of the effective massea aver the range 200 K as Tm 700 K can be approximated by — 2.5.2 Alternative Expressions for () (2.510 X l0in)(v e) — fI’ I’,i,I c www.EasyEngineering.net 56 sesitcoNaucras FUNDAMENTaLs raueice snauLiNa (b) The accepted valae of v, in Si at 300 K has been revised recently to be in agree ment with time experimental a vernal Tdata arqaired by Sproat and Green Jaaenal of Applied Physics. 78, 846 Only 1990). The anthem concluded a, = 1.00 ± 0.03 X l0vaia in Si at 300K. Over the probed Iemprratare range of 275 K ± T 375 K, their esperimensal data raald be fitted by the relationship a = (9.15 x loa)() 9: (a) MATLAn program script. - program script.. %Espenmealal fit of Sproal-Grern ai data (275E 375K) - %ni calcnlatiaa T= 275 :25 : 375 k8.fll7e-5; ci =(9. lSel 9).elTj300).02 aevp(0 5928 /)k°T)) shtaT 5 e Compare the a, cawpated feam this experimental-fit relationship to the part (a) aatpat aver the temperature range of mataal validity. %ssi vs. T ratcalatian far Si (200K (b) MAmAs 57’ 700K) axed in Pig. 2.20 %lnitialiratian format short %Castatassts and T-range k8.Gt7e-S; A2.510et9; Erx=0.0074; %Valae wax adjusted to match S&G ni(300K) valne T200:25:700; %Baad Gap vs. T EGO= 1.17; a4.730c-4; b’036; EGEGO-a. °(T. 2)./(T+b); 5 %Dinplay resalt on screen j=tengtb(T); ni\n’); %There are ten spaces between T and ci. fprintf(’\a\n T for 0=’ l:j, fprintf(’ %- I 0.f%-10.3e\n’,T(ii),ai(ii)); end ww w.E Gatpus from the lava programs in reprodared below. Nate the excellent agreement of the rempasatienal resalts (to svitbia 2%) aver the temperatam mnge of mabel validity. asy En T(K) t ( 5 (a)n ) cw’ 200 275 300 325 350 375 5.246 5< 10 1.059 5< 10 1.000 5< 10:0 6.798 x l0° 3.565 x l0 1.518 x lO 5.449 x lO 400 500 600 700 (cm’ 5 (b)a ) gin 2.716 X lO 3.908 5< lois 2.865 5< 10 %Effective mass ratio (mar=nan/as0, nsprmp°/nt0) wnr 1.028 ÷ (6.1 ie4).nT )3.09a7).cT. 2; 5 sepr0.fllO ± (7.83e-4).°T (4°6e7)T 2 3 1.051 x 10 1.006 X IO’ eer 6.887 5< loin 3.623 5< i5 1.542 5< 10 ing .ne - - %Compatation of ci ni=A.r(IT./300).0(t.5)).c)marowpr).s(0.75)(.aexp(_(EG_Ees)./(2 °k”T)); ¶bl3inplay ontpat as screen jieapsh(T); fprintf(’\n \n T ni\a’); %Tlsrse are tea spares between T and ni. far ii= I:). fpriesf(’%-l 0.f%- 10.3e\n’,T(ii),ai(ii)); end 2.5.4 Charge Neutrality Relationship The relationships established to this point are devoid of an explicit dependence an the dapaat concentrations introdnred into a nemirondarsor. It is the charge neatralsty relation ship that provides she general tie between the earlier and dapaet canrenstasians. To establish the charge centrality relationship, lot av consider a nxmfrrssly doped semi condactar, a semireisdartor wheer the namber af dapant atoms/cm 3 ix the vame every where. Systematically examining little sectians of sIte semicondactor far from any surfaces, and assaming eqnilibriam renditions prevail, one watt inrariably find that each and every section is aharge-nentral, ia., contains canal charge. If this were not the cane, electric fields www.EasyEngineering.net t 55 www.EasyEngineering.net 58 SEMICONDUCTOR FUNDAMENTALS CURRIER MOOnLING svould exist inside the semiconductor. The electric fields in turn would give rise to carrier motion and associated currents—a situation totatly inconsistent with the assumed equilib rium conditions. There are, however, charged entities inside all semiconductors. Electrons, hotes, ionized donors (donor atoms that have become positively charged by donating an electron to the conduction band) and negatively_charged innized acceptors can all esist simultaneously inside any given sensiconductor. For the uniformly doped materiat to be everywhere charge_neutral clearly requires charge —j—qp—q,s+qN —qN;=0 ww (2.23) Or w.E where, by definition, p — n + N N; = 0 2.5.5 Carrier Concentration Calculations We are finally irs a position to calculate the carrier concentrations in a uniformly doped scnnconductor under equilibriutis conditions. In the computations to be preseitted we spe cifically niake the assansptions of NONDEGENERACY (allowing us to use the up product relationship) and TOTAL IONIZATtON of the dopant atoms. Note that n. which appears in the up product expression, has been calculated and platted and must be considered a known quantity. Likewise, N 0 and N , which appear in the charge nentratily relationship, 0 are typically controlled and delcrmiued espcriitmntally and should also be considered kanwn quantities. The only other symbols used in the two eqnutions are u and p. Thus, under the riled assuusptions of nondegeneracy and total ionization of doirant atoms, sve have two equations and two uzknowns frous wInch n and/a can be deduced. Starting with the np product expression, one cart write (2.24) = number of ionized (positively charged) donors/cm , 3 N; = number of iottized (negatively charged) acceptors/cm . 5 — As previously discussed, there is sufficient thermal energy available in a semiconduc tor at room tempcratare to ionize almost all of the shallow-level donor and acceptor sites. Defining eri ng. ne total number of donors/cm , 3 = total number of acceptors/cm , 3 0 N = 0 N x + — 0 (2.27) rt?0 (2.29) 0 N = or na — 0 n(N — ) 0 N — Solving the quadratic equation forts then yields t and setting ° 0 N (2.26) tt Eliminating pin Eq. (2.25) using Eq. (2.2fi) gives N 0 N 2 n —i = p as y En gin e 59 (2.29a) 0 N = and one then obtains = = + Ne — assumes total ionization of dopant atoms 0 N 0 N — 0 N + 0 [(N — Na)S + (2.25) = Onty the plus roots have been retained in Eqs. (2.29) because physically the carrier concen trations must be greater than or equal to zero. Equation (2.25) is the standard forns of the charge neutrality relationship. www.EasyEngineering.net 60 5nMICONDUCTOR FUNDAMENTALS CARRIER MODELING Equations (2.29) are general-ease snlutions. In the vast majority of practical compu tations it is possible to simplify these equations prior to substituting in numerical values for N , N 0 , and ss Special cuses of specific interest are considered nenL 0 0 (t) Intrinsic Se,sicnnductor (N 0 = 0, N 0 = 0), With N 0 and N 0 = 0, Eqs. (2.29) simplify to and n 1 is of course the expected result for the p = n equilibrium cart’ier enncentrations in an intrinsic semiconductor. — 0 N 0 N n, or NA N 0 N 0 N n. N This is the special case of greatest practical interest. The unintentional doping levels in Si are such that the controlled addition of dopants routinely yields N 0 N N 0 or NA N . tVtoreover, the intrinsic carrier concentration in Si at room temperature is about 0 N , while the dominant doping concentration (N 3 /cuv 10 t0 ) is seldom less than 0 0 or N 10 3 /crn Thus the special case considered herein the usual case encountered in prac 0 . /2 and 5 tice. If Nn 0 N 0 N n, the square root in Eq. (2.29a) reduces to N N (2) Doped Semico,iductur where either N 0 — tn seminary, Eqs. (2.29) can always be used to compute the carrier concentrations if the semicondnctor is nondegenerate and the dopanl atoms are totally ionized. In the vast majortty of practical situations, however, it is possible to simplify these equations prior to performing numerical computations. Equations (2.29) mnst be used to compute the carrier conefintrations only in those rare instances when IN 0 n, The simplified relation 0 N ships of greatest practical utility are Eqs. (2.30) and (2.31). - — — Exercise 2.5 P: A Si sample is doped with 1050 boron atoms per cm . 3 (a) Whut are the carrier concentrations in the Si sample at 300 K? (b) What are the carrier concentrations at 470 K? — ri p s,/N NN N , 0 Nn 0 N (nondegenerale, total ionization) (2.30a) (2.30b) Similarly 0 N ii J 0 n/N 0 N Nu, N N 0 N n (nondegenerate, total ionization) (2.3 Ia) (2.31b) As a nutrierical example, suppose a Si sample maintained at room temperature is unI /cm donors. Using Eqs. (2.30), one rapidly concludes 5 lO’ 3 formly doped with N 0 tOo/ems and p /cm 5 10 . 3 (3) Doped Seniiroudnctor where n N N III. Systematically increasing the atnbi eat temperature causes a monotonic rise in the intrinsic carrier concentration (see Fig. 2.20), At sufficiently elevated temperatures, s will eventually equal and then ex ceed the net doping concentration. If n 1 N N 1, the square roots in Eqs. (2.29) 0 N reduce to n and In other words, all semiconductors become intrinsic at . 0 N sufficiently lugh remperulure.s where rs N [N — — (4) Courpenaaled Semiconductor. As is evident from Eqs. (2.29), donors and acceptors teed to negate each other. Indeed, it is possible to produce intrinsic-like material by 0 0 maybe comparable to N making N 0 0 = 0. In some materials, such as GaAs, N N in the as-grown crystal. When N 0 and Na are comparable and nonzero, the material is 0 must be 0 and N said lobe compensated. If the senticonduclor is compensated, both N retained in ull carrier concentration expressions. — S: (a) Boron in Si is an acceptor (see Table 2.2). Thus N,, = 10°/cm . At 300 K, 3 n = tOO x 10 In/ems and the given N 0 is clearly much greater than e. Moreover, since the N 0 doping was omitted from the problem statement, we infer N 0 4 N . 0 With N 0 N n and N 0 N Na, Eqs. (2.31) maybe used to calculate the carrier concen trattons: p = N 0 = 10 °/cm ; n 3 /cm 5 10 . 3 u?/NA (b) As deduced from Fig. 2.20, n 10 3 /cm at 470 K. Becuuse n is comparable 0 to N , Eqs. (2.29) must be used to culculate at least one of the carrier concentra 0 lions. (Once one of the carrier concentrations is known, the second is morn readily computed using the np product expression.) Performing the indicated calculations gives p = N /2 + [(P//2) + n]’ 0 0 = 1.62 X 3 /cm n = n.,/p = 6.18 X 0 10’ ; . 3 /cm 13 10 2.5.6 Determination of EF Kxosvledge concerniog the exact position of the Fermi level on the energy band diagram is often of interest. For example, when discnssing the intrinsic Fermi level, we indicated that N was located somewhere near the middle of the band gap. It woald be usefnl to knaw the precise positioning of E 5 in the band gap. Moreover, we have developed compalational formulas for n and p appropriate for noadegenerate semiconductors. Whether a doped semiconductor is nondegenerale or degenerate depends, of conrse, an the value or position ing of EF. Before running though the mechanics of finding the Fermi level in selected eases of interest, ills useful to make a geueral observation; namely, Eqs. (2.19) or (2.16) [or even mare generally, Eqs. (2.14)1 provide a one-to-one correspondence between the Fermi en ergy and the carrier concentrations. Thus, having computed any one of the three vari ables—u, p. or Es—one can always determine the remaining Iwo variables under equilib rium conditions. 61 www.EasyEngineering.net 58 SEMICONDUCTOR FUNDAMENTALS CURRIER MOOnLING svould exist inside the semiconductor. The electric fields in turn would give rise to carrier motion and associated currents—a situation totatly inconsistent with the assumed equilib rium conditions. There are, however, charged entities inside all semiconductors. Electrons, hotes, ionized donors (donor atoms that have become positively charged by donating an electron to the conduction band) and negatively_charged innized acceptors can all esist simultaneously inside any given sensiconductor. For the uniformly doped materiat to be everywhere charge_neutral clearly requires charge —j—qp—q,s+qN —qN;=0 (2.23) Or p — n + N N; = 0 (2.24) 59 2.5.5 Carrier Concentration Calculations We are finally irs a position to calculate the carrier concentrations in a uniformly doped scnnconductor under equilibriutis conditions. In the computations to be preseitted we spe cifically niake the assansptions of NONDEGENERACY (allowing us to use the up product relationship) and TOTAL IONIZATtON of the dopant atoms. Note that n. which appears in the up product expression, has been calculated and platted and must be considered a known quantity. Likewise, N 0 and N , which appear in the charge nentratily relationship, 0 are typically controlled and delcrmiued espcriitmntally and should also be considered kanwn quantities. The only other symbols used in the two eqnutions are u and p. Thus, under the riled assuusptions of nondegeneracy and total ionization of doirant atoms, sve have two equations and two uzknowns frous wInch n and/a can be deduced. Starting with the np product expression, one cart write ww where, by definition, w.E a 2 n —i = p (2.26) tt syE ngi Eliminating pin Eq. (2.25) using Eq. (2.2fi) gives N = number of ionized (positively charged) donors/cm , 3 N; = number of iottized (negatively charged) acceptors/cm . 5 — As previously discussed, there is sufficient thermal energy available in a semiconduc tor at room tempcratare to ionize almost all of the shallow-level donor and acceptor sites. Defining 0 N total number of donors/cm , 3 = or na — 0 N x + 0 n(N — — ) 0 N 0 N = 0 (2.27) nee r ing . rt?0 — Solving the quadratic equation forts then yields total number of acceptors/cm , 3 0 N and setting (2.29) net (2.29a) ° 0 N = 0 N = and one then obtains = = + Ne — assumes total ionization of dopant atoms 0 N 0 N — 0 N + 0 [(N — Na)S + (2.25) = Onty the plus roots have been retained in Eqs. (2.29) because physically the carrier concen trations must be greater than or equal to zero. Equation (2.25) is the standard forns of the charge neutrality relationship. www.EasyEngineering.net 60 5nMICONDUCTOR FUNDAMENTALS CARRIER MODELING Equations (2.29) are general-ease snlutions. In the vast majority of practical compu tations it is possible to simplify these equations prior to substituting in numerical values for N , N 0 , and ss Special cuses of specific interest are considered nenL 0 0 (t) Intrinsic Se,sicnnductor (N 0 = 0, N 0 = 0), With N 0 and N 0 = 0, Eqs. (2.29) simplify to and n 1 is of course the expected result for the p = n equilibrium cart’ier enncentrations in an intrinsic semiconductor. — 0 N 0 N n, or NA N 0 N 0 N n. N This is the special case of greatest practical interest. The unintentional doping levels in Si are such that the controlled addition of dopants routinely yields N 0 N N 0 or NA N . tVtoreover, the intrinsic carrier concentration in Si at room temperature is about 0 N , while the dominant doping concentration (N 3 /cuv 10 t0 ) is seldom less than 0 0 or N 10 3 /crn Thus the special case considered herein the usual case encountered in prac 0 . /2 and 5 tice. If Nn 0 N 0 N n, the square root in Eq. (2.29a) reduces to N N (2) Doped Semico,iductur where either N 0 — tn seminary, Eqs. (2.29) can always be used to compute the carrier concentrations if the semicondnctor is nondegenerate and the dopanl atoms are totally ionized. In the vast majortty of practical situations, however, it is possible to simplify these equations prior to performing numerical computations. Equations (2.29) mnst be used to compute the carrier conefintrations only in those rare instances when IN 0 n, The simplified relation 0 N ships of greatest practical utility are Eqs. (2.30) and (2.31). - — — Exercise 2.5 P: A Si sample is doped with 1050 boron atoms per cm . 3 (a) Whut are the carrier concentrations in the Si sample at 300 K? (b) What are the carrier concentrations at 470 K? — ri p s,/N NN N , 0 Nn 0 N (nondegenerale, total ionization) (2.30a) (2.30b) Similarly 0 N ii J 0 n/N 0 N Nu, N N 0 N n (nondegenerate, total ionization) (2.3 Ia) (2.31b) As a nutrierical example, suppose a Si sample maintained at room temperature is unI /cm donors. Using Eqs. (2.30), one rapidly concludes 5 lO’ 3 formly doped with N 0 tOo/ems and p /cm 5 10 . 3 (3) Doped Seniiroudnctor where n N N III. Systematically increasing the atnbi eat temperature causes a monotonic rise in the intrinsic carrier concentration (see Fig. 2.20), At sufficiently elevated temperatures, s will eventually equal and then ex ceed the net doping concentration. If n 1 N N 1, the square roots in Eqs. (2.29) 0 N reduce to n and In other words, all semiconductors become intrinsic at . 0 N sufficiently lugh remperulure.s where rs N [N — — (4) Courpenaaled Semiconductor. As is evident from Eqs. (2.29), donors and acceptors teed to negate each other. Indeed, it is possible to produce intrinsic-like material by 0 0 maybe comparable to N making N 0 0 = 0. In some materials, such as GaAs, N N in the as-grown crystal. When N 0 and Na are comparable and nonzero, the material is 0 must be 0 and N said lobe compensated. If the senticonduclor is compensated, both N retained in ull carrier concentration expressions. — S: (a) Boron in Si is an acceptor (see Table 2.2). Thus N,, = 10°/cm . At 300 K, 3 n = tOO x 10 In/ems and the given N 0 is clearly much greater than e. Moreover, since the N 0 doping was omitted from the problem statement, we infer N 0 4 N . 0 With N 0 N n and N 0 N Na, Eqs. (2.31) maybe used to calculate the carrier concen trattons: p = N 0 = 10 °/cm ; n 3 /cm 5 10 . 3 u?/NA (b) As deduced from Fig. 2.20, n 10 3 /cm at 470 K. Becuuse n is comparable 0 to N , Eqs. (2.29) must be used to culculate at least one of the carrier concentra 0 lions. (Once one of the carrier concentrations is known, the second is morn readily computed using the np product expression.) Performing the indicated calculations gives p = N /2 + [(P//2) + n]’ 0 0 = 1.62 X 3 /cm n = n.,/p = 6.18 X 0 10’ ; . 3 /cm 13 10 2.5.6 Determination of EF Kxosvledge concerniog the exact position of the Fermi level on the energy band diagram is often of interest. For example, when discnssing the intrinsic Fermi level, we indicated that N was located somewhere near the middle of the band gap. It woald be usefnl to knaw the precise positioning of E 5 in the band gap. Moreover, we have developed compalational formulas for n and p appropriate for noadegenerate semiconductors. Whether a doped semiconductor is nondegenerale or degenerate depends, of conrse, an the value or position ing of EF. Before running though the mechanics of finding the Fermi level in selected eases of interest, ills useful to make a geueral observation; namely, Eqs. (2.19) or (2.16) [or even mare generally, Eqs. (2.14)1 provide a one-to-one correspondence between the Fermi en ergy and the carrier concentrations. Thus, having computed any one of the three vari ables—u, p. or Es—one can always determine the remaining Iwo variables under equilib rium conditions. 61 58 SEMICONDUCTOR FUNDAMENTALS CURRIER MOOnLING svould exist inside the semiconductor. The electric fields in turn would give rise to carrier motion and associated currents—a situation totatly inconsistent with the assumed equilib rium conditions. There are, however, charged entities inside all semiconductors. Electrons, hotes, ionized donors (donor atoms that have become positively charged by donating an electron to the conduction band) and negatively_charged innized acceptors can all esist simultaneously inside any given sensiconductor. For the uniformly doped materiat to be everywhere charge_neutral clearly requires charge —j—qp—q,s+qN —qN;=0 (2.23) Or p — n + N N; = 0 59 2.5.5 Carrier Concentration Calculations We are finally irs a position to calculate the carrier concentrations in a uniformly doped scnnconductor under equilibriutis conditions. In the computations to be preseitted we spe cifically niake the assansptions of NONDEGENERACY (allowing us to use the up product relationship) and TOTAL IONIZATtON of the dopant atoms. Note that n. which appears in the up product expression, has been calculated and platted and must be considered a known quantity. Likewise, N 0 and N , which appear in the charge nentratily relationship, 0 are typically controlled and delcrmiued espcriitmntally and should also be considered kanwn quantities. The only other symbols used in the two eqnutions are u and p. Thus, under the riled assuusptions of nondegeneracy and total ionization of doirant atoms, sve have two equations and two uzknowns frous wInch n and/a can be deduced. Starting with the np product expression, one cart write (2.24) 2 n —i = p (2.26) tt where, by definition, Eliminating pin Eq. (2.25) using Eq. (2.2fi) gives N = number of ionized (positively charged) donors/cm , 3 N; = number of iottized (negatively charged) acceptors/cm . 5 — As previously discussed, there is sufficient thermal energy available in a semiconduc tor at room tempcratare to ionize almost all of the shallow-level donor and acceptor sites. Defining 0 N total number of donors/cm , 3 = 0 N x + — 0 (2.27) rt?0 (2.29) 0 N = or na — 0 n(N — ) 0 N — Solving the quadratic equation forts then yields total number of acceptors/cm , 3 0 N and setting (2.29a) ° 0 N = 0 N = and one then obtains = = + Ne — assumes total ionization of dopant atoms 0 N 0 N — 0 N + 0 [(N — Na)S + (2.25) = Onty the plus roots have been retained in Eqs. (2.29) because physically the carrier concen trations must be greater than or equal to zero. Equation (2.25) is the standard forns of the charge neutrality relationship. www.EasyEngineering.net 60 5nMICONDUCTOR FUNDAMENTALS CARRIER MODELING Equations (2.29) are general-ease snlutions. In the vast majority of practical compu tations it is possible to simplify these equations prior to substituting in numerical values for N , N 0 , and ss Special cuses of specific interest are considered nenL 0 0 (t) Intrinsic Se,sicnnductor (N 0 = 0, N 0 = 0), With N 0 and N 0 = 0, Eqs. (2.29) simplify to and n 1 is of course the expected result for the p = n equilibrium cart’ier enncentrations in an intrinsic semiconductor. — 0 N 0 N n, or NA N 0 N 0 N n. N This is the special case of greatest practical interest. The unintentional doping levels in Si are such that the controlled addition of dopants routinely yields N 0 N N 0 or NA N . tVtoreover, the intrinsic carrier concentration in Si at room temperature is about 0 N , while the dominant doping concentration (N 3 /cuv 10 t0 ) is seldom less than 0 0 or N 10 3 /crn Thus the special case considered herein the usual case encountered in prac 0 . /2 and 5 tice. If Nn 0 N 0 N n, the square root in Eq. (2.29a) reduces to N N (2) Doped Semico,iductur where either N 0 — ww w tn seminary, Eqs. (2.29) can always be used to compute the carrier concentrations if the semicondnctor is nondegenerate and the dopanl atoms are totally ionized. In the vast majortty of practical situations, however, it is possible to simplify these equations prior to performing numerical computations. Equations (2.29) mnst be used to compute the carrier conefintrations only in those rare instances when IN 0 n, The simplified relation 0 N ships of greatest practical utility are Eqs. (2.30) and (2.31). - — — Exercise 2.5 P: A Si sample is doped with 1050 boron atoms per cm . 3 (a) Whut are the carrier concentrations in the Si sample at 300 K? (b) What are the carrier concentrations at 470 K? — .Ea ri s p yE s,/N Similarly 0 N ii J 0 n/N NN N , 0 (2.30a) Nn 0 N (2.30b) (nondegenerale, total ionization) ngi nee rin g 0 N Nu, N N 0 N n (nondegenerate, total ionization) (2.3 Ia) (2.31b) .ne t As a nutrierical example, suppose a Si sample maintained at room temperature is unI /cm donors. Using Eqs. (2.30), one rapidly concludes 5 lO’ 3 formly doped with N 0 tOo/ems and p /cm 5 10 . 3 (3) Doped Seniiroudnctor where n N N III. Systematically increasing the atnbi eat temperature causes a monotonic rise in the intrinsic carrier concentration (see Fig. 2.20), At sufficiently elevated temperatures, s will eventually equal and then ex ceed the net doping concentration. If n 1 N N 1, the square roots in Eqs. (2.29) 0 N reduce to n and In other words, all semiconductors become intrinsic at . 0 N sufficiently lugh remperulure.s where rs N [N — — (4) Courpenaaled Semiconductor. As is evident from Eqs. (2.29), donors and acceptors teed to negate each other. Indeed, it is possible to produce intrinsic-like material by 0 0 maybe comparable to N making N 0 0 = 0. In some materials, such as GaAs, N N in the as-grown crystal. When N 0 and Na are comparable and nonzero, the material is 0 must be 0 and N said lobe compensated. If the senticonduclor is compensated, both N retained in ull carrier concentration expressions. — www.EasyEngineering.net S: (a) Boron in Si is an acceptor (see Table 2.2). Thus N,, = 10°/cm . At 300 K, 3 n = tOO x 10 In/ems and the given N 0 is clearly much greater than e. Moreover, since the N 0 doping was omitted from the problem statement, we infer N 0 4 N . 0 With N 0 N n and N 0 N Na, Eqs. (2.31) maybe used to calculate the carrier concen trattons: p = N 0 = 10 °/cm ; n 3 /cm 5 10 . 3 u?/NA (b) As deduced from Fig. 2.20, n 10 3 /cm at 470 K. Becuuse n is comparable 0 to N , Eqs. (2.29) must be used to culculate at least one of the carrier concentra 0 lions. (Once one of the carrier concentrations is known, the second is morn readily computed using the np product expression.) Performing the indicated calculations gives p = N /2 + [(P//2) + n]’ 0 0 = 1.62 X 3 /cm n = n.,/p = 6.18 X 0 10’ ; . 3 /cm 13 10 2.5.6 Determination of EF Kxosvledge concerniog the exact position of the Fermi level on the energy band diagram is often of interest. For example, when discnssing the intrinsic Fermi level, we indicated that N was located somewhere near the middle of the band gap. It woald be usefnl to knaw the precise positioning of E 5 in the band gap. Moreover, we have developed compalational formulas for n and p appropriate for noadegenerate semiconductors. Whether a doped semiconductor is nondegenerale or degenerate depends, of conrse, an the value or position ing of EF. Before running though the mechanics of finding the Fermi level in selected eases of interest, ills useful to make a geueral observation; namely, Eqs. (2.19) or (2.16) [or even mare generally, Eqs. (2.14)1 provide a one-to-one correspondence between the Fermi en ergy and the carrier concentrations. Thus, having computed any one of the three vari ables—u, p. or Es—one can always determine the remaining Iwo variables under equilib rium conditions. 61 58 SEMICONDUCTOR FUNDAMENTALS 59 CURRIER MOOnLING svould exist inside the semiconductor. The electric fields in turn would give rise to carrier motion and associated currents—a situation totatly inconsistent with the assumed equilib rium conditions. There are, however, charged entities inside all semiconductors. Electrons, hotes, ionized donors (donor atoms that have become positively charged by donating an electron to the conduction band) and negatively_charged innized acceptors can all esist simultaneously inside any given sensiconductor. For the uniformly doped materiat to be everywhere charge_neutral clearly requires charge —j—qp—q,s+qN —qN;=0 (2.23) Or p — n + N N; = 0 2.5.5 Carrier Concentration Calculations We are finally irs a position to calculate the carrier concentrations in a uniformly doped scnnconductor under equilibriutis conditions. In the computations to be preseitted we spe cifically niake the assansptions of NONDEGENERACY (allowing us to use the up product relationship) and TOTAL IONIZATtON of the dopant atoms. Note that n. which appears in the up product expression, has been calculated and platted and must be considered a known quantity. Likewise, N 0 and N , which appear in the charge nentratily relationship, 0 are typically controlled and delcrmiued espcriitmntally and should also be considered kanwn quantities. The only other symbols used in the two eqnutions are u and p. Thus, under the riled assuusptions of nondegeneracy and total ionization of doirant atoms, sve have two equations and two uzknowns frous wInch n and/a can be deduced. Starting with the np product expression, one cart write (2.24) 2 n —i = p (2.26) tt where, by definition, Eliminating pin Eq. (2.25) using Eq. (2.2fi) gives N = number of ionized (positively charged) donors/cm , 3 N; = number of iottized (negatively charged) acceptors/cm . 5 — As previously discussed, there is sufficient thermal energy available in a semiconduc tor at room tempcratare to ionize almost all of the shallow-level donor and acceptor sites. Defining 0 N total number of donors/cm , 3 = 0 N x + — 0 (2.27) rt?0 (2.29) 0 N = or na 0 n(N — — ) 0 N — Solving the quadratic equation forts then yields total number of acceptors/cm , 3 0 N and setting (2.29a) ° 0 N = 0 N = and one then obtains = = + Ne — assumes total ionization of dopant atoms 0 N 0 N — 0 N + 0 [(N — Na)S + (2.25) = Onty the plus roots have been retained in Eqs. (2.29) because physically the carrier concen trations must be greater than or equal to zero. Equation (2.25) is the standard forns of the charge neutrality relationship. www.EasyEngineering.net 60 5nMICONDUCTOR FUNDAMENTALS Equations (2.29) are general-ease snlutions. In the vast majority of practical compu tations it is possible to simplify these equations prior to substituting in numerical values for N , N 0 , and ss Special cuses of specific interest are considered nenL 0 0 (t) Intrinsic Se,sicnnductor (N 0 = 0, N 0 = 0), With N 0 and N 0 = 0, Eqs. (2.29) simplify to and n 1 is of course the expected result for the p = n equilibrium cart’ier enncentrations in an intrinsic semiconductor. — 0 N 0 N n, or NA N 0 N 0 N n. N This is the special case of greatest practical interest. The unintentional doping levels in Si are such that the controlled addition of dopants routinely yields N 0 N N 0 or NA N . tVtoreover, the intrinsic carrier concentration in Si at room temperature is about 0 N , while the dominant doping concentration (N 3 /cuv 10 t0 ) is seldom less than 0 0 or N 10 3 /crn Thus the special case considered herein the usual case encountered in prac 0 . /2 and 5 tice. If Nn 0 N 0 N n, the square root in Eq. (2.29a) reduces to N N (2) Doped Semico,iductur where either N 0 — — ri p s,/N NN N , 0 Nn 0 N (nondegenerale, total ionization) (2.30a) (2.30b) Similarly 0 N ii J 0 n/N 0 N Nu, N N 0 N n (nondegenerate, total ionization) (2.3 Ia) (2.31b) As a nutrierical example, suppose a Si sample maintained at room temperature is unI /cm donors. Using Eqs. (2.30), one rapidly concludes 5 lO’ 3 formly doped with N 0 tOo/ems and p /cm 5 10 . 3 (3) Doped Seniiroudnctor where n N N III. Systematically increasing the atnbi eat temperature causes a monotonic rise in the intrinsic carrier concentration (see Fig. 2.20), At sufficiently elevated temperatures, s will eventually equal and then ex ceed the net doping concentration. If n 1 N N 1, the square roots in Eqs. (2.29) 0 N reduce to n and In other words, all semiconductors become intrinsic at . 0 N sufficiently lugh remperulure.s where rs N [N — — (4) Courpenaaled Semiconductor. As is evident from Eqs. (2.29), donors and acceptors teed to negate each other. Indeed, it is possible to produce intrinsic-like material by 0 0 maybe comparable to N making N 0 0 = 0. In some materials, such as GaAs, N N in the as-grown crystal. When N 0 and Na are comparable and nonzero, the material is 0 must be 0 and N said lobe compensated. If the senticonduclor is compensated, both N retained in ull carrier concentration expressions. — 61 CARRIER MODELING tn seminary, Eqs. (2.29) can always be used to compute the carrier concentrations if the semicondnctor is nondegenerate and the dopanl atoms are totally ionized. In the vast majortty of practical situations, however, it is possible to simplify these equations prior to performing numerical computations. Equations (2.29) mnst be used to compute the carrier conefintrations only in those rare instances when IN 0 n, The simplified relation 0 N ships of greatest practical utility are Eqs. (2.30) and (2.31). - — — Exercise 2.5 P: A Si sample is doped with 1050 boron atoms per cm . 3 (a) Whut are the carrier concentrations in the Si sample at 300 K? (b) What are the carrier concentrations at 470 K? ww w.E S: (a) Boron in Si is an acceptor (see Table 2.2). Thus N,, = 10°/cm . At 300 K, 3 n = tOO x 10 In/ems and the given N 0 is clearly much greater than e. Moreover, since the N 0 doping was omitted from the problem statement, we infer N 0 4 N . 0 With N 0 N n and N 0 N Na, Eqs. (2.31) maybe used to calculate the carrier concen trattons: p = N 0 = 10 °/cm ; n 3 /cm 5 10 . 3 u?/NA asy En gin (b) As deduced from Fig. 2.20, n 10 3 /cm at 470 K. Becuuse n is comparable 0 to N , Eqs. (2.29) must be used to culculate at least one of the carrier concentra 0 lions. (Once one of the carrier concentrations is known, the second is morn readily computed using the np product expression.) Performing the indicated calculations gives p = N /2 + [(P//2) + n]’ 0 0 = 1.62 X 3 /cm n = n.,/p = 6.18 X 0 10’ ; . 3 /cm 13 10 2.5.6 Determination of EF eer ing .ne Kxosvledge concerniog the exact position of the Fermi level on the energy band diagram is often of interest. For example, when discnssing the intrinsic Fermi level, we indicated that N was located somewhere near the middle of the band gap. It woald be usefnl to knaw the precise positioning of E 5 in the band gap. Moreover, we have developed compalational formulas for n and p appropriate for noadegenerate semiconductors. Whether a doped semiconductor is nondegenerale or degenerate depends, of conrse, an the value or position ing of EF. Before running though the mechanics of finding the Fermi level in selected eases of interest, ills useful to make a geueral observation; namely, Eqs. (2.19) or (2.16) [or even mare generally, Eqs. (2.14)1 provide a one-to-one correspondence between the Fermi en ergy and the carrier concentrations. Thus, having computed any one of the three vari ables—u, p. or Es—one can always determine the remaining Iwo variables under equilib rium conditions. www.EasyEngineering.net t www.EasyEngineering.net r cansiue GEM5eONDGcTOIS FuNouMENvuLu (1) E.cucs pusistisnisig offf. In on intrissoic moseriol u tot-doped aesoicostdoclors maintained at or near room temperature. Sobstitatiug into Eq. (2.37), we therefore conclude Subsataliug for sand p iu Eq. (2.32) using Eqs. (2.16), and setting c Ncetuom = , yields Nveicioc = H,, H, (2.33) Soloing for H,, one obtains ww EnS H lu(1) + = w.E (2.34) as y En gin e Cunscqiseittly, (2.3y) \ot (2.36) eri — ff = — = kT ln(No/ss;) ... N 3> N,, 0 3> n N (2.38a) hTln(Nojj ...N,N’Na, N,N-u (2.38b) Prom Eqs. (2.38) isis ubsious that the Fersoi level moves systematically upward in energy from H with increasing donor doping and systematically downward in energy from H with ittcreasiug acceptor doping. The exact Ferusi IconS positioning in Si at room tem perature, nicely rci,sfocciug the foregoing stalemeus, is displayed in Fig. 2.21. Also note that for a given semicoudartoc material and ambient temperature, there esist maximum noude generate douocand aacepsoreonceuseasious, doping concentrations above which the materiol becomes degesierate. In Si at room temperature the maximum ssoxdegenerale doping con centrations areWu 1.6 x 10°/em 5 mid N,,, 9.1 5< lOi?/rioS. The large Si doping values required for degeneracy, we should inleiject, have led to the common usage of “highly doped” (or ss’-materiul/p°-mater(al) and “degenerate” us interchangeable terms. Finally, the qaestion may arise: What procedure should be followed in computing H,, when one is aol sure whether a material is nondegenerate or degenerate? Unless a material is ksomn to be degenerate, always assume nondegenemey and compute H,, employing the appropriate tsuudrgenecate relationship. If H,, derived from the nondegescrute furmulo lies in the degenerate zone, one must then, of course, cecompate H,, using the more complex fol’mulism valid for degenerate materials. 5(2 0 N 63 (2.32) p = MosinLtNa ng. ne = ut or if T = According to Eq. (2.36), F, lies precisely as midgop only if 0 K. Poe tlte more practical cone of silicon at room temperatore, Toble 2.1 gives —0.0073 eV, ood F, thrrefore lirs 0.0073 eV sn/sn) = 11.69, (3/4)kT ln(so)us°) below midgop. Althssagh potentinily signifleout in certoio problems, this smoll devto tion from midgop is typieolly nrglccted in drowiog energy bood diogroms, etc. t (2) Doped semiconductors (nosdegenecuse, dopossss tosolly ionized). The genecol positioo log of the Fermi level in donoc- nnd occeptor-duped semiconductors nssumed In be nnodegenernte, in equilibrium, nod maintnined at tnmpernsnres svhnen the doponts are fnlly ionized, is readily deduced from Eqs. (2.19). Spneifieally, solving Eqs. (2.19) for E, one nlstuins N &Anoeptonanr 3hz — h•, = — fiT ln(n/n,) = — hT ln(pln,) (2.37) 5 in’ 50 l5’ l0’ ts’ 0 is Ott ° t in 0 tnm’l Na ueN Depending on the simpliflmations iuheeent in n paetienlnr problem, the appropciatweac rice eoneensrnsiun solntinu [Eqs. (2.29). (2.30), (2.31), etc.] is then substituted into Poe exumple, per Eqs. (2.30n) end Eq. (2.37) In detecmine thn positioning of N, in typicnl nccnp (2.3 Sn), ss = N 0 in typical donor-doped semicondnetors nnd p Fncud tnvnt pnsitiuning in Si n1309K use fnnetinu nf the duping aunoenteusius. The solid H,, lines wum established nsing Eq. )2.38a) fur dunue-duped materiut and Eq. (2.3gb) fur accep tue-duped material )hT = 0.0259 cv, and u = tO ‘°/nm ). 5 Figure 2.21 —. www.EasyEngineering.net r 64 - CAROIEn MODELING nnMsenNnnceoe enNnaMnNsucn 2.5.7 Carrier Concentration Temperature Dependence Exerciue 2.6 F: For each of she conditions specified in Eoereise 2.5, determine thr position of H,, compute H,, H, and draw a carefully dimensioned energy baud diagram for the Si sample. Note that H (Si) = 1.08eV and m/m) = 0.71 at 470 K. 0 — 5: (a) In part (a) of Exercise 2.5, the N,,, = 10 ia/ems Si sosssple is moinled at 300 K. Usiitg Eq. (2.36), we cunclude H, is located 0.0073 eV beluss midgap. (The position ing of H, in Si al 300 K is also noted in the text following Eq. 2.36). Next applying Eq. (2.28b), we find H, — H,, = = = bT lu(N,/u,) /l0N) 4 0.0259 ln(.lOi 0.239 eV The energy baud diagram constmcted from she deduced positioning of H, and H,, is shown in Fig. E2.6(a). (b) In part (b) of Exercise 2.5 she Si sample is heated 10470 K. With m/ssi) = 0.71 0.0104eV and H, is dedncrd and kT = 0.0405eV at 470 K, (3/4)kTln(ss/so)) = so be located 0.0 104 eV below midgup. Because N,,, is comparable to iii at 470 K, Eq. (2.37) must be used to compute she positioning of H,,. Specifically, with s , 5 3 and p = 1.62 5< lO’°/cm 10°/cm — H, — H,, = = = fiT ln(p/ss,) 0.0405 1oCt.62 5< 0.0195 eV 54) 0 lOiO/) Here H,, is only slightly removed from H, as pictured in Fig. E2.6(b). c, a a,, Er lbl 1°) Figure e2,6 A number of isolated fuels about the carrier concentration setuperasuen dependence hnvu already been presented at various points in this chapter. The diucnsuiou in Section 2.3 con cerned with dupaut actiun, for uxample, described the increased ionization uf dupont sites und lhe associated increase iu the majority carrier cuucuulratiun when the temperature of a semiconductor is raisud from near T = 0 K toward room temperature. Mute recent sub sections have isclnded a pior uf the intrinsic currier couceutratiun versus temperature (Fig. 2.20) and a calenlatiun indicating chat all semicouducturs become intrinsic (n—s u, p —a ss,) at sufficiently high lrmpecasnres. In this subsection, which concludes the carrier concentration discussion, lumperaturc-eeloted facts ace combined end embellished to pen side a broader, more complete description of how the carrier cosceoleotions vary with temperature. Figure 2.22(a), a typical tuojorily-carcier cuuceutrasiou-oersns-lempcrasure plus con structed assuming a phusphueso-doped N 0 = lOiS/emS Si sample, nicely illusseutes the general features of she cuuceusratiuu-versas-tcmpecasuce dependence. Eoamiuixg Fig. 2.22(a), we find that isis fined at approximately N 0 ever a bread semperasore rouge esseud ing roughly from 150 K to 450 K for the given Si sample. This n 0 or “estriusic N temperature region” cunstitutes the normal operating rouge fur must solid-state devices. Below 100 K or so, in the “freeze-oat temperature region,” n drops significantly below Nu and approaches zero as T —a 0 K. Sn the “intrinsic trmperusore region” at the opposite end of the lemprrature scale, crises above N , usymptotically approaching n, with increas 0 ing T To qualitatively explain she juss-doscribed coxceusrasiou-versus-tempecasure depen dence, it is important to recall that the equilibrium number of carriers within a material is affected by Iwo separate mechanisms. Electrons donated to the conduction bond from do nor atoms and valence baud electrons excited across the baud gap into the conduction baud (broken Si—Si bonds) both contribute to the majority-carrier electron concentration in a donor-doped material. As sesupecolures T—s 0 K the thermal energy available in the system is insufficient to release the weakly bound fifth electron od donor sites and totally insuffi cient 10 excite electrons across she band gap. Hence u = Oat T = 0 K, as visualized on the lefl-haisd side of Fig. 2.22(b). Slightly increasing the mulerial temperature above y 0 K “defrosts” or frees some of the electrons wenkly boand to donor sites. Baud-to-baud cxci laaots, however, remains estresoely unlikely, and therefore the number of observed nIce trotts In the freeze-out tempecutoce region equals the number of insized donors—si = N. Continuing lu increase the system temperature eventually frees almost all of the weakly bound electrons on donor sites, u approaches N , and one enters Ihe extrinsic temperature 0 region. In progressing through the extrinsic temperature region, more and more electrons are uocitrd across Ihu band gap, but the number of elzclcous sapplied in this fashion stays comfortably below N . Ullimotely, of coarse, electrons excised across the bond gup equal, 0 then exceed, and, as pictured on the right-hand side of Fig. 2.22(b), finally swamp she fixed number of electrons derived from the donors. As a practical note, it shoald be pointed out that thu wider the band gap, the greaszc the energy required lo excite electrons from the valence baud into the conductios band, oud 65 www.EasyEngineering.net r cansiue GEM5eONDGcTOIS FuNouMENvuLu (1) E.cucs pusistisnisig offf. In on intrissoic moseriol u tot-doped aesoicostdoclors maintained at or near room temperature. Sobstitatiug into Eq. (2.37), we therefore conclude Subsataliug for sand p iu Eq. (2.32) using Eqs. (2.16), and setting c Ncetuom = , yields Nveicioc = H,, H, (2.33) Soloing for H,, one obtains H lu(1) + = ww (2.34) 5(2 (2.3y) \ot — ff = — = kT ln(No/ss;) ... N 3> N,, 0 3> n N (2.38a) hTln(Nojj ...N,N’Na, N,N-u (2.38b) Prom Eqs. (2.38) isis ubsious that the Fersoi level moves systematically upward in energy from H with increasing donor doping and systematically downward in energy from H with ittcreasiug acceptor doping. The exact Ferusi IconS positioning in Si at room tem perature, nicely rci,sfocciug the foregoing stalemeus, is displayed in Fig. 2.21. Also note that for a given semicoudartoc material and ambient temperature, there esist maximum noude generate douocand aacepsoreonceuseasious, doping concentrations above which the materiol becomes degesierate. In Si at room temperature the maximum ssoxdegenerale doping con centrations areWu 1.6 x 10°/em 5 mid N,,, 9.1 5< lOi?/rioS. The large Si doping values required for degeneracy, we should inleiject, have led to the common usage of “highly doped” (or ss’-materiul/p°-mater(al) and “degenerate” us interchangeable terms. Finally, the qaestion may arise: What procedure should be followed in computing H,, when one is aol sure whether a material is nondegenerate or degenerate? Unless a material is ksomn to be degenerate, always assume nondegenemey and compute H,, employing the appropriate tsuudrgenecate relationship. If H,, derived from the nondegescrute furmulo lies in the degenerate zone, one must then, of course, cecompate H,, using the more complex fol’mulism valid for degenerate materials. EnS 0 N 63 (2.32) p = MosinLtNa Cunscqiseittly, w.E a syE ngi nee r (2.36) ing . = ut or if T = According to Eq. (2.36), F, lies precisely as midgop only if 0 K. Poe tlte more practical cone of silicon at room temperatore, Toble 2.1 gives —0.0073 eV, ood F, thrrefore lirs 0.0073 eV sn/sn) = 11.69, (3/4)kT ln(so)us°) below midgop. Althssagh potentinily signifleout in certoio problems, this smoll devto tion from midgop is typieolly nrglccted in drowiog energy bood diogroms, etc. (2) Doped semiconductors (nosdegenecuse, dopossss tosolly ionized). The genecol positioo log of the Fermi level in donoc- nnd occeptor-duped semiconductors nssumed In be nnodegenernte, in equilibrium, nod maintnined at tnmpernsnres svhnen the doponts are fnlly ionized, is readily deduced from Eqs. (2.19). Spneifieally, solving Eqs. (2.19) for E, one nlstuins net N &Anoeptonanr 3hz — h•, = — fiT ln(n/n,) = — hT ln(pln,) (2.37) 5 in’ 50 l5’ l0’ ts’ 0 is Ott ° t in 0 tnm’l Na ueN Depending on the simpliflmations iuheeent in n paetienlnr problem, the appropciatweac rice eoneensrnsiun solntinu [Eqs. (2.29). (2.30), (2.31), etc.] is then substituted into Poe exumple, per Eqs. (2.30n) end Eq. (2.37) In detecmine thn positioning of N, in typicnl nccnp (2.3 Sn), ss = N 0 in typical donor-doped semicondnetors nnd p Fncud tnvnt pnsitiuning in Si n1309K use fnnetinu nf the duping aunoenteusius. The solid H,, lines wum established nsing Eq. )2.38a) fur dunue-duped materiut and Eq. (2.3gb) fur accep tue-duped material )hT = 0.0259 cv, and u = tO ‘°/nm ). 5 Figure 2.21 —. www.EasyEngineering.net r 64 - CAROIEn MODELING nnMsenNnnceoe enNnaMnNsucn 2.5.7 Carrier Concentration Temperature Dependence Exerciue 2.6 F: For each of she conditions specified in Eoereise 2.5, determine thr position of H,, compute H,, H, and draw a carefully dimensioned energy baud diagram for the Si sample. Note that H (Si) = 1.08eV and m/m) = 0.71 at 470 K. 0 — 5: (a) In part (a) of Exercise 2.5, the N,,, = 10 ia/ems Si sosssple is moinled at 300 K. Usiitg Eq. (2.36), we cunclude H, is located 0.0073 eV beluss midgap. (The position ing of H, in Si al 300 K is also noted in the text following Eq. 2.36). Next applying Eq. (2.28b), we find H, — H,, = = = bT lu(N,/u,) /l0N) 4 0.0259 ln(.lOi 0.239 eV The energy baud diagram constmcted from she deduced positioning of H, and H,, is shown in Fig. E2.6(a). (b) In part (b) of Exercise 2.5 she Si sample is heated 10470 K. With m/ssi) = 0.71 0.0104eV and H, is dedncrd and kT = 0.0405eV at 470 K, (3/4)kTln(ss/so)) = so be located 0.0 104 eV below midgup. Because N,,, is comparable to iii at 470 K, Eq. (2.37) must be used to compute she positioning of H,,. Specifically, with s , 5 3 and p = 1.62 5< lO’°/cm 10°/cm — H, — H,, = = = fiT ln(p/ss,) 0.0405 1oCt.62 5< 0.0195 eV 54) 0 lOiO/) Here H,, is only slightly removed from H, as pictured in Fig. E2.6(b). c, a a,, Er lbl 1°) Figure e2,6 A number of isolated fuels about the carrier concentration setuperasuen dependence hnvu already been presented at various points in this chapter. The diucnsuiou in Section 2.3 con cerned with dupaut actiun, for uxample, described the increased ionization uf dupont sites und lhe associated increase iu the majority carrier cuucuulratiun when the temperature of a semiconductor is raisud from near T = 0 K toward room temperature. Mute recent sub sections have isclnded a pior uf the intrinsic currier couceutratiun versus temperature (Fig. 2.20) and a calenlatiun indicating chat all semicouducturs become intrinsic (n—s u, p —a ss,) at sufficiently high lrmpecasnres. In this subsection, which concludes the carrier concentration discussion, lumperaturc-eeloted facts ace combined end embellished to pen side a broader, more complete description of how the carrier cosceoleotions vary with temperature. Figure 2.22(a), a typical tuojorily-carcier cuuceutrasiou-oersns-lempcrasure plus con structed assuming a phusphueso-doped N 0 = lOiS/emS Si sample, nicely illusseutes the general features of she cuuceusratiuu-versas-tcmpecasuce dependence. Eoamiuixg Fig. 2.22(a), we find that isis fined at approximately N 0 ever a bread semperasore rouge esseud ing roughly from 150 K to 450 K for the given Si sample. This n 0 or “estriusic N temperature region” cunstitutes the normal operating rouge fur must solid-state devices. Below 100 K or so, in the “freeze-oat temperature region,” n drops significantly below Nu and approaches zero as T —a 0 K. Sn the “intrinsic trmperusore region” at the opposite end of the lemprrature scale, crises above N , usymptotically approaching n, with increas 0 ing T To qualitatively explain she juss-doscribed coxceusrasiou-versus-tempecasure depen dence, it is important to recall that the equilibrium number of carriers within a material is affected by Iwo separate mechanisms. Electrons donated to the conduction bond from do nor atoms and valence baud electrons excited across the baud gap into the conduction baud (broken Si—Si bonds) both contribute to the majority-carrier electron concentration in a donor-doped material. As sesupecolures T—s 0 K the thermal energy available in the system is insufficient to release the weakly bound fifth electron od donor sites and totally insuffi cient 10 excite electrons across she band gap. Hence u = Oat T = 0 K, as visualized on the lefl-haisd side of Fig. 2.22(b). Slightly increasing the mulerial temperature above y 0 K “defrosts” or frees some of the electrons wenkly boand to donor sites. Baud-to-baud cxci laaots, however, remains estresoely unlikely, and therefore the number of observed nIce trotts In the freeze-out tempecutoce region equals the number of insized donors—si = N. Continuing lu increase the system temperature eventually frees almost all of the weakly bound electrons on donor sites, u approaches N , and one enters Ihe extrinsic temperature 0 region. In progressing through the extrinsic temperature region, more and more electrons are uocitrd across Ihu band gap, but the number of elzclcous sapplied in this fashion stays comfortably below N . Ullimotely, of coarse, electrons excised across the bond gup equal, 0 then exceed, and, as pictured on the right-hand side of Fig. 2.22(b), finally swamp she fixed number of electrons derived from the donors. As a practical note, it shoald be pointed out that thu wider the band gap, the greaszc the energy required lo excite electrons from the valence baud into the conductios band, oud 65 r cansiue GEM5eONDGcTOIS FuNouMENvuLu (1) E.cucs pusistisnisig offf. In on intrissoic moseriol u tot-doped aesoicostdoclors maintained at or near room temperature. Sobstitatiug into Eq. (2.37), we therefore conclude Subsataliug for sand p iu Eq. (2.32) using Eqs. (2.16), and setting c Ncetuom = , yields Nveicioc = H,, H, (2.33) Soloing for H,, one obtains H lu(1) + = (2.34) 5(2 (2.3y) \ot — ff = — = kT ln(No/ss;) ... N 3> N,, 0 3> n N (2.38a) hTln(Nojj ...N,N’Na, N,N-u (2.38b) Prom Eqs. (2.38) isis ubsious that the Fersoi level moves systematically upward in energy from H with increasing donor doping and systematically downward in energy from H with ittcreasiug acceptor doping. The exact Ferusi IconS positioning in Si at room tem perature, nicely rci,sfocciug the foregoing stalemeus, is displayed in Fig. 2.21. Also note that for a given semicoudartoc material and ambient temperature, there esist maximum noude generate douocand aacepsoreonceuseasious, doping concentrations above which the materiol becomes degesierate. In Si at room temperature the maximum ssoxdegenerale doping con centrations areWu 1.6 x 10°/em 5 mid N,,, 9.1 5< lOi?/rioS. The large Si doping values required for degeneracy, we should inleiject, have led to the common usage of “highly doped” (or ss’-materiul/p°-mater(al) and “degenerate” us interchangeable terms. Finally, the qaestion may arise: What procedure should be followed in computing H,, when one is aol sure whether a material is nondegenerate or degenerate? Unless a material is ksomn to be degenerate, always assume nondegenemey and compute H,, employing the appropriate tsuudrgenecate relationship. If H,, derived from the nondegescrute furmulo lies in the degenerate zone, one must then, of course, cecompate H,, using the more complex fol’mulism valid for degenerate materials. EnS 0 N 63 (2.32) p = MosinLtNa Cunscqiseittly, (2.36) = ut or if T = According to Eq. (2.36), F, lies precisely as midgop only if 0 K. Poe tlte more practical cone of silicon at room temperatore, Toble 2.1 gives —0.0073 eV, ood F, thrrefore lirs 0.0073 eV sn/sn) = 11.69, (3/4)kT ln(so)us°) below midgop. Althssagh potentinily signifleout in certoio problems, this smoll devto tion from midgop is typieolly nrglccted in drowiog energy bood diogroms, etc. (2) Doped semiconductors (nosdegenecuse, dopossss tosolly ionized). The genecol positioo log of the Fermi level in donoc- nnd occeptor-duped semiconductors nssumed In be nnodegenernte, in equilibrium, nod maintnined at tnmpernsnres svhnen the doponts are fnlly ionized, is readily deduced from Eqs. (2.19). Spneifieally, solving Eqs. (2.19) for E, one nlstuins N &Anoeptonanr 3hz — h•, = — fiT ln(n/n,) = — hT ln(pln,) (2.37) 5 in’ 64 l5’ l0’ ts’ 0 is Ott ° t in 0 tnm’l Na ueN Depending on the simpliflmations iuheeent in n paetienlnr problem, the appropciatweac rice eoneensrnsiun solntinu [Eqs. (2.29). (2.30), (2.31), etc.] is then substituted into Poe exumple, per Eqs. (2.30n) end Eq. (2.37) In detecmine thn positioning of N, in typicnl nccnp (2.3 Sn), ss = N 0 in typical donor-doped semicondnetors nnd p www.EasyEngineering.net 50 Fncud tnvnt pnsitiuning in Si n1309K use fnnetinu nf the duping aunoenteusius. The solid H,, lines wum established nsing Eq. )2.38a) fur dunue-duped materiut and Eq. (2.3gb) fur accep tue-duped material )hT = 0.0259 cv, and u = tO ‘°/nm ). 5 Figure 2.21 —. r - CAROIEn MODELING nnMsenNnnceoe enNnaMnNsucn 2.5.7 Carrier Concentration Temperature Dependence Exerciue 2.6 F: For each of she conditions specified in Eoereise 2.5, determine thr position of H,, compute H,, H, and draw a carefully dimensioned energy baud diagram for the Si sample. Note that H (Si) = 1.08eV and m/m) = 0.71 at 470 K. 0 — 5: (a) In part (a) of Exercise 2.5, the N,,, = 10 ia/ems Si sosssple is moinled at 300 K. Usiitg Eq. (2.36), we cunclude H, is located 0.0073 eV beluss midgap. (The position ing of H, in Si al 300 K is also noted in the text following Eq. 2.36). Next applying Eq. (2.28b), we find ww w H, — H,, = = .Ea = bT lu(N,/u,) /l0N) 4 0.0259 ln(.lOi 0.239 eV syE The energy baud diagram constmcted from she deduced positioning of H, and H,, is shown in Fig. E2.6(a). ngi (b) In part (b) of Exercise 2.5 she Si sample is heated 10470 K. With m/ssi) = 0.71 0.0104eV and H, is dedncrd and kT = 0.0405eV at 470 K, (3/4)kTln(ss/so)) = so be located 0.0 104 eV below midgup. Because N,,, is comparable to iii at 470 K, Eq. (2.37) must be used to compute she positioning of H,,. Specifically, with s , 5 3 and p = 1.62 5< lO’°/cm 10°/cm H, — H,, = = = fiT ln(p/ss,) nee rin g 0.0405 1oCt.62 5< 0.0195 eV — 54) 0 lOiO/) Here H,, is only slightly removed from H, as pictured in Fig. E2.6(b). .ne t c, a a,, Er lbl 1°) Figure e2,6 www.EasyEngineering.net A number of isolated fuels about the carrier concentration setuperasuen dependence hnvu already been presented at various points in this chapter. The diucnsuiou in Section 2.3 con cerned with dupaut actiun, for uxample, described the increased ionization uf dupont sites und lhe associated increase iu the majority carrier cuucuulratiun when the temperature of a semiconductor is raisud from near T = 0 K toward room temperature. Mute recent sub sections have isclnded a pior uf the intrinsic currier couceutratiun versus temperature (Fig. 2.20) and a calenlatiun indicating chat all semicouducturs become intrinsic (n—s u, p —a ss,) at sufficiently high lrmpecasnres. In this subsection, which concludes the carrier concentration discussion, lumperaturc-eeloted facts ace combined end embellished to pen side a broader, more complete description of how the carrier cosceoleotions vary with temperature. Figure 2.22(a), a typical tuojorily-carcier cuuceutrasiou-oersns-lempcrasure plus con structed assuming a phusphueso-doped N 0 = lOiS/emS Si sample, nicely illusseutes the general features of she cuuceusratiuu-versas-tcmpecasuce dependence. Eoamiuixg Fig. 2.22(a), we find that isis fined at approximately N 0 ever a bread semperasore rouge esseud ing roughly from 150 K to 450 K for the given Si sample. This n 0 or “estriusic N temperature region” cunstitutes the normal operating rouge fur must solid-state devices. Below 100 K or so, in the “freeze-oat temperature region,” n drops significantly below Nu and approaches zero as T —a 0 K. Sn the “intrinsic trmperusore region” at the opposite end of the lemprrature scale, crises above N , usymptotically approaching n, with increas 0 ing T To qualitatively explain she juss-doscribed coxceusrasiou-versus-tempecasure depen dence, it is important to recall that the equilibrium number of carriers within a material is affected by Iwo separate mechanisms. Electrons donated to the conduction bond from do nor atoms and valence baud electrons excited across the baud gap into the conduction baud (broken Si—Si bonds) both contribute to the majority-carrier electron concentration in a donor-doped material. As sesupecolures T—s 0 K the thermal energy available in the system is insufficient to release the weakly bound fifth electron od donor sites and totally insuffi cient 10 excite electrons across she band gap. Hence u = Oat T = 0 K, as visualized on the lefl-haisd side of Fig. 2.22(b). Slightly increasing the mulerial temperature above y 0 K “defrosts” or frees some of the electrons wenkly boand to donor sites. Baud-to-baud cxci laaots, however, remains estresoely unlikely, and therefore the number of observed nIce trotts In the freeze-out tempecutoce region equals the number of insized donors—si = N. Continuing lu increase the system temperature eventually frees almost all of the weakly bound electrons on donor sites, u approaches N , and one enters Ihe extrinsic temperature 0 region. In progressing through the extrinsic temperature region, more and more electrons are uocitrd across Ihu band gap, but the number of elzclcous sapplied in this fashion stays comfortably below N . Ullimotely, of coarse, electrons excised across the bond gup equal, 0 then exceed, and, as pictured on the right-hand side of Fig. 2.22(b), finally swamp she fixed number of electrons derived from the donors. As a practical note, it shoald be pointed out that thu wider the band gap, the greaszc the energy required lo excite electrons from the valence baud into the conductios band, oud 65 r cansiue GEM5eONDGcTOIS FuNouMENvuLu (1) E.cucs pusistisnisig offf. In on intrissoic moseriol u tot-doped aesoicostdoclors maintained at or near room temperature. Sobstitatiug into Eq. (2.37), we therefore conclude (2.32) p = Subsataliug for sand p iu Eq. (2.32) using Eqs. (2.16), and setting c Ncetuom = , yields Nveicioc = H,, H, (2.33) Soloing for H,, one obtains H lu(1) + = (2.34) 5(2 (2.3y) \ot — ff = — = kT ln(No/ss;) ... N 3> N,, 0 3> n N (2.38a) hTln(Nojj ...N,N’Na, N,N-u (2.38b) Prom Eqs. (2.38) isis ubsious that the Fersoi level moves systematically upward in energy from H with increasing donor doping and systematically downward in energy from H with ittcreasiug acceptor doping. The exact Ferusi IconS positioning in Si at room tem perature, nicely rci,sfocciug the foregoing stalemeus, is displayed in Fig. 2.21. Also note that for a given semicoudartoc material and ambient temperature, there esist maximum noude generate douocand aacepsoreonceuseasious, doping concentrations above which the materiol becomes degesierate. In Si at room temperature the maximum ssoxdegenerale doping con centrations areWu 1.6 x 10°/em 5 mid N,,, 9.1 5< lOi?/rioS. The large Si doping values required for degeneracy, we should inleiject, have led to the common usage of “highly doped” (or ss’-materiul/p°-mater(al) and “degenerate” us interchangeable terms. Finally, the qaestion may arise: What procedure should be followed in computing H,, when one is aol sure whether a material is nondegenerate or degenerate? Unless a material is ksomn to be degenerate, always assume nondegenemey and compute H,, employing the appropriate tsuudrgenecate relationship. If H,, derived from the nondegescrute furmulo lies in the degenerate zone, one must then, of course, cecompate H,, using the more complex fol’mulism valid for degenerate materials. EnS 0 N 63 MosinLtNa Cunscqiseittly, (2.36) = ut or if T = According to Eq. (2.36), F, lies precisely as midgop only if 0 K. Poe tlte more practical cone of silicon at room temperatore, Toble 2.1 gives —0.0073 eV, ood F, thrrefore lirs 0.0073 eV sn/sn) = 11.69, (3/4)kT ln(so)us°) below midgop. Althssagh potentinily signifleout in certoio problems, this smoll devto tion from midgop is typieolly nrglccted in drowiog energy bood diogroms, etc. (2) Doped semiconductors (nosdegenecuse, dopossss tosolly ionized). The genecol positioo log of the Fermi level in donoc- nnd occeptor-duped semiconductors nssumed In be nnodegenernte, in equilibrium, nod maintnined at tnmpernsnres svhnen the doponts are fnlly ionized, is readily deduced from Eqs. (2.19). Spneifieally, solving Eqs. (2.19) for E, one nlstuins N &Anoeptonanr 3hz — h•, = — fiT ln(n/n,) = — hT ln(pln,) (2.37) 5 in’ l5’ l0’ Ott 0 is ts’ ° t in 0 tnm’l Na ueN Depending on the simpliflmations iuheeent in n paetienlnr problem, the appropciatweac rice eoneensrnsiun solntinu [Eqs. (2.29). (2.30), (2.31), etc.] is then substituted into Poe exumple, per Eqs. (2.30n) end Eq. (2.37) In detecmine thn positioning of N, in typicnl nccnp (2.3 Sn), ss = N 0 in typical donor-doped semicondnetors nnd p Fncud tnvnt pnsitiuning in Si n1309K use fnnetinu nf the duping aunoenteusius. The solid H,, lines wum established nsing Eq. )2.38a) fur dunue-duped materiut and Eq. (2.3gb) fur accep tue-duped material )hT = 0.0259 cv, and u = tO ‘°/nm ). 5 Figure 2.21 —. r 64 50 - www.EasyEngineering.net 65 CAROIEn MODELING nnMsenNnnceoe enNnaMnNsucn 2.5.7 Carrier Concentration Temperature Dependence Exerciue 2.6 F: For each of she conditions specified in Eoereise 2.5, determine thr position of H,, compute H,, H, and draw a carefully dimensioned energy baud diagram for the Si sample. Note that H (Si) = 1.08eV and m/m) = 0.71 at 470 K. 0 — 5: (a) In part (a) of Exercise 2.5, the N,,, = 10 ia/ems Si sosssple is moinled at 300 K. Usiitg Eq. (2.36), we cunclude H, is located 0.0073 eV beluss midgap. (The position ing of H, in Si al 300 K is also noted in the text following Eq. 2.36). Next applying Eq. (2.28b), we find H, — H,, = = = bT lu(N,/u,) /l0N) 4 0.0259 ln(.lOi 0.239 eV The energy baud diagram constmcted from she deduced positioning of H, and H,, is shown in Fig. E2.6(a). (b) In part (b) of Exercise 2.5 she Si sample is heated 10470 K. With m/ssi) = 0.71 0.0104eV and H, is dedncrd and kT = 0.0405eV at 470 K, (3/4)kTln(ss/so)) = so be located 0.0 104 eV below midgup. Because N,,, is comparable to iii at 470 K, Eq. (2.37) must be used to compute she positioning of H,,. Specifically, with s , 5 3 and p = 1.62 5< lO’°/cm 10°/cm — H, — H,, = = = fiT ln(p/ss,) 0.0405 1oCt.62 5< 0.0195 eV 54) 0 lOiO/) Here H,, is only slightly removed from H, as pictured in Fig. E2.6(b). c, a a,, Er lbl 1°) Figure e2,6 A number of isolated fuels about the carrier concentration setuperasuen dependence hnvu already been presented at various points in this chapter. The diucnsuiou in Section 2.3 con cerned with dupaut actiun, for uxample, described the increased ionization uf dupont sites und lhe associated increase iu the majority carrier cuucuulratiun when the temperature of a semiconductor is raisud from near T = 0 K toward room temperature. Mute recent sub sections have isclnded a pior uf the intrinsic currier couceutratiun versus temperature (Fig. 2.20) and a calenlatiun indicating chat all semicouducturs become intrinsic (n—s u, p —a ss,) at sufficiently high lrmpecasnres. In this subsection, which concludes the carrier concentration discussion, lumperaturc-eeloted facts ace combined end embellished to pen side a broader, more complete description of how the carrier cosceoleotions vary with temperature. Figure 2.22(a), a typical tuojorily-carcier cuuceutrasiou-oersns-lempcrasure plus con structed assuming a phusphueso-doped N 0 = lOiS/emS Si sample, nicely illusseutes the general features of she cuuceusratiuu-versas-tcmpecasuce dependence. Eoamiuixg Fig. 2.22(a), we find that isis fined at approximately N 0 ever a bread semperasore rouge esseud ing roughly from 150 K to 450 K for the given Si sample. This n 0 or “estriusic N temperature region” cunstitutes the normal operating rouge fur must solid-state devices. Below 100 K or so, in the “freeze-oat temperature region,” n drops significantly below Nu and approaches zero as T —a 0 K. Sn the “intrinsic trmperusore region” at the opposite end of the lemprrature scale, crises above N , usymptotically approaching n, with increas 0 ing T To qualitatively explain she juss-doscribed coxceusrasiou-versus-tempecasure depen dence, it is important to recall that the equilibrium number of carriers within a material is affected by Iwo separate mechanisms. Electrons donated to the conduction bond from do nor atoms and valence baud electrons excited across the baud gap into the conduction baud (broken Si—Si bonds) both contribute to the majority-carrier electron concentration in a donor-doped material. As sesupecolures T—s 0 K the thermal energy available in the system is insufficient to release the weakly bound fifth electron od donor sites and totally insuffi cient 10 excite electrons across she band gap. Hence u = Oat T = 0 K, as visualized on the lefl-haisd side of Fig. 2.22(b). Slightly increasing the mulerial temperature above y 0 K “defrosts” or frees some of the electrons wenkly boand to donor sites. Baud-to-baud cxci laaots, however, remains estresoely unlikely, and therefore the number of observed nIce trotts In the freeze-out tempecutoce region equals the number of insized donors—si = N. Continuing lu increase the system temperature eventually frees almost all of the weakly bound electrons on donor sites, u approaches N , and one enters Ihe extrinsic temperature 0 region. In progressing through the extrinsic temperature region, more and more electrons are uocitrd across Ihu band gap, but the number of elzclcous sapplied in this fashion stays comfortably below N . Ullimotely, of coarse, electrons excised across the bond gup equal, 0 then exceed, and, as pictured on the right-hand side of Fig. 2.22(b), finally swamp she fixed number of electrons derived from the donors. As a practical note, it shoald be pointed out that thu wider the band gap, the greaszc the energy required lo excite electrons from the valence baud into the conductios band, oud ww w.E asy En gin eer ing .ne www.EasyEngineering.net t www.EasyEngineering.net 66 5CM1C0NOaCT0R FuNDAMENTALn CARRIER MOOELING 67 the itiavimuin operating trntperatnces are deduced to be 385 K, 540 K. and > 700 K foe Ge, Si, and GaAv, respectively. Indeed. GaAs and SiC (if > 2 cV) deviccv cotitinue tube 0 under dcvelopntcni for use in high temperature csvironinentv. 2.6 SUMMARY AND CONCLUDING COMMENTS Nn ww w.E — as y En __J gin eer i rpeCt lob o n’s R=RI O=Nu = - Negligible ,\_Nra3uibln Dominant ___\_ SIC Under the general heading of carrier etoricliog we have described, esansinesi, and charac terized list carriers within a semiconductor under “rest” ur eqnilibriuits conditions. The many important topics addressed in ibis chapter included the introduction of two “Visual ization” models: the banding model and the energy band model. The exlremely useful energy band ittode) is actually more than Just a model—it is a sophisticated sign language providing a concise means of communicating on a nonverbal level. Relative to the carriers themselves, the reader by now Iauus been successfolly prodded into thinking of electrons aad holes as classical bull-like “particles,” svhere the charge on an eleciron is q, ihe charge on a hole iv +q, and the effecijvc masses of the particles are in) and rn) respectively. Tue reader sheuld also know that the carrier numbers in an intrinsic material are equal and rclaiively small: the carrier concentrations, however, can be velectively increased by adding spociah impurity atoms or dopanis to the semiconductor. in addressing the problem of determining ike carrier concentrations in doped semi condnctors, we developed or derived u number of useful mulhemuticul relntionships The . density of slates functions (Eqs. 2.6), the Fermi function (Eq. 2.7), the symmeirical nondegenerate relaiionships for tt and p (Eqs. 2.19), the nap product (Eq. 2.22), the charge neutrality relaiionship (Eel. 2.25). and the simplified n and p espressiunv appropriate for a typical semiconductor nsainnained at mom temperature (Eqs. 2.30 and 2.31) deserve special mention. The cited equations and a few others are collected in Table 2.4. With regard to the ase of these relationships, the reader should be cautioned against “no’lhink plug and chug.” Because semiconductor problems are replete with exceptions, special cases, and nonideal situations, ii is impnratsve that the forntulu nser be aware of derivational assump tions and the validity Iinutv of any and all expressions used in an analysis or computation. In addition to the quantitative carrier relationships, the reader sheuld also have a qualitative “feel” for the carrier distributions in the respective energy bands, the temperature depen dence of the intrinsic concentruliun, and the typical temperature dependence of the majority carrier concentration in a doped semicooductor. Finally, some atiention should be given to the many technical terms and the key para metric values presented in this chapler. The terms extrinsic semiconductor, donor, acceptor, nondegrnerote semiconductor, Fermi level, and so on, will be encountered again and again in the discussion of semiconductor devices. Likewise, a knowledge of typical numerical values for key parameters, such as if 0 = 1.12 eV and na t in Si at 300 K, will IW°/cm be invaluable in vnbvequent work when performing bath “back-of-the.envehupr” and computer-assisted computations. Key parameiric values also serve as yardsticks for gang ing whether newly encountered quantities are relatively small or relatively lunge. ng. ne ModerateT L0WT (b) NighT t FIgUre 2.22 (a) Typical icmperature dependence of the majority-carrier conacetrution in a doped 0 = IS I5/cmi Si sample. semiconductor The plot was constructed assuming a phosphorus-doped N 0 versus T(dashed line) has been included for comparison pueposes. (b) Qualitative explanation o,/N of the concrniraiion_versnsdempeeutaee dependence displayed in part (a). tltc higher tine temperature at the onset of the intrinsic remperalure region. Since the tern. perature at the onset of the intrinsic temperature region corresponds to the upper end of the normal operating range for most solid-state devices, GaAs devices can inhereittly operate at a higher maximum temperature than similarly doped Si devices, which in tarn can op erate at a higher rnacimcm temperature than similarly doped Ge devices. If we osseme. for 0 = 10 iSfcmS, and the onset of the intrinsic example, the critical doping concentration ix N temperature region is appeoximated as the temperature where n, , then from Pig. 2.20 0 N www.EasyEngineering.net 68 CARRiEn MODELING nnMtCONDUCtOR FUNDAMENTALS PROBLEMS Table 2.4 Carrier Modeling Equation Summary. CHAPTER 2 PROBLEM INFORMATION TABLE Coeiplere D(fficialQ! suggested Density of Stales arid Feremi Function Short Point_ightivg_j_,_riptio_ , P,obleinl ,nZVEE) f(E) g,(E) = E 0 if, 263 3r p = N N [mhT Fi ( 0 xL) • 2.1 2.2.4 2 10(5 each purl) 2.2 2.3.4 1 10(2 each part) 1 24 (2 each part) E-band model applications 2 10 (2 each part) Si-doped GaAs 2.4 . fl = = Level 2.3 Carrier Concentrntio,i Relationships n Afier if, E = N p = F ( 0 q,) = N e 5 1r,ruuT p 2.3.4 2,5 2.4.1 2 5 3 in thE Stales/cm 2.6 2.4.2 2 8 (u-2, b-3, c-3) Fermi fnncliou questions 2.7 2.5.1 2—3 .J.Z.. n 2sch- 2.3.4 (a—si) = , 10 ne r)Iii n. np-Product, and Chearge Neutrality ep”taj° = • 2.9 “ 2 15 “ 3 20 (u-3, b.17..discnsn-2) Tvuriation of distribution 2.11 “ 2 10 Derive Eqs. (2.14b), (2.l6b) 2.12 “ 2.14 n E,s-+kTln() 2[(2)1 = 0 N ,N 3 N 8 !‘/S’ 0 ’ n, — kTln(n/ni) kTln(p)n,) ‘Plot distribatinns in bnuds 3 15 (a.3. b-12) Hypothetical g, 2 10 (a-7, b.3) Compute 0 N 5 , N constant = 2.5.3 1 8 (4 each part) n comparison “ 1 5 Plot e vs. TferGe Tricky cone. qorstions 2.16 2.5.5 2 12 (a::d-2. e-4) 2.17 “ 1—2 10 (2 each part) Compute n and p 2.11 2.5.6 2 15(3 each purl) “ 2 15 (u-I 2, b.3) Determine E. E if,, etc. Computer check P2.17/2.18 8 10 •2.19 n Find distribution peak Population at E.+6E .2.10 ‘2.15 e, p. and Fermi Level Computational Relationships 10 .........,.... 2,13 n c vs. 7 computation Bonding model applications 2,20 “ 2 ‘2,21 “ 2 2.22 “ — Verify noodegenerale limits ‘Plot E vs. N .N 0 0 GaAs considerations — p ij 0 N — if, E — 2—3 4 12 (a-3, b-3. c-2, d-4) - 25 (a-I, b-b, c-2, d-3, e-2) v variation with 0 0= na 3 0= Na, N kTlu(N / 0 n) N, .N 0= nt N N 5 0 >0 n 2.5.7 ‘ b” is, 0 ,N 0 4 0” N /im) N 0 Er= kTln(N .2.1 0’0 versus TCumputation With increasing tetttperaturc an expansion of the crystal lattice usually leads to a weakeeing of the interatomic bonds and an associaled decrease in the band gap energy. For many semiconductors the cited variation of the band gap energy svith tenspcrature can be nsodeled by the empirical relationship — E ( 0 T) = E ( 3 0) cOTC 69 www.EasyEngineering.net 66 5CM1C0NOaCT0R FuNDAMENTALn CARRIER MOOELING 67 the itiavimuin operating trntperatnces are deduced to be 385 K, 540 K. and > 700 K foe Ge, Si, and GaAv, respectively. Indeed. GaAs and SiC (if > 2 cV) deviccv cotitinue tube 0 under dcvelopntcni for use in high temperature csvironinentv. 2.6 SUMMARY AND CONCLUDING COMMENTS Nn Under the general heading of carrier etoricliog we have described, esansinesi, and charac terized list carriers within a semiconductor under “rest” ur eqnilibriuits conditions. The many important topics addressed in ibis chapter included the introduction of two “Visual ization” models: the banding model and the energy band model. The exlremely useful energy band ittode) is actually more than Just a model—it is a sophisticated sign language providing a concise means of communicating on a nonverbal level. Relative to the carriers themselves, the reader by now Iauus been successfolly prodded into thinking of electrons aad holes as classical bull-like “particles,” svhere the charge on an eleciron is q, ihe charge on a hole iv +q, and the effecijvc masses of the particles are in) and rn) respectively. Tue reader sheuld also know that the carrier numbers in an intrinsic material are equal and rclaiively small: the carrier concentrations, however, can be velectively increased by adding spociah impurity atoms or dopanis to the semiconductor. in addressing the problem of determining ike carrier concentrations in doped semi condnctors, we developed or derived u number of useful mulhemuticul relntionships The . density of slates functions (Eqs. 2.6), the Fermi function (Eq. 2.7), the symmeirical nondegenerate relaiionships for tt and p (Eqs. 2.19), the nap product (Eq. 2.22), the charge neutrality relaiionship (Eel. 2.25). and the simplified n and p espressiunv appropriate for a typical semiconductor nsainnained at mom temperature (Eqs. 2.30 and 2.31) deserve special mention. The cited equations and a few others are collected in Table 2.4. With regard to the ase of these relationships, the reader should be cautioned against “no’lhink plug and chug.” Because semiconductor problems are replete with exceptions, special cases, and nonideal situations, ii is impnratsve that the forntulu nser be aware of derivational assump tions and the validity Iinutv of any and all expressions used in an analysis or computation. In addition to the quantitative carrier relationships, the reader sheuld also have a qualitative “feel” for the carrier distributions in the respective energy bands, the temperature depen dence of the intrinsic concentruliun, and the typical temperature dependence of the majority carrier concentration in a doped semicooductor. Finally, some atiention should be given to the many technical terms and the key para metric values presented in this chapler. The terms extrinsic semiconductor, donor, acceptor, nondegrnerote semiconductor, Fermi level, and so on, will be encountered again and again in the discussion of semiconductor devices. Likewise, a knowledge of typical numerical values for key parameters, such as if 0 = 1.12 eV and na t in Si at 300 K, will IW°/cm be invaluable in vnbvequent work when performing bath “back-of-the.envehupr” and computer-assisted computations. Key parameiric values also serve as yardsticks for gang ing whether newly encountered quantities are relatively small or relatively lunge. ww rpeCt lob o n’s R=RI O=Nu = __J Negligible - ,\_Nra3uibln Dominant ___\_ SIC NighT ModerateT L0WT (b) FIgUre 2.22 (a) Typical icmperature dependence of the majority-carrier conacetrution in a doped 0 = IS I5/cmi Si sample. semiconductor The plot was constructed assuming a phosphorus-doped N 0 versus T(dashed line) has been included for comparison pueposes. (b) Qualitative explanation o,/N of the concrniraiion_versnsdempeeutaee dependence displayed in part (a). tltc higher tine temperature at the onset of the intrinsic remperalure region. Since the tern. perature at the onset of the intrinsic temperature region corresponds to the upper end of the normal operating range for most solid-state devices, GaAs devices can inhereittly operate at a higher maximum temperature than similarly doped Si devices, which in tarn can op erate at a higher rnacimcm temperature than similarly doped Ge devices. If we osseme. for 0 = 10 iSfcmS, and the onset of the intrinsic example, the critical doping concentration ix N temperature region is appeoximated as the temperature where n, , then from Pig. 2.20 0 N w.E a — syE ngi nee r ing . net www.EasyEngineering.net 68 CARRiEn MODELING nnMtCONDUCtOR FUNDAMENTALS PROBLEMS Table 2.4 Carrier Modeling Equation Summary. CHAPTER 2 PROBLEM INFORMATION TABLE Coeiplere D(fficialQ! suggested Density of Stales arid Feremi Function Short Point_ightivg_j_,_riptio_ , P,obleinl ,nZVEE) f(E) g,(E) = E 0 if, 263 3r p = N N [mhT Fi ( 0 xL) • 2.1 2.2.4 2 10(5 each purl) 2.2 2.3.4 1 10(2 each part) 1 24 (2 each part) E-band model applications 2 10 (2 each part) Si-doped GaAs 2.4 . fl = = Level 2.3 Carrier Concentrntio,i Relationships n Afier if, E = N p = F ( 0 q,) = N e 5 1r,ruuT p 2.3.4 2,5 2.4.1 2 5 3 in thE Stales/cm 2.6 2.4.2 2 8 (u-2, b-3, c-3) Fermi fnncliou questions 2.7 2.5.1 2—3 .J.Z.. n 2sch- 2.3.4 (a—si) = , 10 ne r)Iii n. np-Product, and Chearge Neutrality ep”taj° = • 2.9 “ 2 15 “ 3 20 (u-3, b.17..discnsn-2) Tvuriation of distribution 2.11 “ 2 10 Derive Eqs. (2.14b), (2.l6b) 2.12 “ 2.14 n E,s-+kTln() 2[(2)1 = 0 N ,N 3 N 8 !‘/S’ 0 ’ n, — kTln(n/ni) kTln(p)n,) ‘Plot distribatinns in bnuds 3 15 (a.3. b-12) Hypothetical g, 2 10 (a-7, b.3) Compute 0 N 5 , N constant = 2.5.3 1 8 (4 each part) n comparison “ 1 5 Plot e vs. TferGe Tricky cone. qorstions 2.16 2.5.5 2 12 (a::d-2. e-4) 2.17 “ 1—2 10 (2 each part) Compute n and p 2.11 2.5.6 2 15(3 each purl) “ 2 15 (u-I 2, b.3) Determine E. E if,, etc. Computer check P2.17/2.18 8 10 •2.19 n Find distribution peak Population at E.+6E .2.10 ‘2.15 e, p. and Fermi Level Computational Relationships 10 .........,.... 2,13 n c vs. 7 computation Bonding model applications 2,20 “ 2 ‘2,21 “ 2 2.22 “ — Verify noodegenerale limits ‘Plot E vs. N .N 0 0 GaAs considerations — p ij 0 N — if, E — 2—3 4 12 (a-3, b-3. c-2, d-4) - 25 (a-I, b-b, c-2, d-3, e-2) v variation with 0 0= na 3 0= Na, N kTlu(N / 0 n) N, .N 0= nt N N 5 0 >0 n 2.5.7 ‘ b” is, 0 ,N 0 4 0” N /im) N 0 Er= kTln(N .2.1 0’0 versus TCumputation With increasing tetttperaturc an expansion of the crystal lattice usually leads to a weakeeing of the interatomic bonds and an associaled decrease in the band gap energy. For many semiconductors the cited variation of the band gap energy svith tenspcrature can be nsodeled by the empirical relationship — E ( 0 T) = E ( 3 0) cOTC 69 66 5CM1C0NOaCT0R FuNDAMENTALn CARRIER MOOELING 67 the itiavimuin operating trntperatnces are deduced to be 385 K, 540 K. and > 700 K foe Ge, Si, and GaAv, respectively. Indeed. GaAs and SiC (if > 2 cV) deviccv cotitinue tube 0 under dcvelopntcni for use in high temperature csvironinentv. 2.6 SUMMARY AND CONCLUDING COMMENTS Nn Under the general heading of carrier etoricliog we have described, esansinesi, and charac terized list carriers within a semiconductor under “rest” ur eqnilibriuits conditions. The many important topics addressed in ibis chapter included the introduction of two “Visual ization” models: the banding model and the energy band model. The exlremely useful energy band ittode) is actually more than Just a model—it is a sophisticated sign language providing a concise means of communicating on a nonverbal level. Relative to the carriers themselves, the reader by now Iauus been successfolly prodded into thinking of electrons aad holes as classical bull-like “particles,” svhere the charge on an eleciron is q, ihe charge on a hole iv +q, and the effecijvc masses of the particles are in) and rn) respectively. Tue reader sheuld also know that the carrier numbers in an intrinsic material are equal and rclaiively small: the carrier concentrations, however, can be velectively increased by adding spociah impurity atoms or dopanis to the semiconductor. in addressing the problem of determining ike carrier concentrations in doped semi condnctors, we developed or derived u number of useful mulhemuticul relntionships The . density of slates functions (Eqs. 2.6), the Fermi function (Eq. 2.7), the symmeirical nondegenerate relaiionships for tt and p (Eqs. 2.19), the nap product (Eq. 2.22), the charge neutrality relaiionship (Eel. 2.25). and the simplified n and p espressiunv appropriate for a typical semiconductor nsainnained at mom temperature (Eqs. 2.30 and 2.31) deserve special mention. The cited equations and a few others are collected in Table 2.4. With regard to the ase of these relationships, the reader should be cautioned against “no’lhink plug and chug.” Because semiconductor problems are replete with exceptions, special cases, and nonideal situations, ii is impnratsve that the forntulu nser be aware of derivational assump tions and the validity Iinutv of any and all expressions used in an analysis or computation. In addition to the quantitative carrier relationships, the reader sheuld also have a qualitative “feel” for the carrier distributions in the respective energy bands, the temperature depen dence of the intrinsic concentruliun, and the typical temperature dependence of the majority carrier concentration in a doped semicooductor. Finally, some atiention should be given to the many technical terms and the key para metric values presented in this chapler. The terms extrinsic semiconductor, donor, acceptor, nondegrnerote semiconductor, Fermi level, and so on, will be encountered again and again in the discussion of semiconductor devices. Likewise, a knowledge of typical numerical values for key parameters, such as if 0 = 1.12 eV and na t in Si at 300 K, will IW°/cm be invaluable in vnbvequent work when performing bath “back-of-the.envehupr” and computer-assisted computations. Key parameiric values also serve as yardsticks for gang ing whether newly encountered quantities are relatively small or relatively lunge. — rpeCt lob o n’s R=RI O=Nu = __J Negligible - ,\_Nra3uibln Dominant ___\_ SIC NighT ModerateT L0WT (b) FIgUre 2.22 (a) Typical icmperature dependence of the majority-carrier conacetrution in a doped 0 = IS I5/cmi Si sample. semiconductor The plot was constructed assuming a phosphorus-doped N 0 versus T(dashed line) has been included for comparison pueposes. (b) Qualitative explanation o,/N of the concrniraiion_versnsdempeeutaee dependence displayed in part (a). tltc higher tine temperature at the onset of the intrinsic remperalure region. Since the tern. perature at the onset of the intrinsic temperature region corresponds to the upper end of the normal operating range for most solid-state devices, GaAs devices can inhereittly operate at a higher maximum temperature than similarly doped Si devices, which in tarn can op erate at a higher rnacimcm temperature than similarly doped Ge devices. If we osseme. for 0 = 10 iSfcmS, and the onset of the intrinsic example, the critical doping concentration ix N temperature region is appeoximated as the temperature where n, , then from Pig. 2.20 0 N www.EasyEngineering.net 68 CARRiEn MODELING nnMtCONDUCtOR FUNDAMENTALS PROBLEMS Table 2.4 Carrier Modeling Equation Summary. CHAPTER 2 PROBLEM INFORMATION TABLE Coeiplere D(fficialQ! suggested Density of Stales arid Feremi Function Short Point_ightivg_j_,_riptio_ , P,obleinl ,nZVEE) f(E) g,(E) = ww w n = p = N N E 0 if, 263 3r F ( 0 q,) N p = syE . N e 5 1r,ruuT p ep”taj° = = r)Iii , 10 ne nee rin g n 10(5 each purl) 1 10(2 each part) 1 24 (2 each part) E-band model applications 2 10 (2 each part) Si-doped GaAs ,N 3 N 8 !‘/S’ 0 ’ n, — 2.3.4 2,5 2.4.1 2 5 3 in thE Stales/cm 2.4.2 2 8 (u-2, b-3, c-3) Fermi fnncliou questions 2.7 2.5.1 2—3 kTln(n/ni) kTln(p)n,) 10 Find distribution peak Population at E.+6E .........,.... • 2.9 “ 2 15 .2.10 “ 3 20 (u-3, b.17..discnsn-2) Tvuriation of distribution 2.11 “ 2 10 Derive Eqs. (2.14b), (2.l6b) 2.12 “ 2.14 .ne t 0 N 2.3.4 (a—si) c vs. 7 computation Bonding model applications 2.6 ‘2.15 E,s-+kTln() 2[(2)1 = 2 2.3.4 2,13 e, p. and Fermi Level Computational Relationships n 2.2.4 2.2 .J.Z.. n 2sch- ngi = n. np-Product, and Chearge Neutrality n • 2.1 2.4 fl = [mhT .Ea Level 2.3 Carrier Concentrntio,i Relationships Fi ( 0 xL) Afier if, E = ‘Plot distribatinns in bnuds 3 15 (a.3. b-12) Hypothetical g, 2 10 (a-7, b.3) Compute 0 N 5 , N constant = 2.5.3 1 8 (4 each part) n comparison “ 1 5 Plot e vs. TferGe Tricky cone. qorstions 2.16 2.5.5 2 12 (a::d-2. e-4) 2.17 “ 1—2 10 (2 each part) Compute n and p 2.11 2.5.6 2 15(3 each purl) “ 2 15 (u-I 2, b.3) Determine E. E if,, etc. Computer check P2.17/2.18 8 10 •2.19 2,20 “ 2 ‘2,21 “ 2 2.22 “ — Verify noodegenerale limits ‘Plot E vs. N .N 0 0 GaAs considerations — p ij 0 N — if, E — 2—3 4 12 (a-3, b-3. c-2, d-4) - 25 (a-I, b-b, c-2, d-3, e-2) v variation with 0 0= na 3 0= Na, N kTlu(N / 0 n) N, .N 0= nt N N 5 0 >0 n 2.5.7 ‘ b” is, 0 ,N 0 4 0” N /im) N 0 Er= kTln(N .2.1 0’0 versus TCumputation With increasing tetttperaturc an expansion of the crystal lattice usually leads to a weakeeing of the interatomic bonds and an associaled decrease in the band gap energy. For many semiconductors the cited variation of the band gap energy svith tenspcrature can be nsodeled by the empirical relationship — E ( 0 T) www.EasyEngineering.net = E ( 3 0) cOTC 69 66 5CM1C0NOaCT0R FuNDAMENTALn CARRIER MOOELING 67 the itiavimuin operating trntperatnces are deduced to be 385 K, 540 K. and > 700 K foe Ge, Si, and GaAv, respectively. Indeed. GaAs and SiC (if > 2 cV) deviccv cotitinue tube 0 under dcvelopntcni for use in high temperature csvironinentv. 2.6 SUMMARY AND CONCLUDING COMMENTS Nn Under the general heading of carrier etoricliog we have described, esansinesi, and charac terized list carriers within a semiconductor under “rest” ur eqnilibriuits conditions. The many important topics addressed in ibis chapter included the introduction of two “Visual ization” models: the banding model and the energy band model. The exlremely useful energy band ittode) is actually more than Just a model—it is a sophisticated sign language providing a concise means of communicating on a nonverbal level. Relative to the carriers themselves, the reader by now Iauus been successfolly prodded into thinking of electrons aad holes as classical bull-like “particles,” svhere the charge on an eleciron is q, ihe charge on a hole iv +q, and the effecijvc masses of the particles are in) and rn) respectively. Tue reader sheuld also know that the carrier numbers in an intrinsic material are equal and rclaiively small: the carrier concentrations, however, can be velectively increased by adding spociah impurity atoms or dopanis to the semiconductor. in addressing the problem of determining ike carrier concentrations in doped semi condnctors, we developed or derived u number of useful mulhemuticul relntionships The . density of slates functions (Eqs. 2.6), the Fermi function (Eq. 2.7), the symmeirical nondegenerate relaiionships for tt and p (Eqs. 2.19), the nap product (Eq. 2.22), the charge neutrality relaiionship (Eel. 2.25). and the simplified n and p espressiunv appropriate for a typical semiconductor nsainnained at mom temperature (Eqs. 2.30 and 2.31) deserve special mention. The cited equations and a few others are collected in Table 2.4. With regard to the ase of these relationships, the reader should be cautioned against “no’lhink plug and chug.” Because semiconductor problems are replete with exceptions, special cases, and nonideal situations, ii is impnratsve that the forntulu nser be aware of derivational assump tions and the validity Iinutv of any and all expressions used in an analysis or computation. In addition to the quantitative carrier relationships, the reader sheuld also have a qualitative “feel” for the carrier distributions in the respective energy bands, the temperature depen dence of the intrinsic concentruliun, and the typical temperature dependence of the majority carrier concentration in a doped semicooductor. Finally, some atiention should be given to the many technical terms and the key para metric values presented in this chapler. The terms extrinsic semiconductor, donor, acceptor, nondegrnerote semiconductor, Fermi level, and so on, will be encountered again and again in the discussion of semiconductor devices. Likewise, a knowledge of typical numerical values for key parameters, such as if 0 = 1.12 eV and na t in Si at 300 K, will IW°/cm be invaluable in vnbvequent work when performing bath “back-of-the.envehupr” and computer-assisted computations. Key parameiric values also serve as yardsticks for gang ing whether newly encountered quantities are relatively small or relatively lunge. — rpeCt lob o n’s R=RI O=Nu = __J Negligible - ,\_Nra3uibln Dominant ___\_ SIC NighT ModerateT L0WT (b) FIgUre 2.22 (a) Typical icmperature dependence of the majority-carrier conacetrution in a doped 0 = IS I5/cmi Si sample. semiconductor The plot was constructed assuming a phosphorus-doped N 0 versus T(dashed line) has been included for comparison pueposes. (b) Qualitative explanation o,/N of the concrniraiion_versnsdempeeutaee dependence displayed in part (a). tltc higher tine temperature at the onset of the intrinsic remperalure region. Since the tern. perature at the onset of the intrinsic temperature region corresponds to the upper end of the normal operating range for most solid-state devices, GaAs devices can inhereittly operate at a higher maximum temperature than similarly doped Si devices, which in tarn can op erate at a higher rnacimcm temperature than similarly doped Ge devices. If we osseme. for 0 = 10 iSfcmS, and the onset of the intrinsic example, the critical doping concentration ix N temperature region is appeoximated as the temperature where n, , then from Pig. 2.20 0 N www.EasyEngineering.net 68 CARRiEn MODELING nnMtCONDUCtOR FUNDAMENTALS 69 PROBLEMS Table 2.4 Carrier Modeling Equation Summary. CHAPTER 2 PROBLEM INFORMATION TABLE Coeiplere D(fficialQ! suggested Density of Stales arid Feremi Function Short Point_ightivg_j_,_riptio_ , P,obleinl ,nZVEE) f(E) g,(E) = E 0 if, 263 3r p = N N [mhT Fi ( 0 xL) • 2.1 2.2.4 2 10(5 each purl) 2.2 2.3.4 1 10(2 each part) 1 24 (2 each part) E-band model applications 2 10 (2 each part) Si-doped GaAs 2.4 N p = F ( 0 q,) = N e 5 1r,ruuT p 2.3.4 = , 10 ne r)Iii n. np-Product, and Chearge Neutrality 2,5 2.4.1 2 5 3 in thE Stales/cm 2.4.2 2 8 (u-2, b-3, c-3) Fermi fnncliou questions 2.7 2.5.1 • 2.9 “ .2.10 “ 2.11 “ 2.12 “ ep”taj° = 2.14 ‘2.15 e, p. and Fermi Level Computational Relationships n 2[(2)1 = n E,s-+kTln() 0 N ,N 3 N 8 !‘/S’ 0 ’ n, — kTln(n/ni) kTln(p)n,) 2—3 10 Find distribution peak Population at E.+6E .........,.... 2,13 n c vs. 7 computation Bonding model applications 2.6 .J.Z.. n 2sch- 2.3.4 (a—si) ww w.E . fl = = Level 2.3 Carrier Concentrntio,i Relationships n Afier if, E = asy 2 15 3 20 (u-3, b.17..discnsn-2) Tvuriation of distribution 2 10 Derive Eqs. (2.14b), (2.l6b) ‘Plot distribatinns in bnuds En 3 15 (a.3. b-12) 2 10 (a-7, b.3) 2.5.3 1 8 (4 each part) “ 1 5 gin 2.16 2.5.5 2 12 (a::d-2. e-4) 2.17 “ 1—2 10 (2 each part) 2.11 2.5.6 2 15(3 each purl) •2.19 “ 2 15 (u-I 2, b.3) 2,20 “ 2 8 10 ‘2,21 “ 2.22 “ 2 Hypothetical g, constant = Compute 0 N 5 , N eer n comparison Plot e vs. TferGe ing Tricky cone. qorstions Compute n and p .ne Determine E. E if,, etc. Computer check P2.17/2.18 — Verify noodegenerale limits ‘Plot E vs. N .N 0 0 GaAs considerations — p ij 0 N — if, E — 2—3 4 12 (a-3, b-3. c-2, d-4) - 25 (a-I, b-b, c-2, d-3, e-2) v variation with 0 0= na 3 0= Na, N kTlu(N / 0 n) N, .N 0= nt N N 5 0 >0 n 2.5.7 ‘ b” is, 0 ,N 0 4 0” N /im) N 0 Er= kTln(N .2.1 0’0 versus TCumputation With increasing tetttperaturc an expansion of the crystal lattice usually leads to a weakeeing of the interatomic bonds and an associaled decrease in the band gap energy. For many semiconductors the cited variation of the band gap energy svith tenspcrature can be nsodeled by the empirical relationship — E ( 0 T) = cOTC E ( 3 0) www.EasyEngineering.net t www.EasyEngineering.net 70 SEMICONDUCTOR FUNDAMENTALS CARRIER MODAIJNO witere a and $ ore constants choses to ubtois the best fit to esperiweittal data and E (0) is the lisuiting valoe of the hood gap an 0 K. As for as Si is rottcertted, a fit accurate lo foot plrices is obluised by employing E(0l o = :: 1.170 eV 4.730X 10” eV/K $ = 636 K Tin Kelvin = (a) Make a pint of E vernon T far Si spatsning ihe tcmperaiare range from T T 600 K. Specifically sale the valve of a at 300 K. = Go As Ga As ‘Go As Go As Ga As 0 K to (b) Far T> 300 K, the temperature variation is nearly linear. Nays 5 dan fact, barns aa thars have cmplvyed ww w.E E ( 0 T) = 1.205 — T 0 2.fixlO- . . . Figure P2.4 T> 300 K -— flaw does this nitaplified relatiossfiip compare with the mace precise relationship aver the temperatace region af tvintaol validity? as y En gin e 2.9 Develop an espression for the total number of available STATES/cm t in the conduc tion band between ettergies £, and b + ykT where yin an arbitrary ceustael. 2.6 (a) Under equilibrium conditions attd T> 0 K, what is the probnbifity of an electron state being occupied if it is located at the Fermi level? 2.2 Using the banding model far a semicondactor, indicate how one visaaliaes (a) a miss ing atom, (b) an electroa, )c) a hole, Id) a doSor, (e) an acceptor. (b) If Er is positioned at E, determine (numerical answer required) the probability of finding electrons in states at E, + bE 2.3 Uning the energy hassfi model for a semiconductor, indicate how one visnalizen (a) an electron, (hI a, hole, (c) donor sites, (d) acceptor sites, Is) frecce-oai of majority carrier olcctronv at donor sites an the temperatare is lowered towacd 0 K, If) fresco-oat of majority carrier holes at acceptor sites an the tctsperatnre is lowered toward 0 K, (g) the energy distribotion of carriorn in the respective bands, (h) us ielrisnic nemicoodoctoc, (i)an n-typo scnnicondoctor, ))) a p-type semicondactor, (k) a nondegeserale semiconductor, (1) a de generate sconicondactor. (c) TIte probability a slate is filled at Eb jhg,.grobabiliqs u state is empty at 9 hEm equal ) a bY Where is the Fermi level located? - eri 2.7 The carrier distribatinns or numbetv of carrices as a faurtios of energy in the couduc lion and ealouco bands were noted to peak at an energy very close to the bmd edges. (See the carrier distnibatiou sketches is Pig. 2.16.) Taking the semiconductor lobe uondegener ate, show thai the energy at sehich the carrier distributious peak is Eb + kT/2 and fiT/2 for lbs condacrion and valence bonds, respectively. ng. ne — t 2.4 The bonding onodrl for GaAs is pictorod in Fig. P2.4. 2.8 For a nandogonerate senticondactor, the peak iu the electron distribution vursus energy inside the condttction hued soled ie Pig: 2.16 occues at ff + fiT/2. Expressed as a fraction of the electron population at the peak eeergy, what is the electron population in a nosde genrrate semiconductor at £ = E, + SkY? (a) Draw the boaditng toodel for GaAs depicting the rotooval of the slnaded Ga ond As atoms in Fig. P24 HINT: Ga and As take their hoinding electrons with them when they are removed from the lattice. AIss see Fig. 2.4(a) nhowing tho rcselts of rotooving an atom from the Si lattice. • 2.9 The Fermi level in a Si sample maintained at T = 300 K is located at E Compute and plot the electron and hole distribotions (numbers/cm —eV) m a fnsction of t euergy in the cnudnctios and valence bands, rzspectieely. — (b) Kedraw the bonding model far GaAs nhnwing the insorniins of Si atoms into tlte missing Ga aed As 01010 sites. 10) Is the GaAs doped p- or ri-type when Si atoms replace Ga atoms? Esplain. •2.00 Let us investigate boss’ the electron energy distribution in the condnction band varies usa function of temperatare. Id) Is the GaAs doped p- or n-type when Si atoms replace As atoms? Explain. (0) 71 Draw the energy bond diagram for GaAs when the GaAs is doped with Si on (i) Ga sites aod (ii) on An sites. www.EasyEngineering.net 4. 72 SnMtconnaCsoR raNnaMEnTALO CARRiER MODELtNO (a) Avsutoieg tine somicoadactOr lobe oondegoseratc aed employiEg the Eq. (2.160) ox pressioe for n, confirm that the electron distribution is the condsctioe band normalized to the total electron concentration is gtves by gb(E)f(E) n = • 2.15 Confirm that the n versus T curve foe Ge graphed in Pig. 2.20 cm be generated employing the empirical-fit relationship n,(Ge) 2v,/’KZE, — ?s’rikT . . . . = . 10 t/emS. Ar T = OK, what ace (d) For a silicon sample maintained at T = 300 K, the Fermi level is locaEd 0.259 eV above the ietrinsic Fermi level. Whnt are the hole and eleclron concentrations? (e) In a eondegenerate germuuiam sample maintained under equilibrium conditions nuar roam temperature, inn knows that n, = 10 t /cm n = 2 , p, and NA = 0. Dreermite n and iV . 0 2.12 The density of stales is the coedoction band of a hypothetical somicoEdacior is = lOo)Ttfle_otsstar (c) The electron coucentration in a piece of Si maintained at 300 K uuder eqoilibrium conditions is t /cm Whut is the hole coacentration? lO . 2.11 Starling svith Eq. (2.fib) and following a procedare analogous to that outlined ta the test, prosent tho intermediatr stops and arguments loading to Eqs. (2.14b) and )2.lfib). constant N (b) A somicouduclor is doped with an impurity concentration i such that N N n, and all the smpanlim are ionized. Also, n = N and p = n /N. Is the imparily a dsesor or ae 2 acceptor? Explain. — = (l.7fi 2.16 Concentrative qoontious with a twist. (a) A silicon wafer is uniformly doped p-rype with N,,, the equilibrium hole and electron coeccntrutions? (b) Compute and plot the normalized electron distribution is the condection band versus E E for temperataren T = 300 K, 600 K. and 1200 K. Plot the distribution valaes Em0.4eV) EJOarE 20 eV”)asdE aloagthrxaxis(0 m gJE)flE)/e aloeg the y-axis on a single set of coordinates. Dtscass your resalts. g l 4 E) = ts,var el0 V/(bT)xz £ ar < £ 3kT sketch the electron dislribulior ie the conduction hoed of (a) Assomicg tIne hypotheticd semiconductor. — 2.07 Determine the uqailibriam electron and hale concenlrslioss iusidr a nsifermly doped sample of Si under the following conditious: (b) Following the procedore outlined in the text, establish relottoisships fnr the electron cosccssratioe is the hypothetical somicoedactor analogous to Eqs. (2.140) aed (2. Ifia). 2.13 (a) Verify the statement in Sobsection 2.5.1 [haL 01300 K, = (2.510 N lOts/cms)(m0/mvlSO m in compating by. m = 5 = tst’ ie computing .‘s’ and ni where one sels m 9.109 x 10—tI kg; h 6.625 x III 0joalosec; ood q = 1.602 x 10_is coal. i (b) Using Ihe effective mass values recorded in Tablb I. construct o table that liscs rho netecrical values of Nc aad N for Si, Ge, and GaAs at 300 K. 2.14 la) Determine Ihe tempomture at sslsich the ntrinsic carrier concrstrotiov in It) Si and (ii) GaAs are eqnal 10 the room nomTerotnre (300K) intrinsic carrier concentration of Go. Ib) Semiconductor A has n baud gap of I eV, while semicondoctor E has a band gap of 2 oV. Whal is the ratio of the intriesic carrier concentrations is the twa motertals /n at 200 K. Assume any differences in the carrier effective masses may be (ts, ) 0 iseglected. (a) / 5 T300K,Nu4N cmt o,Ns10i . s- (b) T= 300 K, N,, = , N t 10°/cm 5 4 N,,. T= 300K, N 0 = 9 (d) T= 450K, N,, = 0, ND = 10 ia/ems Ic) T= 650K, N,, = 0.5/s = . 3 lOiS/cm x . N t 10°/cm 0 = , _ 0 vi lOiS/cmt. 2.18 (a to e) For each of the conditions specified in Problem 2.1?, determine the pasilion of E,compute Er E, and draw a carefully dimensioned energy baud diagram for the Si sample. NOTE: £u)Si) = 1.06 eV at 450 K and 1,015 eV ut fi50 K. — • 2,19 (a) Assaming a nondegeoerute Si sample aod total impurily atom ionization, con strict a MATLAR program that computes n, p. and E E, given ccccptable input values of T (temperature in Kelvin), N 0 (cm’”), and A’,, (cm”). Incorporate the program presented iu pars (a) of Eaerrise 2.4 Ia compote n 1 01 a specified T Make use of the MATLAS inFut function to enter the input variables Eom the commaud window. — (b) Use yoar program to check the relevant answers to Problems 2.17 and 2.16. 73 www.EasyEngineering.net 70 SEMICONDUCTOR FUNDAMENTALS CARRIER MODAIJNO witere a and $ ore constants choses to ubtois the best fit to esperiweittal data and E (0) is the lisuiting valoe of the hood gap an 0 K. As for as Si is rottcertted, a fit accurate lo foot plrices is obluised by employing E(0l o = :: 1.170 eV 4.730X 10” eV/K $ = 636 K Tin Kelvin = (a) Make a pint of E vernon T far Si spatsning ihe tcmperaiare range from T T 600 K. Specifically sale the valve of a at 300 K. = = 1.205 — T 0 2.fixlO- . . . Go As Ga As ‘Go As Go As Ga As 0 K to (b) Far T> 300 K, the temperature variation is nearly linear. Nays 5 dan fact, barns aa thars have cmplvyed E ( 0 T) T> 300 K -— flaw does this nitaplified relatiossfiip compare with the mace precise relationship aver the temperatace region af tvintaol validity? ww Figure P2.4 w.E a 2.9 Develop an espression for the total number of available STATES/cm t in the conduc tion band between ettergies £, and b + ykT where yin an arbitrary ceustael. 2.6 (a) Under equilibrium conditions attd T> 0 K, what is the probnbifity of an electron state being occupied if it is located at the Fermi level? syE ngi 2.2 Using the banding model far a semicondactor, indicate how one visaaliaes (a) a miss ing atom, (b) an electroa, )c) a hole, Id) a doSor, (e) an acceptor. (b) If Er is positioned at E, determine (numerical answer required) the probability of finding electrons in states at E, + bE 2.3 Uning the energy hassfi model for a semiconductor, indicate how one visnalizen (a) an electron, (hI a, hole, (c) donor sites, (d) acceptor sites, Is) frecce-oai of majority carrier olcctronv at donor sites an the temperatare is lowered towacd 0 K, If) fresco-oat of majority carrier holes at acceptor sites an the tctsperatnre is lowered toward 0 K, (g) the energy distribotion of carriorn in the respective bands, (h) us ielrisnic nemicoodoctoc, (i)an n-typo scnnicondoctor, ))) a p-type semicondactor, (k) a nondegeserale semiconductor, (1) a de generate sconicondactor. (c) TIte probability a slate is filled at Eb jhg,.grobabiliqs u state is empty at 9 hEm equal ) a bY Where is the Fermi level located? nee r - 2.7 The carrier distribatinns or numbetv of carrices as a faurtios of energy in the couduc lion and ealouco bands were noted to peak at an energy very close to the bmd edges. (See the carrier distnibatiou sketches is Pig. 2.16.) Taking the semiconductor lobe uondegener ate, show thai the energy at sehich the carrier distributious peak is Eb + kT/2 and fiT/2 for lbs condacrion and valence bonds, respectively. ing . — 2.4 The bonding onodrl for GaAs is pictorod in Fig. P2.4. net 2.8 For a nandogonerate senticondactor, the peak iu the electron distribution vursus energy inside the condttction hued soled ie Pig: 2.16 occues at ff + fiT/2. Expressed as a fraction of the electron population at the peak eeergy, what is the electron population in a nosde genrrate semiconductor at £ = E, + SkY? (a) Draw the boaditng toodel for GaAs depicting the rotooval of the slnaded Ga ond As atoms in Fig. P24 HINT: Ga and As take their hoinding electrons with them when they are removed from the lattice. AIss see Fig. 2.4(a) nhowing tho rcselts of rotooving an atom from the Si lattice. • 2.9 The Fermi level in a Si sample maintained at T = 300 K is located at E Compute and plot the electron and hole distribotions (numbers/cm —eV) m a fnsction of t euergy in the cnudnctios and valence bands, rzspectieely. — (b) Kedraw the bonding model far GaAs nhnwing the insorniins of Si atoms into tlte missing Ga aed As 01010 sites. 10) Is the GaAs doped p- or ri-type when Si atoms replace Ga atoms? Esplain. •2.00 Let us investigate boss’ the electron energy distribution in the condnction band varies usa function of temperatare. Id) Is the GaAs doped p- or n-type when Si atoms replace As atoms? Explain. (0) 71 Draw the energy bond diagram for GaAs when the GaAs is doped with Si on (i) Ga sites aod (ii) on An sites. www.EasyEngineering.net 4. 72 SnMtconnaCsoR raNnaMEnTALO CARRiER MODELtNO (a) Avsutoieg tine somicoadactOr lobe oondegoseratc aed employiEg the Eq. (2.160) ox pressioe for n, confirm that the electron distribution is the condsctioe band normalized to the total electron concentration is gtves by gb(E)f(E) n = • 2.15 Confirm that the n versus T curve foe Ge graphed in Pig. 2.20 cm be generated employing the empirical-fit relationship n,(Ge) 2v,/’KZE, — ?s’rikT . . . . = . 10 t/emS. Ar T = OK, what ace (d) For a silicon sample maintained at T = 300 K, the Fermi level is locaEd 0.259 eV above the ietrinsic Fermi level. Whnt are the hole and eleclron concentrations? (e) In a eondegenerate germuuiam sample maintained under equilibrium conditions nuar roam temperature, inn knows that n, = 10 t /cm n = 2 , p, and NA = 0. Dreermite n and iV . 0 2.12 The density of stales is the coedoction band of a hypothetical somicoEdacior is = lOo)Ttfle_otsstar (c) The electron coucentration in a piece of Si maintained at 300 K uuder eqoilibrium conditions is t /cm Whut is the hole coacentration? lO . 2.11 Starling svith Eq. (2.fib) and following a procedare analogous to that outlined ta the test, prosent tho intermediatr stops and arguments loading to Eqs. (2.14b) and )2.lfib). constant N (b) A somicouduclor is doped with an impurity concentration i such that N N n, and all the smpanlim are ionized. Also, n = N and p = n /N. Is the imparily a dsesor or ae 2 acceptor? Explain. — = (l.7fi 2.16 Concentrative qoontious with a twist. (a) A silicon wafer is uniformly doped p-rype with N,,, the equilibrium hole and electron coeccntrutions? (b) Compute and plot the normalized electron distribution is the condection band versus E E for temperataren T = 300 K, 600 K. and 1200 K. Plot the distribution valaes Em0.4eV) EJOarE 20 eV”)asdE aloagthrxaxis(0 m gJE)flE)/e aloeg the y-axis on a single set of coordinates. Dtscass your resalts. g l 4 E) = ts,var el0 V/(bT)xz £ ar < £ 3kT sketch the electron dislribulior ie the conduction hoed of (a) Assomicg tIne hypotheticd semiconductor. — 2.07 Determine the uqailibriam electron and hale concenlrslioss iusidr a nsifermly doped sample of Si under the following conditious: (b) Following the procedore outlined in the text, establish relottoisships fnr the electron cosccssratioe is the hypothetical somicoedactor analogous to Eqs. (2.140) aed (2. Ifia). 2.13 (a) Verify the statement in Sobsection 2.5.1 [haL 01300 K, = (2.510 N lOts/cms)(m0/mvlSO m in compating by. m = 5 = tst’ ie computing .‘s’ and ni where one sels m 9.109 x 10—tI kg; h 6.625 x III 0joalosec; ood q = 1.602 x 10_is coal. i (b) Using Ihe effective mass values recorded in Tablb I. construct o table that liscs rho netecrical values of Nc aad N for Si, Ge, and GaAs at 300 K. 2.14 la) Determine Ihe tempomture at sslsich the ntrinsic carrier concrstrotiov in It) Si and (ii) GaAs are eqnal 10 the room nomTerotnre (300K) intrinsic carrier concentration of Go. Ib) Semiconductor A has n baud gap of I eV, while semicondoctor E has a band gap of 2 oV. Whal is the ratio of the intriesic carrier concentrations is the twa motertals /n at 200 K. Assume any differences in the carrier effective masses may be (ts, ) 0 iseglected. (a) / 5 T300K,Nu4N cmt o,Ns10i . s- (b) T= 300 K, N,, = , N t 10°/cm 5 4 N,,. T= 300K, N 0 = 9 (d) T= 450K, N,, = 0, ND = 10 ia/ems Ic) T= 650K, N,, = 0.5/s = . 3 lOiS/cm x . N t 10°/cm 0 = , _ 0 vi lOiS/cmt. 2.18 (a to e) For each of the conditions specified in Problem 2.1?, determine the pasilion of E,compute Er E, and draw a carefully dimensioned energy baud diagram for the Si sample. NOTE: £u)Si) = 1.06 eV at 450 K and 1,015 eV ut fi50 K. — • 2,19 (a) Assaming a nondegeoerute Si sample aod total impurily atom ionization, con strict a MATLAR program that computes n, p. and E E, given ccccptable input values of T (temperature in Kelvin), N 0 (cm’”), and A’,, (cm”). Incorporate the program presented iu pars (a) of Eaerrise 2.4 Ia compote n 1 01 a specified T Make use of the MATLAS inFut function to enter the input variables Eom the commaud window. — (b) Use yoar program to check the relevant answers to Problems 2.17 and 2.16. 73 70 SEMICONDUCTOR FUNDAMENTALS CARRIER MODAIJNO witere a and $ ore constants choses to ubtois the best fit to esperiweittal data and E (0) is the lisuiting valoe of the hood gap an 0 K. As for as Si is rottcertted, a fit accurate lo foot plrices is obluised by employing E(0l o = :: 1.170 eV 4.730X 10” eV/K $ = 636 K Tin Kelvin = (a) Make a pint of E vernon T far Si spatsning ihe tcmperaiare range from T T 600 K. Specifically sale the valve of a at 300 K. = Go As Ga As ‘Go As Go As Ga As 0 K to (b) Far T> 300 K, the temperature variation is nearly linear. Nays 5 dan fact, barns aa thars have cmplvyed E ( 0 T) = 1.205 — T 0 2.fixlO- . . . Figure P2.4 T> 300 K -— flaw does this nitaplified relatiossfiip compare with the mace precise relationship aver the temperatace region af tvintaol validity? 2.6 (a) Under equilibrium conditions attd T> 0 K, what is the probnbifity of an electron state being occupied if it is located at the Fermi level? (b) If Er is positioned at E, determine (numerical answer required) the probability of finding electrons in states at E, + bE 2.3 Uning the energy hassfi model for a semiconductor, indicate how one visnalizen (a) an electron, (hI a, hole, (c) donor sites, (d) acceptor sites, Is) frecce-oai of majority carrier olcctronv at donor sites an the temperatare is lowered towacd 0 K, If) fresco-oat of majority carrier holes at acceptor sites an the tctsperatnre is lowered toward 0 K, (g) the energy distribotion of carriorn in the respective bands, (h) us ielrisnic nemicoodoctoc, (i)an n-typo scnnicondoctor, ))) a p-type semicondactor, (k) a nondegeserale semiconductor, (1) a de generate sconicondactor. (c) TIte probability a slate is filled at Eb jhg,.grobabiliqs u state is empty at 9 hEm equal ) a bY Where is the Fermi level located? - 2.7 The carrier distribatinns or numbetv of carrices as a faurtios of energy in the couduc lion and ealouco bands were noted to peak at an energy very close to the bmd edges. (See the carrier distnibatiou sketches is Pig. 2.16.) Taking the semiconductor lobe uondegener ate, show thai the energy at sehich the carrier distributious peak is Eb + kT/2 and fiT/2 for lbs condacrion and valence bonds, respectively. — 2.4 The bonding onodrl for GaAs is pictorod in Fig. P2.4. 2.8 For a nandogonerate senticondactor, the peak iu the electron distribution vursus energy inside the condttction hued soled ie Pig: 2.16 occues at ff + fiT/2. Expressed as a fraction of the electron population at the peak eeergy, what is the electron population in a nosde genrrate semiconductor at £ = E, + SkY? (a) Draw the boaditng toodel for GaAs depicting the rotooval of the slnaded Ga ond As atoms in Fig. P24 HINT: Ga and As take their hoinding electrons with them when they are removed from the lattice. AIss see Fig. 2.4(a) nhowing tho rcselts of rotooving an atom from the Si lattice. • 2.9 The Fermi level in a Si sample maintained at T = 300 K is located at E Compute and plot the electron and hole distribotions (numbers/cm —eV) m a fnsction of t euergy in the cnudnctios and valence bands, rzspectieely. — (b) Kedraw the bonding model far GaAs nhnwing the insorniins of Si atoms into tlte missing Ga aed As 01010 sites. 10) Is the GaAs doped p- or ri-type when Si atoms replace Ga atoms? Esplain. •2.00 Let us investigate boss’ the electron energy distribution in the condnction band varies usa function of temperatare. Id) Is the GaAs doped p- or n-type when Si atoms replace As atoms? Explain. Draw the energy bond diagram for GaAs when the GaAs is doped with Si on (i) Ga sites aod (ii) on An sites. www.EasyEngineering.net 72 2.9 Develop an espression for the total number of available STATES/cm t in the conduc tion band between ettergies £, and b + ykT where yin an arbitrary ceustael. 2.2 Using the banding model far a semicondactor, indicate how one visaaliaes (a) a miss ing atom, (b) an electroa, )c) a hole, Id) a doSor, (e) an acceptor. (0) 71 4. SnMtconnaCsoR raNnaMEnTALO CARRiER MODELtNO (a) Avsutoieg tine somicoadactOr lobe oondegoseratc aed employiEg the Eq. (2.160) ox pressioe for n, confirm that the electron distribution is the condsctioe band normalized to the total electron concentration is gtves by gb(E)f(E) n = • 2.15 Confirm that the n versus T curve foe Ge graphed in Pig. 2.20 cm be generated employing the empirical-fit relationship n,(Ge) 2v,/’KZE, — = constant = ?s’rikT ngi . . . £ ar < £ 3kT sketch the electron dislribulior ie the conduction hoed of (a) Assomicg tIne hypotheticd semiconductor. — nee rin g = (2.510 N lOts/cms)(m0/mvlSO .ne t i (b) Using Ihe effective mass values recorded in Tablb I. construct o table that liscs rho netecrical values of Nc aad N for Si, Ge, and GaAs at 300 K. 2.14 la) Determine Ihe tempomture at sslsich the ntrinsic carrier concrstrotiov in It) Si and (ii) GaAs are eqnal 10 the room nomTerotnre (300K) intrinsic carrier concentration of Go. Ib) Semiconductor A has n baud gap of I eV, while semicondoctor E has a band gap of 2 oV. Whal is the ratio of the intriesic carrier concentrations is the twa motertals /n at 200 K. Assume any differences in the carrier effective masses may be (ts, ) 0 iseglected. = OK, what ace (a) / 5 T300K,Nu4N cmt o,Ns10i . s- m in compating by. m = 5 = tst’ ie computing .‘s’ and ni where one sels m 9.109 x 10—tI kg; h 6.625 x III 0joalosec; ood q = 1.602 x 10_is coal. . 10 t/emS. Ar T 2.07 Determine the uqailibriam electron and hale concenlrslioss iusidr a nsifermly doped sample of Si under the following conditious: (b) Following the procedore outlined in the text, establish relottoisships fnr the electron cosccssratioe is the hypothetical somicoedactor analogous to Eqs. (2.140) aed (2. Ifia). 2.13 (a) Verify the statement in Sobsection 2.5.1 [haL 01300 K, . = (d) For a silicon sample maintained at T = 300 K, the Fermi level is locaEd 0.259 eV above the ietrinsic Fermi level. Whnt are the hole and eleclron concentrations? (e) In a eondegenerate germuuiam sample maintained under equilibrium conditions nuar roam temperature, inn knows that n, = 10 t /cm n = 2 , p, and NA = 0. Dreermite n and iV . 0 2.12 The density of stales is the coedoction band of a hypothetical somicoEdacior is syE lOo)Ttfle_otsstar (c) The electron coucentration in a piece of Si maintained at 300 K uuder eqoilibrium conditions is t /cm Whut is the hole coacentration? lO . 2.11 Starling svith Eq. (2.fib) and following a procedare analogous to that outlined ta the test, prosent tho intermediatr stops and arguments loading to Eqs. (2.14b) and )2.lfib). g l 4 E) N (b) A somicouduclor is doped with an impurity concentration i such that N N n, and all the smpanlim are ionized. Also, n = N and p = n /N. Is the imparily a dsesor or ae 2 acceptor? Explain. — .Ea (l.7fi 2.16 Concentrative qoontious with a twist. (a) A silicon wafer is uniformly doped p-rype with N,,, the equilibrium hole and electron coeccntrutions? (b) Compute and plot the normalized electron distribution is the condection band versus E E for temperataren T = 300 K, 600 K. and 1200 K. Plot the distribution valaes Em0.4eV) EJOarE 20 eV”)asdE aloagthrxaxis(0 m gJE)flE)/e aloeg the y-axis on a single set of coordinates. Dtscass your resalts. ww w = ts,var el0 V/(bT)xz (b) T= 300 K, N,, = , N t 10°/cm 5 4 N,,. T= 300K, N 0 = 9 (d) T= 450K, N,, = 0, ND = 10 ia/ems Ic) T= 650K, N,, = 0.5/s = . 3 lOiS/cm x . N t 10°/cm 0 = , _ 0 vi lOiS/cmt. 2.18 (a to e) For each of the conditions specified in Problem 2.1?, determine the pasilion of E,compute Er E, and draw a carefully dimensioned energy baud diagram for the Si sample. NOTE: £u)Si) = 1.06 eV at 450 K and 1,015 eV ut fi50 K. — • 2,19 (a) Assaming a nondegeoerute Si sample aod total impurily atom ionization, con strict a MATLAR program that computes n, p. and E E, given ccccptable input values of T (temperature in Kelvin), N 0 (cm’”), and A’,, (cm”). Incorporate the program presented iu pars (a) of Eaerrise 2.4 Ia compote n 1 01 a specified T Make use of the MATLAS inFut function to enter the input variables Eom the commaud window. — (b) Use yoar program to check the relevant answers to Problems 2.17 and 2.16. www.EasyEngineering.net 73 70 SEMICONDUCTOR FUNDAMENTALS witere a and $ ore constants choses to ubtois the best fit to esperiweittal data and E (0) is the lisuiting valoe of the hood gap an 0 K. As for as Si is rottcertted, a fit accurate lo foot plrices is obluised by employing E(0l o = :: 1.170 eV 4.730X 10” eV/K $ = 636 K Tin Kelvin = (a) Make a pint of E vernon T far Si spatsning ihe tcmperaiare range from T T 600 K. Specifically sale the valve of a at 300 K. = Go As Ga As ‘Go As Go As Ga As 0 K to (b) Far T> 300 K, the temperature variation is nearly linear. Nays 5 dan fact, barns aa thars have cmplvyed E ( 0 T) = 1.205 — T 0 2.fixlO- . . . Figure P2.4 T> 300 K -— flaw does this nitaplified relatiossfiip compare with the mace precise relationship aver the temperatace region af tvintaol validity? 2.9 Develop an espression for the total number of available STATES/cm t in the conduc tion band between ettergies £, and b + ykT where yin an arbitrary ceustael. 2.6 (a) Under equilibrium conditions attd T> 0 K, what is the probnbifity of an electron state being occupied if it is located at the Fermi level? 2.2 Using the banding model far a semicondactor, indicate how one visaaliaes (a) a miss ing atom, (b) an electroa, )c) a hole, Id) a doSor, (e) an acceptor. (b) If Er is positioned at E, determine (numerical answer required) the probability of finding electrons in states at E, + bE 2.3 Uning the energy hassfi model for a semiconductor, indicate how one visnalizen (a) an electron, (hI a, hole, (c) donor sites, (d) acceptor sites, Is) frecce-oai of majority carrier olcctronv at donor sites an the temperatare is lowered towacd 0 K, If) fresco-oat of majority carrier holes at acceptor sites an the tctsperatnre is lowered toward 0 K, (g) the energy distribotion of carriorn in the respective bands, (h) us ielrisnic nemicoodoctoc, (i)an n-typo scnnicondoctor, ))) a p-type semicondactor, (k) a nondegeserale semiconductor, (1) a de generate sconicondactor. (c) TIte probability a slate is filled at Eb jhg,.grobabiliqs u state is empty at 9 hEm equal ) a bY Where is the Fermi level located? - 2.7 The carrier distribatinns or numbetv of carrices as a faurtios of energy in the couduc lion and ealouco bands were noted to peak at an energy very close to the bmd edges. (See the carrier distnibatiou sketches is Pig. 2.16.) Taking the semiconductor lobe uondegener ate, show thai the energy at sehich the carrier distributious peak is Eb + kT/2 and fiT/2 for lbs condacrion and valence bonds, respectively. — 2.4 The bonding onodrl for GaAs is pictorod in Fig. P2.4. 2.8 For a nandogonerate senticondactor, the peak iu the electron distribution vursus energy inside the condttction hued soled ie Pig: 2.16 occues at ff + fiT/2. Expressed as a fraction of the electron population at the peak eeergy, what is the electron population in a nosde genrrate semiconductor at £ = E, + SkY? (a) Draw the boaditng toodel for GaAs depicting the rotooval of the slnaded Ga ond As atoms in Fig. P24 HINT: Ga and As take their hoinding electrons with them when they are removed from the lattice. AIss see Fig. 2.4(a) nhowing tho rcselts of rotooving an atom from the Si lattice. • 2.9 The Fermi level in a Si sample maintained at T = 300 K is located at E Compute and plot the electron and hole distribotions (numbers/cm —eV) m a fnsction of t euergy in the cnudnctios and valence bands, rzspectieely. — (b) Kedraw the bonding model far GaAs nhnwing the insorniins of Si atoms into tlte missing Ga aed As 01010 sites. 10) Is the GaAs doped p- or ri-type when Si atoms replace Ga atoms? Esplain. •2.00 Let us investigate boss’ the electron energy distribution in the condnction band varies usa function of temperatare. Id) Is the GaAs doped p- or n-type when Si atoms replace As atoms? Explain. (0) Draw the energy bond diagram for GaAs when the GaAs is doped with Si on (i) Ga sites aod (ii) on An sites. 4. 72 71 CARRIER MODAIJNO www.EasyEngineering.net SnMtconnaCsoR raNnaMEnTALO gb(E)f(E) n = • 2.15 Confirm that the n versus T curve foe Ge graphed in Pig. 2.20 cm be generated employing the empirical-fit relationship n,(Ge) 2v,/’KZE, 2.11 Starling svith Eq. (2.fib) and following a procedare analogous to that outlined ta the test, prosent tho intermediatr stops and arguments loading to Eqs. (2.14b) and )2.lfib). 2.12 The density of stales is the coedoction band of a hypothetical somicoEdacior is = ?s’rikT . . . £ ar ww w.E m in compating by. m = 5 = tst’ ie computing .‘s’ and ni where one sels m 9.109 x 10—tI kg; h 6.625 x III 0joalosec; ood q = 1.602 x 10_is coal. i (b) Using Ihe effective mass values recorded in Tablb I. construct o table that liscs rho netecrical values of Nc aad N for Si, Ge, and GaAs at 300 K. 2.14 la) Determine Ihe tempomture at sslsich the ntrinsic carrier concrstrotiov in It) Si and (ii) GaAs are eqnal 10 the room nomTerotnre (300K) intrinsic carrier concentration of Go. Ib) Semiconductor A has n baud gap of I eV, while semicondoctor E has a band gap of 2 oV. Whal is the ratio of the intriesic carrier concentrations is the twa motertals /n at 200 K. Assume any differences in the carrier effective masses may be (ts, ) 0 iseglected. = OK, what ace asy En gin 2.07 Determine the uqailibriam electron and hale concenlrslioss iusidr a nsifermly doped sample of Si under the following conditious: (b) Following the procedore outlined in the text, establish relottoisships fnr the electron cosccssratioe is the hypothetical somicoedactor analogous to Eqs. (2.140) aed (2. Ifia). (2.510 N lOts/cms)(m0/mvlSO 10 t/emS. Ar T (d) For a silicon sample maintained at T = 300 K, the Fermi level is locaEd 0.259 eV above the ietrinsic Fermi level. Whnt are the hole and eleclron concentrations? (e) In a eondegenerate germuuiam sample maintained under equilibrium conditions nuar roam temperature, inn knows that n, = 10 t /cm n = 2 , p, and NA = 0. Dreermite n and iV . 0 — 2.13 (a) Verify the statement in Sobsection 2.5.1 [haL 01300 K, . . = (c) The electron coucentration in a piece of Si maintained at 300 K uuder eqoilibrium conditions is t /cm Whut is the hole coacentration? lO . < £ 3kT sketch the electron dislribulior ie the conduction hoed of (a) Assomicg tIne hypotheticd semiconductor. = lOo)Ttfle_otsstar (b) A somicouduclor is doped with an impurity concentration i such that N N n, and all the smpanlim are ionized. Also, n = N and p = n /N. Is the imparily a dsesor or ae 2 acceptor? Explain. — constant N 2.16 Concentrative qoontious with a twist. (a) A silicon wafer is uniformly doped p-rype with N,,, the equilibrium hole and electron coeccntrutions? — = (l.7fi = ts,var el0 V/(bT)xz (b) Compute and plot the normalized electron distribution is the condection band versus E E for temperataren T = 300 K, 600 K. and 1200 K. Plot the distribution valaes Em0.4eV) EJOarE 20 eV”)asdE aloagthrxaxis(0 m gJE)flE)/e aloeg the y-axis on a single set of coordinates. Dtscass your resalts. g l 4 E) 73 CARRiER MODELtNO (a) Avsutoieg tine somicoadactOr lobe oondegoseratc aed employiEg the Eq. (2.160) ox pressioe for n, confirm that the electron distribution is the condsctioe band normalized to the total electron concentration is gtves by (a) / 5 T300K,Nu4N cmt o,Ns10i . s- (b) T= 300 K, N,, = , N t 10°/cm 5 4 N,,. T= 300K, N 0 = 9 (d) T= 450K, N,, = 0, ND = 10 ia/ems Ic) T= 650K, N,, = 0.5/s = . 3 lOiS/cm x . N t 10°/cm 0 = lOiS/cmt. eer , vi 0 ing _ .ne 2.18 (a to e) For each of the conditions specified in Problem 2.1?, determine the pasilion of E,compute Er E, and draw a carefully dimensioned energy baud diagram for the Si sample. NOTE: £u)Si) = 1.06 eV at 450 K and 1,015 eV ut fi50 K. — • 2,19 (a) Assaming a nondegeoerute Si sample aod total impurily atom ionization, con strict a MATLAR program that computes n, p. and E E, given ccccptable input values of T (temperature in Kelvin), N 0 (cm’”), and A’,, (cm”). Incorporate the program presented iu pars (a) of Eaerrise 2.4 Ia compote n 1 01 a specified T Make use of the MATLAS inFut function to enter the input variables Eom the commaud window. — (b) Use yoar program to check the relevant answers to Problems 2.17 and 2.16. www.EasyEngineering.net t www.EasyEngineering.net 74 0 FUNDAMENTALS SEMICONOOCTQ 2.20 According to the text, the maxsmoe, noedegenerate donor and acceptor doping can ccntr,itioos in Si at room trmperatsra are N 10, rood N 0 tb x to 0 = 9 t cm respectively Verify the text statement , 3 3 Carrier Action •2.2l Conntrnet a computer prograits to prodace a ptot of versUs N 0 or Nia similar to Fig. 2.2l. Use the program to verify the accaracy of the cited figare. (Yost may find it convenient to employ the MA’rLAn lognpoco fonctiots in cottstrncting yoar prograot.) — 2.22 GaAs considerations. Carrier modeling onder “test” or eqatlibriom (a) Make a sketch similar to Fig. 2.14 that is specifically appropriate for GaAs Be sore to take into accoant the fact that rn: ,n in GaAs (hi Based on yoar answer to part (a), wonid yen expect F, in GaAs to lie above or below nttdgap? Explain. ww conditions, considered in Chapter portant beraase tt esBblisltes 2, is im the proper fraitte of reference Prom a device ntandpaint, however lie arra cnrrcnt observed ander eqxilibei 0 cvnditians is Only svhes a seattcondnetor rather anintnresting systant is gertnehed giving rise to carrier action era net camer ensposise cair cnrrents flnsn withtn and external to the snwicendnctor system Action, car rier action, in the general concern of this chapter Under nornsom opernting eondtttans the three prtmary types of carrier action ocearriag itiside sewicesidactom are drsft, dffisaiomi and rerasnbirsatiae_gesteraiien In Ibis chapter we first desrrtbe each prtmary type of carrier action qoatitatively and then qxantitatively eelote the aclton to the carrent flowsmsg within the sewicondacter Special esnphosin is placed en rharartersatag the “constants af fire tnatiemm” associated with each type of astd wlterever apprapisate actian, the drsenssson is entetsded to sabsidiary topics of a tare. Althoagh inteodoced relevant no individoatly, the varions types of carrier action are nnderataod to orcar sitttsltaoeoasly inside any gtven semicandoeter Mathematicatty combining the varteas carriei activities nest leads to the enlwinatian of oar carrier.action effaeB, tain the baste set of starting we ob eqnamjons employed in solving device problems of an electrical namre Finally, simple example pmblems are considered to illustrate selation approaches and to snirodace key snpplewental raneepts (e) Geteratune the precise position of the intrinsic Fermi level in GaAs at room temperamre (300 K). w.E Cd) Getermtne the mantmaits nondegenexite donor and acceptor ttoping concentrations in GaAs at room temperatare. 2.23 Given an N 0 as y En gin e to 0 /cm doped Si sample: 5 (a) Present a qealifotive argement that tends to the approximate positioning of the Fermi level to the materiol as T—s OK. I = (b) Constract a N5crL,sn (cempater) program to calcalate and plot E as a fcnctton of temperatare for 200K w Tm 500 K eri — N, in the material Cc) What do yen conclade relative to the general behavior of tttc Fertin tenet positioning as a fanction of temperatnre? ng. ne Cd) Ran year post (hi prograits to determine what happar.s if N 5 is progressively itscreased in decade steps from N 0 = 10°/cm’ to N 0 = 10°/cm’. Sammariee year observat in en 3.1 DRIFT t 3.1.1 Defmnition_visuajjzatjon Drift, by definition sa chargcdparo moafian irs responac to on applied Within semirondoctors the drtfting elererjrflrld motion of the carriers en a microscopic scole can be described as follows, When an (e) Hew woald poor foregoing answers he modified if the Si satople wan doped with donorn instead of acceptocs’ electric field () is applied across a semieendncter as visa alseed in Fig. 3.1(a), the resalting force on the carriers tends to accelerate the +q charged holes in she direction of the electric held and the q charged electrons in the direerson Opposite 10 the alnctrstyge” 505 of collisions toith ionieed iwpsrity atoms mally agitated Ia c alams, and ther hosvevnr mIte carrier acceleration is frrqncntly interrapted camees are d to be scattered). The net (the resnmk pictured in Fig. 3 1(b), is carrier motioa generally a oisg the direction of the electric field, bnt in a disjointed repeated periads af acceleratioa fashion involving and snhseqrcnt decelerating collisions The msreescogtc drifting motion of a single crier is obvieanmy camplea and tedioss to analyac in any qnite detail. Portnaately, measUrable qnaotities are macroscopic — - - i www.EasyEngineering.net 76 nnMteonnnevnn FOnnAMENTALn aannsen naTion A let Ibi Figarn 3.3 fisganded view af a biased p-type semicnndsrtsmr bar of cress-sectional area A. Ptgurn 3.1 Visnalieaeion of cawier drift: (a) motion of miners within a biased srmicandnctar bar: (hi drifisog hem no a microscopic or atomic irate: (a) carrier drift on a macmucapin irate. I (cnreeer) observables thot reflect the average or oserall mntion of the carriers. Averaging over all electrons or hales at any given time, we find that the resalmant motion of each corner type can be dmeribed in terma of a constant drift velocity, n. In other words, an a macroscopic ncale, drift may be nisnalized (see Pig. 3.lc) as nothing ntore than all carriers of a given type moving along at a canstaet velocity in a direction parallel or antipnrallel lathe applied electric field. By way of clarificatioc, it is important to point ext that the drifting motion of the carriers arising in response to an applied electric field is acmaolly saperimposed apex the always-present thermal motion of the carriers. Electrons in the condaction bond and hales ix the valence band gain and Iota energy via collisions with the semicandactec lattice and are nowhere near stationary even andec eqnilibrinm candilians. In fact, nndrc eqailibriam 1/1000 the speed of tight at conditions the therntally related carrier velocities average room memgeeatar& As pictared in Pig. 3.2, however, the thermal motion of the carriers is nsa acre on a wacroscapic scale. averages to completely random. Thermal motion therefore dons not contribate to rnrrent transport, and can be caneeplaally neglected. = the charge par anil time crossing an arbitrarily chosen plane of obsersatian oriented normal lathe dircrtian of carrcnt flow. Considering the p-type semtroadaeter bar of crass-sectional area A shown is Fig. 3.3. and specifically noting the arbimraeily chosen na-normal plane lying within the bar, we can organ: eat v r 0 ,4 pn, tA 5 tA qpe qpeaA . . . . . . . . . .. . .. . All holes this distance back from the e,-normal plane will cross the plane in a time r. All holes in this valome will cross the plane in a time I. Holes crossing the plane in a time Charge crossing the plane ie a dme I. Charge crossing the plane per anit time. - The word definstian of the last qoansity is clearly identical to the formal definition of cnr rant. Thns ‘nhwio 3.1.2 Drift Currertfl Let as nest torn to the tos1 of developing an onalyhical espression foe the correct flawing within a semicondoetor as a resolt of corner drift. By definition = A 5 qpe varn Ftgare 3.2 Theemal macan of a nw-rice hole drift cnrrent (3.1) As a practical matter, the eeoss-sectionai area A appearing in Eq. (3.1) and other carrent formolas is often excess baggage. Casient, moreover, in generally thooght of asa scabs qnantity, while in ecality it is obviansly a vector. These deficiencies are overcawe by mIendaring a related parameter keown as the carreal density, J. 3 han the same aeinntatian as the direction of cnrrnnt Bose and ts eqnal in magnitndc to the corrent per anit area (or J = I/A). By inspection, the rasuamst density associated with hole drift is simply 0 qpn (3.2) Since the drift careent arises in easpoese to an applied electric field, it is reasonable to proceed one step farther and seek a farm of the carrent relationship that explicitly erlates ‘brass to the applied electric field. To this end, we make eafaeenca to the representative drift velocity veesas electric field dnta presented in Pig. 3.4. Note that r 0 is gropoesioral toT at 77 www.EasyEngineering.net 74 0 FUNDAMENTALS SEMICONOOCTQ 2.20 According to the text, the maxsmoe, noedegenerate donor and acceptor doping can ccntr,itioos in Si at room trmperatsra are N 10, rood N 0 tb x to 0 = 9 t cm respectively Verify the text statement , 3 3 Carrier Action •2.2l Conntrnet a computer prograits to prodace a ptot of versUs N 0 or Nia similar to Fig. 2.2l. Use the program to verify the accaracy of the cited figare. (Yost may find it convenient to employ the MA’rLAn lognpoco fonctiots in cottstrncting yoar prograot.) — 2.22 GaAs considerations. Carrier modeling onder “test” or eqatlibriom (a) Make a sketch similar to Fig. 2.14 that is specifically appropriate for GaAs Be sore to take into accoant the fact that rn: ,n in GaAs (hi Based on yoar answer to part (a), wonid yen expect F, in GaAs to lie above or below nttdgap? Explain. conditions, considered in Chapter portant beraase tt esBblisltes 2, is im the proper fraitte of reference Prom a device ntandpaint, however lie arra cnrrcnt observed ander eqxilibei 0 cvnditians is Only svhes a seattcondnetor rather anintnresting systant is gertnehed giving rise to carrier action era net camer ensposise cair cnrrents flnsn withtn and external to the snwicendnctor system Action, car rier action, in the general concern of this chapter Under nornsom opernting eondtttans the three prtmary types of carrier action ocearriag itiside sewicesidactom are drsft, dffisaiomi and rerasnbirsatiae_gesteraiien In Ibis chapter we first desrrtbe each prtmary type of carrier action qoatitatively and then qxantitatively eelote the aclton to the carrent flowsmsg within the sewicondacter Special esnphosin is placed en rharartersatag the “constants af fire tnatiemm” associated with each type of astd wlterever apprapisate actian, the drsenssson is entetsded to sabsidiary topics of a tare. Althoagh inteodoced relevant no individoatly, the varions types of carrier action are nnderataod to orcar sitttsltaoeoasly inside any gtven semicandoeter Mathematicatty combining the varteas carriei activities nest leads to the enlwinatian of oar carrier.action effaeB, tain the baste set of starting we ob eqnamjons employed in solving device problems of an electrical namre Finally, simple example pmblems are considered to illustrate selation approaches and to snirodace key snpplewental raneepts ww (e) Geteratune the precise position of the intrinsic Fermi level in GaAs at room temperamre (300 K). Cd) Getermtne the mantmaits nondegenexite donor and acceptor ttoping concentrations in GaAs at room temperatare. 2.23 Given an N 0 = to 0 /cm doped Si sample: 5 (a) Present a qealifotive argement that tends to the approximate positioning of the Fermi level to the materiol as T—s OK. I (b) Constract a N5crL,sn (cempater) program to calcalate and plot E as a fcnctton of temperatare for 200K w Tm 500 K — w.E a syE ngi nee r N, in the material Cc) What do yen conclade relative to the general behavior of tttc Fertin tenet positioning as a fanction of temperatnre? Cd) Ran year post (hi prograits to determine what happar.s if N 5 is progressively itscreased in decade steps from N 0 = 10°/cm’ to N 0 = 10°/cm’. Sammariee year observat in en ing . 3.1 DRIFT net 3.1.1 Defmnition_visuajjzatjon Drift, by definition sa chargcdparo moafian irs responac to on applied Within semirondoctors the drtfting elererjrflrld motion of the carriers en a microscopic scole can be described as follows, When an (e) Hew woald poor foregoing answers he modified if the Si satople wan doped with donorn instead of acceptocs’ electric field () is applied across a semieendncter as visa alseed in Fig. 3.1(a), the resalting force on the carriers tends to accelerate the +q charged holes in she direction of the electric held and the q charged electrons in the direerson Opposite 10 the alnctrstyge” 505 of collisions toith ionieed iwpsrity atoms mally agitated Ia c alams, and ther hosvevnr mIte carrier acceleration is frrqncntly interrapted camees are d to be scattered). The net (the resnmk pictured in Fig. 3 1(b), is carrier motioa generally a oisg the direction of the electric field, bnt in a disjointed repeated periads af acceleratioa fashion involving and snhseqrcnt decelerating collisions The msreescogtc drifting motion of a single crier is obvieanmy camplea and tedioss to analyac in any qnite detail. Portnaately, measUrable qnaotities are macroscopic — - - i www.EasyEngineering.net 76 nnMteonnnevnn FOnnAMENTALn aannsen naTion A let Ibi Figarn 3.3 fisganded view af a biased p-type semicnndsrtsmr bar of cress-sectional area A. Ptgurn 3.1 Visnalieaeion of cawier drift: (a) motion of miners within a biased srmicandnctar bar: (hi drifisog hem no a microscopic or atomic irate: (a) carrier drift on a macmucapin irate. I (cnreeer) observables thot reflect the average or oserall mntion of the carriers. Averaging over all electrons or hales at any given time, we find that the resalmant motion of each corner type can be dmeribed in terma of a constant drift velocity, n. In other words, an a macroscopic ncale, drift may be nisnalized (see Pig. 3.lc) as nothing ntore than all carriers of a given type moving along at a canstaet velocity in a direction parallel or antipnrallel lathe applied electric field. By way of clarificatioc, it is important to point ext that the drifting motion of the carriers arising in response to an applied electric field is acmaolly saperimposed apex the always-present thermal motion of the carriers. Electrons in the condaction bond and hales ix the valence band gain and Iota energy via collisions with the semicandactec lattice and are nowhere near stationary even andec eqnilibrinm candilians. In fact, nndrc eqailibriam 1/1000 the speed of tight at conditions the therntally related carrier velocities average room memgeeatar& As pictared in Pig. 3.2, however, the thermal motion of the carriers is nsa acre on a wacroscapic scale. averages to completely random. Thermal motion therefore dons not contribate to rnrrent transport, and can be caneeplaally neglected. = the charge par anil time crossing an arbitrarily chosen plane of obsersatian oriented normal lathe dircrtian of carrcnt flow. Considering the p-type semtroadaeter bar of crass-sectional area A shown is Fig. 3.3. and specifically noting the arbimraeily chosen na-normal plane lying within the bar, we can organ: eat v r 0 ,4 pn, tA 5 tA qpe qpeaA . . . . . . . . . .. . .. . All holes this distance back from the e,-normal plane will cross the plane in a time r. All holes in this valome will cross the plane in a time I. Holes crossing the plane in a time Charge crossing the plane ie a dme I. Charge crossing the plane per anit time. - The word definstian of the last qoansity is clearly identical to the formal definition of cnr rant. Thns ‘nhwio 3.1.2 Drift Currertfl Let as nest torn to the tos1 of developing an onalyhical espression foe the correct flawing within a semicondoetor as a resolt of corner drift. By definition = A 5 qpe varn Ftgare 3.2 Theemal macan of a nw-rice hole drift cnrrent (3.1) As a practical matter, the eeoss-sectionai area A appearing in Eq. (3.1) and other carrent formolas is often excess baggage. Casient, moreover, in generally thooght of asa scabs qnantity, while in ecality it is obviansly a vector. These deficiencies are overcawe by mIendaring a related parameter keown as the carreal density, J. 3 han the same aeinntatian as the direction of cnrrnnt Bose and ts eqnal in magnitndc to the corrent per anit area (or J = I/A). By inspection, the rasuamst density associated with hole drift is simply 0 qpn (3.2) Since the drift careent arises in easpoese to an applied electric field, it is reasonable to proceed one step farther and seek a farm of the carrent relationship that explicitly erlates ‘brass to the applied electric field. To this end, we make eafaeenca to the representative drift velocity veesas electric field dnta presented in Pig. 3.4. Note that r 0 is gropoesioral toT at 77 74 0 FUNDAMENTALS SEMICONOOCTQ 2.20 According to the text, the maxsmoe, noedegenerate donor and acceptor doping can ccntr,itioos in Si at room trmperatsra are N 10, rood N 0 tb x to 0 = 9 t cm respectively Verify the text statement , 3 3 Carrier Action •2.2l Conntrnet a computer prograits to prodace a ptot of versUs N 0 or Nia similar to Fig. 2.2l. Use the program to verify the accaracy of the cited figare. (Yost may find it convenient to employ the MA’rLAn lognpoco fonctiots in cottstrncting yoar prograot.) — 2.22 GaAs considerations. Carrier modeling onder “test” or eqatlibriom (a) Make a sketch similar to Fig. 2.14 that is specifically appropriate for GaAs Be sore to take into accoant the fact that rn: ,n in GaAs (hi Based on yoar answer to part (a), wonid yen expect F, in GaAs to lie above or below nttdgap? Explain. conditions, considered in Chapter portant beraase tt esBblisltes 2, is im the proper fraitte of reference Prom a device ntandpaint, however lie arra cnrrcnt observed ander eqxilibei 0 cvnditians is Only svhes a seattcondnetor rather anintnresting systant is gertnehed giving rise to carrier action era net camer ensposise cair cnrrents flnsn withtn and external to the snwicendnctor system Action, car rier action, in the general concern of this chapter Under nornsom opernting eondtttans the three prtmary types of carrier action ocearriag itiside sewicesidactom are drsft, dffisaiomi and rerasnbirsatiae_gesteraiien In Ibis chapter we first desrrtbe each prtmary type of carrier action qoatitatively and then qxantitatively eelote the aclton to the carrent flowsmsg within the sewicondacter Special esnphosin is placed en rharartersatag the “constants af fire tnatiemm” associated with each type of astd wlterever apprapisate actian, the drsenssson is entetsded to sabsidiary topics of a tare. Althoagh inteodoced relevant no individoatly, the varions types of carrier action are nnderataod to orcar sitttsltaoeoasly inside any gtven semicandoeter Mathematicatty combining the varteas carriei activities nest leads to the enlwinatian of oar carrier.action effaeB, tain the baste set of starting we ob eqnamjons employed in solving device problems of an electrical namre Finally, simple example pmblems are considered to illustrate selation approaches and to snirodace key snpplewental raneepts (e) Geteratune the precise position of the intrinsic Fermi level in GaAs at room temperamre (300 K). Cd) Getermtne the mantmaits nondegenexite donor and acceptor ttoping concentrations in GaAs at room temperatare. 2.23 Given an N 0 = to 0 /cm doped Si sample: 5 (a) Present a qealifotive argement that tends to the approximate positioning of the Fermi level to the materiol as T—s OK. I (b) Constract a N5crL,sn (cempater) program to calcalate and plot E as a fcnctton of temperatare for 200K w Tm 500 K — N, in the material Cc) What do yen conclade relative to the general behavior of tttc Fertin tenet positioning as a fanction of temperatnre? Cd) Ran year post (hi prograits to determine what happar.s if N 5 is progressively itscreased in decade steps from N 0 = 10°/cm’ to N 0 = 10°/cm’. Sammariee year observat in en 3.1 DRIFT 3.1.1 Defmnition_visuajjzatjon Drift, by definition sa chargcdparo moafian irs responac to on applied Within semirondoctors the drtfting elererjrflrld motion of the carriers en a microscopic scole can be described as follows, When an (e) Hew woald poor foregoing answers he modified if the Si satople wan doped with donorn instead of acceptocs’ electric field () is applied across a semieendncter as visa alseed in Fig. 3.1(a), the resalting force on the carriers tends to accelerate the +q charged holes in she direction of the electric held and the q charged electrons in the direerson Opposite 10 the alnctrstyge” 505 of collisions toith ionieed iwpsrity atoms mally agitated Ia c alams, and ther hosvevnr mIte carrier acceleration is frrqncntly interrapted camees are d to be scattered). The net (the resnmk pictured in Fig. 3 1(b), is carrier motioa generally a oisg the direction of the electric field, bnt in a disjointed repeated periads af acceleratioa fashion involving and snhseqrcnt decelerating collisions The msreescogtc drifting motion of a single crier is obvieanmy camplea and tedioss to analyac in any qnite detail. Portnaately, measUrable qnaotities are macroscopic — - - i www.EasyEngineering.net 76 nnMteonnnevnn FOnnAMENTALn aannsen naTion A let Ibi Figarn 3.3 fisganded view af a biased p-type semicnndsrtsmr bar of cress-sectional area A. Ptgurn 3.1 Visnalieaeion of cawier drift: (a) motion of miners within a biased srmicandnctar bar: (hi drifisog hem no a microscopic or atomic irate: (a) carrier drift on a macmucapin irate. ww w I (cnreeer) observables thot reflect the average or oserall mntion of the carriers. Averaging over all electrons or hales at any given time, we find that the resalmant motion of each corner type can be dmeribed in terma of a constant drift velocity, n. In other words, an a macroscopic ncale, drift may be nisnalized (see Pig. 3.lc) as nothing ntore than all carriers of a given type moving along at a canstaet velocity in a direction parallel or antipnrallel lathe applied electric field. By way of clarificatioc, it is important to point ext that the drifting motion of the carriers arising in response to an applied electric field is acmaolly saperimposed apex the always-present thermal motion of the carriers. Electrons in the condaction bond and hales ix the valence band gain and Iota energy via collisions with the semicandactec lattice and are nowhere near stationary even andec eqnilibrinm candilians. In fact, nndrc eqailibriam 1/1000 the speed of tight at conditions the therntally related carrier velocities average room memgeeatar& As pictared in Pig. 3.2, however, the thermal motion of the carriers is nsa acre on a wacroscapic scale. averages to completely random. Thermal motion therefore dons not contribate to rnrrent transport, and can be caneeplaally neglected. .Ea syE ngi nee rin g = the charge par anil time crossing an arbitrarily chosen plane of obsersatian oriented normal lathe dircrtian of carrcnt flow. Considering the p-type semtroadaeter bar of crass-sectional area A shown is Fig. 3.3. and specifically noting the arbimraeily chosen na-normal plane lying within the bar, we can organ: eat v r 0 ,4 pn, tA 5 tA qpe qpeaA . . . . . . . . . .. . .. . All holes this distance back from the e,-normal plane will cross the plane in a time r. All holes in this valome will cross the plane in a time I. Holes crossing the plane in a time Charge crossing the plane ie a dme I. Charge crossing the plane per anit time. - .ne t 3.1.2 Drift Currertfl Let as nest torn to the tos1 of developing an onalyhical espression foe the correct flawing within a semicondoetor as a resolt of corner drift. By definition The word definstian of the last qoansity is clearly identical to the formal definition of cnr rant. Thns ‘nhwio = A 5 qpe varn Ftgare 3.2 Theemal macan of a nw-rice www.EasyEngineering.net hole drift cnrrent (3.1) As a practical matter, the eeoss-sectionai area A appearing in Eq. (3.1) and other carrent formolas is often excess baggage. Casient, moreover, in generally thooght of asa scabs qnantity, while in ecality it is obviansly a vector. These deficiencies are overcawe by mIendaring a related parameter keown as the carreal density, J. 3 han the same aeinntatian as the direction of cnrrnnt Bose and ts eqnal in magnitndc to the corrent per anit area (or J = I/A). By inspection, the rasuamst density associated with hole drift is simply 0 qpn (3.2) Since the drift careent arises in easpoese to an applied electric field, it is reasonable to proceed one step farther and seek a farm of the carrent relationship that explicitly erlates ‘brass to the applied electric field. To this end, we make eafaeenca to the representative drift velocity veesas electric field dnta presented in Pig. 3.4. Note that r 0 is gropoesioral toT at 77 74 0 FUNDAMENTALS SEMICONOOCTQ 2.20 According to the text, the maxsmoe, noedegenerate donor and acceptor doping can ccntr,itioos in Si at room trmperatsra are N 10, rood N 0 tb x to 0 = 9 t cm respectively Verify the text statement , 3 3 Carrier Action •2.2l Conntrnet a computer prograits to prodace a ptot of versUs N 0 or Nia similar to Fig. 2.2l. Use the program to verify the accaracy of the cited figare. (Yost may find it convenient to employ the MA’rLAn lognpoco fonctiots in cottstrncting yoar prograot.) — 2.22 GaAs considerations. Carrier modeling onder “test” or eqatlibriom (a) Make a sketch similar to Fig. 2.14 that is specifically appropriate for GaAs Be sore to take into accoant the fact that rn: ,n in GaAs (hi Based on yoar answer to part (a), wonid yen expect F, in GaAs to lie above or below nttdgap? Explain. conditions, considered in Chapter portant beraase tt esBblisltes 2, is im the proper fraitte of reference Prom a device ntandpaint, however lie arra cnrrcnt observed ander eqxilibei 0 cvnditians is Only svhes a seattcondnetor rather anintnresting systant is gertnehed giving rise to carrier action era net camer ensposise cair cnrrents flnsn withtn and external to the snwicendnctor system Action, car rier action, in the general concern of this chapter Under nornsom opernting eondtttans the three prtmary types of carrier action ocearriag itiside sewicesidactom are drsft, dffisaiomi and rerasnbirsatiae_gesteraiien In Ibis chapter we first desrrtbe each prtmary type of carrier action qoatitatively and then qxantitatively eelote the aclton to the carrent flowsmsg within the sewicondacter Special esnphosin is placed en rharartersatag the “constants af fire tnatiemm” associated with each type of astd wlterever apprapisate actian, the drsenssson is entetsded to sabsidiary topics of a tare. Althoagh inteodoced relevant no individoatly, the varions types of carrier action are nnderataod to orcar sitttsltaoeoasly inside any gtven semicandoeter Mathematicatty combining the varteas carriei activities nest leads to the enlwinatian of oar carrier.action effaeB, tain the baste set of starting we ob eqnamjons employed in solving device problems of an electrical namre Finally, simple example pmblems are considered to illustrate selation approaches and to snirodace key snpplewental raneepts (e) Geteratune the precise position of the intrinsic Fermi level in GaAs at room temperamre (300 K). Cd) Getermtne the mantmaits nondegenexite donor and acceptor ttoping concentrations in GaAs at room temperatare. 2.23 Given an N 0 = to 0 /cm doped Si sample: 5 (a) Present a qealifotive argement that tends to the approximate positioning of the Fermi level to the materiol as T—s OK. I (b) Constract a N5crL,sn (cempater) program to calcalate and plot E as a fcnctton of temperatare for 200K w Tm 500 K — N, in the material Cc) What do yen conclade relative to the general behavior of tttc Fertin tenet positioning as a fanction of temperatnre? Cd) Ran year post (hi prograits to determine what happar.s if N 5 is progressively itscreased in decade steps from N 0 = 10°/cm’ to N 0 = 10°/cm’. Sammariee year observat in en 3.1 DRIFT 3.1.1 Defmnition_visuajjzatjon Drift, by definition sa chargcdparo moafian irs responac to on applied Within semirondoctors the drtfting elererjrflrld motion of the carriers en a microscopic scole can be described as follows, When an (e) Hew woald poor foregoing answers he modified if the Si satople wan doped with donorn instead of acceptocs’ electric field () is applied across a semieendncter as visa alseed in Fig. 3.1(a), the resalting force on the carriers tends to accelerate the +q charged holes in she direction of the electric held and the q charged electrons in the direerson Opposite 10 the alnctrstyge” 505 of collisions toith ionieed iwpsrity atoms mally agitated Ia c alams, and ther hosvevnr mIte carrier acceleration is frrqncntly interrapted camees are d to be scattered). The net (the resnmk pictured in Fig. 3 1(b), is carrier motioa generally a oisg the direction of the electric field, bnt in a disjointed repeated periads af acceleratioa fashion involving and snhseqrcnt decelerating collisions The msreescogtc drifting motion of a single crier is obvieanmy camplea and tedioss to analyac in any qnite detail. Portnaately, measUrable qnaotities are macroscopic — - - i www.EasyEngineering.net 76 nnMteonnnevnn FOnnAMENTALn 77 aannsen naTion A let Ibi Figarn 3.3 Ptgurn 3.1 Visnalieaeion of cawier drift: (a) motion of miners within a biased srmicandnctar bar: (hi drifisog hem no a microscopic or atomic irate: (a) carrier drift on a macmucapin irate. ww w.E I (cnreeer) observables thot reflect the average or oserall mntion of the carriers. Averaging over all electrons or hales at any given time, we find that the resalmant motion of each corner type can be dmeribed in terma of a constant drift velocity, n. In other words, an a macroscopic ncale, drift may be nisnalized (see Pig. 3.lc) as nothing ntore than all carriers of a given type moving along at a canstaet velocity in a direction parallel or antipnrallel lathe applied electric field. By way of clarificatioc, it is important to point ext that the drifting motion of the carriers arising in response to an applied electric field is acmaolly saperimposed apex the always-present thermal motion of the carriers. Electrons in the condaction bond and hales ix the valence band gain and Iota energy via collisions with the semicandactec lattice and are nowhere near stationary even andec eqnilibrinm candilians. In fact, nndrc eqailibriam 1/1000 the speed of tight at conditions the therntally related carrier velocities average room memgeeatar& As pictared in Pig. 3.2, however, the thermal motion of the carriers is nsa acre on a wacroscapic scale. averages to completely random. Thermal motion therefore dons not contribate to rnrrent transport, and can be caneeplaally neglected. fisganded view af a biased p-type semicnndsrtsmr bar of cress-sectional area A. = the charge par anil time crossing an arbitrarily chosen plane of obsersatian oriented normal lathe dircrtian of carrcnt flow. Considering the p-type semtroadaeter bar of crass-sectional area A shown is Fig. 3.3. and specifically noting the arbimraeily chosen na-normal plane lying within the bar, we can organ: eat v r 0 ,4 pn, tA 5 tA qpe qpeaA . . . . . . . . . .. . .. . asy En All holes this distance back from the e,-normal plane will cross the plane in a time r. All holes in this valome will cross the plane in a time I. Holes crossing the plane in a time Let as nest torn to the tos1 of developing an onalyhical espression foe the correct flawing within a semicondoetor as a resolt of corner drift. By definition = A 5 qpe hole drift cnrrent ing .ne (3.1) As a practical matter, the eeoss-sectionai area A appearing in Eq. (3.1) and other carrent formolas is often excess baggage. Casient, moreover, in generally thooght of asa scabs qnantity, while in ecality it is obviansly a vector. These deficiencies are overcawe by mIendaring a related parameter keown as the carreal density, J. 3 han the same aeinntatian as the direction of cnrrnnt Bose and ts eqnal in magnitndc to the corrent per anit area (or J = I/A). By inspection, the rasuamst density associated with hole drift is simply varn Ftgare 3.2 Theemal macan of a nw-rice eer The word definstian of the last qoansity is clearly identical to the formal definition of cnr rant. Thns ‘nhwio 3.1.2 Drift Currertfl gin Charge crossing the plane ie a dme I. Charge crossing the plane per anit time. - 0 qpn (3.2) Since the drift careent arises in easpoese to an applied electric field, it is reasonable to proceed one step farther and seek a farm of the carrent relationship that explicitly erlates ‘brass to the applied electric field. To this end, we make eafaeenca to the representative drift velocity veesas electric field dnta presented in Pig. 3.4. Note that r 0 is gropoesioral toT at www.EasyEngineering.net t www.EasyEngineering.net CARRIER ACTION SEMICONDOCTO5I FONOAMENTAI.5 38 78 pa, far Respectively kttossu as tite elrctroa otobiliry and haIr ttiohility, are atwatys taken atid to be positine qoantittes. Note that, althongh electrons drift in the directinu opposite to the applied electric Iteld )e,, = pc,, I. tite cttrrent transported by negattiscly charged particles is itt torn rontitcr to the directisto of drtft 1 5 I. TIte net resttlt, as indicated in c/en ’, 5 )J 0 , Eq. (3.4b), is ao electron enrreut in the direction of the-applied electric held. — — 3.1.3 Mobility Mobihty is obniottslp a central paratneter in characterieittg electroit aitd Itole transport dne ww to drift. As farther readings will reveal, the carrier mobilities slsn play a key role in char ttctertctng the perforutatrce of natty denicen. Ii is reasonable therefore to enamine pa, and nag tu same detail to enhance oar geueral fatoiltarity with the paranteters and to establish a core of nscfnl information fer futnrc reference. lot w.E N 101001 Standard Uttits: cola/v_sec. maintained at tarot tctepera FigurR 3.4 Measamd drift selactty of the cartters in altotp:ite silicon Canstracted frost the data fits and tite data tospec 5 ely tare an a latietion of the applied electric hrtd 0t and Sotitlt 01 al. in Jacabani at as y En gin e low electric holds, witile at To ho more prccise, electric fields e saturates and becomes independent ofT. high ftaaff — T 0 pa eri w ng. ne . ta 57 f_[ Va . ‘h —a 0 t0 • (3.3) t n, praporttoe I far holes and w 2 for electrons itt silicon, pa ts the constant of where and T at low to moderate electric fields, and u,, ts the ltmtttng or sataro ality between limit ea ttt non eelociry approached at’vcry high electric holds. Obstoasly, to the higlt-held depeodeoce. in Eq. 132) is simply replaced by e, and Js55 does net eshtbtt an T-held suless spect the low-hold litttit, witich is of greatest practical ietemst and asosoted hereto yields hod otherwise, a = e’ nag for holes) and substitution iittO Eq. (3.2) 8 (No — —— Jr•ass = —fl (3.4a) 4 ONrP’ par nod system temperatare. to yrattering: The word ntabilirt’ in everyday asage refers ma &geoeral freedam of meoemeot. Analogoasly, in semicondnctar work ttte nobility parameter is a mea sare of the ease of carrier motion in a crystal. Increasiug the motion-itnpediog collisious withtn a crystal decreases the mobility of the carriers. In other words, dte carrier mabiliry varies inversely with the autoant of scattering taking place wititie the semiconductor. As visnalized in Pig. 3.1(b), the doetinant scattering mechanisms in noodegeocrately doped materials of device qaality are typically (i) lattice scattering involving collistant with ther inally agitated lattice atoms, and (ii) ionized itnpttrity (i.e., donor-site and/or acceptor-site) scattering. Relative to lattice scatterieg, it should be eutphasiced that it a the thermal vibra ian, the disptorrtneor of lattice atoms from their lattice positions, tlfat leads to carrier scattering. The internal held associafed with the stationary array of atoms in a reystal is already taken into accoaut in tlte effective Inass formatation. Although qaaotitative relationships connecting the mobility aud scattering can become qaite involved, it is readily established that pa = q(r)/in°, where )t-) is the mean free time between collisions and rite is the coudactivity effective mass. Sioch iscreasiug the namber of motion-impeding collisions decreases the mean free timd between collisions, sse again conclude pa varies iuversely wtth tlte amoaet of seatteriog.,However. pa is also noted to vary irverselyi with the carrier effective mass—tighter carriers mayo mare readily. The m’ in GaAs is siguihcantly smaller than the tnt in Si, theruby’esplaioing the higher mobility of the GaAs electrotts. Rnlatiamtahip ‘4 s = Sasttple Ntttncrirol Volaro: pa., I 3h0 cot°! V-sec atid par = 4b0 cm°IV-see at 300 K in lOtS/emS and At 0 = lotS/cm 1 doped St. respectively, to nncontpeosated high-purity 0 N ) GaAs, the rooto-temperatore mobilities are pa, m h000 cm 5 lots/cm 0 nr N (N 0 / V-nec 5 to 400 cast/V_see. The qanted names are usefal for consparison pttrposes and when and performing order-of-toagnittide eonspt:ta:ious. Also note that pa, > pa, for both Si ar,d GaAs. In the major semicosdactors, pa, is cottsistently greater thatt pa for a gtveu doping Similarly, for electrons one obtains (3db) www.EasyEngineering.net CARRIER AC7tON 5EMICONOaCTOR rUNDAMRN1’ALO 80 3.5 exhibits the observed doping dependence of the electron sod hole mohitities iu Si. Ge, and GaAs. All semicoodactars exhibit the same general dependence. Ar tow doping concentrations, below approximately lO 5 in Si, the caerier fcm t5 mobilities are essentially independent of the doping caoceotration. For dopings in excess lotS/canS, of the mabdities monatnnically decrease with increasing N . 0 0 or N With the aid of Fig. 3.b the explanation of the observed doping dependence is ruIn tivety straightforward. tavokiag an electrient analogy, one can associate a retistaoee to motion with each of the scattering mechanisms. These resistances are its series. At safh cieatly law doping levels, ionieed impurity scattering can be neglected compared to lattice m Rc. When lattice scattering, which is scattering, or in the analogy, RTovat = RL + net a function at N , becomes the dominant scattering mechanism, it aatomatically 0 0 or N follows that the carrier mobilities will be likewise independent of N . Far dapings 0 0 or N in eseens of —10 5 in Si, ionized imparity scattering and the attociated reststance to /cm t5 motion eon an longer be neglected. Increasing the snmber of scattering centers by adding more and more acceptors or donors progressively increases the am000t of ionized imparity’ scattering and systematically decresses the carrier mobilities. Doping Dependence: Figare — 111150 b g l tm Na orNu leoIs 0° 2 5 0 ‘°, a, gg 0 tab Hint’ ga s v-y last 357 1352 ‘da°a tO-a. ost 000 ass 055 . ‘ , a :**. toil too tots ‘*- tots 0 or V tcnr°’ N 1°) Tenrtperotare Dependence: The tempcrntnrc dependence of the electron and hole mebili ties in Si n’ith doping as a parameter is displayed in Pig. 3.7. For dopings of N 0 or N w /cm, the data merge irta a single carve and there is a near power-law increase in the t4 10 carrier mabilities as the temperxmrr is decreased. Roaghly, pa, w T_asont and pa 2 w T’tt55t. For progressively higher dopiogs, the carrier mabitities still increase with de creasing temperotare, bat at a systematically decreasing rate. In fact, some N N 0 5 /cm tt tfi experimental data (not shown) exhibit a decreooe in pat as Tin deerensed below 200 K. The general tetaprratare dependence of the carrier mabilities is relatively easy to ex plain in the low doping limit. As noted in the doping dependence discassion, lattice scat tering is the dominant scattering mechanism (RTOTOL R) in lightly doped samples. Decreasing the system temperature castes an ever-decreasing thermal agitation of the semi candactar atoms, which in turn decreases the lattice scattering. The decreased scattering ) (b) ir Ftaurn 3.5 Roano temneratam caorirr muobilitiei nsa funehan of thu dopant eoncestrat,oa (al St hapedaror to motion doe to tathee scattering: : tmpedmce to mohan doe to ianiend tmpnnty scattering: —No doptog dependence. 0 or 1/5 —Inereaset with N —Deareasrs trith drcmaning T.’ —Inatrases ssith decreasing T. FlgurR 3.6 Electrieol analogy far scattering is a srtnteoodsetac R and N 1 represert the impedasar to motion doe to lattice seaneriog and iosieed imparity scattering, respectively. 81 www.EasyEngineering.net CARRIER ACTION SEMICONDOCTO5I FONOAMENTAI.5 38 78 pa, far Respectively kttossu as tite elrctroa otobiliry and haIr ttiohility, are atwatys taken atid to be positine qoantittes. Note that, althongh electrons drift in the directinu opposite to the applied electric Iteld )e,, = pc,, I. tite cttrrent transported by negattiscly charged particles is itt torn rontitcr to the directisto of drtft 1 5 I. TIte net resttlt, as indicated in c/en ’, 5 )J 0 , Eq. (3.4b), is ao electron enrreut in the direction of the-applied electric held. — — 3.1.3 Mobility Mobihty is obniottslp a central paratneter in characterieittg electroit aitd Itole transport dne to drift. As farther readings will reveal, the carrier mobilities slsn play a key role in char ttctertctng the perforutatrce of natty denicen. Ii is reasonable therefore to enamine pa, and nag tu same detail to enhance oar geueral fatoiltarity with the paranteters and to establish a core of nscfnl information fer futnrc reference. ww lot N 101001 low electric holds, witile at To ho more prccise, electric fields e saturates and becomes independent ofT. high ftaaff — T 0 pa . . ta 57 f_[ Va w (3.3) t0 • n, praporttoe I far holes and w 2 for electrons itt silicon, pa ts the constant of where and T at low to moderate electric fields, and u,, ts the ltmtttng or sataro ality between limit ea ttt non eelociry approached at’vcry high electric holds. Obstoasly, to the higlt-held depeodeoce. in Eq. 132) is simply replaced by e, and Js55 does net eshtbtt an T-held suless spect the low-hold litttit, witich is of greatest practical ietemst and asosoted hereto yields hod otherwise, a = e’ nag for holes) and substitution iittO Eq. (3.2) 8 (No — Jr•ass = Sasttple Ntttncrirol Volaro: pa., I 3h0 cot°! V-sec atid par = 4b0 cm°IV-see at 300 K in lOtS/emS and At 0 = lotS/cm 1 doped St. respectively, to nncontpeosated high-purity 0 N ) GaAs, the rooto-temperatore mobilities are pa, m h000 cm 5 lots/cm 0 nr N (N 0 / V-nec 5 to 400 cast/V_see. The qanted names are usefal for consparison pttrposes and when and performing order-of-toagnittide eonspt:ta:ious. Also note that pa, > pa, for both Si ar,d GaAs. In the major semicosdactors, pa, is cottsistently greater thatt pa for a gtveu doping par nod system temperatare. —fl (3.4a) 4 ONrP’ Similarly, for electrons one obtains (3db) syE ngi nee r to yrattering: The word ntabilirt’ in everyday asage refers ma &geoeral freedam of meoemeot. Analogoasly, in semicondnctar work ttte nobility parameter is a mea sare of the ease of carrier motion in a crystal. Increasiug the motion-itnpediog collisious withtn a crystal decreases the mobility of the carriers. In other words, dte carrier mabiliry varies inversely with the autoant of scattering taking place wititie the semiconductor. As visnalized in Pig. 3.1(b), the doetinant scattering mechanisms in noodegeocrately doped materials of device qaality are typically (i) lattice scattering involving collistant with ther inally agitated lattice atoms, and (ii) ionized itnpttrity (i.e., donor-site and/or acceptor-site) scattering. Relative to lattice scatterieg, it should be eutphasiced that it a the thermal vibra ian, the disptorrtneor of lattice atoms from their lattice positions, tlfat leads to carrier scattering. The internal held associafed with the stationary array of atoms in a reystal is already taken into accoaut in tlte effective Inass formatation. Although qaaotitative relationships connecting the mobility aud scattering can become qaite involved, it is readily established that pa = q(r)/in°, where )t-) is the mean free time between collisions and rite is the coudactivity effective mass. Sioch iscreasiug the namber of motion-impeding collisions decreases the mean free timd between collisions, sse again conclude pa varies iuversely wtth tlte amoaet of seatteriog.,However. pa is also noted to vary irverselyi with the carrier effective mass—tighter carriers mayo mare readily. The m’ in GaAs is siguihcantly smaller than the tnt in Si, theruby’esplaioing the higher mobility of the GaAs electrotts. Rnlatiamtahip ‘h —a 0 ‘4 s = —— w.E a Standard Uttits: cola/v_sec. maintained at tarot tctepera FigurR 3.4 Measamd drift selactty of the cartters in altotp:ite silicon Canstracted frost the data fits and tite data tospec 5 ely tare an a latietion of the applied electric hrtd 0t and Sotitlt 01 al. in Jacabani at ing . net www.EasyEngineering.net CARRIER AC7tON 5EMICONOaCTOR rUNDAMRN1’ALO 80 3.5 exhibits the observed doping dependence of the electron sod hole mohitities iu Si. Ge, and GaAs. All semicoodactars exhibit the same general dependence. Ar tow doping concentrations, below approximately lO 5 in Si, the caerier fcm t5 mobilities are essentially independent of the doping caoceotration. For dopings in excess lotS/canS, of the mabdities monatnnically decrease with increasing N . 0 0 or N With the aid of Fig. 3.b the explanation of the observed doping dependence is ruIn tivety straightforward. tavokiag an electrient analogy, one can associate a retistaoee to motion with each of the scattering mechanisms. These resistances are its series. At safh cieatly law doping levels, ionieed impurity scattering can be neglected compared to lattice m Rc. When lattice scattering, which is scattering, or in the analogy, RTovat = RL + net a function at N , becomes the dominant scattering mechanism, it aatomatically 0 0 or N follows that the carrier mobilities will be likewise independent of N . Far dapings 0 0 or N in eseens of —10 5 in Si, ionized imparity scattering and the attociated reststance to /cm t5 motion eon an longer be neglected. Increasing the snmber of scattering centers by adding more and more acceptors or donors progressively increases the am000t of ionized imparity’ scattering and systematically decresses the carrier mobilities. Doping Dependence: Figare — 111150 b g l tm Na orNu leoIs 0° 2 5 0 ‘°, a, gg 0 tab Hint’ ga s v-y last 357 1352 ‘da°a tO-a. ost 000 ass 055 . ‘ , a :**. toil too tots ‘*- tots 0 or V tcnr°’ N 1°) Tenrtperotare Dependence: The tempcrntnrc dependence of the electron and hole mebili ties in Si n’ith doping as a parameter is displayed in Pig. 3.7. For dopings of N 0 or N w /cm, the data merge irta a single carve and there is a near power-law increase in the t4 10 carrier mabilities as the temperxmrr is decreased. Roaghly, pa, w T_asont and pa 2 w T’tt55t. For progressively higher dopiogs, the carrier mabitities still increase with de creasing temperotare, bat at a systematically decreasing rate. In fact, some N N 0 5 /cm tt tfi experimental data (not shown) exhibit a decreooe in pat as Tin deerensed below 200 K. The general tetaprratare dependence of the carrier mabilities is relatively easy to ex plain in the low doping limit. As noted in the doping dependence discassion, lattice scat tering is the dominant scattering mechanism (RTOTOL R) in lightly doped samples. Decreasing the system temperature castes an ever-decreasing thermal agitation of the semi candactar atoms, which in turn decreases the lattice scattering. The decreased scattering ) (b) ir Ftaurn 3.5 Roano temneratam caorirr muobilitiei nsa funehan of thu dopant eoncestrat,oa (al St hapedaror to motion doe to tathee scattering: : tmpedmce to mohan doe to ianiend tmpnnty scattering: —No doptog dependence. 0 or 1/5 —Inereaset with N —Deareasrs trith drcmaning T.’ —Inatrases ssith decreasing T. FlgurR 3.6 Electrieol analogy far scattering is a srtnteoodsetac R and N 1 represert the impedasar to motion doe to lattice seaneriog and iosieed imparity scattering, respectively. 81 CARRIER ACTION SEMICONDOCTO5I FONOAMENTAI.5 38 78 pa, far Respectively kttossu as tite elrctroa otobiliry and haIr ttiohility, are atwatys taken atid to be positine qoantittes. Note that, althongh electrons drift in the directinu opposite to the applied electric Iteld )e,, = pc,, I. tite cttrrent transported by negattiscly charged particles is itt torn rontitcr to the directisto of drtft 1 5 I. TIte net resttlt, as indicated in c/en ’, 5 )J 0 , Eq. (3.4b), is ao electron enrreut in the direction of the-applied electric held. — — 3.1.3 Mobility Mobihty is obniottslp a central paratneter in characterieittg electroit aitd Itole transport dne to drift. As farther readings will reveal, the carrier mobilities slsn play a key role in char ttctertctng the perforutatrce of natty denicen. Ii is reasonable therefore to enamine pa, and nag tu same detail to enhance oar geueral fatoiltarity with the paranteters and to establish a core of nscfnl information fer futnrc reference. lot N 101001 Standard Uttits: cola/v_sec. maintained at tarot tctepera FigurR 3.4 Measamd drift selactty of the cartters in altotp:ite silicon Canstracted frost the data fits and tite data tospec 5 ely tare an a latietion of the applied electric hrtd 0t and Sotitlt 01 al. in Jacabani at low electric holds, witile at To ho more prccise, electric fields e saturates and becomes independent ofT. high ftaaff — T 0 pa . . ta 57 f_[ Va w (3.3) t0 • n, praporttoe I far holes and w 2 for electrons itt silicon, pa ts the constant of where and T at low to moderate electric fields, and u,, ts the ltmtttng or sataro ality between limit ea ttt non eelociry approached at’vcry high electric holds. Obstoasly, to the higlt-held depeodeoce. in Eq. 132) is simply replaced by e, and Js55 does net eshtbtt an T-held suless spect the low-hold litttit, witich is of greatest practical ietemst and asosoted hereto yields hod otherwise, a = e’ nag for holes) and substitution iittO Eq. (3.2) 8 (No — —— Jr•ass = par nod system temperatare. to yrattering: The word ntabilirt’ in everyday asage refers ma &geoeral freedam of meoemeot. Analogoasly, in semicondnctar work ttte nobility parameter is a mea sare of the ease of carrier motion in a crystal. Increasiug the motion-itnpediog collisious withtn a crystal decreases the mobility of the carriers. In other words, dte carrier mabiliry varies inversely with the autoant of scattering taking place wititie the semiconductor. As visnalized in Pig. 3.1(b), the doetinant scattering mechanisms in noodegeocrately doped materials of device qaality are typically (i) lattice scattering involving collistant with ther inally agitated lattice atoms, and (ii) ionized itnpttrity (i.e., donor-site and/or acceptor-site) scattering. Relative to lattice scatterieg, it should be eutphasiced that it a the thermal vibra ian, the disptorrtneor of lattice atoms from their lattice positions, tlfat leads to carrier scattering. The internal held associafed with the stationary array of atoms in a reystal is already taken into accoaut in tlte effective Inass formatation. Although qaaotitative relationships connecting the mobility aud scattering can become qaite involved, it is readily established that pa = q(r)/in°, where )t-) is the mean free time between collisions and rite is the coudactivity effective mass. Sioch iscreasiug the namber of motion-impeding collisions decreases the mean free timd between collisions, sse again conclude pa varies iuversely wtth tlte amoaet of seatteriog.,However. pa is also noted to vary irverselyi with the carrier effective mass—tighter carriers mayo mare readily. The m’ in GaAs is siguihcantly smaller than the tnt in Si, theruby’esplaioing the higher mobility of the GaAs electrotts. Rnlatiamtahip ‘h —a 0 ‘4 s = Sasttple Ntttncrirol Volaro: pa., I 3h0 cot°! V-sec atid par = 4b0 cm°IV-see at 300 K in lOtS/emS and At 0 = lotS/cm 1 doped St. respectively, to nncontpeosated high-purity 0 N ) GaAs, the rooto-temperatore mobilities are pa, m h000 cm 5 lots/cm 0 nr N (N 0 / V-nec 5 to 400 cast/V_see. The qanted names are usefal for consparison pttrposes and when and performing order-of-toagnittide eonspt:ta:ious. Also note that pa, > pa, for both Si ar,d GaAs. In the major semicosdactors, pa, is cottsistently greater thatt pa for a gtveu doping —fl (3.4a) 4 ONrP’ Similarly, for electrons one obtains (3db) www.EasyEngineering.net CARRIER AC7tON 5EMICONOaCTOR rUNDAMRN1’ALO 80 3.5 exhibits the observed doping dependence of the electron sod hole mohitities iu Si. Ge, and GaAs. All semicoodactars exhibit the same general dependence. Ar tow doping concentrations, below approximately lO 5 in Si, the caerier fcm t5 mobilities are essentially independent of the doping caoceotration. For dopings in excess lotS/canS, of the mabdities monatnnically decrease with increasing N . 0 0 or N With the aid of Fig. 3.b the explanation of the observed doping dependence is ruIn tivety straightforward. tavokiag an electrient analogy, one can associate a retistaoee to motion with each of the scattering mechanisms. These resistances are its series. At safh cieatly law doping levels, ionieed impurity scattering can be neglected compared to lattice m Rc. When lattice scattering, which is scattering, or in the analogy, RTovat = RL + net a function at N , becomes the dominant scattering mechanism, it aatomatically 0 0 or N follows that the carrier mobilities will be likewise independent of N . Far dapings 0 0 or N in eseens of —10 5 in Si, ionized imparity scattering and the attociated reststance to /cm t5 motion eon an longer be neglected. Increasing the snmber of scattering centers by adding more and more acceptors or donors progressively increases the am000t of ionized imparity’ scattering and systematically decresses the carrier mobilities. Doping Dependence: Figare — 111150 b g 0 ‘°, a, l tm Na orNu leoIs 0° 2 5 ww Hint’w gg 0 tab ga s v-y last 357 1352 ‘da°a tO-a. .Ea toil ost 000 ass 055 . ‘ , a :**. syE too tots ngi ‘*- tots 0 or V tcnr°’ N 1°) nee rin g .ne t Tenrtperotare Dependence: The tempcrntnrc dependence of the electron and hole mebili ties in Si n’ith doping as a parameter is displayed in Pig. 3.7. For dopings of N 0 or N w /cm, the data merge irta a single carve and there is a near power-law increase in the t4 10 carrier mabilities as the temperxmrr is decreased. Roaghly, pa, w T_asont and pa 2 w T’tt55t. For progressively higher dopiogs, the carrier mabitities still increase with de creasing temperotare, bat at a systematically decreasing rate. In fact, some N N 0 5 /cm tt tfi experimental data (not shown) exhibit a decreooe in pat as Tin deerensed below 200 K. The general tetaprratare dependence of the carrier mabilities is relatively easy to ex plain in the low doping limit. As noted in the doping dependence discassion, lattice scat tering is the dominant scattering mechanism (RTOTOL R) in lightly doped samples. Decreasing the system temperature castes an ever-decreasing thermal agitation of the semi candactar atoms, which in turn decreases the lattice scattering. The decreased scattering ) (b) ir Ftaurn 3.5 Roano temneratam caorirr muobilitiei nsa funehan of thu dopant eoncestrat,oa (al St www.EasyEngineering.net hapedaror to motion doe to tathee scattering: : tmpedmce to mohan doe to ianiend tmpnnty scattering: —No doptog dependence. 0 or 1/5 —Inereaset with N —Deareasrs trith drcmaning T.’ —Inatrases ssith decreasing T. FlgurR 3.6 Electrieol analogy far scattering is a srtnteoodsetac R and N 1 represert the impedasar to motion doe to lattice seaneriog and iosieed imparity scattering, respectively. 81 78 CARRIER ACTION SEMICONDOCTO5I FONOAMENTAI.5 38 pa, far Respectively kttossu as tite elrctroa otobiliry and haIr ttiohility, are atwatys taken atid to be positine qoantittes. Note that, althongh electrons drift in the directinu opposite to the applied electric Iteld )e,, = pc,, I. tite cttrrent transported by negattiscly charged particles is itt torn rontitcr to the directisto of drtft 1 5 I. TIte net resttlt, as indicated in c/en ’, 5 )J 0 , Eq. (3.4b), is ao electron enrreut in the direction of the-applied electric held. — — 3.1.3 Mobility Mobihty is obniottslp a central paratneter in characterieittg electroit aitd Itole transport dne to drift. As farther readings will reveal, the carrier mobilities slsn play a key role in char ttctertctng the perforutatrce of natty denicen. Ii is reasonable therefore to enamine pa, and nag tu same detail to enhance oar geueral fatoiltarity with the paranteters and to establish a core of nscfnl information fer futnrc reference. lot N 101001 Standard Uttits: cola/v_sec. maintained at tarot tctepera FigurR 3.4 Measamd drift selactty of the cartters in altotp:ite silicon Canstracted frost the data fits and tite data tospec 5 ely tare an a latietion of the applied electric hrtd 0t and Sotitlt 01 al. in Jacabani at low electric holds, witile at To ho more prccise, electric fields e saturates and becomes independent ofT. high ftaaff — T 0 pa . . ta 57 f_[ Va w (3.3) t0 • n, praporttoe I far holes and w 2 for electrons itt silicon, pa ts the constant of where and T at low to moderate electric fields, and u,, ts the ltmtttng or sataro ality between limit ea ttt non eelociry approached at’vcry high electric holds. Obstoasly, to the higlt-held depeodeoce. in Eq. 132) is simply replaced by e, and Js55 does net eshtbtt an T-held suless spect the low-hold litttit, witich is of greatest practical ietemst and asosoted hereto yields hod otherwise, a = e’ nag for holes) and substitution iittO Eq. (3.2) 8 (No — —— Jr•ass = par nod system temperatare. to yrattering: The word ntabilirt’ in everyday asage refers ma &geoeral freedam of meoemeot. Analogoasly, in semicondnctar work ttte nobility parameter is a mea sare of the ease of carrier motion in a crystal. Increasiug the motion-itnpediog collisious withtn a crystal decreases the mobility of the carriers. In other words, dte carrier mabiliry varies inversely with the autoant of scattering taking place wititie the semiconductor. As visnalized in Pig. 3.1(b), the doetinant scattering mechanisms in noodegeocrately doped materials of device qaality are typically (i) lattice scattering involving collistant with ther inally agitated lattice atoms, and (ii) ionized itnpttrity (i.e., donor-site and/or acceptor-site) scattering. Relative to lattice scatterieg, it should be eutphasiced that it a the thermal vibra ian, the disptorrtneor of lattice atoms from their lattice positions, tlfat leads to carrier scattering. The internal held associafed with the stationary array of atoms in a reystal is already taken into accoaut in tlte effective Inass formatation. Although qaaotitative relationships connecting the mobility aud scattering can become qaite involved, it is readily established that pa = q(r)/in°, where )t-) is the mean free time between collisions and rite is the coudactivity effective mass. Sioch iscreasiug the namber of motion-impeding collisions decreases the mean free timd between collisions, sse again conclude pa varies iuversely wtth tlte amoaet of seatteriog.,However. pa is also noted to vary irverselyi with the carrier effective mass—tighter carriers mayo mare readily. The m’ in GaAs is siguihcantly smaller than the tnt in Si, theruby’esplaioing the higher mobility of the GaAs electrotts. Rnlatiamtahip ‘h —a 0 ‘4 s = Sasttple Ntttncrirol Volaro: pa., I 3h0 cot°! V-sec atid par = 4b0 cm°IV-see at 300 K in lOtS/emS and At 0 = lotS/cm 1 doped St. respectively, to nncontpeosated high-purity 0 N ) GaAs, the rooto-temperatore mobilities are pa, m h000 cm 5 lots/cm 0 nr N (N 0 / V-nec 5 to 400 cast/V_see. The qanted names are usefal for consparison pttrposes and when and performing order-of-toagnittide eonspt:ta:ious. Also note that pa, > pa, for both Si ar,d GaAs. In the major semicosdactors, pa, is cottsistently greater thatt pa for a gtveu doping —fl (3.4a) 4 ONrP’ Similarly, for electrons one obtains (3db) www.EasyEngineering.net 81 CARRIER AC7tON 5EMICONOaCTOR rUNDAMRN1’ALO 80 3.5 exhibits the observed doping dependence of the electron sod hole mohitities iu Si. Ge, and GaAs. All semicoodactars exhibit the same general dependence. Ar tow doping concentrations, below approximately lO 5 in Si, the caerier fcm t5 mobilities are essentially independent of the doping caoceotration. For dopings in excess lotS/canS, of the mabdities monatnnically decrease with increasing N . 0 0 or N With the aid of Fig. 3.b the explanation of the observed doping dependence is ruIn tivety straightforward. tavokiag an electrient analogy, one can associate a retistaoee to motion with each of the scattering mechanisms. These resistances are its series. At safh cieatly law doping levels, ionieed impurity scattering can be neglected compared to lattice m Rc. When lattice scattering, which is scattering, or in the analogy, RTovat = RL + net a function at N , becomes the dominant scattering mechanism, it aatomatically 0 0 or N follows that the carrier mobilities will be likewise independent of N . Far dapings 0 0 or N in eseens of —10 5 in Si, ionized imparity scattering and the attociated reststance to /cm t5 motion eon an longer be neglected. Increasing the snmber of scattering centers by adding more and more acceptors or donors progressively increases the am000t of ionized imparity’ scattering and systematically decresses the carrier mobilities. Doping Dependence: Figare — 111150 b g l tm Na orNu leoIs 0° 2 5 0 ‘°, a, gg 0 tab Hint’ ga s v-y last 357 1352 ‘da°a tO-a. ost 000 ass 055 . ‘ , a :**. toil too tots ‘*- tots 0 or V tcnr°’ N 1°) ww w.E asy Tenrtperotare Dependence: The tempcrntnrc dependence of the electron and hole mebili ties in Si n’ith doping as a parameter is displayed in Pig. 3.7. For dopings of N 0 or N w /cm, the data merge irta a single carve and there is a near power-law increase in the t4 10 carrier mabilities as the temperxmrr is decreased. Roaghly, pa, w T_asont and pa 2 w T’tt55t. For progressively higher dopiogs, the carrier mabitities still increase with de creasing temperotare, bat at a systematically decreasing rate. In fact, some N N 0 5 /cm tt tfi experimental data (not shown) exhibit a decreooe in pat as Tin deerensed below 200 K. The general tetaprratare dependence of the carrier mabilities is relatively easy to ex plain in the low doping limit. As noted in the doping dependence discassion, lattice scat tering is the dominant scattering mechanism (RTOTOL R) in lightly doped samples. Decreasing the system temperature castes an ever-decreasing thermal agitation of the semi En gin eer ing .ne candactar atoms, which in turn decreases the lattice scattering. The decreased scattering ) (b) hapedaror to motion doe to tathee scattering: : tmpedmce to mohan doe to ianiend tmpnnty scattering: —No doptog dependence. 0 or 1/5 —Inereaset with N —Deareasrs trith drcmaning T.’ —Inatrases ssith decreasing T. FlgurR 3.6 Electrieol analogy far scattering is a srtnteoodsetac R and N 1 represert the impedasar to motion doe to lattice seaneriog and iosieed imparity scattering, respectively. ir Ftaurn 3.5 Roano temneratam caorirr muobilitiei nsa funehan of thu dopant eoncestrat,oa (al St www.EasyEngineering.net t www.EasyEngineering.net 82 CARRIER SEMICONDUCTOR FUNDAMENTALS ww ACflON 83 roughly follows a sintple passer-law dependence. Being inversely proportional to the amount of lattice scattering, the mobility ot tightly doped samples is therefore expected to mcrease mitts decreasing temperature, varying roughly as the temperature to a negative power. The more complex dependence of 4w higher doped samples reflects the added effect of ionized itopurity scattering. In the elecaicsl analogy, R 1 can no longer be neglected. Moreover, whereas lattice scattering (RL) decreases with decreasing T, ionized impurity scattering (Ri) increases with decreasing T. Ionized iospstrities become more and more effective itt dellecting the charged carriers as the temperature and hence the speed of the carriers accreases. Thus ionized impurity scattering becomes a larger and larger percentage of the overgtl scatteriug as the teoslteratnrc is decreased (RTOT,sL —a Ri). Clearly, this enplains the decreased slope or the mobility versus temperature dependence exhibited by the higher doped saioples. w.E (C) Exercise 3.1 as y En gin e There exist surprisiogly accurate ‘empirical-fit’ relationships that are widely em ployed to compute the carrier mobitities at a given doping and temperature. Figures 3.5 and 3.7 were constructed using soch relatioovhips. The forns of a compatatiano] relatIonship is typically established on an empirical basis by noting the general func tional dependencies predicted theoretically and observed experimentally. Parameters In the relationship are than adjusted until on acceptable match is obtained to the best available experimental data. The majority carrier mobiltty secsas doping at room temperature is popularly computed from (a) eri ng. ne t 0 p 1 + (N/N,,) ÷ where a is the carrier mobility (san or tar), His the doping concentration (N,, or N ), 0 and all other quantities ace fit parameters. To model the inmperactsre dependence, one additionally employs T (K) A Figure 3,7 Trnsperaiare dnpendencn of (a) electron and IbI hole mobititim is silican for dapings ranging from l00/cmi to l0Ifciei. The curves were consiniried using lie empirical fit relation ships and parameters presented in Esercise 3.1. The dashed lion portion of the curves corresposd to a slighi evirosino of th, hi beyond the verified 200 K S T 5 500K range of validity. = ) A ( 0 o 3 A in the above equation represents 5.0,,,,, sH. N,, , or a; Asvo is the 300 K valor of the 5 parameter, T is temperature in Kelvin, and n is the temperature exponent. The fit parameters appropriate for Si are listed in the following table: www.EasyEngineering.net 84 CARRIER ACTION SEMICONDUCTOR FUNDAMENTALS Parameter Value at 300 K Holes Electrons The results obtained by runnisg the preceding program should be nomerically identical to Fig. 3.5(a). Temperature Evponrnt (ny) (b) Part (hI is left for the render to complete. ) 3 N,vr(cm 1.3 N 10” Hx10” .u,,,(cm 1 f 2 V-sec) (cm°/V-sec) 5 p a 2.4 92 54.3 —0.57 1268 406.9 —2.33 electrons —2.23 holes 0.91 0.88 —0.146 N,, or 0 for 10’°/cm t Pt (a) Construct a log-log plot of a and ia versus N,,, or N 0 N l0”icm’ using the quoted fit retatiooship aud the listed Si fit parameters. Compote your result with Fig. 3.5(a). 3.1.4 Resistivity Resistivity is an important material parameter that is closely related to carrier drift. Quali tatively, s-esistieiiy is a measure of a material’s inherent resistance to current flow—a “nor malized” resistance that does not depnd mi(hehysical dirneosidi(j of the material. Qaan titativety, resistivity (p) is defined as the proportionality constant between the electric field impressed across a homogeneous material and the total particle current per unit area flow ing in the material: that is, S = pJ (3.5a) Tar 500 K (b) Construct log-log plots of yo, versus T and yc versus T for 200 K 5 to 10°/cm . Compare your 3 0 or N 0 stepped in decade values from 10°/cm ond N results with Figs. 3.7(a) and 3.7(b), respectively. or St (a) MATLAB program srript. where a = l/p is the material conductivity. In a homogeneous material, established svith the aid of Eqs. (3.4), %Mohility versus Dopant Conceatration (Si,300K) %Fit Parameters NDref’t.3el7: NAref=2.35et7: /anmin’92; ,.upmin=5 .3: 4 un0 1268; pcpO 1 .fi: 6 O 4 as=0 91: apO.88 %ialobility Calcnlutioo NHogspace(14.19); 5.05 “poumin-r.oo0./(l +(N/NDrei).°un); . p); 5 p a 0 epmiu-t-yap0./(l+(NfNAref). %Plotting results close loglog(N,.an,N,pp); grid; axis([ l.0e14 I .0el9 l.Oel l.0e4]); xlabel(’NA or ND (cm-3)’); ytahel(Mobility (cm2IV-sec)’); text(l .0e15, l500,’Electrons’); texi( I On l5,500,’Hules’); text( 1 Oct 8,2000;Si,300K’); J jay = aS = -jays, + SOars, --S p = (3.5b) + sup)fl J = J,÷ and, as 3.6) It tbnrefore follows that I (3.7) + pep) In a nottdegenerate donor-doped senaconductor maintained in the extrinsic teiupera_ lure region where N 0 0 n 0 n. This result was established in No and p = n/N Ssbsecltos 2.5.5. Thus, for typical dopings and mobilitiev, pri + 5.up N in an 0 p n-type semiconductor. Similar arguments yield 5.a, n + pp pUN, in a p-type semicon ductor. Consequently, under conditions normally eucountered in Si samples maintained at or near room temperature, Eq. (3.7) simplifies to * = ——— ‘p . . . QNn] n-type semiconductor (3.fia) 85 www.EasyEngineering.net 82 CARRIER SEMICONDUCTOR FUNDAMENTALS ACflON 83 roughly follows a sintple passer-law dependence. Being inversely proportional to the amount of lattice scattering, the mobility ot tightly doped samples is therefore expected to mcrease mitts decreasing temperature, varying roughly as the temperature to a negative power. The more complex dependence of 4w higher doped samples reflects the added effect of ionized itopurity scattering. In the elecaicsl analogy, R 1 can no longer be neglected. Moreover, whereas lattice scattering (RL) decreases with decreasing T, ionized impurity scattering (Ri) increases with decreasing T. Ionized iospstrities become more and more effective itt dellecting the charged carriers as the temperature and hence the speed of the carriers accreases. Thus ionized impurity scattering becomes a larger and larger percentage of the overgtl scatteriug as the teoslteratnrc is decreased (RTOT,sL —a Ri). Clearly, this enplains the decreased slope or the mobility versus temperature dependence exhibited by the higher doped saioples. ww w.E a (C) Exercise 3.1 syE ngi There exist surprisiogly accurate ‘empirical-fit’ relationships that are widely em ployed to compute the carrier mobitities at a given doping and temperature. Figures 3.5 and 3.7 were constructed using soch relatioovhips. The forns of a compatatiano] relatIonship is typically established on an empirical basis by noting the general func tional dependencies predicted theoretically and observed experimentally. Parameters In the relationship are than adjusted until on acceptable match is obtained to the best available experimental data. The majority carrier mobiltty secsas doping at room temperature is popularly computed from (a) nee r p 0 ÷ 1 + (N/N,,) ing . net where a is the carrier mobility (san or tar), His the doping concentration (N,, or N ), 0 and all other quantities ace fit parameters. To model the inmperactsre dependence, one additionally employs T (K) A Figure 3,7 Trnsperaiare dnpendencn of (a) electron and IbI hole mobititim is silican for dapings ranging from l00/cmi to l0Ifciei. The curves were consiniried using lie empirical fit relation ships and parameters presented in Esercise 3.1. The dashed lion portion of the curves corresposd to a slighi evirosino of th, hi beyond the verified 200 K S T 5 500K range of validity. = ) A ( 0 o 3 A in the above equation represents 5.0,,,,, sH. N,, , or a; Asvo is the 300 K valor of the 5 parameter, T is temperature in Kelvin, and n is the temperature exponent. The fit parameters appropriate for Si are listed in the following table: www.EasyEngineering.net 84 CARRIER ACTION SEMICONDUCTOR FUNDAMENTALS Parameter Value at 300 K Holes Electrons The results obtained by runnisg the preceding program should be nomerically identical to Fig. 3.5(a). Temperature Evponrnt (ny) (b) Part (hI is left for the render to complete. ) 3 N,vr(cm 1.3 N 10” Hx10” .u,,,(cm 1 f 2 V-sec) (cm°/V-sec) 5 p a 2.4 92 54.3 —0.57 1268 406.9 —2.33 electrons —2.23 holes 0.91 0.88 —0.146 N,, or 0 for 10’°/cm t Pt (a) Construct a log-log plot of a and ia versus N,,, or N 0 N l0”icm’ using the quoted fit retatiooship aud the listed Si fit parameters. Compote your result with Fig. 3.5(a). 3.1.4 Resistivity Resistivity is an important material parameter that is closely related to carrier drift. Quali tatively, s-esistieiiy is a measure of a material’s inherent resistance to current flow—a “nor malized” resistance that does not depnd mi(hehysical dirneosidi(j of the material. Qaan titativety, resistivity (p) is defined as the proportionality constant between the electric field impressed across a homogeneous material and the total particle current per unit area flow ing in the material: that is, S = pJ (3.5a) Tar 500 K (b) Construct log-log plots of yo, versus T and yc versus T for 200 K 5 to 10°/cm . Compare your 3 0 or N 0 stepped in decade values from 10°/cm ond N results with Figs. 3.7(a) and 3.7(b), respectively. or St (a) MATLAB program srript. where a = l/p is the material conductivity. In a homogeneous material, established svith the aid of Eqs. (3.4), %Mohility versus Dopant Conceatration (Si,300K) %Fit Parameters NDref’t.3el7: NAref=2.35et7: /anmin’92; ,.upmin=5 .3: 4 un0 1268; pcpO 1 .fi: 6 O 4 as=0 91: apO.88 %ialobility Calcnlutioo NHogspace(14.19); 5.05 “poumin-r.oo0./(l +(N/NDrei).°un); . p); 5 p a 0 epmiu-t-yap0./(l+(NfNAref). %Plotting results close loglog(N,.an,N,pp); grid; axis([ l.0e14 I .0el9 l.Oel l.0e4]); xlabel(’NA or ND (cm-3)’); ytahel(Mobility (cm2IV-sec)’); text(l .0e15, l500,’Electrons’); texi( I On l5,500,’Hules’); text( 1 Oct 8,2000;Si,300K’); J jay = aS = -jays, + SOars, --S p = (3.5b) + sup)fl J = J,÷ and, as 3.6) It tbnrefore follows that I (3.7) + pep) In a nottdegenerate donor-doped senaconductor maintained in the extrinsic teiupera_ lure region where N 0 0 n 0 n. This result was established in No and p = n/N Ssbsecltos 2.5.5. Thus, for typical dopings and mobilitiev, pri + 5.up N in an 0 p n-type semiconductor. Similar arguments yield 5.a, n + pp pUN, in a p-type semicon ductor. Consequently, under conditions normally eucountered in Si samples maintained at or near room temperature, Eq. (3.7) simplifies to * = ——— ‘p . . . QNn] n-type semiconductor (3.fia) 85 82 CARRIER SEMICONDUCTOR FUNDAMENTALS ACflON 83 roughly follows a sintple passer-law dependence. Being inversely proportional to the amount of lattice scattering, the mobility ot tightly doped samples is therefore expected to mcrease mitts decreasing temperature, varying roughly as the temperature to a negative power. The more complex dependence of 4w higher doped samples reflects the added effect of ionized itopurity scattering. In the elecaicsl analogy, R 1 can no longer be neglected. Moreover, whereas lattice scattering (RL) decreases with decreasing T, ionized impurity scattering (Ri) increases with decreasing T. Ionized iospstrities become more and more effective itt dellecting the charged carriers as the temperature and hence the speed of the carriers accreases. Thus ionized impurity scattering becomes a larger and larger percentage of the overgtl scatteriug as the teoslteratnrc is decreased (RTOT,sL —a Ri). Clearly, this enplains the decreased slope or the mobility versus temperature dependence exhibited by the higher doped saioples. (C) Exercise 3.1 There exist surprisiogly accurate ‘empirical-fit’ relationships that are widely em ployed to compute the carrier mobitities at a given doping and temperature. Figures 3.5 and 3.7 were constructed using soch relatioovhips. The forns of a compatatiano] relatIonship is typically established on an empirical basis by noting the general func tional dependencies predicted theoretically and observed experimentally. Parameters In the relationship are than adjusted until on acceptable match is obtained to the best available experimental data. The majority carrier mobiltty secsas doping at room temperature is popularly computed from (a) 0 p 1 + (N/N,,) ÷ where a is the carrier mobility (san or tar), His the doping concentration (N,, or N ), 0 and all other quantities ace fit parameters. To model the inmperactsre dependence, one additionally employs T (K) A Figure 3,7 Trnsperaiare dnpendencn of (a) electron and IbI hole mobititim is silican for dapings ranging from l00/cmi to l0Ifciei. The curves were consiniried using lie empirical fit relation ships and parameters presented in Esercise 3.1. The dashed lion portion of the curves corresposd to a slighi evirosino of th, hi beyond the verified 200 K S T 5 500K range of validity. = ) A ( 0 o 3 A in the above equation represents 5.0,,,,, sH. N,, , or a; Asvo is the 300 K valor of the 5 parameter, T is temperature in Kelvin, and n is the temperature exponent. The fit parameters appropriate for Si are listed in the following table: www.EasyEngineering.net 84 CARRIER ACTION SEMICONDUCTOR FUNDAMENTALS Value at 300 K Holes Electrons Parameter The results obtained by runnisg the preceding program should be nomerically identical to Fig. 3.5(a). Temperature Evponrnt (ny) (b) Part (hI is left for the render to complete. 1.3 N 10” Hx10” ) 3 N,vr(cm .u,,,(cm 1 f 2 V-sec) (cm°/V-sec) 5 p ww w 92 54.3 —0.57 1268 406.9 —2.33 electrons —2.23 holes 0.88 0.91 a 2.4 3.1.4 Resistivity —0.146 N,, or 0 for 10’°/cm t Pt (a) Construct a log-log plot of a and ia versus N,,, or N 0 N l0”icm’ using the quoted fit retatiooship aud the listed Si fit parameters. Compote your result with Fig. 3.5(a). .Ea syE Tar 500 K (b) Construct log-log plots of yo, versus T and yc versus T for 200 K 5 to 10°/cm . Compare your 3 0 or N 0 stepped in decade values from 10°/cm ond N results with Figs. 3.7(a) and 3.7(b), respectively. ngi St (a) MATLAB program srript. nee rin g %ialobility Calcnlutioo NHogspace(14.19); 5.05 “poumin-r.oo0./(l +(N/NDrei).°un); . p); 5 p a 0 epmiu-t-yap0./(l+(NfNAref). S = pJ (3.5a) or J aS = --S p (3.5b) where a = l/p is the material conductivity. In a homogeneous material, established svith the aid of Eqs. (3.4), %Mohility versus Dopant Conceatration (Si,300K) %Fit Parameters NDref’t.3el7: NAref=2.35et7: /anmin’92; ,.upmin=5 .3: 4 un0 1268; pcpO 1 .fi: 6 O 4 as=0 91: apO.88 Resistivity is an important material parameter that is closely related to carrier drift. Quali tatively, s-esistieiiy is a measure of a material’s inherent resistance to current flow—a “nor malized” resistance that does not depnd mi(hehysical dirneosidi(j of the material. Qaan titativety, resistivity (p) is defined as the proportionality constant between the electric field impressed across a homogeneous material and the total particle current per unit area flow ing in the material: that is, jay .ne t %Plotting results close loglog(N,.an,N,pp); grid; axis([ l.0e14 I .0el9 l.Oel l.0e4]); xlabel(’NA or ND (cm-3)’); ytahel(Mobility (cm2IV-sec)’); text(l .0e15, l500,’Electrons’); texi( I On l5,500,’Hules’); text( 1 Oct 8,2000;Si,300K’); www.EasyEngineering.net = -jays, + SOars, = + sup)fl J = J,÷ and, as 3.6) It tbnrefore follows that I (3.7) + pep) In a nottdegenerate donor-doped senaconductor maintained in the extrinsic teiupera_ lure region where N 0 0 n 0 n. This result was established in No and p = n/N Ssbsecltos 2.5.5. Thus, for typical dopings and mobilitiev, pri + 5.up N in an 0 p n-type semiconductor. Similar arguments yield 5.a, n + pp pUN, in a p-type semicon ductor. Consequently, under conditions normally eucountered in Si samples maintained at or near room temperature, Eq. (3.7) simplifies to * = ——— ‘p . . . QNn] n-type semiconductor (3.fia) 85 82 CARRIER SEMICONDUCTOR FUNDAMENTALS ACflON 83 roughly follows a sintple passer-law dependence. Being inversely proportional to the amount of lattice scattering, the mobility ot tightly doped samples is therefore expected to mcrease mitts decreasing temperature, varying roughly as the temperature to a negative power. The more complex dependence of 4w higher doped samples reflects the added effect of ionized itopurity scattering. In the elecaicsl analogy, R 1 can no longer be neglected. Moreover, whereas lattice scattering (RL) decreases with decreasing T, ionized impurity scattering (Ri) increases with decreasing T. Ionized iospstrities become more and more effective itt dellecting the charged carriers as the temperature and hence the speed of the carriers accreases. Thus ionized impurity scattering becomes a larger and larger percentage of the overgtl scatteriug as the teoslteratnrc is decreased (RTOT,sL —a Ri). Clearly, this enplains the decreased slope or the mobility versus temperature dependence exhibited by the higher doped saioples. (C) Exercise 3.1 There exist surprisiogly accurate ‘empirical-fit’ relationships that are widely em ployed to compute the carrier mobitities at a given doping and temperature. Figures 3.5 and 3.7 were constructed using soch relatioovhips. The forns of a compatatiano] relatIonship is typically established on an empirical basis by noting the general func tional dependencies predicted theoretically and observed experimentally. Parameters In the relationship are than adjusted until on acceptable match is obtained to the best available experimental data. The majority carrier mobiltty secsas doping at room temperature is popularly computed from (a) 0 p 1 + (N/N,,) ÷ where a is the carrier mobility (san or tar), His the doping concentration (N,, or N ), 0 and all other quantities ace fit parameters. To model the inmperactsre dependence, one additionally employs T (K) A Figure 3,7 Trnsperaiare dnpendencn of (a) electron and IbI hole mobititim is silican for dapings ranging from l00/cmi to l0Ifciei. The curves were consiniried using lie empirical fit relation ships and parameters presented in Esercise 3.1. The dashed lion portion of the curves corresposd to a slighi evirosino of th, hi beyond the verified 200 K S T 5 500K range of validity. = ) A ( 0 o 3 A in the above equation represents 5.0,,,,, sH. N,, , or a; Asvo is the 300 K valor of the 5 parameter, T is temperature in Kelvin, and n is the temperature exponent. The fit parameters appropriate for Si are listed in the following table: www.EasyEngineering.net 84 Parameter 85 CARRIER ACTION SEMICONDUCTOR FUNDAMENTALS Value at 300 K Holes Electrons The results obtained by runnisg the preceding program should be nomerically identical to Fig. 3.5(a). Temperature Evponrnt (ny) (b) Part (hI is left for the render to complete. ) 3 N,vr(cm 1.3 N 10” Hx10” .u,,,(cm 1 f 2 V-sec) (cm°/V-sec) 5 p a 2.4 92 54.3 —0.57 1268 406.9 —2.33 electrons —2.23 holes 0.91 0.88 —0.146 N,, or 0 for 10’°/cm t Pt (a) Construct a log-log plot of a and ia versus N,,, or N 0 N l0”icm’ using the quoted fit retatiooship aud the listed Si fit parameters. Compote your result with Fig. 3.5(a). Tar 500 K (b) Construct log-log plots of yo, versus T and yc versus T for 200 K 5 to 10°/cm . Compare your 3 0 or N 0 stepped in decade values from 10°/cm ond N results with Figs. 3.7(a) and 3.7(b), respectively. St (a) MATLAB program srript. %Mohility versus Dopant Conceatration (Si,300K) %Fit Parameters NDref’t.3el7: NAref=2.35et7: /anmin’92; ,.upmin=5 .3: 4 un0 1268; pcpO 1 .fi: 6 O 4 as=0 91: apO.88 %ialobility Calcnlutioo NHogspace(14.19); 5.05 “poumin-r.oo0./(l +(N/NDrei).°un); . p); 5 p a 0 epmiu-t-yap0./(l+(NfNAref). %Plotting results close loglog(N,.an,N,pp); grid; axis([ l.0e14 I .0el9 l.Oel l.0e4]); xlabel(’NA or ND (cm-3)’); ytahel(Mobility (cm2IV-sec)’); text(l .0e15, l500,’Electrons’); texi( I On l5,500,’Hules’); text( 1 Oct 8,2000;Si,300K’); 3.1.4 Resistivity Resistivity is an important material parameter that is closely related to carrier drift. Quali tatively, s-esistieiiy is a measure of a material’s inherent resistance to current flow—a “nor malized” resistance that does not depnd mi(hehysical dirneosidi(j of the material. Qaan titativety, resistivity (p) is defined as the proportionality constant between the electric field impressed across a homogeneous material and the total particle current per unit area flow ing in the material: that is, ww w.E or S asy = pJ En J aS = (3.5a) --S p (3.5b) gin where a = l/p is the material conductivity. In a homogeneous material, established svith the aid of Eqs. (3.4), jay = -jays, + SOars, = It tbnrefore follows that eer + sup)fl I + pep) J = J,÷ and, as ing 3.6) .ne (3.7) In a nottdegenerate donor-doped senaconductor maintained in the extrinsic teiupera_ lure region where N 0 0 n 0 n. This result was established in No and p = n/N Ssbsecltos 2.5.5. Thus, for typical dopings and mobilitiev, pri + 5.up N in an 0 p n-type semiconductor. Similar arguments yield 5.a, n + pp pUN, in a p-type semicon ductor. Consequently, under conditions normally eucountered in Si samples maintained at or near room temperature, Eq. (3.7) simplifies to * = ——— ‘p . . . n-type semiconductor (3.fia) QNn] www.EasyEngineering.net t www.EasyEngineering.net 66 SEMICONDUCTOR FUNDAMENTALS CARRIER ACTiON _- ——j— .— T=300K —stype — - to’* mH ;;4i L 67 (j’. j ww to_I to—a w.E as y En gin e to—’ l t Na or Nelom” (a) °gt4 . . . tots 1 g at 1 g ai eri ng. ne t ...._!___ tt 10 Figure 3.8 (D) and = 1 g ti this Na at Figure 3.8 Resistivity mesas bryant 0 cost-aetraiias at 300 K in Ia) Si and Ib) otlrer semiconduc tors. )(b) Prirm Scouut, © 1901 by lairs Wiley & Sons, Inc. Reprinted with prrrsisstns.l p t tg p-type semicondoctor 13gb) L When consbined with ailtty-sersos-deplng data, hqs. (3.0) provide a one-ta-one carte spondertce between the resistivity, a directly measurable qaantity. and the doping inside a semiconductor In conjoectian ssith plots of p semns doprag (see Fig. 3.5), tire mrmared . 0 resistivity is in fact rontinety irsed to determine Na or N The memnred resistivity required in deterirnitring the doping can be obtaiaed in a nairs bet of diffewnt ways. A seemingly straightferssaed approach macId be to form the sendconductor into a bar, apply a bias V across contacts attached to the ends of the bar as in Fig. 3.1(a), measure the current I flowing in the circuit, aod thCn deduce from the meu p sneed resistance. (R(resistunee) = I’ll p1/A, where 1 is the bar length and A is the crosssectional area.) Unfortunately, the straightforward approach is deceptively diffirsir, is de stroetive (svmtes semicondsetor material), and is not readily adaptable to the wafets used in device processing. A measurement method finding widespread stage in practice is the four-point probe techniqoe. In the standard foar-point probe tnehniqne, four collinear, evenly spared probes, m shown in Fig. 3.9(a), are brought intu contact with the snrfaee of the semiconductor. A knawn enrrent I is passed throngh the aster twn probes, and the potential thereby devel V oped is meosnred across the inner two probes. The semieondactor resistivity is then com pnted from p = (3.0) 2waF where a is the probe-ta-probe sporing and T is a well-documented “rorrection” factor. The correction factor typically depends on the thickness of the sample and on whether the bot tom of the semiconductor is toaebing on insulator or a metal. Commercial instrnments urn www.EasyEngineering.net 58 neeteoNnaCnoe FANDA5IENTOL5 CARRIER ACTION 1°) avnilabie that nutomaticolly rompate the appropriate correction factor bmed on the sample rhirtsnms entered by the operator. Unlike the semirondactor-bm measurement, the fnar point probe techniqne is obviously easy to implement, causes only slight surface damage is the vicinity of the probe eantacts, and is ideatly salted for svorking with wafers. The sarface damage, although slight, does ecelnde fan technique from being osed on wafers intended for producing high-yield devices and ICs. A second technique worthy of note otilires a noncontorling eddy-rorrent approach. The schematic of a commercial eddy-cnrrent apparatus is pictured in Fig. 3.9(b). There are fringing fields near a ferrite core eceited with on RF coil, If a conducting material such as a samicosdnctor wafer is placed neat the ferrite core, the fringing fields cause locolieed (eddy) currents’ ro’hoss’ in the conducting material. The current flow is lnrn absorbs tome of the RF power. Tttc sheer resistivity of the condoeting material is dednced by monitoring the power consumption in a calibrated system. The ultrasonnd generators and receivers built into the commercial apparatas are for the is-sila delerstination of the svafer thickness. The change in phase of oltrasound bounced off the top and battom wafer serfacea permits the isstramnnt to compute the intercom spacing occupied by the safer. The sheet resistivity mnltiplied by the wafer thickness yields the wafer resistivity. 3.1.5 Band Bending Wafer lit previous encounters with the energy band diagram, svc have consistently draw’s E and to be energies independent of the pasition coordinate a. When an electric held (‘h) enists inside a material, the band energies become a inaction of position. The resnlting variation of E and N,. with position on the energy band diagram. exemplified by Fig. 3.10(a), is popularly referred to a.s “hand bending.” Seekiflg to establish the precise mlatinnahip between the electrir held within semi a conductor and the induced band bending, let as carefully re-enamine the energy band dto eeattt. The diagram itself, as emphasiced in Fig. 3.10(i), is a plot of the allowed electron energies within the semiconductor as a fonetinn of position, where E increasing npward in understood to be the eatnl energy of the electrons. Fnrthrrmorr, sve know from previnos diseossians that if an energy of precisely E is added to break an atom-atom bond, the created electron and hole energies would be N, and K,., respectivety, and the created earners would he effectively motionless. Absorbing on energy in caress of N , an the other hand, 0 weald in all probability give rise to an electron energy greater than E and a hole energy less than E,with both carriers moving around rapidly within the lattice. We are led, there fote, to interpret £ F, to be the kinetic energy (K.E.) of the eleetroas and N,. Eta be the kinetic energy of the helm [see Fig. 3.l0(b)l. Moreover, since the total energy eqnals the sam of the kinetic energy and the potential energy (F. F.), N, minus the energy reference level (E,,) mast equal the electroit potealial energy, us illustrated in Fig. 3.10(c). (Potential energy, it should be noted, is arbitrary to ssithin a constant, and the position-independent reference energy, E,,, may be chosen to be any convenient value.) The potential energy is the key in relating the electric held within a semiconduct or to positional variations in the energy bands. Specifically, asssming norntal operational con ditiors. where magnetic held, temperatttor gradient, and strms-indured effects are negli gible. only the forcr associated with an existing electric held can give rise to changes in the - RF generator (hI FigurE 3.9 Resistisity measawmeot tnetsniqsos. (a) Schematic drawing at the probe arrangomeot. placement, and biasieg is the fosr-point prabs measnrownet. (hI Schematic of a commercial eddyearnest apparatus thawing the RP tails and saRis components. lib) Prom Sclstodorttt, © 1990 by Jabs Wiley th Sans. lac. Reprinted with permissian.l — — 89 www.EasyEngineering.net 66 SEMICONDUCTOR FUNDAMENTALS CARRIER ACTiON _- ——j— .— T=300K —stype — - to’* mH ;;4i L 67 (j’. j to_I ww to—a w.E a to—’ °gt4 t tg syE ngi 1 g ti this tt 10 tots 1 g at 1 g ai Na at Figure 3.8 (D) l t Na or Nelom” ing . (a) Figure 3.8 Resistivity mesas bryant 0 cost-aetraiias at 300 K in Ia) Si and Ib) otlrer semiconduc tors. )(b) Prirm Scouut, © 1901 by lairs Wiley & Sons, Inc. Reprinted with prrrsisstns.l and p = ...._!___ . . . p-type semicondoctor 13gb) L When consbined with ailtty-sersos-deplng data, hqs. (3.0) provide a one-ta-one carte spondertce between the resistivity, a directly measurable qaantity. and the doping inside a semiconductor In conjoectian ssith plots of p semns doprag (see Fig. 3.5), tire mrmared . 0 resistivity is in fact rontinety irsed to determine Na or N The memnred resistivity required in deterirnitring the doping can be obtaiaed in a nairs bet of diffewnt ways. A seemingly straightferssaed approach macId be to form the sendconductor into a bar, apply a bias V across contacts attached to the ends of the bar as in nee r net Fig. 3.1(a), measure the current I flowing in the circuit, aod thCn deduce from the meu p sneed resistance. (R(resistunee) = I’ll p1/A, where 1 is the bar length and A is the crosssectional area.) Unfortunately, the straightforward approach is deceptively diffirsir, is de stroetive (svmtes semicondsetor material), and is not readily adaptable to the wafets used in device processing. A measurement method finding widespread stage in practice is the four-point probe techniqoe. In the standard foar-point probe tnehniqne, four collinear, evenly spared probes, m shown in Fig. 3.9(a), are brought intu contact with the snrfaee of the semiconductor. A knawn enrrent I is passed throngh the aster twn probes, and the potential thereby devel V oped is meosnred across the inner two probes. The semieondactor resistivity is then com pnted from p = (3.0) 2waF where a is the probe-ta-probe sporing and T is a well-documented “rorrection” factor. The correction factor typically depends on the thickness of the sample and on whether the bot tom of the semiconductor is toaebing on insulator or a metal. Commercial instrnments urn www.EasyEngineering.net 58 neeteoNnaCnoe FANDA5IENTOL5 CARRIER ACTION 1°) avnilabie that nutomaticolly rompate the appropriate correction factor bmed on the sample rhirtsnms entered by the operator. Unlike the semirondactor-bm measurement, the fnar point probe techniqne is obviously easy to implement, causes only slight surface damage is the vicinity of the probe eantacts, and is ideatly salted for svorking with wafers. The sarface damage, although slight, does ecelnde fan technique from being osed on wafers intended for producing high-yield devices and ICs. A second technique worthy of note otilires a noncontorling eddy-rorrent approach. The schematic of a commercial eddy-cnrrent apparatus is pictured in Fig. 3.9(b). There are fringing fields near a ferrite core eceited with on RF coil, If a conducting material such as a samicosdnctor wafer is placed neat the ferrite core, the fringing fields cause locolieed (eddy) currents’ ro’hoss’ in the conducting material. The current flow is lnrn absorbs tome of the RF power. Tttc sheer resistivity of the condoeting material is dednced by monitoring the power consumption in a calibrated system. The ultrasonnd generators and receivers built into the commercial apparatas are for the is-sila delerstination of the svafer thickness. The change in phase of oltrasound bounced off the top and battom wafer serfacea permits the isstramnnt to compute the intercom spacing occupied by the safer. The sheet resistivity mnltiplied by the wafer thickness yields the wafer resistivity. 3.1.5 Band Bending Wafer lit previous encounters with the energy band diagram, svc have consistently draw’s E and to be energies independent of the pasition coordinate a. When an electric held (‘h) enists inside a material, the band energies become a inaction of position. The resnlting variation of E and N,. with position on the energy band diagram. exemplified by Fig. 3.10(a), is popularly referred to a.s “hand bending.” Seekiflg to establish the precise mlatinnahip between the electrir held within semi a conductor and the induced band bending, let as carefully re-enamine the energy band dto eeattt. The diagram itself, as emphasiced in Fig. 3.10(i), is a plot of the allowed electron energies within the semiconductor as a fonetinn of position, where E increasing npward in understood to be the eatnl energy of the electrons. Fnrthrrmorr, sve know from previnos diseossians that if an energy of precisely E is added to break an atom-atom bond, the created electron and hole energies would be N, and K,., respectivety, and the created earners would he effectively motionless. Absorbing on energy in caress of N , an the other hand, 0 weald in all probability give rise to an electron energy greater than E and a hole energy less than E,with both carriers moving around rapidly within the lattice. We are led, there fote, to interpret £ F, to be the kinetic energy (K.E.) of the eleetroas and N,. Eta be the kinetic energy of the helm [see Fig. 3.l0(b)l. Moreover, since the total energy eqnals the sam of the kinetic energy and the potential energy (F. F.), N, minus the energy reference level (E,,) mast equal the electroit potealial energy, us illustrated in Fig. 3.10(c). (Potential energy, it should be noted, is arbitrary to ssithin a constant, and the position-independent reference energy, E,,, may be chosen to be any convenient value.) The potential energy is the key in relating the electric held within a semiconduct or to positional variations in the energy bands. Specifically, asssming norntal operational con ditiors. where magnetic held, temperatttor gradient, and strms-indured effects are negli gible. only the forcr associated with an existing electric held can give rise to changes in the - RF generator (hI FigurE 3.9 Resistisity measawmeot tnetsniqsos. (a) Schematic drawing at the probe arrangomeot. placement, and biasieg is the fosr-point prabs measnrownet. (hI Schematic of a commercial eddyearnest apparatus thawing the RP tails and saRis components. lib) Prom Sclstodorttt, © 1990 by Jabs Wiley th Sans. lac. Reprinted with permissian.l — — 89 66 SEMICONDUCTOR FUNDAMENTALS CARRIER ACTiON _- ——j— .— T=300K —stype — - to’* mH ;;4i L 67 (j’. j to_I to—a to—’ °gt4 t tg 1 g ti this tt 10 tots 1 g at 1 g ai Na at Figure 3.8 (D) l t Na or Nelom” (a) Figure 3.8 Resistivity mesas bryant 0 cost-aetraiias at 300 K in Ia) Si and Ib) otlrer semiconduc tors. )(b) Prirm Scouut, © 1901 by lairs Wiley & Sons, Inc. Reprinted with prrrsisstns.l and p = ...._!___ . . . p-type semicondoctor 13gb) L When consbined with ailtty-sersos-deplng data, hqs. (3.0) provide a one-ta-one carte spondertce between the resistivity, a directly measurable qaantity. and the doping inside a semiconductor In conjoectian ssith plots of p semns doprag (see Fig. 3.5), tire mrmared . 0 resistivity is in fact rontinety irsed to determine Na or N The memnred resistivity required in deterirnitring the doping can be obtaiaed in a nairs bet of diffewnt ways. A seemingly straightferssaed approach macId be to form the sendconductor into a bar, apply a bias V across contacts attached to the ends of the bar as in Fig. 3.1(a), measure the current I flowing in the circuit, aod thCn deduce from the meu p sneed resistance. (R(resistunee) = I’ll p1/A, where 1 is the bar length and A is the crosssectional area.) Unfortunately, the straightforward approach is deceptively diffirsir, is de stroetive (svmtes semicondsetor material), and is not readily adaptable to the wafets used in device processing. A measurement method finding widespread stage in practice is the four-point probe techniqoe. In the standard foar-point probe tnehniqne, four collinear, evenly spared probes, m shown in Fig. 3.9(a), are brought intu contact with the snrfaee of the semiconductor. A knawn enrrent I is passed throngh the aster twn probes, and the potential thereby devel V oped is meosnred across the inner two probes. The semieondactor resistivity is then com pnted from p = (3.0) 2waF where a is the probe-ta-probe sporing and T is a well-documented “rorrection” factor. The correction factor typically depends on the thickness of the sample and on whether the bot tom of the semiconductor is toaebing on insulator or a metal. Commercial instrnments urn www.EasyEngineering.net 58 neeteoNnaCnoe FANDA5IENTOL5 ww w CARRIER ACTION avnilabie that nutomaticolly rompate the appropriate correction factor bmed on the sample rhirtsnms entered by the operator. Unlike the semirondactor-bm measurement, the fnar point probe techniqne is obviously easy to implement, causes only slight surface damage is the vicinity of the probe eantacts, and is ideatly salted for svorking with wafers. The sarface damage, although slight, does ecelnde fan technique from being osed on wafers intended for producing high-yield devices and ICs. A second technique worthy of note otilires a noncontorling eddy-rorrent approach. The schematic of a commercial eddy-cnrrent apparatus is pictured in Fig. 3.9(b). There are fringing fields near a ferrite core eceited with on RF coil, If a conducting material such as a samicosdnctor wafer is placed neat the ferrite core, the fringing fields cause locolieed (eddy) currents’ ro’hoss’ in the conducting material. The current flow is lnrn absorbs tome of the RF power. Tttc sheer resistivity of the condoeting material is dednced by monitoring the power consumption in a calibrated system. The ultrasonnd generators and receivers built into the commercial apparatas are for the is-sila delerstination of the svafer thickness. The change in phase of oltrasound bounced off the top and battom wafer serfacea permits the isstramnnt to compute the intercom spacing occupied by the safer. The sheet resistivity mnltiplied by the wafer thickness yields the wafer resistivity. 1°) .Ea Wafer syE 3.1.5 Band Bending ngi nee rin g - .ne t RF lit previous encounters with the energy band diagram, svc have consistently draw’s E and to be energies independent of the pasition coordinate a. When an electric held (‘h) enists inside a material, the band energies become a inaction of position. The resnlting variation of E and N,. with position on the energy band diagram. exemplified by Fig. 3.10(a), is popularly referred to a.s “hand bending.” Seekiflg to establish the precise mlatinnahip between the electrir held within semi a conductor and the induced band bending, let as carefully re-enamine the energy band dto eeattt. The diagram itself, as emphasiced in Fig. 3.10(i), is a plot of the allowed electron energies within the semiconductor as a fonetinn of position, where E increasing npward in understood to be the eatnl energy of the electrons. Fnrthrrmorr, sve know from previnos diseossians that if an energy of precisely E is added to break an atom-atom bond, the created electron and hole energies would be N, and K,., respectivety, and the created earners would he effectively motionless. Absorbing on energy in caress of N , an the other hand, 0 weald in all probability give rise to an electron energy greater than E and a hole energy less than E,with both carriers moving around rapidly within the lattice. We are led, there fote, to interpret £ F, to be the kinetic energy (K.E.) of the eleetroas and N,. Eta be the kinetic energy of the helm [see Fig. 3.l0(b)l. Moreover, since the total energy eqnals the sam of the kinetic energy and the potential energy (F. F.), N, minus the energy reference level (E,,) mast equal the electroit potealial energy, us illustrated in Fig. 3.10(c). (Potential energy, it should be noted, is arbitrary to ssithin a constant, and the position-independent reference energy, E,,, may be chosen to be any convenient value.) The potential energy is the key in relating the electric held within a semiconduct or to positional variations in the energy bands. Specifically, asssming norntal operational con ditiors. where magnetic held, temperatttor gradient, and strms-indured effects are negli gible. only the forcr associated with an existing electric held can give rise to changes in the generator (hI FigurE 3.9 Resistisity measawmeot tnetsniqsos. (a) Schematic drawing at the probe arrangomeot. placement, and biasieg is the fosr-point prabs measnrownet. (hI Schematic of a commercial eddyearnest apparatus thawing the RP tails and saRis components. lib) Prom Sclstodorttt, © 1990 by Jabs Wiley th Sans. lac. Reprinted with permissian.l www.EasyEngineering.net — — 89 66 SEMICONDUCTOR FUNDAMENTALS CARRIER ACTiON _- ——j— .— T=300K —stype — - mH ;;4i L to’* 67 (j’. j to_I to—a to—’ °gt4 t tg 1 g ti this tots tt 10 1 g at 1 g ai Na at Figure 3.8 (D) l t Na or Nelom” (a) Figure 3.8 Resistivity mesas bryant 0 cost-aetraiias at 300 K in Ia) Si and Ib) otlrer semiconduc tors. )(b) Prirm Scouut, © 1901 by lairs Wiley & Sons, Inc. Reprinted with prrrsisstns.l and p = ...._!___ . . . p-type semicondoctor 13gb) L When consbined with ailtty-sersos-deplng data, hqs. (3.0) provide a one-ta-one carte spondertce between the resistivity, a directly measurable qaantity. and the doping inside a semiconductor In conjoectian ssith plots of p semns doprag (see Fig. 3.5), tire mrmared . 0 resistivity is in fact rontinety irsed to determine Na or N The memnred resistivity required in deterirnitring the doping can be obtaiaed in a nairs bet of diffewnt ways. A seemingly straightferssaed approach macId be to form the sendconductor into a bar, apply a bias V across contacts attached to the ends of the bar as in Fig. 3.1(a), measure the current I flowing in the circuit, aod thCn deduce from the meu p sneed resistance. (R(resistunee) = I’ll p1/A, where 1 is the bar length and A is the crosssectional area.) Unfortunately, the straightforward approach is deceptively diffirsir, is de stroetive (svmtes semicondsetor material), and is not readily adaptable to the wafets used in device processing. A measurement method finding widespread stage in practice is the four-point probe techniqoe. In the standard foar-point probe tnehniqne, four collinear, evenly spared probes, m shown in Fig. 3.9(a), are brought intu contact with the snrfaee of the semiconductor. A knawn enrrent I is passed throngh the aster twn probes, and the potential thereby devel V oped is meosnred across the inner two probes. The semieondactor resistivity is then com pnted from p = (3.0) 2waF where a is the probe-ta-probe sporing and T is a well-documented “rorrection” factor. The correction factor typically depends on the thickness of the sample and on whether the bot tom of the semiconductor is toaebing on insulator or a metal. Commercial instrnments urn www.EasyEngineering.net 58 neeteoNnaCnoe FANDA5IENTOL5 89 CARRIER ACTION 1°) avnilabie that nutomaticolly rompate the appropriate correction factor bmed on the sample rhirtsnms entered by the operator. Unlike the semirondactor-bm measurement, the fnar point probe techniqne is obviously easy to implement, causes only slight surface damage is the vicinity of the probe eantacts, and is ideatly salted for svorking with wafers. The sarface damage, although slight, does ecelnde fan technique from being osed on wafers intended for producing high-yield devices and ICs. A second technique worthy of note otilires a noncontorling eddy-rorrent approach. The schematic of a commercial eddy-cnrrent apparatus is pictured in Fig. 3.9(b). There are fringing fields near a ferrite core eceited with on RF coil, If a conducting material such as a samicosdnctor wafer is placed neat the ferrite core, the fringing fields cause locolieed (eddy) currents’ ro’hoss’ in the conducting material. The current flow is lnrn absorbs tome of the RF power. Tttc sheer resistivity of the condoeting material is dednced by monitoring the power consumption in a calibrated system. The ultrasonnd generators and receivers built into the commercial apparatas are for the is-sila delerstination of the svafer thickness. The change in phase of oltrasound bounced off the top and battom wafer serfacea permits the isstramnnt to compute the intercom spacing occupied by the safer. The sheet resistivity mnltiplied by the wafer thickness yields the wafer resistivity. ww w.E asy 3.1.5 Band Bending Wafer - RF generator (hI FigurE 3.9 Resistisity measawmeot tnetsniqsos. (a) Schematic drawing at the probe arrangomeot. placement, and biasieg is the fosr-point prabs measnrownet. (hI Schematic of a commercial eddyearnest apparatus thawing the RP tails and saRis components. lib) Prom Sclstodorttt, © 1990 by Jabs Wiley th Sans. lac. Reprinted with permissian.l En lit previous encounters with the energy band diagram, svc have consistently draw’s E and to be energies independent of the pasition coordinate a. When an electric held (‘h) enists inside a material, the band energies become a inaction of position. The resnlting variation of E and N,. with position on the energy band diagram. exemplified by Fig. 3.10(a), is popularly referred to a.s “hand bending.” Seekiflg to establish the precise mlatinnahip between the electrir held within semi a conductor and the induced band bending, let as carefully re-enamine the energy band dto eeattt. The diagram itself, as emphasiced in Fig. 3.10(i), is a plot of the allowed electron energies within the semiconductor as a fonetinn of position, where E increasing npward in understood to be the eatnl energy of the electrons. Fnrthrrmorr, sve know from previnos diseossians that if an energy of precisely E is added to break an atom-atom bond, the created electron and hole energies would be N, and K,., respectivety, and the created earners would he effectively motionless. Absorbing on energy in caress of N , an the other hand, 0 weald in all probability give rise to an electron energy greater than E and a hole energy less than E,with both carriers moving around rapidly within the lattice. We are led, there fote, to interpret £ F, to be the kinetic energy (K.E.) of the eleetroas and N,. Eta be the kinetic energy of the helm [see Fig. 3.l0(b)l. Moreover, since the total energy eqnals the sam of the kinetic energy and the potential energy (F. F.), N, minus the energy reference level (E,,) mast equal the electroit potealial energy, us illustrated in Fig. 3.10(c). (Potential energy, it should be noted, is arbitrary to ssithin a constant, and the position-independent reference energy, E,,, may be chosen to be any convenient value.) The potential energy is the key in relating the electric held within a semiconduct or to positional variations in the energy bands. Specifically, asssming norntal operational con ditiors. where magnetic held, temperatttor gradient, and strms-indured effects are negli gible. only the forcr associated with an existing electric held can give rise to changes in the gin eer ing .ne — — www.EasyEngineering.net t www.EasyEngineering.net 90 SEMICONDUCTOR FUNDAMENTALS CARRIER ACTION E (Total clectron energy) A 9l potential energy of the carriers. Elcutentary physics, s fact, tells us that the potential nt ergy of a 9 charged particle under such conditions is sitnply related to the electrostatic potential Vata given point by I — E FE. (a) V 9 — (3.10) Having previously concluded that FE. = E (3.11) — we can state ww ri Ev (bI V= —--(E, w.E (d) ) 1 IC, (3.12) By definition, moreover, as y En gin e = —vv (3.13) or. is one dimension. dv ‘if eri (3.14) Consequently, ng. ne I dE, t ( — L____ FIgure 3.10 Relationship betweeu hand bending and the electrostatic variables inside a sentruon dnctoe (a) sample energy band iograrn exhibiting band bending; (b) identification uf the carrier kinetic energies: (cI sperificatius of the electron potential energy: (dl electrostatic putentiat and (e) electric field sersus position dependence deduced From and associated with the part (al energy band diagram. L — sy dx, — I dE,. — 1 I dE (3.15) q The latter forms of Eq. (3.15) follow frotn die fact that E,. E,, and E 1 differ by only an additive constant. The preceding formulation provides a means of readily deducing the general form of the electrostatic variables associated with the “band bending” in Fig. 3.lO(a) and other energy bond diagrams. Making use of Eq. (3.12), or simply inverting E,(x) in Fig. 3.10(a), one obtains the V versus .e dependence presented in Fig. 3.10(d). [Please note that the electrostatic potential, like the poteetial energy, is arbitrary to within a constant—the Fig. 3.10(d) plot can be translated upward or downward ‘6long the voltage axis without modifying the physical situation inside the sensiconducl oLinally, recording the slope of E versus position, us dictated by Eq. (3.15), produces tIm ‘if versus x plot shown in Fig. 3.10(e). In summary, the reader should he usvare of the fact that the energy ba)itl diagram contains information relating to the electrostatic potential and electric field within the semi. conductor. Moreover, the general form of the V and ‘6 dependencies within the semi conductor cas be obtained almost by inspection. To deduce the form of the V versus x www.EasyEngineering.net 92 SEMICONDUCTOR FUNDAMENTALS ) versus x, 1 relationship, merely sketch the upside down” of E (or E or E tlte general ‘6 versus a dependence. simply note the slope of E, (or E, or E) of position. Exercise to CARRtERAaxrON determine as a function (b) The electrtc field,’if, is propnrtionul to tIne slope of the bands: 3.2 F; Consider the following energy band diagram. Take the semtrondnCtor represented 0 /4 at x 0 E ± Land E 0 IC to be Si maintained at 300 K with E, as the enesgy reference level and the identifi 0 /4 at x = 0. Note the choice of E 0 E cation of carriers at various points on the dtugram. —L — Er (c) For the electrons ICE. E E, and P.O. E E,at = E total energy uf the holes EF. Since the increases downward on the diagram, K.E = E, FE. E,, E and E,. E E, for the holes. The energy differences are of course evaluated at the same a. The deduced K.E. and P.O. “alum are summarized in following table: the — — — — — Er eriK.E(eV)jpE(eV) Electron I I I H -L 0 L 0 ‘—“x 0.28 (a) Skelctt the electrostatic potential (V) inside the semiconductor usa functiou of .v. (b) Sketch the electric field (‘6) inside the semiconductor as a fauctton of x. 2 tf : it (c) Ascertain the K.E. and FE. of the electrons and holes pictured un the diagram. (d) Determine the resistivity of then> L portion of the semiconductor. St (a) The V vccscs a relationship mast have the same functional form as the “upside down” of E, (or IC 1 or E,). If the arbitrary voltage reference point ts taken to be V Oat x = L, then one concludes the V versus x dependence is as sketched here. (d) lathe a> Lregiun, E, —_ p — — E (0 Er),cr From Fig. .3 5(a) one dedacesp E/4 = 0.28eV and = lO’° 20tt0 c° 2 = 4.96 x 10 3 /rm 14 459 cma/V-sec, and therefore. h qi.uN,,m -cnr (1.6 X 10- 5)(459)(49fi 5< 10i) Alternatively making use of the Fig. 3.8(o) Si resistivityplo t, one similarly concludes p 25 ohm-etc. 93 www.EasyEngineering.net 90 SEMICONDUCTOR FUNDAMENTALS CARRIER ACTION E (Total clectron energy) A 9l potential energy of the carriers. Elcutentary physics, s fact, tells us that the potential nt ergy of a 9 charged particle under such conditions is sitnply related to the electrostatic potential Vata given point by I — E FE. (a) V 9 — (3.10) Having previously concluded that FE. = E (3.11) — we can state Ev ww (bI ri w.E a V= —--(E, — L____ ) 1 IC, (3.12) By definition, moreover, or. is one dimension. syE ngi = —vv dv ‘if Consequently, I dE, (d) L ( FIgure 3.10 Relationship betweeu hand bending and the electrostatic variables inside a sentruon dnctoe (a) sample energy band iograrn exhibiting band bending; (b) identification uf the carrier kinetic energies: (cI sperificatius of the electron potential energy: (dl electrostatic putentiat and (e) electric field sersus position dependence deduced From and associated with the part (al energy band diagram. — sy dx, (3.13) — I dE,. — nee r 1 I dE q (3.14) ing . (3.15) net The latter forms of Eq. (3.15) follow frotn die fact that E,. E,, and E 1 differ by only an additive constant. The preceding formulation provides a means of readily deducing the general form of the electrostatic variables associated with the “band bending” in Fig. 3.lO(a) and other energy bond diagrams. Making use of Eq. (3.12), or simply inverting E,(x) in Fig. 3.10(a), one obtains the V versus .e dependence presented in Fig. 3.10(d). [Please note that the electrostatic potential, like the poteetial energy, is arbitrary to within a constant—the Fig. 3.10(d) plot can be translated upward or downward ‘6long the voltage axis without modifying the physical situation inside the sensiconducl oLinally, recording the slope of E versus position, us dictated by Eq. (3.15), produces tIm ‘if versus x plot shown in Fig. 3.10(e). In summary, the reader should he usvare of the fact that the energy ba)itl diagram contains information relating to the electrostatic potential and electric field within the semi. conductor. Moreover, the general form of the V and ‘6 dependencies within the semi conductor cas be obtained almost by inspection. To deduce the form of the V versus x www.EasyEngineering.net 92 SEMICONDUCTOR FUNDAMENTALS ) versus x, 1 relationship, merely sketch the upside down” of E (or E or E tlte general ‘6 versus a dependence. simply note the slope of E, (or E, or E) of position. Exercise to CARRtERAaxrON determine as a function (b) The electrtc field,’if, is propnrtionul to tIne slope of the bands: 3.2 F; Consider the following energy band diagram. Take the semtrondnCtor represented 0 /4 at x 0 E ± Land E 0 IC to be Si maintained at 300 K with E, as the enesgy reference level and the identifi 0 /4 at x = 0. Note the choice of E 0 E cation of carriers at various points on the dtugram. —L — Er (c) For the electrons ICE. E E, and P.O. E E,at = E total energy uf the holes EF. Since the increases downward on the diagram, K.E = E, FE. E,, E and E,. E E, for the holes. The energy differences are of course evaluated at the same a. The deduced K.E. and P.O. “alum are summarized in following table: the — — — — — Er eriK.E(eV)jpE(eV) Electron I I I H -L 0 L 0 ‘—“x 0.28 (a) Skelctt the electrostatic potential (V) inside the semiconductor usa functiou of .v. (b) Sketch the electric field (‘6) inside the semiconductor as a fauctton of x. 2 tf : it (c) Ascertain the K.E. and FE. of the electrons and holes pictured un the diagram. (d) Determine the resistivity of then> L portion of the semiconductor. St (a) The V vccscs a relationship mast have the same functional form as the “upside down” of E, (or IC 1 or E,). If the arbitrary voltage reference point ts taken to be V Oat x = L, then one concludes the V versus x dependence is as sketched here. (d) lathe a> Lregiun, E, —_ p — — E (0 Er),cr From Fig. .3 5(a) one dedacesp E/4 = 0.28eV and = lO’° 20tt0 c° 2 = 4.96 x 10 3 /rm 14 459 cma/V-sec, and therefore. h qi.uN,,m -cnr (1.6 X 10- 5)(459)(49fi 5< 10i) Alternatively making use of the Fig. 3.8(o) Si resistivityplo t, one similarly concludes p 25 ohm-etc. 93 90 SEMICONDUCTOR FUNDAMENTALS CARRIER ACTION E (Total clectron energy) A 9l potential energy of the carriers. Elcutentary physics, s fact, tells us that the potential nt ergy of a 9 charged particle under such conditions is sitnply related to the electrostatic potential Vata given point by I — E FE. (a) V 9 — (3.10) Having previously concluded that FE. = E (3.11) — we can state ri Ev (bI V= —--(E, — L____ ) 1 IC, (3.12) By definition, moreover, = —vv (3.13) or. is one dimension. dv ‘if (3.14) Consequently, I dE, (d) L ( FIgure 3.10 Relationship betweeu hand bending and the electrostatic variables inside a sentruon dnctoe (a) sample energy band iograrn exhibiting band bending; (b) identification uf the carrier kinetic energies: (cI sperificatius of the electron potential energy: (dl electrostatic putentiat and (e) electric field sersus position dependence deduced From and associated with the part (al energy band diagram. — sy dx, — I dE,. — 1 I dE (3.15) q The latter forms of Eq. (3.15) follow frotn die fact that E,. E,, and E 1 differ by only an additive constant. The preceding formulation provides a means of readily deducing the general form of the electrostatic variables associated with the “band bending” in Fig. 3.lO(a) and other energy bond diagrams. Making use of Eq. (3.12), or simply inverting E,(x) in Fig. 3.10(a), one obtains the V versus .e dependence presented in Fig. 3.10(d). [Please note that the electrostatic potential, like the poteetial energy, is arbitrary to within a constant—the Fig. 3.10(d) plot can be translated upward or downward ‘6long the voltage axis without modifying the physical situation inside the sensiconducl oLinally, recording the slope of E versus position, us dictated by Eq. (3.15), produces tIm ‘if versus x plot shown in Fig. 3.10(e). In summary, the reader should he usvare of the fact that the energy ba)itl diagram contains information relating to the electrostatic potential and electric field within the semi. conductor. Moreover, the general form of the V and ‘6 dependencies within the semi conductor cas be obtained almost by inspection. To deduce the form of the V versus x www.EasyEngineering.net 92 SEMICONDUCTOR FUNDAMENTALS ) versus x, 1 relationship, merely sketch the upside down” of E (or E or E tlte general ‘6 versus a dependence. simply note the slope of E, (or E, or E) of position. Exercise to CARRtERAaxrON determine as a function (b) The electrtc field,’if, is propnrtionul to tIne slope of the bands: 3.2 F; Consider the following energy band diagram. Take the semtrondnCtor represented 0 /4 at x 0 E ± Land E 0 IC to be Si maintained at 300 K with E, as the enesgy reference level and the identifi 0 /4 at x = 0. Note the choice of E 0 E cation of carriers at various points on the dtugram. —L — ww w .Ea (c) For the electrons ICE. E E, and P.O. E E,at = E total energy uf the holes EF. Since the increases downward on the diagram, K.E = E, FE. E,, E and E,. E E, for the holes. The energy differences are of course evaluated at the same a. The deduced K.E. and P.O. “alum are summarized in following table: the Er — — — — — syE Er ngi I I -L 0 H L eriK.E(eV)jpE(eV) nee rin g Electron I 0 ‘—“x 0.28 (a) Skelctt the electrostatic potential (V) inside the semiconductor usa functiou of .v. .ne t (b) Sketch the electric field (‘6) inside the semiconductor as a fauctton of x. 2 tf : it (c) Ascertain the K.E. and FE. of the electrons and holes pictured un the diagram. (d) Determine the resistivity of then> L portion of the semiconductor. St (a) The V vccscs a relationship mast have the same functional form as the “upside down” of E, (or IC 1 or E,). If the arbitrary voltage reference point ts taken to be V Oat x = L, then one concludes the V versus x dependence is as sketched here. (d) lathe a> Lregiun, E, —_ p — — E (0 Er),cr From Fig. .3 5(a) one dedacesp E/4 = 0.28eV and = lO’° 20tt0 c° 2 = 4.96 x 10 3 /rm 14 459 cma/V-sec, and therefore. h qi.uN,,m -cnr (1.6 X 10- 5)(459)(49fi 5< 10i) Alternatively making use of the Fig. 3.8(o) Si resistivityplo t, one similarly concludes p 25 ohm-etc. www.EasyEngineering.net 93 90 SEMICONDUCTOR FUNDAMENTALS CARRIER ACTION E (Total clectron energy) A 9l potential energy of the carriers. Elcutentary physics, s fact, tells us that the potential nt ergy of a 9 charged particle under such conditions is sitnply related to the electrostatic potential Vata given point by I — E FE. (a) V 9 — (3.10) Having previously concluded that FE. E = (3.11) — we can state ri Ev (bI V= —--(E, — L____ ) 1 IC, (3.12) By definition, moreover, —vv = (3.13) or. is one dimension. dv ‘if (3.14) Consequently, I dE, (d) L ( FIgure 3.10 Relationship betweeu hand bending and the electrostatic variables inside a sentruon dnctoe (a) sample energy band iograrn exhibiting band bending; (b) identification uf the carrier kinetic energies: (cI sperificatius of the electron potential energy: (dl electrostatic putentiat and (e) electric field sersus position dependence deduced From and associated with the part (al energy band diagram. sy — dx, I dE,. — — 1 I dE (3.15) q The latter forms of Eq. (3.15) follow frotn die fact that E,. E,, and E 1 differ by only an additive constant. The preceding formulation provides a means of readily deducing the general form of the electrostatic variables associated with the “band bending” in Fig. 3.lO(a) and other energy bond diagrams. Making use of Eq. (3.12), or simply inverting E,(x) in Fig. 3.10(a), one obtains the V versus .e dependence presented in Fig. 3.10(d). [Please note that the electrostatic potential, like the poteetial energy, is arbitrary to within a constant—the Fig. 3.10(d) plot can be translated upward or downward ‘6long the voltage axis without modifying the physical situation inside the sensiconducl oLinally, recording the slope of E versus position, us dictated by Eq. (3.15), produces tIm ‘if versus x plot shown in Fig. 3.10(e). In summary, the reader should he usvare of the fact that the energy ba)itl diagram contains information relating to the electrostatic potential and electric field within the semi. conductor. Moreover, the general form of the V and ‘6 dependencies within the semi conductor cas be obtained almost by inspection. To deduce the form of the V versus x www.EasyEngineering.net 92 SEMICONDUCTOR FUNDAMENTALS ) versus x, 1 relationship, merely sketch the upside down” of E (or E or E tlte general ‘6 versus a dependence. simply note the slope of E, (or E, or E) of position. Exercise to CARRtERAaxrON determine as a function (b) The electrtc field,’if, is propnrtionul to tIne slope of the bands: 3.2 F; Consider the following energy band diagram. Take the semtrondnCtor represented 0 /4 at x 0 E ± Land E 0 IC to be Si maintained at 300 K with E, as the enesgy reference level and the identifi 0 /4 at x = 0. Note the choice of E 0 E cation of carriers at various points on the dtugram. —L — Er Er ww w.E (c) For the electrons ICE. E E, and P.O. E E,at = E total energy uf the holes EF. Since the increases downward on the diagram, K.E = E, FE. E,, E and E,. E E, for the holes. The energy differences are of course evaluated at the same a. The deduced K.E. and P.O. “alum are summarized in following table: the — — — — asy — En eriK.E(eV)jpE(eV) Electron I I I H -L 0 L ‘—“x (a) Skelctt the electrostatic potential (V) inside the semiconductor usa functiou of .v. (b) Sketch the electric field (‘6) inside the semiconductor as a fauctton of x. gin 0 0.28 eer 2 tf : it (c) Ascertain the K.E. and FE. of the electrons and holes pictured un the diagram. ing (d) Determine the resistivity of then> L portion of the semiconductor. St (a) The V vccscs a relationship mast have the same functional form as the “upside down” of E, (or IC 1 or E,). If the arbitrary voltage reference point ts taken to be V Oat x = L, then one concludes the V versus x dependence is as sketched here. (d) lathe a> Lregiun, E, —_ p — — E (0 Er),cr From Fig. .3 5(a) one dedacesp .ne E/4 = 0.28eV and = lO’° 20tt0 c° 2 = 4.96 x 10 3 /rm 14 459 cma/V-sec, and therefore. h qi.uN,,m -cnr (1.6 X 10- 5)(459)(49fi 5< 10i) Alternatively making use of the Fig. 3.8(o) Si resistivityplo t, one similarly concludes p 25 ohm-etc. www.EasyEngineering.net t 93 _______ www.EasyEngineering.net 94 SEMICONDUCTOR FUNDAMENTALS CARRIER ACTION 3.2 DIFFUSION 1024 ,, : 3.2.1 Definition—Visualization 5 a OC55 whereby particles cod to spread oat or redistribute as a resolt of their iaudom thermal marion. migrathsg on a macroscopic scale front regions of high partIcle colscentratiOs into regions 0 f low particle cencenrration. if allnsved so progress snabated, the diffosion process operates so as so prodtlce a asiforre distribstiau of particles. The diffssirsg entity, is stsoald be noted, reed 1101 be charged; thermal motion, tot inrerparttcle repalsioo, is the enabling action behind the diffasian process. DIffusion tra Li 512 To cite an everyday esample of diffUsion, ssppnse aIr apes bottle of perfame is ptaced in one corner of a room. Escn in the absence of air esereels, randons tlrerroal esotins wf I spread tire perfume molecales thcoaghaot the rosIn ill a rclalivety sirort period of nbc, with intermolecular collisions helping to uniformly redisrribsre the peefarne to esery nook and cearrny within the roamo. Seeking to obtain a more detailed anderstasding of the diffnsion process, let us nest conceptsally “monitor” the process on d osicroscopie scale employing a simple hypotheti cal system. The system we propose tm monitor is a one-dimesrsiosal hex centainrng four cotepartmemsts and 1024 mobile particles (see Fig. 3.11). The particles within the hon obey certain stringent mles. Specificalty, thermal motion canoes all particles in a gisro compart melts to “jump” isle an adjacetsr cempartnnertr eset’y e seconds. In keeping wish the randmss nasare of the motion, each and every particle has an eqcal probability ofjsnsping to the left nod to the right. Hitting an “esternal wall” while attempting to jarssp to the left or right reflects the pursrele back so its pre-Jnmp posItion. Ftnally, nI rinse s = 0 st is assumed that all of the particles are confined in the lefs-moss compaetnserst. Pigore 3.11 records she esolnlsoms of one 1024 parricle system as n fsnction of time. As time I T, 512 ef the 1024 particles originally in compartment 1 jamp to the riglts and come sorest in compartmens 2. The remaining 512 particles jump so the left and are re flected back into the left-moss compartment. The end result is 512 parnicles each In com partments I and 2 after e seconds. As time I = 2e, 256 of the particles in compartment 2 jamp into comsmpartmens 3 and the remainder jump back into compartment 1. In the mcmlrime, 256 of the particles from compartrssemms I jamp into compartmens 2 and 256 nndergo a reflection at the left-Isand wall. The ncr resuls after 2e seconds is 512 parsicles in com partment I and 256 particles each is oompartmenss 2 and 3. TIse stare of she system after 3e and be seconds, also shosvn in Pip. 3.11, can be dedaced in a similar manner. By 5 = fiT, the particles. once confined to she lrfs-moss compartmens, have become utnross aniformly distribosed shrouglsoot she hon. and it it nnnecessary to consider later states. Indeed, she fnndamensal nature of the diffnsion process is clearly self-evident frosn an enamsnasion of the enisssng states. In semicondactors she diffusion precens on a micrnscopie scale in similar so thaI oc currsng in the hyposhcsical system esecps, of coUrse, she mndom morion of the diffusing parsicles is three-dimensional arid nor “comparsmentalieed.” On n macroscopic scale she net effecs of diffusion is precisely she same witlnin both the hypothetical system and semi- ww 95 eri ng. ne t aso 52e w.E as y En gin e ass 384 354 I san r5e 255 am 52 s6e Figure 3.11 PuPation usa microsenpio scale in a hypnthetirat ann-dimensional system. The nnm bees once the arrows iodicaso shn number of partirlnu in a given oosnpaetmons; abseesusion simm me listed so the nssreme eight conductors; there is an cnu I3L]P(mti0n of parttcles from ceurrutton so”9i0iiso law parttcle concentratIon Wtthsn semscondnctnru sheiG]s Ic par tihlks.Ethe electrons and holes—are charged, and diffnsion-celuted carrier transport therefore given rise to particle currents us pictured in Fig. 3.12. narrate —S S see sees Figure 112 181 oliruse —0 0 see sees , Vssualimtian of eloetenu and hole diffusion non mnrensrnpio teals. www.EasyEngineering.net 96 CARRIEu1 ACTiON 5EMtCONDUCTOR FSNnA5IENTALn (c) Ecperimnnr with initially placing pursmcles in mom than one hoc and changing she number in the pnsruo statements. You msght also Iry inceeming the namber of par (C) Exercise 3.3 The “DiffOemo” MAmAS file listed below was svrissen to help she user nrsualrze the diffusion process. The program provider n psendo-ansmasron of u ouo-dmmenssOnnl particle system similar so than described in the rent. The y 11 statement tu the program controls the initial condition, N specifies the masimum namber of moni tored “jnmps,” and she nnmber in the pause statements controls the time between jumps. tick hones. Sm Sample outpnt is reprodnced in Pig. E3.3. 12 5 dO I I 12 I , 0 I I I 511 to %Simulation of Diffusion (DifiDemo) %One-dimensional system, right and left jumps eqoally probable %Inisiahiaat ion close n=40.5 1.5 2.5 3.5 4.5]; y=[l .Oeb 0000]; %NOTE: initial pouitinn can bn changed [np.yp] =barcy]; islot(np,yp]; tens (0.5.1 .leb,’s = 0’); onis([tJ,S,0,l .2c6)]; pause (0.5) %NOTE: increase N foe ousended run N= 15; %Cnsnpusaninns and Plorsing for dt:N, %l2iffasion step calcalution bin(l]eodnd(y(1)/2 + y(2)/ ]; 2 hin(2)Honnd(y(l]12 + y(3]/ ); 2 bin(3)ronnd(y(2]/2 + 2 ]; 4 y( ) / + bin(4)raand(y(3)/2 ); 2 y(5)J ); 2 biu(5]roand(y(4]/2 + y(5)/ ybin; IhPlbning the resalt [vp,yp] bar(n.y); 0. 4 5 Figure 63.3 m[Th ered here because it simalsaneoosly ptovidm as isformasise eucmple of the diffusion ,nsm2ssr(fi]]]; (b) Rerun she program after changing the mmml conditions so thus all of she carriers = 23 3.2.2 Hot-Point Probe Measurement Pr (a) Enter she program inro yotur compnter or locate the copy supplsed on dssk. Run the piograns. (The csotresnrd-pcriod on a Macintosh compnter or break on an IBM corepasible compnser can ho ased so premararely terminate the program.) are in the middle box ass ‘1 1 Before establishing the carrent associated with diffasion, let us digress somewhat nod briefly consider the hot-poins probe measnremcns. The hot-point probe mcuanremene is common lcchssiqce for napiØly determining whether a semiconductor is s- or p-type. Prom a practical standpoint, knowledge of the semicondncror type is essential in device process Ing and moss be known even before determining the doping concentration fronr resisnisiry meannremennn (refer back to Fig. 3.8). The hot-point probe “typing” experiment is consid aniu(axis); plot)xp.yp]; sest(O.S, I. leb,l ‘5 eb]]; 2 anis((0,5.0,l. pause (0.5] end 4[. process. Examining Pig. 3.13(n), we find the only egaipment required for performing the hot point probe nrensureteent is u hot-point probe, a cold-poinn probe, nod a censee-cero mil lmammeter. The hot-point probe is sonmetimes a rebsgee from a wood burning set or simply a soldering irou: the csld-poinl probe sypically assumes the form of an electrical probe like than used with hand-held malsimeters. No special reqauremenu are imposed on the centar oem muhliacsmetec connecsed beswcen the probes. TIme nmnasnmment procedure itself is also extremely simple: After nllowsng the hot probe to heat np, one brings the two probes into contact with the semicondactor sample. nod the onnosener defleens so the right or left, rhereby indicating she semiconductor type. Observe thus nbc spacing benween the probes in set arbitrarily and can be redaced to enhance she ammeter deflection. A simplified explunation of how Ihe hot-point probe meu.sncement works is presented tn Fig. 3.13(b). In she vicinily of nbc probe coctact the heated probe creates an increased 97 _______ www.EasyEngineering.net 94 SEMICONDUCTOR FUNDAMENTALS CARRIER ACTION 3.2 DIFFUSION 95 1024 ,, : 3.2.1 Definition—Visualization 5 a OC55 whereby particles cod to spread oat or redistribute as a resolt of their iaudom thermal marion. migrathsg on a macroscopic scale front regions of high partIcle colscentratiOs into regions 0 f low particle cencenrration. if allnsved so progress snabated, the diffosion process operates so as so prodtlce a asiforre distribstiau of particles. The diffssirsg entity, is stsoald be noted, reed 1101 be charged; thermal motion, tot inrerparttcle repalsioo, is the enabling action behind the diffasian process. DIffusion tra Li 512 To cite an everyday esample of diffUsion, ssppnse aIr apes bottle of perfame is ptaced in one corner of a room. Escn in the absence of air esereels, randons tlrerroal esotins wf I spread tire perfume molecales thcoaghaot the rosIn ill a rclalivety sirort period of nbc, with intermolecular collisions helping to uniformly redisrribsre the peefarne to esery nook and cearrny within the roamo. Seeking to obtain a more detailed anderstasding of the diffnsion process, let us nest conceptsally “monitor” the process on d osicroscopie scale employing a simple hypotheti cal system. The system we propose tm monitor is a one-dimesrsiosal hex centainrng four cotepartmemsts and 1024 mobile particles (see Fig. 3.11). The particles within the hon obey certain stringent mles. Specificalty, thermal motion canoes all particles in a gisro compart melts to “jump” isle an adjacetsr cempartnnertr eset’y e seconds. In keeping wish the randmss nasare of the motion, each and every particle has an eqcal probability ofjsnsping to the left nod to the right. Hitting an “esternal wall” while attempting to jarssp to the left or right reflects the pursrele back so its pre-Jnmp posItion. Ftnally, nI rinse s = 0 st is assumed that all of the particles are confined in the lefs-moss compaetnserst. Pigore 3.11 records she esolnlsoms of one 1024 parricle system as n fsnction of time. As time I T, 512 ef the 1024 particles originally in compartment 1 jamp to the riglts and come sorest in compartmens 2. The remaining 512 particles jump so the left and are re flected back into the left-moss compartment. The end result is 512 parnicles each In com partments I and 2 after e seconds. As time I = 2e, 256 of the particles in compartment 2 jamp into comsmpartmens 3 and the remainder jump back into compartment 1. In the mcmlrime, 256 of the particles from compartrssemms I jamp into compartmens 2 and 256 nndergo a reflection at the left-Isand wall. The ncr resuls after 2e seconds is 512 parsicles in com partment I and 256 particles each is oompartmenss 2 and 3. TIse stare of she system after 3e and be seconds, also shosvn in Pip. 3.11, can be dedaced in a similar manner. By 5 = fiT, the particles. once confined to she lrfs-moss compartmens, have become utnross aniformly distribosed shrouglsoot she hon. and it it nnnecessary to consider later states. Indeed, she fnndamensal nature of the diffnsion process is clearly self-evident frosn an enamsnasion of the enisssng states. In semicondactors she diffusion precens on a micrnscopie scale in similar so thaI oc currsng in the hyposhcsical system esecps, of coUrse, she mndom morion of the diffusing parsicles is three-dimensional arid nor “comparsmentalieed.” On n macroscopic scale she net effecs of diffusion is precisely she same witlnin both the hypothetical system and semi- ww ass aso 52e w.E a 384 354 I r5e syE ngi san 255 am 52 nee r s6e Figure 3.11 PuPation usa microsenpio scale in a hypnthetirat ann-dimensional system. The nnm bees once the arrows iodicaso shn number of partirlnu in a given oosnpaetmons; abseesusion simm me listed so the nssreme eight ing . net conductors; there is an cnu I3L]P(mti0n of parttcles from ceurrutton so”9i0iiso law parttcle concentratIon Wtthsn semscondnctnru sheiG]s Ic par tihlks.Ethe electrons and holes—are charged, and diffnsion-celuted carrier transport therefore given rise to particle currents us pictured in Fig. 3.12. narrate —S S see sees Figure 112 181 oliruse —0 0 see sees , Vssualimtian of eloetenu and hole diffusion non mnrensrnpio teals. www.EasyEngineering.net 96 CARRIEu1 ACTiON 5EMtCONDUCTOR FSNnA5IENTALn (c) Ecperimnnr with initially placing pursmcles in mom than one hoc and changing she number in the pnsruo statements. You msght also Iry inceeming the namber of par (C) Exercise 3.3 The “DiffOemo” MAmAS file listed below was svrissen to help she user nrsualrze the diffusion process. The program provider n psendo-ansmasron of u ouo-dmmenssOnnl particle system similar so than described in the rent. The y 11 statement tu the program controls the initial condition, N specifies the masimum namber of moni tored “jnmps,” and she nnmber in the pause statements controls the time between jumps. tick hones. Sm Sample outpnt is reprodnced in Pig. E3.3. 12 5 dO I I 12 I , 0 I I I 511 to %Simulation of Diffusion (DifiDemo) %One-dimensional system, right and left jumps eqoally probable %Inisiahiaat ion close n=40.5 1.5 2.5 3.5 4.5]; y=[l .Oeb 0000]; %NOTE: initial pouitinn can bn changed [np.yp] =barcy]; islot(np,yp]; tens (0.5.1 .leb,’s = 0’); onis([tJ,S,0,l .2c6)]; pause (0.5) %NOTE: increase N foe ousended run N= 15; %Cnsnpusaninns and Plorsing for dt:N, %l2iffasion step calcalution bin(l]eodnd(y(1)/2 + y(2)/ ]; 2 hin(2)Honnd(y(l]12 + y(3]/ ); 2 bin(3)ronnd(y(2]/2 + 2 ]; 4 y( ) / + bin(4)raand(y(3)/2 ); 2 y(5)J ); 2 biu(5]roand(y(4]/2 + y(5)/ ybin; IhPlbning the resalt [vp,yp] bar(n.y); 0. 4 5 Figure 63.3 m[Th ered here because it simalsaneoosly ptovidm as isformasise eucmple of the diffusion ,nsm2ssr(fi]]]; (b) Rerun she program after changing the mmml conditions so thus all of she carriers = 23 3.2.2 Hot-Point Probe Measurement Pr (a) Enter she program inro yotur compnter or locate the copy supplsed on dssk. Run the piograns. (The csotresnrd-pcriod on a Macintosh compnter or break on an IBM corepasible compnser can ho ased so premararely terminate the program.) are in the middle box ass ‘1 1 Before establishing the carrent associated with diffasion, let us digress somewhat nod briefly consider the hot-poins probe measnremcns. The hot-point probe mcuanremene is common lcchssiqce for napiØly determining whether a semiconductor is s- or p-type. Prom a practical standpoint, knowledge of the semicondncror type is essential in device process Ing and moss be known even before determining the doping concentration fronr resisnisiry meannremennn (refer back to Fig. 3.8). The hot-point probe “typing” experiment is consid aniu(axis); plot)xp.yp]; sest(O.S, I. leb,l ‘5 eb]]; 2 anis((0,5.0,l. pause (0.5] end 4[. process. Examining Pig. 3.13(n), we find the only egaipment required for performing the hot point probe nrensureteent is u hot-point probe, a cold-poinn probe, nod a censee-cero mil lmammeter. The hot-point probe is sonmetimes a rebsgee from a wood burning set or simply a soldering irou: the csld-poinl probe sypically assumes the form of an electrical probe like than used with hand-held malsimeters. No special reqauremenu are imposed on the centar oem muhliacsmetec connecsed beswcen the probes. TIme nmnasnmment procedure itself is also extremely simple: After nllowsng the hot probe to heat np, one brings the two probes into contact with the semicondactor sample. nod the onnosener defleens so the right or left, rhereby indicating she semiconductor type. Observe thus nbc spacing benween the probes in set arbitrarily and can be redaced to enhance she ammeter deflection. A simplified explunation of how Ihe hot-point probe meu.sncement works is presented tn Fig. 3.13(b). In she vicinily of nbc probe coctact the heated probe creates an increased 97 _______ 94 SEMICONDUCTOR FUNDAMENTALS CARRIER ACTION 3.2 DIFFUSION 95 1024 ,, : 3.2.1 Definition—Visualization 5 a OC55 whereby particles cod to spread oat or redistribute as a resolt of their iaudom thermal marion. migrathsg on a macroscopic scale front regions of high partIcle colscentratiOs into regions 0 f low particle cencenrration. if allnsved so progress snabated, the diffosion process operates so as so prodtlce a asiforre distribstiau of particles. The diffssirsg entity, is stsoald be noted, reed 1101 be charged; thermal motion, tot inrerparttcle repalsioo, is the enabling action behind the diffasian process. DIffusion tra Li 512 To cite an everyday esample of diffUsion, ssppnse aIr apes bottle of perfame is ptaced in one corner of a room. Escn in the absence of air esereels, randons tlrerroal esotins wf I spread tire perfume molecales thcoaghaot the rosIn ill a rclalivety sirort period of nbc, with intermolecular collisions helping to uniformly redisrribsre the peefarne to esery nook and cearrny within the roamo. Seeking to obtain a more detailed anderstasding of the diffnsion process, let us nest conceptsally “monitor” the process on d osicroscopie scale employing a simple hypotheti cal system. The system we propose tm monitor is a one-dimesrsiosal hex centainrng four cotepartmemsts and 1024 mobile particles (see Fig. 3.11). The particles within the hon obey certain stringent mles. Specificalty, thermal motion canoes all particles in a gisro compart melts to “jump” isle an adjacetsr cempartnnertr eset’y e seconds. In keeping wish the randmss nasare of the motion, each and every particle has an eqcal probability ofjsnsping to the left nod to the right. Hitting an “esternal wall” while attempting to jarssp to the left or right reflects the pursrele back so its pre-Jnmp posItion. Ftnally, nI rinse s = 0 st is assumed that all of the particles are confined in the lefs-moss compaetnserst. Pigore 3.11 records she esolnlsoms of one 1024 parricle system as n fsnction of time. As time I T, 512 ef the 1024 particles originally in compartment 1 jamp to the riglts and come sorest in compartmens 2. The remaining 512 particles jump so the left and are re flected back into the left-moss compartment. The end result is 512 parnicles each In com partments I and 2 after e seconds. As time I = 2e, 256 of the particles in compartment 2 jamp into comsmpartmens 3 and the remainder jump back into compartment 1. In the mcmlrime, 256 of the particles from compartrssemms I jamp into compartmens 2 and 256 nndergo a reflection at the left-Isand wall. The ncr resuls after 2e seconds is 512 parsicles in com partment I and 256 particles each is oompartmenss 2 and 3. TIse stare of she system after 3e and be seconds, also shosvn in Pip. 3.11, can be dedaced in a similar manner. By 5 = fiT, the particles. once confined to she lrfs-moss compartmens, have become utnross aniformly distribosed shrouglsoot she hon. and it it nnnecessary to consider later states. Indeed, she fnndamensal nature of the diffnsion process is clearly self-evident frosn an enamsnasion of the enisssng states. In semicondactors she diffusion precens on a micrnscopie scale in similar so thaI oc currsng in the hyposhcsical system esecps, of coUrse, she mndom morion of the diffusing parsicles is three-dimensional arid nor “comparsmentalieed.” On n macroscopic scale she net effecs of diffusion is precisely she same witlnin both the hypothetical system and semi- ass aso 52e 384 354 I san r5e 255 am 52 s6e Figure 3.11 PuPation usa microsenpio scale in a hypnthetirat ann-dimensional system. The nnm bees once the arrows iodicaso shn number of partirlnu in a given oosnpaetmons; abseesusion simm me listed so the nssreme eight conductors; there is an cnu I3L]P(mti0n of parttcles from ceurrutton so”9i0iiso law parttcle concentratIon Wtthsn semscondnctnru sheiG]s Ic par tihlks.Ethe electrons and holes—are charged, and diffnsion-celuted carrier transport therefore given rise to particle currents us pictured in Fig. 3.12. narrate —S S see sees Figure 112 181 oliruse —0 0 see sees , Vssualimtian of eloetenu and hole diffusion non mnrensrnpio teals. www.EasyEngineering.net 96 CARRIEu1 ACTiON 5EMtCONDUCTOR FSNnA5IENTALn (c) Ecperimnnr with initially placing pursmcles in mom than one hoc and changing she number in the pnsruo statements. You msght also Iry inceeming the namber of par (C) Exercise 3.3 The “DiffOemo” MAmAS file listed below was svrissen to help she user nrsualrze the diffusion process. The program provider n psendo-ansmasron of u ouo-dmmenssOnnl particle system similar so than described in the rent. The y 11 statement tu the program controls the initial condition, N specifies the masimum namber of moni tored “jnmps,” and she nnmber in the pause statements controls the time between jumps. tick hones. Sm Sample outpnt is reprodnced in Pig. E3.3. 12 5 dO I I 12 I , 0 I I I 511 to %Simulation of Diffusion (DifiDemo) %One-dimensional system, right and left jumps eqoally probable ww w %Inisiahiaat ion close n=40.5 1.5 2.5 3.5 4.5]; y=[l .Oeb 0000]; %NOTE: initial pouitinn can bn changed [np.yp] =barcy]; islot(np,yp]; tens (0.5.1 .leb,’s = 0’); onis([tJ,S,0,l .2c6)]; pause (0.5) %NOTE: increase N foe ousended run N= 15; .Ea 4[. ‘1 syE ngi %Cnsnpusaninns and Plorsing for dt:N, %l2iffasion step calcalution bin(l]eodnd(y(1)/2 + y(2)/ ]; 2 hin(2)Honnd(y(l]12 + y(3]/ ); 2 bin(3)ronnd(y(2]/2 + 2 ]; 4 y( ) / + bin(4)raand(y(3)/2 ); 2 y(5)J ); 2 biu(5]roand(y(4]/2 + y(5)/ ybin; IhPlbning the resalt [vp,yp] bar(n.y); 1 nee rin g .ne t ,nsm2ssr(fi]]]; (b) Rerun she program after changing the mmml conditions so thus all of she carriers = 5 m[Th 3.2.2 Hot-Point Probe Measurement Pr (a) Enter she program inro yotur compnter or locate the copy supplsed on dssk. Run the piograns. (The csotresnrd-pcriod on a Macintosh compnter or break on an IBM corepasible compnser can ho ased so premararely terminate the program.) are in the middle box ass 4 Figure 63.3 aniu(axis); plot)xp.yp]; sest(O.S, I. leb,l ‘5 eb]]; 2 anis((0,5.0,l. pause (0.5] end 23 0. www.EasyEngineering.net Before establishing the carrent associated with diffasion, let us digress somewhat nod briefly consider the hot-poins probe measnremcns. The hot-point probe mcuanremene is common lcchssiqce for napiØly determining whether a semiconductor is s- or p-type. Prom a practical standpoint, knowledge of the semicondncror type is essential in device process Ing and moss be known even before determining the doping concentration fronr resisnisiry meannremennn (refer back to Fig. 3.8). The hot-point probe “typing” experiment is consid ered here because it simalsaneoosly ptovidm as isformasise eucmple of the diffusion process. Examining Pig. 3.13(n), we find the only egaipment required for performing the hot point probe nrensureteent is u hot-point probe, a cold-poinn probe, nod a censee-cero mil lmammeter. The hot-point probe is sonmetimes a rebsgee from a wood burning set or simply a soldering irou: the csld-poinl probe sypically assumes the form of an electrical probe like than used with hand-held malsimeters. No special reqauremenu are imposed on the centar oem muhliacsmetec connecsed beswcen the probes. TIme nmnasnmment procedure itself is also extremely simple: After nllowsng the hot probe to heat np, one brings the two probes into contact with the semicondactor sample. nod the onnosener defleens so the right or left, rhereby indicating she semiconductor type. Observe thus nbc spacing benween the probes in set arbitrarily and can be redaced to enhance she ammeter deflection. A simplified explunation of how Ihe hot-point probe meu.sncement works is presented tn Fig. 3.13(b). In she vicinily of nbc probe coctact the heated probe creates an increased 97 _______ 94 SEMICONDUCTOR FUNDAMENTALS 95 CARRIER ACTION 3.2 DIFFUSION 1024 ,, : 3.2.1 Definition—Visualization 5 a OC55 whereby particles cod to spread oat or redistribute as a resolt of their iaudom thermal marion. migrathsg on a macroscopic scale front regions of high partIcle colscentratiOs into regions 0 f low particle cencenrration. if allnsved so progress snabated, the diffosion process operates so as so prodtlce a asiforre distribstiau of particles. The diffssirsg entity, is stsoald be noted, reed 1101 be charged; thermal motion, tot inrerparttcle repalsioo, is the enabling action behind the diffasian process. DIffusion tra Li 512 To cite an everyday esample of diffUsion, ssppnse aIr apes bottle of perfame is ptaced in one corner of a room. Escn in the absence of air esereels, randons tlrerroal esotins wf I spread tire perfume molecales thcoaghaot the rosIn ill a rclalivety sirort period of nbc, with intermolecular collisions helping to uniformly redisrribsre the peefarne to esery nook and cearrny within the roamo. Seeking to obtain a more detailed anderstasding of the diffnsion process, let us nest conceptsally “monitor” the process on d osicroscopie scale employing a simple hypotheti cal system. The system we propose tm monitor is a one-dimesrsiosal hex centainrng four cotepartmemsts and 1024 mobile particles (see Fig. 3.11). The particles within the hon obey certain stringent mles. Specificalty, thermal motion canoes all particles in a gisro compart melts to “jump” isle an adjacetsr cempartnnertr eset’y e seconds. In keeping wish the randmss nasare of the motion, each and every particle has an eqcal probability ofjsnsping to the left nod to the right. Hitting an “esternal wall” while attempting to jarssp to the left or right reflects the pursrele back so its pre-Jnmp posItion. Ftnally, nI rinse s = 0 st is assumed that all of the particles are confined in the lefs-moss compaetnserst. Pigore 3.11 records she esolnlsoms of one 1024 parricle system as n fsnction of time. As time I T, 512 ef the 1024 particles originally in compartment 1 jamp to the riglts and come sorest in compartmens 2. The remaining 512 particles jump so the left and are re flected back into the left-moss compartment. The end result is 512 parnicles each In com partments I and 2 after e seconds. As time I = 2e, 256 of the particles in compartment 2 jamp into comsmpartmens 3 and the remainder jump back into compartment 1. In the mcmlrime, 256 of the particles from compartrssemms I jamp into compartmens 2 and 256 nndergo a reflection at the left-Isand wall. The ncr resuls after 2e seconds is 512 parsicles in com partment I and 256 particles each is oompartmenss 2 and 3. TIse stare of she system after 3e and be seconds, also shosvn in Pip. 3.11, can be dedaced in a similar manner. By 5 = fiT, the particles. once confined to she lrfs-moss compartmens, have become utnross aniformly distribosed shrouglsoot she hon. and it it nnnecessary to consider later states. Indeed, she fnndamensal nature of the diffnsion process is clearly self-evident frosn an enamsnasion of the enisssng states. In semicondactors she diffusion precens on a micrnscopie scale in similar so thaI oc currsng in the hyposhcsical system esecps, of coUrse, she mndom morion of the diffusing parsicles is three-dimensional arid nor “comparsmentalieed.” On n macroscopic scale she net effecs of diffusion is precisely she same witlnin both the hypothetical system and semi- ass aso 52e 384 354 I san r5e 255 am 52 s6e Figure 3.11 PuPation usa microsenpio scale in a hypnthetirat ann-dimensional system. The nnm bees once the arrows iodicaso shn number of partirlnu in a given oosnpaetmons; abseesusion simm me listed so the nssreme eight conductors; there is an cnu I3L]P(mti0n of parttcles from ceurrutton so”9i0iiso law parttcle concentratIon Wtthsn semscondnctnru sheiG]s Ic par tihlks.Ethe electrons and holes—are charged, and diffnsion-celuted carrier transport therefore given rise to particle currents us pictured in Fig. 3.12. narrate —S S see sees Figure 112 181 oliruse —0 0 see sees , Vssualimtian of eloetenu and hole diffusion non mnrensrnpio teals. www.EasyEngineering.net 96 CARRIEu1 ACTiON 5EMtCONDUCTOR FSNnA5IENTALn 97 (c) Ecperimnnr with initially placing pursmcles in mom than one hoc and changing she number in the pnsruo statements. You msght also Iry inceeming the namber of par (C) Exercise 3.3 The “DiffOemo” MAmAS file listed below was svrissen to help she user nrsualrze the diffusion process. The program provider n psendo-ansmasron of u ouo-dmmenssOnnl particle system similar so than described in the rent. The y 11 statement tu the program controls the initial condition, N specifies the masimum namber of moni tored “jnmps,” and she nnmber in the pause statements controls the time between jumps. tick hones. Sm Sample outpnt is reprodnced in Pig. E3.3. 12 5 dO I I 12 I , 0 I I I 511 to %Simulation of Diffusion (DifiDemo) %One-dimensional system, right and left jumps eqoally probable %Inisiahiaat ion close n=40.5 1.5 2.5 3.5 4.5]; y=[l .Oeb 0000]; %NOTE: initial pouitinn can bn changed [np.yp] =barcy]; islot(np,yp]; tens (0.5.1 .leb,’s = 0’); onis([tJ,S,0,l .2c6)]; pause (0.5) %NOTE: increase N foe ousended run N= 15; %Cnsnpusaninns and Plorsing for dt:N, %l2iffasion step calcalution bin(l]eodnd(y(1)/2 + y(2)/ ]; 2 hin(2)Honnd(y(l]12 + y(3]/ ); 2 bin(3)ronnd(y(2]/2 + 2 ]; 4 y( ) / + bin(4)raand(y(3)/2 ); 2 y(5)J ); 2 biu(5]roand(y(4]/2 + y(5)/ ybin; IhPlbning the resalt [vp,yp] bar(n.y); 0. 4 5 En Figure 63.3 m[Th gin eer ing .ne ered here because it simalsaneoosly ptovidm as isformasise eucmple of the diffusion ,nsm2ssr(fi]]]; (b) Rerun she program after changing the mmml conditions so thus all of she carriers = ‘1 asy 23 3.2.2 Hot-Point Probe Measurement Pr (a) Enter she program inro yotur compnter or locate the copy supplsed on dssk. Run the piograns. (The csotresnrd-pcriod on a Macintosh compnter or break on an IBM corepasible compnser can ho ased so premararely terminate the program.) are in the middle box ass 1 4[. Before establishing the carrent associated with diffasion, let us digress somewhat nod briefly consider the hot-poins probe measnremcns. The hot-point probe mcuanremene is common lcchssiqce for napiØly determining whether a semiconductor is s- or p-type. Prom a practical standpoint, knowledge of the semicondncror type is essential in device process Ing and moss be known even before determining the doping concentration fronr resisnisiry meannremennn (refer back to Fig. 3.8). The hot-point probe “typing” experiment is consid aniu(axis); plot)xp.yp]; sest(O.S, I. leb,l ‘5 eb]]; 2 anis((0,5.0,l. pause (0.5] end ww w.E process. Examining Pig. 3.13(n), we find the only egaipment required for performing the hot point probe nrensureteent is u hot-point probe, a cold-poinn probe, nod a censee-cero mil lmammeter. The hot-point probe is sonmetimes a rebsgee from a wood burning set or simply a soldering irou: the csld-poinl probe sypically assumes the form of an electrical probe like than used with hand-held malsimeters. No special reqauremenu are imposed on the centar oem muhliacsmetec connecsed beswcen the probes. TIme nmnasnmment procedure itself is also extremely simple: After nllowsng the hot probe to heat np, one brings the two probes into contact with the semicondactor sample. nod the onnosener defleens so the right or left, rhereby indicating she semiconductor type. Observe thus nbc spacing benween the probes in set arbitrarily and can be redaced to enhance she ammeter deflection. A simplified explunation of how Ihe hot-point probe meu.sncement works is presented tn Fig. 3.13(b). In she vicinily of nbc probe coctact the heated probe creates an increased www.EasyEngineering.net t www.EasyEngineering.net 98 sEMicONeuuTou r Fariraavtu’raLn CaRRieR ACItON 99 The esestosis of proportiooahty, D aud D 5 have units of cm /sec and are ceferced to ss 2 the (role end electron diffusion coefficients, respectively. Upon examining Eqs. 13.17), note that the current directions deduced from the eqas ions see consisreirt with the Pig. 3.12 visualization of the maaroscopic diffusion currents. Per the positive concentration gradient shown in Pig. 3.12 (dpldn >0 and dri/dc >0 foe the pictured one-dimensional situation), both holes and electrons ssill diffuse in the —x direction. ssill therefore he negesise or directed in the x direction, while main will be oriented in rhc -cx direction. - — fsesgri:r sates airraie-uueuv Enrrgrve sinitrasi dirtuse awap Total Currents lab lab The total or set carrier cui-i-ents iso seusicosdsctoe arise m the combined resslr of drift ond diffssioe. Sumovng sue respective n and p segments of Eqs. (3.4) end Eqs. (3.17). one obtains Figure 313 The hot-point probe measurement: (a) required equipment: ib) uimplihed onptusetinn of hose rho weessrnmnni irorbs. ww - w.E number of higher-energy carriers. These energetic carriers will be predominantly boles is the ease of a p-type material end etecsrons in en s-type materiel. With more energetic carriers near the heated penhe thus elsewhere, diffosins acts so as to spread the higher esergy carriers throughout the seuncunductor wafer. The net effect is a deficit of holes ore net negative charge in thu vicinity of the hot-point probe for a p-type materiel, end a posi tree charge buildup near the heated probe within an n-type materint. Accordingty, the center-cern meter deflects in a different direction for p- end n-type materiets. as y En gin e 3.2.3 Diffusion and Total Currents Diffusion Currentn r:a,ssIrIa,o 3 [ (3.10 a) t LN = + drift diffssion 5I,0 = The total particle correct fleming in u semiconductor is in mm computed from (3.10) eri ng. ne The donbte boxes emphasize the importance of the blat-current relationships; they are used directly or indirectly in the vest majority of device ooalyses. In defining the diffusion process end in citing diffesinn examples, we have sought In em phasize the direct correlation between diffusion arid a spatial variation in particle numbers. For diffusion to occur, more of the diffusing particles must enist at one point than another points or, in methemoticot terms, there must he a nonzero concentration gradient (Vp 0 for boles, Vii ar 0 for electrons). Logically, moreover, the greater the coucentrelion gradient, the larger the expected fan of parlicles. Qeantilelive analysis of the diffusion process in deed confirms the foregoing aed leads to what is known us Pick’s lnw: 3.2.4 Relating Diffusion Coefficients/Mobilities t = = The diffusion ceefficients, the constants of the motion associated with diffissien, are obvi ously central parunsetees)n characterizing c-airier transport due to diffusion. Gives the im portance of the diffusion coefficieurs, one might anricipsle an extended examination of relevant properties paralleling the mobility presentation in Snbsecsieu 3.1.3. Fortunately, an extended examination is unnecessary because the D’s end the ye’s are alt iulerrnlaled. It is only necessary so establish the cosuecting fomnsute known as the Einstein relationship. In deriving the Einstein relationship, we consider a norisuifurruty doped semiconduc tor meiotaieed under equilibrium renditions. Special facts related te the sonanifnrm dop ing and the equilibrium state are invoked in the derivation. These facts, important in them selves, are reviewed prior to presenting the derivation proper. )3.lfi) —DVq where 3i is the flux or parlietes/em -sec crossing a plane perpendicular to the particle flow, 2 q is the particle concentration, and D is the diff’iusiou coefficient, a positive proporlionatity foctor. The diffusiou current density due In electrons and holes is obtained by simply mul tiplying the carrier flux by the carrier charge: Constancy ot the Fermi Level (3.17a) “miami = Consider a nondegenerate, nounsifoemly doped ri-type semiconductor ssmple, a sample where the doping concentration varies us a function of position. A concrete example of what ma hove in mind is shusvn in Pig. 3.14(o). Assuming equilibrium conditions prevail, — (3.17b) www.EasyEngineering.net r 100 nEutcounncTou FuNDAMENTALs cannien acomN the energy bond diagram characterizing the sample wit) hove the forro sketched in Fig. 3.14(b). In Chapter 2 the Fermi level in uniformly doped n-type semiconductors sees fosed In move closer and closer to E sxhee the donor doping mm systematically increased )see Fig. 2.21). Consistent with this fact, ff was drawn closer tu in going from x = 0 to x = L on tire Fig. 3.14(h) d:agrein. Conssrsction of the diagram, hoscever, contd not hove been completed mishear making use of a critical new piece of information. Specificolly, oxder eqailibriosu coridisioes, elffv/do = dff/dy = dEr/dc = 0; i.e., the Fenni level inside o moserin) am group ofrnoieriiuis in insimesie cousocs is iuvnriurss us afisuction ofposiiiou. Thr coussuocy of the Fermi level means that Er is to appear as o horizouto) linens equilib rium energy heed diagrams. /The posaioo independence of the Fermi energy is established by examining the leans- for of carriers between el;osvcd crates with the same energy but at adjoarot positions in an energy band. It is concluded the probability of filling the states at a given energy,f)E), must be the same everywhere in the sample under equilibrium conditions. If Ibis wore not the ease, carriers mould preferentially transfer between states and thereby give rise to 5 net current. The existence of a set current is inconsisleor with the specified equilibrium con ditions. Referring to the Eq. (2.7) expression forf(E), we find that thp constancy of the Fernsi function is turn requires the Fermi level to be independent of pnsf?ion. Current Flom Under Equilihrium Conditions Uuoer eqaihberusmm conditions the total current is of course identically zero. Brrunse elec tron and hole activity is totatty decoupled under equilibrium conditions, the electron and hole current densities. ,1 and J,, most also independently vanish. Setting .J = J. = 0 in Eq. (3. It), however, leads to the conclusion that the drift and diffusion currents assariated with e given corner are merely reqnimd lobe of equal mugnitude and opposite polerity. Is fact, the dnft and diffusion components wilt vanish undue eqsilibrinm conditions only if 0 and Vu Vp = 0. To provide a concrete illustration of eon-nenishieg equilibrium current components, let as retsru to en examination of the noousiformly doped semiconductor sample charec runeed by Fig. 3.14. The dopumsr variation piclured in Fiy. 3.14(a) clearly gives rise to a significant electron concentration gradient. An electron diffusion earreut flossing in the +x direction mnsl exist mime the sample. The band bending shows in the hand diagram of Pig. 3. t4)b), moreover, implies the esistence of a “built-in” electric field oriented in the x direetiun. This gives ole to u drift current also in the x dition. Netc that the drift and diffusion components are of opposite polarity. Since equilibrium cooditiom are as sumed to prevail, the components must also be of equal magnitude. In point of fact, the electric field arises inside the sesoicondactur to counteract the diffusive tendeeeies of the carriers caused by the nonuniform dapiug. The major point herein that, eves under equilib cow condition, nonuniform doping will give rise to carrier concentration gradients, a built m electric field, and non-zero current components. — — L Einstein Relstionship Eu —+------———-——-----------j--u’ S o t Having lard the proper foundation, sve can now proceed to derive the connecting formula between the D’s and the ye’s knnwu as the Einstein relationship. To simplify the develop ment, we work in only one dimension, Thr sample under analysis iu luken to he a uonde generate, sonasiformly doped semiconductor maintained nuder equilibrium conditions. Citing the fact that she net carrier eurreuls musl be identically zero nuder equilibrinm con ditions, and focusing on the electrons, we cue state )b) Figure 3.14 Nooaniformly duped sewicoodoeiav (a) essumed doping veeiaaon miih pnsiiiios: (hi eorrespsodisg equilibrium energy band diagram. iviaov + iula,n = nE + 5 qys qD4fi = 0 (3.20) 101 www.EasyEngineering.net r 98 sEMicONeuuTou Fariraavtu’raLn CaRRieR ACItON 99 The esestosis of proportiooahty, D aud D 5 have units of cm /sec and are ceferced to ss 2 the (role end electron diffusion coefficients, respectively. Upon examining Eqs. 13.17), note that the current directions deduced from the eqas ions see consisreirt with the Pig. 3.12 visualization of the maaroscopic diffusion currents. Per the positive concentration gradient shown in Pig. 3.12 (dpldn >0 and dri/dc >0 foe the pictured one-dimensional situation), both holes and electrons ssill diffuse in the —x direction. ssill therefore he negesise or directed in the x direction, while main will be oriented in rhc -cx direction. - — fsesgri:r sates airraie-uueuv Enrrgrve sinitrasi dirtuse awap Total Currents lab lab The total or set carrier cui-i-ents iso seusicosdsctoe arise m the combined resslr of drift ond diffssioe. Sumovng sue respective n and p segments of Eqs. (3.4) end Eqs. (3.17). one obtains Figure 313 The hot-point probe measurement: (a) required equipment: ib) uimplihed onptusetinn of hose rho weessrnmnni irorbs. ww number of higher-energy carriers. These energetic carriers will be predominantly boles is the ease of a p-type material end etecsrons in en s-type materiel. With more energetic carriers near the heated penhe thus elsewhere, diffosins acts so as to spread the higher esergy carriers throughout the seuncunductor wafer. The net effect is a deficit of holes ore net negative charge in thu vicinity of the hot-point probe for a p-type materiel, end a posi tree charge buildup near the heated probe within an n-type materint. Accordingty, the center-cern meter deflects in a different direction for p- end n-type materiets. - w.E a r:a,ssIrIa,o 3 [ LN = drift diffssion syE ngi + 5I,0 = nee r Diffusion Currentn (3.10) ing . The donbte boxes emphasize the importance of the blat-current relationships; they are used directly or indirectly in the vest majority of device ooalyses. In defining the diffusion process end in citing diffesinn examples, we have sought In em phasize the direct correlation between diffusion arid a spatial variation in particle numbers. For diffusion to occur, more of the diffusing particles must enist at one point than another points or, in methemoticot terms, there must he a nonzero concentration gradient (Vp 0 for boles, Vii ar 0 for electrons). Logically, moreover, the greater the coucentrelion gradient, the larger the expected fan of parlicles. Qeantilelive analysis of the diffusion process in deed confirms the foregoing aed leads to what is known us Pick’s lnw: 3.2.4 Relating Diffusion Coefficients/Mobilities net The diffusion ceefficients, the constants of the motion associated with diffissien, are obvi ously central parunsetees)n characterizing c-airier transport due to diffusion. Gives the im portance of the diffusion coefficieurs, one might anricipsle an extended examination of relevant properties paralleling the mobility presentation in Snbsecsieu 3.1.3. Fortunately, an extended examination is unnecessary because the D’s end the ye’s are alt iulerrnlaled. It is only necessary so establish the cosuecting fomnsute known as the Einstein relationship. In deriving the Einstein relationship, we consider a norisuifurruty doped semiconduc tor meiotaieed under equilibrium renditions. Special facts related te the sonanifnrm dop ing and the equilibrium state are invoked in the derivation. These facts, important in them selves, are reviewed prior to presenting the derivation proper. )3.lfi) —DVq (3.10 a) t The total particle correct fleming in u semiconductor is in mm computed from 3.2.3 Diffusion and Total Currents = = where 3i is the flux or parlietes/em -sec crossing a plane perpendicular to the particle flow, 2 q is the particle concentration, and D is the diff’iusiou coefficient, a positive proporlionatity foctor. The diffusiou current density due In electrons and holes is obtained by simply mul tiplying the carrier flux by the carrier charge: Constancy ot the Fermi Level (3.17a) “miami = Consider a nondegenerate, nounsifoemly doped ri-type semiconductor ssmple, a sample where the doping concentration varies us a function of position. A concrete example of what ma hove in mind is shusvn in Pig. 3.14(o). Assuming equilibrium conditions prevail, — (3.17b) www.EasyEngineering.net r 100 nEutcounncTou FuNDAMENTALs cannien acomN the energy bond diagram characterizing the sample wit) hove the forro sketched in Fig. 3.14(b). In Chapter 2 the Fermi level in uniformly doped n-type semiconductors sees fosed In move closer and closer to E sxhee the donor doping mm systematically increased )see Fig. 2.21). Consistent with this fact, ff was drawn closer tu in going from x = 0 to x = L on tire Fig. 3.14(h) d:agrein. Conssrsction of the diagram, hoscever, contd not hove been completed mishear making use of a critical new piece of information. Specificolly, oxder eqailibriosu coridisioes, elffv/do = dff/dy = dEr/dc = 0; i.e., the Fenni level inside o moserin) am group ofrnoieriiuis in insimesie cousocs is iuvnriurss us afisuction ofposiiiou. Thr coussuocy of the Fermi level means that Er is to appear as o horizouto) linens equilib rium energy heed diagrams. /The posaioo independence of the Fermi energy is established by examining the leans- for of carriers between el;osvcd crates with the same energy but at adjoarot positions in an energy band. It is concluded the probability of filling the states at a given energy,f)E), must be the same everywhere in the sample under equilibrium conditions. If Ibis wore not the ease, carriers mould preferentially transfer between states and thereby give rise to 5 net current. The existence of a set current is inconsisleor with the specified equilibrium con ditions. Referring to the Eq. (2.7) expression forf(E), we find that thp constancy of the Fernsi function is turn requires the Fermi level to be independent of pnsf?ion. Current Flom Under Equilihrium Conditions Uuoer eqaihberusmm conditions the total current is of course identically zero. Brrunse elec tron and hole activity is totatty decoupled under equilibrium conditions, the electron and hole current densities. ,1 and J,, most also independently vanish. Setting .J = J. = 0 in Eq. (3. It), however, leads to the conclusion that the drift and diffusion currents assariated with e given corner are merely reqnimd lobe of equal mugnitude and opposite polerity. Is fact, the dnft and diffusion components wilt vanish undue eqsilibrinm conditions only if 0 and Vu Vp = 0. To provide a concrete illustration of eon-nenishieg equilibrium current components, let as retsru to en examination of the noousiformly doped semiconductor sample charec runeed by Fig. 3.14. The dopumsr variation piclured in Fiy. 3.14(a) clearly gives rise to a significant electron concentration gradient. An electron diffusion earreut flossing in the +x direction mnsl exist mime the sample. The band bending shows in the hand diagram of Pig. 3. t4)b), moreover, implies the esistence of a “built-in” electric field oriented in the x direetiun. This gives ole to u drift current also in the x dition. Netc that the drift and diffusion components are of opposite polarity. Since equilibrium cooditiom are as sumed to prevail, the components must also be of equal magnitude. In point of fact, the electric field arises inside the sesoicondactur to counteract the diffusive tendeeeies of the carriers caused by the nonuniform dapiug. The major point herein that, eves under equilib cow condition, nonuniform doping will give rise to carrier concentration gradients, a built m electric field, and non-zero current components. — — L Einstein Relstionship Eu —+------———-——-----------j--u’ S o t Having lard the proper foundation, sve can now proceed to derive the connecting formula between the D’s and the ye’s knnwu as the Einstein relationship. To simplify the develop ment, we work in only one dimension, Thr sample under analysis iu luken to he a uonde generate, sonasiformly doped semiconductor maintained nuder equilibrium conditions. Citing the fact that she net carrier eurreuls musl be identically zero nuder equilibrinm con ditions, and focusing on the electrons, we cue state )b) Figure 3.14 Nooaniformly duped sewicoodoeiav (a) essumed doping veeiaaon miih pnsiiiios: (hi eorrespsodisg equilibrium energy band diagram. iviaov + iula,n = nE + 5 qys qD4fi = 0 (3.20) 101 r 98 sEMicONeuuTou Fariraavtu’raLn CaRRieR ACItON 99 The esestosis of proportiooahty, D aud D 5 have units of cm /sec and are ceferced to ss 2 the (role end electron diffusion coefficients, respectively. Upon examining Eqs. 13.17), note that the current directions deduced from the eqas ions see consisreirt with the Pig. 3.12 visualization of the maaroscopic diffusion currents. Per the positive concentration gradient shown in Pig. 3.12 (dpldn >0 and dri/dc >0 foe the pictured one-dimensional situation), both holes and electrons ssill diffuse in the —x direction. ssill therefore he negesise or directed in the x direction, while main will be oriented in rhc -cx direction. - — fsesgri:r sates airraie-uueuv Enrrgrve sinitrasi dirtuse awap Total Currents lab lab The total or set carrier cui-i-ents iso seusicosdsctoe arise m the combined resslr of drift ond diffssioe. Sumovng sue respective n and p segments of Eqs. (3.4) end Eqs. (3.17). one obtains Figure 313 The hot-point probe measurement: (a) required equipment: ib) uimplihed onptusetinn of hose rho weessrnmnni irorbs. - number of higher-energy carriers. These energetic carriers will be predominantly boles is the ease of a p-type material end etecsrons in en s-type materiel. With more energetic carriers near the heated penhe thus elsewhere, diffosins acts so as to spread the higher esergy carriers throughout the seuncunductor wafer. The net effect is a deficit of holes ore net negative charge in thu vicinity of the hot-point probe for a p-type materiel, end a posi tree charge buildup near the heated probe within an n-type materint. Accordingty, the center-cern meter deflects in a different direction for p- end n-type materiets. r:a,ssIrIa,o 3 [ = (3.10 a) t LN = + drift diffssion 5I,0 = The total particle correct fleming in u semiconductor is in mm computed from (3.10) 3.2.3 Diffusion and Total Currents Diffusion Currentn The donbte boxes emphasize the importance of the blat-current relationships; they are used directly or indirectly in the vest majority of device ooalyses. In defining the diffusion process end in citing diffesinn examples, we have sought In em phasize the direct correlation between diffusion arid a spatial variation in particle numbers. For diffusion to occur, more of the diffusing particles must enist at one point than another points or, in methemoticot terms, there must he a nonzero concentration gradient (Vp 0 for boles, Vii ar 0 for electrons). Logically, moreover, the greater the coucentrelion gradient, the larger the expected fan of parlicles. Qeantilelive analysis of the diffusion process in deed confirms the foregoing aed leads to what is known us Pick’s lnw: = 3.2.4 Relating Diffusion Coefficients/Mobilities The diffusion ceefficients, the constants of the motion associated with diffissien, are obvi ously central parunsetees)n characterizing c-airier transport due to diffusion. Gives the im portance of the diffusion coefficieurs, one might anricipsle an extended examination of relevant properties paralleling the mobility presentation in Snbsecsieu 3.1.3. Fortunately, an extended examination is unnecessary because the D’s end the ye’s are alt iulerrnlaled. It is only necessary so establish the cosuecting fomnsute known as the Einstein relationship. In deriving the Einstein relationship, we consider a norisuifurruty doped semiconduc tor meiotaieed under equilibrium renditions. Special facts related te the sonanifnrm dop ing and the equilibrium state are invoked in the derivation. These facts, important in them selves, are reviewed prior to presenting the derivation proper. )3.lfi) —DVq where 3i is the flux or parlietes/em -sec crossing a plane perpendicular to the particle flow, 2 q is the particle concentration, and D is the diff’iusiou coefficient, a positive proporlionatity foctor. The diffusiou current density due In electrons and holes is obtained by simply mul tiplying the carrier flux by the carrier charge: Constancy ot the Fermi Level (3.17a) “miami = Consider a nondegenerate, nounsifoemly doped ri-type semiconductor ssmple, a sample where the doping concentration varies us a function of position. A concrete example of what ma hove in mind is shusvn in Pig. 3.14(o). Assuming equilibrium conditions prevail, — (3.17b) www.EasyEngineering.net 100 r nEutcounncTou FuNDAMENTALs cannien acomN the energy bond diagram characterizing the sample wit) hove the forro sketched in Fig. 3.14(b). In Chapter 2 the Fermi level in uniformly doped n-type semiconductors sees fosed In move closer and closer to E sxhee the donor doping mm systematically increased )see Fig. 2.21). Consistent with this fact, ff was drawn closer tu in going from x = 0 to x = L on tire Fig. 3.14(h) d:agrein. Conssrsction of the diagram, hoscever, contd not hove been completed mishear making use of a critical new piece of information. Specificolly, oxder eqailibriosu coridisioes, elffv/do = dff/dy = dEr/dc = 0; i.e., the Fenni level inside o moserin) am group ofrnoieriiuis in insimesie cousocs is iuvnriurss us afisuction ofposiiiou. Thr coussuocy of the Fermi level means that Er is to appear as o horizouto) linens equilib rium energy heed diagrams. /The posaioo independence of the Fermi energy is established by examining the leans- ww w .Ea syE ngi nee rin g L for of carriers between el;osvcd crates with the same energy but at adjoarot positions in an energy band. It is concluded the probability of filling the states at a given energy,f)E), must be the same everywhere in the sample under equilibrium conditions. If Ibis wore not the ease, carriers mould preferentially transfer between states and thereby give rise to 5 net current. The existence of a set current is inconsisleor with the specified equilibrium con ditions. Referring to the Eq. (2.7) expression forf(E), we find that thp constancy of the Fernsi function is turn requires the Fermi level to be independent of pnsf?ion. Current Flom Under Equilihrium Conditions Uuoer eqaihberusmm conditions the total current is of course identically zero. Brrunse elec tron and hole activity is totatty decoupled under equilibrium conditions, the electron and hole current densities. ,1 and J,, most also independently vanish. Setting .J = J. = 0 in Eq. (3. It), however, leads to the conclusion that the drift and diffusion currents assariated with e given corner are merely reqnimd lobe of equal mugnitude and opposite polerity. Is fact, the dnft and diffusion components wilt vanish undue eqsilibrinm conditions only if 0 and Vu Vp = 0. To provide a concrete illustration of eon-nenishieg equilibrium current components, let as retsru to en examination of the noousiformly doped semiconductor sample charec runeed by Fig. 3.14. The dopumsr variation piclured in Fiy. 3.14(a) clearly gives rise to a significant electron concentration gradient. An electron diffusion earreut flossing in the +x direction mnsl exist mime the sample. The band bending shows in the hand diagram of Pig. 3. t4)b), moreover, implies the esistence of a “built-in” electric field oriented in the x direetiun. This gives ole to u drift current also in the x dition. Netc that the drift and diffusion components are of opposite polarity. Since equilibrium cooditiom are as sumed to prevail, the components must also be of equal magnitude. In point of fact, the electric field arises inside the sesoicondactur to counteract the diffusive tendeeeies of the carriers caused by the nonuniform dapiug. The major point herein that, eves under equilib cow condition, nonuniform doping will give rise to carrier concentration gradients, a built m electric field, and non-zero current components. — — .ne t Einstein Relstionship Eu —+------———-——-----------j--u’ S o t Having lard the proper foundation, sve can now proceed to derive the connecting formula between the D’s and the ye’s knnwu as the Einstein relationship. To simplify the develop ment, we work in only one dimension, Thr sample under analysis iu luken to he a uonde generate, sonasiformly doped semiconductor maintained nuder equilibrium conditions. Citing the fact that she net carrier eurreuls musl be identically zero nuder equilibrinm con ditions, and focusing on the electrons, we cue state )b) Figure 3.14 Nooaniformly duped sewicoodoeiav (a) essumed doping veeiaaon miih pnsiiiios: (hi eorrespsodisg equilibrium energy band diagram. www.EasyEngineering.net iviaov + iula,n = nE + 5 qys qD4fi = 0 (3.20) 101 r 98 sEMicONeuuTou Fariraavtu’raLn CaRRieR ACItON 99 The esestosis of proportiooahty, D aud D 5 have units of cm /sec and are ceferced to ss 2 the (role end electron diffusion coefficients, respectively. Upon examining Eqs. 13.17), note that the current directions deduced from the eqas ions see consisreirt with the Pig. 3.12 visualization of the maaroscopic diffusion currents. Per the positive concentration gradient shown in Pig. 3.12 (dpldn >0 and dri/dc >0 foe the pictured one-dimensional situation), both holes and electrons ssill diffuse in the —x direction. ssill therefore he negesise or directed in the x direction, while main will be oriented in rhc -cx direction. - — fsesgri:r sates airraie-uueuv Enrrgrve sinitrasi dirtuse awap Total Currents lab lab The total or set carrier cui-i-ents iso seusicosdsctoe arise m the combined resslr of drift ond diffssioe. Sumovng sue respective n and p segments of Eqs. (3.4) end Eqs. (3.17). one obtains Figure 313 The hot-point probe measurement: (a) required equipment: ib) uimplihed onptusetinn of hose rho weessrnmnni irorbs. - number of higher-energy carriers. These energetic carriers will be predominantly boles is the ease of a p-type material end etecsrons in en s-type materiel. With more energetic carriers near the heated penhe thus elsewhere, diffosins acts so as to spread the higher esergy carriers throughout the seuncunductor wafer. The net effect is a deficit of holes ore net negative charge in thu vicinity of the hot-point probe for a p-type materiel, end a posi tree charge buildup near the heated probe within an n-type materint. Accordingty, the center-cern meter deflects in a different direction for p- end n-type materiets. r:a,ssIrIa,o 3 [ = (3.10 a) t LN = drift diffssion 5I,0 = + The total particle correct fleming in u semiconductor is in mm computed from (3.10) 3.2.3 Diffusion and Total Currents Diffusion Currentn The donbte boxes emphasize the importance of the blat-current relationships; they are used directly or indirectly in the vest majority of device ooalyses. In defining the diffusion process end in citing diffesinn examples, we have sought In em phasize the direct correlation between diffusion arid a spatial variation in particle numbers. For diffusion to occur, more of the diffusing particles must enist at one point than another points or, in methemoticot terms, there must he a nonzero concentration gradient (Vp 0 for boles, Vii ar 0 for electrons). Logically, moreover, the greater the coucentrelion gradient, the larger the expected fan of parlicles. Qeantilelive analysis of the diffusion process in deed confirms the foregoing aed leads to what is known us Pick’s lnw: = 3.2.4 Relating Diffusion Coefficients/Mobilities The diffusion ceefficients, the constants of the motion associated with diffissien, are obvi ously central parunsetees)n characterizing c-airier transport due to diffusion. Gives the im portance of the diffusion coefficieurs, one might anricipsle an extended examination of relevant properties paralleling the mobility presentation in Snbsecsieu 3.1.3. Fortunately, an extended examination is unnecessary because the D’s end the ye’s are alt iulerrnlaled. It is only necessary so establish the cosuecting fomnsute known as the Einstein relationship. In deriving the Einstein relationship, we consider a norisuifurruty doped semiconduc tor meiotaieed under equilibrium renditions. Special facts related te the sonanifnrm dop ing and the equilibrium state are invoked in the derivation. These facts, important in them selves, are reviewed prior to presenting the derivation proper. )3.lfi) —DVq where 3i is the flux or parlietes/em -sec crossing a plane perpendicular to the particle flow, 2 q is the particle concentration, and D is the diff’iusiou coefficient, a positive proporlionatity foctor. The diffusiou current density due In electrons and holes is obtained by simply mul tiplying the carrier flux by the carrier charge: Constancy ot the Fermi Level (3.17a) “miami = Consider a nondegenerate, nounsifoemly doped ri-type semiconductor ssmple, a sample where the doping concentration varies us a function of position. A concrete example of what ma hove in mind is shusvn in Pig. 3.14(o). Assuming equilibrium conditions prevail, — (3.17b) r 100 www.EasyEngineering.net nEutcounncTou FuNDAMENTALs cannien acomN the energy bond diagram characterizing the sample wit) hove the forro sketched in Fig. 3.14(b). In Chapter 2 the Fermi level in uniformly doped n-type semiconductors sees fosed In move closer and closer to E sxhee the donor doping mm systematically increased )see Fig. 2.21). Consistent with this fact, ff was drawn closer tu in going from x = 0 to x = L on tire Fig. 3.14(h) d:agrein. Conssrsction of the diagram, hoscever, contd not hove been completed mishear making use of a critical new piece of information. Specificolly, oxder eqailibriosu coridisioes, elffv/do = dff/dy = dEr/dc = 0; i.e., the Fenni level inside o moserin) am group ofrnoieriiuis in insimesie cousocs is iuvnriurss us afisuction ofposiiiou. Thr coussuocy of the Fermi level means that Er is to appear as o horizouto) linens equilib rium energy heed diagrams. /The posaioo independence of the Fermi energy is established by examining the leans- 101 for of carriers between el;osvcd crates with the same energy but at adjoarot positions in an energy band. It is concluded the probability of filling the states at a given energy,f)E), must be the same everywhere in the sample under equilibrium conditions. If Ibis wore not the ease, carriers mould preferentially transfer between states and thereby give rise to 5 net current. The existence of a set current is inconsisleor with the specified equilibrium con ditions. Referring to the Eq. (2.7) expression forf(E), we find that thp constancy of the Fernsi function is turn requires the Fermi level to be independent of pnsf?ion. Current Flom Under Equilihrium Conditions ww w.E Uuoer eqaihberusmm conditions the total current is of course identically zero. Brrunse elec tron and hole activity is totatty decoupled under equilibrium conditions, the electron and hole current densities. ,1 and J,, most also independently vanish. Setting .J = J. = 0 in Eq. (3. It), however, leads to the conclusion that the drift and diffusion currents assariated with e given corner are merely reqnimd lobe of equal mugnitude and opposite polerity. Is fact, the dnft and diffusion components wilt vanish undue eqsilibrinm conditions only if 0 and Vu Vp = 0. To provide a concrete illustration of eon-nenishieg equilibrium current components, let as retsru to en examination of the noousiformly doped semiconductor sample charec runeed by Fig. 3.14. The dopumsr variation piclured in Fiy. 3.14(a) clearly gives rise to a significant electron concentration gradient. An electron diffusion earreut flossing in the +x direction mnsl exist mime the sample. The band bending shows in the hand diagram of Pig. 3. t4)b), moreover, implies the esistence of a “built-in” electric field oriented in the x direetiun. This gives ole to u drift current also in the x dition. Netc that the drift and diffusion components are of opposite polarity. Since equilibrium cooditiom are as sumed to prevail, the components must also be of equal magnitude. In point of fact, the electric field arises inside the sesoicondactur to counteract the diffusive tendeeeies of the carriers caused by the nonuniform dapiug. The major point herein that, eves under equilib cow condition, nonuniform doping will give rise to carrier concentration gradients, a built m electric field, and non-zero current components. asy En — gin eer — L ing .ne Einstein Relstionship Eu —+------———-——-----------j--u’ S o t Having lard the proper foundation, sve can now proceed to derive the connecting formula between the D’s and the ye’s knnwu as the Einstein relationship. To simplify the develop ment, we work in only one dimension, Thr sample under analysis iu luken to he a uonde generate, sonasiformly doped semiconductor maintained nuder equilibrium conditions. Citing the fact that she net carrier eurreuls musl be identically zero nuder equilibrinm con ditions, and focusing on the electrons, we cue state )b) Figure 3.14 Nooaniformly duped sewicoodoeiav (a) essumed doping veeiaaon miih pnsiiiios: (hi eorrespsodisg equilibrium energy band diagram. iviaov + iula,n = nE + 5 qys qD4fi = 0 (3.20) www.EasyEngineering.net t www.EasyEngineering.net trw’-. - ronuu. 102 cnneinnae’non nnMIeONnttCTON FaNnAMENTAtS However, IdE, , (3.21) qdx (sanse as 3.15) and n ww Moreover, with dkr/d.n eqailibrium conditions), = (3.22) 0,1/kr 0 (dee to the positional incartanre of the Fermi level nrsder = = — dx (3.23) — kT rIo kT as y En gin e dslclr from Eq. (3.23) into Eq. (3.20). and reareongaag the reselt slightly, one obtains rials. We shonld emphasian again that the prelitoittary resnlts, sneb an the positinnal mean atice of the eqsnlibrsam Fnrnti level end the sitaation inside a nonanifoemly doped semi rondactor ander eqniliheinm eomtdilions, are important in themselves. Relative to nnntnrieaJ salary, note that kT/q is a voltage, and at room tensperalare (300 K) is eqaal to 0.025fiV. Heiten, for an Na = lola/ems Si sample maintained at room temperatame, D 5 5 (kT/q)p = )O.0259)(135fi ema/Vsee) = 35.2 em /see. Finally, the Einstein relationship is one of t the easiest nqaatinns to remember beranne it rhymes internally—D over ja rqaals fiT nver q. The rhyme holds even if the equation is ittnerled—M over D eqnals q nseç fiT Esnercinn 3.4 Pt In this eseresse we conlinne the evamination of the semieondnetor sample repre sented by the energy band diagram presented in Eaereisn 3.2. w.E Sebstitating it, etnr = 103 (qn’fl) s 1 , — (3.24) 0 (qn’O)fDv eri ng. ne Einstein relationship for electrons (b) What is the electron earrent density (J) and hole current density (J ) at a 0 (e) Roughly nketeh is and p versns = inside the sample. (d) Is there an electron diffnsion current am a = ± L/2? If there is a diffusion enrrent at a given poisst, indicate the direction of earrent floss. Since ‘6 itO (a conseqoence of the nonnoiforin doping), it follows from Eq. (3.24) that Is, (a) The semicondsetor in in nqnilibrinm. How does one dedane this fact from the given energy bnssd diagram? (3.25a) t In) Noting the solution for the electric field peesented in Enoreise 3.2, is thorn an electron drift carrent at a = 2t L/2 7 If there isa drift eamnnnt at a given point, indicate the direction of csrrnnt flow. (f) What is the hole diffusion coefficient (Dv) in thn a > L rneian of the semi rondnriar? A similm argament for holes yields St (a) The semicandoetor is concluded to be in nqnilibeinm beeanse the Fermi level is invariant as a function of position. Dr (3.25b) Einstein relationship for holes Althoogh it was established while assnming eqnitibrinm conditions, wn can present more elaborate mgaments that shove the Einstnis relationship to be valid even nnder non eqnitibrinm conditions. The nondngenernte restriction, however, sttll applies; slightly modified farms of Eqs. (3.25) resnlt when the orgament is entendnd to degenerate mate- (h) nod at both a = L/2 and a = + L/2. Thn net electron and hole earernis me always identically zero everywhere ander eqailibrinm conditions. — Ai roan inwporaiarr at’ i.a a tO°l joutn/caai = 0.0250 ,v 0.0250 V = it.f 50 t0 “))o.saaol jonle. Thur 5T/q = im.a a t0 “1)0.0250)1 - www.EasyEngineering.net 104 aesilcoNnnCron raNnaMEMTAtS (e) Since it = n,espfrEr — eAnesen AcTION - E)/kT( and p = nrspRE = Er)/hTf. we coorlede 3.3 RECOMBINATION-GENERAT1ON 3.3.1 flefiniticn—Visualization )Log scala) When a sentiroisdertor is pcrtaebed from the eqnitibrinm stote, an caress or deficit in the carrier concentrations relative to their eqnitibriatn salons is iisvaniably created inside the semicoddnctor. Kecomhination—gnneeatinn (R—G) is namer’s order-restoring mechanism, the means whereby the carrier caress or deficit inside the snmieendactnr in atabitiand (if the pertarbation is maintained) or eliminated (if the pertarbation in removed). Since non eqailibriam conditions prevail doning device operation, rerombination—generation mono often than not plays a major rote in shaping the characteristics eahibited by a device. For mally, rerombination and generation ran be defined as follows: —L L Rerowb/nation—a process whereby electrons and holes (carriers) are arnihitated or destroyed. + L12. From the L12 and .n Id) There is an electron diffasinti csrrent at both it = answer to the preceding qneslion we note dsat dn/dv it 0 at the cited points. With dn/rdv>0, J. 0 at it = L12 flows hi the +x direction. Conversely, c/n/d.c <Oat L12 and J, 5 at this point flows in the a direction. — Gennrarioo—a procesa whereby electrons and holes are created. — — (o) Therein an elnrtcois drift corretti at both a = LI 2 and a = +L12. Since both it and ‘6 am non-zero at a = ± L12, it follows that J 11 = wa 0. The drift 5 n’S component of the enreent always has the same direction as the electric field; is in the —a direction at a = L/2 and in the +.r direction at a = +L/2. The drift component of the carrent mast of coarse caecrl the diffosion component of the carroot so that 55 = + sIav = 0 under cqaitibninm conditions. The diractisin related ansssers to parts (dl and (e), snmmarizvd nest, arc consistent with this — Unlike drift and diffasion, the terms reronibinutios and grnrration dn net refen to a single process. Rather, they are collective names for a grnnp of similar processes; carriers can be created and destroyed within a nemirondeclor in a nambee of ways. The most common R—G processns are visnaliand in Pig. 3.15. The individaal processes are described and discassed neat. — requiwmeot; it -‘elan —L/2 2 n+L/ Band-la-Band Recambination - Baud-to-band rerombinatiots is eonceptnally the simplest of all encombinalion processes. As pirtared in Fig. 3.15(a). it merely involves the direct annihilation of a enodartian band electron and a valence band hole, An electron and hate loosing in the sewicondactar lattice stray into 1hz same spatial vicinity and eap)—llte electron and hole annihilate each other The oseess energy released dnrinp the process typically goes into the peodaction of a pho ton (light). — vla’,a 1 If) lv working part Id) of Esrrcise 3.2, we cooctaded the a > L region of the setei condaclor (Si, 300 K) had a doping of NA w 5 X 5 1cm and a corresponding 1 l0’ hole mobility of , = 459 cmi/Vscc. Thas. employing the Einstein relationship, = (hTIq)pu = (0 0259)(459) = r(Tg emnIsec. R—G Cenler Recombinalion The process pietared in Fig. 3.15(b) involves a “third panty,” or intermediary, and takns place only at special locations wittsin the sewicoisdactor known as k—S renters. Plsysically. K—S centcrs arc lattice defecis or special impnrity atoms anch as gold in Si. Lattice defects and the special atooss in the form of nnintentionat iwparities arc present even in scmiean dartara of the higltest available pneity. The K—C center eancnntration, howcver, is oartnally ocry low compared so tIme acerptcsr and donar concentrations in des)ce-qnality materials. The most important propcrty of the K—C centers is the introdnetion of allowed electronic levels nmr the center of the band gap. These levels are identified by the th r energy label in Fig. 3.15(b). Thr near midgap positioning of the levels is alt-important becanse it disrin gn)shes K—S centers from donors and acceptors. The inidgap levels iotrodacnd by select K—C eerier imparities in Si are snmmariacd in Fig. 3.16. 105 trw’-. www.EasyEngineering.net - ronuu. 102 cnneinnae’non nnMIeONnttCTON FaNnAMENTAtS However, IdE, , (3.21) qdx (sanse as 3.15) and n Moreover, with dkr/d.n eqailibrium conditions), = rials. We shonld emphasian again that the prelitoittary resnlts, sneb an the positinnal mean atice of the eqsnlibrsam Fnrnti level end the sitaation inside a nonanifoemly doped semi rondactor ander eqniliheinm eomtdilions, are important in themselves. Relative to nnntnrieaJ salary, note that kT/q is a voltage, and at room tensperalare (300 K) is eqaal to 0.025fiV. Heiten, for an Na = lola/ems Si sample maintained at room temperatame, D 5 5 (kT/q)p = )O.0259)(135fi ema/Vsee) = 35.2 em /see. Finally, the Einstein relationship is one of t the easiest nqaatinns to remember beranne it rhymes internally—D over ja rqaals fiT nver q. The rhyme holds even if the equation is ittnerled—M over D eqnals q nseç fiT (3.22) 0,1/kr 0 (dee to the positional incartanre of the Fermi level nrsder ww Esnercinn 3.4 Pt In this eseresse we conlinne the evamination of the semieondnetor sample repre sented by the energy band diagram presented in Eaereisn 3.2. = = — dx Sebstitating it, etnr = 103 (3.23) — kT rIo kT dslclr from Eq. (3.23) into Eq. (3.20). and reareongaag the reselt slightly, one obtains (qn’fl) s 1 , — (3.24) 0 (qn’O)fDv Since ‘6 itO (a conseqoence of the nonnoiforin doping), it follows from Eq. (3.24) that Einstein relationship for electrons (3.25a) Is, w.E a (a) The semicondsetor in in nqnilibrinm. How does one dedane this fact from the given energy bnssd diagram? syE ngi (b) What is the electron earrent density (J) and hole current density (J ) at a 0 (e) Roughly nketeh is and p versns = inside the sample. nee r (d) Is there an electron diffnsion current am a = ± L/2? If there is a diffusion enrrent at a given poisst, indicate the direction of earrent floss. ing . In) Noting the solution for the electric field peesented in Enoreise 3.2, is thorn an electron drift carrent at a = 2t L/2 7 If there isa drift eamnnnt at a given point, indicate the direction of csrrnnt flow. net (f) What is the hole diffusion coefficient (Dv) in thn a > L rneian of the semi rondnriar? A similm argament for holes yields St (a) The semicandoetor is concluded to be in nqnilibeinm beeanse the Fermi level is invariant as a function of position. Dr (3.25b) Einstein relationship for holes Althoogh it was established while assnming eqnitibrinm conditions, wn can present more elaborate mgaments that shove the Einstnis relationship to be valid even nnder non eqnitibrinm conditions. The nondngenernte restriction, however, sttll applies; slightly modified farms of Eqs. (3.25) resnlt when the orgament is entendnd to degenerate mate- (h) nod at both a = L/2 and a = + L/2. Thn net electron and hole earernis me always identically zero everywhere ander eqailibrinm conditions. — Ai roan inwporaiarr at’ i.a a tO°l joutn/caai = 0.0250 ,v 0.0250 V = it.f 50 t0 “))o.saaol jonle. Thur 5T/q = im.a a t0 “1)0.0250)1 - www.EasyEngineering.net 104 aesilcoNnnCron raNnaMEMTAtS (e) Since it = n,espfrEr — eAnesen AcTION - E)/kT( and p = nrspRE = Er)/hTf. we coorlede 3.3 RECOMBINATION-GENERAT1ON 3.3.1 flefiniticn—Visualization )Log scala) When a sentiroisdertor is pcrtaebed from the eqnitibrinm stote, an caress or deficit in the carrier concentrations relative to their eqnitibriatn salons is iisvaniably created inside the semicoddnctor. Kecomhination—gnneeatinn (R—G) is namer’s order-restoring mechanism, the means whereby the carrier caress or deficit inside the snmieendactnr in atabitiand (if the pertarbation is maintained) or eliminated (if the pertarbation in removed). Since non eqailibriam conditions prevail doning device operation, rerombination—generation mono often than not plays a major rote in shaping the characteristics eahibited by a device. For mally, rerombination and generation ran be defined as follows: —L L Rerowb/nation—a process whereby electrons and holes (carriers) are arnihitated or destroyed. + L12. From the L12 and .n Id) There is an electron diffasinti csrrent at both it = answer to the preceding qneslion we note dsat dn/dv it 0 at the cited points. With dn/rdv>0, J. 0 at it = L12 flows hi the +x direction. Conversely, c/n/d.c <Oat L12 and J, 5 at this point flows in the a direction. — Gennrarioo—a procesa whereby electrons and holes are created. — — (o) Therein an elnrtcois drift corretti at both a = LI 2 and a = +L12. Since both it and ‘6 am non-zero at a = ± L12, it follows that J 11 = wa 0. The drift 5 n’S component of the enreent always has the same direction as the electric field; is in the —a direction at a = L/2 and in the +.r direction at a = +L/2. The drift component of the carrent mast of coarse caecrl the diffosion component of the carroot so that 55 = + sIav = 0 under cqaitibninm conditions. The diractisin related ansssers to parts (dl and (e), snmmarizvd nest, arc consistent with this — Unlike drift and diffasion, the terms reronibinutios and grnrration dn net refen to a single process. Rather, they are collective names for a grnnp of similar processes; carriers can be created and destroyed within a nemirondeclor in a nambee of ways. The most common R—G processns are visnaliand in Pig. 3.15. The individaal processes are described and discassed neat. — requiwmeot; it -‘elan —L/2 2 n+L/ Band-la-Band Recambination - Baud-to-band rerombinatiots is eonceptnally the simplest of all encombinalion processes. As pirtared in Fig. 3.15(a). it merely involves the direct annihilation of a enodartian band electron and a valence band hole, An electron and hate loosing in the sewicondactar lattice stray into 1hz same spatial vicinity and eap)—llte electron and hole annihilate each other The oseess energy released dnrinp the process typically goes into the peodaction of a pho ton (light). — vla’,a 1 If) lv working part Id) of Esrrcise 3.2, we cooctaded the a > L region of the setei condaclor (Si, 300 K) had a doping of NA w 5 X 5 1cm and a corresponding 1 l0’ hole mobility of , = 459 cmi/Vscc. Thas. employing the Einstein relationship, = (hTIq)pu = (0 0259)(459) = r(Tg emnIsec. R—G Cenler Recombinalion The process pietared in Fig. 3.15(b) involves a “third panty,” or intermediary, and takns place only at special locations wittsin the sewicoisdactor known as k—S renters. Plsysically. K—S centcrs arc lattice defecis or special impnrity atoms anch as gold in Si. Lattice defects and the special atooss in the form of nnintentionat iwparities arc present even in scmiean dartara of the higltest available pneity. The K—C center eancnntration, howcver, is oartnally ocry low compared so tIme acerptcsr and donar concentrations in des)ce-qnality materials. The most important propcrty of the K—C centers is the introdnetion of allowed electronic levels nmr the center of the band gap. These levels are identified by the th r energy label in Fig. 3.15(b). Thr near midgap positioning of the levels is alt-important becanse it disrin gn)shes K—S centers from donors and acceptors. The inidgap levels iotrodacnd by select K—C eerier imparities in Si are snmmariacd in Fig. 3.16. 105 trw’-. - ronuu. 102 cnneinnae’non nnMIeONnttCTON FaNnAMENTAtS However, IdE, , (3.21) qdx (sanse as 3.15) and n Moreover, with dkr/d.n eqailibrium conditions), = rials. We shonld emphasian again that the prelitoittary resnlts, sneb an the positinnal mean atice of the eqsnlibrsam Fnrnti level end the sitaation inside a nonanifoemly doped semi rondactor ander eqniliheinm eomtdilions, are important in themselves. Relative to nnntnrieaJ salary, note that kT/q is a voltage, and at room tensperalare (300 K) is eqaal to 0.025fiV. Heiten, for an Na = lola/ems Si sample maintained at room temperatame, D 5 5 (kT/q)p = )O.0259)(135fi ema/Vsee) = 35.2 em /see. Finally, the Einstein relationship is one of t the easiest nqaatinns to remember beranne it rhymes internally—D over ja rqaals fiT nver q. The rhyme holds even if the equation is ittnerled—M over D eqnals q nseç fiT (3.22) 0,1/kr 0 (dee to the positional incartanre of the Fermi level nrsder Esnercinn 3.4 Pt In this eseresse we conlinne the evamination of the semieondnetor sample repre sented by the energy band diagram presented in Eaereisn 3.2. = = — dx Sebstitating it, etnr = 103 (3.23) — kT rIo kT dslclr from Eq. (3.23) into Eq. (3.20). and reareongaag the reselt slightly, one obtains (qn’fl) s 1 , — (3.24) 0 (qn’O)fDv Since ‘6 itO (a conseqoence of the nonnoiforin doping), it follows from Eq. (3.24) that (3.25a) Einstein relationship for electrons Is, (a) The semicondsetor in in nqnilibrinm. How does one dedane this fact from the given energy bnssd diagram? (b) What is the electron earrent density (J) and hole current density (J ) at a 0 (e) Roughly nketeh is and p versns = inside the sample. (d) Is there an electron diffnsion current am a = ± L/2? If there is a diffusion enrrent at a given poisst, indicate the direction of earrent floss. In) Noting the solution for the electric field peesented in Enoreise 3.2, is thorn an electron drift carrent at a = 2t L/2 7 If there isa drift eamnnnt at a given point, indicate the direction of csrrnnt flow. (f) What is the hole diffusion coefficient (Dv) in thn a > L rneian of the semi rondnriar? A similm argament for holes yields St (a) The semicandoetor is concluded to be in nqnilibeinm beeanse the Fermi level is invariant as a function of position. Dr (3.25b) Einstein relationship for holes Althoogh it was established while assnming eqnitibrinm conditions, wn can present more elaborate mgaments that shove the Einstnis relationship to be valid even nnder non eqnitibrinm conditions. The nondngenernte restriction, however, sttll applies; slightly modified farms of Eqs. (3.25) resnlt when the orgament is entendnd to degenerate mate- (h) nod at both a = L/2 and a = + L/2. Thn net electron and hole earernis me always identically zero everywhere ander eqailibrinm conditions. — Ai roan inwporaiarr at’ i.a a tO°l joutn/caai = 0.0250 ,v 0.0250 V = it.f 50 t0 “))o.saaol jonle. Thur 5T/q = im.a a t0 “1)0.0250)1 - www.EasyEngineering.net 104 aesilcoNnnCron raNnaMEMTAtS (e) Since it = n,espfrEr — eAnesen AcTION - E)/kT( and p = nrspRE = Er)/hTf. we coorlede 3.3 RECOMBINATION-GENERAT1ON 3.3.1 flefiniticn—Visualization )Log scala) When a sentiroisdertor is pcrtaebed from the eqnitibrinm stote, an caress or deficit in the ww w carrier concentrations relative to their eqnitibriatn salons is iisvaniably created inside the semicoddnctor. Kecomhination—gnneeatinn (R—G) is namer’s order-restoring mechanism, the means whereby the carrier caress or deficit inside the snmieendactnr in atabitiand (if the pertarbation is maintained) or eliminated (if the pertarbation in removed). Since non eqailibriam conditions prevail doning device operation, rerombination—generation mono often than not plays a major rote in shaping the characteristics eahibited by a device. For mally, rerombination and generation ran be defined as follows: —L .Ea L Rerowb/nation—a process whereby electrons and holes (carriers) are arnihitated or destroyed. + L12. From the L12 and .n Id) There is an electron diffasinti csrrent at both it = answer to the preceding qneslion we note dsat dn/dv it 0 at the cited points. With dn/rdv>0, J. 0 at it = L12 flows hi the +x direction. Conversely, c/n/d.c <Oat L12 and J, 5 at this point flows in the a direction. — syE — ngi (o) Therein an elnrtcois drift corretti at both a = LI 2 and a = +L12. Since both it and ‘6 am non-zero at a = ± L12, it follows that J 11 = wa 0. The drift 5 n’S component of the enreent always has the same direction as the electric field; is in the —a direction at a = L/2 and in the +.r direction at a = +L/2. The drift component of the carrent mast of coarse caecrl the diffosion component of the carroot so that 55 = + sIav = 0 under cqaitibninm conditions. The diractisin related ansssers to parts (dl and (e), snmmarizvd nest, arc consistent with this — — requiwmeot; it -‘elan Gennrarioo—a procesa whereby electrons and holes are created. — —L/2 nee rin g 2 n+L/ .ne t Unlike drift and diffasion, the terms reronibinutios and grnrration dn net refen to a single process. Rather, they are collective names for a grnnp of similar processes; carriers can be created and destroyed within a nemirondeclor in a nambee of ways. The most common R—G processns are visnaliand in Pig. 3.15. The individaal processes are described and discassed neat. Band-la-Band Recambination - Baud-to-band rerombinatiots is eonceptnally the simplest of all encombinalion processes. As pirtared in Fig. 3.15(a). it merely involves the direct annihilation of a enodartian band electron and a valence band hole, An electron and hate loosing in the sewicondactar lattice stray into 1hz same spatial vicinity and eap)—llte electron and hole annihilate each other The oseess energy released dnrinp the process typically goes into the peodaction of a pho ton (light). — R—G Cenler Recombinalion vla’,a 1 If) lv working part Id) of Esrrcise 3.2, we cooctaded the a > L region of the setei condaclor (Si, 300 K) had a doping of NA w 5 X 5 1cm and a corresponding 1 l0’ hole mobility of , = 459 cmi/Vscc. Thas. employing the Einstein relationship, = (hTIq)pu = (0 0259)(459) = r(Tg emnIsec. www.EasyEngineering.net The process pietared in Fig. 3.15(b) involves a “third panty,” or intermediary, and takns place only at special locations wittsin the sewicoisdactor known as k—S renters. Plsysically. K—S centcrs arc lattice defecis or special impnrity atoms anch as gold in Si. Lattice defects and the special atooss in the form of nnintentionat iwparities arc present even in scmiean dartara of the higltest available pneity. The K—C center eancnntration, howcver, is oartnally ocry low compared so tIme acerptcsr and donar concentrations in des)ce-qnality materials. The most important propcrty of the K—C centers is the introdnetion of allowed electronic levels nmr the center of the band gap. These levels are identified by the th r energy label in Fig. 3.15(b). Thr near midgap positioning of the levels is alt-important becanse it disrin gn)shes K—S centers from donors and acceptors. The inidgap levels iotrodacnd by select K—C eerier imparities in Si are snmmariacd in Fig. 3.16. 105 trw’-. - ronuu. 102 cnneinnae’non nnMIeONnttCTON FaNnAMENTAtS However, IdE, , (3.21) qdx (sanse as 3.15) and n Moreover, with dkr/d.n eqailibrium conditions), = rials. We shonld emphasian again that the prelitoittary resnlts, sneb an the positinnal mean atice of the eqsnlibrsam Fnrnti level end the sitaation inside a nonanifoemly doped semi rondactor ander eqniliheinm eomtdilions, are important in themselves. Relative to nnntnrieaJ salary, note that kT/q is a voltage, and at room tensperalare (300 K) is eqaal to 0.025fiV. Heiten, for an Na = lola/ems Si sample maintained at room temperatame, D 5 5 (kT/q)p = )O.0259)(135fi ema/Vsee) = 35.2 em /see. Finally, the Einstein relationship is one of t the easiest nqaatinns to remember beranne it rhymes internally—D over ja rqaals fiT nver q. The rhyme holds even if the equation is ittnerled—M over D eqnals q nseç fiT (3.22) 0,1/kr 0 (dee to the positional incartanre of the Fermi level nrsder Esnercinn 3.4 Pt In this eseresse we conlinne the evamination of the semieondnetor sample repre sented by the energy band diagram presented in Eaereisn 3.2. = = — dx Sebstitating it, etnr = 103 (3.23) — kT rIo kT dslclr from Eq. (3.23) into Eq. (3.20). and reareongaag the reselt slightly, one obtains (qn’fl) s 1 , — (3.24) 0 (qn’O)fDv Since ‘6 itO (a conseqoence of the nonnoiforin doping), it follows from Eq. (3.24) that Einstein relationship for electrons (3.25a) Is, (a) The semicondsetor in in nqnilibrinm. How does one dedane this fact from the given energy bnssd diagram? (b) What is the electron earrent density (J) and hole current density (J ) at a 0 (e) Roughly nketeh is and p versns = inside the sample. (d) Is there an electron diffnsion current am a = ± L/2? If there is a diffusion enrrent at a given poisst, indicate the direction of earrent floss. In) Noting the solution for the electric field peesented in Enoreise 3.2, is thorn an electron drift carrent at a = 2t L/2 7 If there isa drift eamnnnt at a given point, indicate the direction of csrrnnt flow. (f) What is the hole diffusion coefficient (Dv) in thn a > L rneian of the semi rondnriar? A similm argament for holes yields St (a) The semicandoetor is concluded to be in nqnilibeinm beeanse the Fermi level is invariant as a function of position. Dr (3.25b) Einstein relationship for holes Althoogh it was established while assnming eqnitibrinm conditions, wn can present more elaborate mgaments that shove the Einstnis relationship to be valid even nnder non eqnitibrinm conditions. The nondngenernte restriction, however, sttll applies; slightly modified farms of Eqs. (3.25) resnlt when the orgament is entendnd to degenerate mate- (h) nod at both a = L/2 and a = + L/2. Thn net electron and hole earernis me always identically zero everywhere ander eqailibrinm conditions. — Ai roan inwporaiarr at’ i.a a tO°l joutn/caai = 0.0250 ,v 0.0250 V it.f = 50 t0 “))o.saaol jonle. Thur 5T/q = im.a a t0 “1)0.0250)1 - www.EasyEngineering.net 104 aesilcoNnnCron raNnaMEMTAtS (e) Since it = n,espfrEr — 105 eAnesen AcTION - E)/kT( and p = nrspRE = Er)/hTf. we coorlede 3.3 RECOMBINATION-GENERAT1ON 3.3.1 flefiniticn—Visualization )Log scala) When a sentiroisdertor is pcrtaebed from the eqnitibrinm stote, an caress or deficit in the carrier concentrations relative to their eqnitibriatn salons is iisvaniably created inside the semicoddnctor. Kecomhination—gnneeatinn (R—G) is namer’s order-restoring mechanism, the means whereby the carrier caress or deficit inside the snmieendactnr in atabitiand (if the pertarbation is maintained) or eliminated (if the pertarbation in removed). Since non eqailibriam conditions prevail doning device operation, rerombination—generation mono often than not plays a major rote in shaping the characteristics eahibited by a device. For mally, rerombination and generation ran be defined as follows: —L L ww w.E Rerowb/nation—a process whereby electrons and holes (carriers) are arnihitated or destroyed. + L12. From the L12 and .n Id) There is an electron diffasinti csrrent at both it = answer to the preceding qneslion we note dsat dn/dv it 0 at the cited points. With dn/rdv>0, J. 0 at it = L12 flows hi the +x direction. Conversely, c/n/d.c <Oat L12 and J, 5 at this point flows in the a direction. — — — (o) Therein an elnrtcois drift corretti at both a = LI 2 and a = +L12. Since both it and ‘6 am non-zero at a = ± L12, it follows that J 11 = wa 0. The drift 5 n’S component of the enreent always has the same direction as the electric field; is in the —a direction at a = L/2 and in the +.r direction at a = +L/2. The drift component of the carrent mast of coarse caecrl the diffosion component of the carroot so that 55 = + sIav = 0 under cqaitibninm conditions. The diractisin related ansssers to parts (dl and (e), snmmarizvd nest, arc consistent with this — Gennrarioo—a procesa whereby electrons and holes are created. asy Unlike drift and diffasion, the terms reronibinutios and grnrration dn net refen to a single process. Rather, they are collective names for a grnnp of similar processes; carriers can be created and destroyed within a nemirondeclor in a nambee of ways. The most common R—G processns are visnaliand in Pig. 3.15. The individaal processes are described and discassed neat. En — requiwmeot; it -‘elan —L/2 2 n+L/ Band-la-Band Recambination If) lv working part Id) of Esrrcise 3.2, we cooctaded the a > L region of the setei condaclor (Si, 300 K) had a doping of NA w 5 X 5 1cm and a corresponding 1 l0’ hole mobility of , = 459 cmi/Vscc. Thas. employing the Einstein relationship, = (hTIq)pu = (0 0259)(459) = r(Tg emnIsec. eer - ing Baud-to-band rerombinatiots is eonceptnally the simplest of all encombinalion processes. As pirtared in Fig. 3.15(a). it merely involves the direct annihilation of a enodartian band electron and a valence band hole, An electron and hate loosing in the sewicondactar lattice stray into 1hz same spatial vicinity and eap)—llte electron and hole annihilate each other The oseess energy released dnrinp the process typically goes into the peodaction of a pho ton (light). — vla’,a 1 gin .ne R—G Cenler Recombinalion The process pietared in Fig. 3.15(b) involves a “third panty,” or intermediary, and takns place only at special locations wittsin the sewicoisdactor known as k—S renters. Plsysically. K—S centcrs arc lattice defecis or special impnrity atoms anch as gold in Si. Lattice defects and the special atooss in the form of nnintentionat iwparities arc present even in scmiean dartara of the higltest available pneity. The K—C center eancnntration, howcver, is oartnally ocry low compared so tIme acerptcsr and donar concentrations in des)ce-qnality materials. The most important propcrty of the K—C centers is the introdnetion of allowed electronic levels nmr the center of the band gap. These levels are identified by the th r energy label in Fig. 3.15(b). Thr near midgap positioning of the levels is alt-important becanse it disrin gn)shes K—S centers from donors and acceptors. The inidgap levels iotrodacnd by select K—C eerier imparities in Si are snmmariacd in Fig. 3.16. www.EasyEngineering.net t Thermal www.EasyEngineering.net 106 r nueicosuncvon FasuneeNyALs eanetun -t Light RJJ (d) Band-to-band generation As enorgy w.E Midgap a.. (a) tdand-io.ha recoinbinaflon ww 107 . Thermal enorgy E, acTioN Cs Mn Cr Fe Figure 3.16 Neac-midgap osergy tnsnls ininodnend by some cnmmnn impooties in Si. When an impnri’y introduces maltipln tnsnts, one sf the tesets tends to dominate in a given aemicondactor sample. Themmal energy Auger Recombinetion (hi E—G coitier eecombinnaeo as y En gin e (ci R—G center generaaon In the Anger (pronounced Gb-jay) process piclsred in Fig. 3.15(c), band-to-band cecombt notion occars simaltaneousty wilh the cottiainn between two like carriers. The energy re leased by the recombination is transferred dnring the colliainn to the surviving cnrriec This highly energetic carrier snbseqaenlty “thertnaticev”—loses energy in small steps throagh heat-prodncing collisions with the ncosicondnctoc lattice. The “staircme” in Fig. 3.15(c) represents the envisioned vtepwise loss of energy. Generstion Processes eri Any of the foregoing recombinamion processes con be reversed to generate corners. Bandto-band generation, where an etcclroe is excited directly from the valence band into the condoction band, is pictnred in Fig. 3.15(d). Note that either thermal energy or tight can provide the energy required for the bend-to-band transition. If thermal energy is absorbed, the process is alternatively referred teas direct rhertnol generation; if externally introdnced light iv absorbed, the process is called photogetseration. The thermally assisted generation of carriers with R—G centers acting as intermediaries is envisioned in Fig. 3.15(e). Finally, impact ionicntion, the inverse of Anger recombinolion, is viouolieed in Ftg. 3.15(f). In lhts process an electron—hale pnir is pradaced as a cesnlt of energy released vvheu a highly energetic cornier collides with the crystal lattice. The generation of carriers throogh impact ionieation routinely occars in the high B -field regions of devices. We will have more to say abnat this process when treating breakdown in pn janctions. ng. ne t (e) Ao er vecowbinomioo 0 (0 Cawiergenernm via impact ionization Figure 3.15 Energy hand visuotieatioo of recombination and generutioe processes As ceted in Fig. 3.15(h), recombjnatjon at on R—G center is a two-step process. First, eec type of carrier, say an electron, strays into the Vicinity of on R—G center, is canght by the potential well associated with the center, loses energy, end is trapped Snhseqneetiy, hole comes along, is attracted to the trapped electron, loses energy, and aesihilates the electron within the center. Alternatively, as also shown in Fig. 3.15(b), one can thick of the electron as losing energy a second time and annihilating the hole in the satence band. R—G center recowbinalion also called indirect rocnnthinotion typically releases thermal energy (heat) doring the process or, eqnisatenlly, produces lattice vibrations 3.3,2 Momentum Considerstions All of the varioss recombination—generatinn procmses occur at all times in all seottcon doctors—evon nnder eqoilibriam conditions. The critical issue in not whether the processes are occnrring, hot rather, the rates at which the various processes arc occurring. Typically, one need be concerned only with the dominant prncess, the process proceeding at the fastest rate. A number of the proemses are important only nader apecint conditions or are highly improbable, occurring at a mach slower rate than competing processes. Anger recombinn www.EasyEngineering.net r 108 neetcoNnucvon FonnaeusvaLs eeenieencnlos tion provides a cane in point. Becanse the catcher of carrier-carrier collisions increases with titcreased cacrier concentration, the freqnency of Anger recombinatine likewise in creases with carrier concentration. Anger recombinatien mast be considered, for ecamplc, in treating highly doped regions of o device stractare, bat it is asnally negligible otherwise. Similarly, significant impact ionication occnrs only in the high B-field regions of a device. In a somewhat different vein, phntogeneratinn at room temperatare becomes n significant process only when the semicondector is cxpnsed to external illominatios. What then is the R—G process pair desersing of special attention, the process pair that typically dominates in the lcw B -field regions of a nondegenerntety doped semicondactor maintained at room temperatore? From the information prnvided, the choice is obvionsly between thermal band-to-band k—G and recombination—generation via R—G centers. From the energy band explanation alone one might specatete that band-to-band cecombination—generation wanld dominate ander the cited “standard” conditions. How ever, visaatieation of R—G processes nsing the energy band diagram can be mistnndisg. The F—n plot examines only changes in energy, whereas crystal motoestum in additiott to eneegy mast be conserved in any tZ—G process. Momentom conservation ceqnirements, as it tnrns out, ploy an important role in setting the process rare. As first noted in Snbseciien 2.2.3. the momentsm of an electron in an energy band, like the clectroti energy, can assame only certain qnanticcd values. Momenlam-related as pects of R—G prcccsscs are conveniently discasoed with the aid of plots where the allowed electron energies in the condoctinn and valcitce bands are plotted versas the allowed mo mentom. These are referred to as dC—k plots, where k is a parameter proportional to the electron crystal momentum. The F—k pInts associated with semicondactors fall into two grn&dIcategcrieiJthe first, sketched in Fig. 3.l7(a), both the minimum condnction baud ecergy and maximarn valence band energy occar at k = 0. In the second, pictnred in Fig. 3.17(b), the condoction band minimam is displaced took a 0. Semiconductors eshib iting the fortoer type of plot are referred to as dirvcr seinicondornors, and semicondnctors exhibiting the latter type of plot, as indirect semiconductors. GaAs is a notabte member of thc dircet setoicondnctor family; Ge and Si nrc both indirect semictundactors. lot Direct inwiecodarier Figure 3.17 tbl todisromewiceodacror General forms of Id—h plots for direct avd indirect semicondocioo. Phosss(s( Wm (a) Direct eroicondacior Figure 3.18 F—k plot I tat tedireci senienedanior visaatiaations of eecembinotinn in dirmi and indirect semiconductors. To make nse of the F—k plots in visnalicing an R—G process, one needs to know the noince of transitions associated with the obsorptien or emission of photons (light) and lat tice vibration qnanta called phonom. Photons, being mmslcns entities, carry very little momentnm, and a photon-assisted transition is essentially vertical on the F—k plot. Con versely, the thermal energy associated with lattice vibmtiona (phonous) is very small (in the 10—50 meV range), whereas the phonon momeutam is cnmparatively large. Than on an F—k plot a phonon-asnisted transition in essentially horleontal. It is also important to point out that, as pictured in Fig. 3.11, electrons and holes normally only occupy staten very close to the c minimom and E maximum, respectively. Thin is of coarse consistent with oar earlier discnssiou of the dinlnibation of carriers in the bands. Let us now specifically re-examine the band-to-band recombinanion process. In a direct nemicondnctor where the k-vnlnes of electrons and holes are all bnuched neon k = 0, little change in momentam is reqaired for the recombination process to proceed. The conserva tion of both energy and momenmm in readily met simply by the emission of a photon (see Fig. 3.110). In on indirect nemicondoclor, on the other bond, therein a large change in momentnm associated with the recombination process. The emission of a photon will con serve ettergy but cannot aimaltaneonsly conserve momentam. Thus foe band-to-band cccombination to proceed in an indirect nemicondoctor, the emission of a photon mnnt be accompanied by the emission or absorption nf a phonon (see Fig. 3.1 fib). The rather involved natore of the hood-to-bond procens in indirect semiconductors anderstandably leads to a vastly diminished recosabinotion raIn. Bond-to-band recombina lion in in fact totally negligible compared to R—G center recnmbination in Si and other indirect semicondnctoca. Band-to-band recombinotion does proceed at a much foster rate in direct semicandoctors and is the process prodacing the light observed from LEDs and jonctioo lasers. Even in direct materials, however, the R—G center mechanism in often the dominant process. Given the universal importance of the R—G center process, and the fact that most devices ore made from Si, which in an indirect material, the q000titutive consid erations in the next snbaecmion ore devoted primarily to the R—G center mechanism. Giber processes are considered as the need arises. 109 Thermal 106 www.EasyEngineering.net r nueicosuncvon FasuneeNyALs eanetun -t Light RJJ (d) Band-to-band generation As enorgy (hi E—G coitier eecombinnaeo Midgap a.. (a) tdand-io.ha recoinbinaflon 107 . Thermal enorgy E, acTioN Cs Mn Cr Fe Figure 3.16 Neac-midgap osergy tnsnls ininodnend by some cnmmnn impooties in Si. When an impnri’y introduces maltipln tnsnts, one sf the tesets tends to dominate in a given aemicondactor sample. ww Themmal energy w.E a Auger Recombinetion (ci R—G center generaaon In the Anger (pronounced Gb-jay) process piclsred in Fig. 3.15(c), band-to-band cecombt notion occars simaltaneousty wilh the cottiainn between two like carriers. The energy re leased by the recombination is transferred dnring the colliainn to the surviving cnrriec This highly energetic carrier snbseqaenlty “thertnaticev”—loses energy in small steps throagh heat-prodncing collisions with the ncosicondnctoc lattice. The “staircme” in Fig. 3.15(c) represents the envisioned vtepwise loss of energy. Generstion Processes syE ngi nee r Any of the foregoing recombinamion processes con be reversed to generate corners. Bandto-band generation, where an etcclroe is excited directly from the valence band into the condoction band, is pictnred in Fig. 3.15(d). Note that either thermal energy or tight can provide the energy required for the bend-to-band transition. If thermal energy is absorbed, the process is alternatively referred teas direct rhertnol generation; if externally introdnced light iv absorbed, the process is called photogetseration. The thermally assisted generation of carriers with R—G centers acting as intermediaries is envisioned in Fig. 3.15(e). Finally, impact ionicntion, the inverse of Anger recombinolion, is viouolieed in Ftg. 3.15(f). In lhts process an electron—hale pnir is pradaced as a cesnlt of energy released vvheu a highly energetic cornier collides with the crystal lattice. The generation of carriers throogh impact ionieation routinely occars in the high B -field regions of devices. We will have more to say abnat this process when treating breakdown in pn janctions. ing . (e) Ao er vecowbinomioo 0 (0 Cawiergenernm via impact ionization Figure 3.15 Energy hand visuotieatioo of recombination and generutioe processes As ceted in Fig. 3.15(h), recombjnatjon at on R—G center is a two-step process. First, eec type of carrier, say an electron, strays into the Vicinity of on R—G center, is canght by the potential well associated with the center, loses energy, end is trapped Snhseqneetiy, hole comes along, is attracted to the trapped electron, loses energy, and aesihilates the electron within the center. Alternatively, as also shown in Fig. 3.15(b), one can thick of the electron as losing energy a second time and annihilating the hole in the satence band. R—G center recowbinalion also called indirect rocnnthinotion typically releases thermal energy (heat) doring the process or, eqnisatenlly, produces lattice vibrations net 3.3,2 Momentum Considerstions All of the varioss recombination—generatinn procmses occur at all times in all seottcon doctors—evon nnder eqoilibriam conditions. The critical issue in not whether the processes are occnrring, hot rather, the rates at which the various processes arc occurring. Typically, one need be concerned only with the dominant prncess, the process proceeding at the fastest rate. A number of the proemses are important only nader apecint conditions or are highly improbable, occurring at a mach slower rate than competing processes. Anger recombinn www.EasyEngineering.net r 108 neetcoNnucvon FonnaeusvaLs eeenieencnlos tion provides a cane in point. Becanse the catcher of carrier-carrier collisions increases with titcreased cacrier concentration, the freqnency of Anger recombinatine likewise in creases with carrier concentration. Anger recombinatien mast be considered, for ecamplc, in treating highly doped regions of o device stractare, bat it is asnally negligible otherwise. Similarly, significant impact ionication occnrs only in the high B-field regions of a device. In a somewhat different vein, phntogeneratinn at room temperatare becomes n significant process only when the semicondector is cxpnsed to external illominatios. What then is the R—G process pair desersing of special attention, the process pair that typically dominates in the lcw B -field regions of a nondegenerntety doped semicondactor maintained at room temperatore? From the information prnvided, the choice is obvionsly between thermal band-to-band k—G and recombination—generation via R—G centers. From the energy band explanation alone one might specatete that band-to-band cecombination—generation wanld dominate ander the cited “standard” conditions. How ever, visaatieation of R—G processes nsing the energy band diagram can be mistnndisg. The F—n plot examines only changes in energy, whereas crystal motoestum in additiott to eneegy mast be conserved in any tZ—G process. Momentom conservation ceqnirements, as it tnrns out, ploy an important role in setting the process rare. As first noted in Snbseciien 2.2.3. the momentsm of an electron in an energy band, like the clectroti energy, can assame only certain qnanticcd values. Momenlam-related as pects of R—G prcccsscs are conveniently discasoed with the aid of plots where the allowed electron energies in the condoctinn and valcitce bands are plotted versas the allowed mo mentom. These are referred to as dC—k plots, where k is a parameter proportional to the electron crystal momentum. The F—k pInts associated with semicondactors fall into two grn&dIcategcrieiJthe first, sketched in Fig. 3.l7(a), both the minimum condnction baud ecergy and maximarn valence band energy occar at k = 0. In the second, pictnred in Fig. 3.17(b), the condoction band minimam is displaced took a 0. Semiconductors eshib iting the fortoer type of plot are referred to as dirvcr seinicondornors, and semicondnctors exhibiting the latter type of plot, as indirect semiconductors. GaAs is a notabte member of thc dircet setoicondnctor family; Ge and Si nrc both indirect semictundactors. lot Direct inwiecodarier Figure 3.17 tbl todisromewiceodacror General forms of Id—h plots for direct avd indirect semicondocioo. Phosss(s( Wm (a) Direct eroicondacior Figure 3.18 F—k plot I tat tedireci senienedanior visaatiaations of eecembinotinn in dirmi and indirect semiconductors. To make nse of the F—k plots in visnalicing an R—G process, one needs to know the noince of transitions associated with the obsorptien or emission of photons (light) and lat tice vibration qnanta called phonom. Photons, being mmslcns entities, carry very little momentnm, and a photon-assisted transition is essentially vertical on the F—k plot. Con versely, the thermal energy associated with lattice vibmtiona (phonous) is very small (in the 10—50 meV range), whereas the phonon momeutam is cnmparatively large. Than on an F—k plot a phonon-asnisted transition in essentially horleontal. It is also important to point out that, as pictured in Fig. 3.11, electrons and holes normally only occupy staten very close to the c minimom and E maximum, respectively. Thin is of coarse consistent with oar earlier discnssiou of the dinlnibation of carriers in the bands. Let us now specifically re-examine the band-to-band recombinanion process. In a direct nemicondnctor where the k-vnlnes of electrons and holes are all bnuched neon k = 0, little change in momentam is reqaired for the recombination process to proceed. The conserva tion of both energy and momenmm in readily met simply by the emission of a photon (see Fig. 3.110). In on indirect nemicondoclor, on the other bond, therein a large change in momentnm associated with the recombination process. The emission of a photon will con serve ettergy but cannot aimaltaneonsly conserve momentam. Thus foe band-to-band cccombination to proceed in an indirect nemicondoctor, the emission of a photon mnnt be accompanied by the emission or absorption nf a phonon (see Fig. 3.1 fib). The rather involved natore of the hood-to-bond procens in indirect semiconductors anderstandably leads to a vastly diminished recosabinotion raIn. Bond-to-band recombina lion in in fact totally negligible compared to R—G center recnmbination in Si and other indirect semicondnctoca. Band-to-band recombinotion does proceed at a much foster rate in direct semicandoctors and is the process prodacing the light observed from LEDs and jonctioo lasers. Even in direct materials, however, the R—G center mechanism in often the dominant process. Given the universal importance of the R—G center process, and the fact that most devices ore made from Si, which in an indirect material, the q000titutive consid erations in the next snbaecmion ore devoted primarily to the R—G center mechanism. Giber processes are considered as the need arises. 109 Thermal 106 r nueicosuncvon FasuneeNyALs eanetun -t Light 107 . Thermal enorgy E, acTioN RJJ Midgap a.. (a) tdand-io.ha recoinbinaflon (d) Band-to-band generation As Themmal energy enorgy Cs Mn Cr Fe Figure 3.16 Neac-midgap osergy tnsnls ininodnend by some cnmmnn impooties in Si. When an impnri’y introduces maltipln tnsnts, one sf the tesets tends to dominate in a given aemicondactor sample. Auger Recombinetion (hi E—G coitier eecombinnaeo (ci R—G center generaaon In the Anger (pronounced Gb-jay) process piclsred in Fig. 3.15(c), band-to-band cecombt notion occars simaltaneousty wilh the cottiainn between two like carriers. The energy re leased by the recombination is transferred dnring the colliainn to the surviving cnrriec This highly energetic carrier snbseqaenlty “thertnaticev”—loses energy in small steps throagh heat-prodncing collisions with the ncosicondnctoc lattice. The “staircme” in Fig. 3.15(c) represents the envisioned vtepwise loss of energy. Generstion Processes Any of the foregoing recombinamion processes con be reversed to generate corners. Bandto-band generation, where an etcclroe is excited directly from the valence band into the condoction band, is pictnred in Fig. 3.15(d). Note that either thermal energy or tight can provide the energy required for the bend-to-band transition. If thermal energy is absorbed, the process is alternatively referred teas direct rhertnol generation; if externally introdnced light iv absorbed, the process is called photogetseration. The thermally assisted generation of carriers with R—G centers acting as intermediaries is envisioned in Fig. 3.15(e). Finally, impact ionicntion, the inverse of Anger recombinolion, is viouolieed in Ftg. 3.15(f). In lhts process an electron—hale pnir is pradaced as a cesnlt of energy released vvheu a highly energetic cornier collides with the crystal lattice. The generation of carriers throogh impact ionieation routinely occars in the high B -field regions of devices. We will have more to say abnat this process when treating breakdown in pn janctions. (e) Ao er vecowbinomioo 0 (0 Cawiergenernm via impact ionization Figure 3.15 Energy hand visuotieatioo of recombination and generutioe processes As ceted in Fig. 3.15(h), recombjnatjon at on R—G center is a two-step process. First, eec type of carrier, say an electron, strays into the Vicinity of on R—G center, is canght by the potential well associated with the center, loses energy, end is trapped Snhseqneetiy, hole comes along, is attracted to the trapped electron, loses energy, and aesihilates the electron within the center. Alternatively, as also shown in Fig. 3.15(b), one can thick of the electron as losing energy a second time and annihilating the hole in the satence band. R—G center recowbinalion also called indirect rocnnthinotion typically releases thermal energy (heat) doring the process or, eqnisatenlly, produces lattice vibrations www.EasyEngineering.net 108 3.3,2 Momentum Considerstions All of the varioss recombination—generatinn procmses occur at all times in all seottcon doctors—evon nnder eqoilibriam conditions. The critical issue in not whether the processes are occnrring, hot rather, the rates at which the various processes arc occurring. Typically, one need be concerned only with the dominant prncess, the process proceeding at the fastest rate. A number of the proemses are important only nader apecint conditions or are highly improbable, occurring at a mach slower rate than competing processes. Anger recombinn r neetcoNnucvon FonnaeusvaLs eeenieencnlos tion provides a cane in point. Becanse the catcher of carrier-carrier collisions increases with titcreased cacrier concentration, the freqnency of Anger recombinatine likewise in creases with carrier concentration. Anger recombinatien mast be considered, for ecamplc, in treating highly doped regions of o device stractare, bat it is asnally negligible otherwise. Similarly, significant impact ionication occnrs only in the high B-field regions of a device. In a somewhat different vein, phntogeneratinn at room temperatare becomes n significant process only when the semicondector is cxpnsed to external illominatios. What then is the R—G process pair desersing of special attention, the process pair that typically dominates in the lcw B -field regions of a nondegenerntety doped semicondactor maintained at room temperatore? From the information prnvided, the choice is obvionsly between thermal band-to-band k—G and recombination—generation via R—G centers. From the energy band explanation alone one might specatete that band-to-band ww w cecombination—generation wanld dominate ander the cited “standard” conditions. How ever, visaatieation of R—G processes nsing the energy band diagram can be mistnndisg. The F—n plot examines only changes in energy, whereas crystal motoestum in additiott to eneegy mast be conserved in any tZ—G process. Momentom conservation ceqnirements, as it tnrns out, ploy an important role in setting the process rare. As first noted in Snbseciien 2.2.3. the momentsm of an electron in an energy band, like the clectroti energy, can assame only certain qnanticcd values. Momenlam-related as pects of R—G prcccsscs are conveniently discasoed with the aid of plots where the allowed electron energies in the condoctinn and valcitce bands are plotted versas the allowed mo mentom. These are referred to as dC—k plots, where k is a parameter proportional to the electron crystal momentum. The F—k pInts associated with semicondactors fall into two .Ea syE ngi nee rin g grn&dIcategcrieiJthe first, sketched in Fig. 3.l7(a), both the minimum condnction baud ecergy and maximarn valence band energy occar at k = 0. In the second, pictnred in Fig. 3.17(b), the condoction band minimam is displaced took a 0. Semiconductors eshib iting the fortoer type of plot are referred to as dirvcr seinicondornors, and semicondnctors exhibiting the latter type of plot, as indirect semiconductors. GaAs is a notabte member of thc dircet setoicondnctor family; Ge and Si nrc both indirect semictundactors. .ne t lot Direct inwiecodarier Figure 3.17 tbl todisromewiceodacror General forms of Id—h plots for direct avd indirect semicondocioo. www.EasyEngineering.net Phosss(s( Wm (a) Direct eroicondacior Figure 3.18 F—k plot I tat tedireci senienedanior visaatiaations of eecembinotinn in dirmi and indirect semiconductors. To make nse of the F—k plots in visnalicing an R—G process, one needs to know the noince of transitions associated with the obsorptien or emission of photons (light) and lat tice vibration qnanta called phonom. Photons, being mmslcns entities, carry very little momentnm, and a photon-assisted transition is essentially vertical on the F—k plot. Con versely, the thermal energy associated with lattice vibmtiona (phonous) is very small (in the 10—50 meV range), whereas the phonon momeutam is cnmparatively large. Than on an F—k plot a phonon-asnisted transition in essentially horleontal. It is also important to point out that, as pictured in Fig. 3.11, electrons and holes normally only occupy staten very close to the c minimom and E maximum, respectively. Thin is of coarse consistent with oar earlier discnssiou of the dinlnibation of carriers in the bands. Let us now specifically re-examine the band-to-band recombinanion process. In a direct nemicondnctor where the k-vnlnes of electrons and holes are all bnuched neon k = 0, little change in momentam is reqaired for the recombination process to proceed. The conserva tion of both energy and momenmm in readily met simply by the emission of a photon (see Fig. 3.110). In on indirect nemicondoclor, on the other bond, therein a large change in momentnm associated with the recombination process. The emission of a photon will con serve ettergy but cannot aimaltaneonsly conserve momentam. Thus foe band-to-band cccombination to proceed in an indirect nemicondoctor, the emission of a photon mnnt be accompanied by the emission or absorption nf a phonon (see Fig. 3.1 fib). The rather involved natore of the hood-to-bond procens in indirect semiconductors anderstandably leads to a vastly diminished recosabinotion raIn. Bond-to-band recombina lion in in fact totally negligible compared to R—G center recnmbination in Si and other indirect semicondnctoca. Band-to-band recombinotion does proceed at a much foster rate in direct semicandoctors and is the process prodacing the light observed from LEDs and jonctioo lasers. Even in direct materials, however, the R—G center mechanism in often the dominant process. Given the universal importance of the R—G center process, and the fact that most devices ore made from Si, which in an indirect material, the q000titutive consid erations in the next snbaecmion ore devoted primarily to the R—G center mechanism. Giber processes are considered as the need arises. 109 Thermal 106 r nueicosuncvon FasuneeNyALs eanetun -t . Thermal enorgy Light E, RJJ (d) Band-to-band generation As enorgy (hi E—G coitier eecombinnaeo Midgap a.. (a) tdand-io.ha recoinbinaflon 107 acTioN Cr Mn Cs Fe Figure 3.16 Neac-midgap osergy tnsnls ininodnend by some cnmmnn impooties in Si. When an impnri’y introduces maltipln tnsnts, one sf the tesets tends to dominate in a given aemicondactor sample. Themmal energy Auger Recombinetion (ci R—G center generaaon In the Anger (pronounced Gb-jay) process piclsred in Fig. 3.15(c), band-to-band cecombt notion occars simaltaneousty wilh the cottiainn between two like carriers. The energy re leased by the recombination is transferred dnring the colliainn to the surviving cnrriec This highly energetic carrier snbseqaenlty “thertnaticev”—loses energy in small steps throagh heat-prodncing collisions with the ncosicondnctoc lattice. The “staircme” in Fig. 3.15(c) represents the envisioned vtepwise loss of energy. Generstion Processes Any of the foregoing recombinamion processes con be reversed to generate corners. Bandto-band generation, where an etcclroe is excited directly from the valence band into the condoction band, is pictnred in Fig. 3.15(d). Note that either thermal energy or tight can provide the energy required for the bend-to-band transition. If thermal energy is absorbed, the process is alternatively referred teas direct rhertnol generation; if externally introdnced light iv absorbed, the process is called photogetseration. The thermally assisted generation of carriers with R—G centers acting as intermediaries is envisioned in Fig. 3.15(e). Finally, impact ionicntion, the inverse of Anger recombinolion, is viouolieed in Ftg. 3.15(f). In lhts process an electron—hale pnir is pradaced as a cesnlt of energy released vvheu a highly energetic cornier collides with the crystal lattice. The generation of carriers throogh impact ionieation routinely occars in the high B -field regions of devices. We will have more to say abnat this process when treating breakdown in pn janctions. (e) Ao er vecowbinomioo 0 (0 Cawiergenernm via impact ionization Figure 3.15 Energy hand visuotieatioo of recombination and generutioe processes As ceted in Fig. 3.15(h), recombjnatjon at on R—G center is a two-step process. First, eec type of carrier, say an electron, strays into the Vicinity of on R—G center, is canght by the potential well associated with the center, loses energy, end is trapped Snhseqneetiy, hole comes along, is attracted to the trapped electron, loses energy, and aesihilates the electron within the center. Alternatively, as also shown in Fig. 3.15(b), one can thick of the electron as losing energy a second time and annihilating the hole in the satence band. R—G center recowbinalion also called indirect rocnnthinotion typically releases thermal energy (heat) doring the process or, eqnisatenlly, produces lattice vibrations 3.3,2 Momentum Considerstions All of the varioss recombination—generatinn procmses occur at all times in all seottcon doctors—evon nnder eqoilibriam conditions. The critical issue in not whether the processes are occnrring, hot rather, the rates at which the various processes arc occurring. Typically, one need be concerned only with the dominant prncess, the process proceeding at the fastest rate. A number of the proemses are important only nader apecint conditions or are highly improbable, occurring at a mach slower rate than competing processes. Anger recombinn r 108 www.EasyEngineering.net neetcoNnucvon FonnaeusvaLs 109 eeenieencnlos tion provides a cane in point. Becanse the catcher of carrier-carrier collisions increases with titcreased cacrier concentration, the freqnency of Anger recombinatine likewise in creases with carrier concentration. Anger recombinatien mast be considered, for ecamplc, in treating highly doped regions of o device stractare, bat it is asnally negligible otherwise. Similarly, significant impact ionication occnrs only in the high B-field regions of a device. In a somewhat different vein, phntogeneratinn at room temperatare becomes n significant process only when the semicondector is cxpnsed to external illominatios. What then is the R—G process pair desersing of special attention, the process pair that typically dominates in the lcw B -field regions of a nondegenerntety doped semicondactor maintained at room temperatore? From the information prnvided, the choice is obvionsly between thermal band-to-band k—G and recombination—generation via R—G centers. From the energy band explanation alone one might specatete that band-to-band cecombination—generation wanld dominate ander the cited “standard” conditions. How ever, visaatieation of R—G processes nsing the energy band diagram can be mistnndisg. The F—n plot examines only changes in energy, whereas crystal motoestum in additiott to eneegy mast be conserved in any tZ—G process. Momentom conservation ceqnirements, as it tnrns out, ploy an important role in setting the process rare. As first noted in Snbseciien 2.2.3. the momentsm of an electron in an energy band, like the clectroti energy, can assame only certain qnanticcd values. Momenlam-related as pects of R—G prcccsscs are conveniently discasoed with the aid of plots where the allowed electron energies in the condoctinn and valcitce bands are plotted versas the allowed mo mentom. These are referred to as dC—k plots, where k is a parameter proportional to the electron crystal momentum. The F—k pInts associated with semicondactors fall into two grn&dIcategcrieiJthe first, sketched in Fig. 3.l7(a), both the minimum condnction baud ecergy and maximarn valence band energy occar at k = 0. In the second, pictnred in Fig. 3.17(b), the condoction band minimam is displaced took a 0. Semiconductors eshib iting the fortoer type of plot are referred to as dirvcr seinicondornors, and semicondnctors exhibiting the latter type of plot, as indirect semiconductors. GaAs is a notabte member of thc dircet setoicondnctor family; Ge and Si nrc both indirect semictundactors. lot Direct inwiecodarier Figure 3.17 tbl todisromewiceodacror General forms of Id—h plots for direct avd indirect semicondocioo. Phosss(s( Wm ww w.E I (a) Direct eroicondacior Figure 3.18 F—k plot tat tedireci senienedanior visaatiaations of eecembinotinn in dirmi and indirect semiconductors. asy To make nse of the F—k plots in visnalicing an R—G process, one needs to know the noince of transitions associated with the obsorptien or emission of photons (light) and lat tice vibration qnanta called phonom. Photons, being mmslcns entities, carry very little momentnm, and a photon-assisted transition is essentially vertical on the F—k plot. Con En versely, the thermal energy associated with lattice vibmtiona (phonous) is very small (in the 10—50 meV range), whereas the phonon momeutam is cnmparatively large. Than on an F—k plot a phonon-asnisted transition in essentially horleontal. It is also important to gin eer point out that, as pictured in Fig. 3.11, electrons and holes normally only occupy staten very close to the c minimom and E maximum, respectively. Thin is of coarse consistent with oar earlier discnssiou of the dinlnibation of carriers in the bands. Let us now specifically re-examine the band-to-band recombinanion process. In a direct nemicondnctor where the k-vnlnes of electrons and holes are all bnuched neon k = 0, little change in momentam is reqaired for the recombination process to proceed. The conserva tion of both energy and momenmm in readily met simply by the emission of a photon (see Fig. 3.110). In on indirect nemicondoclor, on the other bond, therein a large change in momentnm associated with the recombination process. The emission of a photon will con serve ettergy but cannot aimaltaneonsly conserve momentam. Thus foe band-to-band cccombination to proceed in an indirect nemicondoctor, the emission of a photon mnnt be accompanied by the emission or absorption nf a phonon (see Fig. 3.1 fib). The rather involved natore of the hood-to-bond procens in indirect semiconductors anderstandably leads to a vastly diminished recosabinotion raIn. Bond-to-band recombina lion in in fact totally negligible compared to R—G center recnmbination in Si and other indirect semicondnctoca. Band-to-band recombinotion does proceed at a much foster rate in direct semicandoctors and is the process prodacing the light observed from LEDs and jonctioo lasers. Even in direct materials, however, the R—G center mechanism in often the dominant process. Given the universal importance of the R—G center process, and the fact that most devices ore made from Si, which in an indirect material, the q000titutive consid erations in the next snbaecmion ore devoted primarily to the R—G center mechanism. Giber processes are considered as the need arises. ing .ne www.EasyEngineering.net t www.EasyEngineering.net / •, 110 SEMICONDUCTOR FUNDAMENTALS CARRIERACTION 3.3.3 R—G Statistics 111 Light (Ac) R—G statistics is the technical name given to dtc mathematical characterization of recom hssalsan—gcnerarioa processes. “Mathematical characterieation” in the cane of recombi nation—generation does snot mean the development of a corceat-deitsity retaniooship. As R—O event occars at lacalized positions in the crystal, at a given x-valoe, and therefore the R—O action does eon lead per Sc to charge transport. Rather, recombination—geeeratios Somicoodartar Z acts to change the carrier concentrations, thereby indirectly affecting the cnrrertt flow. It is the time rote of change in the carrier concentrations (fluids, op/fit) that mast he specified to achieve the desired mathematical characterization. Because its characterication is relatively simple and its involvement is device operation quite common, we begin by roesideriog photogeiseratioo. The major portioo of tine sabsecsios in of coarse devoted to recoonbisa ww tions—gearration via R—O Figure 3.19 Semiooedsrtar, light propagation, and coardinato arientation in the phatogesoratiuo asatpsis. The semiconductor is Unnamed to be saffiriestip thick IL F fail sa that bsttam sarfsee reflections may be isogleetod. centers, alteroatively referred to as indirect thermal recombiaa tioe—generatioa. w.E Photogenerstioo as y En gin e Light striking tine sarface of a semicosdactor as pictared in Fig. 3.19 will be partially regected and partially transmitted into the msaterial. Assame the tight to be monochromatic with wavelesgth A and freqaeecy p. If the photon energy (he) is greater than the baad gap energy, then the light will be absorbed sad electron—hole pairs will he created an the light passes throsigla the semicondnrtor. The decrease in intensity as monochromatic tight passes through a material is gives by I = I r’ 5 (3.26) eri where 4 is the light iatensity jast inside the material at x = 0 and a is the obsorptioaa reeffiriess. Note fross Fig. 3.20 that a is material dependent and a strong foaction of A. Since there is a one-to-ate correspondence between the absorption of photons and the creation of electron—hole pairs, the carrier creation mte shontd likewise eshibit an exp(—m.a) dependence. Moreover, referring to Fig. 3.15(d), the phatogeneration process always acts sa as to create an eqonf nnmher of electrons and holes. We therefore tanelode ng. ne t = liP, = QL(X,A) (3.27) wtsers, for the sitaotioa analyzed, GL(x.A) Grre (3.2fl) G is 1hz simplified symbol for the phatogenerosion rate (a namber/cm -sec), white O, is t tIne photageneratine rate at x 0. The as, designation means “dne so light” and is nec essary because, as we have seen, at and peas be affected by a namber of processes. in working problems involving the ittamination of a sample or device, we will often invoke one of swa simplifying assamptions: (i) The illnmination is msamed to be onifarm everywhere inside the sample and (ii) the light is assamed to be absorbed in on fl.4 fl.A fl.S i.fl 1.2 1.4 l.A 1.1 Alpm) Figure 3.20 Thn absorption eeaffieiant as a fonetian af wnveteogth in Si and other scIon semicaa dnosars. (Prom Sehredrrl i, 0 1990 by Jabs Wiley & Seas, Inn. Oeprintud with permiusian.) 5 www.EasyEngineering.net 112 SEM5CONSUCTON FUNnAMENTALS CARR5ENACOON infinitesimally thie layer near the semiconductor sarfare. Seeking to identify when the assamed conditions are approached in practice, we note first that I Ia, which has the dimen sions of a length, represents the average depth nf penetraliou of the tight into a materiel. At wavelengths where he , the absorption coefficient is very small and I/u is very large, 5 N shoot 1 cm in Si. This snakes exp(—ua) m t far alt practical depths. To a very good approxamation, 0 m constant and the tight is being oaiformly absorbed. On the other L hand, if A = 0.4 pm, an u(Si) m IN cm—’ is dedaced from Pig. 3.20. At this wavelength the light pesntmtiaa depth is only e few thousand angstroms arid the assumption of sarfare absorption is closely eppraximated. Indirect Thermal Recombination—Generation Althoagh the general case development of R—O center statistics is beyond the scope of this text, mis passable to presesas argamests leading to the special-ease expression employed in many practical problems. Let as begie by carefully defining the varioas carrier and center conceasaorieas involved is she aaalysis. S 5 p . as, p . m a NT — n,,. p— p 5 . . . . . . carrier concentrations in the material ander analysis when equihib near conditions prevail. carrier eoneentmtions in she material under arbitrary conditions. deviations in the carrier coneentrasiosas from their eqaitibriam votoes. ass nod Ap can be bath positive and negative, where a positive devia tion corresponds to a carrier excess and a negative deviation corre sponds to a carrier deficit. oamber of R—O centers/cm . 3 In the special-case development, pertorbolios of the carrier concentrations from their eqailibnam values must correspoad to low-level iasjeeaioas. This reqairement is jest an ol seraattve way of saying the perrarbasios must be relatively small. To be more precise, p 4 ne Lz pa law-level iasjeetfox implies it n in on v-type material p 5 p so a p-type material Consider a specific example of 0 N = tOlSfcmi doped Si at room temperolare sabjeet to a = Ass = 10°/em . Poe the given material, as 3 5a N 5 = t /em and 5 t0’ 5 nCr/N p 0 3 /cso Couseqaeatly, as a 5 l0 . 5 + As 5 and Ap v 3 4ai 10°/cm 5 = 10’/ . The sitaotion is cleorly one of law-level injeesiox. Observe, however, that Ap 3 cm perlarbatioss where rhp F’ Pa Atshongh the majority carrier doncentrotioia remeins essentially eapertarbed ander low-level isjecsioa, the minority carrier concentration can, and ransinely does, increase by many orders of mognisxde. Pesisabasian s-naN I eee...e. Cv Ftgure 3.21 Situation inside so n-type sennicoadactar sfier a prrtsrbaniaa mating the low-Invel aajecnsos of caress hales. We are sow ready no asalyas the specific Situation envisiossed in Pig. 321. A pertnr botion hon caused a Ap 5 excess of holes in on S-type semicosdoetor sample Avsemiaag the system is an the midst of rrloxnxg back no the eqoilibrissm state from the pictured per tarbed stole via the R—O venIce interaction, what factors woold yoo expect to have the greatest effect on dp/fltJg, the cole of hole recombination? Well, to eliminsose abate, the hole most make the transition from the valence bossd to on electron-filled R—O center. Logically, the greater the Somber of filled R—O centers, the greater the probability of a hole annihilating transitions and the faster the rate of recombination. Under eqaihibriom condi tions, esneotially all of the R—O cexsern ore filled wish electrons becoose the eqoihibnmom Fermi 1 usd ts comfortably above Wsah Ap 4 as, electrons always vastly aatssmber holes and rapidly fill R—O levels that become voroot This keeps the somber of filled R—O rooters during the relaxation process NT. Than, we espect p0I to be approximately 0 proportiouol to NT. Moreover, is also seems logical that the samber of hale-annihilating transitions shoold increase almost Itacarly with the camber of holes. All ether factors being eqaol, the mare hales available for asnilsilosion, the greater the somber of holes removed from the valence bead per second. Conseqoestly, we also expect Op//nj 5 to be approxi mately proportional to p. Cossidenieg additiaaol factors leads to no additiasot dependex ties. Hence, iotrodsscing a positive proportionality resistant, cc, and realizing is negoisvo becooss p in decreasing, we renelade = —eNp (3.29) 113 www.EasyEngineering.net / •, 110 SEMICONDUCTOR FUNDAMENTALS 111 CARRIERACTION 3.3.3 R—G Statistics Light (Ac) R—G statistics is the technical name given to dtc mathematical characterization of recom hssalsan—gcnerarioa processes. “Mathematical characterieation” in the cane of recombi nation—generation does snot mean the development of a corceat-deitsity retaniooship. As R—O event occars at lacalized positions in the crystal, at a given x-valoe, and therefore the R—O action does eon lead per Sc to charge transport. Rather, recombination—geeeratios Somicoodartar Z acts to change the carrier concentrations, thereby indirectly affecting the cnrrertt flow. It is the time rote of change in the carrier concentrations (fluids, op/fit) that mast he specified to achieve the desired mathematical characterization. Because its characterication is relatively simple and its involvement is device operation quite common, we begin by roesideriog photogeiseratioo. The major portioo of tine sabsecsios in of coarse devoted to recoonbisa tions—gearration via R—O centers, alteroatively referred to as indirect thermal recombiaa tioe—generatioa. Photogenerstioo Light striking tine sarface of a semicosdactor as pictared in Fig. 3.19 will be partially regected and partially transmitted into the msaterial. Assame the tight to be monochromatic with wavelesgth A and freqaeecy p. If the photon energy (he) is greater than the baad gap energy, then the light will be absorbed sad electron—hole pairs will he created an the light passes throsigla the semicondnrtor. The decrease in intensity as monochromatic tight passes through a material is gives by I = I r’ 5 (3.26) Figure 3.19 Semiooedsrtar, light propagation, and coardinato arientation in the phatogesoratiuo asatpsis. The semiconductor is Unnamed to be saffiriestip thick IL F fail sa that bsttam sarfsee reflections may be isogleetod. ww w.E a nee r where 4 is the light iatensity jast inside the material at x = 0 and a is the obsorptioaa reeffiriess. Note fross Fig. 3.20 that a is material dependent and a strong foaction of A. Since there is a one-to-ate correspondence between the absorption of photons and the creation of electron—hole pairs, the carrier creation mte shontd likewise eshibit an exp(—m.a) dependence. Moreover, referring to Fig. 3.15(d), the phatogeneration process always acts sa as to create an eqonf nnmher of electrons and holes. We therefore tanelode = liP, = QL(X,A) syE ngi ing . (3.27) net wtsers, for the sitaotioa analyzed, GL(x.A) Grre (3.2fl) G is 1hz simplified symbol for the phatogenerosion rate (a namber/cm -sec), white O, is t tIne photageneratine rate at x 0. The as, designation means “dne so light” and is nec essary because, as we have seen, at and peas be affected by a namber of processes. in working problems involving the ittamination of a sample or device, we will often invoke one of swa simplifying assamptions: (i) The illnmination is msamed to be onifarm everywhere inside the sample and (ii) the light is assamed to be absorbed in on fl.4 fl.A fl.S i.fl 1.2 1.4 l.A 1.1 Alpm) Figure 3.20 Thn absorption eeaffieiant as a fonetian af wnveteogth in Si and other scIon semicaa dnosars. (Prom Sehredrrl i, 0 1990 by Jabs Wiley & Seas, Inn. Oeprintud with permiusian.) 5 www.EasyEngineering.net 112 SEM5CONSUCTON FUNnAMENTALS CARR5ENACOON infinitesimally thie layer near the semiconductor sarfare. Seeking to identify when the assamed conditions are approached in practice, we note first that I Ia, which has the dimen sions of a length, represents the average depth nf penetraliou of the tight into a materiel. At wavelengths where he , the absorption coefficient is very small and I/u is very large, 5 N shoot 1 cm in Si. This snakes exp(—ua) m t far alt practical depths. To a very good approxamation, 0 m constant and the tight is being oaiformly absorbed. On the other L hand, if A = 0.4 pm, an u(Si) m IN cm—’ is dedaced from Pig. 3.20. At this wavelength the light pesntmtiaa depth is only e few thousand angstroms arid the assumption of sarfare absorption is closely eppraximated. Indirect Thermal Recombination—Generation Althoagh the general case development of R—O center statistics is beyond the scope of this text, mis passable to presesas argamests leading to the special-ease expression employed in many practical problems. Let as begie by carefully defining the varioas carrier and center conceasaorieas involved is she aaalysis. S 5 p . as, p . m a NT — n,,. p— p 5 . . . . . . carrier concentrations in the material ander analysis when equihib near conditions prevail. carrier eoneentmtions in she material under arbitrary conditions. deviations in the carrier coneentrasiosas from their eqaitibriam votoes. ass nod Ap can be bath positive and negative, where a positive devia tion corresponds to a carrier excess and a negative deviation corre sponds to a carrier deficit. oamber of R—O centers/cm . 3 In the special-case development, pertorbolios of the carrier concentrations from their eqailibnam values must correspoad to low-level iasjeeaioas. This reqairement is jest an ol seraattve way of saying the perrarbasios must be relatively small. To be more precise, p 4 ne Lz pa law-level iasjeetfox implies it n in on v-type material p 5 p so a p-type material Consider a specific example of 0 N = tOlSfcmi doped Si at room temperolare sabjeet to a = Ass = 10°/em . Poe the given material, as 3 5a N 5 = t /em and 5 t0’ 5 nCr/N p 0 3 /cso Couseqaeatly, as a 5 l0 . 5 + As 5 and Ap v 3 4ai 10°/cm 5 = 10’/ . The sitaotion is cleorly one of law-level injeesiox. Observe, however, that Ap 3 cm perlarbatioss where rhp F’ Pa Atshongh the majority carrier doncentrotioia remeins essentially eapertarbed ander low-level isjecsioa, the minority carrier concentration can, and ransinely does, increase by many orders of mognisxde. Pesisabasian s-naN I eee...e. Cv Ftgure 3.21 Situation inside so n-type sennicoadactar sfier a prrtsrbaniaa mating the low-Invel aajecnsos of caress hales. We are sow ready no asalyas the specific Situation envisiossed in Pig. 321. A pertnr botion hon caused a Ap 5 excess of holes in on S-type semicosdoetor sample Avsemiaag the system is an the midst of rrloxnxg back no the eqoilibrissm state from the pictured per tarbed stole via the R—O venIce interaction, what factors woold yoo expect to have the greatest effect on dp/fltJg, the cole of hole recombination? Well, to eliminsose abate, the hole most make the transition from the valence bossd to on electron-filled R—O center. Logically, the greater the Somber of filled R—O centers, the greater the probability of a hole annihilating transitions and the faster the rate of recombination. Under eqaihibriom condi tions, esneotially all of the R—O cexsern ore filled wish electrons becoose the eqoihibnmom Fermi 1 usd ts comfortably above Wsah Ap 4 as, electrons always vastly aatssmber holes and rapidly fill R—O levels that become voroot This keeps the somber of filled R—O rooters during the relaxation process NT. Than, we espect p0I to be approximately 0 proportiouol to NT. Moreover, is also seems logical that the samber of hale-annihilating transitions shoold increase almost Itacarly with the camber of holes. All ether factors being eqaol, the mare hales available for asnilsilosion, the greater the somber of holes removed from the valence bead per second. Conseqoestly, we also expect Op//nj 5 to be approxi mately proportional to p. Cossidenieg additiaaol factors leads to no additiasot dependex ties. Hence, iotrodsscing a positive proportionality resistant, cc, and realizing is negoisvo becooss p in decreasing, we renelade = —eNp (3.29) 113 / •, 110 SEMICONDUCTOR FUNDAMENTALS CARRIERACTION 3.3.3 R—G Statistics 111 Light (Ac) R—G statistics is the technical name given to dtc mathematical characterization of recom hssalsan—gcnerarioa processes. “Mathematical characterieation” in the cane of recombi nation—generation does snot mean the development of a corceat-deitsity retaniooship. As R—O event occars at lacalized positions in the crystal, at a given x-valoe, and therefore the R—O action does eon lead per Sc to charge transport. Rather, recombination—geeeratios Somicoodartar Z acts to change the carrier concentrations, thereby indirectly affecting the cnrrertt flow. It is the time rote of change in the carrier concentrations (fluids, op/fit) that mast he specified to achieve the desired mathematical characterization. Because its characterication is relatively simple and its involvement is device operation quite common, we begin by roesideriog photogeiseratioo. The major portioo of tine sabsecsios in of coarse devoted to recoonbisa tions—gearration via R—O Figure 3.19 Semiooedsrtar, light propagation, and coardinato arientation in the phatogesoratiuo asatpsis. The semiconductor is Unnamed to be saffiriestip thick IL F fail sa that bsttam sarfsee reflections may be isogleetod. centers, alteroatively referred to as indirect thermal recombiaa tioe—generatioa. Photogenerstioo Light striking tine sarface of a semicosdactor as pictared in Fig. 3.19 will be partially regected and partially transmitted into the msaterial. Assame the tight to be monochromatic with wavelesgth A and freqaeecy p. If the photon energy (he) is greater than the baad gap energy, then the light will be absorbed sad electron—hole pairs will he created an the light passes throsigla the semicondnrtor. The decrease in intensity as monochromatic tight passes through a material is gives by I = I r’ 5 (3.26) where 4 is the light iatensity jast inside the material at x = 0 and a is the obsorptioaa reeffiriess. Note fross Fig. 3.20 that a is material dependent and a strong foaction of A. Since there is a one-to-ate correspondence between the absorption of photons and the creation of electron—hole pairs, the carrier creation mte shontd likewise eshibit an exp(—m.a) dependence. Moreover, referring to Fig. 3.15(d), the phatogeneration process always acts sa as to create an eqonf nnmher of electrons and holes. We therefore tanelode = liP, = (3.27) QL(X,A) wtsers, for the sitaotioa analyzed, GL(x.A) (3.2fl) Grre G is 1hz simplified symbol for the phatogenerosion rate (a namber/cm -sec), white O, is t tIne photageneratine rate at x 0. The as, designation means “dne so light” and is nec essary because, as we have seen, at and peas be affected by a namber of processes. in working problems involving the ittamination of a sample or device, we will often invoke one of swa simplifying assamptions: (i) The illnmination is msamed to be onifarm everywhere inside the sample and (ii) the light is assamed to be absorbed in on fl.4 fl.A fl.S i.fl 1.2 1.4 l.A 1.1 Alpm) Figure 3.20 Thn absorption eeaffieiant as a fonetian af wnveteogth in Si and other scIon semicaa dnosars. (Prom Sehredrrl i, 0 1990 by Jabs Wiley & Seas, Inn. Oeprintud with permiusian.) 5 www.EasyEngineering.net 112 SEM5CONSUCTON FUNnAMENTALS CARR5ENACOON infinitesimally thie layer near the semiconductor sarfare. Seeking to identify when the assamed conditions are approached in practice, we note first that I Ia, which has the dimen sions of a length, represents the average depth nf penetraliou of the tight into a materiel. At wavelengths where he , the absorption coefficient is very small and I/u is very large, 5 N shoot 1 cm in Si. This snakes exp(—ua) m t far alt practical depths. To a very good approxamation, 0 m constant and the tight is being oaiformly absorbed. On the other L hand, if A = 0.4 pm, an u(Si) m IN cm—’ is dedaced from Pig. 3.20. At this wavelength the light pesntmtiaa depth is only e few thousand angstroms arid the assumption of sarfare absorption is closely eppraximated. Indirect Thermal Recombination—Generation ww w s-naN Althoagh the general case development of R—O center statistics is beyond the scope of this text, mis passable to presesas argamests leading to the special-ease expression employed in many practical problems. Let as begie by carefully defining the varioas carrier and center conceasaorieas involved is she aaalysis. S 5 p . as, p . m a NT — n,,. p— p 5 . .Ea . . . . . carrier concentrations in the material ander analysis when equihib near conditions prevail. syE carrier eoneentmtions in she material under arbitrary conditions. ngi deviations in the carrier coneentrasiosas from their eqaitibriam votoes. ass nod Ap can be bath positive and negative, where a positive devia tion corresponds to a carrier excess and a negative deviation corre sponds to a carrier deficit. oamber of R—O centers/cm . 3 nee rin g .ne t In the special-case development, pertorbolios of the carrier concentrations from their eqailibnam values must correspoad to low-level iasjeeaioas. This reqairement is jest an ol seraattve way of saying the perrarbasios must be relatively small. To be more precise, p 4 ne Lz pa law-level iasjeetfox implies it n in on v-type material p 5 p Pesisabasian so a p-type material Consider a specific example of 0 N = tOlSfcmi doped Si at room temperolare sabjeet to a = Ass = 10°/em . Poe the given material, as 3 5a N 5 = t /em and 5 t0’ 5 nCr/N p 0 3 /cso Couseqaeatly, as a 5 l0 . 5 + As 5 and Ap v 3 4ai 10°/cm 5 = 10’/ . The sitaotion is cleorly one of law-level injeesiox. Observe, however, that Ap 3 cm perlarbatioss where rhp F’ Pa Atshongh the majority carrier doncentrotioia remeins essentially eapertarbed ander low-level isjecsioa, the minority carrier concentration can, and ransinely does, increase by many orders of mognisxde. eee...e. Cv Ftgure 3.21 Situation inside so n-type sennicoadactar sfier a prrtsrbaniaa mating the low-Invel aajecnsos of caress hales. We are sow ready no asalyas the specific Situation envisiossed in Pig. 321. A pertnr botion hon caused a Ap 5 excess of holes in on S-type semicosdoetor sample Avsemiaag the system is an the midst of rrloxnxg back no the eqoilibrissm state from the pictured per tarbed stole via the R—O venIce interaction, what factors woold yoo expect to have the greatest effect on dp/fltJg, the cole of hole recombination? Well, to eliminsose abate, the hole most make the transition from the valence bossd to on electron-filled R—O center. Logically, the greater the Somber of filled R—O centers, the greater the probability of a hole annihilating transitions and the faster the rate of recombination. Under eqaihibriom condi tions, esneotially all of the R—O cexsern ore filled wish electrons becoose the eqoihibnmom Fermi 1 usd ts comfortably above Wsah Ap 4 as, electrons always vastly aatssmber holes and rapidly fill R—O levels that become voroot This keeps the somber of filled R—O rooters during the relaxation process NT. Than, we espect p0I to be approximately 0 proportiouol to NT. Moreover, is also seems logical that the samber of hale-annihilating transitions shoold increase almost Itacarly with the camber of holes. All ether factors being eqaol, the mare hales available for asnilsilosion, the greater the somber of holes removed from the valence bead per second. Conseqoestly, we also expect Op//nj 5 to be approxi mately proportional to p. Cossidenieg additiaaol factors leads to no additiasot dependex ties. Hence, iotrodsscing a positive proportionality resistant, cc, and realizing is negoisvo becooss p in decreasing, we renelade = www.EasyEngineering.net I —eNp (3.29) 113 / •, 110 SEMICONDUCTOR FUNDAMENTALS 111 CARRIERACTION 3.3.3 R—G Statistics Light (Ac) R—G statistics is the technical name given to dtc mathematical characterization of recom hssalsan—gcnerarioa processes. “Mathematical characterieation” in the cane of recombi nation—generation does snot mean the development of a corceat-deitsity retaniooship. As R—O event occars at lacalized positions in the crystal, at a given x-valoe, and therefore the R—O action does eon lead per Sc to charge transport. Rather, recombination—geeeratios Somicoodartar Z acts to change the carrier concentrations, thereby indirectly affecting the cnrrertt flow. It is the time rote of change in the carrier concentrations (fluids, op/fit) that mast he specified to achieve the desired mathematical characterization. Because its characterication is relatively simple and its involvement is device operation quite common, we begin by roesideriog photogeiseratioo. The major portioo of tine sabsecsios in of coarse devoted to recoonbisa tions—gearration via R—O Figure 3.19 Semiooedsrtar, light propagation, and coardinato arientation in the phatogesoratiuo asatpsis. The semiconductor is Unnamed to be saffiriestip thick IL F fail sa that bsttam sarfsee reflections may be isogleetod. centers, alteroatively referred to as indirect thermal recombiaa tioe—generatioa. Photogenerstioo Light striking tine sarface of a semicosdactor as pictared in Fig. 3.19 will be partially regected and partially transmitted into the msaterial. Assame the tight to be monochromatic with wavelesgth A and freqaeecy p. If the photon energy (he) is greater than the baad gap energy, then the light will be absorbed sad electron—hole pairs will he created an the light passes throsigla the semicondnrtor. The decrease in intensity as monochromatic tight passes through a material is gives by I = I r’ 5 (3.26) where 4 is the light iatensity jast inside the material at x = 0 and a is the obsorptioaa reeffiriess. Note fross Fig. 3.20 that a is material dependent and a strong foaction of A. Since there is a one-to-ate correspondence between the absorption of photons and the creation of electron—hole pairs, the carrier creation mte shontd likewise eshibit an exp(—m.a) dependence. Moreover, referring to Fig. 3.15(d), the phatogeneration process always acts sa as to create an eqonf nnmher of electrons and holes. We therefore tanelode = liP, = QL(X,A) (3.27) wtsers, for the sitaotioa analyzed, GL(x.A) Grre (3.2fl) G is 1hz simplified symbol for the phatogenerosion rate (a namber/cm -sec), white O, is t tIne photageneratine rate at x 0. The as, designation means “dne so light” and is nec essary because, as we have seen, at and peas be affected by a namber of processes. in working problems involving the ittamination of a sample or device, we will often invoke one of swa simplifying assamptions: (i) The illnmination is msamed to be onifarm everywhere inside the sample and (ii) the light is assamed to be absorbed in on fl.4 fl.A fl.S i.fl 1.2 1.4 l.A 1.1 Alpm) Figure 3.20 Thn absorption eeaffieiant as a fonetian af wnveteogth in Si and other scIon semicaa dnosars. (Prom Sehredrrl i, 0 1990 by Jabs Wiley & Seas, Inn. Oeprintud with permiusian.) 5 www.EasyEngineering.net 112 SEM5CONSUCTON FUNnAMENTALS CARR5ENACOON infinitesimally thie layer near the semiconductor sarfare. Seeking to identify when the assamed conditions are approached in practice, we note first that I Ia, which has the dimen sions of a length, represents the average depth nf penetraliou of the tight into a materiel. At wavelengths where he , the absorption coefficient is very small and I/u is very large, 5 N shoot 1 cm in Si. This snakes exp(—ua) m t far alt practical depths. To a very good approxamation, 0 m constant and the tight is being oaiformly absorbed. On the other L hand, if A = 0.4 pm, an u(Si) m IN cm—’ is dedaced from Pig. 3.20. At this wavelength the light pesntmtiaa depth is only e few thousand angstroms arid the assumption of sarfare absorption is closely eppraximated. Indirect Thermal Recombination—Generation Althoagh the general case development of R—O center statistics is beyond the scope of this text, mis passable to presesas argamests leading to the special-ease expression employed in many practical problems. Let as begie by carefully defining the varioas carrier and center conceasaorieas involved is she aaalysis. S 5 p . as, p . m a NT — n,,. p— p 5 . . . . . . carrier concentrations in the material ander analysis when equihib near conditions prevail. carrier eoneentmtions in she material under arbitrary conditions. deviations in the carrier coneentrasiosas from their eqaitibriam votoes. ass nod Ap can be bath positive and negative, where a positive devia tion corresponds to a carrier excess and a negative deviation corre sponds to a carrier deficit. oamber of R—O centers/cm . 3 In the special-case development, pertorbolios of the carrier concentrations from their eqailibnam values must correspoad to low-level iasjeeaioas. This reqairement is jest an ol seraattve way of saying the perrarbasios must be relatively small. To be more precise, law-level iasjeetfox implies it n in on v-type material p 4 ne Lz pa p 5 p so a p-type material Consider a specific example of 0 N = tOlSfcmi doped Si at room temperolare sabjeet to a = Ass = 10°/em . Poe the given material, as 3 5a N 5 = t /em and 5 t0’ 5 nCr/N p 0 3 /cso Couseqaeatly, as a 5 l0 . 5 + As 5 and Ap v 3 4ai 10°/cm 5 = 10’/ . The sitaotion is cleorly one of law-level injeesiox. Observe, however, that Ap 3 cm perlarbatioss where rhp F’ Pa Atshongh the majority carrier doncentrotioia remeins essentially eapertarbed ander low-level isjecsioa, the minority carrier concentration can, and ransinely does, increase by many orders of mognisxde. 113 Pesisabasian s-naN ww w.E I eee...e. Cv asy Ftgure 3.21 Situation inside so n-type sennicoadactar sfier a prrtsrbaniaa mating the low-Invel aajecnsos of caress hales. En gin We are sow ready no asalyas the specific Situation envisiossed in Pig. 321. A pertnr botion hon caused a Ap 5 excess of holes in on S-type semicosdoetor sample Avsemiaag the eer system is an the midst of rrloxnxg back no the eqoilibrissm state from the pictured per tarbed stole via the R—O venIce interaction, what factors woold yoo expect to have the greatest effect on dp/fltJg, the cole of hole recombination? Well, to eliminsose abate, the hole most make the transition from the valence bossd to on electron-filled R—O center. Logically, the greater the Somber of filled R—O centers, the greater the probability of a hole annihilating transitions and the faster the rate of recombination. Under eqaihibriom condi tions, esneotially all of the R—O cexsern ore filled wish electrons becoose the eqoihibnmom Fermi 1 usd ts comfortably above Wsah Ap 4 as, electrons always vastly aatssmber holes and rapidly fill R—O levels that become voroot This keeps the somber of filled R—O rooters during the relaxation process NT. Than, we espect p0I to be approximately 0 proportiouol to NT. Moreover, is also seems logical that the samber of hale-annihilating transitions shoold increase almost Itacarly with the camber of holes. All ether factors being eqaol, the mare hales available for asnilsilosion, the greater the somber of holes removed from the valence bead per second. Conseqoestly, we also expect Op//nj 5 to be approxi mately proportional to p. Cossidenieg additiaaol factors leads to no additiasot dependex ties. Hence, iotrodsscing a positive proportionality resistant, cc, and realizing is negoisvo becooss p in decreasing, we renelade = —eNp ing .ne (3.29) www.EasyEngineering.net t ___________ __________ www.EasyEngineering.net • 114 SEMICONDUCTOR FUNDAMENTALS CANFIIDNACTIDN tf the hate generation process is analyzed in a siatilae matinee, iplit is deduced to depend only ae the camber of empty R—G centers. Titia camber, suhich is small foe the situatton nader coaaideratioe, is held approximatuty constant at its eqoilibriam same acer the range of perturbolloes where hole generation is significustl. Tltis means lhut can be replaced by iP/dtlx.wdI,s,im,. Mamoser, the recombiteulion and generation rates must precisely balance under equilibriuet renditions, t or dpfdtl 0 = dP/dtIa.e,rfs,ss,,,s, = Than, maksng use of Eq. (3.29), we obtain dP/itJvca,.b. Ill = OP/itici = ww E’7” (3.33u) “j’ (3.33b( s-s . — NTPO 5 r (3.30) which, when substitated into Eqs. (3.32), yield Finally, the eel rate of change in the hole concentration due to the R—O renter inter action is given by w.E —erNT(p as y En gin e or it = + = — i-ssesml = rrNvAp — = Pu) for holes in an n-type material 5 Ns-An r (3.32u) ng. ne far electrons in a p-type material for holes in ate a-type material .( 3 34a) for electrons in a p-type material (3.34b) (331) eri Au analaguns set of arguments yields iussss,t — 115 t (3.32b) c, like re in a positive proportionality constant. c, and en see mferred to as the eleereun and hole rapture coefficients, renpeetively. Although completely fuaetioeul as is, it is desieable to manipulate Eqs. (3.32) into a slightly more compact and meaningfal furm. An examination of the left-hand sides of Eqs. (3.32) reveals the dintensional un/Is are ihose of a concentration divided by time. Since Ap and An on the right-hand sides of the sasne equations are also concentrations, the cue stunts e . and e,,N utsai have units of I/time. It is thrtefam reasonable to inteadace lice N 5 time constants Equuttuns (3,34) are the desired end result, the special-ruse characterization of R—G center (indseect thermal) recombiuatiun—generstion, Although steady state or slowly varying conditions are implicitly assumed in the development of Eqs. (3.34), the relation ships con be applied mtth tItle error to most transient problems of iatermt. Ii should be restated chat a Ap < 0 is passibte and will give rise to a tsp/it’, , 50 > 0. A positive . u-n simply indicates that a carrier deficit 5 , 5155 ip/itJ,. exists inside the semicoedertor and geaeraanu is occurring at a more mpid rate than rernmbinutioa. ip/it ivesmui n-a and 1 Ua it mast he remembered, characterize the net effect of the thermal reeom binatian and thermal geueeatian processes. As duly emphasized, the Eq. (3.34) relationships apply only to minority carriers and as stluuuoos meeting the low-level injectina requirement. The more general steady state , valid for arbitrary Injection levels and both 151 result carrier types in a enndegenerate semi conductor, is nated for completeness sad fature referenue to be imt/itlissr,e,,t dpi it iui,,,m,a in it n-c rl(—up T(n + n) ± s-rIP p ) 1 -shewsu n-a (335) where t.tsdss eqaitibdam ussditisee each tnedamessat process ants its’ scares must selt-baleece iedspenuevt at ashes psocees uses may be scccmieu inside the materiel. This is beaus mae Prievspla of Detailed aateree. 1 n any a,elcse, like (3.3 flu) (3.36b) www.EasyEngineering.net 116 SEMICONDUCTOR FuNDAMENTALS CARNIENACTION It is left as an exercise to shuss tlsul the general-case relationship redeem to Eqs. (3.34) under the assumed special-case conditions. Light pctses 3.3.4 Minority Carrier Lifetimes General Information The lime constants 5 , which were introduced without comment in writing down 5 ’e and aEqs. (3.34), are obviously the “coastants of the action” asocialed with recambinateon— generation. Seeking to pranids insight relatise to the standard interpretation and naneeng of the a’s, let as consider ance again the situation pictured an Fig. 3.21. Enamsutng the change in the hole caeceutration with time, it goes almost wtthaal saying that the excess hales do not alt disappear at the same time. Rather, the hale excess present at r = 0 is systematecally eliminated, with same af she hales esistiug far only a shoes period and others “living” for comparatively bag periads of time. If thermal recombsaatioe—gennratman is the sole pro cess acting to relax the semicondnctor, the average excess hole lifetime, (r), can hr com puted in a relatively straightforward mueeer. Without going into details, the computation yields Q) = s- (or er). Physically, therefore, s5 and r have come to he interpreted us the axeruge rinse all excess mieterity carrier mill live in a sea of majority carriers. Par dents fication purpuses, s’, and tv are simply referred to ua the miearity currter lifetimes. Like thC ic’s and the Os, the a’s are important material parameters invariably reqatred in the modeling of devices. Unlike use ia’s and the 0’s, them me fesv plots indicatung the s--values to he employed in a given device structure. In fact, subsidiary experimental mea snmments (see the following subsectiox) mest he performed to determine the mieartty carrier lifetime in a given somicondectar sample. The reason for the luck uf catalogued information can be traced tu the extreme variability of the a and e’r parameters. Referring to Eqs. (3.33), we see that the carrier lifetimes depend an the often poarly cuetralled R—G center concentration (NT), stat on the carefully controlled doping pucuaneters (N ). 0 5 and N Moreover, the physical uutnre of the dominant R—G center conceotraiiaa chuoges eves svithin a given sample during device fabrication. A fabrication procedure rolled getrering can redcce lice R—G rearer concentration to a very low level and give rise to a s’e(s-t) I msec in Si. The inreumioaul introduction of gold into Si, on the other hand, ran control lubly increase the R—G ceeter concentration ned give rise to a Te(s’r) I nser. Minority carrier lifetimes ice cnmpleted Si devices tend to lie about midsxuy between the cited F/gem 3.22 Schematic illasceutiun u/the photmasduetiaity decay meoeureneeei. coaduetor daring the measurement. The perturbation is in the farm of a light pulse that gives risc to a carrier excess inside the semiconductor and a detectable change in conduc tivity. Once the light is removed the excess carriers are eliminated via rocombittutiun and the conductivity decoys back to its value in the dark. The carrier lifetime is determined by monitoring the conductivity decay. The experiment is schemntically illustrated its Pig. 3.22. N 5 is the sample resistance, a load resistor, V the applied d.c. voltage, and n, the measured laud or output valtugo. Obviously, N 5 and therefore n ace functions of time, with v 5 reflecting the changes in conductivity inside the semiconductor sample. We are spreiheully interested in how e ehnngrs with time after the light is turned off. n is related lathe conductivity, wleich in turs is related to the excess carrier concentrations. Given an st-type sample and assuming uniform phatogeneratiox throughout the semicon ductor, we will verify later in the chapter (Sectiun 3.5) that the decay of the excess minority carrier hate concentralian (Ap) is described by Ap(t) Ap is the excess hole concentration at r 0 the eovduclivity, we note = = e 0 Ap (3.37) use 0 when the light is turned off. Next considering - rxtremrs. C = UP p) 1 t + u 5 q(ia (3.38u) 0 + An) + iae(Pn + Ap)] 91cc (a A Lifetime Measurement The carrier lifetimes are measured using a variety of different methods. The maarity of measurements employ a device stractare of some sort and deduces-a and/or s-p by matching the theoretical and experimentally observed device characteristics. The measurement to hr described employs a bar-like piece of semiroadartor with ohmic contacts at its two ends. In a conemeecial implementation this structure is called u pharveondartar, a type of photo detector. A situation very similar to that envisioned in Pig. 3.21 is created inside the semi- q/uaNa + qCeic + /0e)AP (3,39) I U O’dask (3.30b) Aar(t) 1 h0 lie establishing Eq. (5.39), we mude use of the fact that n 0 m i Pt in an n-type semi cnttductmr. Also Asa was assumed eqnul to Ap. is the unpnrtorbsd sumple conductivity in the dark and Au’(t) a p represents the time decaying component of the conductivity. 117 ___________ __________ www.EasyEngineering.net • 114 SEMICONDUCTOR FUNDAMENTALS CANFIIDNACTIDN tf the hate generation process is analyzed in a siatilae matinee, iplit is deduced to depend only ae the camber of empty R—G centers. Titia camber, suhich is small foe the situatton nader coaaideratioe, is held approximatuty constant at its eqoilibriam same acer the range of perturbolloes where hole generation is significustl. Tltis means lhut can be replaced by iP/dtlx.wdI,s,im,. Mamoser, the recombiteulion and generation rates must precisely balance under equilibriuet renditions, t or dpfdtl 0 = dP/dtIa.e,rfs,ss,,,s, = Than, maksng use of Eq. (3.29), we obtain dP/itJvca,.b. Ill = OP/itici E’7” (3.33u) “j’ (3.33b( s-s . — = NTPO 5 r (3.30) Finally, the eel rate of change in the hole concentration due to the R—O renter inter action is given by = = + —erNT(p — Pu) which, when substitated into Eqs. (3.32), yield ww (331) or it — i-ssesml = rrNvAp for holes in an n-type material (3.32u) Au analaguns set of arguments yields iussss,t — = 5 Ns-An r far electrons in a p-type material (3.32b) c, like re in a positive proportionality constant. c, and en see mferred to as the eleereun and hole rapture coefficients, renpeetively. Although completely fuaetioeul as is, it is desieable to manipulate Eqs. (3.32) into a slightly more compact and meaningfal furm. An examination of the left-hand sides of Eqs. (3.32) reveals the dintensional un/Is are ihose of a concentration divided by time. Since Ap and An on the right-hand sides of the sasne equations are also concentrations, the cue stunts e . and e,,N utsai have units of I/time. It is thrtefam reasonable to inteadace lice N 5 time constants 115 for holes in ate a-type material w.E a .( 3 34a) syE ngi for electrons in a p-type material (3.34b) Equuttuns (3,34) are the desired end result, the special-ruse characterization of R—G center (indseect thermal) recombiuatiun—generstion, Although steady state or slowly varying conditions are implicitly assumed in the development of Eqs. (3.34), the relation ships con be applied mtth tItle error to most transient problems of iatermt. Ii should be restated chat a Ap < 0 is passibte and will give rise to a tsp/it’, , 50 > 0. A positive . u-n simply indicates that a carrier deficit 5 , 5155 ip/itJ,. exists inside the semicoedertor and geaeraanu is occurring at a more mpid rate than rernmbinutioa. ip/it ivesmui n-a and 1 Ua it mast he remembered, characterize the net effect of the thermal reeom binatian and thermal geueeatian processes. As duly emphasized, the Eq. (3.34) relationships apply only to minority carriers and as stluuuoos meeting the low-level injectina requirement. The more general steady state , valid for arbitrary Injection levels and both 151 result carrier types in a enndegenerate semi conductor, is nated for completeness sad fature referenue to be nee r ing . imt/itlissr,e,,t dpi it iui,,,m,a in it n-c rl(—up T(n + n) ± s-rIP p ) 1 -shewsu n-a net (335) where t.tsdss eqaitibdam ussditisee each tnedamessat process ants its’ scares must selt-baleece iedspenuevt at ashes psocees uses may be scccmieu inside the materiel. This is beaus mae Prievspla of Detailed aateree. 1 n any a,elcse, like (3.3 flu) (3.36b) www.EasyEngineering.net 116 SEMICONDUCTOR FuNDAMENTALS CARNIENACTION It is left as an exercise to shuss tlsul the general-case relationship redeem to Eqs. (3.34) under the assumed special-case conditions. Light pctses 3.3.4 Minority Carrier Lifetimes General Information The lime constants 5 , which were introduced without comment in writing down 5 ’e and aEqs. (3.34), are obviously the “coastants of the action” asocialed with recambinateon— generation. Seeking to pranids insight relatise to the standard interpretation and naneeng of the a’s, let as consider ance again the situation pictured an Fig. 3.21. Enamsutng the change in the hole caeceutration with time, it goes almost wtthaal saying that the excess hales do not alt disappear at the same time. Rather, the hale excess present at r = 0 is systematecally eliminated, with same af she hales esistiug far only a shoes period and others “living” for comparatively bag periads of time. If thermal recombsaatioe—gennratman is the sole pro cess acting to relax the semicondnctor, the average excess hole lifetime, (r), can hr com puted in a relatively straightforward mueeer. Without going into details, the computation yields Q) = s- (or er). Physically, therefore, s5 and r have come to he interpreted us the axeruge rinse all excess mieterity carrier mill live in a sea of majority carriers. Par dents fication purpuses, s’, and tv are simply referred to ua the miearity currter lifetimes. Like thC ic’s and the Os, the a’s are important material parameters invariably reqatred in the modeling of devices. Unlike use ia’s and the 0’s, them me fesv plots indicatung the s--values to he employed in a given device structure. In fact, subsidiary experimental mea snmments (see the following subsectiox) mest he performed to determine the mieartty carrier lifetime in a given somicondectar sample. The reason for the luck uf catalogued information can be traced tu the extreme variability of the a and e’r parameters. Referring to Eqs. (3.33), we see that the carrier lifetimes depend an the often poarly cuetralled R—G center concentration (NT), stat on the carefully controlled doping pucuaneters (N ). 0 5 and N Moreover, the physical uutnre of the dominant R—G center conceotraiiaa chuoges eves svithin a given sample during device fabrication. A fabrication procedure rolled getrering can redcce lice R—G rearer concentration to a very low level and give rise to a s’e(s-t) I msec in Si. The inreumioaul introduction of gold into Si, on the other hand, ran control lubly increase the R—G ceeter concentration ned give rise to a Te(s’r) I nser. Minority carrier lifetimes ice cnmpleted Si devices tend to lie about midsxuy between the cited F/gem 3.22 Schematic illasceutiun u/the photmasduetiaity decay meoeureneeei. coaduetor daring the measurement. The perturbation is in the farm of a light pulse that gives risc to a carrier excess inside the semiconductor and a detectable change in conduc tivity. Once the light is removed the excess carriers are eliminated via rocombittutiun and the conductivity decoys back to its value in the dark. The carrier lifetime is determined by monitoring the conductivity decay. The experiment is schemntically illustrated its Pig. 3.22. N 5 is the sample resistance, a load resistor, V the applied d.c. voltage, and n, the measured laud or output valtugo. Obviously, N 5 and therefore n ace functions of time, with v 5 reflecting the changes in conductivity inside the semiconductor sample. We are spreiheully interested in how e ehnngrs with time after the light is turned off. n is related lathe conductivity, wleich in turs is related to the excess carrier concentrations. Given an st-type sample and assuming uniform phatogeneratiox throughout the semicon ductor, we will verify later in the chapter (Sectiun 3.5) that the decay of the excess minority carrier hate concentralian (Ap) is described by Ap(t) Ap is the excess hole concentration at r 0 the eovduclivity, we note = = e 0 Ap (3.37) use 0 when the light is turned off. Next considering - rxtremrs. C = UP p) 1 t + u 5 q(ia (3.38u) 0 + An) + iae(Pn + Ap)] 91cc (a A Lifetime Measurement The carrier lifetimes are measured using a variety of different methods. The maarity of measurements employ a device stractare of some sort and deduces-a and/or s-p by matching the theoretical and experimentally observed device characteristics. The measurement to hr described employs a bar-like piece of semiroadartor with ohmic contacts at its two ends. In a conemeecial implementation this structure is called u pharveondartar, a type of photo detector. A situation very similar to that envisioned in Pig. 3.21 is created inside the semi- q/uaNa + qCeic + /0e)AP (3,39) I U O’dask (3.30b) Aar(t) 1 h0 lie establishing Eq. (5.39), we mude use of the fact that n 0 m i Pt in an n-type semi cnttductmr. Also Asa was assumed eqnul to Ap. is the unpnrtorbsd sumple conductivity in the dark and Au’(t) a p represents the time decaying component of the conductivity. 117 ___________ __________ • 114 SEMICONDUCTOR FUNDAMENTALS CANFIIDNACTIDN tf the hate generation process is analyzed in a siatilae matinee, iplit is deduced to depend only ae the camber of empty R—G centers. Titia camber, suhich is small foe the situatton nader coaaideratioe, is held approximatuty constant at its eqoilibriam same acer the range of perturbolloes where hole generation is significustl. Tltis means lhut can be replaced by iP/dtlx.wdI,s,im,. Mamoser, the recombiteulion and generation rates must precisely balance under equilibriuet renditions, t or dpfdtl 0 = dP/dtIa.e,rfs,ss,,,s, = Than, maksng use of Eq. (3.29), we obtain dP/itJvca,.b. Ill = OP/itici E’7” (3.33u) “j’ (3.33b( s-s . — = NTPO 5 r (3.30) which, when substitated into Eqs. (3.32), yield Finally, the eel rate of change in the hole concentration due to the R—O renter inter action is given by = —erNT(p + = — — i-ssesml = rrNvAp for holes in an n-type material (3.32u) far electrons in a p-type material (3.32b) Au analaguns set of arguments yields iussss,t — = 5 Ns-An r for holes in ate a-type material .( 3 34a) for electrons in a p-type material (3.34b) (331) Pu) or it 115 c, like re in a positive proportionality constant. c, and en see mferred to as the eleereun and hole rapture coefficients, renpeetively. Although completely fuaetioeul as is, it is desieable to manipulate Eqs. (3.32) into a slightly more compact and meaningfal furm. An examination of the left-hand sides of Eqs. (3.32) reveals the dintensional un/Is are ihose of a concentration divided by time. Since Ap and An on the right-hand sides of the sasne equations are also concentrations, the cue stunts e . and e,,N utsai have units of I/time. It is thrtefam reasonable to inteadace lice N 5 time constants Equuttuns (3,34) are the desired end result, the special-ruse characterization of R—G center (indseect thermal) recombiuatiun—generstion, Although steady state or slowly varying conditions are implicitly assumed in the development of Eqs. (3.34), the relation ships con be applied mtth tItle error to most transient problems of iatermt. Ii should be restated chat a Ap < 0 is passibte and will give rise to a tsp/it’, , 50 > 0. A positive . u-n simply indicates that a carrier deficit 5 , 5155 ip/itJ,. exists inside the semicoedertor and geaeraanu is occurring at a more mpid rate than rernmbinutioa. ip/it ivesmui n-a and 1 Ua it mast he remembered, characterize the net effect of the thermal reeom binatian and thermal geueeatian processes. As duly emphasized, the Eq. (3.34) relationships apply only to minority carriers and as stluuuoos meeting the low-level injectina requirement. The more general steady state , valid for arbitrary Injection levels and both 151 result carrier types in a enndegenerate semi conductor, is nated for completeness sad fature referenue to be imt/itlissr,e,,t dpi it iui,,,m,a in it n-c rl(—up T(n + n) ± s-rIP p ) 1 -shewsu n-a (335) where t.tsdss eqaitibdam ussditisee each tnedamessat process ants its’ scares must selt-baleece iedspenuevt at ashes psocees uses may be scccmieu inside the materiel. This is beaus mae Prievspla of Detailed aateree. 1 n any a,elcse, like (3.3 flu) (3.36b) www.EasyEngineering.net 116 SEMICONDUCTOR FuNDAMENTALS CARNIENACTION It is left as an exercise to shuss tlsul the general-case relationship redeem to Eqs. (3.34) under the assumed special-case conditions. Light pctses 3.3.4 Minority Carrier Lifetimes General Information The lime constants 5 , which were introduced without comment in writing down 5 ’e and aEqs. (3.34), are obviously the “coastants of the action” asocialed with recambinateon— generation. Seeking to pranids insight relatise to the standard interpretation and naneeng of the a’s, let as consider ance again the situation pictured an Fig. 3.21. Enamsutng the change in the hole caeceutration with time, it goes almost wtthaal saying that the excess hales do not alt disappear at the same time. Rather, the hale excess present at r = 0 is systematecally eliminated, with same af she hales esistiug far only a shoes period and others “living” for comparatively bag periads of time. If thermal recombsaatioe—gennratman is the sole pro cess acting to relax the semicondnctor, the average excess hole lifetime, (r), can hr com puted in a relatively straightforward mueeer. Without going into details, the computation yields Q) = s- (or er). Physically, therefore, s5 and r have come to he interpreted us the axeruge rinse all excess mieterity carrier mill live in a sea of majority carriers. Par dents fication purpuses, s’, and tv are simply referred to ua the miearity currter lifetimes. Like thC ic’s and the Os, the a’s are important material parameters invariably reqatred in the modeling of devices. Unlike use ia’s and the 0’s, them me fesv plots indicatung the s--values to he employed in a given device structure. In fact, subsidiary experimental mea snmments (see the following subsectiox) mest he performed to determine the mieartty carrier lifetime in a given somicondectar sample. The reason for the luck uf catalogued information can be traced tu the extreme variability of the a and e’r parameters. Referring to Eqs. (3.33), we see that the carrier lifetimes depend an the often poarly cuetralled R—G center concentration (NT), stat on the carefully controlled doping pucuaneters (N ). 0 5 and N Moreover, the physical uutnre of the dominant R—G center conceotraiiaa chuoges eves svithin a given sample during device fabrication. A fabrication procedure rolled getrering can redcce lice R—G rearer concentration to a very low level and give rise to a s’e(s-t) I msec in Si. The inreumioaul introduction of gold into Si, on the other hand, ran control lubly increase the R—G ceeter concentration ned give rise to a Te(s’r) I nser. Minority carrier lifetimes ice cnmpleted Si devices tend to lie about midsxuy between the cited ww w .Ea syE ngi nee rin g .ne t F/gem 3.22 Schematic illasceutiun u/the photmasduetiaity decay meoeureneeei. coaduetor daring the measurement. The perturbation is in the farm of a light pulse that gives risc to a carrier excess inside the semiconductor and a detectable change in conduc tivity. Once the light is removed the excess carriers are eliminated via rocombittutiun and the conductivity decoys back to its value in the dark. The carrier lifetime is determined by monitoring the conductivity decay. The experiment is schemntically illustrated its Pig. 3.22. N 5 is the sample resistance, a load resistor, V the applied d.c. voltage, and n, the measured laud or output valtugo. Obviously, N 5 and therefore n ace functions of time, with v 5 reflecting the changes in conductivity inside the semiconductor sample. We are spreiheully interested in how e ehnngrs with time after the light is turned off. n is related lathe conductivity, wleich in turs is related to the excess carrier concentrations. Given an st-type sample and assuming uniform phatogeneratiox throughout the semicon ductor, we will verify later in the chapter (Sectiun 3.5) that the decay of the excess minority carrier hate concentralian (Ap) is described by Ap(t) Ap is the excess hole concentration at r 0 the eovduclivity, we note = = e 0 Ap (3.37) use 0 when the light is turned off. Next considering - rxtremrs. C = UP p) 1 t + u 5 q(ia (3.38u) 0 + An) + iae(Pn + Ap)] 91cc (a A Lifetime Measurement q/uaNa + qCeic + /0e)AP The carrier lifetimes are measured using a variety of different methods. The maarity of measurements employ a device stractare of some sort and deduces-a and/or s-p by matching the theoretical and experimentally observed device characteristics. The measurement to hr described employs a bar-like piece of semiroadartor with ohmic contacts at its two ends. In a conemeecial implementation this structure is called u pharveondartar, a type of photo detector. A situation very similar to that envisioned in Pig. 3.21 is created inside the semi- www.EasyEngineering.net (3,39) I U O’dask (3.30b) Aar(t) 1 h0 lie establishing Eq. (5.39), we mude use of the fact that n 0 m i Pt in an n-type semi cnttductmr. Also Asa was assumed eqnul to Ap. is the unpnrtorbsd sumple conductivity in the dark and Au’(t) a p represents the time decaying component of the conductivity. 117 ___________ __________ • 114 SEMICONDUCTOR FUNDAMENTALS CANFIIDNACTIDN tf the hate generation process is analyzed in a siatilae matinee, iplit is deduced to depend only ae the camber of empty R—G centers. Titia camber, suhich is small foe the situatton nader coaaideratioe, is held approximatuty constant at its eqoilibriam same acer the range of perturbolloes where hole generation is significustl. Tltis means lhut can be replaced by iP/dtlx.wdI,s,im,. Mamoser, the recombiteulion and generation rates must precisely balance under equilibriuet renditions, t or dpfdtl 0 = dP/dtIa.e,rfs,ss,,,s, = Than, maksng use of Eq. (3.29), we obtain dP/itJvca,.b. Ill = OP/itici E’7” (3.33u) “j’ (3.33b( s-s . — = NTPO 5 r (3.30) which, when substitated into Eqs. (3.32), yield Finally, the eel rate of change in the hole concentration due to the R—O renter inter action is given by = = + —erNT(p — Pu) — i-ssesml = rrNvAp for holes in an n-type material (3.32u) far electrons in a p-type material (3.32b) Au analaguns set of arguments yields iussss,t — = 5 Ns-An r for holes in ate a-type material .( 3 34a) for electrons in a p-type material (3.34b) (331) or it 115 c, like re in a positive proportionality constant. c, and en see mferred to as the eleereun and hole rapture coefficients, renpeetively. Although completely fuaetioeul as is, it is desieable to manipulate Eqs. (3.32) into a slightly more compact and meaningfal furm. An examination of the left-hand sides of Eqs. (3.32) reveals the dintensional un/Is are ihose of a concentration divided by time. Since Ap and An on the right-hand sides of the sasne equations are also concentrations, the cue stunts e . and e,,N utsai have units of I/time. It is thrtefam reasonable to inteadace lice N 5 time constants Equuttuns (3,34) are the desired end result, the special-ruse characterization of R—G center (indseect thermal) recombiuatiun—generstion, Although steady state or slowly varying conditions are implicitly assumed in the development of Eqs. (3.34), the relation ships con be applied mtth tItle error to most transient problems of iatermt. Ii should be restated chat a Ap < 0 is passibte and will give rise to a tsp/it’, , 50 > 0. A positive . u-n simply indicates that a carrier deficit 5 , 5155 ip/itJ,. exists inside the semicoedertor and geaeraanu is occurring at a more mpid rate than rernmbinutioa. ip/it ivesmui n-a and 1 Ua it mast he remembered, characterize the net effect of the thermal reeom binatian and thermal geueeatian processes. As duly emphasized, the Eq. (3.34) relationships apply only to minority carriers and as stluuuoos meeting the low-level injectina requirement. The more general steady state , valid for arbitrary Injection levels and both 151 result carrier types in a enndegenerate semi conductor, is nated for completeness sad fature referenue to be imt/itlissr,e,,t dpi it iui,,,m,a in it n-c rl(—up T(n + n) ± s-rIP p ) 1 -shewsu n-a (335) where t.tsdss eqaitibdam ussditisee each tnedamessat process ants its’ scares must selt-baleece iedspenuevt at ashes psocees uses may be scccmieu inside the materiel. This is beaus mae Prievspla of Detailed aateree. 1 n any a,elcse, like (3.3 flu) (3.36b) www.EasyEngineering.net 116 SEMICONDUCTOR FuNDAMENTALS 117 CARNIENACTION It is left as an exercise to shuss tlsul the general-case relationship redeem to Eqs. (3.34) under the assumed special-case conditions. Light pctses 3.3.4 Minority Carrier Lifetimes General Information The lime constants 5 , which were introduced without comment in writing down 5 ’e and aEqs. (3.34), are obviously the “coastants of the action” asocialed with recambinateon— generation. Seeking to pranids insight relatise to the standard interpretation and naneeng of the a’s, let as consider ance again the situation pictured an Fig. 3.21. Enamsutng the change in the hole caeceutration with time, it goes almost wtthaal saying that the excess hales do not alt disappear at the same time. Rather, the hale excess present at r = 0 is systematecally eliminated, with same af she hales esistiug far only a shoes period and others “living” for comparatively bag periads of time. If thermal recombsaatioe—gennratman is the sole pro cess acting to relax the semicondnctor, the average excess hole lifetime, (r), can hr com puted in a relatively straightforward mueeer. Without going into details, the computation yields Q) = s- (or er). Physically, therefore, s5 and r have come to he interpreted us the axeruge rinse all excess mieterity carrier mill live in a sea of majority carriers. Par dents fication purpuses, s’, and tv are simply referred to ua the miearity currter lifetimes. Like thC ic’s and the Os, the a’s are important material parameters invariably reqatred in the modeling of devices. Unlike use ia’s and the 0’s, them me fesv plots indicatung the s--values to he employed in a given device structure. In fact, subsidiary experimental mea snmments (see the following subsectiox) mest he performed to determine the mieartty carrier lifetime in a given somicondectar sample. The reason for the luck uf catalogued information can be traced tu the extreme variability of the a and e’r parameters. Referring to Eqs. (3.33), we see that the carrier lifetimes depend an the often poarly cuetralled R—G center concentration (NT), stat on the carefully controlled doping pucuaneters (N ). 0 5 and N Moreover, the physical uutnre of the dominant R—G center conceotraiiaa chuoges eves svithin a given sample during device fabrication. A fabrication procedure rolled getrering can redcce lice R—G rearer concentration to a very low level and give rise to a s’e(s-t) I msec in Si. The inreumioaul introduction of gold into Si, on the other hand, ran control lubly increase the R—G ceeter concentration ned give rise to a Te(s’r) I nser. Minority carrier lifetimes ice cnmpleted Si devices tend to lie about midsxuy between the cited 3.22 Schematic illasceutiun u/the photmasduetiaity decay meoeureneeei. ww w.E F/gem coaduetor daring the measurement. The perturbation is in the farm of a light pulse that gives risc to a carrier excess inside the semiconductor and a detectable change in conduc tivity. Once the light is removed the excess carriers are eliminated via rocombittutiun and the conductivity decoys back to its value in the dark. The carrier lifetime is determined by monitoring the conductivity decay. The experiment is schemntically illustrated its Pig. 3.22. N 5 is the sample resistance, a load resistor, V the applied d.c. voltage, and n, the measured laud or output valtugo. Obviously, N 5 and therefore n ace functions of time, with v 5 reflecting the changes in conductivity inside the semiconductor sample. We are spreiheully interested in how e ehnngrs with time after the light is turned off. n is related lathe conductivity, wleich in turs is related to the excess carrier concentrations. Given an st-type sample and assuming uniform phatogeneratiox throughout the semicon ductor, we will verify later in the chapter (Sectiun 3.5) that the decay of the excess minority carrier hate concentralian (Ap) is described by asy En Ap(t) Ap is the excess hole concentration at r 0 the eovduclivity, we note = = gin e 0 Ap eer ing .ne (3.37) use 0 when the light is turned off. Next considering - rxtremrs. C = UP p) 1 t + u 5 q(ia (3.38u) 0 + An) + iae(Pn + Ap)] 91cc (a A Lifetime Measurement The carrier lifetimes are measured using a variety of different methods. The maarity of measurements employ a device stractare of some sort and deduces-a and/or s-p by matching the theoretical and experimentally observed device characteristics. The measurement to hr described employs a bar-like piece of semiroadartor with ohmic contacts at its two ends. In a conemeecial implementation this structure is called u pharveondartar, a type of photo detector. A situation very similar to that envisioned in Pig. 3.21 is created inside the semi- q/uaNa + qCeic + /0e)AP (3,39) I U O’dask (3.30b) Aar(t) 1 h0 lie establishing Eq. (5.39), we mude use of the fact that n 0 m i Pt in an n-type semi cnttductmr. Also Asa was assumed eqnul to Ap. is the unpnrtorbsd sumple conductivity in the dark and Au’(t) a p represents the time decaying component of the conductivity. www.EasyEngineering.net t www.EasyEngineering.net 118 SEMiCONDUCTOR FUNDAMENTALS The last step is to relate ty CAERIERACTt0N 119 and thu. Inspecting Fig. 3.22, one coectades = iR = Va .JL... (3.45) bat e!* R A cA , + thir)A 5 (a =R ( 55 cC 1(nvana 55 + tharj (34) where us the length, A the cross-sectional area, and 5 A 5 = 0sirk’t the dack resistance of the sample, respectively. Sabstitatiog Eq. (3.41) into Eq. (3.40) and reacranging yields ww w.E CL = ÷ (3.42) A I + iher)ec, as y En gin e or, if AL is watched to R and the light intensity restricted so specifying tow-level injection coeditians), we obtain m (t + tho/irS,,k aS I )eqnivalettt to = t’. + vc’”a (3.43) ‘St LiLJ d.c. eri decay transient An esponeotial decay is predicted with en being the decay constant. ng. ne .t 2 . 3 The eeqnired V, An actant itnplcmentatinn of the measnremcnt is shown in Fig. 3 is sapplied hy the Tektrottin FS5004 power snppty (jast nboat any power sapply woald t do), white the Tektronix 11401 Digitizing Osciltascope is nsnd to captore the photocon dnctive decay. The bar-shaped Si tent steactares are hoased in a special measarements hon along with the AL at A 55 load cesistar. Ttte box permits convenient handling of the samples and facilitates swttching hetweea samples. The tight pnlncs eeqniced in the measarement are derived from the Oeneral Radio 153 l-AE Stroboscope. Thn OR Stroboncnpe pnLv out high-intensity tight flashes of— I 0 asec daration spaced at controllable time intervals rang ing from 2.5 msec to 0.5 we. Fairly anifoem photogexeration can be achieved in a sample This hning the Oat tmt rnfeaaem. [tin pnthapn caethwhite reitmatisc the Dasceat tnsradacsan atninment that meassaninene panontnen, inctndnd ct nations points in isa tent, anc dnrinnd two enpoeinaona pnarnnnmd in an endaan En tabmntnrp adninieteod by ike nathor. A nonsense enp.nndcd ainccnnsn orbankgnnaed theney. 0 nndcr thc iecn.ineeneni eoaein. tad nmesnement pmeedaecn can ha teend in E. c Pietist, Scenicandsetar Mcannrr nenec Labcrnsoro Dperaeinnn Manant, Sepplenent A, in the Measlar Seems on Solid State Dnsieee, Addienn waster PahlenhennCn., Ecndinn MA, © toOt. - Figure 3.23 Phntnnnndantino decay eteanaremnet system. by first panning the ttcohetcnpe light throagh a small-diameter Si wafer. The Si wafnr acts as a fitter attowtng only near-bandgap radiation to reach the sample nedcr test. Althnngh the 11401 Oscilloscope in capable of in nito data analysis, a compatnr in connected to the onetlloscope to add data mantipalation and display llexibilitvt An example of the photocondnctive decay as displayed on the compoter screen is en peodaced m Fig. 3.24. The transient component of ne in millivolts is plotted on the y-axis verses time tn tmtlisecondn on the x-axis. The part (a) linear-scale plot nicely exhibits the generally expected dependence. The pact (b) semitog plot verifies the simple evpooential natara of the decay (at leant for times 0.1 msec S P 5 0.6 msec) mtd in more atefal for www.EasyEngineering.net / 120 neMiconnacvoe PUNnAMnNTALn CARNtnRACrtnN olE—S 3.4.1 Continuity Equations En Each and every type af carrier acdon—whether it be drift, diffation, indirect or direct thermal recombinatioo, indirect ar direct geoeratinn, or some other type of carrice action— gives risc to a change in the easier concentrations with time. The combined effect of all types of carrier action can therefore be taken into accoant by eqnating the overall change in the cacrier caacentmtions per nnit time (do/Sn or dp/dt) to the snm of the do/St’s or dy/dIn due to the individasl procensco; that in, ISO 0 dt an aan dt Se toenna4 St a tr 1 dr n—v dt ie In—a dt nt ÷52E Sc 010 0.2 0.4 0.6 0.0 1.0 n 0—3 SECONDS (a) ntk—3 SECONDS (3.44a) - eIe.t t (144b) . - St aac t The overall effect of the individaal processes in enlablished, in ensencn, by invoking the reqnieement of conservation of carriers. Electrons and holes cannot mysterionnly appear and disappear at a given point, bat mast be traosparted to or created at the given point via some type of otigoing carrier action. There mast be a spatial and time continaity in the carrier conceotratines. For this reason, Eqn. (3.44) ace known as the contittaity eqaatiotn.n. The continaity eqaationn can be written in a somewhat more compact form by voting (hi + Figute 3.24 Pltnmanvdnctivitg transient response. The tune-varying component of eeL in millivolts is plotted on the y-anis venan time in millieecnndn on the a-anin. (a) in a linnan and (b) is a nnntitag plat. dt St extracting the minarity carrier lifetime. Specifically, from the slope of the straight-lute region in the latter plot, the minority carrier lifetime in the probed sample is teadily de dnced lobe yr m 150 gsec. _!(tn÷Itse÷Lai’ ,,JV.J dy dc J q q\ dx Ann + dt as = _!(!!ga + a dy q\ dx Sc J = (3.45a) (145b) q Eqaations (3.45), which can be established by a straightforward mathematical manipala tion, merely state that there will be a change in the cavcinr concentrations within a given small region of the nemicondactor if an imbalance nxistn betsvcnn the total carrier earrents into and oat of the region. Utilizing Eqs. (3,45), we obtain 3.4 EQUATIONS OF STATE In the hrnt three sectinttn of this chapter ac examined and separately madeted the primary types nf catTier action Ia leg place ittvidc aeitticnndnctors. Withia actanl aemicnndactncn all the various types of carrier action accar at the snatte time, and the state of any seoticon dnctor can be determined sinly by taking into accoant the cnmbioed effect of the individaal types of carrier action. “Patting it all tngcthet,” solo speak, leads to the basic set of starting eqaationn emylnyrd in solving device problems, herein referred In as the equations nfatatc. The first pnrtian of this sectinn is devoted to developing the eqaatioes of state: the latter portion iectndcs a snnatoaey of common simplificatinns, a listing nf special-case nolntines, and peablem-solving enamptes. do! Sn Sn at St to St 4 = jp + aevva (3A6a) (3.46b) + otLncnnia The (3.46) continaity eqnntions arc ctsmpletety general and direcfiy or indirectly con stitatn the Starting point in mont device analyses. In compatcr simalatians the continaity 121 www.EasyEngineering.net 118 SEMiCONDUCTOR FUNDAMENTALS The last step is to relate ty CAERIERACTt0N 119 and thu. Inspecting Fig. 3.22, one coectades = iR = Va .JL... (3.45) bat R e!* A cA , + thir)A 5 (a =R ( 55 cC 1(nvana 55 + tharj (34) where us the length, A the cross-sectional area, and 5 A 5 = 0sirk’t the dack resistance of the sample, respectively. Sabstitatiog Eq. (3.41) into Eq. (3.40) and reacranging yields CL = or, if AL is watched to R and the light intensity restricted so specifying tow-level injection coeditians), we obtain m (t + (3.42) A ÷ I + iher)ec, tho/irS,,k aS I )eqnivalettt to = t’. + vc’”a ww w.E a (3.43) nee r LiLJ d.c. syE n ‘St gi decay transient ing . An esponeotial decay is predicted with en being the decay constant. .t 2 . 3 The eeqnired V, An actant itnplcmentatinn of the measnremcnt is shown in Fig. 3 is sapplied hy the Tektrottin FS5004 power snppty (jast nboat any power sapply woald do), white the Tektronix 11401 Digitizing Osciltascope is nsnd to captore the photocon dnctive decay. The bar-shaped Si tent steactares are hoased in a special measarements hon along with the AL at A 55 load cesistar. Ttte box permits convenient handling of the samples and facilitates swttching hetweea samples. The tight pnlncs eeqniced in the measarement are derived from the Oeneral Radio 153 l-AE Stroboscope. Thn OR Stroboncnpe pnLv out high-intensity tight flashes of— I 0 asec daration spaced at controllable time intervals rang ing from 2.5 msec to 0.5 we. Fairly anifoem photogexeration can be achieved in a sample This hning the Oat tmt rnfeaaem. [tin pnthapn caethwhite reitmatisc the Dasceat tnsradacsan atninment that meassaninene panontnen, inctndnd ct nations points in isa tent, anc dnrinnd two enpoeinaona pnarnnnmd in an endaan En tabmntnrp adninieteod by ike nathor. A nonsense enp.nndcd ainccnnsn orbankgnnaed theney. 0 nndcr thc iecn.ineeneni eoaein. tad nmesnement pmeedaecn can ha teend in E. c Pietist, Scenicandsetar Mcannrr nenec Labcrnsoro Dperaeinnn Manant, Sepplenent A, in the Measlar Seems on Solid State Dnsieee, Addienn waster PahlenhennCn., Ecndinn MA, © toOt. - Figure 3.23 Phntnnnndantino decay eteanaremnet system. net by first panning the ttcohetcnpe light throagh a small-diameter Si wafer. The Si wafnr acts as a fitter attowtng only near-bandgap radiation to reach the sample nedcr test. Althnngh the 11401 Oscilloscope in capable of in nito data analysis, a compatnr in connected to the onetlloscope to add data mantipalation and display llexibilitvt An example of the photocondnctive decay as displayed on the compoter screen is en peodaced m Fig. 3.24. The transient component of ne in millivolts is plotted on the y-axis verses time tn tmtlisecondn on the x-axis. The part (a) linear-scale plot nicely exhibits the generally expected dependence. The pact (b) semitog plot verifies the simple evpooential natara of the decay (at leant for times 0.1 msec S P 5 0.6 msec) mtd in more atefal for www.EasyEngineering.net / 120 neMiconnacvoe PUNnAMnNTALn CARNtnRACrtnN olE—S 3.4.1 Continuity Equations En Each and every type af carrier acdon—whether it be drift, diffation, indirect or direct thermal recombinatioo, indirect ar direct geoeratinn, or some other type of carrice action— gives risc to a change in the easier concentrations with time. The combined effect of all types of carrier action can therefore be taken into accoant by eqnating the overall change in the cacrier caacentmtions per nnit time (do/Sn or dp/dt) to the snm of the do/St’s or dy/dIn due to the individasl procensco; that in, ISO 0 dt an aan dt Se toenna4 St a tr 1 dr n—v dt ie In—a dt nt ÷52E Sc 010 0.2 0.4 0.6 0.0 1.0 n 0—3 SECONDS (a) ntk—3 SECONDS (3.44a) - eIe.t t (144b) . - St aac t The overall effect of the individaal processes in enlablished, in ensencn, by invoking the reqnieement of conservation of carriers. Electrons and holes cannot mysterionnly appear and disappear at a given point, bat mast be traosparted to or created at the given point via some type of otigoing carrier action. There mast be a spatial and time continaity in the carrier conceotratines. For this reason, Eqn. (3.44) ace known as the contittaity eqaatiotn.n. The continaity eqaationn can be written in a somewhat more compact form by voting (hi + Figute 3.24 Pltnmanvdnctivitg transient response. The tune-varying component of eeL in millivolts is plotted on the y-anis venan time in millieecnndn on the a-anin. (a) in a linnan and (b) is a nnntitag plat. dt St extracting the minarity carrier lifetime. Specifically, from the slope of the straight-lute region in the latter plot, the minority carrier lifetime in the probed sample is teadily de dnced lobe yr m 150 gsec. _!(tn÷Itse÷Lai’ ,,JV.J dy dc J q q\ dx Ann + dt as = _!(!!ga + a dy q\ dx Sc J = (3.45a) (145b) q Eqaations (3.45), which can be established by a straightforward mathematical manipala tion, merely state that there will be a change in the cavcinr concentrations within a given small region of the nemicondactor if an imbalance nxistn betsvcnn the total carrier earrents into and oat of the region. Utilizing Eqs. (3,45), we obtain 3.4 EQUATIONS OF STATE In the hrnt three sectinttn of this chapter ac examined and separately madeted the primary types nf catTier action Ia leg place ittvidc aeitticnndnctors. Withia actanl aemicnndactncn all the various types of carrier action accar at the snatte time, and the state of any seoticon dnctor can be determined sinly by taking into accoant the cnmbioed effect of the individaal types of carrier action. “Patting it all tngcthet,” solo speak, leads to the basic set of starting eqaationn emylnyrd in solving device problems, herein referred In as the equations nfatatc. The first pnrtian of this sectinn is devoted to developing the eqaatioes of state: the latter portion iectndcs a snnatoaey of common simplificatinns, a listing nf special-case nolntines, and peablem-solving enamptes. do! Sn Sn at St to St 4 = jp + aevva (3A6a) (3.46b) + otLncnnia The (3.46) continaity eqnntions arc ctsmpletety general and direcfiy or indirectly con stitatn the Starting point in mont device analyses. In compatcr simalatians the continaity 121 118 SEMiCONDUCTOR FUNDAMENTALS The last step is to relate ty CAERIERACTt0N 119 and thu. Inspecting Fig. 3.22, one coectades = iR = .JL... Va (3.45) bat e!* R cA A , + thir)A 5 (a =R ( 55 cC 1(nvana 55 (34) + tharj where us the length, A the cross-sectional area, and 5 A 5 = 0sirk’t the dack resistance of the sample, respectively. Sabstitatiog Eq. (3.41) into Eq. (3.40) and reacranging yields CL = ÷ or, if AL is watched to R and the light intensity restricted so specifying tow-level injection coeditians), we obtain m (t + (3.42) A I + iher)ec, tho/irS,,k aS I )eqnivalettt to = t’. + vc’”a (3.43) ‘St LiLJ d.c. decay transient An esponeotial decay is predicted with en being the decay constant. .t 2 . 3 The eeqnired V, An actant itnplcmentatinn of the measnremcnt is shown in Fig. 3 is sapplied hy the Tektrottin FS5004 power snppty (jast nboat any power sapply woald do), white the Tektronix 11401 Digitizing Osciltascope is nsnd to captore the photocon dnctive decay. The bar-shaped Si tent steactares are hoased in a special measarements hon along with the AL at A 55 load cesistar. Ttte box permits convenient handling of the samples and facilitates swttching hetweea samples. The tight pnlncs eeqniced in the measarement are derived from the Oeneral Radio 153 l-AE Stroboscope. Thn OR Stroboncnpe pnLv out high-intensity tight flashes of— I 0 asec daration spaced at controllable time intervals rang ing from 2.5 msec to 0.5 we. Fairly anifoem photogexeration can be achieved in a sample This hning the Oat tmt rnfeaaem. [tin pnthapn caethwhite reitmatisc the Dasceat tnsradacsan atninment that meassaninene panontnen, inctndnd ct nations points in isa tent, anc dnrinnd two enpoeinaona pnarnnnmd in an endaan En tabmntnrp adninieteod by ike nathor. A nonsense enp.nndcd ainccnnsn orbankgnnaed theney. 0 nndcr thc iecn.ineeneni eoaein. tad nmesnement pmeedaecn can ha teend in E. c Pietist, Scenicandsetar Mcannrr nenec Labcrnsoro Dperaeinnn Manant, Sepplenent A, in the Measlar Seems on Solid State Dnsieee, Addienn waster PahlenhennCn., Ecndinn MA, © toOt. - Figure 3.23 Phntnnnndantino decay eteanaremnet system. by first panning the ttcohetcnpe light throagh a small-diameter Si wafer. The Si wafnr acts as a fitter attowtng only near-bandgap radiation to reach the sample nedcr test. Althnngh the 11401 Oscilloscope in capable of in nito data analysis, a compatnr in connected to the onetlloscope to add data mantipalation and display llexibilitvt An example of the photocondnctive decay as displayed on the compoter screen is en peodaced m Fig. 3.24. The transient component of ne in millivolts is plotted on the y-axis verses time tn tmtlisecondn on the x-axis. The part (a) linear-scale plot nicely exhibits the generally expected dependence. The pact (b) semitog plot verifies the simple evpooential natara of the decay (at leant for times 0.1 msec S P 5 0.6 msec) mtd in more atefal for www.EasyEngineering.net / 120 neMiconnacvoe PUNnAMnNTALn CARNtnRACrtnN olE—S 3.4.1 Continuity Equations En Each and every type af carrier acdon—whether it be drift, diffation, indirect or direct thermal recombinatioo, indirect ar direct geoeratinn, or some other type of carrice action— gives risc to a change in the easier concentrations with time. The combined effect of all types of carrier action can therefore be taken into accoant by eqnating the overall change in the cacrier caacentmtions per nnit time (do/Sn or dp/dt) to the snm of the do/St’s or dy/dIn due to the individasl procensco; that in, ISO 0 ww w 0.2 an aan dt Se toenna4 St a tr 1 dr n—v dt ie In—a dt nt ÷52E Sc 010 dt .Ea 0.4 syE 0.6 0.0 1.0 n 0—3 ngi SECONDS (a) ntk—3 SECONDS nee rin g (3.44a) - eIe.t t (144b) . - St aac t The overall effect of the individaal processes in enlablished, in ensencn, by invoking the reqnieement of conservation of carriers. Electrons and holes cannot mysterionnly appear and disappear at a given point, bat mast be traosparted to or created at the given point via some type of otigoing carrier action. There mast be a spatial and time continaity in the carrier conceotratines. For this reason, Eqn. (3.44) ace known as the contittaity eqaatiotn.n. The continaity eqaationn can be written in a somewhat more compact form by voting (hi + Figute 3.24 Pltnmanvdnctivitg transient response. The tune-varying component of eeL in millivolts is plotted on the y-anis venan time in millieecnndn on the a-anin. (a) in a linnan and (b) is a nnntitag plat. .ne t extracting the minarity carrier lifetime. Specifically, from the slope of the straight-lute region in the latter plot, the minority carrier lifetime in the probed sample is teadily de dnced lobe yr m 150 gsec. dt St _!(tn÷Itse÷Lai’ ,,JV.J dy dc J q q\ dx Ann + dt as = _!(!!ga + a dy q\ dx Sc J = (3.45a) (145b) q Eqaations (3.45), which can be established by a straightforward mathematical manipala tion, merely state that there will be a change in the cavcinr concentrations within a given small region of the nemicondactor if an imbalance nxistn betsvcnn the total carrier earrents into and oat of the region. Utilizing Eqs. (3,45), we obtain 3.4 EQUATIONS OF STATE In the hrnt three sectinttn of this chapter ac examined and separately madeted the primary types nf catTier action Ia leg place ittvidc aeitticnndnctors. Withia actanl aemicnndactncn all the various types of carrier action accar at the snatte time, and the state of any seoticon dnctor can be determined sinly by taking into accoant the cnmbioed effect of the individaal types of carrier action. “Patting it all tngcthet,” solo speak, leads to the basic set of starting eqaationn emylnyrd in solving device problems, herein referred In as the equations nfatatc. The first pnrtian of this sectinn is devoted to developing the eqaatioes of state: the latter portion iectndcs a snnatoaey of common simplificatinns, a listing nf special-case nolntines, and peablem-solving enamptes. www.EasyEngineering.net do! Sn Sn at St to St 4 = jp + aevva (3A6a) (3.46b) + otLncnnia The (3.46) continaity eqnntions arc ctsmpletety general and direcfiy or indirectly con stitatn the Starting point in mont device analyses. In compatcr simalatians the continaity 121 118 SEMiCONDUCTOR FUNDAMENTALS The last step is to relate ty CAERIERACTt0N 119 and thu. Inspecting Fig. 3.22, one coectades = iR = Va .JL... (3.45) bat R e!* A cA , + thir)A 5 (a =R ( 55 cC 1(nvana 55 + tharj (34) where us the length, A the cross-sectional area, and 5 A 5 = 0sirk’t the dack resistance of the sample, respectively. Sabstitatiog Eq. (3.41) into Eq. (3.40) and reacranging yields CL = ÷ or, if AL is watched to R and the light intensity restricted so specifying tow-level injection coeditians), we obtain m (t + (3.42) A I + iher)ec, tho/irS,,k aS I )eqnivalettt to = t’. + vc’”a (3.43) ‘St LiLJ d.c. decay transient An esponeotial decay is predicted with en being the decay constant. .t 2 . 3 The eeqnired V, An actant itnplcmentatinn of the measnremcnt is shown in Fig. 3 is sapplied hy the Tektrottin FS5004 power snppty (jast nboat any power sapply woald do), white the Tektronix 11401 Digitizing Osciltascope is nsnd to captore the photocon dnctive decay. The bar-shaped Si tent steactares are hoased in a special measarements hon along with the AL at A 55 load cesistar. Ttte box permits convenient handling of the samples and facilitates swttching hetweea samples. The tight pnlncs eeqniced in the measarement are derived from the Oeneral Radio 153 l-AE Stroboscope. Thn OR Stroboncnpe pnLv out high-intensity tight flashes of— I 0 asec daration spaced at controllable time intervals rang ing from 2.5 msec to 0.5 we. Fairly anifoem photogexeration can be achieved in a sample This hning the Oat tmt rnfeaaem. [tin pnthapn caethwhite reitmatisc the Dasceat tnsradacsan atninment that meassaninene panontnen, inctndnd ct nations points in isa tent, anc dnrinnd two enpoeinaona pnarnnnmd in an endaan En tabmntnrp adninieteod by ike nathor. A nonsense enp.nndcd ainccnnsn orbankgnnaed theney. 0 nndcr thc iecn.ineeneni eoaein. tad nmesnement pmeedaecn can ha teend in E. c Pietist, Scenicandsetar Mcannrr nenec Labcrnsoro Dperaeinnn Manant, Sepplenent A, in the Measlar Seems on Solid State Dnsieee, Addienn waster PahlenhennCn., Ecndinn MA, © toOt. - Figure 3.23 Phntnnnndantino decay eteanaremnet system. by first panning the ttcohetcnpe light throagh a small-diameter Si wafer. The Si wafnr acts as a fitter attowtng only near-bandgap radiation to reach the sample nedcr test. Althnngh the 11401 Oscilloscope in capable of in nito data analysis, a compatnr in connected to the onetlloscope to add data mantipalation and display llexibilitvt An example of the photocondnctive decay as displayed on the compoter screen is en peodaced m Fig. 3.24. The transient component of ne in millivolts is plotted on the y-axis verses time tn tmtlisecondn on the x-axis. The part (a) linear-scale plot nicely exhibits the generally expected dependence. The pact (b) semitog plot verifies the simple evpooential natara of the decay (at leant for times 0.1 msec S P 5 0.6 msec) mtd in more atefal for www.EasyEngineering.net / 120 neMiconnacvoe PUNnAMnNTALn CARNtnRACrtnN olE—S 121 3.4.1 Continuity Equations En Each and every type af carrier acdon—whether it be drift, diffation, indirect or direct thermal recombinatioo, indirect ar direct geoeratinn, or some other type of carrice action— gives risc to a change in the easier concentrations with time. The combined effect of all types of carrier action can therefore be taken into accoant by eqnating the overall change in the cacrier caacentmtions per nnit time (do/Sn or dp/dt) to the snm of the do/St’s or dy/dIn due to the individasl procensco; that in, ISO 0 dt an aan dt Se ww w.E Sc 010 0.2 0.4 0.6 0.0 1.0 n 0—3 SECONDS (a) ntk—3 SECONDS dr n—v dt ie In—a dt nt ÷52E (3.44a) - eIe.t t (144b) . - St aac t The overall effect of the individaal processes in enlablished, in ensencn, by invoking the reqnieement of conservation of carriers. Electrons and holes cannot mysterionnly appear and disappear at a given point, bat mast be traosparted to or created at the given point via some type of otigoing carrier action. There mast be a spatial and time continaity in the carrier conceotratines. For this reason, Eqn. (3.44) ace known as the contittaity eqaatiotn.n. The continaity eqaationn can be written in a somewhat more compact form by voting asy En (hi + Figute 3.24 Pltnmanvdnctivitg transient response. The tune-varying component of eeL in millivolts is plotted on the y-anis venan time in millieecnndn on the a-anin. (a) in a linnan and (b) is a nnntitag plat. dt St extracting the minarity carrier lifetime. Specifically, from the slope of the straight-lute region in the latter plot, the minority carrier lifetime in the probed sample is teadily de dnced lobe yr m 150 gsec. toenna4 St a tr 1 + gin eer _!(tn÷Itse÷Lai’ ,,JV.J dy dc J q q\ dx Ann dt as = _!(!!ga + a dy q\ dx Sc J = q (3.45a) ing (145b) .ne Eqaations (3.45), which can be established by a straightforward mathematical manipala tion, merely state that there will be a change in the cavcinr concentrations within a given small region of the nemicondactor if an imbalance nxistn betsvcnn the total carrier earrents into and oat of the region. Utilizing Eqs. (3,45), we obtain 3.4 EQUATIONS OF STATE In the hrnt three sectinttn of this chapter ac examined and separately madeted the primary types nf catTier action Ia leg place ittvidc aeitticnndnctors. Withia actanl aemicnndactncn all the various types of carrier action accar at the snatte time, and the state of any seoticon dnctor can be determined sinly by taking into accoant the cnmbioed effect of the individaal types of carrier action. “Patting it all tngcthet,” solo speak, leads to the basic set of starting eqaationn emylnyrd in solving device problems, herein referred In as the equations nfatatc. The first pnrtian of this sectinn is devoted to developing the eqaatioes of state: the latter portion iectndcs a snnatoaey of common simplificatinns, a listing nf special-case nolntines, and peablem-solving enamptes. do! Sn Sn at St to St 4 = jp + aevva (3A6a) (3.46b) + otLncnnia The (3.46) continaity eqnntions arc ctsmpletety general and direcfiy or indirectly con stitatn the Starting point in mont device analyses. In compatcr simalatians the continaity www.EasyEngineering.net t www.EasyEngineering.net 122 SEMICONDUCTOR FUNDAMENTALS CARRIER ACTION equations are often employed directly. The appropriate relationships for Ifl/dt’.;,a n-c’ [which may or may not be the spectal-case relationships given by Eqs. (3.34)], along with the concentration changes due to “other processes.” arc substituted into Eqs. (3.46), and numerical solutions ann sought for ;,].r y, z, r) and p(x, y, z, t). In problems where a closed-form type of solution is desired, the continuity eqautions are typically utilized only in an indirect fashion. The actual starling point in such analyses is simplified version of the continuity equations to be establishcd in the next sabsection. 6,i — dAn tn + — lix dx = — dx 3.4.2 Minority Carrier Diffusion Equations D 5 dx - (I) The particular system under analysis is one-dimesaio,tal; i.e., all variables are at most function ofjnvt one coordinate (say the x.coordtnate). w.E = 0 in the semiconductor or regions of the semiconductor subject to analysts. (3.51) — 7,, n-O (2) The analysis is limited or mutricted to minority carriers. as y En gin e (3.50) Turntng to the remaining terms in the contiaaily equation for electnons, the assumed dominance of rccombination—generution via R—G centers, combined with the low-level injection and minority carrier restrictions, allows as to replace the thermal R—G term with the Eq. (3.34) special-case expression. The “workhorse” minority carrier diffusion eqnations are derived from the continuity equations by invoking the following set of sintplilytng assamptions: (3) ‘6 (3.49] dr Conshining Eqs. (3.47) through (3.49) yields q ww dAn = In addition, applying simplification (7) yields (4) The equilibrium minority carrier concentrations are nor a function of posItion. In other words, n 0 a (c) Pa Pt(x). t (3.52) = (5) I,ou’-let’el injection conditions prevail. (6) Indirect thermal recombitsation—generation is the dottunattt thermal R—G tncchanism. where it is understood that G 1 0 if the semiconductor is not subject to illumination. Finally, the equilibrium electron concentration is never a fur,csion of time, 0 nn * (t), and 0 sve can therefore write (7) Three are no “other processes,” eucept possibly phosogeuerutton, taking place within the system. eri Working on the continuity equation for electrons, we note that ng. ne t if the syotem is one-dimensional. Moreover, — at (3.47) q4x q qD? at at (3.53) at Sabstittating Eqs. (3.50) through (3.53) into the (3.46a) continuity equation, mid simalta neonsly recording the analogous result for holes, one ohtuins (3.48) qDxfix 6.e 123 tD?Attc+G when ‘6 0 and one is concerned only with minority carriers [simplificutious (2) and (3)]. By way of explanation, the drift component cats be neglected in the current density expres sion because ‘6 is small by assumption and minority carrier concentrations are also small, making the eN product extremely small. (Note that the same argument cannot be applied An, we 5 rs n so majority caruiens.) Since by assumption n (x), and by definition ii 0 can also svrite D’’ + — (3.54a) Minority carrier diffusion equations ,,j (3.54b) Subscripts are added to the carrier concentrations in Eqs. (3.54)10 rensind the user that the equations are valid only for minority carriers, applying to electrotis in p-type materials and to hales in n-type materials. - www.EasyEngineering.net SEMiCONDUCTOR FUNDAMENTALS CARRiEN AC1SON Table 3.1 Common Diffusion Eauation Simnlificutions. Sinsplifiration Effect Steady state No concentration gradient or no diss 2 a D3 diffusion Current No drift carrent orN = 0 (dAp, 1, at 0 61 Table 3.2 t 0 No further simplification. (‘10 in the derivation.) NothermalR-G — No light G —a 0 luition no, 1 9 S s._.Gt’VEN; Steady state, no light. SIMPLIFiED DIFF.EQN; 0 = DN!z o) (‘ —a Common Special-Case Diffusion Equation Solutions o) SOLUTION; 0 is assumed where SOLUTION; GIVEN; In the course of performing device analyses, the conditions of a problem often permit ad ditional simphificutions thai drastically reduce the complexity of the minority carrier diffu sion eqnattons. Common simplificatiuns and their effect on the minority carrier diffusion eqaations are summarized in Table 3.1. Extensively utilized solutions to simplified forms of the minority carrier diffusion equations are collected for future reference in Table 3.2. An(0)e ,‘c 0 ——° 7, SOLUTION; 0 An + GL = Solution no. 4 GIVEN: Steady state, no R—G, no light. SIMPLIFIED DIFF EQN; 0 or 2 eLn SOLUTION: (x) = A + Bx 0 rbn 3.4.4 Problem Solving Devicu analyses of coarse provide examples of “problem” solutions, and a number of Pt A uniformly donor-doped silicon wafer maintainnd at room temperature is suddenly An ( 0 r) Steady state, no concentration gradient. SIMPLIFIED DIFF.EQIs’; Although we have presented all necessary information, it may not be completely obvious how one works with the diffusion equations to obtain the carrier concentration solutions. illuminated with light at timer Lw Solution no. 3 3.4.3 Simplifications and Solutions Sample Problem No.1 — AetLn + Be”u Solution no. 2 GIVEN,’ No concentration gradient, no light. SIMPLIFIED DJFFi EQN.’ -0 0 - = and A, Bare solution constants. (v —o) device analyses are presented later in the text. Nevertheless, it is worthwhile to examine a few well-deE ned siniple problems to illustrate problem_solving procedures. The chosen sample problems also provide a basis for the two supplemental concepts introduced in the next section. An(x) 0 The semiconductor is silicon, T = 300 K, the donor doping is the same everyivhere wish iVn = I0°/cm’, and -sec at all points inside the semiconducior. t /cm t3 L = l0 0 Also, the statement of the problem implies eqailibriam conditions exist for t < 0. Step l—Charactertze the system under equilibrium conditions. In Si at room temperature ti = 10°/cm . Since N 5 0 fi. n, n 0 = Na = lO°Icm 3 and = n /N 2 /cm With the doping beiitg uniform, the equilibrium 0 5 lO . 3 n and p 0 values are the = 0. Assuming N 0 = 10°/cm , r = 10° see, and alight3 i7 electrons and holes per induced creation of 10 -sec throughoat the semiconductor, 5 cm determine Ap,, (I) for r> 0. 0 p St Step I—Review precisely what information is given or implied in the statement of the probiem Step 3—Analyze the problem qualitatively. Prior to r = 0, equilibrium conditions prevail and Ap saute everywhere throughoat the setssiconductor. = 0. ‘Starting at t 0 the tight creates added electrons and holes and Ap, will begin to increase. The growing excess 125 www.EasyEngineering.net 122 SEMICONDUCTOR FUNDAMENTALS 6,i — dAn tn + — lix dx = — dx 3.4.2 Minority Carrier Diffusion Equations The “workhorse” minority carrier diffusion eqnations are derived from the continuity equations by invoking the following set of sintplilytng assamptions: (I) The particular system under analysis is one-dimesaio,tal; i.e., all variables are at most function ofjnvt one coordinate (say the x.coordtnate). (2) The analysis is limited or mutricted to minority carriers. dAn = D 5 dx - ww 0 in the semiconductor or regions of the semiconductor subject to analysts. w.E a = (3.51) — 7,, n-O In addition, applying simplification (7) yields syE ngi (3.52) = (5) I,ou’-let’el injection conditions prevail. (6) Indirect thermal recombitsation—generation is the dottunattt thermal R—G tncchanism. nee r where it is understood that G 1 0 if the semiconductor is not subject to illumination. Finally, the equilibrium electron concentration is never a fur,csion of time, 0 nn * (t), and 0 sve can therefore write (7) Three are no “other processes,” eucept possibly phosogeuerutton, taking place within the system. Working on the continuity equation for electrons, we note that at (3.47) q4x (3.50) Turntng to the remaining terms in the contiaaily equation for electnons, the assumed dominance of rccombination—generution via R—G centers, combined with the low-level injection and minority carrier restrictions, allows as to replace the thermal R—G term with the Eq. (3.34) special-case expression. (4) The equilibrium minority carrier concentrations are nor a function of posItion. In other words, n 0 a (c) Pa Pt(x). t q (3.49] dr Conshining Eqs. (3.47) through (3.49) yields q (3) ‘6 123 CARRIER ACTION equations are often employed directly. The appropriate relationships for Ifl/dt’.;,a n-c’ [which may or may not be the spectal-case relationships given by Eqs. (3.34)], along with the concentration changes due to “other processes.” arc substituted into Eqs. (3.46), and numerical solutions ann sought for ;,].r y, z, r) and p(x, y, z, t). In problems where a closed-form type of solution is desired, the continuity eqautions are typically utilized only in an indirect fashion. The actual starling point in such analyses is simplified version of the continuity equations to be establishcd in the next sabsection. at at at ing . (3.53) neonsly recording the analogous result for holes, one ohtuins if the syotem is one-dimensional. Moreover, — qD? (3.48) qDxfix 6.e net Sabstittating Eqs. (3.50) through (3.53) into the (3.46a) contin